advertisement

PRINCIPLES OF COMPOSITE MATERIAL MECHANICS FOURTH EDITION MECHANICAL ENGINEERING A Series of Textbooks and Reference Books Founding Editor L. L. Faulkner Columbus Division, Battelle Memorial Institute and Department of Mechanical Engineering The Ohio State University Columbus, Ohio RECENTLY PUBLISHED TITLES Principles of Composite Material Mechanics, Fourth Edition Ronald F. Gibson Steam Generators and Waste Heat Boilers: For Process and Plant Engineers V. Ganapathy Maintenance, Replacement, and Reliability: Theory and Applications, Second Edition Andrew K.S. Jardine and Albert H.C. Tsang Heat Exchanger Design Handbook, Second Edition, Kuppan Thulukkanam Vehicle Dynamics, Stability, and Control, Second Edition, Dean Karnopp HVAC Water Chillers and Cooling Towers: Fundamentals, Application, and Operation, Second Edition, Herbert W. Stanford III Ultrasonics: Fundamentals, Technologies, and Applications, Third Edition, Dale Ensminger and Leonard J. Bond Mechanical Tolerance Stackup and Analysis, Second Edition, Bryan R. Fischer Asset Management Excellence, John D. Campbell, Andrew K. S. Jardine, and Joel McGlynn Solid Fuels Combustion and Gasiication: Modeling, Simulation, and Equipment Operations, Second Edition, Third Edition, Marcio L. de Souza-Santos Mechanical Vibration Analysis, Uncertainties, and Control, Third Edition, Haym Benaroya and Mark L. Nagurka Principles of Biomechanics, Ronald L. Huston Practical Stress Analysis in Engineering Design, Third Edition, Ronald L. Huston and Harold Josephs PRINCIPLES OF COMPOSITE MATERIAL MECHANICS FOURTH EDITION Ronald F. Gibson Boca Raton London New York CRC Press is an imprint of the Taylor & Francis Group, an informa business CRC Press Taylor & Francis Group 6000 Broken Sound Parkway NW, Suite 300 Boca Raton, FL 33487-2742 © 2016 by Taylor & Francis Group, LLC CRC Press is an imprint of Taylor & Francis Group, an Informa business No claim to original U.S. Government works Version Date: 20151215 International Standard Book Number-13: 978-1-4987-2072-4 (eBook - PDF) This book contains information obtained from authentic and highly regarded sources. Reasonable efforts have been made to publish reliable data and information, but the author and publisher cannot assume responsibility for the validity of all materials or the consequences of their use. The authors and publishers have attempted to trace the copyright holders of all material reproduced in this publication and apologize to copyright holders if permission to publish in this form has not been obtained. If any copyright material has not been acknowledged please write and let us know so we may rectify in any future reprint. Except as permitted under U.S. Copyright Law, no part of this book may be reprinted, reproduced, transmitted, or utilized in any form by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying, microfilming, and recording, or in any information storage or retrieval system, without written permission from the publishers. For permission to photocopy or use material electronically from this work, please access www.copyright.com (http://www.copyright.com/) or contact the Copyright Clearance Center, Inc. (CCC), 222 Rosewood Drive, Danvers, MA 01923, 978-750-8400. CCC is a not-for-profit organization that provides licenses and registration for a variety of users. For organizations that have been granted a photocopy license by the CCC, a separate system of payment has been arranged. Trademark Notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation without intent to infringe. Visit the Taylor & Francis Web site at http://www.taylorandfrancis.com and the CRC Press Web site at http://www.crcpress.com To my wonderful family, Maryanne, Tracy, Tola, Sophie, and Aidan, and the memory of my parents, Jim and Lora Gibson Contents Preface to the First Edition................................................................................. xiii Preface to the Second Edition ........................................................................... xvii Preface to the Third Edition .............................................................................. xix Preface to This Edition ....................................................................................... xxi Author ................................................................................................................. xxiii 1. Introduction .....................................................................................................1 1.1 Basic Concepts ....................................................................................... 1 1.2 Constituent Materials for Composites ...............................................5 1.2.1 Reinforcement Materials including Nanoreinforcements .............................................................10 1.2.2 Matrix and Filler Materials................................................... 12 1.3 Structural Applications of Composites ............................................ 18 1.4 Multifunctional Applications of Composites.................................. 28 1.5 Fabrication Processes .......................................................................... 31 1.6 Elements of Mechanical Behavior of Composites ..........................42 1.7 Review of Basic Mechanics of Materials Equations .......................44 References ....................................................................................................... 55 2. Lamina Stress–Strain Relationships ........................................................ 57 2.1 Introduction ......................................................................................... 57 2.2 Effective Moduli in Stress–Strain Relationships ............................ 58 2.3 Symmetry in Stress–Strain Relationships ....................................... 62 2.4 Orthotropic and Isotropic Engineering Constants ........................ 69 2.5 Specially Orthotropic Lamina........................................................... 73 2.6 Generally Orthotropic Lamina ......................................................... 78 References ....................................................................................................... 94 3. Effective Moduli of a Continuous Fiber-Reinforced Lamina ............. 95 3.1 Introduction ......................................................................................... 95 3.2 Elementary Mechanics of Materials Models ................................. 104 3.2.1 Longitudinal Modulus ........................................................ 106 3.2.2 Transverse Modulus ............................................................ 110 3.2.3 Shear Modulus and Poisson’s Ratio .................................. 112 3.3 Improved Mechanics of Materials Models .................................... 120 3.4 Elasticity Models ............................................................................... 124 3.4.1 Finite Difference Models..................................................... 126 3.4.2 Finite Element Models......................................................... 129 vii viii Contents 3.4.3 Closed-Form and Variational Models ............................... 133 3.5 Semiempirical Models ...................................................................... 134 References ..................................................................................................... 140 4. Strength of a Continuous Fiber-Reinforced Lamina .......................... 143 4.1 Introduction ....................................................................................... 143 4.2 Multiaxial Strength Criteria ............................................................ 146 4.2.1 Maximum Stress Criterion ................................................. 147 4.2.2 Maximum Strain Criterion ................................................. 151 4.2.3 Quadratic Interaction Criteria ............................................ 153 4.3 Micromechanics Models for Lamina Strength ............................. 167 4.3.1 Longitudinal Strength......................................................... 168 4.3.2 Transverse Strength ............................................................. 176 4.3.3 In-Plane Shear Strength ...................................................... 180 4.3.4 Multiaxial Strength.............................................................. 181 References ..................................................................................................... 186 5. Analysis of Lamina Hygrothermal Behavior ....................................... 191 5.1 Introduction ....................................................................................... 191 5.2 Hygrothermal Degradation of Properties ..................................... 193 5.3 Lamina Stress–Strain Relationships including Hygrothermal Effects ....................................................................... 208 5.4 Micromechanics Models for Hygrothermal Properties .............. 217 References ..................................................................................................... 228 6. Analysis of a Discontinuously Reinforced Lamina ............................ 231 6.1 Introduction ....................................................................................... 231 6.2 Aligned Discontinuous Fibers ........................................................ 232 6.2.1 Stress and Strength Analysis ............................................. 233 6.2.2 Modulus Analysis ................................................................ 239 6.3 Off-Axis-Aligned Discontinuous Fibers ........................................ 249 6.3.1 Stress and Strength Analysis ............................................. 249 6.3.2 Modulus Analysis ................................................................ 251 6.4 Randomly Oriented Discontinuous Fibers ................................... 260 6.4.1 Stress and Strength Analysis ............................................. 261 6.4.2 Modulus Analysis ................................................................ 262 6.5 Nanoibers and Nanotubes.............................................................. 271 6.5.1 Stress and Strength Analysis ............................................. 274 6.5.2 Modulus Analysis ................................................................ 275 6.6 Particulates ......................................................................................... 279 6.6.1 Stress and Strength Analysis ............................................. 280 6.6.2 Modulus Analysis ................................................................ 282 6.7 Hybrid Multiscale Reinforcements.................................................284 References ..................................................................................................... 294 Contents ix 7. Analysis of Laminates ............................................................................... 299 7.1 Introduction ....................................................................................... 299 7.2 Theory of Laminated Beams ...........................................................300 7.2.1 Flexural Stresses and Delections ......................................300 7.2.2 Shear Stresses and Delections ..........................................305 7.3 Theory of Laminated Plates with Coupling.................................. 317 7.4 Stiffness Characteristics of Selected Laminate Conigurations..............................................................................324 7.4.1 Specially Orthotropic Laminates....................................... 325 7.4.2 Generally Orthotropic Laminates ..................................... 325 7.4.3 Symmetric Laminates ......................................................... 326 7.4.4 Antisymmetric Laminates.................................................. 327 7.4.5 Quasi-Isotropic Laminates ................................................. 327 7.5 Derivation and Use of Laminate Compliances ............................. 335 7.5.1 Inversion of Laminate Force–Deformation Equations ...... 335 7.5.2 Determination of Lamina Stresses and Strains............... 337 7.5.3 Determination of Laminate Engineering Constants ...... 338 7.5.4 Comparison of Measured and Predicted Compliances .....................................................................341 7.6 Hygrothermal Effects in Laminates ............................................... 350 7.6.1 Hygrothermal Degradation of Laminates........................ 350 7.6.2 Hygrothermal Stresses in Laminates................................ 350 7.6.3 Laminate Hygrothermal Expansion Coeficients ........... 353 7.7 Interlaminar Stresses ........................................................................354 7.8 Laminate Strength Analysis ............................................................ 360 7.8.1 First Ply Failure and Subsequent Ply Failures Due to In-Plane Stresses .............................................................. 360 7.8.2 Delamination Due to Interlaminar Stresses .................... 363 7.9 Delection and Buckling of Laminates .......................................... 383 7.9.1 Analysis of Small Transverse Delections ........................384 7.9.2 Buckling Analysis ................................................................ 390 7.10 Selection of Laminate Designs ........................................................ 394 7.11 Application of Laminate Analysis to Composite Structures ...... 401 7.11.1 Composite Sandwich Structures ....................................... 401 7.11.2 Composite Grid Structures .................................................404 References ..................................................................................................... 417 8. Analysis of Viscoelastic and Dynamic Behavior ................................. 421 8.1 Introduction ....................................................................................... 421 8.2 Linear Viscoelastic Behavior of Composites .................................425 8.2.1 Boltzmann Superposition Integrals for Creep and Relaxation ...................................................................... 428 8.2.2 Differential Equations and Spring–Dashpot Models ........ 432 8.2.3 Quasielastic Analysis ..........................................................442 Contents x 8.2.4 Sinusoidal Oscillations and Complex Modulus Notation.................................................................................445 8.2.5 Elastic–Viscoelastic Correspondence Principle ............... 449 8.2.6 Temperature and Aging Effects ......................................... 455 8.3 Dynamic Behavior of Composites .................................................. 474 8.3.1 Longitudinal Wave Propagation and Vibrations in Specially Orthotropic Composite Bars ......................... 475 8.3.2 Flexural Vibration of Composite Beams ........................... 481 8.3.3 Transverse Vibration of Laminated Plates .......................485 8.3.4 Analysis of Damping in Composites ................................ 492 8.4 Nanoenhancement of Viscoelastic and Dynamic Properties......... 502 References ..................................................................................................... 514 9. Analysis of Fracture ................................................................................... 519 9.1 Introduction ....................................................................................... 519 9.2 Fracture Mechanics Analyses of Through-Thickness Cracks .........519 9.2.1 Stress Intensity Factor Approach....................................... 522 9.2.2 Strain Energy Release Rate Approach .............................. 526 9.2.3 Virtual Crack Closure Technique ...................................... 530 9.3 Stress Fracture Criteria for Through-Thickness Notches............ 536 9.4 Interlaminar Fracture .......................................................................543 9.5 Nanoenhancement of Fracture Toughness ................................... 555 References ..................................................................................................... 562 10. Mechanical Testing of Composites and Their Constituents ............. 569 10.1 Introduction ....................................................................................... 569 10.2 Measurement of Constituent Material Properties........................ 570 10.2.1 Fiber Tests ............................................................................. 570 10.2.2 Neat Resin Matrix Tests ...................................................... 573 10.2.3 Constituent Volume Fraction Measurement .................... 576 10.3 Measurement of Basic Composite Properties ............................... 578 10.3.1 Tensile Tests .......................................................................... 578 10.3.2 Compressive Tests................................................................ 582 10.3.3 Shear Tests............................................................................. 585 10.3.4 Flexure Tests ......................................................................... 594 10.3.5 Interlaminar Fracture Tests ................................................ 595 10.3.6 Fiber/Matrix Interface Tests ............................................... 599 10.3.7 Open-Hole and Filled-Hole Tests ...................................... 601 10.3.8 Bearing Tests......................................................................... 602 10.3.9 Pull-Through Tests...............................................................604 10.4 Measurement of Viscoelastic and Dynamic Properties .............. 613 10.4.1 Creep Tests ............................................................................ 613 10.4.2 Vibration Tests ...................................................................... 617 Contents xi 10.5 Measurement of Hygrothermal Properties ................................... 624 10.5.1 Glass Transition Temperature Tests .................................. 625 10.5.2 Thermal Expansion Tests.................................................... 625 10.5.3 Moisture Absorption Tests ................................................. 626 References .....................................................................................................630 11. Answers to Selected Problems ................................................................. 639 Appendix A: Matrix Concepts and Operations ........................................... 641 Appendix B: Stress Equilibrium Equations ................................................. 651 Appendix C: Strain–Displacement Equations ............................................. 655 Preface to the First Edition Composite materials is truly an interdisciplinary subject, and the number of students taking courses in this area is steadily increasing. Books on the subject tend to emphasize either the mechanics or the materials science aspects of composites. Principles of Composite Material Mechanics is mechanics oriented. Composite materials technology is new enough for many working engineers who have had no training in this area, and so, a textbook in composite material mechanics should be useful not only for the education of new engineers, but also for the continuing education of practicing engineers and for reference. The high level of interest in composite materials, the interdisciplinary nature of the subject, the need to reeducate practicing engineers, and the need for a new composite mechanics textbook at the introductory level all led to my decision to write this book. Chapters 1 through 7 form the basis of a one-semester senior/graduatelevel course in mechanical engineering, which I have taught for the last 15 years. Chapters 8 through 10, along with selected papers from technical journals and student research projects/presentations, form the basis of a second one-semester course, which is taken only by graduate students, and which I have taught for the last 4 years. The book could also be the basis for a twoquarter sequence by omitting some topics. The prerequisites for the course are knowledge of mechanics of materials, introduction to materials engineering, and ordinary differential equations, and the previous exposure to linear algebra is highly desirable. For some of the graduate-level material, earlier courses in advanced mechanics of materials, elasticity, and partial differential equations are recommended, but not required. Some of the basic elements of composite mechanics covered in this book have not changed since the irst books on the subject were published in the 1960s and 1970s, and, where possible, I have tried to use the accepted terminology and nomenclature. For example, the coverage of stress–strain relationships and transformation of properties for anisotropic materials in Chapter 2 and the classical lamination theory in Chapter 7 is consistent with that of the previous textbooks such as the Primer on Composite Materials by Ashton, Halpin, and Petit, and Mechanics of Composite Materials by Jones. However, rather than beginning the study of laminates by jumping directly into classical lamination theory, I have concluded that a better pedagogical approach is to irst introduce the basic laminate concepts by using the simpler theory of laminated beams in pure lexure. Also, I believe that the concept of an effective modulus of an equivalent homogeneous material, which had previously been covered only in advanced books such as Mechanics of Composite Materials by Christensen, is essential for the proper development of heterogeneous composite micromechanics. Thus, effective modulus–concepts are xiii xiv Preface to the First Edition emphasized from their introduction in Chapter 2 to their use in the analysis of viscoelastic and dynamic behavior in Chapter 8. Although many basic concepts have been presented in the earlier textbooks, numerous new developments in composite mechanics over the last two decades have made it increasingly necessary to supplement these books with my own notes. Thus, I have an added coverage of important topics such as hygrothermal effects in Chapter 5, discontinuous iber composites in Chapter 6, viscoelastic behavior and dynamic behavior in Chapter 8, fracture in Chapter 9, and mechanical testing in Chapter 10. The coverage of experimental mechanics of composites has been expanded to include summaries of the most important ASTM standard test methods, many of which did not exist when the early mechanics of composites books were published. A variety of example problems and homework problems, a number of them related to practical composite structures, are also included. The contents of this book represent the cumulative effects of more than 25 years of interactions with colleagues and students, and I would be remiss if I did not mention at least some of them. My fascination with composites began in 1965 with my irst engineering position in what is now a part of Oak Ridge National Laboratory in Tennessee, where I was involved in the design and development of a high-speed rotating equipment. At that time, I realized that the advantages of using composites in a rotating equipment are numerous, as is the case in many other applications. My experiences working with Dean Waters and other colleagues in the mechanical development group in Oak Ridge have had a strong inluence on my later career decision to emphasize composites research and education. My doctoral research on vibration-damping characteristics of composites with Robert Plunkett at the University of Minnesota further cemented my desire to continue working in the composites area and ultimately led to my career in university teaching and research. After beginning my academic career at Iowa State University in 1975, I began a long and productive association with C.T. Sun, and later had the pleasure of spending a 1-year leave working with C.T. and his colleagues Robert Sierakowski and Shive Chaturvedi at the University of Florida. I owe much of my understanding of composite mechanics to interactions with them. The notes leading to this book were developed by teaching composite mechanics courses at Iowa State University, the University of Idaho, the University of Florida, Michigan State University, and Wayne State University (WSU), and I am indebted to the students who took my classes and helped me to “debug” these notes over the years. Most recently, my students at WSU have been particularly effective at inding the inevitable errors in my notes. Interaction with my graduate students over the years has immeasurably contributed to my understanding of composite mechanics, and the work of several of those students has been referred to in this book. I am particularly indebted to Stalin Suarez, Lyle Deobald, Raju Mantena, and Jimmy Hwang, all former graduate students at the University of Idaho. Preface to the First Edition xv Serious work on this book actually began during a sabbatical leave at Michigan State University in 1987, and I am indebted to Larry Drzal and his colleagues for our many stimulating discussions during that year. Particularly important was the interaction with Cornelius Horgan, with whom I team taught a course on advanced mechanics of composites. Most recently, my collaboration with John Sullivan and his colleagues of the Ford Scientiic Research Laboratory has proved to be very rewarding, and I am indebted to John for his careful review of the book and helpful comments. I am grateful to Carl Johnson, also of the Ford Scientiic Research Laboratory, for his encouragement and support and for providing several of the igures in Chapter 1. The strong support of WSU, which made it possible to establish the Advanced Composites Research Laboratory there in 1989, is gratefully acknowledged. The support and encouragement of my department chairman, Ken Kline, has been particularly important. Generous support for my composites research from numerous funding agencies over the years has also helped to make this book possible. Grants from the Air Force Ofice of Scientiic Research, the National Science Foundation, the Army Research Ofice, the Boeing Company, and the Ford Motor Company have been particularly important. McGraw-Hill and I would like to thank the following reviewers for their many helpful comments and suggestions: Charles W. Bert, University of Oklahoma; Olivier A. Bauchau, Rensselaer Polytechnic Institute; Shive Chaturvedi, Ohio State University; Vincent Choo, New Mexico State University; John M. Kennedy, Clemson University; Vikram K. Kinra, Texas A & M University; C.T. Sun, University of Florida; and Steven W. Yurgartis, Clarkson University. Finally, my wife and best friend, Maryanne, has been my strongest supporter as I labored on this project, and there is no way that I could have done it without her love, encouragement, patience, and understanding. Ronald F. Gibson Preface to the Second Edition There have been many developments in mechanics of composite materials since the irst edition of this book was published. Accordingly, the second edition has new sections on recent applications of composite mechanics to nanocomposites, composite grid structures, and composite sandwich structures. To strengthen the emphasis on the basic principles of mechanics, I have added a review of the basic mechanics of materials equations in the introduction, and appendices covering the derivations of stress equilibrium equations and strain–displacement relations from elasticity theory. Coverage of micromechanics in Chapter 3 has been revised to include more detailed discussions of elasticity and inite-element models. Chapter 4 on strength analysis has been updated to include results from the World Wide Failure Exercise. Chapter 8 has been improved by adding a phenomenological approach to understanding the linear viscoelastic behavior of composites. Chapter 9 on fracture has been updated to include coverage of the initeelement implementation of the virtual crack closure technique. Chapter 10 on testing of composites and their constituents has been extensively updated to include coverage of both new and revised ASTM standard test methods. Finally, more example problems and homework problems have been added to most chapters, and new references have been cited throughout. As with the irst edition, I am indebted to many colleagues, graduate students, and sponsors. I am grateful to WSU for providing a nurturing environment for my teaching and research, and for granting me sabbatical leave, which were essential to the completion of this project. My graduate students have been particularly helpful in identifying the inevitable errors in the irst edition, and their thesis research indings have enabled me to add important new dimensions in the second edition. And as with the irst edition, my wife and best friend, Maryanne, has continued to be my strongest supporter, and I will be forever grateful for her love, encouragement, patience, and understanding. Ronald F. Gibson xvii Preface to the Third Edition The goals for the third edition are to continue to present a unique blended coverage of classical and state-of-the-art mechanics of composites technologies, while striving to incorporate the most worked-out example problems and homework problems of any available textbook on mechanics of composite materials. A high priority has been placed on writing a textbook that is easily understood by students. Pedagogical improvements include a total of 81 worked-out example problems (25 of which are new for the third edition); 177 homework problems (25 of which are new); 388 igures (46 of which are new); a new appendix on matrix concepts and operations; new coverage of particle composites, nanocomposites, nanoenhancement of conventional iber composites, hybrid multiscale composites; and additional coverage of inite-element modeling and test methods. Although the book is written irst as a textbook covering classical methods, frequent references to the current state-of-the-art composites technology and research indings are included. Extensive references are provided, including many current journal articles along with classic and historical publications. I continue to be indebted to my colleagues, graduate students, and sponsors for their encouragement and support over the years. Most recently, my professional afiliations with WSU and the University of Nevada, Reno (UNR) have provided the necessary positive environments for teaching and research that made the development of this new edition possible. I have been particularly motivated by the interactions with students in my composites classes at WSU and UNR. As with the earlier editions of this book, my wife and best friend, Maryanne, continues to be my most enthusiastic supporter, and there is no way that I could have completed this project without her. Ronald F. Gibson xix Preface to This Edition My interactions with students and colleagues and my continued compositesrelated activities since the third edition was published in 2012 have motivated me to think of a number of improvements that could be made in the fourth edition. In the previous editions, I have tried to maintain a practical balance between the traditional classical and current state-of-the-art coverage, and previous improvements have emphasized the current state-of-theart technologies. In contrast, the fourth edition puts an increased emphasis on pedagogy. I have kept careful notes on errors that were found in the third edition, and those are corrected in the fourth edition. New workedout example problems and homework problems are added in most chapters. The number of worked-out examples has been increased by about 20% to 95, while the number of homework problems has been increased by about 12% to 212. Rather than continuing to place all homework problems at the end of the chapters, these problems are integrated within the chapters following the most relevant sections, similar to the way worked-out example problems are currently presented. With this change, it will no longer be necessary for instructors and students to determine to which section a particular homework problem is most relevant. This is the pedagogical approach used in many basic mechanics textbooks. One of the most frequent requests from students has been to provide answers to selected homework problems. In my classes, I have been providing such answers on the course website, but in the fourth edition, I am including them in the back of the book instead. Finally, I greatly appreciate the constructive feedback regarding the book from my students and colleagues, along with instructors at other universities who have adopted the book. My wife and best friend, Maryanne, continues to be my most enthusiastic supporter, and this project would not have been possible without her. Ronald F. Gibson xxi Author Ronald F. Gibson, PhD, is currently an adjunct professor of mechanical engineering at the University of Nevada, Reno. He earned his PhD in mechanics from the University of Minnesota, an MS in mechanical engineering from the University of Tennessee, and a BS in mechanical engineering from the University of Florida. His industrial/government experience includes a position as a development engineer for Union Carbide Corporation, Nuclear Division and a summer faculty fellowship at the NASA Langley Research Center. He has held full-time faculty positions at Iowa State University, The University of Idaho, and Wayne State University, as well as visiting faculty positions at Stanford University, the University of Florida, and Michigan State University. He is an elected Fellow of the American Society of Mechanical Engineers, the American Society for Composites, and the Society for Advancement of Material and Process Engineering. He is a member of the American Society for Engineering Education, the American Institute for Aeronautics and Astronautics, and the Society for Experimental Mechanics. He served as the president of the American Society for Composites in 2004–2005, and as the vice president during 2002–2003. Dr. Gibson’s awards include the Hetenyi Award for Best Research Paper of the Year from the Society for Experimental Mechanics, the College of Engineering Outstanding Faculty Award from the University of Idaho, the Distinguished Faculty Fellowship Award, the DeVlieg Professorship, and the Outstanding Graduate Faculty Mentor Award from WSU. The results of his research have been published in numerous scholarly journal articles and presented at a variety of national and international meetings. His current research interests include mechanical characterization of composite materials and structures, noise and vibration control with composites, design and manufacturing of composite structures, characterization of energy-absorbing materials, multifunctional composites, and nanocomposites. xxiii 1 Introduction 1.1 Basic Concepts Structural materials can be divided into four basic categories: metals, polymers, ceramics, and composites. Composites, which consist of two or more separate materials combined in a structural unit, are typically made from various combinations of the other three materials. In the early days of modern man-made composite materials, the constituents were typically macroscopic. As composites technology advanced over the last few decades, the constituent materials, particularly the reinforcement materials, steadily decreased in size. Most recently, there has been considerable interest in “nanocomposites” having nanometer-sized reinforcements such as carbon nanoparticles, nanoibers, and nanotubes, because of the extraordinary properties of these materials. The relative importance of the four basic materials in a historical context has been presented by Ashby [1], as shown schematically in Figure 1.1 that clearly shows the steadily increasing importance of polymers, composites, and ceramics, and the decreasing role of metals. Composites are generally used because they have desirable properties that cannot be achieved by any of the constituent materials acting alone. The most common example is the ibrous composite consisting of reinforcing ibers embedded in a binder or matrix material. Particle or lake reinforcements are also used, but they are generally not as effective as ibers. Although it is dificult to say with certainty when or where humans irst learned about ibrous composites, nature provides us with numerous examples. Wood consists mainly of ibrous cellulose in a matrix of lignin, whereas most mammalian bone is made up of layered and oriented collagen ibrils in a protein–calcium phosphate matrix [2]. The book of Exodus in the Old Testament recorded what surely must be one of the irst examples of man-made ibrous composites, the straw-reinforced clay bricks used by the Israelites. The early natives of South America and Central America apparently used plant ibers in their pottery. These early uses of ibrous reinforcement, however, were probably based on the desire to keep the clay from cracking during drying rather than on structural reinforcement. Much later, 1 Principles of Composite Material Mechanics 2 10,000 5000 0 1000 1500 1800 Gold Copper Bronze Iron 1900 1940 1990 2000 2010 2020 Glassy metals Aluminum–lithium alloys Cast iron Dual phase steels Steels Wood Skins Fibers 1980 Metals Metals Polymers Relative importance 1960 Alloy steels Glues Microalloyed steels Development stow: Mostly quality control and processing New super alloys Light alloys Polymers Conducting Super alloys Composites polymers Straw brick paper High-temperature Titanium polymers zirconium, Alloys etc. Stone High-modulus Composites Flint polymers Bakeline Ceramic composites Pottery Polyesters Metal-matrix Glass Nylon Epoxies composites Cement PE PMMAAcrylics Kevlar FRP Ceramics Refractories Ceramics CFRP PC PS PP CFRP Portland Fused Tough engineering cement silica Cemets Pyro, ceramics (Al2O3Si3N4 PCZ, etc.) ceramics 10,000 Rubber 5000 0 1000 1500 1800 1900 1940 1960 1980 1990 2000 2010 2020 Year FIGURE 1.1 Relative importance of metals, polymers, composites, and ceramics as a function of time. The diagram is schematic and describes neither tonnage nor value. The timescale is nonlinear. (From Ashby, M. F. 1987. Technology of the 1990s: Advanced materials and predictive design. Philosophical Transactions of the Royal Society of London, A322, 393–407. Reproduced by permission of The Royal Society.) humans developed structural composites such as steel-reinforced concrete, polymers reinforced with ibers such as glass and carbon, and many other materials. Fibrous reinforcement is very effective because many materials are much stronger and stiffer in iber form than they are in bulk form. It is believed that this phenomenon was irst demonstrated scientiically in 1920 by Grifith [3], who measured the tensile strengths of glass rods and glass ibers of different diameters. Grifith found that as the rods and ibers got thinner, they got stronger (see Figure 1.2 from Reference 3, as shown in Reference 4), apparently because the smaller the diameter, the smaller the likelihood that failure-inducing surface cracks would be generated during fabrication and handling. By extrapolating these results, Grifith found that for very small diameters, the iber strength approached the theoretical cohesive strength between adjacent layers of atoms, whereas for large diameters, the iber strength dropped to nearly the strength of bulk glass. Results similar to those published by Grifith have been reported for a wide variety of other materials. The reasons for the differences between iber and bulk behavior, however, are not necessarily the same for the other materials. For example, polymeric ibers are stronger and stiffer than bulk polymers Introduction 3 600,000 Extrapolates to 1,600,000 psi (11,000 MN/m 2) Tensile strength (lb/in.2) 500,000 400,000 Extrapolates to approximate strength of bulk glass 25,000 psi (170 MN/m2) 300,000 200,000 100,000 1 1000 10 μ 20 μ 2 3 4 1000 1000 1000 Thickness of fiber (in.) FIGURE 1.2 Grifith’s measurements of tensile strength as a function of iber thickness for glass ibers. (From Grifith, A. A. 1920. The phenomena of rupture and low in solids. Philosophical Transactions of the Royal Society, 221A, 163–198. Reproduced by permission of The Royal Society; Gordon, J. E. 1976. The New Science of Strong Materials, 2nd ed. Princeton University Press, Princeton, NJ. With permission.) because of the highly aligned and extended polymer chains in the ibers and the randomly oriented polymer chains in the bulk polymer. A similar effect occurs in crystalline materials such as graphite. In addition, a single crystal tends to have a lower dislocation density than a polycrystalline solid; so single-crystal “whisker” materials are much stronger than the same material in polycrystalline bulk form. Whiskers typically have dimensions in the micrometer range, and for many years, it was thought that whiskers were the strongest and stiffest reinforcement materials available. However, it is now believed that carbon nanotubes (CNTs), which have dimensions in the nanometer range, are the strongest and stiffest reinforcement materials in existence [5,6]. There can be no doubt that ibers allow us to obtain the maximum tensile strength and stiffness of a material, but there are obvious disadvantages of using a material in iber form. Fibers alone cannot support longitudinal compressive loads and their transverse mechanical properties are often not as good as the corresponding longitudinal properties. Thus, ibers are generally useless as structural materials unless they are held together in a structural unit with a binder or matrix material and unless some transverse reinforcement is provided. Fortunately, the geometrical coniguration of ibers also turns out to be very eficient from the point of view of interaction with the binder or matrix. As shown in Figure 1.3 from Reference 7, the ratio of surface area to volume for a cylindrical particle is greatest when the particle is in either Principles of Composite Material Mechanics l/3 4 Platelet Area/volume ratio A/V in units of 2π V Fiber 20 15 10 5 0 0.01 0.1 1 10 a (log scale) 100 1000 FIGURE 1.3 Surface area-to-volume ratio A/V of a cylindrical particle of given volume plotted versus particle aspect ratio a = l/d. (From McCrum, N. G., Buckley, C. P., and Bucknall, C. B. Principles of Polymer Engineering, 1988, New York, NY, by permission of Oxford University Press.) platelet or iber form. For a platelet, the particle aspect ratio, that is, a = l/d (i.e., the length-to-diameter ratio) is very small, whereas for a iber, the aspect ratio is very large. Thus, the iber/matrix interfacial area available for stress transfer per unit volume of iber increases with increasing iber length-to-diameter ratio. It is also important to note that, for a iber-reinforced composite, the total iber/matrix interfacial area will be increased if the iber diameter is decreased while maintaining constant iber volume and iber length. The matrix also serves to protect the ibers from external damage and environmental attack. Transverse reinforcement is generally provided by orienting ibers at various angles according to the stress ield in the component of interest. Filler particles are also commonly used in composites for a variety of reasons such as weight reduction, cost reduction, lame and smoke suppression, and prevention of ultraviolet degradation due to exposure to sunlight. The need for iber placement in different directions according to the particular application has led to various types of composites, as shown in Figure 1.4. In the continuous iber composite laminate (Figure 1.4a), individual continuous iber/matrix laminae are oriented in the required directions and bonded together to form a laminate. Although the continuous iber laminate is used extensively, the potential for delamination, or separation of the laminae, is still a major problem because the interlaminar strength is matrix dominated. Woven iber composites (Figure 1.4b) do not have distinct laminae and are not susceptible to delamination, but strength and stiffness are sacriiced because the ibers are not as straight as in the continuous iber laminate. Chopped iber composites may have short ibers randomly dispersed in the matrix, Introduction 5 (a) (b) (c) (d) FIGURE 1.4 Types of iber-reinforced composites. (a) Continuous iber composite, (b) woven composite, (c) chopped iber composite, and (d) hybrid composite. as shown in Figure 1.4c. Chopped iber composites are used extensively in high-volume applications due to their low manufacturing cost, but their mechanical properties are considerably poorer than those of continuous iber composites. Finally, hybrid composites may consist of mixed chopped and continuous ibers, as shown in Figure 1.4d or mixed iber types such as glass and carbon. Another common composite coniguration, the sandwich structure (Figure 1.5), consists of high-strength composite facing sheets (which could be any of the composites shown in Figure 1.4) bonded to a lightweight foam or honeycomb core. Sandwich structures have extremely high lexural stiffness-to-weight ratios and are widely used in aerospace structures. The design lexibility offered by these and other composite conigurations is obviously quite attractive to designers, and the potential exists to design not only the structure but also the structural material itself. 1.2 Constituent Materials for Composites Fiberglass-reinforced plastics were one of the irst structural composites. Composites incorporating glass or other relatively low-modulus ibers (<83 GPa [12 × 106 psi]) are used in many high-volume applications such as Principles of Composite Material Mechanics 6 Film adhesive bonds facings to core High strength composite laminate facings Low density honeycomb core FIGURE 1.5 Composite sandwich structure. automotive vehicles because of their low cost, and are sometimes referred to as “basic” composites. The so-called “advanced” composites made from carbon, silicon carbide, aramid polymer, boron, or other higher-modulus ibers are used mainly in more demanding applications such as aerospace structures, where their higher cost can be justiied by improved performance. The tremendous advantages of advanced ibers over glass ibers and conventional bulk materials are shown in Table 1.1, by comparing selected properties. The main advantages are higher modulus, higher strength, and lower density. In many applications such as aerospace and automotive structures, structural weight is very important. Depending on whether the structural design is strength-critical or stiffness-critical, the material used should have a high strength-to-weight ratio (or speciic strength) or a high stiffness-toweight ratio (or speciic stiffness). As shown in Figure 1.6, advanced ibers also have signiicant advantages over conventional materials in both these attributes, and this is the principal reason that composites will be used with increasing frequency in aerospace structures, iber-reinforced automotive structures, and other structures where these properties are important. When the reinforcing ibers are combined with a matrix or binder material to form a composite, there is obviously some reduction in the tremendously high speciic strengths and speciic moduli shown for the reinforcing ibers in Figure 1.6, but the composites still have an overwhelming advantage with respect to these properties. Table 1.1 also shows that the ultimate strain or strain to failure (a measure of ductility), is one attribute where reinforcing ibers are typically not as good as conventional bulk metals and polymers, but are still better than bulk ceramics. Many advanced ibers exhibit nearly linear stress–strain curves to failure, and such behavior is generally considered to 4.1 4.7 4.1 3.3 3.2 9.3 3.5 4.1 86 2.8 2.4 3.1 69 200 45 114 Tensile Modulus (GPa) 99 121 83 56 86 158 97 75 65 40 Bulk Polymers Nylon 6/6 Polycarbonate Polyvinylchloride Bulk Polymer Matrix Materials Hexply 8551-7 epoxy Hexply 8552 epoxy CYCOM 934 epoxy Hexply 954-3A cyanate Derakane 411-350 vinylester Ultem 2300 polyetherimide Victrex 150G polyetheretherketone Fortron 0214B1 polyphenylene sulide 310 1030 345 880 Bulk Metals 6061T6 Aluminum 4340 Steel AZ80 Magnesium 6AL4V Titanium Material Tensile Strength (MPa) Selected Properties of Bulk and Fibrous Materials TABLE 1.1 1.4 1.27 1.3 1.3 1.19 1.14 1.51 1.3 1.14 1.2 1.44 2.71 7.83 1.8 4.43 Density (g/cm3) 61.4 78 93.1 63.8 47 75.4 104.6 74.6 65.8 54.2 27.8 114.4 131.5 191.7 198.6 Speciic Strength (MPa/[g/cm3]) 2.9 3.2 3.6 3.1 2.8 2.8 6.2 2.7 2.5 2 2.2 25.5 25.5 25 25.7 Speciic Modulus (GPa/[g/cm3]) 0.03 0.044 0.017 0.007 0.019 0.05 0.03 0.6 0.5 1.1 0.4 0.17 0.19 0.06 0.14 Ultimate Strain (Continued) Ticona Hexcel Hexcel Cytec Hexcel Ashland Sabic Victrex Manufacturer Introduction 7 2600a 3900a 1100a 2100a 3448 4890 4475 5670 6140 6964 3650 4550 4410 2740 4900 5880 6370 Bulk Ceramics Alumina (Al2O3) Silicon carbide (SiC) Silica (SiO2) Aluminum nitride (AlN) Glass Fibers E-glass S-2 glass PAN-Based Carbon Fibers AS4, 12K ilaments IM7, 12K IM9, 12K IM10, 12K T-300, 12K T-650/35, 12K T-400H, 6K M-40, 12K T700S, 12K T-800S, 24K T-1000G, 12K Material Tensile Strength (MPa) 231 276 304 303 231 248 250 392 230 294 294 72 87 375a 410a 73a 330a Tensile Modulus (GPa) Selected Properties of Bulk and Fibrous Materials TABLE 1.1 (Continued) 1.79 1.78 1.8 1.79 1.76 1.7 1.8 1.81 1.8 1.8 1.8 2.54 2.46 3.89 3.1 2.2 3.26 Density (g/cm3) 2500 3185.4 3411.1 3890.5 2073.9 2676.4 2450.0 1513.8 2722.2 3266.7 3538.9 1357.5 1987.8 668.3 1258 500 644.2 Speciic Strength (MPa/[g/cm3]) 129 155 168.9 169.3 131.3 145.9 138.9 216.6 127.8 163.3 163.3 28.3 35.8 96.4 132.2 33.2 101.2 Speciic Modulus (GPa/[g/cm3]) 0.018 0.0178 0.019 0.021 0.014 0.0175 0.018 0.007 0.021 0.02 0.022 0.048 0.057 Ultimate Strain Hexcel Hexcel Hexcel Hexcel Cytec Cytec Toray Toray Toray Toray Toray (Continued) Owens-Corning Owens-Corning Accuratus Accuratus Accuratus Accuratus Manufacturer 8 Principles of Composite Material Mechanics 13,000–52,000 2700–7000 Carbon nanotubes Carbon nanoibers Denotes compressive property. 3900 SCS-6 silicon carbide a 3600 320–1470 400–600 380 400 73 180 110 3430 5800 3500 Other Fibers Boron 4.0 mil dia 124 3340 380 760 830 70 112 79 Pitch-Based Carbon Fibers P-55S, 2K P-100S, 2K P-120S, 2K Tensile Modulus (GPa) 3620 3620 2600 1900 2100 2240 Material Polymeric Fibers Kevlar 29 aramid Kevlar 49 aramid Spectra 900/650 polyethylene Spectra 2000/100 polyethylene Technora aramid Zylon-AS PBO Dyneema SK60 polyethylene Tensile Strength (MPa) Selected Properties of Bulk and Fibrous Materials TABLE 1.1 (Continued) 1.3–1.4 1.8–2.1 3 2.54 1.39 1.54 0.97 0.97 1.44 1.44 0.97 2.0 2.13 2.13 Density (g/cm3) 1300 1417.3 2467.6 3766.2 3608.2 3443.3 2514 2514 2680 950 985.9 1051.6 Speciic Strength (MPa/[g/cm3]) 126.7 157.5 52.5 116.9 113.4 127.8 48.6 77.8 81.4 190 356.8 389.7 Speciic Modulus (GPa/[g/cm3]) 0.0013 0.008 0.046 0.035 0.03 0.036 0.024 0.036 0.005 0.002 0.0042 Ultimate Strain Applied sciences Specialty materials Specialty materials Teijin Toyobo Toyobo Honeywell DuPont DuPont Honeywell Cytec Cytec Cytec Manufacturer Introduction 9 Principles of Composite Material Mechanics 10 450 Specific modulus, GPa/(g/cm3) 400 P-120S fiber 350 P-100S fiber 300 250 200 P-55S fiber IM-7 fiber IM-9 fiber T-650/35 fiber AS-4 fiber Zylon-AS Boron fiber 150 SCS-6 fiber Bulk silicon carbide 100 Kevlar 49 fiber Spectra 900 fiber 50 E-glass fiber Bulk aluminum Bulk nylon 0 0 1000 fiber S-2 glass fiber 2000 3000 4000 Specific strength, MPa/(g/cm3) FIGURE 1.6 Speciic modulus versus speciic strength for a variety of ibers and conventional bulk materials. The speciic value is the value of the property divided by the density. be characteristic of brittle materials. It is important to remember, however, that the iber strength, iber modulus, and iber ultimate strain values in Table 1.1 are based on tensile tests with the load acting along the iber axis. As shown later, these properties all change substantially for off-axis loading, and applied loads are rarely aligned perfectly with the iber axis. It will be shown later, for example, that a composite laminate can be constructed in such a way that its overall behavior is similar to that of ductile metals, even though the reinforcing ibers may exhibit brittle behavior. 1.2.1 Reinforcement Materials including Nanoreinforcements Glass ibers consist primarily of silica (silicon dioxide) and metallic oxide modifying elements and are generally produced by mechanical drawing of molten glass through a small oriice. E-glass (named for its electrical properties) accounts for most of the glass iber production and is the most widely used reinforcement for composites. The second most popular glass iber, S-glass, has roughly 40% greater tensile strength and 20% greater modulus of elasticity than E-glass (Table 1.1), but it is not as widely used, because of its higher cost. S-glass actually has greater strength and elongation than many advanced ibers, but its relatively low modulus limits its application. Glass/ epoxy and glass/polyester composites are used extensively in applications ranging from ishing rods to storage tanks and aircraft parts. Introduction 11 Graphite or carbon ibers are the most widely used advanced ibers, and graphite/epoxy or carbon/epoxy composites are now used routinely in aerospace structures. Unfortunately, the names “carbon” and “graphite” are often used interchangeably to describe ibers based on the element carbon. These ibers are usually produced by subjecting organic precursor ibers such as polyacrylonitrile (PAN) or rayon to a sequence of heat treatments, so that the precursor is converted to carbon by pyrolysis. The major difference is that graphite ibers are subjected to higher-temperature pyrolysis than carbon ibers. The result is that carbon ibers typically are less than 95% carbon, whereas graphite ibers are at least 99% carbon [8]. Although carbon ibers were once prohibitively expensive, the cost has dropped signiicantly as production capacity and demand has increased. Development of new carbon and graphite ibers continues at a rapid pace. For example, ibers based on a pitch precursor (P-120S) with a modulus more than four times that of steel are now available (Table 1.1). High-strength carbon ibers such as IM10 and T-1000G, which are based on a PAN precursor, have a tensile strength more than six times that of steel. Either high strength or high modulus is obtained by using the appropriate heat treatment. Advanced polymeric ibers such as Kevlar® aramid ibers by DuPont, Spectra® polyethylene ibers by Honeywell, Technora® aramid ibers by Teijin, and Zylon® para-phenylene benzobisoxazole (PBO) ibers by Toyobo have extremely high speciic strengths because of their combinations of high strength and low density. The polymeric ibers also have higher failure strains (i.e., better ductility) than the glass or carbon ibers. The main disadvantages of the polymeric ibers are that they are generally not suitable for use at extremely high temperatures, and some of them are also susceptible to moisture-induced degradation. The effects of temperature and moisture on polymers and polymer composites will be discussed in more detail in Chapter 5. Boron ibers are actually composites consisting of a boron coating on a substrate of tungsten or carbon, and the diameter of boron ibers is among the largest of all the advanced ibers, typically 0.002–0.008 in. (0.05–0.2 mm). Boron ibers not only have much higher moduli than most carbon ibers (Table 1.1), but they also have higher density. Boron/epoxy and boron/aluminum composites are widely used in aerospace structures where high stiffness is needed, but high cost still prevents more widespread use. Silicon carbide (SiC) ibers are used primarily in high-temperature metal and ceramic matrix composites because of their excellent oxidation resistance and high-temperature strength retention. At room temperature, the strength and stiffness of SiC ibers are about the same as those of boron. SiC whisker-reinforced metals are also receiving considerable attention as alternatives to unreinforced metals and continuous iber-reinforced metals. SiC whiskers are very small, typically 8–20 µin. (20–51 nm) in diameter and about 0.0012 in. (0.03 mm) long, so that standard metal-forming processes such as extrusion, rolling, and forging can be easily used [7]. 12 Principles of Composite Material Mechanics The ultimate reinforcement material to date is the carbon nanotube (CNT). CNTs, which were irst observed in 1991, are two-dimensional (2D) hexagonal networks of carbon atoms (graphene sheets) that have been rolled up to form a cage-like hollow tube having a diameter of several nanometers [5,6]. The properties for nanotubes presented in Table 1.1 are only approximate, as nanotubes have so many different possible conigurations. For example, they can be single walled or multiwalled, and they may occur in the form of bundles or ropes. Carbon nanoibers have greater diameters and lengths, but lower mechanical properties than CNTs. Nanoibers are typically less expensive than nanotubes. Both CNTs and nanoibers are discontinuous, having rather low aspect ratios compared to conventional ibers such as glass and carbon. Discontinuous reinforcement is discussed in Chapter 6. Particulate reinforcements, especially nanoparticles, are increasingly used to improve the mechanical and/or thermal properties of polymer matrix materials in iber-reinforced composites. The longitudinal compressive strength, transverse tensile strength, and shear strength of iber composites can be signiicantly enhanced by reinforcing the matrix with particles. Ceramic particles and nanoparticles such as silicon dioxide (SiO2) have much lower thermal expansion coeficients than polymer matrix materials, and can be used to reduce undesirable thermal expansion mismatches between iber and matrix materials in iber composites. Hybrids consisting of mixed iber materials can be used when a single iber material does not have all the desired properties. More complete descriptions of iber materials and their properties can be found in several composite handbooks [8–13]. Chapter 3 deals with further discussion on iber properties, including anisotropic behavior. 1.2.2 Matrix and Filler Materials Polymers, metals, and ceramics are all used as matrix materials in composites, depending on the particular requirements. The matrix holds the ibers together in a structural unit and protects them from external damage, transfers and distributes the applied loads to the ibers, and, in many cases, contributes some needed property such as ductility, toughness, or electrical insulation. A strong interface bond between the iber and matrix is obviously desirable, and so the matrix must be capable of developing a mechanical or chemical bond with the iber. The iber and matrix materials should also be chemically compatible, so that undesirable reactions do not take place at the interface. Such reactions tend to be more of a problem in high-temperature composites. Service temperature is often the main consideration in the selection of a matrix material. Thus, the materials will be discussed below in order of increasing temperature capability. Polymers are unquestionably the most widely used matrix materials in modern composites (Table 1.1). Polymers are described as being either Introduction 13 thermosets (e.g., epoxy, polyester, and phenolic) or thermoplastics (e.g., polyimide [PI], polysulfone [PSU], polyetheretherketone [PEEK], and polyphenylene sulide [PPS]). On curing, thermosets form a highly cross-linked, three-dimensional (3D) molecular network that does not melt at high temperatures. Thermoplastics, however, are based on polymer chains that do not cross-link. As a result, thermoplastics will soften and melt at high temperatures, then harden again on cooling. Epoxies and polyesters have been the principal polymer matrix materials for several decades, but advanced thermoplastics such as PEEK and PPS are now receiving considerable attention for their excellent toughness and low moisture absorption properties, their simple processing cycles, and their higher-temperature capabilities. Aerospace grade epoxies are typically cured at about 177°C (350°F) and are generally not used at temperatures above 150°C (300°F), whereas advanced thermoplastics such as PPS, PI, and PEEK have melting temperatures in the range 315–370°C (600–700°F). At this time, it appears that polymer matrix materials for use up to 425°C (800°F) are feasible. For higher temperatures, metal, ceramic, or carbon matrix materials are required. By using lightweight metals such as aluminum, titanium, and magnesium and their alloys and intermetallics such as titanium aluminide and nickel aluminide, operating temperatures can be extended to about 1250°C (2280°F). Other advantages of metal matrices are higher strength, stiffness, and ductility than polymers but at the expense of higher density. Ceramic matrix materials such as silicon carbide and silicon nitride can be used at temperatures up to 1650°C (3000°F). Ceramics have poor tensile strength and are notoriously brittle, however, and there is a need for much research before these materials can be routinely used. Finally, carbon iber/carbon matrix composites can be used at temperatures approaching 2760°C (5000°F), but the cost of these materials is such that they are used only in a few critical aerospace applications. For further details on matrix materials and their properties, the reader is referred to any of several handbooks [8–13]. The third constituent material of a composite, the iller material, is mixed in with the matrix material during fabrication. Fillers are not generally used to improve mechanical properties but, rather, are used to enhance some other aspect of composite behavior. For example, hollow glass microspheres are used to reduce weight, clay or mica particles are used to reduce cost, carbon black particles are used for protection against ultraviolet radiation, and alumina trihydrate is used for lame and smoke suppression [11]. Fillers truly add another dimension to the design lexibility we have in composites. EXAMPLE 1.1 Compare the total iber surface area of a group of N small-diameter ibers with that of a single large-diameter iber having the same length and volume. Principles of Composite Material Mechanics 14 Solution Assuming that the ibers are perfectly round, for a single large-diameter iber of diameter dL, the circumferential iber surface area per unit length is AL = πdL whereas the iber volume per unit length is VL = πdL2 4 For a single small-diameter iber of diameter dS, the corresponding circumferential surface area and volume per unit length are, respectively, AS = πdS and VS = πds2 4 For N small-diameter ibers having the same volume and length as a single large-diameter iber, NVS = VL so that N= VL dL = VS dS 2 The ratio of the total surface area of N small-diameter ibers to the surface area of a single large-diameter iber having the same volume and length is then 2 R= NAS NdS dL dS dL = = = dS dL dS AL dL For example, if a large iber is replaced by a group of ibers having diameters 1000 times smaller, dL = 1000 dS, and the total iber surface area for a constant iber length and volume will increase by a factor of 1000. It can be easily shown that the same result holds for spherical particles. So in addition to their superior strength and stiffness, small-diameter Introduction 15 ibers such as nanoibers have the additional advantage of signiicantly larger iber/matrix interfacial surface area per unit volume than largerdiameter ibers. EXAMPLE 1.2 A structural design for which the governing design criterion is limiting the maximum working stress is sometimes referred to as a “strengthcritical design” and a structural design in which the governing design criterion is limiting the maximum working deformation is sometimes referred to as a “stiffness-critical design.” (a) Considering only the mechanical properties of carbon iber-reinforced composites, which types of carbon ibers would be the most desirable for use in strengthcritical composite designs and (b) which types of carbon ibers would be the most desirable for use in stiffness-critical composite designs? (c) If minimization of structural weight is an additional consideration, would this change the answers to (a) and (b)? Solution a. According to Table 1.1, among the available carbon ibers, PANbased carbon ibers have the highest tensile strength values, so they would be the most desirable for use in strength-critical composite designs. b. Similarly, among the available carbon ibers, pitch-based carbon ibers have the highest tensile modulus values, so they would be the most desirable for use in stiffness-critical composite designs. c. From Table 1.1, the PAN-based carbon ibers have the highest speciic strength values and the pitch-based carbon ibers have the highest speciic modulus values, so the additional consideration of structural weight would not change the answers to (a) and (b). EXAMPLE 1.3 A thin-walled pressure vessel of mean radius r and wall thickness t is to contain gas at an internal pressure p. Compare the maximum internal pressures that can be withstood by an IM10 carbon iber composite vessel and a 6061T6 aluminum vessel. Assume that both vessels have the same radius and wall thickness, that the carbon ibers are all oriented in the circumferential direction, and neglect the contribution of the matrix in the composite. Solution From the mechanics of materials thin-walled pressure vessel theory, the circumferential hoop stress in the vessel is given by σ= pr t Principles of Composite Material Mechanics 16 so the pressure is given by p= σt r Therefore, for the same radius and thickness, the ratio of the pressures that can be withstood by the two vessels is given by the ratio of the tensile strengths for the two materials, as given in Table 1.1. pIM10 6964 σ = IM10 = = 22.46 310 p6061T 6 σ 6061T 6 So the IM10 carbon iber vessel can withstand 22.46 times the pressure that the 6061T6 vessel can withstand. EXAMPLE 1.4 A cantilever beam of rectangular cross section and made of 6061T6 aluminum is to be replaced by an IM10 carbon iber composite beam having the same length L and width b, and it must have the same tip delection w under the same tip load P. Compare the thicknesses and weights of the two beams, neglecting the contribution of the matrix material in the composite. Solution From the mechanics of materials beam theory, the tip delection of the cantilever beam is given by w= PL3 3EI where I = bh3/12 is the area moment of inertia of the cross section about the neutral axis or centroidal axis, b is the width, h is the thickness, and E is the modulus of elasticity from Table 1.1. The ratio of the tip delections for the two beams having the same length, width, and load is 3 hIM10 EIM10 =1 h 6061T6 E6061T6 So the corresponding ratio of thicknesses is hIM10 E6061T6 = h6061T6 EIM10 1/3 69 = 303 1/3 = 0.61 and the carbon iber beam only needs to be 61% as thick as the aluminum beam. The ratio of the weights of the two beams is given by Introduction 17 WIM10 bhIM10 LρIM10 h ρ 1.79 = 0.403 = = IM10 IM10 = 0.61 W6061T6 bh6061T6 Lρ6061T6 h6061T6ρ6061T 6 2.71 where W is the beam weight and ρ is the beam material density from Table 1.1. So the carbon iber composite beam only weighs 40% as much as the aluminum beam, but it satisies the same design criteria. These examples demonstrate some of the advantages of composites over conventional materials without considering the matrix material. The contributions of the matrix material will be discussed in later chapters, especially in Chapters 3 and 4. PROBLEM 1.1 For a cylindrical particle, derive the relationship between the ratio of surface area to volume, A/V, and the particle aspect ratio, l/d, and verify the shape of the curve shown in Figure 1.3. PROBLEM 1.2 Compare the total surface area of a group of N small-diameter spherical particles with that of a single large-diameter spherical particle having the same volume. PROBLEM 1.3 Explain qualitatively why sandwich structures (Figure 1.5) have such high lexural stiffness-to-weight ratios. Describe the key parameters affecting the lexural stiffness-to-weight ratio of a sandwich panel. PROBLEM 1.4 Which of the reinforcing ibers listed in Table 1.1 would be best for use in an orbiting space satellite antenna structure that is subjected to relatively low stresses but has very precise dimensional stability requirements? The answer should be based only on the properties given in Table 1.1. PROBLEM 1.5 A support cable in a structure must be 5 m long and must withstand a tensile load of 5 kN with a safety factor of 2.0 against tensile failure. Assuming a solid cylindrical cross section for the cable as an approximation, (a) determine and compare the weights of cables made of 4340 steel and AS-4 carbon ibers that meet the above requirements and (b) for an AS-4 carbon iber cable having the same weight, length, and safety factor as the 4340 steel cable from part (a), how much tensile load will the carbon iber cable be able to withstand? Principles of Composite Material Mechanics 18 ω t r L FIGURE 1.7 Simpliied model of lywheel for Problem 1.6. PROBLEM 1.6 A lywheel for energy storage is modeled as a rotating thin-walled cylindrical ring (t ≪ r) as shown in Figure 1.7. Find the equation for the tensile stress in the ring as a function of the mean radius, r, the rotational speed, ω, and the mass density, ρ, of the ring, then compare the maximum peripheral speed (tangential velocity) and the kinetic energy stored per unit mass of a ring made from 4340 steel with that of a ring made from IM-7 carbon ibers. For the carbon iber ring, assume that the ibers are oriented in the circumferential direction, and that the entire tensile load is supported by the ibers. 1.3 Structural Applications of Composites Composite structural elements are now used in a variety of components for automotive, aerospace, marine, and architectural structures in addition to consumer products such as skis, golf clubs, and tennis rackets. Since much of the current composites technology evolved from aerospace applications, it is appropriate to begin this brief overview from there. Military aircraft designers were among the irst to realize the tremendous potential of composites with high speciic strength and high speciic stiffness, since performance and maneuverability of those vehicles depend so heavily on weight. Composite construction also leads to smooth surfaces (no rivets or sharp transitions as in metallic construction), which reduce drag. Since boron and graphite ibers were irst developed in the early 1960s, applications of advanced composites in military aircraft have accelerated quickly. Carbon iber composite structural elements such as horizontal and vertical stabilizers, laps, wing skins, and various control surfaces have been used in Introduction 19 FIGURE 1.8 Lockheed Martin F-35 Lightning II Joint Strike Fighter with composite fuselage and wing structures. (Courtesy of Lockheed Martin Corporation.) ighter aircraft for many years. More recently, carbon iber composite fuselage and wing structures have been incorporated in ighter aircraft such as the F-35 Lightning II Joint Strike Fighter (Figure 1.8) and in the entire structure of the B2 stealth bomber (Figure 1.9). The steady growth in the use of composite structures in military ighter aircraft over the years has been documented in Reference 14. Composites applications in commercial aircraft have been steadily increasing as material costs come down, as design and manufacturing technology evolves, and as the experience with composites in aircraft continues to build. A 1994 NASA report [15] indicated excellent in-service performance of composite components in commercial aircraft over a 15-year evaluation period, and such results have encouraged increased usage of composites in aircraft structures, including small business-type aircraft and large, commercialtransport aircraft. Initial use in these aircraft was restricted to smaller, lightly loaded secondary structures, but recently, composites are being used increasingly in large, heavily loaded primary structures such as the wings and fuselage. For example, the Cirrus SR-22 single-engine, a four-passenger aircraft shown in Figure 1.10, has a composite fuselage and wings. As an excellent example of innovative design made possible by composites, the use of composites in this airplane resulted in enough weight savings to accommodate the extra weight of an airframe parachute system for safe descent of the entire aircraft in the event of a loss of engine power. The application of composites in commercial airliners has shown steady, conservative growth, but based on the increased prices of fuels, demands by airlines for more 20 Principles of Composite Material Mechanics FIGURE 1.9 Northrup Grumman B2 Spirit stealth bomber with composite structure. (Courtesy of Northrup Grumman Corporation.) FIGURE 1.10 Cirrus SR-22 single-engine, four-passenger composite aircraft. (Courtesy of Cirrus Design Corporation.) Introduction 21 eficient aircraft, and other recent trends, this growth promises to be rapid in the future. For example, the Boeing 787 (Figure 1.11) is the irst commercial airliner with a composite fuselage and wings. As much as 50% of the primary structure—including the fuselage and wings—on the 787 consists of carbon iber/epoxy composite materials or carbon iber-reinforced plastics. The Airbus A350 XWB is another composites-intensive commercial airliner similar to the Boeing 787. The level of sophistication attained in aircraft composite construction is strikingly illustrated by the composite helicopter rotor blade in Figure 1.12. The construction of such a component obviously requires a multistep fabrication procedure involving many materials, and some of these fabrication processes will be discussed in the next section. Owing to the tremendous cost per unit weight to place an object in space, the value of weight saved is even greater for spacecraft. Thus, composites are extremely attractive for spacecraft applications. The NASA Space Shuttle has a number of composite parts, including graphite/epoxy cargo bay doors and experimental graphite/epoxy solid rocket-booster motor cases. For large space structures such as the proposed space station, the key properties of the structural materials are high stiffness-to-weight ratio, low thermal expansion coeficient, and good vibration-damping characteristics. In all three of these areas, composites offer signiicant advantages over conventional metallic materials. CFRP skin CFRP sandwich Fiberglass Aluminum Aluminum/steel/titanium struts FIGURE 1.11 Boeing 787—irst commercial airliner with composite fuselage and wings. (Courtesy of Boeing Company.) Principles of Composite Material Mechanics 22 Outer carbon/epoxy wrap Inner carbon/epoxy wrap Aramid paper honeycomb Titanium erosion shield Electrical heater mat ±45° woven glass/epoxy skins Tube for balance weights Unidirectional Unidirectional glass/epoxy glass/epoxy Unidirectional back wall nose module hybrid glasscarbon/epoxy side packs FIGURE 1.12 Composite construction of a helicopter rotor blade. (From McCrum, N. G., Buckley, C. P., and Bucknall, C. B. Principles of Polymer Engineering, 1988, New York, NY, by permission of Oxford University Press.) Scaled Composite’s SpaceShipOne (Figure 1.13), the irst private manned spacecraft to achieve suborbital light, is constructed primarily from composite materials, and promises to lead the way to commercial manned space travel. In other spacecraft components such as precision relectors (Figure 1.14), special composite structures such as carbon iber-reinforced isogrids are used for their superior dimensional stability characteristics. As shown later, some advanced ibers such as carbon have extremely low (and in some FIGURE 1.13 SpaceShipOne and its mother ship White Knight. (Copyright 2004, Mojave Aerospace Ventures LLC, photograph by Scaled Composites. SpaceShipOne is a Paul G. Allen project.) Introduction 23 FIGURE 1.14 Composite isogrid spacecraft relector. (Courtesy of Composite Optics, Inc.) cases, negative) thermal expansion coeficients, which makes it possible to design composite structures having excellent dimensional stability. Structural weight is also very important in automotive vehicles, and the use of composite automotive components continues to grow. Glass iberreinforced polymers (FRPs) continue to dominate the automotive composites market, but advanced composites with carbon iber reinforcement are getting increased attention as the cost of carbon ibers continues to drop. In cargo trucks, the reduced weight of composite components translates into increased payloads, which can have a signiicant economic impact. For example, the composite concrete mixer drum shown in Figure 1.15 weighs 2000 lb less than the conventional steel mixer drum that it replaced. According to the manufacturer, this means that an additional one-half cubic yard of concrete per load can be transported, which translates into an estimated productivity gain of $7500 per year. 24 Principles of Composite Material Mechanics FIGURE 1.15 Composite mixer drum on concrete transporter truck weighs 2000 lb less than conventional steel mixer drum. (Courtesy of Oshkosh Truck Corporation.) Weight savings on speciic components such as composite leaf springs can exceed 70% compared with steel springs (composite leaf springs have also proved to be more fatigue resistant). Experimental composite engine blocks have been fabricated from graphite-reinforced thermoplastics, but the ultimate goal is a ceramic composite engine that would not require water cooling. Chopped glass FRPs have been used extensively in body panels where stiffness and appearance are the principal design criteria. Composite structures such as Automotive Composites Consortium’s composite underbody (Figure 1.16) are only experimental at this point, but they offer weight reduction, fewer parts, and smaller assembly and manufacturing costs. So far, the applications of composites in automotive vehicles have been mainly in secondary structural elements and appearance parts, and the full potential of composite primary structures remains to be explored. With the increased interest in electric vehicles comes a need for composite structures to reduce vehicle structural weight to compensate for the heavy batteries that are required. For example, the proposed BMW Megacity electric vehicle in Figure 1.17 would have a carbon iber composite passenger compartment integrated with an aluminum spaceframe. Other applications of structural composites are numerous, and so only a few examples will be given here. I-beams, channel sections, and other structural elements (Figure 1.18) used in civil infrastructure may be made of iberreinforced plastic using the pultrusion process, which will be discussed in Introduction 25 Steel assembly (16 stampings) Composite assembly (1-piece molding) FIGURE 1.16 Automotive Composite Consortium’s preliminary composite underbody design, replacing 16 steel stampings with one molded component. This work was sponsored by an agency of the U.S. Government. Neither the U.S. Government nor any agency thereof, nor any of their employees makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy completeness, or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any speciic commercial product, process, or service by trade name, trademark, manufacturer, or otherwise does not necessarily constitute or imply its endorsement, recommendation, or favoring by the U.S. Government or any agency thereof. The views and opinions of authors expressed herein do not necessarily state or relect those of the U.S. Government or any agency thereof. (This material is based on the work supported by the Department of Energy National Energy Technology Laboratory under Award Number DE-FC26-02OR22910. With permission.) the next section. Corrosion resistance and electrical and thermal insulation are added advantages of composites over steel in such applications. Wind turbines (Figure 1.19) are getting increased attention as environmentally attractive, alternative energy sources, and their blades are typically made from composites due to their high strength-to-weight ratio, high stiffness-toweight ratio, excellent vibration damping, and fatigue resistance. The bodies of large mass-transportation vehicles such as airport people movers (Figure 1.20) are often fabricated from composites for the same reasons that they are used in many other transportation vehicles, and because, as shown in the next section, high-volume, low-cost processes for fabricating such large structures are now believed to be relatively mature technologies. One of the fastest-growing applications of composites in civil infrastructure is in prefabricated bridge decks for either new bridges or rehabilitation of older bridges. FRP composite bridge decks (Figure 1.21) have many advantages over conventional concrete and steel decks: FRP decks weigh much less, are more resistant to corrosion and freeze−thaw cycles, and are more easily and 26 Principles of Composite Material Mechanics FIGURE 1.17 Concept sketch, carbon iber composite cockpit and aluminum spaceframe for BMW Megacity electric vehicle. (Courtesy of BMW.) FIGURE 1.18 Pultruded iberglass composite structural elements. (Courtesy of Strongwell Corporation.) Introduction 27 FIGURE 1.19 Composite wind turbine blades. (Courtesy of GE Energy.) quickly installed. A major related application is the now common practice of seismic retroitting of conventional concrete–steel bridge columns by wrapping them with composite tapes in earthquake-prone areas. In these examples, as well as in many of the previous examples, cost is a major consideration limiting the more widespread use of composites. The fabrication FIGURE 1.20 Airport people mover with composite body. (Courtesy of TPI Composites.) 28 Principles of Composite Material Mechanics FIGURE 1.21 Installation of FRP composite deck for bridge rehabilitation. (Courtesy of Strongwell Corporation.) process is the key to cost control, and Section 1.5 will describe the fabrication processes used to make the components described here. 1.4 Multifunctional Applications of Composites Interest in the mechanics of multifunctional materials and structures has increased markedly in recent years [16]. The increased interest in multifunctional materials and structures is driven by the need for the development of new materials and structures that simultaneously perform (a) multiple structural functions, (b) combined nonstructural and structural functions, or (c) both. One example of a multifunctional structure of type (a) would be a composite structure that has high strength, high stiffness, low thermal expansion, and high damping. An example of type (b) would be a loadbearing structure that has the capability of providing its own noise and vibration control, self-repair, thermal insulation, and energy harvesting/ storage, whereas an example of type (c) would be a structure combining the functions of both types (a) and (b). Most of the recent developments in multifunctional materials and structures tend to be of type (b). Multifunctional materials are necessarily composite materials, and the strong growth in the use of composites has been greatly inluenced by multifunctional design requirements. The traditional approach to the development of structures is to address the load-carrying function and other functional Introduction 29 requirements separately, resulting in a suboptimal load-bearing structure with add-on attachments that perform the nonstructural functions with the penalty of added weight. Recently, however, there has been increased interest in the development of load-bearing materials and structures that have integral nonload-bearing functions, guided by recent discoveries about how multifunctional biological systems work. Among the most important nonstructural functions that a structure may need are electrical and thermal conductivity, but the most widely used composites have polymer matrix materials, which are typically poor conductors. So, conductive polymer nanocomposites are being investigated as possible replacements for nonconducting polymer matrix materials. Very small concentrations of CNTs or other conducting nanoreinforcements in polymers lead to disproportionately large improvements in the electrical conductivity of the nanocomposite. Figure 1.22 shows that the electrical conductivity of CNT/epoxy nanocomposites increases by nearly six decades when the CNT concentration is increased by only two decades [17]. The “percolation threshold,” φc which is the CNT concentration in the polymer that characterizes the insulator–conductor transition, is only 0.04 wt.% in this case. Sensing and actuation are two closely related nonstructural functions, and in many cases, the same material or device can be used for both functions, as well as for other functions like energy harvesting/storage and structural health monitoring. Piezoelectric materials such as lead zirconate titanate (PZT) can be embedded in structures for sensing and actuation, as they 1 0.1 Conductivity, σ (s/m) 0.01 1E-3 1E-4 1E-5 1E-6 1E-7 φc = 0.04 wt.% t = 3.6 1E-8 1E-9 0.01 0.1 1 CNT concentration, φ (wt.%) FIGURE 1.22 Electrical conductivity of CNT/epoxy nanocomposites at various CNT concentrations. Percolation threshold is 0.04 wt.%. (Reprinted from Composites Science and Technology, 69(10), Bauhofer, W. and Kovacs, J. Z., A review and analysis of electrical percolation in carbon nanotube polymer composites, 1486–1498, Copyright 2009, with permission from Elsevier.) Principles of Composite Material Mechanics 30 naturally possess the required electromechanical coupling. As shown in Figure 1.23, piezoelectric structural ibers for sensing and actuation consist of conductive structural ibers such as carbon coated with a piezoelectric interphase layer and an outer electrode layer [18]. Piezoelectric structural iber composites are suitable for vibration control, damping, energy harvesting, or structural health monitoring. A truly autonomous multifunctional structure will be capable of healing itself when damaged, as a biological system would, and recent research has demonstrated the feasibility of self-healing polymers and polymer composites based on the use of a microencapsulated healing agent and a catalyst for polymerizing the healing agent [19]. As shown in Figure 1.24, when damage causes cracks in the polymer, the cracks break open the microcapsules, causing the healing agent to leak into the crack by capillary action. The healing agent then reacts with the catalyst, causing polymerization that bonds the crack faces together. Structurally integrated electronics such as batteries for energy storage are another recent application of multifunctional structure design. The effectiveness of a multifunctional system is best deined by using a metric that characterizes the particular system such as light endurance time for an aircraft vehicle. For example, by integrating a polymer lithium–ion battery in the carbon/epoxy composite wing skin structure of the DARPA Wasp micro air vehicle (MAV), a record-setting light endurance time for the vehicle was achieved [20]. A photo of this vehicle is shown in Figure 1.25. Electrode 3 r0 t Piezoelectric material 1 Carbon fiber FIGURE 1.23 Multifunctional piezoelectric structural iber. (Reprinted from Composites Science and Technology, 68(7–8), Lin, Y. and Sodano, H. A., Concept and model of a piezoelectric structural iber for multifunctional composites, 1911–1918, Copyright 2008, with permission from Elsevier.) Introduction 31 (a) Catalyst Microcapsule Crack (b) Healing agent (c) Polymerized healing agent FIGURE 1.24 Illustration of self-healing of cracks in polymers by the use of a microencapsulated healing agent and a catalyst for polymerizing the healing agent. (a) Cracks form in the matrix; (b) the crack ruptures the microcapsules, releasing the healing agent into the crack through capillary action; and (c) the healing agent contacts the catalyst, triggering polymerization that bonds the crack faces closed. (With kind permission from Springer Science + Business Media: Experimental Mechanics, Fracture testing of a selfhealing polymer composite, 42(4), 2002, 372–379, Brown, E. N., Sottos, N. R., and White, S. R.) Other important nonstructural functions that are being integrated into multifunctional composite structures include thermal stability, thermal conductivity, electromagnetic interference shielding, recyclability and biodegradability, optical transparency, and morphing capability. A more detailed review of research on the mechanics of multifunctional composite materials and structures can be found in Reference 16. 1.5 Fabrication Processes Although this book is concerned primarily with the mechanics of composite materials, it is essential for the reader to know how these materials are made. 32 Principles of Composite Material Mechanics FIGURE 1.25 First generation DARPA Wasp MAV with polymer lithium–ion battery (silver quadrilaterals) integrated in composite wing skin structure. (With kind permission from Springer Science + Business Media: Journal of the Minerals, Metals and Materials Society, The design and application of multifunctional structure-battery material systems, 57(3), 2005, 18–24. Thomas, J. P. and Qidwai, M. A.) This is because, with composites, we design and build not only the structure, but also the structural material itself. The selection of a fabrication process obviously depends on the constituent materials in the composite, with the matrix material being the key (i.e., the processes for polymer matrix, metal matrix, and ceramic matrix composites are generally quite different). In this summary of fabrication processes, only those used for polymer matrix composite fabrication will be discussed, and the reader is referred to other books for details on metal matrix and ceramic matrix composite fabrication [8–13]. More details on composites manufacturing processes and analytical modeling of the processes can be found in Reference 21. A summary of fabrication processes used for polymer composites with various types of iber reinforcement is given in Table 1.2. The open-mold process with hand lay-up of woven iber mat or chopped strand mat (Figure 1.26) or spray-up of chopped ibers (Figure 1.27) is used for development work, prototype fabrication, and production of large components in relatively small quantities. A mold having the desired shape is irst coated with a mold release, which prevents bonding of the resin matrix material to the mold. If a smooth surface on the part is desired (i.e., boat hulls or aircraft exterior parts), a gel coat is then applied to the mold, followed by a thermosetting polymer resin and the ibers. A roller may then be used for consolidation, followed by curing the polymer resin at the required temperature. A major breakthrough in composite manufacturing technology was the development of “prepreg tape,” which is a tape consisting of ibers precoated with the polymer resin. This innovation means that the fabricator no longer Introduction 33 TABLE 1.2 Fabrication Processes for Polymer Matrix Composites Type of Reinforcement Process Continuous Open mold Hand lay-up Spray-up Autoclave Compression molding Filament winding Roll wrapping Pultrusion Liquid composite molding Reinforced reaction injection molding Resin infusion Automated iber placement Thermoplastic molding Programmable powdered preform process X X X X X X Chopped Woven X X X X X X X X X X Resin Mat Gel coat Roller Wax coating on mold (or mold release) Mold FIGURE 1.26 Open-mold, hand lay-up composite fabrication. Fibers Chopper-spray gun Mold Resin FIGURE 1.27 Open-mold, spray-up composite fabrication. X X X X X X X X X X X X Hybrid X X Principles of Composite Material Mechanics 34 Hot-melt prepregging reinforcement Resin film on carrier interleaf Scrap top film carrier take-up roll Pull rolls Cooling rolls Prepreg with Slitting devices Film/prepreg carrier interleaf take-up scrap edges take-up roll Heat and pressure rolls FIGURE 1.28 Hot-melt prepregging process. (Courtesy of Suppliers of Advanced Composite Materials Association [SACMA].) has to worry about consistently mixing the resin components in the right proportions and combining the resin with the ibers in the correct fashion. Most prepreg tapes are made by the hot-melt process (Figure 1.28). If a thermosetting resin is used, the resin coating is partially cured, and the tape must be kept refrigerated to prevent full curing until inal use. If a thermoplastic resin is used, the tape can be stored at room temperature until it is melted during inal use. The fabrication of a laminated structure with prepreg tape involves simply “laying-up” the tapes at the required orientations on a mold, stacking layers of tape in the required stacking sequence, and then curing the assembly under elevated temperature and pressure. Autoclave molding (Figure 1.29) is the standard aerospace industry process for fabrication with prepreg tapes. The autoclave is simply a heated pressure vessel into which the mold (with lay-up) is placed and subjected to the required temperature and pressure for curing. The mold and lay-up Pressure chamber Vacuum bag Lay-up (prepreg) Compressor Mold Heaters Vacuum pump FIGURE 1.29 Autoclave molding. Introduction 35 are often covered with a release fabric, a bleeder cloth, and a vacuum bag. A vacuum line is then attached to the mold for evacuation of volatile gases during the cure process. Without the vacuum bagging, these gases would be trapped and could cause void contents of greater than 5% in the cured laminate. With the vacuum bag, void contents of the order of 0.1% are attainable. Autoclaves come in a wide range of sizes, from bench-top laboratory versions to the room-sized units used to cure large aircraft structures. Owing to the expense and physical size of autoclaves for large structures, there is considerable interest in the development of “out-of-autoclave (OOA)” processes and prepreg materials. One such process, Quickstep™, involves the use of a luid-illed, balanced pressure, heated loating mold technology, and works by rapid heating of the laminate that is positioned between a mold that loats in a special heat transfer luid. The mold and laminate are separated from the circulating heat transfer luid by a lexible bladder. The autoclave-style press cure [22] is often used to cure small samples for research. In this case, a vacuum-bagged mold assembly (Figure 1.30) is inserted between the heated platens of a hydraulic press, and the press then generates the temperature and pressure required for curing. A vacuum press is a variation on this concept involving the use of a vacuum chamber surrounding the platen–mold assembly, and a sealed door on this chamber eliminates the need for a vacuum bag. Owing to the cost and energy consumption of autoclaves (especially the large room-sized autoclaves in use by the aerospace industry), increased research activity has been directed toward the development of OOA processing of prepreg composite lay-ups using specially formulated prepreg resins with different cure cycles that enable the lay-up to be cured using vacuum pressure alone. One version of the OOA, vacuum bag only processing, involves the use of an oven and a vacuum bag instead of an autoclave. Another version involves direct heating of the lay-up from the mold itself instead of an external oven. Owing to the reduced pressure on the mold in Vacuum bag mount O-ring Spacer plate Vacuum bag Vacuum Pressure plate Bleeder cloth Release fabric Laminate To l Heated platen FIGURE 1.30 Lay-up sequence for autoclave-style press molding. Rubber dam Principles of Composite Material Mechanics 36 OOA processing, the required tooling can be made of lightweight composites instead of heavy metallic materials such as Invar. Signiicant advances in OOA have been made in recent years, and it has been demonstrated that OOA-cured prepregs have properties essentially equivalent to those of autoclave-cured prepregs that have been previously qualiied for aerospace primary structure use. Sheet-molding compounds (SMCs) are an important innovation in composite manufacturing that are used extensively in the automobile industry. SMCs are similar to prepreg tape in that the ibers and the resin are “prepackaged” in a form that is more easily utilized by fabricators. SMCs consist of a relatively thick, chopped iber-reinforced resin sheet, whereas a prepreg usually has continuous ibers in a thin tape. A machine for producing SMCs is shown schematically in Figure 1.31. An alternative to SMCs are bulk-molding compounds (BMCs), which consist of the chopped iber/resin mixture in bulk form. SMCs or BMCs may be molded by using the matched metal die process (Figure 1.32). Filament winding (Figure 1.33) which involves winding resin-coated ibers onto a rotating mandrel, may be used to produce any composite structure having the form of a body of revolution. Fiber orientation is controlled by the traverse speed of the iber winding head and the rotational speed of the mandrel. Another advantage of this process is that by controlling the winding tension on the ibers, they can be packed together very tightly to produce Chopper Paste doctor blade Continuous strand roving Resin filler paste Resin filler paste Doctor blade Plastic carrier film Take-up roll Plastic carrier film Chopped roving Compaction section FIGURE 1.31 Machine for producing SMCs. (From Reinhart, T. J. et al. eds. 1987. Engineered Materials Handbook, Composites, Vol. 1. ASM International, Materials Park, OH. Reprinted by permission of ASM International.) Introduction 37 Prepreg tape or sheet-molding compound (SMC) Heated die FIGURE 1.32 Compression molding with matched metal dies. high-iber-volume fractions. On completion of the winding process, the composite structure may be cured by placing the mandrel in an oven or by passing hot luid through the mandrel itself. Filament winding is widely used to produce such structures as rocket motor cases, pressure vessels, power transmission shafts, piping, and tubing. Prepreg tape is often produced by ilament winding and removing the tape from the mandrel before curing. Imaginative variations on the ilamentwinding process have produced a variety of structures such as leaf springs for automotive vehicles. A composite leaf spring may be fabricated by winding on an ellipsoidal mandrel, then cutting the cured shell into the required pieces. Experimental programs are underway to produce large, complex structures such as aircraft fuselages and automobile body structures by ilament winding. Filament-winding machines for such structures will require the liberal use of computer control and robotics. The roll wrapping (or tube rolling) process also involves the placement of resin-impregnated ibers on a cylindrical mandrel to produce a composite tube or other body of revolution. However, in the case of roll wrapping, sheets of composite prepreg tape are wrapped around the mandrel by rolling the Tension adjust Resin-coated fibers Fiber roving Rotating mandrel FIGURE 1.33 Filament-winding process. Resin bath Principles of Composite Material Mechanics 38 mandrel over the prepreg, which lies lat on a table. In this manner, prepreg tape is wrapped around the mandrel at a rate of one layer per revolution, and the mandrel is indexed after each revolution so that the abutting joints of prepreg tape are offset by some amount, thus avoiding an undesirable region of weakness that would be generated if all the abutting joints line up along a radial line. Once the wrapping process is completed, the mandrel is externally pressurized and heated at the required cure pressure and temperature. One advantage of roll wrapping over ilament winding is that the ibers can be oriented in the true circumferential direction for maximum hoop strength, whereas in ilament winding, some amount of deviation from circumferential iber orientation will be introduced as the winding head traverses along the rotating mandrel. Either unidirectional iber or woven fabric-reinforced prepreg can be used in roll wrapping, whereas ilament winding is typically restricted to unidirectional iber tows. Roll wrapping is often used to produce ishing rods, golf club shafts, hockey sticks, and tubing for bicycle frames. Many of the processes described above are fairly time consuming. Processes with faster production cycles are needed for high-volume applications such as automotive parts. For example, reinforced reaction injection molding (RRIM) is a very fast process that is widely used to produce such components as automobile body panels. The RRIM process (Figure 1.34) involves the injection of a chopped iber/resin mixture into a mold under high pressure and then curing it at the required temperature. Pultrusion (Figure 1.35) is the process of pulling a continuous iber/resin mixture through a heated die to form structural elements such as I-beams and channel sections (Figure 1.18). This process is relatively fast but is restricted to structures whose shapes do not change along the length. In the thermoplastic molding process (Figure 1.36), a blank (an uncured laminate consisting of thermoplastic prepreg tape layers) is passed through an infrared oven where it is heated to near the melting point of the thermoplastic resin. Thermoplastic yarn or woven textiles consisting of commingled reinforcing ibers and thermoplastic matrix ibers (Figure 1.37) are also used. The heated blank is then quickly placed in a matched metal die mold for inal forming. In another form of thermoplastic molding, solid cylindrical pellets containing either long or short chopped Resin + fibers Heated mold Mix head Hardener FIGURE 1.34 RRIM process. Introduction 39 Heated die Puller Fiber roving Resin bath FIGURE 1.35 Pultrusion process. Press Infrared oven Blank Conveyor belt Mold FIGURE 1.36 Thermoplastic molding process. ibers in a thermoplastic resin are melted and molded by using a screw injection machine or by compression molding. Resin transfer molding (RTM) and structural reaction injection molding (SRIM) are attracting considerable attention because of their relatively fast production cycles and the near-netshape of resulting parts. In both the RTM process (Figure 1.38) and the SRIM Reinforcing fibers Thermoplastic fibers which form matrix after melting FIGURE 1.37 Commingled reinforcing ibers and thermoplastic matrix ibers in a thermoplastic yarn. Principles of Composite Material Mechanics 40 High speed resin transfer molding process composite cross-member Oven Dry glass fiber mat with thermoplastic binder Steel shaping and trimming die Low-pressure stamping press Resin pump Heated precut glass material Foam core stell mold Top glass preform shell Clamp press Foam core Molded foam core Bottom glass preform shell Low-pressure press Oven Low-pressure stamping press HSRTM heated steel mold Heated precut glass material Steel shaping and trimming die Engineered Perform glass eye assembly station preforms Resin pump Molded cross-member FIGURE 1.38 RTM process. (Courtesy of Ford Motor Company, Research Staff.) process, a “preform” consisting of ibers and possibly a foam core is irst produced in the general shape of the inished part. The preform is then placed in a closed metal mold and the liquid resin is injected under pressure. The major difference between the two processes is that with RTM, the resin and hardener are premixed before injection into the mold, whereas with SRIM, the resin and hardener are mixed by impingement as they are injected into the mold. 3D shaped parts with foam cores can be produced with both RTM and SRIM, but SRIM tends to be faster than RTM. In the vacuum-assisted RTM (VARTM) process, a vacuum pump is connected to the closed mold to pull the resin through the iber preform. The SCRIMP™ (Seeman composites resin infusion molding process), shown in Figure 1.39, is an open-mold/vacuum bag version of the VARTM process; it is effective for fabricating very large composite structures. The resin ilm infusion (RFI) process is similar to the SCRIMP™ process except that a solid resin ilm is used instead of a liquid resin. In RFI, the lay-up consists of the iber preform and a solid resin ilm covered with a vacuum bag in an open mold, followed by heating and melting of the resin ilm, which infuses the iber preform. Finally, the composite part is cured and released from the mold. The automated iber placement process involves robotic placement of thermoset or thermoplastic prepreg tapes on a mold and is widely used in the aerospace industry. In processing methods that involve iber preforms, one of the costliest and most time-consuming steps is the fabrication of the iber preform Introduction 41 Vacuum bag Resin flow medium Laminate Core Laminate Mold Typical SCRIMP schematic Catalyzed resin Vacuum pump FIGURE 1.39 Schematic of SCRIMP™ (Seeman composites resin infusion molding process). (Courtesy of TPI Composites.) itself. An innovative breakthrough in preform fabrication involves the use of robotic iber placement in the so-called P4 (programmable powder preform process). In the P4 process, continuous ibers are chopped and sprayed onto a mold screen by a programmable robot, along with a small amount of resin binder to hold the ibers in place. A vacuum also helps to hold the ibers in place on the screen. The completed iber preform is removed from the screen and placed in a mold where it is iniltrated with resin that is cured to form the composite part. In conclusion, many innovative processes exist for manufacturing polymer composites. Much of the success that composite materials have had in the past several decades is due to innovative fabrication technology, and the future success of composites will surely depend on further advances in this area. Computer-aided manufacturing technology and robotics are expected to play important roles in the continuing drive to reduce cost and to improve the quality of composite structures. EXAMPLE 1.5 Innovations in manufacturing processes are responsible for much of the growth in the application of composite materials and structures. In some cases, it may not be intuitively obvious as to which process or processes could be used to manufacture a particular composite component. For example, how can the ilament-winding process be used to manufacture composite leaf springs for automotive vehicles? Solution One way is to wind resin-impregnated unidirectional ibers on a highly elliptical mandrel, where the major axis of the ellipse corresponds to the winding axis and the span of the leaf spring. After winding and curing Principles of Composite Material Mechanics 42 the composite on the mandrel, the resulting elliptical composite shell could be mechanically cut in such a way that the resulting pieces are the leaf springs. EXAMPLE 1.6 One form of multifunctionality in composites involves the integration of mechanical and electrical properties. One way to increase the electrical conductivity of nonconducting polymers is to combine the polymer with conducting reinforcements such as carbon. Which form of carbon would you expect to be more effective in increasing the electrical conductivity of a carbon/polymer composite—CNTs or carbon nanoparticles? Solution CNTs have a much higher aspect ratio (or length-to-diameter ratio) than carbon nanoparticles, so in a carbon/polymer composite it is much easier for CNTs to develop a conducting path through the nonconducting polymer matrix. As a result, the so-called “percolation threshold” (i.e., the CNT concentration in the polymer which characterizes the insulator– conductor transition) for CNTs would typically be much lower for CNTs than for carbon particles. PROBLEM 1.7 Describe some practical physical limitations on the use of the RRIM process in molding of chopped FRP matrix composites. PROBLEM 1.8 Describe some practical physical limitations on the use of the RTM process in fabrication of composite sandwich structures which consist of composite face sheets and foam or honeycomb core. PROBLEM 1.9 Describe a possible sequence of fabrication processes that might be used to manufacture the helicopter rotor blade in Figure 1.12. Note that several different materials and iber lay-ups are used. 1.6 Elements of Mechanical Behavior of Composites This book is concerned with the analysis of both the micromechanical and the macromechanical behavior of iber-reinforced composite materials. As shown schematically in Figure 1.40, micromechanics is concerned with the mechanical behavior of constituent materials (in this case, iber and matrix materials), the interaction of these constituents, and the resulting behavior of the basic Introduction 43 Micromechanics Matrix (binder) Macromechanics Structure Lamina Laminate Reinforcing fibers FIGURE 1.40 Micromechanics and macromechanics of composites. composite (in this case, a single lamina in a laminate). Macromechanics is concerned with the gross mechanical behavior of composite materials and structures (in this case, lamina, laminate, and structure), without regard for the constituent materials or their interactions. As we will see in Chapter 2, this macromechanical behavior may be characterized by averaged stresses and strains and averaged, or “effective,” mechanical properties in an equivalent homogeneous material. As shown in Chapters 3 through 6, the focus in micromechanics is on the relationships between the effective composite properties and the effective constituent properties. Subsequent chapters deal with macromechanical behavior of laminates and structures. When dealing with composite materials, we ind very quickly that we can no longer draw upon the “intuition” about material behavior that we developed from years of experience with conventional metallic structural materials, and that we must learn to “think composites.” Most metallic structural materials are homogeneous (properties do not vary from point to point in the material) and isotropic (properties do not depend on orientation), whereas most composites are heterogeneous and anisotropic. That is, the properties in a composite change as we move from matrix to iber and as we change the direction along which they are measured. For example, in a “unidirectional” composite having reinforcement in only one direction, the strength and stiffness are much greater along the reinforcement direction than in the transverse direction. The relationships between forces and deformations (or between stresses and strains) are much more complicated in anisotropic composites than in conventional isotropic materials, and this can lead to unexpected behavior. For example, in an isotropic material, a normal stress induces only normal strains (extensions and/or contractions), and a shear stress induces only shear strains (distortions). In an anisotropic composite, however, a normal 44 Principles of Composite Material Mechanics stress may induce both normal strains and shear strains and a shear stress may induce both shear strains and normal strains. A temperature change in an isotropic material causes expansion or contraction that is uniform in all directions, whereas a temperature change in an anisotropic material may cause nonuniform expansion or contraction plus distortion. These so-called “coupling” effects have important implications not only for the analytical mechanics of composites, but also for the experimental characterization of composite behavior as well. It is hoped that these general observations regarding composite materials will provide motivation for further study in subsequent chapters, where the analytical and experimental characterization of mechanical behavior of composites is discussed in more detail. 1.7 Review of Basic Mechanics of Materials Equations The basic equations of the mechanics of materials are used throughout this book, and this section briely reviews and reinforces those equations, with examples of application to composite systems. As shown in many textbooks on the mechanics of solids [23,24], when the loading is static or quasistatic in nature, three basic categories of equations are typically used, separately or in combination, to solve problems in the elementary mechanics of materials. They are • Equations of static equilibrium based on Newton’s Second Law • Force–deformation or stress–strain relationships for the materials • Geometric compatibility equations or assumed relationships regarding the geometry of deformation In addition, using accurate free-body diagrams is essential to set up the correct equations of static equilibrium. The equations of mechanics of materials are often algebraic, but in some cases involving differential equations, a fourth category of equations, usually referred to as boundary conditions, is also needed. For example, the well-known beam-delection equations are second-order ordinary linear differential equations whose solution requires two boundary conditions. In problems involving dynamic loading, equations of motion are used instead of static equilibrium equations, and the equations of motion may be either ordinary or partial differential equations, depending on whether the mass is assumed to be discretely or continuously distributed, respectively. Most of the cases considered in this book will involve static or quasistatic loading, and dynamic loading is discussed mainly in Chapter 8. Finally, it is important to recognize that, for statically determinant systems, the three categories of equations described above can Introduction 45 be solved independently, but for statically indeterminate systems, they must be solved simultaneously. The remainder of this section consists of examples demonstrating the application of the basic equations of mechanics of materials to the analysis of composite systems. These preliminary examples involve only simple composite systems having isotropic constituents, and the force–deformation and stress–strain relationships of isotropic materials should be familiar from previous studies of the elementary mechanics of materials. However, it is important to realize that many composites and their constituents are anisotropic, and the corresponding force–deformation and stress–strain relationships of anisotropic materials are complex compared with those of isotropic materials. The study of anisotropic materials will begin in Chapter 2. EXAMPLE 1.7 We wish to ind the stresses and deformations in the axially loaded composite bar system in Figure 1.41a. The composite bar consists of two bars made of different isotropic materials A and B having different diameters and which are securely bonded together in a series arrangement and loaded by an axial load P. The bar of material A has length L A, crosssectional area A A, and modulus of elasticity EA, whereas the bar of material B has length LB, cross-sectional area AB, and modulus of elasticity EB. Free-body diagrams of the two bars are shown in Figure 1.41b. Solution For static equilibrium of bar A, which has internal force PA, ∑F = P x A −P=0 Bonded joint (a) P Bar B Bar A P LB LA (b) y P Bar A PA Bar B P PB x FIGURE 1.41 Composite bar system for Example 1.7. (a) Series arrangement of axially loaded bars and (b) free-body diagrams for bars A and B. Principles of Composite Material Mechanics 46 Similarly, for bar B, which has internal force PB, ∑F = P − P = 0 x B so that P = PA = PB and the load is the same for each bar in the series arrangement. The axial stresses in the two bars are therefore σA = PA AA and σ B = PB AB The axial elongations of the bars are given by the familiar force–deformation equations δA = PA LA AAEA and δ B = PB LB ABEB Since the bars are assumed to be securely joined together in a series arrangement, the total axial elongation is given by the geometric compatibility equation, δ total = δ A + δ B So, for the series arrangement, the forces are the same in each member, and the total deformation is the sum of the deformations in the members. This is also an example of a statically determinate system, since the forces in the members can be determined from the static equilibrium equations alone. For such a system, the force–deformation equations and the geometric compatibility equation are not needed to ind the forces in the members. The next example will be a statically indeterminate composite system, where the three basic types of equations must be solved simultaneously to ind the forces in the members. EXAMPLE 1.8 Now, we wish to ind the stresses and deformations in the composite system of Figure 1.42a, where a solid isotropic bar A is securely bonded inside a hollow isotropic bar B of the same length and both bars are axially loaded by a load P that is transmitted through rigid plates. The free-body diagrams for the bars and one of the rigid plates are shown in Figure 1.42b. Solution The static equilibrium of the rigid plate requires that the applied force P must be related to the internal forces in the members, PA and PB, by the equation Introduction 47 Rigid plates (a) Hollow bar B P P Solid bar A (b) Solid bar A PA PA Rigid plate PA y PB Hollow bar B PB P PB x FIGURE 1.42 Composite bar system for Example 1.8. (a) Parallel arrangement of axially loaded bars and (b) free-body diagrams of members. ∑F = P x A + PB − P = 0 or P = PA + PB This is the only nontrivial static equilibrium equation for this system, but the equation contains two unknown forces, PA and PB. Thus, unlike Example 1.7, the forces in the members cannot be determined from the static equilibrium equations alone, and the system is said to be statically indeterminate. A second equation is needed to solve for the two unknown forces, and that equation may be generated by combining the force–deformation relationships and the geometric compatibility condition. As with Example 1.7, the force–deformation relationships for the bars are δA = PA LA AAEA and δ B = PB LB ABEB Since the bars are assumed to be securely bonded together, the geometric compatibility condition for the parallel arrangement is δ A = δB So for the parallel arrangement, the deformations in the members are equal and the total applied force is equal to the sum of the member forces. By combining the force–deformation and geometric compatibility equations, we obtain a second equation in the two unknown forces PA and PB that can be solved simultaneously with the static equilibrium Principles of Composite Material Mechanics 48 equation. Once the forces PA and PB are found, the stresses and deformations in the members can be found. EXAMPLE 1.9 In the composite system shown in Figure 1.43a, a rigid L-shaped bar is hinged at point O and is also supported by a wood post and a steel cable. Before the load P is applied, the system is unstressed, and we wish to ind the stresses and deformations in the steel cable and the wood post after the load P is applied. (a) Ls b • a • P Steel cable c •O Hinge Rigid bar Lw Wood post (b) Fs • P • Ox Fw Oy (c) δs Undeformed a Deformed • δw O b FIGURE 1.43 Composite system for Example 1.9. (a) Arrangement of composite system, (b) free-body diagram of rigid L-shaped bar, and (c) geometry of deformation for rigid L-shaped bar. Introduction 49 Solution For a 2D problem such as this, three static equilibrium equations are available, but from the free-body diagram of the L-shaped bar in Figure 1.43b, it is seen that there are four unknown reaction forces: the force in the steel cable, Fs, the hinge forces Ox and Oy, and the force in the wood post, Fw. The hinge forces are not of interest here, and can be eliminated from the problem by writing the equation for static equilibrium of moments about an axis through the hinge point O, as ∑M O = Pc − Fw b − Fs a = 0 We now have one equation in two unknowns, Fw and Fs, and although there are two remaining available static equations, those equations would involve the hinge forces Ox and Oy, and so nothing can be gained by considering them. Thus, the problem is statically indeterminate, and we must develop the geometric compatibility and force–deformation equations and solve all the equations simultaneously. The geometry of deformation of the rigid L-shaped bar that rotates about the hinge point O is shown in Figure 1.43c. From this drawing, it is clear that the geometric compatibility equation is δw δs = b a where δw and δs are the deformations in the wood post and the steel cable, respectively. The corresponding force–deformation equations are δw = Fw Lw Aw Ew and δ s = Fs Ls As Es where Aw and As are the cross-sectional areas and Ew and Es are the elastic moduli of the wood post and the steel cable, respectively. Now the equilibrium, compatibility, and force–deformation equations can be solved simultaneously for the forces Fw and Fs; the forces and areas can then be used to determine the stresses. Thus, the general procedure for analyzing statically indeterminate structures is to solve the static equilibrium equations, the force–deformation equations, and the geometric compatibility equations simultaneously for the forces in the members, then use the member forces to ind the corresponding stresses and deformations. Although these same basic principles are used throughout this book, we ind that it is often more convenient and practical to work with the stresses rather than the forces, the strains rather than the deformations, and the stress–strain relationships rather than the force–deformation relationships. Example 1.10 illustrates these concepts. EXAMPLE 1.10 The composite ring assembly in Figure 1.44a consists of a thin steel inner ring of mean radius rs, wall thickness ts, modulus of elasticity Es, and Principles of Composite Material Mechanics 50 coeficient of thermal expansion αs, which just its inside an aluminum outer ring of mean radius ra, wall thickness ta, modulus of elasticity Ea, and coeficient of thermal expansion αa, so that both rings are initially unstressed at room temperature. We wish to determine the stresses in each ring after the assembly has been cooled by an amount ΔT < 0, where ΔT is the temperature drop. Solution From material property tables, we ind that αa ≫ αs, so that when the assembly is cooled, the aluminum ring tries to contract more than the steel ring. As a result of this differential contraction, a radial pressure, p, develops at the aluminum–steel interface, as shown in the free-body diagrams in Figure 1.44b. The effect of the interface pressure p is to put the inner steel ring in compression and the outer aluminum ring in tension. From the static equilibrium analysis of thin-walled cylinders or rings, which is found in any mechanics of materials book, the tangential (hoop) stresses in the two rings are σa = pra ta and σ s = − prs ts (a) ta Aluminum outer ring 2rs Steel inner ring 2ra ts (b) p p Steel inner ring Aluminum outer ring FIGURE 1.44 Composite ring system for Example 1.10. (a) Assembled rings and (b) free-body diagrams of rings after cooling. Introduction 51 However, it is clear from the free-body diagrams in Figure 1.44b that the pressure p and the corresponding stresses above cannot be found from the static equilibrium equations alone. Thus, the system must be statically indeterminate, and we must develop additional equations based on geometric compatibility and stress–strain relationships. From the mechanics of materials, the tangential (hoop) strains in the rings must be εa = ∆ra ra and ε s = ∆rs rs where Δra and Δrs are the radial displacements in the aluminum and steel rings, respectively. Since the two rings are securely bonded together, geometric compatibility requires that Δra = Δrs, so that εa = rs εs ra The tangential stress–strain relationships for the two materials including thermal effects are εa = σa σ + α a ∆T and ε s = s + α s ∆T Ea Es By combining the above equations, we can reduce the problem to one equation in one unknown, the interfacial pressure p, as shown below. pra r prs + α a ∆T = s − + α s ∆T ra tsEs ta E a By substituting the known geometrical and material properties along with the temperature change, we can solve this equation for p. Once p is determined, the corresponding stresses in the rings can be easily calculated. PROBLEM 1.10 A thin-walled ilament-wound composite pressure vessel has ibers wound at a helical angle θ, as shown in Figure 1.45. Ignore the resin matrix material and assume that the ibers carry the entire load. Also assume that all ibers are uniformly stressed in tension. This gross oversimpliication is the basis of the socalled “netting analysis,” which is actually more appropriate for stress analysis of all-iber textile fabrics. Using this simpliied analysis, show that the angle θ must be 54.74° in order to support both the hoop (tangential) and axial stresses that are generated in a thin-walled pressure vessel. (See any mechanics of materials book for the stress analysis of a thin-walled pressure vessel.) Principles of Composite Material Mechanics 52 Y θ θ X d t FIGURE 1.45 Filament-wound composite pressure vessel for Problem 1.10. PROBLEM 1.11 A ilament-wound E-glass/epoxy pressure vessel has a diameter of 50 in. (127 cm), a wall thickness of 0.25 in. (6.35 mm), and a helical wrap angle θ = 54.74°. Using a netting analysis and a safety factor of 2, estimate the allowable internal pressure in the vessel. Compare with the allowable internal pressure in a 6061-T6 aluminum alloy pressure vessel having the same dimensions. For the aluminum vessel, assume that the tensile yield stress is 40,000 psi (276 MPa) and use the maximum shear stress yield criterion. Although the netting analysis is greatly oversimpliied, these approximate results should demonstrate the signiicant advantages of iber composite construction over conventional metallic construction. PROBLEM 1.12 The 2000 mm long composite bar shown in Figure 1.46 consists of an aluminum bar having a modulus of elasticity EAl = 70 GPa and length LAl = 500 mm, which is securely fastened to a steel bar having modulus of elasticity ESt = 210 GPa and length LSt = 1500 mm. After the force P is applied, a tensile normal strain of εAL = 1000 × 10−6 is measured in the aluminum bar. Find the tensile normal stress in each bar and the total elongation of the composite bar. Introduction 53 P Aluminum Steel P 500 mm 1500 mm FIGURE 1.46 Composite bar system for Problem 1.12. PROBLEM 1.13 The concrete composite post in Figure 1.47 is 1.2 m long with a 0.3 m × 0.3 m square cross section. The post is reinforced by four vertical steel rods of the same length having a cross-sectional area of As = 0.00125 m2 each, and is loaded by a single vertical load P = 500 kN applied on the rigid cover plate as shown below. The modulus of elasticity for concrete is Ec = 17 GPa, whereas the modulus of elasticity of steel is Es = 200 GPa. Determine the stresses in the steel rods and concrete. PROBLEM 1.14 The composite bar system in Figure 1.48 consists of a steel bar and a bronze bar that are both securely attached to a rigid block and rigid supports. The system is loaded with a total load P at the rigid block. If the total applied load is P = 42,000 lb, determine the stresses in the two bars. PROBLEM 1.15 The composite post in Figure 1.49 has the same properties and dimensions as in Problem 1.13, except that there is a gap Δ = 0.1 mm between the top of the P = 500 kN Rigid cover plate Postcross section 1.2 m Steel rods (4) As = 0.00125 m2 each Concrete 0.3 m × 0.3 m FIGURE 1.47 Concrete composite post for Problem 1.13. 0.3 m 0.3 m Principles of Composite Material Mechanics 54 6′ P 2 Es = 30 × 106 psi A s = 1 in.2 Steel bar S P 2 Rigid block 2′ Bronze bar B EB = 15 × 106 psi AB = 4 in.2 FIGURE 1.48 Composite bar system for Problem 1.14. cover plate on the post and the upper support. An upward load P is applied to the rigid cover plate, which is securely attached to the concrete and the steel reinforcing rods. If the deformation due to the load P is just enough to close the gap Δ, determine the resulting stresses in the concrete and the steel rods, and the magnitude of the load P. Note that Figure 1.49 shows the position of the cover plate before the gap Δ has been closed. PROBLEM 1.16 For the original concrete composite post design of Problem 1.13, assume that the steel rods are made of 4340 steel, and that the rods are to be replaced Δ = gap distance = 0.1 mm Rigid cover plate Postcross section P 1.2 m Steel rods (4) As = 0.00125 m2 each Concrete 0.3 m × 0.3 m 0.3 m 0.3 m FIGURE 1.49 Composite post for Problem 1.15. See Problem 1.13 for material properties. Introduction 55 by IM9 carbon iber bundles of the same length in a new design. The new design also calls for the load and deformation in the carbon iber bundles to be the same as in the steel rods of the original design. Compare the weight of the carbon iber bundles in the new design with the weight of the steel rods in the original design. As with the original design, assume that the applied load P is just enough to close the gap Δ. PROBLEM 1.17 For the original 4340 steel-reinforced concrete post design of Problem 1.13 and the new IM9 carbon iber-reinforced concrete post design of Problem 1.16, compare the tensile stress-to-tensile strength ratio for the steel rod with the corresponding stress-to-strength ratio for the carbon iber bundles. References 1. Ashby, M. F. 1987. Technology of the 1990s: Advanced materials and predictive design. Philosophical Transactions of the Royal Society of London, A322, 393–407. 2. Wainwright, S. A., Biggs, W. D., Currey, J. D., and Gosline, J. M. 1976. Mechanical Design in Organisms. Princeton University Press, Princeton, NJ. 3. Grifith, A. A. 1920. The phenomena of rupture and low in solids. Philosophical Transactions of the Royal Society, 221A, 163–198. 4. Gordon, J. E. 1976. The New Science of Strong Materials, 2nd ed. Princeton University Press, Princeton, NJ. 5. Thostenson, E. R., Ren, Z., and Chou, T.-W. 2001. Advances in the science and technology of carbon nanotubes and their composites: A review. Composites Science and Technology, 61, 1899–1912. 6. Qian, D., Wagner, J. G., Liu, W. K., Yu, M. F., and Ruoff, R. S. 2002. Mechanics of carbon nanotubes. Applied Mechanics Reviews, 55(6), 495–533. 7. McCrum, N. G., Buckley, C. P., and Bucknall, C. B. 1988. Principles of Polymer Engineering. Oxford University Press, New York, NY. 8. Schwartz, M. M. 1984. Composite Materials Handbook. McGraw-Hill, Inc., New York, NY. 9. Weeton, J. W., Peters, D. M., and Thomas, K. L., eds. 1987. Engineer’s Guide to Composite Materials. ASM International, Materials Park, OH. 10. Lubin, G. ed. 1982. Handbook of Composites, Van Nostrand Reinhold Co., New York, NY. 11. Katz, H. S. and Milewski, J. V., eds. 1978. Handbook of Fillers and Reinforcements for Plastics. Van Nostrand Reinhold Co., New York, NY. 12. Reinhart, T. J. et al. eds. 1987. Engineered Materials Handbook, Composites, Vol. 1. ASM International, Materials Park, OH. 13. Mallick, P. K. ed. 1997. Composites Engineering Handbook. Marcel Dekker, Inc., New York, NY. 56 Principles of Composite Material Mechanics 14. Harris, C. E., Starnes, J. H., Jr., and Shuart, M. J. 2001. An assessment of the state-of-the-art in the design and manufacturing of large composite structures for aerospace vehicles. NASA TM-2001–210844. 15. Dexter, H. B. and Baker, D. J. 1994. Flight service environmental effects on composite materials and structures. Advanced Performance Materials, 1, 51–85. 16. Gibson, R. F. 2010. A review of recent research on mechanics of multifunctional composite materials and structures. Composite Structures, 92(12), 2793–2810. 17. Bauhofer W. and Kovacs, J. Z. 2009. A review and analysis of electrical percolation in carbon nanotube polymer composites. Composites Science and Technology, 69(10), 1486–1498. 18. Lin, Y. and Sodano, H. A. 2008. Concept and model of a piezoelectric structural iber for multifunctional composites. Composites Science and Technology, 68(7–8), 1911–1918. 19. Brown, E. N., Sottos, N. R., and White, S. R. 2002. Fracture testing of a selfhealing polymer composite. Experimental Mechanics, 42(4), 372–379. 20. Thomas, J. P. and Qidwai, M. A. 2005. The design and application of multifunctional structure-battery material systems. Journal of the Minerals, Metals and Materials Society, 57(3), 18–24. 21. Gutowski, T. G. ed. 1997. Advanced Composites Manufacturing. John Wiley & Sons, Inc., New York, NY. 22. Gibson, R. F., Suarez, S. A., and Deobald, L. R. 1985. Laboratory production of discontinuous-aligned iber composite plates using an autoclave-style press cure. Journal of Composites Technology and Research, 7(2), 391–400. 23. Crandall, S. H., Dahl, N. C., and Lardner, T. J. 1978. An Introduction to the Mechanics of Solids, 2nd ed. with SI units. McGraw-Hill, New York, NY. 24. Riley, W. F., Sturges, L. D., and Morris, D. H. 2002. Statics and Mechanics of Materials—An Integrated Approach, 2nd ed. John Wiley & Sons, Inc., New York, NY. 2 Lamina Stress–Strain Relationships 2.1 Introduction The basic building block of a composite structure is the lamina, which usually consists of one of the iber/matrix conigurations shown in Figure 1.4. For the purposes of mechanics analysis, however, the “unidirectionally reinforced” or “unidirectional” lamina with an arrangement of parallel, continuous ibers is the most convenient starting point. As shown in subsequent chapters, the stress–strain relationships for the unidirectional lamina form the basis for the analysis of not only the continuous iber composite laminate (Figure 1.4a), but also of woven iber (Figure 1.4b), chopped iber (Figure 1.4c), and hybrid chopped/continuous iber (Figure 1.4d) composites. A composite material is obviously heterogeneous at the constituent material level, with properties possibly changing from point to point. For example, the stress–strain relationships at a point are different for a point in the iber material than for a point in the matrix material. If we take the composite lamina as the basic building block, however, the “macromechanical” stress–strain relationships of the lamina can be expressed in terms of average stresses and strains and effective properties of an equivalent homogeneous material [1]. This chapter is concerned with the development and manipulation of these macromechanical stress–strain relationships. The “micromechanical” relationships between the constituent material properties and the effective lamina properties will be discussed in more detail in Chapter 3, but the basic concept of an effective modulus will be discussed here. To complicate matters further, the properties of a composite are usually anisotropic. That is, the properties associated with an axis passing through a point in the material generally depend on the orientation of the axis. By comparison, conventional metallic materials are nearly isotropic since their properties are essentially independent of orientation. Fortunately, each type of composite has characteristic material property symmetries that make it possible to simplify general anisotropic stress–strain relationships. In particular, the symmetry possessed by the unidirectional lamina makes it a socalled orthotropic material. The symmetries associated with various types of composite laminae and the resulting lamina stress–strain relationships 57 Principles of Composite Material Mechanics 58 are discussed in this chapter, along with certain mathematical manipulations that make it easier to deal with the directional nature of composite properties. 2.2 Effective Moduli in Stress–Strain Relationships A general three-dimensional (3D) state of stress at a point in a material can be described by nine stress components σij (where i, j = 1, 2, 3), as shown in Figure 2.1. According to the conventional subscript notation, when i = j, the stress component σij is a normal stress; and when i ≠ j, the stress component is a shear stress. The irst subscript refers to the direction of the outward normal to the face on which the stress component acts, and the second subscript refers to the direction in which the stress component itself acts. Corresponding to each of the stress components, there is a strain component εij describing the deformation at the point. Normal strains (i = j) describe the extension or contraction per unit length along the xi direction, and shear strains (i ≠ j) describe the distortional deformations associated with lines that were originally parallel to the xi and xj axes. It is very important to distinguish between the “tensor” strain εij and the “engineering” strain γij. In the case of normal strain, the engineering strain is the same as the tensor strain, but for shear strain, εij = γij/2. Thus, the engineering shear strain γij describes the total distortional change in the angle between lines 2 σ22 σ21 σ23 σ12 σ32 σ33 3 FIGURE 2.1 3D state of stress. σ11 σ31 σ13 1 Lamina Stress–Strain Relationships 59 that were originally parallel to the xi and xj axes, but the tensor shear strain εij describes the amount of rotation of either of the lines (Figure 2.2). In the most general stress–strain relationship at a point in an elastic material, each stress component is related to each of the nine strain components by an equation of the form σ ij = f ij (ε11 , ε12 , ε13 , ε 21 , ε 22 , ε 23 , ε 31 , ε 32 , ε 33 ) (2.1) where the functions fij may be nonlinear. For linear elastic material, which is of primary concern in this book, the most general linear stress–strain relationships at a point in the material (excluding effects of environmental conditions) are given by equations of the form σ 11 C1111 σ C 22 2211 σ 33 C3311 σ 23 … σ 31 = … σ 12 … σ 32 … σ … 13 σ 21 C2111 C1122 C2222 C3322 … … … … … C2122 C1133 C22233 C3333 … … … … … C2133 C1123 C2223 C3323 … … … … … C2123 C1131 C2231 C3331 … … … … … C2131 C1112 C2212 C3312 … … … … … C2112 C1132 C2232 C3332 … … … … … C2132 C1113 C2213 C3313 … … … … … C2113 C1121 C2221 C3321 … … … … … C2121 ε11 ε 22 ε 33 ε 23 ε 31 ε12 ε 32 ε 13 ε 21 (2.2) εxy = γxy 2 γxy = Engineering strain εxy = Tensor strain εxy = γxy 2 Total change in original angle = γxy Amount each edge rotates = γ xy /2 = εxy FIGURE 2.2 Geometric interpretation of engineering shear strain and tensor shear strain. Principles of Composite Material Mechanics 60 where [C] is a fully populated 9 × 9 matrix of stiffnesses or elastic constants (or moduli) having 81 components. Note that the irst two subscripts on the elastic constants correspond to those of the stress, whereas the last two subscripts correspond to those of the strain. If no further restrictions are placed on the elastic constants, the material is called anisotropic and Equation 2.2 is referred to as the generalized Hooke’s law for anisotropic materials. In practice, there is no need to deal with this equation and its 81 elastic constants because various symmetry conditions simplify the equations considerably. As shown in any mechanics of materials book [2], both stresses and strains are symmetric (i.e., σij = σji and εij = εji), so that there are only six independent stress components and six independent strain components. This means that the elastic constants must be symmetric with respect to the irst two subscripts and with respect to the last two subscripts (i.e., Cijkl = Cjikl and Cijkl = Cijlk, where i, j, k, and l each take on the values 1, 2, and 3) and that the number of nonzero elastic constants is now reduced to 36. These simpliications lead to a contracted notation that reduces the number of subscripts based on the following changes in notation [3–6]: σ11 = σ1 σ 22 = σ 2 σ 33 = σ 3 σ 23 = σ 32 = σ 4 σ13 = σ 31 = σ 5 σ12 = σ 21 = σ 6 ε11 = ε1 ε 22 = ε 2 ε 33 = ε 3 2ε 23 = 2ε 32 = γ 23 = γ 32 = ε 4 2ε13 = 2ε 31 = γ 13 = γ 31 = ε 5 2ε12 = 2ε 21 = γ 12 = γ 21 = ε 6 With this contracted notation, the generalized Hooke’s law can now be written as σ i = Cij ε j , i , j = 1, 2, . . ., 6 (2.3) and the repeated subscript j implies summation on that subscript. Alternatively, in matrix form, {σ} = [C]{ε} (2.4) where the elastic constant matrix or stiffness matrix [C] is now 6 × 6 with 36 components and the stresses {σ} and strains {ε} are column vectors, each having six elements. Alternatively, the generalized Hooke’s law relating strains to stresses can be written as ε i = Sijσ j , i , j = 1, 2, … , 6 (2.5) Lamina Stress–Strain Relationships 61 or in matrix form as {ε} = [S]{σ} (2.6) where [S] is the compliance matrix, which is the inverse of the stiffness matrix ([S] = [C]−1). For a brief review of matrix operations, please refer to Appendix A. As shown later, due to the existence of the strain energy density, the stiffness and compliance matrices are symmetric. Note that nothing has been said thus far about any symmetry that the material itself may have. All real materials have some form of symmetry, however, and no known material is completely anisotropic. Before discussing the various simpliications of the stress–strain relationships, it is appropriate to deal with the problem of heterogeneity in the composite material. Recall that the stress–strain relationships presented up to now are only valid at a point in the material, and that the stresses, strains, and elastic moduli will change as we move from point to point in a composite (i.e., the elastic moduli for the matrix material are different from those of the iber). In order to analyze the macromechanical behavior of the composite, it is more convenient to deal with averaged stresses and strains that are related by “effective moduli” of an equivalent homogeneous material. Figure 2.3 shows schematically how the stresses in a heterogeneous composite may be nonuniform even though the imposed strain is uniform. Heterogeneous composite under varying stresses and strains x3 σ2 x3 ε2 d σ2 L σ2 Strain, ε2 Stress, σ2 Equivalent homogeneous material under average stresses and strains σ2 x3 σ2 x3 ε2 σ2 Stress, σ2 FIGURE 2.3 Concept of an effective modulus of an equivalent homogeneous material. Strain, ε2 Principles of Composite Material Mechanics 62 As shown in Figure 2.3, if the scale of the inhomogeneity in a material can be characterized by some length dimension, d, then the length dimension, L, over which the macromechanical averaging is to take place, must be much larger than d if the average stresses and strains are to be related by effective moduli of an equivalent homogeneous material. We now deine the average stresses, σ i , and the average strains, εi , (i = 1, 2, …, 6) to be averaged over a volume V, which is characterized by the dimension L, so that [1] σi = ∫ σ dV = ∫ σ dV V ∫ dV (2.7) ∫ ε dV = ∫ ε dV V ∫ dV (2.8) i i V V V εi = i i V V V where i = 1, 2, …, 6 and σi and εi are the position-dependent stresses and strains at a point, respectively. If these averaged stresses and strains are used in place of the stresses and strains at a point, the generalized Hooke’s law (i.e., Equation 2.3) becomes σ i = Cij ε j (2.9) and the elastic moduli Cij then become the “effective moduli” of the equivalent homogeneous material in volume V. Similarly, the “effective compliances” Sij may be deined by εi = Sijσ j (2.10) For example, in Figure 2.3, the scale of the inhomogeneity is assumed to be the diameter of the iber, d, and the averaging dimension, L, is assumed to be a characteristic lamina dimension such that L ≫ d. The effective modulus C22 of the lamina is thus deined as C22 = σ 2 / ε2 . In the remainder of this book, lamina properties are assumed to be effective properties as described above. 2.3 Symmetry in Stress–Strain Relationships In this section, the generalized anisotropic Hooke’s law will be simpliied and specialized using various symmetry conditions. The irst symmetry Lamina Stress–Strain Relationships 63 condition, which has nothing to do with material symmetry, is strictly a result of the existence of a strain energy density function [3,6]. The strain energy density function, W, is such that the stresses can be derived according to the equation σi = ∂W = Cij ε j ∂ε i (2.11) 1 Cij ε i ε j 2 (2.12) where W= By taking a second derivative of W, we ind that ∂ 2W = Cij ∂ε i ∂ε j (2.13) and by reversing the order of differentiation, we ind that ∂ 2W = C ji ∂ε j ∂ε i (2.14) Since the result must be the same regardless of the order of the differentiation, Cij = Cji, the stiffness matrix is symmetric. Similarly, W can be expressed in terms of compliances and stresses, and by taking two derivatives with respect to stresses, it can be shown that Sij = Sji. Thus, the compliance matrix is also symmetric. Due to these mathematical manipulations, only 21 of the 36 anisotropic elastic moduli or compliances are independent, and we still have not said anything about any inherent symmetry of the material itself. According to the above developments, the stiffness matrix for the linear elastic anisotropic material without any material property symmetry is of the form C11 Cij = C12 C22 SYM C13 C23 C33 C14 C24 C34 C44 C15 C25 C35 C45 C55 C16 C26 C36 C46 C56 C66 (2.15) Principles of Composite Material Mechanics 64 Further simpliications of the stiffness matrix are possible only if the material properties have some form of symmetry. For example, a monoclinic material has one plane of material property symmetry. It can be shown [3,7] that since the Cij for such a material must be invariant under a transformation of coordinates corresponding to relection in the plane of symmetry, the number of independent elastic constants for the monoclinic material is reduced to 13. Such a symmetry condition is generally not of practical interest in composite material analysis, however. As shown in Figure 2.4, a unidirectional composite lamina has three mutually orthogonal planes of material property symmetry (i.e., the 12, 23, and 13 planes) and is called an orthotropic material. The term “orthotropic” alone is not suficient to describe the form of the stiffness matrix, however. Unlike the anisotropic stiffness matrix (Equation 2.15), which has the same form (but different terms) for different coordinate systems, the form of the stiffness matrix for the orthotropic material depends on the coordinate system used. The 123 coordinate axes in Figure 2.5 are referred to as the principal material coordinates since they are associated with the reinforcement directions. Invariance of the Cij under transformations of coordinates corresponding to relections in two orthogonal planes [3,7] may be used to show that the stiffness matrix for a so-called specially orthotropic material associated with the principal material coordinates is of the form C11 Cij = C12 C22 C13 C23 C33 SYM 0 0 0 0 0 0 C44 0 0 0 C66 0 0 0 C55 3, z θ y 2 1 x FIGURE 2.4 Orthotropic lamina with principal (123) and nonprincipal (xyz) coordinate systems. (2.16) Lamina Stress–Strain Relationships 65 3 r e Fib 1 ec dir n tio 2 Fibers are randomly packed in the 2–3 planes FIGURE 2.5 Specially orthotropic, transversely isotropic material. A stiffness matrix of this form in terms of engineering constants will be obtained in the next section using observations from simple experiments. Note that there are only 12 nonzero elastic constants and nine independent elastic constants for the specially orthotropic material. Table 2.1 summarizes similar results for the different combinations of materials and coordinate systems used in this book. If the stress–strain relationships for the specially orthotropic material are transformed to a nonprincipal coordinate system such as xyz as shown in Figure 2.4, the material is called generally orthotropic. Note that the number of independent coeficients in the stress–strain relationships for a material is the same, regardless of whether the material is described in principal or nonprincipal coordinates. Other important types of material symmetry will be developed in the next section, but the general forms of the stiffness matrices are given here for completeness. In most composites, the iberpacking arrangement is statistically random in nature (Figure 2.5), so that the properties are nearly the same in any direction perpendicular to the ibers (i.e., properties along the 2 direction are the same as those along the 3 direction, and properties are invariant to rotations about the 1 axis), and the material is transversely isotropic. If the ibers were packed in a regular array, such as a square array or a triangular array, the material would not be transversely isotropic. As shown later in Chapter 3, real composites typically have random iber packing, and can be considered transversely isotropic. For such a material, we would expect that C22 = C33, C12 = C13, C55 = C66, and that C44 would not be independent from the other stiffnesses. It can be shown [1] that the complete stiffness matrix for a specially orthotropic, transversely isotropic material is of the form Principles of Composite Material Mechanics 66 TABLE 2.1 Elastic Coeficients in the Stress–Strain Relationships for Different Materials and Coordinate Systems Material and Coordinate System Number of Nonzero Coeficients 3D Case Anisotropic Generally orthotropic (nonprincipal coordinates) Specially orthotropic (principal coordinates) Specially orthotropic, transversely isotropic Isotropic 2D Case (Lamina) Anisotropic Generally orthotropic (nonprincipal coordinates) Specially orthotropic (principal coordinates) Balanced orthotropic, or square symmetric (principal coordinates) Isotropic C11 Cij = C12 C22 SYM C12 C23 C22 Number of Independent Coeficients 36 20 21 9 12 9 12 5 12 2 9 9 6 4 5 4 5 3 5 2 0 0 0 0 0 0 (C22 − C23 ) 2 0 C66 0 0 C66 0 0 0 (2.17) where the 23 plane and all parallel planes are assumed to be planes of isotropy. In the next section, a stiffness matrix of the same form will be derived, except that the so-called engineering constants will be used instead of the Cij. Note that now there are still 12 nonzero elastic moduli but that only ive are independent (Table 2.1). The simplest form of the stress–strain relationship occurs when the material is isotropic and every coordinate axis is an axis of symmetry. Now we would expect that C11 = C22 = C33, C12 = C13 = C23, that C44 = C55 = C66, and that Lamina Stress–Strain Relationships 67 C44 again would not be independent from the other Cij. The isotropic stiffness matrix is of the form [1] C11 Cij = C12 C11 SYM 0 0 0 0 0 0 (C11 − C12 ) 2 0 C12 C12 C11 (C11 − C12 ) 2 0 (2.18) 0 C11 − C12 ) (C 2 0 0 0 Now, there are still 12 nonzero elastic constants, but only two are independent (Table 2.1). Similar equations based on the engineering constants will be derived in the next section. Equations of this form can be found in any mechanics of materials book, and the design of metallic components is usually based on such formulations. EXAMPLE 2.1 A representative volume element (RVE) from a iber-reinforced composite lamina is shown in Figure 2.6, along with the longitudinal stress and strain distributions across the iber and matrix materials in the section. The iber has a uniform longitudinal stress of 4000 psi (along the 1 direction) and a diameter of 0.0003 in., whereas the matrix has a uniform longitudinal stress of 1000 psi. A uniform longitudinal strain of 0.000423 in./in. acts over the entire section. The RVE has edge dimensions 0.0004 in. × 0.0004 in. in the 23 plane. Assume that the crosssectional dimensions of the section do not change along the longitudinal 4000 psi Fiber direction 0.000423 1000 psi Matrix Fiber 2 Matrix 1 3 Fiber Matrix Stress, σ1 Strain, ε1 FIGURE 2.6 Stress and strain distributions for calculation of effective modulus in Example 2.1. Principles of Composite Material Mechanics 68 direction, and use the concept of the effective modulus of an equivalent homogeneous material to ind the numerical value of the effective longitudinal modulus, E1 (or E11) of the composite. Solution The effective longitudinal modulus is given by E1 = σ1 ε1 where the average stress is σ1 = ∫ σ dV = ∫ σ dA = σ A + σ A A +A ∫ dV dA 1 1 f f f = m m m ( 4000)(π/4)(0.0003)2 + (1000)[(0.0004)2 − (π/4)(0.0003)2 ] = 2325 psi (0.0004)2 and the stresses and cross-sectional areas of the iber and matrix are denoted by the subscripts f and m, respectively. The average strain is ε1 = 0.000423, so the effective modulus is E1 = 2325 σ1 = = 5.496 (10 6 ) psi ε1 0.000423 EXAMPLE 2.2 If a specially orthotropic, transversely isotropic material is subjected to a pure shear strain γ23 = ε4, use the contracted notation to determine all of the resulting stresses associated with 1, 2, 3 axes. Solution Substituting the stiffness matrix for a specially orthotropic, transversely isotropic material from Equation 2.17 in the stress–strain relationships of the form {σ} = [C]{ε} in Equation 2.4 and solving for the stresses resulting from the shear strain γ23 = ε4, it is seen that σ23 = σ4 = C44ε4 = ((C22 − C23)/2)ε4 and all other stresses are equal to zero. PROBLEM 2.1 Using an example of static equilibrium of an element in pure two-dimensional (2D) shear stress, prove that the shear stresses are symmetric (i.e., prove that σij = σji when i ≠ j). Lamina Stress–Strain Relationships 69 x3 x3 0.0015 0.001 20 10 σ2 σ2 0.1 mm 1 mm 0.1 mm Stress, σ2 (MPa) Strain, ε2 FIGURE 2.7 Transverse stress and strain distribution over a section of lamina. PROBLEM 2.2 A representative section from a composite lamina is shown in Figure 2.7 along with the transverse stress and strain distributions across the iber and matrix materials in the section. The composite section is 1 × 1 mm square, and the diameter of each of the four ibers is 0.1 mm. Assuming that the dimensions of the section do not change along the longitudinal direction (perpendicular to the page), ind the numerical value of the effective transverse modulus for the section. PROBLEM 2.3 The stiffness matrix [C] for a specially orthotropic material associated with the principal material axes (1, 2, 3) is given in Equation 2.16. Prove that, when the material is specially orthotropic and transversely isotropic in the 2–3 planes (i.e., the properties are invariant to rotations about the 1 axis) the stiffness matrix [C] is given by Equation 2.17. Hint: to prove that C44 = (C22 − C23)/2, consider the stresses and strains acting on an element under pure shear stress σ23 and the corresponding stresses and strains acting on the same element, which has been rotated by a convenient angle in the 2–3 planes. 2.4 Orthotropic and Isotropic Engineering Constants In the previous section, symmetry conditions were shown to reduce the number of elastic constants (the Cij or Sij) in the stress–strain relationships for several important classes of materials and the general forms of the relationships were presented. When a material is characterized experimentally, however, the so-called “engineering constants” such as Young’s modulus (or modulus of elasticity), shear modulus, and Poisson’s ratio are usually measured instead of the Cij or the Sij. The engineering constants are also widely Principles of Composite Material Mechanics 70 used in analysis and design because they are easily deined and interpreted in terms of simple states of stress and strain. In this section, several simple tests and their resulting states of stress and strain will be used to develop the 3D and 2D stress–strain relationships for orthotropic and isotropic materials. Consider a simple uniaxial tensile test consisting of an applied longitudinal normal stress, σ1, along the reinforcement direction (i.e., the 1 direction) of a specimen from an orthotropic material, as shown in Figure 2.8a. It is assumed that all other stresses are equal to zero. Typical experimental stress–strain data from such a test on a carbon/epoxy composite are shown in Figure 2.9a from Reference 8, where both longitudinal strains ε1 and transverse Poisson strains ε2 are shown. More details on testing of composites will be provided in Chapter 10. Within the linear range the experimental observation is that the resulting strains associated with the 123 axes can be expressed empirically in terms of “engineering constants” as ε1 = σ1 E1 ε 2 = − ν12ε1 = − ε 3 = − ν13 ε1 = − ν12σ 1 E1 (2.19) ν13σ 1 E1 γ 12 = γ 23 = γ 13 = 0 where E1 = longitudinal modulus of elasticity associated with the 1 direction, and νij = −εj/εi is the Poisson’s ratio, the ratio of the strain in the j direction to the strain in the perpendicular i direction when the applied stress is in the i direction. Recall from mechanics of materials [2] that for isotropic materials, no subscripts are needed on properties such as the modulus of elasticity and Poisson’s ratio because the properties are the same in all directions. This is (a) σ1 (b) σ2 σ1 (c) τ12 σ2 τ12 FIGURE 2.8 Simple states of stress used to deine lamina engineering constants. (a) Applied longitudinal normal stress, (b) applied transverse normal stress, and (c) applied in-plane shear stress. Lamina Stress–Strain Relationships (b) Carbon/epoxy, [0]8 2000 –ε2 ε1 1500 1000 500 0 0 Carbon/epoxy, [90]16 60 Stress (σ2), MPa Stress (σ1), MPa (a) 71 50 40 30 20 10 0.2 0.4 0.6 0.8 1.0 1.2 1.4 1.6 Strain, % 0 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 Strain (ε2), % FIGURE 2.9 Typical stress–strain data from (a) longitudinal tensile test and (b) transverse tensile test of carbon/epoxy composite. (Reprinted from Adams, D. F., Carlsson, L. A., and Pipes, R. B. 2003. Experimental Characterization of Advanced Composite Materials, 3rd ed. CRC Press, Boca Raton, FL. With permission.) not the case with orthotropic materials, however, and subscripts are needed on these properties because of their directional nature. For example, E1 ≠ E2 and ν12 ≠ ν21. Note that, as with isotropic materials, a negative sign must be used in the deinition of the Poisson’s ratio. A property like ν12 is usually called a major Poisson’s ratio, whereas a property like ν21 is called a minor Poisson’s ratio. As with isotropic materials, a normal stress induces only normal strains, and all shear strains are equal to zero. This lack of shear/normal interaction is observed only for the principal material coordinate system, however. For any other set of coordinates, the so-called “shear-coupling” effect is present. This effect will be discussed in detail later. Now consider a similar experiment where a transverse normal stress, σ2, is applied to the same material as shown in Figure 2.8b, with all other stresses being equal to zero. Typical stress–strain data from such a test on a carbon/ epoxy composite are shown in Figure 2.9b from Reference 8. Now the experimental observation is that the resulting strains can be expressed as ε2 = σ2 E2 ε1 = − ν21ε 2 = − ν21σ 2 E2 (2.20) ν σ ε 3 = − ν23 ε 2 = − 23 2 E2 γ 12 = γ 23 = γ 13 = 0 where E2 is the transverse modulus of elasticity associated with the 2 direction. A similar result for an applied transverse normal stress, σ3, can be obtained by changing the appropriate subscripts in Equation 2.20. Principles of Composite Material Mechanics 72 Next, consider a shear test where a pure shear stress, σ12 = τ12, is applied to the material in the 12 plane, as shown in Figure 2.8c. Now the experimental observation is that the resulting strains can be written as γ 12 = τ12 G12 (2.21) ε1 = ε 2 = ε 3 = γ 13 = γ 23 = 0 where G12 is the shear modulus associated with the 12 plane. Similar results can be obtained for pure shear in the 13 and 23 planes by changing the appropriate subscripts in Equation 2.21. Again, notice that there is no shear/ normal interaction (or shear coupling). As before, however, this is only true for the principal material axes. Finally, consider a general 3D state of stress consisting of all possible normal and shear stresses associated with the 123 axes as shown in Figures 2.1 and 2.5. Since we are dealing with linear behavior, it is appropriate to use superposition and add all the resulting strains due to the simple uniaxial and shear tests, as given in Equations 2.19 through 2.21, and similar equations as described above. The resulting set of equations is given below: 1 E1 − ν12 ε1 E1 ε 2 − ν13 ε 3 E1 = γ 23 0 γ 31 γ 12 0 0 S11 S 21 S31 = 0 0 0 − ν21 E2 1 E2 − ν23 E2 − ν31 E3 − ν32 E3 1 E3 0 0 0 0 0 0 0 0 1 G23 0 0 0 0 1 G31 0 0 0 0 S12 S22 S32 0 0 0 S13 S23 S33 0 0 0 0 0 0 S44 0 0 0 0 0 0 S55 0 0 0 σ 1 σ 2 0 σ 3 τ 0 23 τ 31 0 τ12 1 G12 0 σ1 0 σ 2 0 σ 3 0 τ 23 0 τ 31 S66 τ12 (2.22) Lamina Stress–Strain Relationships 73 Note that the compliance matrix is of the same form as the stiffness matrix for a specially orthotropic material (Equation 2.16) as it should be because [S] = [C]−1. Note also that due to symmetry of the compliance matrix, Sij = Sji, νij/Ei = νji/Ej and only nine of the engineering constants are independent. If we now consider a simple uniaxial tensile test consisting of an applied normal stress, σx, along some arbitrary x axis as shown in Figure 2.4, we ind that the full complement of normal strains and shear strains are developed. The generation of shear strains due to normal stresses and normal strains due to shear stresses is often referred to as the “shear-coupling effect.” As a result of shear coupling, all the zeros disappear in the compliance matrix and it becomes fully populated for the general 3D state of stress associated with the arbitrary xyz axes; this is the generally orthotropic material. The stiffness or compliance matrices for the generally orthotropic material are of the same form as those for the generally anisotropic material (Equation 2.15), although the material still has its orthotropic symmetries with respect to the principal material axes. Obviously then, the experimental characterization of such a material is greatly simpliied by testing it as a specially orthotropic material along the principal material directions. As shown later, once we have the stiffnesses or compliances associated with the 123 axes, we can obtain those for an arbitrary off-axis coordinate system such as xyz by transformation equations involving the angles between the axes. If the material being tested is specially orthotropic and transversely isotropic as shown in Figure 2.5, the subscripts 2 and 3 in Equation 2.22 are interchangeable, and we have G13 = G12, E2 = E3, ν21 = ν31, and ν23 = ν32. In addition, the familiar relationship among the isotropic engineering constants [2] is now valid for the engineering constants associated with the 23 plane, so that G23 = E2 2(1 + ν32 ) (2.23) Now, the compliance matrix is of the same form as Equation 2.17 and only ive of the engineering constants are independent. Finally, for the isotropic material, there is no need for subscripts and G13 = G23 = G12 = G, E1 = E2 = E3 = E, ν12 = ν23 = ν13 = ν, and G = E/2(1 + ν). Now the compliance matrix is of the same form as Equation 2.18 and only two of the engineering constants are independent. 2.5 Specially Orthotropic Lamina As shown later in the analysis of laminates, the lamina is often assumed to be in a simple 2D state of stress (or plane stress). In this case, the specially Principles of Composite Material Mechanics 74 orthotropic stress–strain relationships in Equation 2.22 can be simpliied by letting σ3 = τ23 = τ31 = 0, so that ε1 S11 ε 2 = S21 γ 0 12 S12 S22 0 σ1 σ2 S66 τ12 0 0 (2.24) where the compliances Sij and the engineering constants are related by the equations S11 = 1 1 , S22 = , E1 E2 1 ν ν S12 = S21 = − 21 = − 12 , S66 = E2 E1 G12 (2.25) Thus, there are ive nonzero compliances and only four independent compliances for the specially orthotropic lamina (Table 2.1). The lamina stresses in terms of tensor strains are given by σ 1 Q11 σ 2 = Q21 τ 0 12 Q12 Q22 0 0 ε1 0 ε2 2Q66 γ 12 2 (2.26) where the Qij are the components of the lamina stiffness matrix, which are related to the compliances and the engineering constants by (see the discussion of matrix inversion in Appendix A) Q11 = S22 E1 = 2 1 − ν12 ν21 S11S22 − S12 Q12 = − S12 ν12E2 = = Q21 2 S11S22 − S12 1 − ν12 ν21 S11 E2 Q22 = = 2 1 − ν12 ν21 S11S22 − S12 Q66 = (2.27) 1 = G12 S66 Note that the factor of 2 has been introduced in the Q66 term of Equation 2.26 to compensate for the use of tensor shear strain ε12 = γ12/2. The reason Lamina Stress–Strain Relationships 75 TABLE 2.2 Typical Values of Lamina Engineering Constants for Several Composites Having Fiber Volume Fraction υf Material T300/934 carbon/epoxy AS/3501 carbon/epoxy P-100/ERL 1962 pitch/ carbon/epoxy IM7/8551-7 carbon/ toughened epoxy AS4/APC2 carbon/PEEK Boron/6061 boron/ aluminum Kevlar™ 49/934 aramid/ epoxy Scotchply™ 1002 E-glass/ epoxy Boron/5505 boron/epoxy Spectra™ 900/826 polyethylene/epoxy E-glass/470-36 E-glass/ vinylester E1 [Msi (GPa)] E2 [Msi (GPa)] G12 [Msi (GPa)] ν12 υf 19.0 (131) 20.0 (138) 68.0 (468.9) 1.5 (10.3) 1.3 (9.0) 0.9 (6.2) 1.0 (6.9) 1.0 (6.9) 0.81 (5.58) 0.22 0.3 0.31 0.65 0.65 0.62 23.5 (162) 1.21 (8.34) 0.3 (2.07) 0.34 0.6 19.1 (131) 34.1 (235) 1.26 (8.7) 19.9 (137) 0.73 (5.0) 6.8 (47.0) 0.28 0.3 0.58 0.5 11.0 (75.8) 0.8 (5.5) 0.33 (2.3) 0.34 0.65 5.6 (38.6) 1.2 (8.27) 0.6 (4.14) 0.26 0.45 29.6 (204.0) 4.45 (30.7) 2.68 (18.5) 0.51 (3.52) 0.81 (5.59) 0.21 (1.45) 0.23 0.32 0.5 0.65 3.54 (24.4) 1.0 (6.87) 0.42 (2.89) 0.32 0.30 Note: Kevlar™ is a registered trademark of DuPont Company, Wilmington, Delaware; Scotchply™ is a registered trademark of 3M Company, St. Paul, Minnesota; and Spectra™ is a registered trademark of Honeywell International, Inc. for this will become apparent in the next section. As shown later, the experimental characterization of the orthotropic lamina involves the measurement of four independent engineering constants such as E1, E2, G12, and ν12. Typical values of these properties for several composites are shown in Table 2.2. The balanced orthotropic lamina shown schematically in Figure 2.10 often occurs in practice when the iber reinforcement is woven or cross-plied at 0° and 90°. In this case, the number of independent elastic constants in FIGURE 2.10 Balanced orthotropic lamina consisting of ibers oriented at 0° and 90°. Principles of Composite Material Mechanics 76 Equations 2.24 through 2.27 is reduced to 3 because of the double symmetry of properties with respect to the 1 and 2 axes (Table 2.1). Thus, for the balanced orthotropic lamina, we have E1 = E2, Q11 = Q22, and S11 = S22. EXAMPLE 2.3 An orthotropic, transversely isotropic material is subjected to a 2D stress condition along the principal material axes 1, 2, 3 as shown in Figure 2.11 and the engineering constants for the material are as follows: E1 = 20 × 10 6 psi , G12 = 1 × 10 6 psi , E2 = 1.5 × 10 6 psi , ν12 = 0.3, ν23 = 0.2 Determine all strains associated with the 1, 2, 3 axes. Solution Due to symmetry of the compliance matrix in Equation 2.22 ν21 ν12 = E2 E1 and due to transverse isotropy, ν13 = ν12. Therefore, from Equation 2.22, the strains are ε1 = 10 × 10 3 0.3(20 × 10 3 ) σ 1 ν12 = 0.0002 − − σ2 = E1 E1 20 × 10 6 20 × 10 6 ε2 = − σ 0.3(10 × 10 3 ) 20 × 10 3 ν12 σ1 + 2 = − = 0.01318 + E1 E2 20 × 106 1.5 × 106 ε3 = − ν 0.3(10 × 10 3 ) 0.2(20 × 10 3 ) ν12 = −0.002816 − σ 1 − 23 σ 2 = − E1 E2 20 × 106 1.5 × 10 6 σ2 = 20,000 psi τ12 = 5000 psi 2 1 σ1 = 10,000 psi 3 Note: σ3 = τ13 = τ23 = 0 FIGURE 2.11 Stress condition for Example 2.3. Lamina Stress–Strain Relationships γ 12 = τ12 5 × 10 3 = 0.005 = G12 1 × 10 6 γ 31 = τ 31 =0 G31 γ 23 = τ 23 =0 G23 77 So even though the stress condition is 2D, the resulting strains are 3D due to the Poisson strain ε3. PROBLEM 2.4 A balanced orthotropic, or square symmetric lamina, is made up of 0° and 90° ibers woven into a fabric and bonded together, as shown in Figure 2.10. a. Describe the stress–strain relationships for such a lamina in terms of the appropriate engineering constants. b. For a typical glass/epoxy composite lamina of this type, sketch the expected variations of all the engineering constants for the lamina from 0° to 90°. Numerical values are not required. PROBLEM 2.5 Derive Equation 2.27. PROBLEM 2.6 Find all components of the stiffness and compliance matrices for a specially orthotropic lamina made of AS/3501 carbon/epoxy. PROBLEM 2.7 For a specially orthotropic, transversely isotropic material the “plane strain bulk modulus,” K 23, is an engineering constant that is deined by the stress conditions σ2 = σ3 = σ and the strain conditions ε1 = 0, ε2 = ε3 = ε. Show that these conditions lead to the stress–strain relationship σ = 2K 23 ε, and ind the relationship among K 23, E1, E2, G23, and ν12. PROBLEM 2.8 Describe the measurements that would have to be taken and the equations that would have to be used to determine G23, ν32, and E2 for a specially orthotropic, transversely isotropic material from a single tensile test. Principles of Composite Material Mechanics 78 2.6 Generally Orthotropic Lamina In the analysis of laminates having multiple laminae, it is often necessary to know the stress–strain relationships for the generally orthotropic lamina in non principal coordinates (or “off-axis” coordinates) such as x and y in Figure 2.5. Fortunately, the elastic constants in these so-called “off-axis” stress–strain relationships are related to the four independent elastic constants in the principal material coordinates and the lamina orientation angle. The sign convention for the lamina orientation angle, θ, is given in Figure 2.12. The relationships are found by combining the equations for transformation of stress and strain components from the 12 axes to the xy axes. Relationships for transformation of stress components between coordinate axes may be obtained by writing the equations of static equilibrium for the wedge-shaped differential element in Figure 2.13. For example, the force equilibrium along the x direction is given by ∑ F = σ dA − σ dA cos θ − σ dA sin θ + 2τ x 1 x 2 2 2 12 dA sin θ cos θ = 0 (2.28) which, after dividing through by dA, gives an equation relating σx to the stresses in the 12 system: σ x = σ 1 cos 2 θ + σ 2 sin 2 θ − 2τ12 sin θ cos θ (2.29) Using a similar approach, the complete set of transformation equations for the stresses in the xy-coordinate system can be developed and written in matrix form as σ x c2 2 σ y = s τ cs xy 2 −2cs σ 1 σ1 −1 2cs σ 2 = [T ] σ 2 τ c 2 − s2 τ12 12 s2 c2 −cs y y (2.30) 2 1 +θ x –θ x 1 Positive θ FIGURE 2.12 Sign convention for lamina orientation. Negative θ Lamina Stress–Strain Relationships 79 σ 2 dA sin θ τ12 dA sin θ 2 τxy dA y 1 σ1 dA cos θ σx dA θ θ x τ12 dA cos θ dA FIGURE 2.13 Differential element under static equilibrium with forces in two coordinate systems. and the stresses in the 12 system can be written as σx σ1 σ 2 = [T ] σ y τ τ 12 xy (2.31) where c = cos θ , s = sin θ, and the transformation matrix, [T], is deined as c2 [T ] = s2 −cs s2 c2 cs 2cs −2cs c 2 − s2 (2.32) A procedure for determining the matrix inverse [T]−1 is described in Appendix A. It can also be shown [2,3] that the tensor strains transform the same way as the stresses, and that εx ε1 ε 2 = [T ] ε y γ γ 12 xy 2 2 (2.33) Substituting Equation 2.33 into Equation 2.26, and then substituting the resulting equations into Equation 2.30, we ind that Principles of Composite Material Mechanics 80 εx σx −1 * σ y = [T ] [Q ][T ] ε y γ τ xy xy 2 (2.34) where the components of the stiffness matrix [Q*] in Equation 2.34 are * deined as Qij* = Qij for all ij except Q66 = 2Q66 as shown in Equation 2.26. Carrying out the indicated matrix multiplications and converting back to engineering strains, we ind that σ x Q11 σ y = Q12 τ Q xy 16 Q12 Q22 Q26 Q16 ε x Q26 ε y Q66 γ xy (2.35) where the Qij are the components of the transformed lamina stiffness matrix, which are deined as follows: Q11 = Q11c 4 + Q22s 4 + 2(Q12 + 2Q66 )s2c 2 Q12 = (Q11 + Q22 − 4Q66 )s2c 2 + Q12 (cc 4 + s 4 ) Q22 = Q11s 4 + Q22c 4 + 2(Q12 + 2Q66 )s2c 2 Q16 = (Q11 − Q12 − 2Q66 )c 3 s − (Q22 − Q12 − 2Q66 )cs3 (2.36) Q26 = (Q11 − Q12 − 2Q66 )cs3 − (Q22 − Q12 − 2Q66 )c 3 s Q66 = (Q11 + Q22 − 2Q12 − 2Q66 )s2c 2 + Q66 (s 4 + c 4 ) Although the transformed lamina stiffness matrix now has the same form as that of an anisotropic material with nine nonzero coeficients, only four of the coeficients are independent because they can all be expressed in terms of the four independent lamina stiffnesses of the specially orthotropic material. That is, the material is still orthotropic, but it is not recognizable as such in the off-axis coordinates. As in the 3D case, it is obviously much easier to characterize the lamina experimentally in the principal material coordinates than in the off-axis coordinates. Recall that the engineering constants, the properties that are normally measured, are related to the lamina stiffnesses by Equation 2.27. Lamina Stress–Strain Relationships 81 Alternatively, the strains can be expressed in terms of the stresses as ε x S11 ε y = S12 γ S xy 16 S12 S22 S26 S16 σ x S26 σ y S66 τ xy (2.37) where the Sij are the components of the transformed lamina compliance matrix that are deined by [S ] = [Q]−1 , or in expanded form S11 = S11c 4 + (2S12 + S66 )s2c 2 + S22s 4 S12 = S12 (s 4 + c 4 ) + (S11 + S22 − S66 )ss2c 2 S22 = S11s 4 + (2S12 + S66 )s2c 2 + S22c 4 S16 = (2S11 − 2S12 − S66 )sc 3 − (2S22 − 2S12 − S66 )s3c (2.38) S26 = (2S11 − 2S12 − S66 )s3c − (2S22 − 2S12 − S66 )sc 3 S66 = 2(2S11 + 2S22 − 4S12 − S66 )s2c 2 + S66 (s 4 + c 4 ) The lamina engineering constants can also be transformed from the principal material axes to the off-axis coordinates. For example, the off-axis longitudinal modulus of elasticity associated with uniaxial loading along the x direction as shown in Figure 2.14 is deined as Ex = σx σx 1 = = ε x S11σ x S11 (2.39) where the strain εx in the denominator has been found by substituting the stress conditions σx ≠ 0, σy = τxy = 0 in Equation 2.37. y 1 2 σx θ x FIGURE 2.14 Off-axis loading for determination of off-axis longitudinal modulus of elasticity Ex. 82 Principles of Composite Material Mechanics By substituting S11 from the irst of Equation 2.38 into Equation 2.39 and then using Equation 2.25, we get the irst of Equation 2.40: 1 2ν 1 1 Ex = c 4 + − 12 s2c 2 + s 4 G12 E1 E2 E1 −1 1 2ν 1 1 Ey = s 4 + − 12 s2c 2 + c 4 G12 E1 E2 E1 −1 1 4 4 1 2 ν12 1 2 2 1 Gxy = sc (s + c ) + 4 + − + E1 E2 E1 2G12 G12 −1 (2.40) ν 1 1 2 2 1 νxy = Ex 12 (s 4 + c 4 ) − + sc − E1 E2 G12 E1 where c = cos θ and s = sin θ as before. The rest of Equation 2.40 for the offaxis transverse modulus Ey, the off-axis shear modulus Gxy, and the off-axis major Poisson’s ratio νxy can be obtained from similar derivations. The variation of these properties with lamina orientation for several composites is shown graphically in Figure 2.15 from Reference 9. As intuitively expected, Ex varies from a maximum at θ = 0° to a minimum at θ = 90° for this particular material. It is not necessarily true that the extreme values of such material properties occur along the principal material directions, however [6]. What may not be intuitively expected is the sharp drop in the offaxis modulus Ex as the angle changes slightly from 0° and the fact that over much of the range of lamina orientations the modulus Ex is very low. This is why transverse reinforcement is needed in unidirectional iber composites, which are subjected to multiaxial loading. The maximum value of the off-axis shear modulus Gxy at θ = 45° and minimum values of Gxy at θ = 0° and θ = 90° indicate that off-axis reinforcement is also essential for good shear stiffness in unidirectional composites. A good analogy here is the effect of diagonal bracing in a truss structure—without such bracing, the structure would be much more susceptible to collapse under shear loading. For ilament-wound composite power transmission shafts under torsional loading, off-axis reinforcement is required for acceptable shear stiffness. Later in Chapter 7, it will become clear that off-axis laminae are essential in the design of laminates, which are subjected to shear loading. The shear-coupling effect has been described previously as the generation of shear strains by off-axis normal stresses and the generation of normal strains by off-axis shear stresses. One way to quantify the degree of shear coupling is by deining dimensionless shear-coupling ratios [4,5] or mutual inluence coeficients [10] or shear-coupling coeficients [11]. For example, when the state of stress is deined as σx ≠ 0, σy = τxy = 0, the ratio Lamina Stress–Strain Relationships 83 1.4 14 Carbon/epoxy Boron/aluminum Glass/epoxy 12 1.2 1 10 Ex E2 G xy 8 E2 0.8 6 0.6 4 0.4 2 0.2 0 Carbon/epoxy Boron/aluminum Glass/epoxy 0 10 20 30 40 50 60 70 80 90 θ° 0.6 0 1 Carbon/epoxy Boron/aluminum Glass/epoxy 0.5 0.5 0.4 0 νxy 0.3 ηx,xy –0.5 0.2 –1 0.1 –1.5 0 0 10 20 30 40 50 60 70 80 90 θ° 0 10 20 30 40 50 60 70 80 90 θ° –2 Carbon/epoxy Boron/aluminum Glass/epoxy 0 10 20 30 40 50 60 70 80 90 θ° FIGURE 2.15 Variations of off-axis engineering constants with lamina orientation for unidirectional carbon/ epoxy, boron/aluminum, and glass/epoxy composites. (From Sun, C. T. Mechanics of Aircraft Structures. 1998. Copyright Wiley-VCH Verlag GmbH & Co. KGaA. New York, NY. Reproduced with permission.) ηx , xy = 2 2 ν γ xy S16 1 3 2 2 ν12 1 3 sc − + = = Ex + 12 − sc − E2 S11 E1 G12 E1 εx G12 E1 (2.41) is a measure of the amount of shear strain generated in the xy plane per unit normal strain along the direction of the applied normal stress, σx. Thus, the shear-coupling ratio is analogous to the Poisson’s ratio, which is a measure of the coupling between normal strains. As shown in Figure 2.15, ηx,xy strongly depends on orientation and has its maximum value at some intermediate angle, which depends on the material. Since there is no coupling along principal material directions, ηx,xy = 0 for θ = 0° and θ = 90°. As the shear-coupling Principles of Composite Material Mechanics 84 ratio increases, the amount of shear coupling increases. Other shear-coupling ratios can be deined for different states of stress. For example, when the stresses are τxy ≠ 0, σx = σy = 0, the ratio ηxy , y = 2 2 ν εy S 1 3 1 3 2 2 ν12 = 26 = Gxy + 12 − s c − E + E − G sc E E G γ xy S66 1 12 2 1 12 1 (2.42) characterizes the normal strain response along the y direction due to a shear stress in the xy plane. Finally, for a generally orthotropic lamina under plane stress, the stress– strain relationship for the normal strain εx in terms of off-axis engineering constants can be expressed as εx = ν yx ηxy , x 1 σx − σy + τ xy Ex Ey Gxy (2.43) with similar relationships for εy and γxy. As with the specially orthotropic case and the general anisotropic case, the stiffness and compliance matrices are still symmetric. So, for example, the off-axis compliances S12 = S21 , or in terms of off-axis engineering constants, (νyx/Ey) = (νxy/Ex). The effects of lamina orientation on stiffness are dificult to assess from a quick inspection of stiffness transformation equations such as Equations 2.36 and 2.40. In addition, the eventual incorporation of lamina stiffnesses into laminate analysis requires integration of lamina stiffnesses over the laminate thickness, and integration of such complicated equations is also dificult. In view of these dificulties, a more convenient “invariant” form of the lamina stiffness transformation equations has been proposed by Tsai and Pagano [12]. By using trigonometric identities to convert from power functions to multiple angle functions and then using additional mathematical manipulations, Tsai and Pagano showed that Equation 2.36 could also be written as Q11 = U1 + U 2 cos 2θ + U 3 cos 4θ Q12 = U 4 − U 3 cos 4θ Q22 = U1 − U 2 cos 2θ + U 3 cos 4θ Q16 = U2 sin 2θ + U 3 sin 4θ 2 Q26 = U2 sin 2θ − U 3 sin 4θ 2 Q66 = 1 (U1 − U 4 ) − U 3 cos 4θ 2 (2.44) Lamina Stress–Strain Relationships 85 where the set of “invariants” is deined as 1 (3Q11 + 3Q22 + 2Q12 + 4Q66 ) 8 1 U 2 = (Q11 − Q22 ) 2 1 U 3 = (Q11 + Q22 − 2Q12 − 4Q66 ) 8 1 U 4 = (Q11 + Q22 + 6Q12 − 4Q66 ) 8 U1 = (2.45) As the name implies, the invariants, which are simply linear combinations of the Qij, are invariant to rotations in the plane of the lamina. Note that there are four independent invariants, just as there are four independent elastic constants. Equation 2.44 is obviously easier to manipulate and interpret than Equation 2.36. For example, all the stiffness expressions except those for the coupling stiffnesses consist of one constant term and terms that vary with lamina orientation. Thus, the effects of lamina orientation on stiffness are easier to interpret. Invariant formulations of lamina compliance transformations are also useful. It can be shown [5,11] that the off-axis compliance components in Equation 2.37 can be written as S11 = V1 + V2 cos 2θ + V3 cos 4θ S12 = V4 − V3 cos 4θ S22 = V1 − V2 cos 2θ + V3 cos 4θ (2.46) S16 = V2 sin 2θ + 2V3 sin 4θ S26 = V2 sin 2θ − 2V3 sin 4θ S66 = 2(V1 − V4 ) − 4V3 cos 4θ where the invariants are V1 = 1 (3S11 + 3S22 + 2S12 + S66 ) 8 V2 = 1 (S11 − S22 ) 2 1 V3 = (S11 + S22 − 2S12 − S66 ) 8 V4 = 1 (S11 + S22 + 6S12 − S66 ) 8 (2.47) Principles of Composite Material Mechanics 86 Invariant formulations also lend themselves well to graphical interpretation. As shown in any mechanics of materials book [2], stress transformation equations such as Equation 2.30 can be combined and manipulated so as to generate the equation of Mohr’s circle. As shown in Figure 2.16, the transformation of a normal stress component σx can be described by the invariant formulation σ x = I1 + I 2 cos 2θ p (2.48) where I1 = σx + σy = invariant 2 2 σx − σy 2 I2 = + τ xy = invariant 2 θ p = angle between the x axis and the principal stress axis In this case, the invariants are I1, which deines the position of the center of the circle, and I2, which is the radius of the circle. Note the similarity between Equation 2.48 and the irst of Equation 2.44 in that the invariant formulation typically consists of a constant term and a term or terms that vary with orientation. Similarly, the invariant forms of the stiffness transformations can also be interpreted graphically using Mohr’s circles. For example, Tsai and Hahn [11] have shown that the stiffness transformation equation Q11 = U1 + U 2 cos 2θ + U 3 cos 4θ (2.49) σx τ τxy 2θp σ I1 FIGURE 2.16 Mohr’s circle for stress transformation. I2 Lamina Stress–Strain Relationships 87 Q11 U4 2θ 4θ U3 U2 U1 Q11 FIGURE 2.17 Mohr’s circles for stiffness transformation. (From Tsai, S. W. and Hahn, H. T. 1980. Introduction to Composite Materials. Technomic Publishing Co., Lancaster, PA. Reprinted by permission of Technomic Publishing Co.) can be represented graphically by using two Mohr’s circles, as shown in Figure 2.17. The distance between points on each of the two circles represents the total stiffness Q11 , whereas the distance between the centers of the two circles is given by U1. The radius and angle associated with one circle are U2 and 2θ, respectively, and the radius and angle associated with the other circle are U3 and 4θ, respectively. Thus, the distance between the centers of the circles is a measure of the isotropic component of stiffness, whereas the radii of the circles indicate the strength of the orthotropic component. If U2 = U3 = 0, the circles collapse to points and the material is isotropic. Invariants will prove to be very useful later in the analysis of randomly oriented short iber composites and laminated plates. For additional applications of invariants in composite analysis, the reader is referred to books by Halpin [5] and Tsai and Hahn [11]. EXAMPLE 2.4 A 45° off-axis tensile test is conducted on a generally orthotropic test specimen by applying a normal stress σx as shown in Figure 2.18. The specimen has strain gages attached so as to measure the normal strains εx and εy along the x and y directions, respectively. How many engineering constants for this material can be determined from the measured parameters σx, εx, and εy? Solution The off-axis modulus of elasticity along the x direction is determined from Ex = σx εx Principles of Composite Material Mechanics 88 45° off-axis tensile test specimen y 2 1 σx 45° x Strain gage for measuring εy Strain gage for measuring εx FIGURE 2.18 Strain-gaged specimen for a 45° off-axis tensile test. The off-axis major Poisson’s ratio is given by νxy = − εy εx Although it may not seem obvious, the in-plane shear modulus G12 may also be found from these measurements by using the appropriate transformations of stress and strain. Using θ = 45° in Equation 2.33, the shear strain γ12 is found from γ xy γ 12 = − cos 45° sin 45°ε x + cos 45° sin 45°ε y + (cos 2 45° − sin 2 45°) 2 2 or γ 12 = − ε x + ε y Note that the γxy term drops out of the above equation only when θ = 45°. For any other value of θ, we would need to know γxy as well as εx and εy in order to ind γ12 from this transformation equation. Likewise, the shear stress τ12 is found by substituting the tensile test conditions σx ≠ 0, σy = τxy = 0 in Equation 2.31: τ12 = − cos 45° sin 45°σ x = − σx 2 Finally, the shear modulus G12 may now be calculated from the third line of Equation 2.24 as G12 = 1 τ = 12 S66 γ 12 Note that this equation holds even though the stresses σ1 ≠ 0 and σ2 ≠ 0 in the irst two lines of Equation 2.24. Lamina Stress–Strain Relationships EXAMPLE 2.5 A ilament-wound cylindrical pressure vessel (Figure 2.19) of mean diameter d = 1 m and wall thickness t = 20 mm is subjected to an internal pressure, p. The ilament-winding angle θ = 53.1° from the longitudinal axis of the pressure vessel, and the glass/epoxy material has the following properties: E1 = 40 GPa = 40(103) MPa, E2 = 10 GPa, G12 = 3.5 GPa, and ν12 = 0.25. By the use of a strain gage, the normal strain along the iber direction is determined to be ε1 = 0.001. Determine the internal pressure in the vessel. Solution From mechanics of materials, the stresses in a thin-walled cylindrical pressure vessel are given by σx = pr 0.5 p = = 12.5 p, τ xy = 0 2t 2(0.02) σy = pr 0.5 p = = 25 p t 0.02 (Note that r = d/2 = 0.5 m.) These equations are based on static equilibrium and geometry only. Thus, they apply to a vessel made of any material. Since the given strain is along the iber direction, we must transform the above stresses to the 12 axes. Recall that in the “netting analysis” in Problems 1.10 and 1.11 of Chapter 1, only the iber longitudinal normal stress was considered. This was because the matrix was ignored, and the ibers alone cannot support transverse or shear stresses. In the current problem, however, the transverse normal stress, σ2, and the shear stress, τ12, are also considered because the iber and matrix are now assumed to act as a composite. From Equation 2.31, the stresses along the 12 axes are σ 1 = σ x cos 2 θ + σ y sin 2 θ + 2τ xy sin θ cos θ = (12.5 p)(0.6)2 + (25 p)(0.8)2 + 0 = 20.5 p(MPa) σ 2 = σ x sin 2 θ + σ y cos 2 θ − 2τ xy sin θ cos θ = (12.5 p)(0.8)2 + (25 p)(0.6)2 − 0 = 17.0 p(MPa) τ12 = −σ x sin θ cos θ + σ y sin θ cos θ + τ xy (cos 2 θ − sin 2 θ) = −(12.5 p)(0.8)(0.6) + (25 p)(0.6)(0.8) + 0 = 6.0 p(MPa) where the pressure p is in MPa. From the irst of Equation 2.24, the normal strain ε1 is ε1 = 20.5 p 0.25(17.0 p) σ 1 ν12σ 2 − = − = 0.001 E1 E1 40(10 3 ) 40(10 3 ) and the resulting pressure is p = 2.46 MPa. 89 Principles of Composite Material Mechanics 90 y 2 1 θ x FIGURE 2.19 Filament-wound vessel. EXAMPLE 2.6 A tensile test specimen is cut out along the x direction of the pressure vessel described in Example 2.5. What effective modulus of elasticity would you expect to get during a test of this specimen? Solution The off-axis modulus of elasticity, Ex, associated with the x direction is given by the irst of Equation 2.40 with θ = 53.1°. Ex = 1 (1/E1 )c 4 + [−(2 ν12 /E1 ) + 1/G12 ]c 2 s2 + (1/E2 )s 4 Ex = 1 (1/40)(0.6)4 + [−(2(0.25)/40) + (1/3.5)](0.6)2 (0.8)2 + (1/10)(0.8)4 = 9.33 GP Pa EXAMPLE 2.7 A lamina consisting of continuous ibers randomly oriented in the plane of the lamina is said to be “planar isotropic,” and the elastic properties in the plane are isotropic in nature. Find expressions for the lamina stiffnesses for a planar isotropic lamina. Solution Since the ibers are assumed to be randomly oriented in the plane, the “planar isotropic stiffnesses” can be found by averaging the transformed lamina stiffnesses as follows: Qɶ ij = ∫ π Qij dθ 0 ∫ π dθ 0 where the superscript (~) denotes an averaged property. Lamina Stress–Strain Relationships 91 It is convenient to use the invariant forms of the transformed lamina stiffnesses because they are easily integrated. For example, if we substitute the irst of Equation 2.44 in the above equation, we get Qɶ 11 ∫ = π Q11 dθ 0 ∫ π π ∫ [U + U cos 2θ + U cos 4θ]dθ = U = 1 2 3 0 dθ π 1 0 Note that the averaged stiffness equals the isotropic part of the transformed lamina stiffness, and that the orthotropic parts drop out in the averaging process. Similarly, the other averaged stiffnesses can be found in terms of the invariants. The derivations of the remaining expressions are left as an exercise. PROBLEM 2.9 Derive the irst of Equation 2.40 for the off-axis modulus, Ex. PROBLEM 2.10 Derive the third of Equation 2.40 for the off-axis shear modulus, Gxy. PROBLEM 2.11 Using the result from Problem 2.10 a. Find the value of the angle θ (other than 0° or 90°), where the curve of Gxy versus θ has a possible maximum, minimum, or inlection point. b. For the value of θ found in part (a), ind the bounds on G12, which must be satisied if Gxy is to have a maximum or minimum. c. Qualitatively sketch the variation of Gxy versus θ for the different cases and identify each curve by the corresponding bounds on G12, which give that curve. d. Using the bounds on G12 from part (b), ind which conditions apply for E-glass/epoxy composites. The bounds on G12 in part (b) should be expressed in terms of E1, E2, and ν12. PROBLEM 2.12 Describe a series of tensile tests that could be used to measure the four independent engineering constants for an orthotropic lamina without using a pure shear test. Give the necessary equations for the data reduction. Principles of Composite Material Mechanics 92 PROBLEM 2.13 An element of a balanced orthotropic carbon/epoxy lamina is under the state of stress shown in Figure 2.20. If the properties of the woven carbon fabric/ epoxy material are E1 = 70 GPa, ν12 = 0.25, and G12 = 5 GPa, determine all the strains along the iber directions. PROBLEM 2.14 Express the stress–strain relationships in Equation 2.37 in terms of offaxis engineering constants such as the moduli of elasticity, shear modulus, Poisson’s ratios, and shear-coupling ratios. PROBLEM 2.15 Derive the irst two equations of Equation 2.44. PROBLEM 2.16 Using the results of Problem 2.6, determine the invariants Ui and Vi for the AS/3501 lamina, where i = 1, 2, 3, 4. PROBLEM 2.17 Using the results of Problem 2.6 or Problem 2.16, compare the transformed lamina stiffnesses for AS/3501 carbon/epoxy plies oriented at +45° and −45°. 50 MPa 50 MPa 100 MPa 2 y 1 30° x FIGURE 2.20 Stresses acting on an element of balanced orthotropic lamina. Lamina Stress–Strain Relationships 93 PROBLEM 2.18 Show how the Mohr’s circles in Figure 2.17 can be used to interpret the transformed lamina stiffness Q12 . PROBLEM 2.19 Using the approach described in Example 2.6, derive the expressions for all the averaged stiffnesses for the planar isotropic lamina in terms of invariants. Use these results to ind the corresponding averaged engineering constants (modulus of elasticity, shear modulus, and Poisson’s ratio) in terms of invariants. PROBLEM 2.20 A 45° off-axis tensile test specimen has three strain gages attached. Two of the gages are mounted as shown in Figure 2.18 so as to measure the normal strains εx and εy, and a third gage is mounted at θ = 45° so as to measure the normal strain ε1. If the applied stress σx = 100 MPa and the measured strains are εx = 0.00647, εy = −0.00324, and ε1 = 0.00809, determine the off-axis modulus of elasticity Ex, the off-axis major Poisson’s ratio νxy, and the shearcoupling ratio ηx,xy. PROBLEM 2.21 A off-axis tensile test (Figure 2.14) of a unidirectional AS/3501 carbon/epoxy specimen is conducted with θ = 45° and the applied stress is found to be σx = 15.44 MPa. Determine the resulting strain εx. PROBLEM 2.22 An element of an orthotropic lamina is subjected to an off-axis shear stress τxy at an angle θ as shown in Figure 2.21. (a) For an angle θ = 45°, determine the value of the applied shear stress τxy that would generate the following stresses along the 1,2 axes: σ1 = 1000 MPa, σ2 = −1000 MPa, and τ12 = 0. τxy (MPa) y τxy (MPa) 2 1 θ x FIGURE 2.21 Description of off-axis lamina and stresses for Problem 2.22. 94 Principles of Composite Material Mechanics (b) Assuming that the lamina described in part (a) is made from T300/934 carbon/epoxy and that the stresses are also given in part (a), determine the strains along the 1,2 axes. PROBLEM 2.23 Use invariants to ind the optimum lamina orientation for maximizing the shear stiffness Q66 , then ind the corresponding maximum shear stiffness in terms of invariants. References 1. Christensen, R. M. 1979. Mechanics of Composite Materials. John Wiley & Sons, New York, NY. 2. Crandall, S. H., Dahl, N. C., and Lardner, T. J. 1978. An Introduction to the Mechanics of Solids, 2nd ed. with SI units. McGraw-Hill, Inc., New York, NY. 3. Sokolnikoff, I. S. 1956. Mathematical Theory of Elasticity. McGraw-Hill, Inc., New York, NY. 4. Ashton, J. E., Halpin, J. C., and Petit, P. H. 1969. Primer on Composite Materials: Analysis. Technomic Publishing Co., Lancaster, PA. 5. Halpin, J. C. 1984. Primer on Composite Materials: Analysis, rev. ed. Technomic Publishing Co., Lancaster, PA. 6. Jones, R. M. 1999. Mechanics of Composite Materials, 2nd ed. Taylor and Francis, Inc., Philadelphia, PA. 7. Vinson, J. R. and Sierakowski, R. L. 1986. The Behavior of Structures Composed of Composite Materials. Martinus Nijhoff Publishers, Dordrecht, The Netherlands. 8. Adams, D. F., Carlsson, L. A., and Pipes, R. B. 2003. Experimental Characterization of Advanced Composite Materials, 3rd ed. CRC Press, Boca Raton, FL. 9. Sun, C. T. 1998. Mechanics of Aircraft Structures. John Wiley & Sons, New York, NY. 10. Lekhnitski, S. G. 1981. Theory of Elasticity of an Anisotropic Body. Mir Publishing Co., Moscow, USSR. 11. Tsai, S. W. and Hahn, H. T. 1980. Introduction to Composite Materials. Technomic Publishing Co., Lancaster, PA. 12. Tsai, S. W. and Pagano, N. J. 1968. Invariant properties of composite materials. In Tsai, S. W., Halpin, J. C., and Pagano N. J., eds., Composite Materials Workshop, pp. 233–253. Technomic Publishing Co., Lancaster, PA. 3 Effective Moduli of a Continuous Fiber-Reinforced Lamina 3.1 Introduction In the previous chapter, the concept of an effective modulus was found to be essential to the development of practical engineering stress–strain relationships for composite materials. Recall that for some representative volume element (RVE) in a heterogeneous composite, the volume-averaged stresses can be related to the volume-averaged strains by the effective moduli of an equivalent homogeneous material. Chapter 2 was primarily concerned with the development and manipulation of macromechanical stress–strain relationships involving the lamina effective moduli, however, and the roles of lamina constituent materials were not examined in detail. In this chapter, we will discuss various micromechanical models for predicting the effective moduli of continuous iber-reinforced laminae in terms of the corresponding material properties, relative volume contents, and geometric arrangements of the iber and matrix materials. Corresponding models for predicting strength and hygrothermal properties will be presented in Chapters 4 and 5, respectively. Micromechanics of discontinuously reinforced composites, including nanocomposites, are covered in Chapter 6. Before proceeding further, it is appropriate to briely discuss the term “micromechanics.” To a materials scientist, the term may imply the study of mechanical behavior at the level of molecular or crystal structures. Since the behavior of composite material structures such as laminates is referred to as “macromechanics,” it has been suggested that, perhaps, mechanics of composites at the constituent material level should be referred to as “minimechanics” [1]. In the present context, and in much of the composites literature, however, the analysis of effective composite properties in terms of constituent material properties is called “micromechanics.” The terms “structure– property relationships” and “effective modulus theories” are also used in the literature. Many analytical approaches have been developed over the years, and comprehensive literature surveys have been published by Chamis and Sendeckyj [2], Christensen [3], Hashin [1], and Halpin [4]. 95 96 Principles of Composite Material Mechanics Micromechanical analyses are based on either the mechanics of materials or the elasticity theory. In the mechanics of materials approach, simplifying assumptions make it unnecessary to specify the details of the stress and strain distributions at the micromechanical level, and iber-packing geometry is generally arbitrary. The theory of elasticity models involve the solution for actual stresses and strains at the micromechanical level, and iber-packing geometry is taken into account. The elasticity approach often involves numerical solutions of the governing equations because of the complex geometries and boundary conditions. Although the simplifying assumptions used in the mechanics of materials approach violate some of the laws of elasticity theory, some of the results are suficiently accurate that they are often used in design. A third category involves empirical solutions that are based on curve-itting to elasticity solutions or experimental data, and some of these equations are often used along with the mechanics of materials equations to formulate a complete set of simple lamina design equations. Ideally, micromechanical models should enable us to answer quickly “What if?” questions regarding the effects of various iber/matrix combinations without actually fabricating and testing the composites in question. On the other hand, experience has shown that there are pitfalls in such an approach and that there is no substitute for experimental characterization. Experimental data on the constituent material properties are required as input to the models, and similar data on the corresponding composite properties are required to assess the validity of the models. Indeed, as we will see later, some properties such as iber transverse moduli are usually inferred from the micromechanical model and other measured properties because of the dificulty of direct measurement. Once a micromechanical model has been shown to be suficiently accurate by comparison with experiment, however, it can become part of a powerful design methodology that enables us to design the material as well as the structure. Aside from design implications, micromechanical analysis and experimental characterization are both essential if we are to understand better “how composites work.” One of the key elements in micromechanical analysis is the characterization of the relative volume or weight contents of the various constituent materials. We will ind that the micromechanics equations involve constituent volume fractions, but actual measurements are often based on weight fractions. Measurements are discussed later, but the relationships between volume fractions and weight fractions will be presented here. For any number of constituent materials, n, the sum of the constituent volume fractions must be unity: n ∑υ = 1 i i =1 (3.1) Effective Moduli of a Continuous Fiber-Reinforced Lamina 97 where υi = Vi/Vc = volume fraction of the ith constituent, Vi = volume of the ith constituent, and Vc = total volume of the composite. In many cases, this equation reduces to υf + υm + υ v = 1 (3.2) where υf, υm, and υv are the volume fractions of the iber, matrix, and voids, respectively. The corresponding equations for weight fractions are n ∑w = 1 (3.3) wf + wm =1 (3.4) i i =1 and where wi = Wi/Wc, wf = Wf/Wc, wm = Wm /Wc, and Wi, Wf, Wm, and Wc are the weights of the ith constituent, iber, matrix, and composite, respectively. Note that the weight of the voids has been neglected here. Substituting the product of density and volume for weight in each term of Equations 3.3 and 3.4 and solving for the composite density, we get the “rule of mixtures”: n ρc = ∑ρ υ i i (3.5) i =1 or ρc = ρf υf + ρm υm (3.6) where ρi, ρf, ρm, and ρc are the densities of the ith constituent, iber, matrix, and composite, respectively. Similarly, Equations 3.1 and 3.2 can be rearranged as ρc = 1 ∑ n (wi /ρi ) (3.7) i =1 and ρc = 1 (wf /ρf ) + (wm /ρm ) (3.8) Principles of Composite Material Mechanics 98 Equation 3.2 can also be rearranged so that the void fraction can be calculated from measured weights and densities: υv = 1 − (Wf /ρf ) + (Wc − Wf )/ρm Wc /ρc (3.9) Typical autoclave-cured composites may have void fractions in the range 0.1%–1%. Without vacuum bagging, however, volatiles trapped in the composite during the cure cycle can cause void contents of the order of 5%. Since micromechanics equations are typically expressed in terms of volume fractions, but measurements are usually based on weight fractions, it is useful to know the relationships between these two parameters. For example, the iber weight fraction is related to the iber volume fraction by wf = Wf ρfVf ρf = = υf Wc ρcVc ρc (3.10) ρc wf ρf (3.11) So that υf = Similarly, the matrix weight fractions and volume fractions are related by wm = Wm ρmVm ρm = = υm Wc ρcVc ρc (3.12) ρc wm ρm (3.13) and υm = In order to get some idea as to the range of constituent volume fractions that may be expected in iber composites, it is useful to consider representative area elements for idealized iber-packing geometries such as the square and triangular arrays shown in Figure 3.1. It is assumed that ibers are oriented perpendicular to the page, that the iber center-to-center spacing, s, and the iber diameter, d, do not change along the iber length, and that the area fractions are equal to the volume fractions. Indeed, measurement of such area fractions is possible from photomicrographs and image analysis software. The iber volume fraction for the square array is found by dividing the area of iber enclosed in the shaded square by the total area of the shaded square [5]: Effective Moduli of a Continuous Fiber-Reinforced Lamina 99 Fiber Fiber s s d d s s FIGURE 3.1 Representative area elements for idealized square and triangular iber-packing geometries. υf = π d 4 s 2 (3.14) Clearly, the maximum theoretical iber volume fraction occurs when s = d. In this case, υf max = π = 0.785 4 (3.15) A similar calculation for the triangular array shows that υf = π d 2 3 s 2 (3.16) and when s = d, the maximum iber volume fraction is υf max = π = 0.907 2 3 (3.17) The close packing of ibers required to produce these theoretical limits is generally not achievable in practice, however. In most continuous iber composites, the ibers are not perfectly round and are packed in a random fashion as shown in Figure 3.2, so that the iber volume fractions typically range from 0.5 to 0.8. In short iber composites, iber volume fractions are usually much lower due to processing limitations (e.g., the viscosity of the iber/ resin mixture must be controlled for proper low during molding) and the random orientation of ibers. Since iber-packing geometry is never entirely reproducible from one piece of material to another, we should not expect our micromechanics predictions to be exact. Principles of Composite Material Mechanics 100 FIGURE 3.2 Photomicrograph of carbon/epoxy composite showing actual iber-packing geometry at 400× magniication. The random nature of the iber-packing geometry in real composites such as the one shown in Figure 3.2 can be quantiied by the use of the Voronoi cell (Figure 3.3) and a statistical distribution describing the Voronoi cell size [6]. Each point within the space of a Voronoi cell for a particular iber is closer to the center of that iber than it is to the center of any other iber. If we can approximate the Voronoi cell in Figure 3.3a as an equivalent square area as shown in Figure 3.3b and c, then Equation 3.14 can be used to describe the relationship between the iber diameter d, the iber volume fraction υf, and the Voronoi cell size s (which is assumed to be the same as the center-tocenter spacing). Yang and Colton [6] have used digital image processing to show that the Wiebull distribution f (s) = β s−γ δ δ β −1 s − γ β exp − when s ≥ γ δ (3.18) f (s) = 0 oth herwise adequately characterizes the probability density function for the Voronoi cell size for several composites, where β, δ, and γ are the Wiebull parameters associated with the shape, scale, and location of the distribution, respectively. A typical histogram of measured Voronoi distances for a thermoplastic matrix composite and the corresponding Wiebull distribution from regression analysis are shown in Figure 3.4. Effective Moduli of a Continuous Fiber-Reinforced Lamina 101 (b) (a) (c) s s r d FIGURE 3.3 Voronoi cell and its approximation. (a) Irregularly shaped Voronoi cells, (b) nearest square approximations to Voronoi cells, and (c) unit cell corresponding to part (b). (Yang, H. and Colton, J. S., Polymer Composites, 15(1), 34–41, 1994, Copyright Wiley-VCH Verlag GmbH & Co. KGaA. Reproduced with permission.) EXAMPLE 3.1 The ibers in a unidirectional composite have square cross sections with iber dimensions, a, on each side and iber center-to-center spacing, s, arranged in a square array similar to that shown in Figure 3.1. Assuming that the ibers are oriented perpendicular to the page and that the dimensions a and s do not change along the length of the composite, ind the expression for the iber volume fraction for the composite in terms of the dimensions a and s, then determine the maximum theoretical iber volume fraction. Solution Using an approach similar to that used to derive Equation 3.14 from Figure 3.1, and replacing the round ibers with square ibers in the representative area element of four ibers in a square array, the iber volume fraction is υf = 4( a/2)2 a 2 = 2 s2 s Principles of Composite Material Mechanics 102 0.3 β = 1.08643 δ = 3.974265 γ = 4.783992 Probability density 0.25 0.2 0.15 0.1 0.05 0 0 10 20 30 Voronoi distance (μm) 40 FIGURE 3.4 Typical histogram of Voronoi distances and corresponding Wiebull distribution for a thermoplastic matrix composite. (Yang, H. and Colton, J. S., Polymer Composites, 15(1), 34–41, 1994, Copyright Wiley-VCH Verlag GmbH & Co. KGaA. Reproduced with permission.) The maximum theoretical iber volume fraction υf max = 1 occurs when s = a, in which case the material is all iber and no matrix. EXAMPLE 3.2 A carbon/epoxy composite specimen has dimensions of 2.54 cm × 2.54 cm × 0.3 cm and a weight of 2.98 g. After “resin digestion” in an acid solution, the remaining carbon ibers weigh 1.863 g. From independent tests, the densities of the carbon ibers and epoxy matrix materials are found to be 1.9 and 1.2 g/cm3, respectively. Determine the volume fractions of ibers, epoxy matrix, and voids in the specimen. Solution The composite density is ρc = 2.98 g = 1.54 g/cm 3 (2.54)(2.54)(0.3) cm 3 From Equation 3.9, the void fraction is υv = 1 − (1.863/1.9) + (2.98 − 1.863)/1.2 = 0.0122 or 1.22% 2.98/1.54 Effective Moduli of a Continuous Fiber-Reinforced Lamina 103 From Equation 3.2, υf + υm = 1 − υ v = 1.0 − 0.0122 = 0.988 Then, from Equation 3.6, 1.54 = 1.9υf + 1.2(0.988 − υf ) Therefore, the iber volume fraction is υf = 0.506 or 50.6% and the matrix volume fraction is υm = 0.988 − 0.506 = 0.482 or 48.2% EXAMPLE 3.3 Assume that the carbon ibers in the specimen from Example 3.2 have been uniformly coated with an epoxy “sizing” of thickness t before bonding of the ibers and matrix together to form a unidirectional composite. If the bare ibers have a diameter d = 0.0005 in. (0.0127 mm) and the coated ibers are assumed to be packed together in the tightest possible square array, what is the thickness of the sizing? Solution The iber spacing, s, which in this case must be equal to the coated iber diameter, dc, can be found from Equation 3.14: s = dc = πd 2 = 4 vf π(0.0005)2 = 0.000623 in. (0.0158 mm) 4(0.506) The thickness is then t = (dc − d)/2 = 0.0000615 in. (0.00156 mm). PROBLEM 3.1 A rectangular array of elliptical ibers is shown in Figure 3.5. Derive the relationship between the iber volume fraction and the given geometrical parameters. What is the maximum possible iber volume fraction for this packing geometry? PROBLEM 3.2 A face-centered cubic array of round ibers is shown in Figure 3.6. Derive the relationship between the iber volume fraction and the given geometrical parameters. What is the maximum possible iber volume fraction for this iber-packing geometry? Principles of Composite Material Mechanics 104 a b sa sb FIGURE 3.5 Rectangular array of elliptical ibers. 45º 2s s d s FIGURE 3.6 Face-centered cubic array of round ibers. 3.2 Elementary Mechanics of Materials Models The objective of this section is to present the elementary mechanics of materials models for predicting four independent effective moduli of an orthotropic continuous iber-reinforced lamina. In the elementary mechanics of Effective Moduli of a Continuous Fiber-Reinforced Lamina 105 materials approach to micromechanical modeling, iber-packing geometry is not speciied, so that the RVE may be a generic composite block consisting of iber material bonded to matrix material, as shown in Figure 3.7. More sophisticated mechanics of materials models, which do consider iberpacking geometry, will be discussed later. The constituent volume fractions in the RVE are assumed to be the same as those in the actual composite. Since it is assumed that the ibers remain parallel and that the dimensions do not change along the length of the element, the area fractions must equal the volume fractions. Perfect bonding (a) Lm 2 L2 Lf Lm 2 2 Matrix A1 = Total area 1 Fiber Af = Fiber area Matrix Am = Matrix area (b) σc1 σc2 (c) σc12 (d) FIGURE 3.7 RVE and simple stress states used in elementary mechanics of materials models. (a) Representative volume element, (b) longitudinal normal stress, (c) transverse normal stress, and (d) in-plane shear stress. Principles of Composite Material Mechanics 106 at the interface is assumed, so that no slip occurs between iber and matrix materials. The iber and matrix materials are assumed to be linearly elastic and homogeneous. The matrix is assumed to be isotropic, but the iber can be either isotropic or orthotropic. Following the concept of the RVE, the lamina is assumed to be macroscopically homogeneous, linearly elastic, and orthotropic. Micromechanics equations will be developed from either equilibrium or compatibility relationships, and assumptions about either stresses or strains in the RVE that has been subjected to a simple state of stress. Since the mechanics of materials approach does not require speciication of the stresses, strains, and displacements at each point, we only deal with the corresponding volume-averaged quantities. Finally, since it is assumed that the stresses, strains, displacements, and RVE dimensions do not change along the length, we can just use area averages: σ= 1 1 σ dV = σ dA V A (3.19) ε= 1 1 ε dV = ε dA V A (3.20) δ= 1 1 δ dV = δ dA V A (3.21) ∫ ∫ ∫ ∫ ∫ ∫ where the overbar denotes an averaged quantity, and σ = stress, ε = strain, δ = displacement, V = volume, and A = area associated with the face on which loading is applied. The volume averaging (or area averaging) may occur over the composite lamina, the iber, or the matrix, and the corresponding parameters will be identiied by using subscripts as deined in the following derivations. 3.2.1 Longitudinal Modulus If the RVE in Figure 3.7a is subjected to a longitudinal normal stress, σ c1, as shown in Figure 3.7b, the response is governed by the effective longitudinal modulus, E1. Static equilibrium requires that the total resultant force on the element must equal the sum of the forces acting on the iber and matrix. Combining the static equilibrium condition with Equation 3.19, we get σ c1 A1 = σ f1 Af + σ m1 Am (3.22) where subscripts c, f, and m refer to composite, iber, and matrix, respectively, and the second subscript refers to the direction. Since area fractions Effective Moduli of a Continuous Fiber-Reinforced Lamina 107 are equal to the corresponding volume fractions, Equation 3.22 can be rearranged to give a “rule of mixtures” for longitudinal stress: σ c1 = σ f1υf + σ m1υm (3.23) Under the assumptions that the matrix is isotropic, that the iber is orthotropic, and that all materials follow a one-dimensional (1D) Hooke’s law (i.e., Poisson strains are neglected), σ c1 = E1 εc1 ; σ f1 = Ef1 εf1 ; σ m1 = Em εm1 (3.24) and Equation 3.23 becomes E1 εc1 = Ef 1 εf1υf + Em εm1υm (3.25) Double subscripts are used for the iber modulus since the iber is assumed to be orthotropic. That is, the longitudinal iber modulus, Ef1, is not necessarily equal to the transverse iber modulus, Ef2. For example, carbon and aramid ibers exhibit orthotropic behavior, whereas glass and boron are practically isotropic. For the isotropic case, it is a simple matter to let Ef1 = Ef2. Since the matrix is assumed to be isotropic, the matrix modulus, Em, does not need a second subscript. Finally, the key assumption is that, due to perfect bonding the average displacements and strains in the composite, iber, and matrix along the 1 direction are all equal: εc1 = εf1 = εm1 (3.26) Substitution of Equation 3.26 into Equation 3.25 then yields the rule of mixtures for the longitudinal modulus: E1 = Ef 1υf + Em υm (3.27) This equation predicts a linear variation of the longitudinal modulus with iber volume fraction, as shown in Figure 3.8. Although simple in form, Equation 3.27 agrees well with experimental data from Reference 7 (Figure 3.8b) and is a useful design equation. The validity of the key assumptions leading to this equation will now be examined by using a strain energy approach. Further insight into the micromechanics of the longitudinal loading case is possible by using a strain energy approach. Under the given state of stress, the total strain energy stored in the composite, Uc, can be represented as Principles of Composite Material Mechanics 108 (b) 50 45 6.0 40 Composite modulus (a) Ef Equation 3.27 EI (GPa) Rule of mixtures 25 3 20 15 d = 10 μm d = 30 μm d = 20 μm d = 50 μm 10 Em 5 Equation 3.40 0 0 0.5 Fiber volume fraction 1 4.5 30 EI (106 psi) 35 1.5 0.1 0.2 0.3 0.4 0.5 0.6 0.7 Fiber volume fraction (υf) 0 FIGURE 3.8 Variation of composite moduli with iber volume fraction (a) predicted E1 and E2 from elementary mechanics of materials models and (b) comparison of predicted and measured E1 for E-glass/polyester. (From Adams, R. D. 1987. In Reinhart, T. J. et al., Engineered Materials Handbook, Composites, Vol. 1, pp. 206–217. ASM International, Materials Park, OH. With permission.) the sum of the strain energy in the ibers, Uf, and the strain energy in the matrix, Um: Uc = Uf + Um (3.28) Again making the mechanics of materials assumption that the stresses and strains are uniform over the RVE and using Equation 3.24, the strain energy terms can be simpliied as Uc = Uf = Um = 1 2 1 2 ∫ 1 2 ∫ σ c1ε c1 dV = 1 E1 εc21Vc 2 (3.29a) σ f1ε f1 dV = 1 Ef1 εf21Vf 2 (3.29b) 1 Em1 εm2 1Vm 2 (3.29c) Vε ∫ Vm Vf σ m1ε m1 dV = In this approximation, the strain energy due to the mismatch in Poisson strains at the iber/matrix interface has been neglected (recall the Effective Moduli of a Continuous Fiber-Reinforced Lamina 109 assumptions leading to Equation 3.24). This neglected term has been shown to be of the order of the square of the difference between the Poisson’s ratios of the iber and the matrix, so the approximation is justiied [8]. It is easily shown that substitution of Equation 3.29 into Equation 3.28, along with the assumption of equal strains from Equation 3.26, again leads to the rule of mixtures given by Equation 3.27. But the strain energy approach also allows us to ask, “What happens if the assumption of equal strains is not made?” In order to proceed, let the stresses in the ibers and the matrix be deined in terms of the composite stress as follows: σ f1 = a1σ c1 ; σ m1 = b1σ c1 (3.30) where a1 and b1 are constants. Substitution of Equation 3.30 in the rule of mixtures for stress, Equation 3.23, leads to a1υf + b1υm = 1 (3.31) Substitution of Equation 3.24, Equation 3.29, and Equation 3.30 into Equation 3.28 leads to 1 υ υ = a12 f + b12 m E1 Ef1 Em (3.32) Note that we did not assume equal strains in ibers and matrix to derive these equations. In order to check the strain distribution, however, Equations 3.31 and 3.32 can be solved simultaneously for a1 and b1 when composite, iber, and matrix properties are known. The ratio of the iber strain to the matrix strain can then be found. For example, using the measured properties of an E-glass/epoxy composite [9], E1 = 5.05 × 106 psi (34.82 GPa); υm = 0.55 E2 = 1.53 × 106 psi (10.55 GPa); υf = 0.45 Ef1 = Ef 2 = 10.5 × 106 psi (72.4 GPa) (3.33) Em = 0.55 × 106 psi (3.79 GPa) we ind that a1 = 2.0884, b1 = 0.1093, a1/b1 = σ f1/σ m1 = 19.1 , and εf1/ εm1 = 1.00. Thus, the assumption of equal strains, which led to Equation 3.27, is valid for this material, as it apparently is for other composites. The strain energy approach will be used again in the next section to check the validity of an assumption leading to the equation for the transverse modulus. Principles of Composite Material Mechanics 110 3.2.2 Transverse Modulus If the RVE in Figure 3.7a is subjected to a transverse normal stress, σ c2, as shown in Figure 3.5c, the response is governed by the effective transverse modulus, E2. Geometric compatibility requires that the total transverse composite displacement, δc2, must equal the sum of the corresponding transverse displacements in the iber, δf 2, and the matrix, δm2: δc 2 = δf 2 + δm 2 (3.34) It follows from the deinition of normal strain that δc2 = εc2L2 , δf 2 = εf 2Lf , δm 2 = εm 2Lm (3.35) and Equation 3.34 now becomes εc2L2 = εf 2Lf + εm 2Lm (3.36) Since the dimensions of the RVE do not change along the 1 direction, the length fractions must be equal to the volume fractions, and Equation 3.36 can be rearranged to get the rule of mixtures for transverse strains: εc 2 = εf 2υf + εm 2υm (3.37) The 1D Hooke’s laws for this case are σ c2 = E2 εc2 , σ f 2 = Ef 2 εf 2 , σ m2 = Em εm2 (3.38) where the Poisson strains have again been neglected. As with the longitudinal case, the inclusion of such strains would lead to a much more complex state of stress due to the mismatch in Poisson strains at the interface [10,11]. This is another example of the difference between a mechanics of materials solution and a more rigorous theory of elasticity solution. Combining Equations 3.37 and 3.38, we get σc2 σf 2 σ υf + m 2 υm = E2 Ef 2 Em (3.39) If we assume that the stresses in the composite, matrix, and iber are all equal, Equation 3.39 reduces to the “inverse rule of mixtures” for the transverse modulus: 1 υ υ = f + m E2 Ef 2 Em (3.40) Effective Moduli of a Continuous Fiber-Reinforced Lamina 111 From the RVE in Figure 3.7, it would seem that the assumption of equal stresses is valid because equilibrium requires that the forces must be equal for the series arrangement, and both iber and matrix blocks have equal areas normal to the 2 direction. In the actual composite, however, the iber-packing arrangement is such that the forces and areas for the iber and matrix are not necessarily equal, and we will use a strain energy approach to show that the resulting stresses are not equal. Thus, Equation 3.40 is generally not acceptable for design use. As shown in Figure 3.8a, Equation 3.40 gives the same result as Equation 3.27 at the extreme values of iber volume fraction (i.e., υf = 0 and υf = 1.0), but it predicts signiicant improvement in the transverse modulus E2 only at high iber volume fractions. This turns out to be the correct trend, but, as shown in Section 3.5, the experimental data fall well above the predicted curve based on Equation 3.40. As with the longitudinal case, the strain energy approach provides additional insight into the micromechanics of the transverse loading case. We now express the iber and matrix strains in terms of the composite strain: εf 2 = a2 εc 2 , εm2 = b2 εc2 (3.41) where a2 and b2 are constants. Substitution of Equation 3.41 in the compatibility expression, Equation 3.37 yields a2υf + b2υm = 1 (3.42) By substituting Equations 3.38 and 3.41 in equations analogous to Equation 3.29 for the transverse loading case and the strain energy expression, Equation 3.28, we ind that E2 = a22Ef 2υf + b22Em υm (3.43) where the strain energy due to the Poisson strain mismatch at the interface has again been neglected. It is important to note that we did not assume equal stresses in the ibers and the matrix to obtain Equation 3.43. Using the properties for the E-glass/epoxy given in Equation 3.33 and solving Equations 3.42 and 3.43 simultaneously, we ind that a2 = 0.432, b2 = 1.465, the strain ratio a2/b2 = εf 2/εm2 = 0.295, and the corresponding stress ratio is σ f2/σ m 2 = 5.63. Thus, the assumption of equal stresses in ibers and matrix, which led to Equation 3.40, is not justiied for this material and is apparently not valid for most other composites as well. More accurate alternative design equations for the transverse modulus will be discussed later. 112 Principles of Composite Material Mechanics 3.2.3 Shear Modulus and Poisson’s Ratio The major Poisson’s ratio, ν12, and the in-plane shear modulus, G12, are most often used as the two remaining independent elastic constants for the orthotropic lamina. The major Poisson’s ratio, which is deined as ν12 = − εc 2 εc1 (3.44) when the only nonzero stress is a normal stress along the 1 direction (Figure 3.7b), can be found by solving the geometric compatibility relationships associated with both the 1 and the 2 directions. The result is another rule of mixtures formulation: ν12 = νf 12υf + νm υm (3.45) where νf12 is the major Poisson’s ratio of the iber and νm is the Poisson’s ratio of the matrix. Equation 3.45 is generally accepted as being suficiently accurate for design purposes. As in the case for the longitudinal modulus, the geometric compatibility relationships leading to the solution are valid. The effective in-plane shear modulus is deined as (Figure 3.7d) G12 = σ c12 γ c12 (3.46) where σ c12 is the average composite shear stress in the 12 plane and γ c12 = 2 ε c 12 , the average engineering shear strain in the 12 plane. An equation for the in-plane shear modulus can be derived using an approach similar to that which was used for the transverse modulus. That is, geometric compatibility of the shear deformations, along with the assumption of equal shear stresses in ibers and matrix, leads to another inverse rule of mixtures: 1 υ υ = f + m G12 Gf 12 Gm (3.47) where Gf12 is the shear modulus of the iber in the 12 plane and Gm is the shear modulus of the matrix. As we might expect, this equation is not very accurate because the shear stresses are not equal as assumed. A strain energy approach similar to that used in Section 3.2.2 can be used here to show that the shear stresses are in fact not equal. As with the transverse modulus, we need to ind better equations for estimating the in-plane shear modulus. Such equations will be discussed in the following sections. Effective Moduli of a Continuous Fiber-Reinforced Lamina EXAMPLE 3.4 Determine the longitudinal modulus E1 of the reinforced concrete post described in Problem 1.13 of Chapter 1. Assume that the steel rods and the concrete are linear elastic and isotropic, and that they are perfectly bonded together. Solution In this case, the steel rods act as the ibers and the concrete acts as the matrix. The iber volume fraction (same as the area fraction, if the rod and post cross sections do not change along the length) is υf = 4(0.00125) = 0.055 (0.3)2 Therefore, the matrix volume fraction is υm = 1 − 0.055 = 0.945 From Equation 3.27, the longitudinal modulus is E1 = Ef1υf + Em υm = 200(0.055) + 17(0.945) = 27.065 GPa Note that, even though the volume fraction of the steel rods is only 5.5%, the steel contributes about 40% of the longitudinal composite modulus because of the high modulus of steel (200 GPa) relative to that of concrete (17 GPa). EXAMPLE 3.5 As shown in Figure 3.9, an RVE for a three-phase unidirectional composite is approximated by three concentric cylinders representing the iber, the matrix, and the iber/matrix interphase. The iber/matrix interphase is a region surrounding the iber, which has different properties from either the iber or the matrix. Interphase regions may be created during processing as a result of interactions between the matrix materials and either the iber material or a iber-sizing material. Since the geometrical features of this model are not associated with any speciic iber-packing array geometry, it has been referred to as a “self-consistent model” [8]. Assuming that the three materials are linear elastic, isotropic, and securely bonded together, derive the micromechanics equation for the longitudinal modulus, E1, of the composite. Solution The three constituent materials are arranged in parallel; so static equilibrium requires that the total resultant force on the composite must equal the sum of the forces acting on the three materials. Accordingly, the rule of mixtures for longitudinal composite stress in Equation 3.23 applies 113 Principles of Composite Material Mechanics 114 2 Matrix, Em Df Interphase, Ei Di Dm 1 Fiber, Ef 3 FIGURE 3.9 Self-consistent RVE for three-phase composite, including iber, matrix, and iber/matrix interphase. here, with the addition of a third term representing the interphase, as denoted by the subscript i σ c1 = σ f υf + σ m υm + σ i υi Now supplementing Equation 3.24 with a similar stress–strain relationship for the interphase material and extending the assumption of equal strains in the constituents (Equation 3.26) to the interphase material as well, we get another rule of mixtures: D2 D2 − D2 D2 − D2 E1 = Ef υf + Em υm + Ei υi = Ef 2f + Em m 2 i + Ei i 2 f Dm Dm Dm where the diameters Df, Dm, and Di are deined in Figure 3.9. Indeed, for a composite having any number of constituents, n, that are securely bonded together and arranged in parallel as in Figure 3.9, the generalized rule of mixtures for the longitudinal composite modulus is n E1 = ∑E υ j j j =1 where Ej and υj are the modulus and volume fraction of the jth constituent, respectively, and j = 1, 2, …, n. EXAMPLE 3.6 The constituent materials in the composite described in Examples 3.1 and 3.2 have the properties Ef1 = 32.0 × 106 psi (220 GPa), Ef2 = 2.0 × 106 psi (13.79 GPa), and Em = 0.5 × 106 psi (3.45 GPa). Estimate the longitudinal and transverse moduli of the composite. Given these iber and matrix materials, what are the maximum possible values of E1 and E2? Effective Moduli of a Continuous Fiber-Reinforced Lamina Solution The longitudinal modulus is given by the rule of mixtures in Equation 3.27 E1 = (32 × 10 6 ) 0.506 + (0.5 × 10 6 ) 0.482 = 16.43 × 10 6 psi(113 GPa) The transverse modulus is roughly estimated by the inverse rule of mixtures in Equation 3.40: E2 = 1 = 0.82 × 10 6 psi (5.65 GPa) (0.506/2 × 10 6 ) + (0.482/0.5 × 10 6 ) However, as shown later, the inverse rule of mixtures prediction is typically well below the actual values of E2, and is not recommended for design use. As expected, the composite is highly anisotropic with E1 ≫ E2. If the composite has the theoretical maximum iber volume fraction of 0.907 for a close-packed triangular array (Equation 3.17), the corresponding composite properties are still highly anisotropic, with E1 = 29 × 106 psi (200 GPa) and E2 = 1.56 × 106 psi (10.75 GPa). Note that even with this maximum iber content, the transverse modulus is still very low. Thus, some transverse reinforcement is usually necessary in practical applications. Note also that the longitudinal modulus of the carbon/epoxy composite is now about the same as the modulus of steel, but the density of the composite is only about 20% of the density of steel. Composites typically have much greater stiffness-to-weight ratios than conventional metallic structural materials. EXAMPLE 3.7 For longitudinal loading of the composites in Example 3.6, compare the stresses in the iber and matrix materials. Compare the strain energy stored in the ibers with that stored in the matrix. Solution From Equations 3.24 and 3.26, the ratio of iber stress to matrix stress is σ f1 E ε E 32.0 = 64.0 = f1 f 1 = f1 = σ m1 Em εm1 Em 0.5 Thus, the iber carries most of the stress since the iber modulus is always higher than the matrix modulus. From Equations 3.26, 3.29b, and 3.29c, the ratio of iber strain energy to matrix strain energy is 32.0(0.506) Uf E υ = f1 f = = 67.0 0.5(0.482) U m Em υm that is almost the same as the stress ratio. If the composite had the maximum possible iber volume fraction of 0.907, the stress ratio would remain 115 Principles of Composite Material Mechanics 116 the same since it is independent of the iber volume fraction. However, the strain energy ratio would increase dramatically to 624, since it is proportional to the ratio of iber volume fraction to the matrix volume fraction. PROBLEM 3.3 A unidirectional IM-9 carbon iber/Hexply 8551-7 epoxy composite is to be designed to replace a 6061-T6 aluminum alloy rod which is to be loaded in longitudinal tension. (a) What iber volume fraction of the carbon ibers would be required if the composite longitudinal modulus is to be equal to that of the 6061-T6 aluminum? (b) For the composite rod of part (a), what would be the percentage reduction in density compared with that of the aluminum rod? Use the properties in Table 1.1, and neglect voids in the composite. PROBLEM 3.4 A hybrid carbon–aramid/epoxy composite is made by randomly mixing continuous aligned ibers of the same diameter, so that there are two carbon ibers for each aramid iber. The ibers are assumed to be arranged in a square array with the closest possible packing. The stress–strain curves for longitudinal tensile loading of iber and matrix materials are shown in Figure 3.10. Determine the composite longitudinal modulus E1. PROBLEM 3.5 Derive Equation 3.45. PROBLEM 3.6 Derive Equation 3.47. Stress (GPa) 2.8 2.1 Carbon fiber Aramid fiber 0.72 Epoxy matrix 0.1 0.0164 0.0054 0.021 Strain 0.033 FIGURE 3.10 Stress–strain curves for iber and matrix materials in a hybrid composite. Effective Moduli of a Continuous Fiber-Reinforced Lamina 117 PROBLEM 3.7 Using an elementary mechanics of materials approach, ind the micromechanics equation for predicting the minor Poisson’s ratio, ν21, for a unidirectional iber composite in terms of the corresponding iber and matrix properties and volume fractions. Assume that the ibers are orthotropic, the matrix is isotropic, and all materials are linear elastic. This derivation should be independent of the one in Problem 3.5. PROBLEM 3.8 A composite shaft is fabricated by bonding an isotropic solid shaft having shear modulus G1, and outside radius r1, inside a hollow isotropic shaft having shear modulus G2 and outside radius r2. The composite shaft is to be loaded by a twisting moment, T, that is distributed over the end of the shaft, as shown in Figure 3.11. Using an elementary mechanics of materials approach, derive the equations for the stresses and deformations at any radius and the equation for the effective torsional shear modulus of the composite shaft in terms of the material and geometrical properties of shafts 1 and 2. PROBLEM 3.9 An RVE from a particle-reinforced composite is shown in Figure 3.12. The particle has a cross-sectional area Ap(x) that varies with the distance x, and the stresses and strains in particle and matrix materials also vary with x. Find the expression for the effective Young’s modulus of the composite, Ex, along the x direction. The answer should be left in terms of an integral involving the length, L; the particle modulus, Ep; the matrix modulus, Em; and the particle area fraction ap(x) = Ap(x)/Ac, where Ac is the total composite crosssectional area. Assume that both the particle and the matrix are isotropic. PROBLEM 3.10 Using the result from Problem 3.9, determine the effective Young’s modulus, Ex, for the RVE shown in Figure 3.13. In Figure 3.13, the reinforcing particle has a square cross section and is oriented as shown. For a particle having a Young’s modulus Ep = 10 × 106 psi (68.95 GPa) and a matrix having a Young’s Material 1 T 2r2 2r1 FIGURE 3.11 Composite shaft under torsional load. Material 2 T Principles of Composite Material Mechanics 118 Matrix σx Ap(x) σx Particle Matrix x L FIGURE 3.12 RVE for a particle-reinforced composite with a particle that has a varying cross-sectional area Ap(x). L L Matrix Matrix L σx σx Particle L Matrix Matrix FIGURE 3.13 RVE for a composite reinforced with a square particle and loaded along the diagonal of the particle. modulus Em = 0.5 × 106 psi (3.45 GPa), determine the value of Ex and compare with the values from the rule of mixtures Equation 3.27 and the inverse rule of mixtures Equation 3.40. PROBLEM 3.11 A unidirectional composite is to be modeled by the RVE shown in Figure 3.14a, where the iber and matrix materials are assumed to be isotropic and perfectly bonded together. Using a mechanics of materials approach, derive the micromechanics equations for the effective in-plane shear modulus, G12, for the following cases: a. The ends of the RVE are perfectly bonded to supports that are rigid against rotation, then subjected to uniform in-plane shear stress, τ12, by the nonrotating supports, as shown in Figure 3.14b. Effective Moduli of a Continuous Fiber-Reinforced Lamina (a) 2 (b) 119 (c) τ12 Fiber τ12 Fiber Matrix Fiber Matrix 1 Matrix τ12 τ12 FIGURE 3.14 RVE with two different loading and boundary conditions for problem 15. (a) RVE, (b) ends of RVE ixed against rotation, and (c) ends of RVE free to rotate. b. The top and bottom surfaces of the RVE are subjected to uniform inplane shear stress, τ12, and the ends of the RVE are free to rotate, as shown in Figure 3.14c. PROBLEM 3.12 Figure 3.15 shows an RVE for an elementary mechanics of materials model of the same type as shown in Figure 3.7, but with transverse deformation along the 2 direction prevented by rigid supports along the top and bottom edges. For an applied longitudinal normal stress as shown in Figure 3.15, ind a micromechanics equation for the longitudinal modulus E1. Do not neglect the Poisson strains in the general derivation, and show what happens to the general equation for E1 when the Poisson’s ratios for composite, iber, and matrix are all equal. 2 Matrix σc1 σc1 Fiber 1 Matrix FIGURE 3.15 RVE for elementary mechanics of materials model with rigid supports that prevent transverse deformation. Principles of Composite Material Mechanics 120 3.3 Improved Mechanics of Materials Models As shown in the previous section, the elementary mechanics of materials models for E1 and ν12 are good enough for design use. However, the corresponding models for E2 and G12 are of questionable value, because they are based on invalid assumptions, and agreement with experimental results is generally poor. We will now discuss several reinements of the elementary mechanics of materials models. Due to the simpliied RVE that was used for the elementary mechanics of materials approach (Figure 3.7), the resulting equations were not tied to any particular iber-packing geometry. Since the results for E1 and ν12 were so favorable, we can conclude that those properties must be essentially independent of iber-packing geometry. By the same reasoning, it appears that E2 and G12 may be more sensitive to iber-packing geometry. Thus, the assumption of a speciic iber-packing array is one possible reinement of the models. Although real composites have random-packing arrays, the assumption of a regular array is a logical simpliication if we are to have any hope of developing simple design equations. Such an assumption allows us to use simple relations among iber size, spacing, and volume fraction. Hopkins and Chamis [12] have developed a reined model for transverse and shear properties based on a square iber-packing array and a method of dividing the RVE into subregions. The following derivation is adapted from Reference 12. A square array of ibers is shown in Figure 3.1, and the RVE for such an array is shown in Figure 3.16. The RVE is easily divided into subregions for more detailed analysis if we convert to a square iber having the same area as the round iber. The equivalent square iber shown in Figure 3.16 must then have the dimension sf = π d 4 (3.48) and from Equation 3.14, the size of the RVE is A d s B A A sf sf B A FIGURE 3.16 Division of RVE into subregions based on square iber having equivalent iber volume fraction. Effective Moduli of a Continuous Fiber-Reinforced Lamina π d 4 υf s= 121 (3.49) The RVE is divided into subregions A and B, as shown in Figure 3.16. In order to ind the effective transverse modulus for the RVE, we irst subject the series arrangement of iber and matrix in subregion B to a transverse normal stress. Following the procedure of Section 3.2.2, the effective transverse modulus for this subregion, EB2, is found to be 1 1 sf 1 sm = + EB2 Ef 2 s Em s (3.50) where the matrix dimension is sm = s − sf. From Equations 3.48 and 3.49, it is seen that sf = υf s and sm = 1 − υf s (3.51) so that Equation 3.50 now becomes EB2 = Em 1 − υf (1 − Em /Ef 2 ) (3.52) The parallel combination of subregions A and B is now loaded by a transverse normal stress and the procedure of Section 3.2.1 is followed to ind the effective transverse modulus of the RVE. The result, of course, is the rule of mixtures analogous to Equation 3.27 E2 = EB 2 sf s + Em m s s (3.53) Substitution of Equations 3.51 and 3.52 in Equation 3.53 then gives the inal result, υf E2 = Em 1 − υf + 1 − υf (1 − Em /Ef 2 ) ( ) (3.54) A similar result may be found for G12. The detailed derivation in Reference 12 also includes the effect of a third phase, a iber/matrix interphase material, which is assumed to be an annular volume surrounding the iber. Such interphase regions exist in many metal matrix [12] and polymer matrix [13] Principles of Composite Material Mechanics 122 composites. When the iber diameter is equal to the interphase diameter, the equation for E2 in Reference 12 reduces to Equation 3.54. The complete set of equations for effective moduli of the three-phase model is given in Reference 12. In separate publications, Chamis [14,15] presented the so-called simpliied micromechanics equations (SMEs), which are based on this same method of subregions, except that only the terms for subregion B (Figure 3.16) are retained. Thus, the SME for E2 would be the same as that for EB2 in Equation 3.52, and similar equations for the other effective moduli are given in References 14 and 15. Also included in these references are tables of iber and matrix properties to be used as input to the SME, and these tables are reproduced here in Tables 3.1 and 3.2. It is important to note that in such tables, the transverse iber modulus, Ef2, and the longitudinal iber shear modulus, Gf12, are not actually measured but are inferred by substitution of measured composite properties and matrix properties in the SME. The inferred properties show that ibers such as carbon and aramid are highly anisotropic, whereas glass and boron are essentially isotropic. Similar back-calculations of anisotropic iber properties using other analytical models have been reported by Kriz and Stinchcomb [16] and by Kowalski [17]. More recently, direct measurement of iber transverse moduli has been reported by Kawabata [18]. Kawabata’s measurements, based on transverse diametral compression of single carbon and aramid ibers, show even greater anisotropy than the inferred properties in Tables 3.1 and 3.2. However, Caruso and Chamis [19] have shown that the SME and the corresponding tables of properties give results that agree well with three-dimensional (3D) inite element models, as shown in Figure 3.17. Finite element models will be discussed in more detail in the next section. Since the SME for E1 and υ12 are the same as Equations 3.27 and 3.45, respectively, this comparison provides further evidence of the validity of those equations. Another set of equations for E2 and G12 has been derived by Spencer [20] who used a square array model that included the effects of the strain concentration at points of minimum clearance between ibers in the RVE. Spencer’s equation is 2Γ Γ+k Mc Γ − 1 1 π = + − + tan −1 2 2 Γ Γ−k Mm k 2 Γ −k (3.55) where Mc = E2, Mm = Em, and k = 1 − Em/Ef2 for the transverse modulus equation and Mc = G12, Mm = Gm, and k = 1 – Gm/Gf12 for the longitudinal shear modulus equation. The parameter Γ = s/d in both the equations. Spencer also suggests that Γ can be accurately approximated for a variety of packing geometries over the full range of iber volume fractions, υf, by the equation Γ= (1.1υ 1 2 f ) − 2.1υf + 2.2 υf (3.56) – – – btu/1b/°F btu/h/ft2/°F/in. btu/h/ft2/°F/in. 10−6 in./in./°F 10−6 in./in./°F ksi ksi ksi in. 1b/in.3 106 psi 106 psi 106 psi 106 psi Units 1 0.0056 0.095 58 58 24.2 24.2 0.20 0.20 0.31 22 22 2.8 2.8 600 700 100 Boron 10,000 0.0003 0.070 55.0 0.90 1.1 0.7 0.20 0.00327 0.20 580 58 –0.55 5.6 250 200 – HMS 10,000 0.0003 0.063 31.0 2.0 2.0 1.0 0.20 0.0129 0.20 580 58 –0.55 5.6 350 260 – AS 3000 0.0003 0.064 32.0 2.0 1.3 0.7 0.20 0.0125 0.22 580 58 –0.55 5.6 350 300 – T300 580 0.00046 0.053 22 0.6 0.42 0.22 0.35 0.00954 0.25 1.7 1.7 –2.2 30 400 75 – KEV 204 0.00036 0.090 12.4 12.4 5.17 5.17 0.20 0.20 0.17 21 21 2.8 2.8 600 – – S-G 204 0.00036 0.090 10.6 10.6 4.37 4.37 0.22 0.22 0.17 7.5 7.5 2.8 2.8 400 – – E-G Source: From Chamis, C. C. 1987. In Weeton, J. W., Peters, D. M., and Thomas, K. L., eds., Engineers’ Guide to Composite Materials. ASM International, Materials Park, OH. With permission. Note: Transverse, shear, and compression properties are estimates inferred from corresponding composite properties. HMS, AS, and T300 are carbon ibers, KEV is Kevlar, S-G is S-glass, and E-G is E-glass. a Estimates of transverse Poisson’s ratio based on assumed symmetry of iber compliance matrix. Number of ibers per end Fiber diameter Density Longitudinal modulus Transverse modulus Longitudinal shear modulus Transverse shear modulus Longitudinal Poisson’s ratio Transverse Poisson’s ratioa Heat capacity Longitudinal heat conductivity Transverse heat conductivity Longitudinal thermal expansion coeficient Transverse thermal expansion coeficient Longitudinal tensile strength Longitudinal compression strength Shear strength Properties Fiber Properties for Use in Chamis SMEs TABLE 3.1 Effective Moduli of a Continuous Fiber-Reinforced Lamina 123 Principles of Composite Material Mechanics 124 TABLE 3.2 Matrix Properties for Use in Chamis SMEs Parameters Density Modulus Shear modulus Poisson’s ratio Heat capacity Heat conductivity Thermal expansion coeficient Diffusivity Moisture expansion coeficient Tensile strength Compression strength Shear strength Tensile fracture strain Compressive fracture strain Shear fracture strain Air heat conductivity Glass transition temperature (dry) Units LM IMLS IMHS HM Polyimide PMR – btu/1b/°F btu/h/ft2/°F/in. 10−6 in./in./°F 0.042 0.32 – 0.43 0.25 1.25 57 0.046 0.50 – 0.41 0.25 1.25 57 0.044 0.50 – 0.35 0.25 1.25 36 0.045 0.75 – 0.35 0.25 1.25 40 0.044 0.50 – 0.35 0.25 1.25 20 0.044 0.47 – 0.36 0.25 1.25 28 10−10 in.2/s in./in./M 0.6 0.33 0.6 0.33 0.6 0.33 0.6 0.33 0.6 0.33 0.6 0.33 ksi ksi ksi in./in. (%) in./in. (%) 8 15 8 8.1 15 7 21 7 1.4 4.2 15 35 13 2.0 5.0 20 50 15 2.0 5.0 15 30 13 2.0 4.0 8 16 8 2.0 3.5 in./in. (%) btu/h/ft2/°F/in. °F 10 0.225 350 3.2 0.225 420 3.5 0.225 420 4.0 0.225 420 3.5 0.225 700 5.0 0.225 700 1b/in.3 106 psi 106 psi Source: From Chamis, C. C. 1987. In Weeton, J. W., Peters, D. M., and Thomas, K. L., eds., Engineers’ Guide to Composite Materials. ASM International, Materials Park, OH. With permission. Note: LM, low modulus; IMLS, intermediate modulus low strength; IMHS, intermediate modulus high strength; HM, high modulus. Thermal, hygral, compression, and shear properties are estimates only; Gm = Em/2(1 + υm). LM, IMLS, IMHS, and HM refer to typical epoxy matrix resins. Spencer does not include a table of suggested properties for use with these equations. 3.4 Elasticity Models The theory of elasticity approach to micromechanical modeling begins in the same way as the mechanics of materials approach, by selecting the RVE and then subjecting it to uniform stress or displacement at the boundary. The two approaches differ substantially in the solution of the resulting boundary value problem, however. The equations of elasticity must be satisied at every Effective Moduli of a Continuous Fiber-Reinforced Lamina 1.6 15 3 10 Multicell 1 0 0.8 Single cell 0.6 0.2 0.4 Fiber volume ratio Multicell 1 0.2 0 3 0.8 Multicell 0.4 1 0 0.8 2 Single cell 0.2 0.4 0.6 Fiber volume ratio 0.8 SC MC CCMC SME 0.4 2 Single cell 0.6 0.4 1.2 SC MC CCMC SME 3 1.0 Modulus (G12), 106 psi 2 5 Modulus (E2, E3), 106 psi 20 SC MC CCMC SME SC MC CCMC SME 0.6 0.2 0.4 Fiber volume ratio 0.8 Poisson’s ratio (ν12) Modulus (E1), 106 psi 25 125 0.3 3 0.2 Multicell 2 0.1 1 0 Single cell 0.6 0.2 0.4 Fiber volume ratio 0.8 FIGURE 3.17 Comparison of 3D inite element results for lamina elastic constants with predictions from SMEs for carbon/epoxy. (From Caruso, J. J. and Chamis, C. C. 1986. Journal of Composites Technology and Research, 8(3), 77–83. With permission.) point in the model, and no simplifying assumptions are made regarding the stress or strain distributions as in the mechanics of materials approach. Fiber-packing geometry is generally speciied in the elasticity approach. A variety of closed-form and numerical solutions of the governing equations of elasticity have been reported in the literature [1–4], and a complete review of the work in this area is beyond the scope of this book. However, the stress equilibrium equations and the strain–displacement relations from elasticity theory are derived in Appendices B and C, respectively. The objective here is to discuss several representative numerical and closed-form solutions in order to show what additional knowledge of micromechanical behavior can be obtained from the more rigorous elasticity approach. Particular emphasis is placed on inite element numerical solutions. Principles of Composite Material Mechanics 126 3.4.1 Finite Difference Models Numerical solutions of the governing elasticity equations are often necessary for complex structural geometries such as those found in the RVEs used in micromechanics models. For example, Adams and Doner [21] used a inite difference solution to determine the shear modulus G12 for a rectangular array of ibers. A displacement boundary value problem was solved for one quadrant of the RVE, as shown in Figure 3.18. Note that Adams and Doner use the z axis to deine the iber direction, whereas the x and y axes correspond to the transverse directions. The displacement components u, v, and w correspond to the displacements along the x, y, and z axes, respectively. The imposed displacement w* along x = a causes a displacement ield of the form u = v = 0, w = w(x , y ) (3.57) From the strain–displacement equations (Appendix C) and Hooke’s law, the only nonvanishing stress components are τ zx = G ∂w ∂x and τ zy = G ∂w ∂y (3.58) where the shear modulus, G, may be either the iber shear modulus, Gf, or the matrix shear modulus, Gm, depending on whether the coordinates x and y locate a point in the iber or in the matrix. Isotropic behavior was assumed y a b τxz z w∗ x FIGURE 3.18 One quadrant of an RVE from Adams and Doner elasticity solution for shear modulus G12. (From Adams, D. F. and Doner, D. R. 1967. Journal of Composite Materials, 1, 4–17. With permission.) Effective Moduli of a Continuous Fiber-Reinforced Lamina 127 for both iber and matrix materials. Substitution of Equation 3.58 in the only nontrivial stress equilibrium equation (Appendix B) yielded the governing partial differential equation ∂ 2w ∂ 2w G 2 + 2 = 0 ∂y ∂x (3.59) which was solved subject to the displacement boundary conditions w(0, y ) = 0, w( a, y ) = w* G ∂w = 0 along y = 0 and y = b ∂y (3.60) and continuity conditions at the iber/matrix interface by using a inite difference scheme. The solution yielded the values of the displacements w(x, y) at each node of the inite difference grid. Stresses were found by substituting these displacements in the inite difference forms of Equation 3.58, and the effective shear modulus was then determined from Gxz = τxz w*/a (3.61) where τxz is the average shear stress along x = a. A similar boundary value problem for shear along y = b yields the associated shear modulus Gyz. Typical results are shown in Figure 3.19, where the ratio of the composite shear modulus to the matrix shear modulus, G12/Gm is plotted versus the shear modulus ratio Gf/Gm for various iber volume fractions. In a separate paper, Adams and Doner [22] used a similar approach to determine the transverse modulus E2 and typical results are shown in Figure 3.20. It is seen in Figures 3.19 and 3.20 that the reinforcement effect for both G12 and E2 only becomes signiicant for iber volume fractions above about 50%, but that combinations of high iber stiffness and high iber volume fractions can signiicantly increase G12 and E2. Unfortunately, these same combinations also generate very high stress concentration factors at the iber/matrix interfaces, as shown in the same papers [21,22]. One of the advantages of the elasticity approach is that the complete stress and strain distributions in the RVE are generated, and the calculation of stress concentration factors is possible. One advantage of numerical solutions such as inite differences is the capability for analysis of complex geometries. For example, stiffness and stress concentration factors were also obtained for a variety of iber cross-sectional shapes such as squares and ellipses in a rectangular array [21,22]. Principles of Composite Material Mechanics 128 28 Composite shear stiﬀness (G12/Gm) 26 δ 24 Filament volume (υf ) r [Filament spacing (δ/r)] 78% (0.012) δ 22 20 Circular ﬁlaments in a square array 18 16 75% (0.044) 14 12 10 70% (0.118) 8 6 55% (0.39) 4 40% (0.80) 4% (0.88) 2 0 1 2 40 60 100 6 8 10 20 Shear modulus ratio (Gf /Gm) 4 200 400 600 1000 FIGURE 3.19 Normalized composite shear stiffness, G12/Gm, versus shear modulus ratio, Gf/Gm, for circular ibers in a square array. (From Adams, D. F. and Doner, D. R. 1967. Journal of Composite Materials, 1, 4–17. With permission.) Normalized composite transverse stiffness (E2/Em) 28 Filament volume (υf ) 26 [Filament spacing (δ/r)] 24 r 22 78% (0.012) δ σx σx 20 75% (0.044) 18 16 Circular filaments in a square array 14 12 70% (0.118) 10 8 6 55% (0.39) 4 40% (0.80) 2 4% (6.88) 0 1 2 4 40 60 100 6 8 10 20 Constituent stiffness ratio (E f /Em) 200 400 600 1000 FIGURE 3.20 Normalized composite transverse stiffness, E2/Em, versus modulus ratio, Ef/Em, for circular ibers in a square array. (From Adams, D. F. and Doner, D. R. 1967. Journal of Composite Materials, 1, 152–164. With permission.) Effective Moduli of a Continuous Fiber-Reinforced Lamina 129 3.4.2 Finite Element Models The most widely used numerical approach to micromechanics modeling is inite element analysis (FEA). The previously mentioned FEA of Caruso and Chamis [19] and Caruso [23] is one example of such an approach. In this case, a singlecell (SC) inite element model was developed from 192 3D isoparametric brick elements (Figure 3.21). This SC model was then used as a building block for a multicell (MC) model consisting of nine SC models in a 3 × 3 array (Figure 3.17). A third model, center cell of multicell model (CCMC) used only the center cell in the nine-cell MC model for the calculations. Boundary and load conditions were consistent with those used for the previously discussed SME mechanics of materials solutions, so that the inite element results could be compared with the SME results. For example, Equation 3.61 and similar equations were used to determine stiffnesses from inite element results. Material properties for AS graphite ibers in an intermediate modulus high strength (IMHS) epoxy matrix were used (Tables 3.1 and 3.2). Fibers were assumed to be orthotropic, whereas 3, Z, w (a) (b) 3, Z, w c 2, Y, v c a b b 1, X, u 1, X, u a 2, Y, v 3, Z, w (c) c 1, X, u b a 2, Y, v FIGURE 3.21 3D inite element models of RVEs. (a) The SC model used for the SC calculation, (b) the MC model which is used for the MC calculation, and (c) the MC model which only the center cell is used for the CCMC calculation. (From Caruso, J. J. and Chamis, C. C. 1986. Journal of Composites Technology and Research, 8(3), 77–83. Copyright ASTM. With permission.) 130 Principles of Composite Material Mechanics FIGURE 3.22 Examples of 2D and 3D inite element quarter domain micromechanics models. (From Finegan, I. C. and Gibson, R. F. 1997. In Farabee, T. M. ed., Proceedings of ASME Noise Control and Acoustics Division, NCA-Vol. 24, pp. 127–138. American Society of Mechanical Engineers, New York, NY. With permission.) the matrix was assumed to be isotropic. As shown in Figure 3.17, the inite element results show good agreement with the SME results. As with the previously discussed inite difference approach used in References 21 and 22, the quarter domain model of a representative volume can also be analyzed by using inite elements. Typical two-dimensional (2D) and 3D quarter domain inite element models are shown in Figure 3.22 from Reference 24. For example, in one study, 3D inite element quarter domain models similar to the one in Figure 3.22 were subjected to transverse normal loading as in Figure 3.23 [24,25], and the effect of model aspect ratio L/(D/2) on the transverse modulus was determined, as shown in Figure 3.24. In this model, the iber axis is assumed to lie along the z direction, while x and y are transverse to the iber axis. This particular model included a iber coating or interphase region between the iber and the matrix (see Example 3.5 for further discussion of the interphase). For the quarter domain model, boundary conditions are that along the plane x = 0, displacements perpendicular to the plane are prevented, while along the plane y = 0, displacements perpendicular to that plane are also prevented. The transverse modulus was calculated by imposing a uniform displacement Ux along the plane x = D/2 and then using the calculated stresses from the inite element model to evaluate Equation 3.62: σ x Ex = = εx ∫ σ dV/V ∫ ε dV/V x V x V (3.62) Effective Moduli of a Continuous Fiber-Reinforced Lamina 131 Matrix Coating (interphase) Transverse loading Fiber y x z Df /2 Dc/2 (Di/2) L D/2 FIGURE 3.23 Quarter domain of RVE under transverse normal loading. (From Finegan, I. C. and Gibson, R. F. 1998. Journal of Vibration and Acoustics, 120(2), 623–627. With permission.) where σ x = average stress acting along plane x = D/2 in Figure 3.15, εx = Ux = average strain along plane x = D/2 (D/2) where D/2 = dimension deined in Figure 3.23 Ux = imposed displacement along x = D/2 L = length of model along z, the iber direction V = volume It is seen from Figure 3.24 that the transverse modulus varies from a minimum value for low-model aspect ratios to a maximum for high-model aspect ratios [24,25]. It was also shown that the low-model aspect ratio results from 3D models coincided with the results obtained by using 2D plane stress elements (i.e., with longitudinal stress σz = 0), while the high-model aspect ratio results from 3D models coincided with the results obtained by using 2D plane strain elements (i.e., with longitudinal strain εz = 0). For a unidirectional composite having continuous ibers oriented along the z direction, the plane strain condition is more realistic than the plane stress condition. The importance of this observation is that 2D plane strain elements can be used for these types of models instead of 3D elements, and this leads to Principles of Composite Material Mechanics 132 10.0 Transverse modulus (GPa) 9.5 Plane strain 9.0 8.5 Plane stress 8.0 7.5 7.0 0.0001 1 10 0.01 0.1 Model aspect ratio (L/(D/2)) 100 FIGURE 3.24 Variation of transverse modulus with model aspect ratio for graphite/epoxy composite from 3D inite element models. (From Finegan, I. C. and Gibson, R. F. 1998. Journal of Vibration and Acoustics, 120(2), 623–627. With permission.) signiicant reductions in the number of elements and the corresponding computation time. Proper treatment of boundary conditions on the RVEs of micromechanical FEA models is particularly important [26]. Since the composite is assumed to consist of large numbers of identical and adjacent RVEs as repeating elements, the deformations on the boundaries of a given RVE must be geometrically compatible with those of the adjacent RVEs. Figure 3.25a shows an example of a boundary deformation pattern that is not geometrically compatible with that of the adjacent identical RVEs (i.e., symmetry arguments tell us that the deformed RVEs will not “it together” to form a continuous composite without gaps). By contrast, Figure 3.25b shows a boundary deformation pattern that is geometrically compatible with that of its neighboring RVEs (i.e., the deformed RVEs will all “it together” to form a continuous composite without gaps). These are often referred to as “periodic boundary conditions,” since they are repeated over and over again from one RVE to another as we move through the composite. For normal loading as in Figure 3.23, geometric compatibility is assured if each boundary surface is constrained to deform parallel to itself as in Figure 3.25b. Such constraints on displacements of a plane can be accomplished in FEA by using the so-called multipoint constraint (MPC) elements which are available in many FEA codes. MPC Effective Moduli of a Continuous Fiber-Reinforced Lamina (a) 133 Examples of deformed (b) RVE boundaries Undeformed RVEs FIGURE 3.25 Boundary deformations for RVEs of micromechanical models: (a) boundary deformations are geometrically incompatible with those of identical adjacent RVEs and (b) boundary deformations are geometrically compatible with those of identical adjacent RVEs. elements allow the user to specify a “master node” in a plane such that all nodes in that plane will have the same displacement under load. For shear loading as in Figure 3.18, geometric compatibility is assured if the deformed shape is a parallelogram, although, as pointed out by Sun and Vaidya [26], it is not necessary for the edges of the parallelogram to remain straight as they rotate in shear distortion. Note that, when the displacement is imposed, as in the example described above and in Reference 25, geometric compatibility is assured by the imposed planar displacement. When the applied stress is imposed, however, displacement constraints must be speciied to assure geometric compatibility. 3.4.3 Closed-Form and Variational Models As an example of a closed-form elasticity solution, Whitney and Riley [8] used axisymmetric Airy stress functions to solve for the stresses and strains in a so-called “self-consistent” model having a single isotropic iber embedded in a concentric cylinder of isotropic matrix material. The cylindrical geometry of the self-consistent model is such that the model is not associated with any speciic iber-packing geometry. The resulting micromechanical stresses and strains were then used in energy balance equations similar to Equations 3.28 through 3.29 to solve for E1 and E2. The equation for E1 reduces to the rule of mixtures when the Poisson’s ratio of the iber is equal to that of the matrix. The additional term is due to the mismatch in Poisson strains at the iber/matrix interface (recall that this term was neglected in Equations 3.28 through 3.29). Predictions showed good agreement with experimental data for boron/epoxy. In a later paper, Whitney extended the analysis to include anisotropic, transversely isotropic ibers [27]. 134 Principles of Composite Material Mechanics Another closed-form micromechanical elasticity approach, the method of cells was developed by Aboudi [28]. A representative cell consisting of a square iber embedded in a square of matrix material was divided into four subcells. Equilibrium equations were then solved subject to continuity of displacements and tractions at the interfaces between the subcells and between neighboring cells on an average basis, along with the assumption of linear variations of displacements in each subcell. The equations are too lengthy to present here, but excellent agreement was observed with the experimental data on graphite/epoxy from Reference 16. One advantage of this approach is that it yields not only the in-plane lamina properties, but also the throughthe-thickness properties such as G23 and ν23. Paul [29] obtained closed-form solutions for the bounds on the transverse modulus of a iber composite (or Young’s modulus of an isotropic-particlereinforced composite) by using a variational approach. By applying the theorem of minimum complementary energy to the situation where the composite is subjected to a uniaxial normal stress, Paul found the lower bound on E2 to be the inverse rule of mixtures (Equation 3.40). The application of the theorem of minimum potential energy to the situation where the composite is subjected to a simple extensional strain gave the upper bound on E2, which reduces to the rule of mixtures (Equation 3.27) when the Poisson’s ratios of iber and matrix materials are taken to be the same. The bounds derived by Paul [29] are independent of packing geometry and are referred to as the elementary bounds. Thus, it should be no surprise that the bounds are very far apart, as shown in Figure 3.8. Tighter bounds require the speciication of packing geometry. For example, Hashin and Rosen [30] applied the principles of minimum potential and complementary energy to iber composites with hexagonal and random arrays. Detailed summaries of these and other related results have been reported by Hashin [1] and Christensen [3]. More recently, Torquato [31] has reviewed advances in the calculation of improved bounds on the effective properties of random heterogeneous media. Such improved bounds are determined by using statistical correlation functions to model the random variations in the microstructure. Since the iber-packing geometry in composites is of a random nature, such bounds should be more realistic than the bounds that are based on some idealized iber-packing array. 3.5 Semiempirical Models In Section 3.3, improved mechanics of materials models for the prediction of E2 and G12 were discussed. Another general approach to estimating these properties involves the use of semiempirical equations that are adjusted to Effective Moduli of a Continuous Fiber-Reinforced Lamina 135 match experimental results or elasticity results by the use of curve-itting parameters. The equations are referred to as being “semiempirical” because, although they have terms containing curve-itting parameters, they also have some basis in mechanics. The most widely used semiempirical equations were developed by Halpin and Tsai [32]. The Halpin–Tsai equation for the transverse modulus is E2 1 + ξηυf = Em 1 − ηυf (3.63) (Ef /Em ) − 1 (Ef /Em ) + ξ (3.64) where η= and ξ is the curve-itting parameter, which is also a measure of the degree of reinforcement of the matrix by the ibers. The corresponding equation for G12 is obtained by replacing Young’s moduli E2, Ef, and Em in the above equations by the shear moduli G12, Gf, and Gm, respectively. Note that the values for the curve-itting parameter may be different for E2 and G12. Halpin and Tsai found that the value ξ = 2 gave an excellent it to the inite difference elasticity solution of Adams and Doner [22] for the transverse modulus of a square array of circular ibers having a iber volume fraction of 0.55. For the same material and iber volume fraction, a value of ξ = 1 gave excellent agreement with the Adams and Doner solution for G12 [21]. Jones [11] shows that when ξ = 0, the Halpin–Tsai equation reduces to the inverse rule of mixtures (Equation 3.40), whereas a value of ξ = ∞ yields the rule of mixtures (Equation 3.27). Recall that Paul [29] proved that these equations also represent the bounds on E2. Thus, the interpretation of the curveitting parameter, ξ, as a measure of the degree of iber reinforcement has a theoretical basis. The use of the Halpin–Tsai equations in a variety of other applications and related empirical equations for estimating the curve-itting parameter are discussed in more detail by Jones [11] and Halpin [4]. Zhu et al. [33] have shown that the predicted elastic constants for Kevlar/epoxy from the Halpin–Tsai equations agree closely with predictions from inite element micromechanics models similar to those discussed in Section 3.4.2. Tsai and Hahn [10] have proposed another semiempirical approach to calculating E2 and G12, that is based on the fact that the stresses in the ibers and the matrix are not equal under the corresponding loading conditions. Recall that the proof of such differences was demonstrated using a strain energy approach in Section 3.2.2. The method involves the use of empirical “stress-partitioning parameters” in derivations paralleling those used for the elementary mechanics of materials models. For example, the Tsai–Hahn Principles of Composite Material Mechanics 136 equation for E2 is found by introducing a stress-partitioning parameter, η2, and using the relationship σ m2 = η2σ f2 (3.65) in a derivation similar to that used for the elementary mechanics of materials model for E2 in Section 3.2.2. The derivation was also based on the assumption that a rule of mixtures for stress similar to Equation 3.23 also held for the transverse direction (2 direction). Although such an assumption is obviously not consistent with the RVE coniguration and the loading condition shown in Figure 3.7c, it would be valid for a real composite with iber packing such as that shown in Figure 3.2. The result of this derivation is 1 1 = E2 υf + η2υm υf η2υm E + E m f (3.66) Note that Equation 3.66 reduces to the inverse rule of mixtures (Equation 3.40) when the stress-partitioning parameter η2 = 1.0. This is to be expected since Equation 3.40 was based on the assumption that the stresses in the iber and the matrix are the same. A similar equation can be derived for the shear modulus, G12, as shown in Reference 10. Figure 3.26 from Reference 10 Transverse modulus (GPa) 20 15 η2 = 0.5 10 η2 = 1.0 5 Experimental data Equation 3.66 0 0 0.2 0.4 0.6 0.8 Fiber volume fraction 10 FIGURE 3.26 Transverse modulus for glass/epoxy according to Tsai–Hahn Equation 3.66. (From Tsai, S. W. and Hahn, H. T. 1980. Introduction to Composite Materials. Technomic Publishing Co., Lancaster, PA. With permission.) Effective Moduli of a Continuous Fiber-Reinforced Lamina 137 shows experimental data for the transverse modulus of a glass/epoxy composite compared with the predicted values from Equation 3.66 for two different assumed values of the stress-partitioning parameter. Clearly, the experimental data fall well above the prediction for η2 = 1.0, which corresponds to the inverse rule of mixtures (Equation 3.40). This further validates the statement following Equation 3.40 that the inverse rule of mixtures is not acceptable for design use. A much better agreement is seen for η2 = 0.5, which means that the stress in the matrix is only one-half of the stress in the iber. The stress-partitioning parameter η2 = 0.5 was also found to yield accurate predictions of G12 based on comparisons with experimental data for the same glass/epoxy [10]. Formulas for estimating the stresspartitioning parameters from constituent material properties are also given in Reference 10. EXAMPLE 3.8 For the composite in Example 3.6, compare the transverse modulus values calculated by the inverse rule of mixtures (3.40), the method of subregions (3.54), Spencer’s Equation 3.55, the Halpin–Tsai Equation 3.63, and the Tsai–Hahn Equation 3.66. Solution The result from the inverse rule of mixtures (3.40), as previously calculated in Example 3.6, is E2 = 0.82 × 10 6 psi (5.65 GPa) For the method of subregions (3.54): υf E 2 = Em 1 − υf + / υ ( ( )) 1 − 1 − E E f m f2 ( ) 0.506 = 0.5 × 10 6 1 − 0.506 + . ( ( . / )) 1 − 0 506 1 − 0 5 2 ( ) = 0.9 × 10 6 psi (6.2 GPa) For Spencer’s Equation 3.55: First estimate Γ = 1.18 from Equation 3.56. Note that the actual value of Γ from example 3.2 is Γ = s/d = 0.000623/0.0005 = 1.25. Using Γ = 1.18 in Equation 3.55, we have E2 = 0.98 × 106 psi (6.76 GPa). For the Halpin–Tsai Equation 3.63: η= (Ef /Em ) − 1 (2/0.5) − 1 = = 0.5 (Ef /Em ) + ξ (2/0.5) + 2 Principles of Composite Material Mechanics 138 1 + 2(0.5)(0.506) 1 + ξηυf = 0.5 × 10 6 E2 = Em 1 − ηυf 1 − 0.5(0.506) = 1.00 × 10 6 psi ( 6.89 GPa) For the Tsai–Hahn Equation 3.66: υ f η2 υ m 0.506 0.5 (0.482) 1 1 1 + = = + 0.5 × 10 6 E2 υf + η 2 υm Ef Em 0.506 + 0.5(0.482) 2 × 106 so that E2 = 1.016 × 106 psi (7 GPa). As previously mentioned, the inverse rule of mixtures prediction for the transverse modulus is considerably lower than experimentally determined values. However, the higher values given by the method of subregions, Spencer’s equation, the Halpin–Tsai equation, and the Tsai– Hahn equation are in good agreement with each other and with experimental values, and so these equations are recommended for design use. EXAMPLE 3.9 The Tsai–Hahn stress-partitioning factor for transverse loading, η2, deined in Equation 3.65 is used to derive Equation 3.66 for the transverse composite modulus, E2. Using a similar approach with a strainpartitioning parameter for longitudinal loading, η1, derive an equation for the longitudinal composite modulus, E1. Solution The strain-partitioning parameter for longitudinal loading is deined by the relationship εm1 = η1 εf 1 The static equilibrium equation and the Hooke’s Laws leading to Equation 3.25 are still valid, but now instead of substituting the geometric compatibility Equation 3.26 in Equation 3.25, we substitute the above equation for the strain-partitioning parameter in Equation 3.25, which leads to E1 εc1 = Ef1 εf1vf + Em η1 εf 1vm or E1 = εf1 (Ef1vf + Em η1vm ) εc1 In order to use this equation to ind E1, the ratio εf1/ εc1 must be known. For example, if the longitudinal iber modulus is the dominant factor in Effective Moduli of a Continuous Fiber-Reinforced Lamina 139 the longitudinal composite modulus, one might assume that ( εf1/ εc1 ) = 1.0, then the properties Ef1, Em, vf, and vm can be used in the above equation to ind the value of the strain-partitioning factor, η1, that gives the best agreement between the predicted and experimental values of E1. PROBLEM 3.13 Using the method of subregions, derive an equation for the transverse modulus, E2, for the RVE, which includes a iber/matrix interphase region, as shown in Figure 3.27. Hint: The equation should reduce to Equation 3.54 when the iber diameter is the same as the interphase diameter. PROBLEM 3.14 Derive Equation 3.59. PROBLEM 3.15 For a unidirectional composite with a rectangular iber array (Figure 3.18), use the equations of elasticity to set up the displacement boundary value problem for the determination of the transverse modulus, E2. That is, ind the governing partial differential equations for displacements u and v in the RVE, and specify the boundary and continuity conditions. Assume plane strain (εz = 0). Do not attempt to solve the equations, but explain briely how E2 would be found. Assume that both iber and matrix are isotropic. PROBLEM 3.16 For the quarter domain of an RVE in Figure 3.23, a uniform transverse normal stress σ x is applied on the plane x = D/2. Set up the equations describing the boundary conditions and the constraints on geometrically compatible displacements for a inite element micromechanics analysis of this model. Matrix sc d i Fiber df Interphase sc FIGURE 3.27 RVE with iber/matrix interphase region. 140 Principles of Composite Material Mechanics PROBLEM 3.17 The ibers in a E-glass/epoxy composite are 0.0005 in. (0.0127 mm) in diameter before coating with an epoxy sizing 0.0001 in. (0.00254 mm) thick. After the sizing has been applied, the ibers are bonded together with more epoxy of the same type. What is the maximum iber volume fraction that can be achieved? Using the iber and matrix moduli given in Equation 3.33, determine the composite longitudinal modulus E1 and the composite transverse modulus E2 corresponding to the maximum iber volume fraction. PROBLEM 3.18 Derive Equation 3.66. PROBLEM 3.19 Show that a value of ξ = 0 reduces the Halpin–Tsai equation (Equation 3.63) to the inverse rule of mixtures Equation 3.40, whereas a value ξ = ∞ reduces it to the rule of mixtures Equation 3.27. References 1. Hashin, Z. 1983. Analysis of composite materials—A survey. Journal of Applied Mechanics, 50, 481–505. 2. Chamis, C. C. and Sendeckyj, G. P. 1968. Critique on theories predicting thermo-elastic properties of ibrous composites. Journal of Composite Materials, 2(3), 332–358. 3. Christensen, R. M. 1979. Mechanics of Composite Materials. John Wiley & Sons, New York, NY. 4. Halpin, J. C. 1984. Primer on Composite Materials: Analysis (rev.). Technomic Publishing Co., Lancaster, PA. 5. Gibson, R. F. 1975. Elastic and dissipative properties of iber reinforced composite materials in lexural vibration. PhD dissertation, University of Minnesota, Minneapolis, MN. 6. Yang, H. and Colton, J. S. 1994. Microstructure-based processing parameters of thermoplastic composite materials. Part I: Theoretical models. Polymer Composites, 15(1), 34–41. 7. Adams, R. D. 1987. Damping properties analysis of composites. In Reinhart, T. J., Dostal, C. A., Woods, M. S., Frissell, H. J., and Ronke, A. W., eds., Engineered Materials Handbook, Composites, Vol. 1, pp. 206–217. ASM International, Materials Park, OH. 8. Whitney, J. M. and Riley, M. B. 1966. Elastic properties of iber reinforced composite materials. AIAA Journal, 4(9), 1537–1542. 9. Gibson, R. F. and Plunkett, R. 1976. Dynamic mechanical behavior of iber-reinforced composites: Measurement and analysis. Journal of Composite Materials, 10, 325–341. Effective Moduli of a Continuous Fiber-Reinforced Lamina 141 10. Tsai, S. W. and Hahn, H. T. 1980. Introduction to Composite Materials. Technomic Publishing Co., Lancaster, PA. 11. Jones, R. M. 1999. Mechanics of Composite Materials, 2nd ed. Taylor & Francis, Philadelphia, PA. 12. Hopkins, D. A. and Chamis, C. C. 1988. A unique set of micromechanics equations for high temperature metal matrix composites. In DiGiovanni, P. R. and Adsit, N. R., eds., Testing Technology of Metal Matrix Composites, ASTM STP 964, pp. 159–176. American Society for Testing and Materials, Philadelphia, PA. 13. Drzal, L. T., Rich, M. J., Koenig, M. F., and Lloyd, P. F. 1983. Adhesion of graphite ibers to epoxy matrices: II. The effect of iber inish. Journal of Adhesion, 16, 133–152. 14. Chamis, C. C. 1984. Simpliied composite micromechanics equations for hygral, thermal and mechanical properties. SAMPE Quarterly, 15(3), 14–23. 15. Chamis, C. C. 1987. Simpliied composite micromechanics equations for mechanical, thermal and moisture-related properties. In Weeton, J. W., Peters, D. M., and Thomas, K. L., eds., Engineers’ Guide to Composite Materials. ASM International, Materials Park, OH. 16. Kriz, R. D. and Stinchcomb, W. W. 1979. Elastic moduli of transversely isotropic graphite ibers and their composites. Experimental Mechanics, 19, 41–49. 17. Kowalski, I. M. 1986. Determining the transverse modulus of carbon ibers. SAMPE Journal, 22(4), 38–42. 18. Kawabata, S. 1988. Measurements of anisotropic mechanical property and thermal conductivity of single iber for several high performance ibers. Proceedings of 4th Japan–U.S. Conference on Composite Materials, pp. 253–262, Washington, D.C. 19. Caruso, J. J. and Chamis, C. C. 1986. Assessment of simpliied composite micromechanics using three-dimensional inite element analysis. Journal of Composites Technology and Research, 8(3), 77–83. 20. Spencer, A. 1986. The transverse moduli of ibre composite material. Composites Science and Technology, 27, 93–109. 21. Adams, D. F. and Doner, D. R. 1967. Longitudinal shear loading of a unidirectional composite. Journal of Composite Materials, 1, 4–17. 22. Adams, D. F. and Doner, D. R. 1967. Transverse normal loading of a unidirectional composite. Journal of Composite Materials, 1, 152–164. 23. Caruso, J. J. 1984. Application of inite element substructuring to composite micromechanics. NASA TM 83729. 24. Finegan, I. C. and Gibson, R. F. 1997. Analytical and experimental characterization of damping and stiffness in polymer composites having coated ibers as reinforcement. In Farabee, T. M. ed., Proceedings of ASME Noise Control and Acoustics Division, NCA-Vol. 24, pp. 127–138. American Society of Mechanical Engineers, New York, NY. 25. Finegan, I. C. and Gibson, R. F. 1998. Improvement of damping at the micromechanical level in polymer composite materials under transverse normal loading by the use of special iber coatings. Journal of Vibration and Acoustics, 120(2), 623–627. 26. Sun, C. T. and Vaidya R. S. 1996. Prediction of composite properties from a representative volume element. Composites Science and Technology, 56, 171–179. 27. Whitney, J. M. 1967. Elastic moduli of unidirectional composites with anisotropic ibers. Journal of Composite Materials, 1, 188–193. 142 Principles of Composite Material Mechanics 28. Aboudi, J. 1989. Micromechanical analysis of composites by the method of cells. Applied Mechanics Reviews, 42(7), 193–221. 29. Paul, B. 1960. Prediction of elastic constants of multi-phase materials. Transactions of AIME, 218, 36–41. 30. Hashin, Z. and Rosen, B. W. 1964. The elastic moduli of iber reinforced materials. Journal of Applied Mechanics, 31, 223–232. Errata, p. 219 (March 1965). 31. Torquato, S. 1991. Random heterogeneous media: Microstructure and improved bounds on effective properties. Applied Mechanics Reviews, 44(2), 37–76. 32. Halpin, J. C. and Tsai, S. W. 1969. Effects of environmental factors on composite materials. AFML-TR-67–423. 33. Zhu, H., Sankar, B. V., and Marrey, R. V., 1998. Evaluation of failure criteria for iber composites using inite element micromechanics. Journal of Composite Materials, 32, 766–782. 4 Strength of a Continuous Fiber-Reinforced Lamina 4.1 Introduction Because of the variety of failure modes that can occur in composites, the analysis of composite strength is more dificult than the analysis of elastic behavior, which was discussed in Chapters 2 and 3. As shown in Chapter 1, the strength of a composite is derived from the strength of the ibers, but this strength is highly directional in nature. For example, the longitudinal strength of the continuous iber-reinforced lamina, sL, is much greater than the transverse strength, sT. In addition, the compressive strengths sL(− ) and sT(− ) associated with these directions may be different from the corresponding tensile strengths sL(+ ) and sT(+ ), and the transverse tensile strength sT(+ ) is typically the smallest of all the lamina strengths for reasons that will be explained later. The in-plane shear strength sLT associated with the principal material axes is still another independent property. These ive lamina strengths form the basis of a simpliied lamina strength analysis, which, in turn, will be used later in a simpliied laminate strength analysis. The relationships among these ive lamina strengths and the allowable lamina strengths under off-axis or multiaxial loading are discussed in this chapter, as are several micromechanical models for predicting the lamina strengths. Interlaminar strengths will be discussed in Chapters 7 and 9. As shown in Chapters 2 and 3, the linear elastic stress–strain relationships for the orthotropic lamina are simpliied by the use of “effective moduli.” The effective moduli, which relate the volume-averaged lamina stresses to the volume-averaged lamina strains (recall Equations 2.7 through 2.9), are deined by simple uniaxial or shear stress conditions associated with the lamina principal material axes. Using a similar approach, the “effective strengths” of the lamina may be deined as ultimate values of the volume-averaged stresses that cause failure of the lamina under these same simple states of stress. The stress–strain curves in Figure 4.1 show the graphical interpretation of these simple states of stress, the effective strengths sL( + ), sL( − ), sT( + ), sT( − ), and sLT, and the corresponding ultimate strains eL( + ), eL( − ), eT( + ), eT( − ), and eLT. If we 143 Principles of Composite Material Mechanics 144 Longitudinal uniaxial loading σ1 σ1 sL(+) eL(–) σ1 ε1 eL(+) sL(–) Transverse uniaxial loading σ2 σ2 eT(–) sT(+) σ2 ε2 eT(+) sT(–) Shear loading τ12 τ12 sLT eLT γ12 FIGURE 4.1 Stress–strain curves for uniaxial and shear loading showing lamina in-plane strengths and ultimate strains. assume linear elastic behavior up to failure, the ultimate stresses are related to the ultimate strains by sL( + ) = E1eL( + ) ; sT( + ) = E2eT( + ) ; sLT = G12eLT sL( − ) = E1eL( − ) ; sT( − ) = E2eT(− ) (4.1) Typical experimental values of the effective lamina strengths for selected composites are given in Table 4.1 [1,2]. Note that the transverse tensile Strength of a Continuous Fiber-Reinforced Lamina 145 TABLE 4.1 Typical Values of Lamina Strengths for Several Composites at Room Temperature Material Boron/5505 boron/epoxy υf = 0.5a AS/3501 carbon/epoxy υf = 0.6a T300/5208 carbon/epoxy υf = 0.6a IM7/8551-7 carbon/ epoxy υf = 0.6b AS4/APC2 carbon/PEEK υf = 0.58c B4/6061 boron/ aluminum υf = 0.50c Kevlar® 49/epoxy aramid/epoxy υf = 0.6a Scotchply® 1002 E-glass/ epoxy υf = 0.45a E-glass/470–36 E-glass/ vinyl ester υf = 0.30d SL(+ ) Ksi (MPa) SL( − ) Ksi (MPa ) ST( + ) Ksi (MPa ) ST( − ) Ksi (MPa ) SLT Ksi (MPa) 230(1586) 360(2482) 9.1(62.7) 35.0(241) 12.0(82.7) 210(1448) 170(1172) 7.0(48.3) 36.0(248) 9.0(62.1) 210(1448) 210(1448) 6.5(44.8) 36.0(248) 9.0(62.1) 400(2578) 235(1620) 11.0(75.8) 298.6(2060) 156.6(1080) 11.3(78) 28.4(196) 22.8(157) 199(1373) 228(1573) 17.1(118) 22.8(157) 18.5(128) 200(1379) 40(276) 4.0(27.6) 9.4(64.8) 8.7(60.0) 160(1103) 90(621) 4.0(27.6) 20.0(138) 12.0(82.7) 85(584) 116(803) 6.2(43) 27.1(187) 9.3(64.0) Note: Kevlar® is a registered trademark of DuPont Company, and Scotchply® is a registered trademark of 3M Company. a From Chamis, C. C. 1987. In Weeton, J. W., Peters, D. M., and Thomas, K. L., eds., Engineers’ Guide to Composite Materials, pp. 3-8–3-24. ASM International, Materials Park, OH. With permission. b From Hexcel Website, http://www.hexcel.com. c From Daniel, I. M. and Ishai, O., Engineering Mechanics of Composite Materials, 1994, New York, NY, by permission of Oxford University Press. d Courtesy of Ford Motor Company, Research Staff. strength, sT(+ ), is the lowest of all the strengths. This is because, when the loading is perpendicular to the ibers as shown in Figure 4.2, stress and strain concentrations occur in the matrix around the ibers (i.e., the ibers create discontinuities in the matrix) and this reduces the tensile strength of the matrix material. As shown later, this condition is often responsible for the so-called “irst ply failure” in a laminate. It is also interesting to note in Table 4.1 that the compressive strengths are not necessarily equal to the corresponding tensile strengths; the transverse compressive strengths are generally greater than the transverse tensile strengths, and the longitudinal compressive strengths are usually less than or equal to the longitudinal tensile strengths. The intrinsic compressive strength of composites has always been dificult to determine experimentally, however, and the validity of such compression test results is a subject of continuing debate. Recent test results indicate that Principles of Composite Material Mechanics 146 σ2 σ2 FIGURE 4.2 For composites under transverse loading, the ibers create discontinuities in the matrix that lead to stress and strain concentrations. if the proper technique is used, the compression strength may be about the same as the tensile strength. Measurement of composite properties will be discussed in more detail later in Chapter 10. In this section, the lamina effective strengths under simple states of stress have been deined. In the next section, we will discuss the use of these properties in several theories for predicting lamina strength under off-axis or multiaxial loading conditions. Elementary mechanics of materials models for micromechanical prediction of several of the lamina strengths will also be described in this chapter for illustrative purposes. 4.2 Multiaxial Strength Criteria In the cases of off-axis or multiaxial loading, we assume that lamina failure can be characterized by using a multiaxial strength criterion (or failure criterion) that incorporates the gross mechanical strengths described in the previous section. The objective of such a theory is to provide the designer with the capability to estimate quickly when lamina failure will occur under complex loading conditions other than simple uniaxial or shear stresses. In this semiempirical “mechanics of materials” approach, we do not concern ourselves with the details of speciic micromechanical failure modes such as iber pullout, iber breakage, iber microbuckling, matrix cracking, and delamination. The actual failure process is complicated by the fact that these microfailure modes may occur in various combinations and sequences. Indeed, as pointed out by Hashin [3], our knowledge of the details of failure at the micromechanical level is so incomplete that “the failure process cannot be followed analytically.” The existence and growth of cracks and other defects in the composite are also ignored with this approach. Studies of micromechanical failure modes generally require the use of more advanced approaches such as fracture mechanics and are the subjects of numerous journal publications. Additional discussion of such topics will be made in Section 4.3 and in Chapter 9. Available multiaxial composite failure criteria have been reviewed and discussed by Hashin [4], Wu [5], Sendeckyj [6], Chamis [7], Kaminski and Lantz [8], Franklin [9], Tsai [10], Christensen [11], and Zhu et al. [12]. During Strength of a Continuous Fiber-Reinforced Lamina 147 the period from 1998 to 2004, Soden, Hinton, and Kaddour reported on the various aspects of the so-called world-wide failure exercise (WWFE) in a series of journal articles [13–22] and a book [23]. The WWFE was an international exercise in which the developers of 19 leading composite material failure theories were asked to apply their theories to predict failure in unidirectional laminae and in multiply laminates under 14 different test cases involving complex states of stress. The results from the different theories were compared with each other and with experimental data. Since this chapter only covers prediction of failure in unidirectional laminae, only the key results of the WWFE that are relevant to lamina failure prediction will be discussed here, and the results that are relevant to laminate failure prediction will be deferred until later in Chapter 7. Complete coverage of the WWFE is beyond the scope of this book, and the reader is referred to the previously mentioned journal articles [13–22] and the book [23] for details. All the criteria are phenomenological, having evolved from attempts to develop analytical models to describe experimental observations of failure under combined stresses. As pointed out by Wu [5], a large experimental database alone could form the basis for an empirical failure criterion, but the semiempirical mathematical model is preferable because it can reduce the number of required experiments and provide a more systematic approach to design. None of the available theories has been shown to accurately predict failure for all materials and loading conditions, however, and there is no universal agreement as to which theory is best. Many of the failure criteria for anisotropic composites are based on generalizations of previously developed criteria for predicting the transition from elastic to plastic behavior in isotropic metallic materials. As such, they make use of the concept of a “failure surface” or “failure envelope” generated by plotting stress components in stress space. The coordinate axes for the stress space generally correspond to the stresses along the principal material axes. The theory predicts that those combinations of stresses whose loci fall inside the failure surface will not cause failure, whereas those combinations of stresses whose loci fall on or outside the surface will cause failure. Thus, in the application of all the failure criteria, the irst step is the transformation of calculated stresses to the principal material axes using transformation equations like Equation 2.31. Since we are only dealing with twodimensional (2D) stress states in a lamina at this point, the failure surface would be 2D. Failure surfaces for each of the criteria will be presented as they are discussed here. 4.2.1 Maximum Stress Criterion The maximum stress criterion for orthotropic laminae was apparently irst suggested in 1920 by Jenkins [24] as an extension of the maximum normal stress theory (or Rankine’s theory) for isotropic materials, which is covered Principles of Composite Material Mechanics 148 in elementary mechanics of materials courses [25]. This criterion predicts failure when any principal material axis stress component exceeds the corresponding strength. Thus, to avoid failure according to this criterion, the following set of inequalities must be satisied: − sL( − ) < σ 1 < sL( + ) − sT( − ) < σ 2 < sT( + ) (4.2) |τ12|< sLT where the numerical values of sL(− ) and sT(− ) are assumed to be positive. It is assumed that shear failure along the principal material axes is independent of the sign of the shear stress τ12. Thus, only the magnitude of τ12 is important, as shown in the last of Equation 4.2. As shown later, however, the shear strength for off-axis loading may depend on the sign of the shear stress. The failure surface for the maximum stress criterion in σ1, σ2 space is a rectangle, as shown in Figure 4.3. Note that this failure surface is independent of the shear stress τ12, and that the criterion does not account for possible interaction between the stress components. That is, the predicted limiting value of a particular stress component is the same whether or not other stress components are present. Figure 4.4 shows a comparison of theoretical failure surfaces with experimental biaxial failure data for a unidirectional graphite/ epoxy composite [26]. Since the strengths along the principal material directions provide the input to the criterion, we would expect the agreement to be good when the applied stress is uniaxial along those directions. Due to lack of stress interaction in the maximum stress criterion, however, the agreement is not so good in biaxial stress situations. The scatter in the experimental data is unfortunately typical for composite strength tests. σ2 Maximum stress (+) sT Maximum strain ν21 1 ν12 Tsai–Hill (+) (–) sL sL σ1 (–) sT FIGURE 4.3 Maximum stress, maximum strain, and Tsai–Hill failure surfaces in σ1, σ2 space. Strength of a Continuous Fiber-Reinforced Lamina 149 σ2 kpsi 20 10 –120 Maximum stress –80 –60 –40 –20 0 20 –10 40 60 80 100 120 σ1 kpsi 160 σ2 Tsai–Wu Maximum strain –30 Tsai–Hill σ1 Test data (typical) 0° σ1 σ2 FIGURE 4.4 Comparison of predicted failure surfaces with experimental failure data for graphite/epoxy. (From Burk, R. C. 1983. Standard failure criteria needed for advanced composites. Astronautics and Aeronautics, 21(6), 58–62. Copyright AIAA. Reprinted with permission.) Experimental biaxial failure data for comparison with predicted failure surfaces can be obtained by applying biaxial loading directly to the test specimens. Biaxial stress ields can also be generated indirectly by using offaxis uniaxial loading tests [27] or off-axis shear-loading tests. According to Equation 2.31, the applied normal stress, σx, in the off-axis uniaxial loading test shown in Figure 4.5 produces the following biaxial stress state along the principal material axes: σ 1 = σ x cos 2 θ σ 2 = σ x sin 2 θ (4.3) τ12 = −σ x sin θ cos θ where the applied normal stress, σx, may be positive or negative. The importance of the sign of the applied stress in the interpretation of the test results here is obvious. These stress components may then be substituted into y 1 2 θ x FIGURE 4.5 Off-axis uniaxial test of a unidirectional lamina specimen. σx Principles of Composite Material Mechanics 150 (+) SL cos2 θ (+) ST sin2 θ σx SLT sin θ cos θ 0° 45° 90° θ FIGURE 4.6 Predicted values of off-axis uniaxial tensile strength for various off-axis iber orientations according to the maximum stress criterion. equations similar to Equation 4.2 to generate failure surfaces. By plotting the predicted and measured values of σx at failure versus lamina orientation, θ, the various failure criteria can be evaluated [28]. For example, for the off-axis tensile test in Figure 4.5, the predicted values of the failure stress σx as functions of θ according to this theory are shown as three curves in Figure 4.6. For a given angle θ, the corresponding predicted failure stress σx would be found by drawing a vertical line at that angle θ and inding where it intersects the three curves. Predicted failure would correspond to the smallest of the three resulting values of σx. It is seen that, for small θ near θ = 0°, predicted failure is governed by the longitudinal tensile strength, sL(+ ) , for intermediate values of θ, failure is dominated by the shear strength, sLT, and for large θ near θ = 90°, failure is dominated by the transverse tensile strength, sT(+ ) . The predictions of the maximum stress criterion agree reasonably well with experimental off-axis tensile test data when θ is near 0° or 90°, but not so well for intermediate angles. In addition, the cusps and discontinuities in the predicted curves are not relected in experimental data, which tend to be smoother and more continuous. For the off-axis shear test described in Figure 4.7, the applied shear stress, τxy, generates the following biaxial stress state along the principal material axes according to Equation 2.31: σ 1 = 2τ xy cos θ sin θ σ 2 = −2τ xy cos θ sin θ (4.4) τ12 = τ xy (cos 2 θ − sin 2 θ) The importance of the sign of the applied shear stress in the interpretation of test results may not be so obvious here, and further discussion Strength of a Continuous Fiber-Reinforced Lamina (a) 151 (b) θ θ τxy τxy σ2 σ1 σ2 σ1 FIGURE 4.7 Off-axis shear test of a unidirectional lamina specimen. (a) Positive τxy at θ = 45° and resulting stresses along 1,2 axes and (b) negative τxy at θ = 45° and resulting stresses along 1,2 axes. is warranted. For example, if the angle θ = 45°, Equation 4.4 reduces to σ1 = τxy, σ2 = −τxy, and τ12 = 0. Thus, a positive applied shear stress, τxy, would produce longitudinal tension and transverse compression along the principal material axes, as shown in the lower part of Figure 4.7a. On the other hand, a negative applied shear stress would produce longitudinal compression and transverse tension, as shown in the lower part of Figure 4.7b. Given the fact that the transverse tensile strength is so much lower than the other strengths (Table 4.1), the importance of the sign of the applied off-axis shear stress should now be obvious. It is easy to visualize a situation, where a negative shear stress of a certain magnitude could cause transverse tensile failure, whereas a positive shear stress of the same magnitude would not cause failure. A similar development for pure shear along the principal material axes shows that the sign of the shear stress makes no difference in that case. Similarly, recall from elementary mechanics of materials that the sign of the shear stress also has no effect on the failure of isotropic materials. The importance of the sign of the shear stress for orthotropic materials extends beyond the interpretation of tests results as described here; it has implications for all phases of stress analysis in composite materials. 4.2.2 Maximum Strain Criterion In 1967, Waddoups [29] proposed the maximum strain criterion for orthotropic laminae as an extension of the maximum normal strain theory (or Saint Venant’s theory) for isotropic materials, which is also discussed in elementary mechanics of materials courses [25]. This criterion predicts failure when any principal material axis strain component exceeds the corresponding Principles of Composite Material Mechanics 152 ultimate strain. In order to avoid failure according to this criterion, the following set of inequalities must be satisied: − eL( − ) < ε1 < eL( + ) − eT( − ) < ε 2 < eT( + ) (4.5) |γ 12|< eLT where the numerical values of eL(− ) and eT(− ) are assumed to be positive and the ultimate strains are all engineering strains as deined by Equation 4.1. As with the maximum stress criterion, it is assumed that shear failure along the principal material axes is independent of the sign of the shear strain γ12. Due to the similarity of Equations 4.5 and 4.2, the failure surface for the maximum strain criterion in ε1, ε2 space is a rectangle similar to that of the maximum stress criterion in σ1, σ2 space. In σ1, σ2 space, however, the maximum strain criterion failure surface is a skewed parallelogram, as shown in Figures 4.3 and 4.4. The shape of the parallelogram can be deduced by combining the lamina stress–strain relationships in Equation 2.24, with the relationships given in Equation 4.1. For example, the limiting strain associated with the positive 1 direction is ε1 = sL(+ ) σ 1 ν12σ 2 = − E1 E1 E1 (4.6) σ 1 − sL(+ ) ν12 (4.7) Therefore, σ2 = which is the equation of a straight line having intercept (sL(+ ), 0) and slope 1/ν12 (Figure 4.3). A similar development using the limiting strain along the positive 2 direction yields the equation σ 2 = ν21σ 1 + sT(+ ) (4.8) which is the equation for a straight line having intercept (0, sT(+ )) and slope ν21. These lines form the right and top sides, respectively, of the parallelogram shown in Figure 4.3, and similar consideration of the limiting strains in the negative 1 and 2 directions yields equations for the remaining two sides. It should be noted, however, that depending on the magnitudes of the lamina strengths and stiffnesses, the intercepts of the maximum strain criterion parallelogram may not be the same as those of the maximum stress criterion rectangle in stress space. For some materials, the lines deining the Strength of a Continuous Fiber-Reinforced Lamina 153 top and bottom of the maximum strain criterion parallelogram intercept the horizontal axis at stresses less than the measured tensile and compressive longitudinal strengths, which contradicts experimental evidence [5,8]. According to Wu [5], such contradictions develop as a result of an ambiguous conversion from strain space to stress space unless certain mathematical constraints on the properties are satisied. Only for isotropic materials, the intercepts are always the same for the maximum stress and maximum strain criteria. As with the maximum stress criterion, the maximum strain criterion does not account for possible interaction between stress components, and the predicted failure surface does not show good agreement with experimental biaxial failure data for graphite/epoxy in Figure 4.4. Off-axis uniaxial test data have led to similar conclusions [28], but both criteria are still used for orthotropic materials because the resulting equations are relatively simple. 4.2.3 Quadratic Interaction Criteria The so-called quadratic interaction criteria also evolved from early failure theories for isotropic materials, but they differ from the maximum stress and maximum strain criteria in that they include terms to account for interaction between the stress components, and the quadratic forms of the equations for plane stress lead to elliptical failure surfaces. As shown in any mechanics of materials book, the maximum distortional energy criterion or von Mises criterion (circa early 1900s) is the most widely used quadratic interaction criteria for predicting the onset of yielding in isotropic metals [25]. In 1948, Hill [30] suggested that the von Mises criterion could be modiied to include the effects of induced anisotropic behavior in initially isotropic metals during large plastic deformations. For a general three-dimensional (3D) state of stress along the principal axes of anisotropy (the 123 axes) in such a material, the failure surface (or yield surface) for the Hill criterion in σ1, σ2, σ3 space is described by the equation 2 A(σ 2 − σ 3 )2 + B(σ 3 − σ 1 )2 + C(σ 1 − σ 2 )2 + 2Dτ 223 + 2Eτ 231 + 2F τ12 =1 (4.9) where A, B, C, D, E, and F are determined from yield strengths in uniaxial or shear loading. In order to avoid failure, the left-hand side of Equation 4.9 must be <1, and failure is predicted if the left-hand side is ≥1. For a uniaxial test along the 1 direction with σ1 = Y1 and all other stresses equal to zero, Equation 4.9 reduces to B+C = 1 Y12 (4.10) where Yl is the yield strength along 1 direction. Similarly, uniaxial tests along the 2 and 3 directions give the equations Principles of Composite Material Mechanics 154 A+C = 1 1 ; A+B = 2 Y22 Y3 (4.11) where Y2 and Y3 are the uniaxial yield strengths along the 2 and 3 directions, respectively. The yield strengths in tension and compression are assumed to be the same. Solving Equations 4.10 and 4.11 simultaneously for A, B, and C, we ind that 2A = 1 1 1 + − Y22 Y32 Y12 2B = 1 1 1 + − Y32 Y12 Y22 2C = 1 1 1 + 2− 2 2 Y1 Y2 Y3 (4.12) Similarly, for pure shear tests along the 23, 31, and 12 planes, Equation 4.9 gives 2D = 1 1 1 ; 2E = 2 ; 2F = 2 2 Y23 Y31 Y12 (4.13) where Y12, Y23, and Y31 are the yield strengths in shear associated with the 12, 23, and 31 planes, respectively. The extension of the Hill criterion to prediction of failure in an orthotropic, transversely isotropic lamina was suggested by Azzi and Tsai [31] and Tsai [32]; the resulting equation is often referred to as the Tsai–Hill criterion. If the 123 directions are assumed to be the principal material axes of the orthotropic transversely isotropic lamina, with the 1 direction being along the reinforcement direction, if plane stress is assumed (σ3 = τ31 = τ23 = 0), and if Hill’s anisotropic yield strengths are replaced by the corresponding effective lamina strengths, then Y1 = sL, Y2 = Y3 = sT, and Y12 = sLT, and Equations 4.9, 4.12, and 4.13 reduce to the equation for the Tsai–Hill failure surface: 2 σ 12 σ 1σ 2 σ 22 τ12 − 2 + 2 + 2 =1 2 sL sL sT sLT (4.14) As with the Hill equation, failure is avoided if the left-hand side of Equation 4.14 is <1, and failure is predicted if the left-hand side is ≥l. The failure surface generated by this equation is an ellipse, as shown in Figure 4.3. The ellipse shown in Figure 4.3 is symmetric about the origin because of the assumption of equal strengths in tension and compression. The Tsai–Hill Strength of a Continuous Fiber-Reinforced Lamina 155 equation can be used when tensile and compressive strengths are different by simply using the appropriate value of sL and sT for each quadrant of stress space. For example, if σ1 is positive and σ2 is negative, the values of sL(+ ) and sT(− ) would be used in Equation 4.14. The resulting failure surface is no longer symmetric about the origin, as shown for the case of graphite/epoxy in Figure 4.4. Although such a procedure is inconsistent with the assumptions used in formulating the original von Mises and Hill criteria, it has been successfully used for some composites [25,32]. As shown in Figure 4.4, the procedure seems to work reasonably well for the graphite/epoxy material except for the fourth quadrant of stress space. One way to account for different strengths in tension and compression is to include terms that are linear in the normal stresses σ1, σ2, and σ3, as suggested by Hoffman [33]. The off-axis tensile test can also be used to evaluate the Tsai–Hill criterion. When the off-axis stress transformation Equation 4.3 is substituted into Equation 4.14, the resulting off-axis failure stress is 1/2 1 σx = 2 4 2 2 2 2 4 2 (cos θ/sL ) + (1/sLT ) − (1/sL ) sin θ cos θ + (sin θ/sT ) ( ) (4.15) and the corresponding curve of σx versus θ is shown in Figure 4.8. Note that Equation 4.15 yields a single continuous curve in Figure 4.8, which varies from σx = sL when θ = 0° to σx = sT when θ = 90°, as opposed to the three separate curves produced by the maximum stress criterion in Figure 4.6. Experimental data tend to follow continuous curves such as the one in Figure 4.8 more closely than the discontinuous curves of Figure 4.6. In addition to the previously mentioned limitations of the quadratic interaction criteria based on the von Mises model, there is another problem. Since the von Mises and Hill criteria are phenomenological theories for the prediction of yielding in ductile metals, the equations are based on principal stress sL Equation 4.15 σx sT 0° 45° 90° θ FIGURE 4.8 Predicted values of off-axis uniaxial tensile strength for various off-axis iber orientations according to the Tsai–Hill criterion. Principles of Composite Material Mechanics 156 differences and the corresponding shear stresses and strains that drive slip and dislocation movement in metallic crystals. Experimental evidence suggests that a hydrostatic state of stress does not cause the slip and dislocation movements that are associated with yielding, and the Hill criterion predicts that failure will never occur under a hydrostatic state of stress σ1 = σ2 = σ3, and τ12 = τ23 = τ31 = 0. Due to shear coupling, however, a hydrostatic state of stress in an anisotropic material can produce shear strains and failure. Hoffman’s equation [33], by virtue of its linear terms, could predict failure for the hydrostatic state of stress. However, all these theories turn out to be special cases of a more general quadratic interaction criterion, which will be discussed next. In 1971, Tsai and Wu [34] proposed an improved and simpliied version of a tensor polynomial failure theory for anisotropic materials that had been suggested earlier by Gol’denblat and Kopnov [35]. In the Tsai–Wu general quadratic interaction criteria, the failure surface in stress space is described by the tensor polynomial: Fiσ i + Fijσ iσ j = 1 (4.16) where the contracted notation i, j = 1, 2, …, 6 is used, and Fi and Fij are experimentally determined strength tensors of the second and fourth rank, respectively. In order to avoid failure, the left-hand side of Equation 4.16 must be <1, and failure is predicted when the left-hand side is ≥1. For the case of plane stress with σ3 = σ33 = 0, σ4 = τ23 = 0, and σ5 = τ31 = 0, Equation 4.16 becomes F11σ 12 + F22σ 22 + F66σ 62 + F1σ 1 + F2σ 2 + 2F12σ 1σ 2 = 1 (4.17) where the linear terms in the shear stress σ6 = τ12 have been dropped because the shear strength along the principal material axes is not affected by the sign of the shear stress. Thus, only a quadratic term in the shear stress σ6 remains. However, the linear terms in the normal stresses σ1 = σ11 and σ2 = σ22 are retained because they take into account the different strengths in tension and compression. In addition, the term 2F12σ1σ2 takes into account interaction between the normal stresses. With the exception of Fl2, all the strength tensors in Equation 4.17 can be expressed in terms of the uniaxial and shear strengths using the same approach that was used with the Hill criterion. For example, for the tension and compression tests with uniaxial stresses σ 1 = sL(+ ) and σ 1 = sL(− ) , respectively, simultaneous solution of the two equations resulting from Equation 4.17 yields F11 = 1 s s (+ ) (−) L L and F1 = 1 (+ ) L s − 1 (−) L s (4.18) where the numerical value of sL(− ) is assumed to be positive as in Table 4.1. From similar uniaxial and shear tests, it can be shown that Strength of a Continuous Fiber-Reinforced Lamina F22 = 1 1 1 1 ; F2 = ( + ) − ( − ) ; F66 = 2 sT( + )sT( − ) sT sT sLT 157 (4.19) where the numerical value of sT(− ) is assumed to be positive. In order to ind the interaction parameter, F12, it is necessary to use a biaxial test involving both σ1 and σ2. For example, an expression for F12 can be obtained by substituting the biaxial stress conditions σ1 = σ2 = P and σ6 = 0 into Equation 4.17, where P is the biaxial failure stress [34]. Thus, to ind F12 for this condition, we need to know P in addition to the previously deined uniaxial and shear failure stresses. There is no a priori reason that σ1 must equal σ2, however. Indeed, as pointed out by Hashin [3], F12 can have four different values, because there are four different failure pairs σ1, σ2. Wu [5,36] has suggested that in order to determine F12 accurately, the biaxial ratio B = σ1/σ2 must be optimized to account for the sensitivity of F12 to experimental scatter in the applied stresses. The optimization procedure is complicated, however, and the reader is referred to the articles by Wu [5,36] for details. The Tsai–Wu failure surface for graphite/epoxy shown in Figure 4.4 was based on such an optimization procedure for Fl2. In Figure 4.4, the agreement with experimental data seems to be much better for the Tsai–Wu failure surface than for the others, particularly in the fourth quadrant. More recently, Tsai and Hahn [37] have proposed the equation F12 = − ( F11F22 )1/2 2 (4.20) which causes Equation 4.17 to take on the form of a generalized von Mises criteron for the yielding of isotropic materials. It is also interesting to note that Equation 4.17 reduces to Equation 4.14, the Tsai–Hill criterion, when the tensile and compressive strengths are assumed to be equal and F12 = − 1 2sL2 (4.21) On the basis of the quantitative evaluation procedure used in the previously mentioned WWFE [13–23], the organizers of the exercise selected what they considered to be the best ive of the original 19 failure theories with regard to recommended use by designers. The predicted failure surfaces for the ive selected criteria are compared with experimental test results for unidirectional E-glass/epoxy materials under the biaxial normal stresses σx and σy in Figure 4.9 and under combined transverse normal stresses σy and in-plane shear stresses τxy in Figure 4.10. In Figures 4.9 and 4.10, the notations Zinoviev, Bogetti, Tsai, Puck, and Cuntze refer to the following failure criteria: Principles of Composite Material Mechanics 158 Zinoviev et al. [38,39] used the maximum stress criterion (i.e., Equation 4.2) to predict failure of a single lamina. Linear elastic behavior was assumed up to initial failure. For laminate failure prediction, additional features were included after irst ply failure. Bogetti et al. [40,41] employed a 3D version of the maximum strain criterion (i.e., Equation 4.5 is for the 2D version only). Linear elastic behavior was assumed up to initial failure in the normal stress– normal strain relationships, but nonlinear shear stress–shear strain behavior was assumed. Additional features including progressive lamina failure were included for laminate analysis. Tsai et al. [42,43] used the Tsai–Wu criterion (i.e., Equation 4.17) and assumed linear elastic behavior up to initial ply failure. For laminate failure prediction, a progressive failure analysis feature was added. Puck and Schurmann [44,45] and Cuntze et al. [46,47] employed similar 3D progressive failure theories, which are beyond the scope of this book. From Figures 4.9 and 4.10, the organizers of the WWFE observed that the predictions of Tsai, Puck, and Cuntze gave the best overall agreement with available experimental data [19]. However, the Tsai predictions were believed to be potentially unconservative in the compression–compression quadrant of Figure 4.9, where there is a lack of experimental data. The Puck predictions appeared to be unconservative in the tension–compression of SR = σc /σy 200 σy MPa 100 SR = SR = 32:1 7.8:1 0 −100 1 −14:– SR = −200 −300 −1800 SR = SR 1 :– 3.7 −1200 −600 Tsai Puck 0 σx MPa Zinoviev Bogetti 600 =8 .83: 1200 –1 1800 Cuntze Experiments FIGURE 4.9 Comparison of predicted and measured biaxial failure surface for unidirectional E-glass/ epoxy laminae under combined normal stresses in directions parallel (σx) and perpendicular (σy) to the ibers. (Reprinted from Composites Science and Technology, 64(3–4), Soden, P. D., Kaddour, A. S., and Hinton, M. J., Recommendations for designers and researchers resulting from the world-wide failure exercise, 589–604, Copyright 2004, with permission from Elsevier.) Strength of a Continuous Fiber-Reinforced Lamina = 1: 2. 1 SR = σy: τxy SR −1 .5 SR = 100 159 τxy MPa 8:1 50 0 −150 −100 −50 σy MΓkx 0 Tsai Zinoviev Bogetti Puck Cuntze Test results 50 FIGURE 4.10 Comparison of predicted and measured failure surfaces for unidirectional E-glass/epoxy laminae under combined in-plane shear stress (τxy) and normal stress perpendicular to the ibers (σy). (Reprinted from Composites Science and Technology, 64(3–4), Soden, P. D., Kaddour, A. S., and Hinton, M. J., Recommendations for designers and researchers resulting from the world-wide failure exercise, 589–604, Copyright 2004, with permission from Elsevier.) Figure 4.9, but fared better overall in Figure 4.10. The predictions of Zinoviev and Bogetti were observed to be unconservative in several regions of both Figures 4.9 and 4.10. Finally, it was recommended that the combined theories of Tsai, Puck, and Cuntze be used in such a way that, for a given quadrant of the failure surface, the theory that produces the innermost portion of the failure surface in that quadrant should be selected for the purpose of lamina design. The development of improved multiaxial strength criteria for composites continues to be the subject of numerous publications. For example, Hashin [3,4] has suggested that for a given composite, each failure mode and its contributing stresses should be identiied, and that each of these failure modes should be modeled separately by a quadratic criterion. Tennyson et al. [48] have extended the tensor polynomial criterion to include cubic terms. Obviously, the evaluation of the strength parameters in such an equation is a formidable task. It was shown, however, that in the particular case of failure in laminated tubes under internal pressure loading, the cubic criterion is more accurate than the quadratic criterion. Although considerable progress has been made, there is still a need for systematic experimental veriication of the various theories for a variety of stress conditions. Finally, the theories discussed in this section are based on the macromechanical behavior of the composite without regard for the Principles of Composite Material Mechanics 160 micromechanical behavior of iber and matrix materials. In the next section, several micromechanical models for predicting composite strength will be presented. EXAMPLE 4.1 A generally orthotropic lamina made from E-glass/470-36 vinylester composite material has the strength properties listed in Table 4.1 and the lamina orientation is θ = 30°. If the applied stresses in the off-axis coordinate system x,y are σx = 200 MPa, σy = −100 MPa, and τxy = 100 MPa, determine whether the lamina will fail or not according to the maximum stress criterion. Solution The irst step in the analysis is to use Equation 2.31 to transform the stresses from the off-axis coordinates x,y oriented at θ = 30° to the principal material coordinates 1,2 as follows: σ x c 2 s2 σ1 2cs σ x 2 2 c −2cs σ y σ 2 = [T ] σ y = s τ −cs cs c 2 − s2 τ τ 12 xy xy 0.25 0.866 200 212 0.75 = 0.25 0.75 −0.866 −100 = −112 MPa −0.433 0.433 0.5 100 −880 Applying the maximum stress criterion, the irst two inequalities of Equation 4.2 are satisied, since σ1 = 212 MPa lies between − sL( − ) = −803 MPa and sL( + ) = 584 MPa, whereas σ2 = −112 MPa lies between − sT( − ) = −187 MPa and sT( + ) = 43 MPa. However, the third inequality in Equation 4.2 is violated, since |τ12| = 80 MPa is greater than SLT = 64 MPa. Therefore, according to the maximum stress criterion, the lamina would fail, and the governing mode of failure would be in-plane shear along the principal material axes. EXAMPLE 4.2 An element of an orthotropic lamina made of T300/5208 carbon/epoxy material is subjected to a positive off-axis shear stress, τxy, at an angle θ = 45° as shown in Figure 4.7a. Determine the value of the off-axis shear stress τxy that would cause failure according to the maximum stress criterion. Solution From Figure 4.7a, it is seen that a positive off-axis shear stress produces longitudinal tension and transverse compression along the principal material axes. Employing Equation 2.31 and the maximum stress criterion, along with the strength data for T300/5208 from Table 4.1, the calculations are as follows: Strength of a Continuous Fiber-Reinforced Lamina For failure by the longitudinal tensile stress, σ1 = 2τ xy cos θ sin θ = 2τ xy cos 45° sin 45° = τ xy = sL( + ) = 1448 MPa So the corresponding off-axis shear stress required to produce this mode of failure is τ xy = 1448 MPa For failure by the transverse compressive stress, σ 2 = −2τ xy cos θ sin θ = −2τ xy cos 45° sin 45° = − τ xy = − sT( − ) = −248 MPa So the corresponding off-axis shear stress required to produce this mode of failure is τ xy = 248 MPa There is no shear stress along the principal material axes, since τ12 = τ xy (cos 2 θ − sin 2 θ) = τ xy (cos 2 45° − sin 2 45°) = 0 So transverse compression is the governing mode of failure, and the value of the off-axis shear stress required to produce failure is τ xy = 248 MPa EXAMPLE 4.3 Repeat Example 4.2 if the off-axis shear stress in Example 4.2 is negative, as shown in Figure 4.7b. Solution From Figure 4.7b, it is seen that a negative off-axis shear stress produces longitudinal compression and transverse tension along the principal material axes. Employing Equation 2.31 and the maximum stress criterion, along with the strength data for T300/5208 from Table 4.1, the calculations are now as follows: For failure by the longitudinal compressive stress, σ 1 = −2τ xy cos θ sin θ = −2τ xy cos 45° sin 45° = − τ xy = − sL( − ) = −1448 MPa So the corresponding off-axis shear stress required to produce this mode of failure is τ xy = 1448 MPa 161 Principles of Composite Material Mechanics 162 For failure by the transverse tensile stress, σ 2 = 2τ xy cos θ sin θ = 2τ xy cos 45° sin 45° = τ xy = ST( + ) = 44.8 MPa So the corresponding off-axis shear stress required to produce this mode of failure is τ xy = 44.8 MPa Again there is no shear stress along the principal material axes, since τ12 = τ xy (cos 2 θ − sin 2 θ) = τ xy (cos 2 45° − sin 2 45°) = 0 So transverse tension is now the governing mode of failure, and the corresponding value of the off-axis shear stress required to produce failure is now only τ xy = 44.8 MPa So, simply changing the sign of the off-axis shear stress from positive to negative produces a completely different mode of failure and a much lower failure stress. EXAMPLE 4.4 The ilament-wound pressure vessel described in Example 2.5 is fabricated from E-glass/epoxy having the lamina strengths listed in Table 4.1. Determine the internal pressure p, which would cause failure of the vessel according to (a) the maximum stress criterion and (b) the Tsai–Hill criterion. Solution The irst step in the application of both theories is to determine the stresses along the principal material axes. From the results of Example 2.5, σ1 = 20.5 p, σ2 = 17.0 p, and τ12 = 6.0 p (all in MPa). Note that both normal stresses are positive, so that the tensile strengths should be used in the failure theories. a. For the maximum stress criterion, the three possible values of p at failure are found as follows: σ 1 = 20.5 p = sL( + ) = 1103 MPa; therefore , p = 53.8 MPa σ 2 = 17.0 p = sT( + ) = 27.6 MPa; therefore , p = 1.62 MPa τ12 = 6.0 p = sLT = 82.7 MPa; therefore, p = 13.78 MPa Strength of a Continuous Fiber-Reinforced Lamina Thus, the transverse tensile failure governs, and failure occurs irst at p = 1.62 MPa. b. For the Tsai–Hill criterion, Equation 4.14 yields 2 2 2 20.5 p ( 20.5 p)(17.0 p) 17.0 p 6.0 p + − + =1 1103 (1103)2 27.6 82.7 Solving for p, we ind that p = 1.61 MPa. Thus, for this case, the two criteria yield approximately the same result. This is not always true, however. EXAMPLE 4.5 Using the maximum strain criterion, determine the uniaxial failure stress, σx, for off-axis loading of the unidirectional lamina in Figure 4.5 if the material is AS/3501 carbon/epoxy and the angle θ = 30°. Solution First, the strains along the principal material axes must be found in terms of the applied stress, σx. On substituting the stress transformation (Equation 4.3) in the lamina stress–strain Equations 2.24 and 2.25, we ind that ε1 = 1 (cos 2 θ − ν12sin 2 θ)σ x E1 ε2 = 1 (sin 2 θ − ν21cos 2 θ)σ x E2 and γ 12 = − 1 (sin θ cos θ)σ x G12 Assuming linear elastic behavior up to failure and using the stress– strain relations in Equation 4.1, the maximum strain criterion (Equation 4.5) becomes σx < sL( + ) cos θ − ν12 sin 2 θ σx < sT( + ) sin θ − ν21 cos 2 θ σx < sLT sin θ cos θ 2 2 where only the tensile strengths have been used because σx is positive. Using the AS/3501 data in Tables 2.2 and 4.1, we ind that to avoid longitudinal tensile failure 163 Principles of Composite Material Mechanics 164 σx < 1448 MPa or σ x < 2145 MPa (0.886)2 − 0.3(0.5)2 In order to avoid transverse tensile failure, σx < 48.3 MPa or σ x < 205 MPa (0.5)2 − 0.0195(0.866)2 and to avoid shear failure, σx < 62.1 MPa or σ x < 143 MPa 0.886(0.5) Thus, according to the maximum strain criterion, the mode of failure is shear, and the applied stress at failure is σx = 143 MPa. The reader is encouraged to check that for compressive loading or other loading angles both the mode of failure and the failure stress may be different. The off-axis tensile test has been used to check the validity of the various failure criteria [27, 28]. PROBLEM 4.1 A unidirectional lamina specimen made of AS/3501 carbon/epoxy is subjected to an off-axis tensile test with θ = 45° as shown in Figure 4.5. Using the maximum stress criterion, determine (a) the value of the applied stress σx that would be required to produce longitudinal tensile failure, (b) the value of the applied stress σx that would be required to produce in-plane shear failure, (c) the value of the applied stress σx that would be required to produce transverse tensile failure, and (d) which of the failure modes described in parts (a), (b), and (c) would actually cause failure of the specimen, and why. PROBLEM 4.2 If the applied stress σx is compressive in Problem 4.1, use the maximum stress criterion to determine (a) the value of the applied stress σx that would be required to produce longitudinal compressive failure, (b) the value of the applied stress σx that would be required to produce in-plane shear failure, (c) the value of the applied stress σx that would be required to produce transverse compressive failure, and (d) which of the failure modes described in parts (a), (b), and (c) would actually cause failure of the specimen, and why. PROBLEM 4.3 An orthotropic lamina has the following properties: E1 = 160 GPa sL( + ) = 1800 MPa Strength of a Continuous Fiber-Reinforced Lamina 165 E2 = 10 GPa sL( − ) = 1400 MPa ν12 = 0.3 sT( + ) = 40 MPa G12 = 7 GPa sT( − ) = 230 MPa sLT = 100 MPa Construct the failure surfaces in the σ1 − σ2 stress space for this material according to: (a) the maximum stress criterion, (b) the maximum strain criterion, and (c) the Tsai–Hill criterion. PROBLEM 4.4 Using the material properties from Problem 4.3 and assuming that the stiffnesses are the same in tension and compression, determine the allowable off-axis shear stress, τxy, at θ = 45° (refer to Figure 4.7) according to: (a) the maximum stress criterion, (b) the maximum strain criterion, and (c) the Tsai– Hill criterion. Compare and discuss the results and check both positive and negative values of τxy. PROBLEM 4.5 An element of a balanced orthotropic lamina is under the state of stress shown in Figure 4.11. The properties of the lamina are: E1 = E2 = 7 0 GPa sL( + ) = sL( − ) = sT( + ) = sT( − ) = 560 MPa ν12 = ν21 = 0.25 sLT = 25 MPa G12 = 5 GPa 50 MPa 2 y 50 MPa 100 MPa 1 30° x FIGURE 4.11 Stresses acting on element of balanced orthotropic lamina. Principles of Composite Material Mechanics 166 σ2 Maximum stress (+) sT (–) sL (+) (σ1, 0) sL σ1 (–) sT Maximum strain FIGURE 4.12 Example showing that intercepts for maximum strain criterion failure surface are not always the same as those for maximum stress criterion. Using the maximum strain criterion, determine whether or not failure will occur. PROBLEM 4.6 If some of the compliances and strengths of an orthotropic lamina satisfy certain conditions, the maximum strain criterion failure surface will intercept the horizontal axis at a point like (σ1, 0) instead of at (sL( − ) , 0), as shown in Figure 4.12. Express these conditions in terms of an inequality. PROBLEM 4.7 An element of an orthotropic lamina having the properties given in Problem 4.3 is subjected to an off-axis tensile test, as shown in Figure 4.5. Using the maximum strain criterion, determine the values of σx at failure and the mode of failure for each of the following values of the angle θ: (a) 2°, (b) 30°, and (c) 75°. PROBLEM 4.8 Repeat Problem 4.7 for an off-axis compression test. PROBLEM 4.9 A material having the properties given in Problem 4.3 is subjected to a biaxial tension test, and the biaxial failure stress is found to be σ1 = σ2 = 35 MPa. Determine the Tsai–Wu interaction parameter F12 and then use the Tsai– Wu criterion to determine whether or not failure will occur for the stress condition σ1 = 100 MPa, σ2 = −50 MPa, and σ1 = 90 MPa. Strength of a Continuous Fiber-Reinforced Lamina 167 PROBLEM 4.10 The Tsai–Wu interaction parameter F12 is determined from biaxial failure stress data. One way to generate a biaxial state of stress is by using a uniaxial 45° off-axis tension test. Derive the expression for F12 based on such a test, assuming that all the uniaxial and shear strengths are known. PROBLEM 4.11 An element of an orthotropic lamina is subjected to an off-axis shear stress, τxy, as shown in Figure 4.7a. Using the Tsai–Hill criterion and assuming that the lamina strengths are the same in tension and compression, develop an equation relating the allowable value of τxy to the lamina strengths, sL, sT, and sLT, and the iber orientation θ. PROBLEM 4.12 A uniaxial off-axis tensile test is conducted as shown in Figure 4.5. Using the Tsai–Hill criterion and assuming that the lamina strengths are the same in tension and compression, develop an equation relating the applied stress, σx, to the lamina strengths sL, sT, and sLT, and the lamina orientation, θ, and (b) using the result from part (a), for a unidirectional composite having strengths sL = 1500 MPa, sT = 100 MPa, sLT = 70 MPa, and iber orientation θ = 60°, determine whether or not an applied stress σx = 200 MPa would cause failure according to the Tsai–Hill criterion. PROBLEM 4.13 An orthotropic AS/3501 carbon/epoxy lamina (see Tables 2.2 and 4.1) is subjected to the plane stress condition σx = 1000 MPa, σy = 50 MPa, and τxy = 50 MPa. If the lamina orientation is θ = 0°, will the lamina fail according to (a) the maximum stress criterion or (b) the maximum strain criterion? 4.3 Micromechanics Models for Lamina Strength In this section, the use of elementary mechanics of materials approaches to micromechanical modeling of lamina strength will be described. We should not expect such simple models for strength to be as accurate as those for stiffness, because the strength is affected more than the stiffness by material and geometric nonhomogeneity and the resulting local perturbations in the stress and strain distributions. As shown in Chapter 3, the effects of such local stress and strain perturbations on stiffness are reduced due to the smoothing effect of integration in the effective modulus theories. On the other hand, material failure is often initiated at the sites of such stress and Principles of Composite Material Mechanics 168 Average strength, 518 ksi; coeﬃcient of variation, 15% Number of tests 1600 1200 800 400 360 400 440 480 520 560 Tensile strength, ksi 600 FIGURE 4.13 Statistical distribution of tensile strength for boron ilaments. (From Weeton, J. W., Peters, D. M., and Thomas, K. L., eds. 1987. Engineers’ Guide to Composite Materials. ASM International, Materials Park, OH. Reprinted by permission of ASM International.) strain concentrations, so the effect on strength is much greater. For example, as shown in Figure 4.13 from Reference 49, the variability of strength in reinforcing ibers alone may be quite signiicant and statistical methods must be used for accurate analysis. In addition, differences between tensile and compressive modes of failure make it necessary to develop different micromechanics models for tensile strengths and compressive strengths. 4.3.1 Longitudinal Strength Simple micromechanics models for composite longitudinal tensile strength can be developed from the rule of mixtures for longitudinal stress (Equation 3.23), and the representative stress–strain curves for iber, matrix, and composite materials are shown in Figure 4.14a and b. In Figure 4.14a, the matrix (+ ) (+ ) failure strain, em1 , is assumed to be greater than the iber failure strain, ef1 , which is typical for many polymer matrix composites. A model for this case by Kelly and Davies [50] will be summarized here. Figure 4.14b shows the case where the iber failure strain is greater than the matrix failure strain, which is typical for ceramic matrix composites. A model based on the one proposed by Hull [51] will be described for this case. For both cases shown in Figure 4.14, the analyses will be developed on the assumptions of (1) equal strengths in all ibers, (2) linear elastic behavior up to failure, and (3) equal longitudinal strains in composite, iber, and matrix (recall Equation 3.26). For the case described in Figure 4.14a, the composite must fail at a strain level corresponding to the iber tensile failure strain, ef1( + ) = sf1( + )/Ef1. Theoretically, if the matrix could support the full applied load after iber failure, the strain could be increased to the matrix failure strain. For all practical purposes, Strength of a Continuous Fiber-Reinforced Lamina 169 (a) Stress (+) sf 1 (+) sL (+) sm1 Fiber failure mode Fiber Composite (υf > υcrit) Composite (υf < υcrit ) Matrix (+) sL (+) sm f1 (+) e(+) m1 ef 1 Strain (b) Stress (+) Fiber sf 1 Matrix failure mode (+) sf m1 (+) sL (+) sm1 Composite Matrix (+) em1 (+) ef 1 Strain FIGURE 4.14 Representative stress–strain curves for typical iber, matrix, and composite materials. (a) Matrix failure strain greater than iber failure strain and (b) iber failure strain greater than matrix failure strain. however, iber failure means composite failure. Thus, when the iber longi(+ ) , the matrix longitudinal tudinal stress reaches the iber tensile strength, sf1 (+ ) (+ ) stress reaches a value smf 1 = Em ef 1 , the composite longitudinal stress reaches the composite tensile strength, sL(+ ), and Equation 3.23 becomes (+ ) (+) (+ ) sL( + ) = sf( 1+ )υf + smf 1υm = sf 1 υf + smf 1 (1 − υf ) (4.22) However, Equation 4.22 only has a meaning if the iber volume fraction is suficiently large. As shown in Figures 4.14a and 4.15a, if the iber volume fraction υf < υfcrit, the composite strength from Equation 4.22 is less than the matrix strength, where Principles of Composite Material Mechanics 170 (a) (+) sf1 Strength Equation 4.22 (+) sm1 Equation 4.24 (+) smf1 0 υ fmin υ fcrit 1.0 Fiber volume fraction (b) (+) sf1 Strength Equation 4.27 (+) sfm1 (+) sm1 Equation 4.26 0 υ fmin Fiber volume fraction FIGURE 4.15 Variation of composite longitudinal tensile strength with iber volume fraction for composite having (a) matrix failure strain greater than iber failure strain and (b) iber failure strain greater than matrix failure strain. υfcrit = (+ ) (+ ) sm1 − smf1 (+ ) (+ ) sf1 − smf1 (4.23) Once the ibers fail in composites having υf < υfcrit, however, the remaining cross-sectional area of matrix that can support the load is such that (+ ) (+ ) sL( + ) = sm1 υm = sm1 (1 − υf ) (4.24) As shown in Figure 4.15a, Equations 4.22 and 4.24 intersect at υfmin = (+ ) (+ ) sm1 − smf 1 (+ ) (+ ) sf( 1+ ) − smf 1 + sm 1 (4.25) For practical composites, however, υfcrit, is generally less than 5%. Since υfmin < υfcrit, both of these values must be much smaller than the actual Strength of a Continuous Fiber-Reinforced Lamina 171 volume fraction of the composite, and the composite longitudinal strength for the case of Figure 4.14a would therefore be given by Equation 4.22. For the case described in Figure 4.14b, composite failure may be deined in two ways, depending on whether we choose to use iber failure or matrix failure as the criterion. If matrix failure is the criterion, composite failure will occur at the strain level corresponding to the matrix tensile failure strain, (+ ) (+ ) eml . Thus, when the matrix stress reaches the matrix tensile strength, sml , the (+ ) (+ ) iber stress reaches the value sfm1 = Ef 1em1 , the composite stress reaches the composite strength, sL(+ ) , and Equation 3.23 becomes (+ ) (+ ) sL( + ) = sfm1 υf + sm1 (1 − υf ) (4.26) As with Equation 4.22, this equation only has a physical meaning for a certain range of iber volume fractions. As shown in Figure 4.14b, if the ibers could still withstand additional loading after matrix failure, the iber strain may reach the iber failure strain, efl(+ ) . Due to the matrix failure, however, the remaining load-bearing area of ibers is such that the composite strength is now given by sL( + ) = sf1( + ) υf (4.27) As shown in Figure 4.15b, Equations 4.26 and 4.27 intersect at υfmin = (+ ) sm1 (+ ) (+) sf1( + ) − sfm1 + sm1 (4.28) Thus, for υf < υfmin, the composite strength would be given by Equation 4.26, and for υf > υfmin, the composite strength would be given by Equation 4.27. For practical composites, however, υfmin is much smaller than the actual iber volume fraction, so the composite longitudinal strength for the case of Figure 4.14b would be given by Equation 4.27. Of the three assumptions made at the beginning of this section, the weakest one is that all ibers in the composite have the same strength, sfl(+ ) . As shown in Figure 4.13, iber strength is not uniform, and some ibers fail at stresses well below the ultimate composite strength. In addition, iber strength decreases with increasing iber length due to the increased probability of imperfections in the iber. Various statistical models have been proposed for the sequence of events beginning with the irst iber failure and culminating with overall composite failure [52,53]. Such analyses are beyond the scope of this book, however, and the reader is referred to the article by Rosen [54] for a review of the various models. While the assumption regarding linear elastic behavior up to failure is not valid for many ductile matrix materials, the errors generated by this assumption are believed to be small. For example, the contribution of the matrix 172 Principles of Composite Material Mechanics strength to the composite strength in Equation 4.22 is small, and the matrix strength does not appear at all in Equation 4.27. If the matrix has yielded before or during iber failure, the term smi in Equations 4.22, 4.23, and 4.25 can be replaced by the matrix yield strength, sy. Excellent agreement has been reported between Equation 4.22 modiied in this way, and experimental results for a tungsten iber/copper matrix system over a wide range of iber volume fractions [55]. It has long been assumed that the models for longitudinal tensile strength cannot be used for longitudinal compressive strength, because the modes of failure are different. This assumption has been supported by observed differences in measured tensile and compressive strengths, as shown in Table 4.1. Accurate measurement of the intrinsic compressive strength has proved to be very dificult, however, and test results to date typically depend on specimen geometry and/or test method. Whitney [56] has pointed out that the failure mode is the key issue because different compression test methods may produce different failure modes. Whether the failure mode in the test is the same as the failure mode in the composite structure being designed is another question. There appears to be three basic longitudinal compression failure modes, which are shown schematically in Figure 4.16: 1. Microbuckling of ibers in either shear or extensional mode 2. Transverse tensile rupture due to Poisson strains 3. Shear failure of ibers without buckling Variations on these basic mechanisms have also been observed. For example, the shear mode of iber microbuckling (Figure 4.16) often leads to “shear crippling” due to kink band formation [51,57]. Although these problems make it dificult to assess the accuracy of various micromechanics models for compressive strength, several representative models will be summarized. Mechanics of materials models for local buckling or microbuckling of ibers in the matrix have been developed by Rosen [58] and Schuerch [59]. It is assumed that iber buckling occurs in either the extensional mode, where ibers buckle in an out-of-phase pattern and the matrix is extended or compressed, or the shear mode, where ibers buckle in an in-phase pattern and the matrix is sheared (Figure 4.16). 2D models were used, with the ibers represented as plates separated by matrix blocks. By the energy method, the work done by external forces during deformation, W, is equal to the corresponding change in the strain energy of the ibers, ΔUf, plus the change in the strain energy of the matrix, ΔUm: ∆U f + ∆U m = W (4.29) Assuming a sinusoidally buckled shape, the buckling stress (or compressive strength) for the extensional, or out-of-phase mode, was found to be Strength of a Continuous Fiber-Reinforced Lamina Shear mode 173 Extensional mode Fiber microbucking Transverse tensile rupture due to Poisson strains Shear failure without buckling FIGURE 4.16 Three possible failure modes for longitudinal compressive loading of a unidirectional composite. υE E sL( − ) = 2υf f m f1 3(1 − υf ) 1/2 (4.30) whereas the buckling stress for the shear, or in-phase mode, was found to be sL( − ) = Gm (1 − υf ) (4.31) Principles of Composite Material Mechanics 174 The extensional mode turns out to be important only for very low iber volume fractions, where it predicts the lowest buckling stress and is not important for practical composites (Figure 4.17). While the shear mode gives the lowest buckling stress over the range of practical iber volume fractions, it overpredicts considerably by comparing with test results. One way to reduce the buckling stress predicted by Equation 4.31 is to take into account the possible inelastic deformation of the matrix material by using a reduced value of the matrix shear modulus, Gm, but predictions still tend to be too high. The nonlinear model of Hahn and Williams [57] includes the effects of initial iber curvature and material nonlinearity, and reasonable predictions of compressive strength for graphite/epoxy were reported. Greszczuk [60] has shown that if the matrix shear modulus is high enough, the mode of failure shifts from microbuckling to compressive failure of the reinforcement. Since advanced composites tend to have high-modulus matrix materials, this may explain why attempts to apply microbuckling failure theories to these materials have not succeeded. For such cases, Greszczuk recommended that (−) (+ ) . It should be added, however, Equation 4.22 be used with sf1 in place of sf1 that this conclusion was based on tests of laminates consisting of aluminum sio Ex ten Longitudinal compressive strength, s L(–) MPa n 104 Shear Em = 3.45 GPa stic Ela Inelastic 0.69 GPa 103 Em = 3.45 GPa (+) e m = 0.05 0.69 GPa (+) e m = 0.02 102 101 Experimental points Transverse tensile rupture Fiber microbuckling 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 Fiber volume fraction FIGURE 4.17 Variation of predicted compressive strength of glass/epoxy with iber volume fraction for iber microbuckling and transverse tensile rupture modes of failure. (Agarwal, B. D. and Broutman, L. J. Analysis and Performance of Fiber Composites, 2nd ed., 1990. Copyright Wiley-VCH Verlag GmbH & Co. KGaA. New York, NY. Reproduced with permission.) Strength of a Continuous Fiber-Reinforced Lamina 175 strips bonded together with urethane or epoxy resins. The dificulty in (−) measurement of iber compressive strength, sfT , may preclude the use of this model for iber composites. A model for transverse tensile rupture due to Poisson strains (Figure 4.16) has been presented by Agarwal and Broutman [61]. The model is based on the application of the maximum strain criterion to the tensile transverse Poisson strain under longitudinal compressive loading. Under the applied longitudinal stress, σ1, the resulting transverse Poisson strain is ε 2 = − ν12ε1 = − ν12 σ1 E1 (4.32) Thus, when the Poisson strain ε 2 = eT(+ ) , the corresponding longitudinal stress is σ 1 = − sL(− ) , and the compressive strength is sL( − ) = E1eT( + ) ν12 (4.33) As shown in Figure 4.17, Equation 4.33 shows better agreement with measured compressive strengths of glass/epoxy than the microbuckling theories do [61]. Failure of the ibers in direct shear due to the maximum shear stress τ max = sL( − )/2 at an angle of 45° to the loading axis is a third possible failure mode under longitudinal compression (Figure 4.16). Hull [51] reports good agreement with experimental data for graphite/epoxy when the maximum shear stress is given by a rule of mixtures, so that the compressive strength is sL( − ) = 2(sf 12υf + sm12υm ) (4.34) where sf12 and sm12 are the shear strengths of iber and matrix, respectively. The direct shear mode of failure for graphite/epoxy has been reported in several other publications as well [62,63]. For example, Crasto and Kim [63] have used a novel mini-sandwich beam to attain shear failure of the ibers in the composite facing without buckling—the resulting compressive strengths are much higher than those obtained with conventional compression testing. A number of other factors have been shown to affect longitudinal compressive strength, and this continues to be a very active research area. For example, although the iber/matrix interfacial strength does not appear in any of the equations presented here, it would appear to be very important in the case of transverse tensile rupture due to Poisson strains. The experiments of Madhukar and Drzal [64] have shown that the compressive strength of graphite/epoxy is strongly related to the interfacial shear strength, and that iber surface treatments that improve the interfacial shear strength also improve the compressive strength. Principles of Composite Material Mechanics 176 4.3.2 Transverse Strength Since failure of the lamina under transverse tension occurs at such low stresses (Table 4.1), this mode of failure is often the irst to occur. In laminates, the so-called “irst ply failure” is generally due to transverse tension. The low value of the transverse tensile strength, sT(+ ) , and the corresponding transverse failure strain, eT(+ ) , are due to strain concentration in the matrix around the ibers, as shown in Equation 4.35: eT( + ) = (+ ) e( + ) em2 = m F F (4.35) (+ ) (+ ) where em2 = em , the matrix tensile failure strain (matrix is assumed to be isotropic) and F is the strain concentration factor (F > 1). Thus, the strain concentration causes the composite transverse tensile failure strain to be less than the matrix failure strain. The strain concentration factor is more appropriate than the stress concentration factor here because the stress–strain relationships for transverse loading are often nonlinear, relecting the nonlinear behavior of many matrix materials. However, if linear behavior to failure can be assumed, the corresponding transverse strength is sT( + ) = (+ ) E2sm Em F (4.36) It is assumed here that the iber is perfectly bonded to the matrix, and so in composites having poor interfacial strength, the composite transverse strength would be less than that predicted by Equation 4.36. For example, de Kok and Peijs [65] conducted experiments and incorporated an interfacial model in a inite element micromechanics model to show that, although the iber/matrix interface does not affect the transverse modulus, it has a signiicant effect on the transverse strength. More speciically, it was found that the transverse strength increases in proportion to the interfacial bond strength when the interfacial bond failure is the dominant mode of failure, but this proportionality does not hold when matrix failure dominates. A mechanics of materials approximation for the strain concentration factor has been developed by Kies [66], who considered an element in a transversely loaded lamina, as shown in Figure 4.18a. For the shaded strip shown in Figure 4.18a, the total elongation is found by summing the deformations in the iber and matrix δc2 = δf2 + δm2 = s εc2 = d εf2 + (s − d) εm2 (4.37) Strength of a Continuous Fiber-Reinforced Lamina (a) Fiber 177 Matrix σc2 σc2 d s (b) d d s τc12 τc12 Matrix Fiber FIGURE 4.18 (a) Mechanics of materials model for strain concentration under transverse loading. (b) Mechanics of materials model for strain concentration under in-plane shear loading. where the symbols are deined in Section 3.2.2 and Figure 4.18a. For the series arrangement of iber and matrix materials in the shaded strip, it is assumed that the stresses in composite, matrix, and iber are equal and that each material satisies Hooke’s law (Equation 3.38), as in Section 3.2.2. Equation 4.37 can then be written as E s εc2 = d m2 + s − d εm2 Ef2 (4.38) which can be rearranged to give the expression for the strain concentration factor F= εm 1 = εc2 (d/s) (Em /Ef2 ) − 1 + 1 (4.39) Principles of Composite Material Mechanics 178 where the subscript “2” for matrix properties has been dropped due to the assumption of isotropy. Recall from Equations 3.14 and 3.16 that the ratio of iber diameter to iber spacing, d/s, is related to the iber volume fraction, υf. For example, from substitution of the properties listed in Equation 3.33 in Equations 3.16 and 4.39, the strain concentration factor for a triangular array of E-glass ibers in an epoxy matrix (υf = 0.45) is F = 3.00. This value is in good agreement with experimentally determined values based on the ratio of matrix failure strain to transverse composite failure strain or the ratio of matrix yield strain to transverse composite yield strain [67]. A slightly higher value is predicted by a inite difference solution of the theory of elasticity model [68]. It is important to note that according to Equation 4.39, the strain concentration factor increases with increasing υf and increasing Ef2. For example, the variation of F with iber volume fraction is shown in Figure 4.19 for Em /Ef2 ≪ 1 [69]. The sharp rise in F for υf > 0.6 is particularly noteworthy. Thus, as we strive to improve the composite longitudinal properties by using higher iber volume fractions and higher modulus ibers, we pay the penalty of lower composite transverse strength. The same method outlined above can be used to estimate the transverse compressive strength, sL(− ), by replacing the tensile strains or strengths with the corresponding compressive strains or strengths. Alternatively, the corresponding matrix strength can be used as an upper bound on the composite strength, but the actual composite strength would be lower because γc12 Strain concentration factor, F or Fs 50 σc2 s 40 s εc2 30 20 10 0 0.2 0.6 0.4 Fiber volume fraction, υf 0.8 FIGURE 4.19 Variation of strain concentration factor F or Fs with iber volume fraction. Valid for F when Em/Ef2 ≪ 1 and for Fs when Gm/Gf12 ≪ 1. (From Chamis, C. C. 1974. In Broutman, L. J. ed., Composite Materials, Fracture and Fatigue, Vol. 5, Chapter 3. Academic Press, New York, NY. With permission.) Strength of a Continuous Fiber-Reinforced Lamina 179 of iber/matrix interfacial bond failure, strain concentrations around ibers and/or voids, or longitudinal iber splitting [70]. While substitution of Equation 4.39 in 4.36 shows that sT(+ ) decreases with increasing υf, there is some evidence in the literature that sT(+ ) increases slightly with increasing υf. For example, de Kok and Meijer [71] studied the effect of iber volume fraction on the transverse strength of glass/epoxy using experiments and inite element micromechanical models. Experiments and a inite element micromechanical model based on the von Mises failure criterion for the epoxy matrix showed that the transverse strength of the composite increased slightly with increasing iber volume fraction (Figure 4.20), but since the transverse modulus, E2, also increases with increasing υf, the transverse failure strain decreased with increasing υf (Figure 4.21). According to the von Mises yield criterion, yielding occurs in the matrix when the equivalent axial stress or von Mises stress σ eq = 1 ( σ a − σ b )2 + ( σ b − σ c ) 2 + ( σ c − σ a ) 2 2 (4.40) reaches the uniaxial yield strength of the matrix material, where σa, σb, and σc are the three principal stresses in the matrix. The corresponding Transverse strength (MPa) 125 100 von Mises stress 75 50 Principal stress 25 0 30 40 50 60 70 Fiber volume fraction (%) 80 FIGURE 4.20 Transverse strength of E-glass/epoxy composite as a function of iber volume fraction, as measured in tension (⚬) and three-point bending (•), and predicted with the square (solid lines) and hexagonal (dotted lines) iber packing models, using a von Mises criterion and an ultimate stress criterion. (Reprinted from Composites Part A: Applied Science and Manufacturing, 30(7), de Kok, J. M. M. and Peijs, T., Deformation, yield and fracture of unidirectional composites in transverse loading: 2. Inluence of ibre-matrix adhesion, 917–932. Copyright 1999, with permission from Elsevier.) Principles of Composite Material Mechanics 180 Transverse failure strain (%) 1.5 1.0 von Mises stress 0.5 Principal stress 0.0 30 40 50 60 70 Fiber volume fraction (%) 80 FIGURE 4.21 Transverse failure strain of E-glass/epoxy composite as a function of iber volume fraction, as measured in tension (⚬) and three-point bending (•), and predicted with the square (solid lines) and hexagonal (dotted lines) iber packing models, using a von Mises criterion and an ultimate stress criterion. (Reprinted from Composites Part A: Applied Science and Manufacturing, 30(7), de Kok, J. M. M. and Peijs, T., Deformation, yield and fracture of unidirectional composites in transverse loading: 2. Inluence of ibre-matrix adhesion, 917–932. Copyright 1999, with permission from Elsevier.) predicted transverse strength decreased with increasing υf when only the ultimate principal stress in the matrix was considered in the micromechanics model. In addition, the predicted transverse strength based on the von Mises criterion was signiicantly higher than that predicted by the ultimate principal stress model (Figure 4.20). So, it appears that the predicted transverse strength based on the one-dimensional stress model described in Equations 4.35 through 4.39 is conservative by comparison with the corresponding prediction based on the actual triaxial state of stress and the von Mises failure criterion. 4.3.3 In-Plane Shear Strength The in-plane shear strength, sLT, can also be estimated using the procedure outlined in the previous section. For the shaded element shown in Figure 4.18b, the expression analogous to Equation 4.37 for the in-plane shear strain is sγ c12 = d γ f12 + (s − d)γ m12 (4.41) Strength of a Continuous Fiber-Reinforced Lamina 181 and the in-plane shear strain concentration factor is Fs = γ m12 1 = γ c12 (d/s) [(Gm12 /Gf12 ) − 1] + 1 (4.42) where γ m12 = average matrix in-plane shear strain γ c12 = average composite in-plane shear strain γ f12 = average iber in-plane shear strain Gf12 = iber in-plane shear modulus Note that this equation has the same form as Equation 4.39. Thus, Figure 4.19 also gives the variation of Fs with υf when Gm /Gf12 ≪ 1, and the previous comments regarding the effect of υf on F are also valid for Fs. The other necessary equations are obtained by replacing the tensile strains or strengths in Equations 4.35 and 4.36 with the corresponding in-plane shear strains or strengths. Again, the matrix shear strength can be used as an upper bound on the composite shear strength, as the actual composite strength would be lower for the same reasons mentioned in the previous section. 4.3.4 Multiaxial Strength Sections 4.3.1 through 4.3.3 have summarized micromechanical models for the prediction of the ive basic unidirectional lamina strengths, and most of the micromechanical strength modeling efforts have been focused in these areas. However, micromechanical models have also been used to evaluate multiaxial strength criteria such as those described in Section 4.2. For example, Zhu et al. [12] developed inite element unit cell micromechanics models and used them to evaluate the maximum stress, maximum strain and Tsai–Wu criteria as well as the combination of Tsai–Wu and maximum stress criteria for several biaxial loading conditions on a unidirectional composite. The approach was referred to as a direct micromechanics method (DMM). As shown in Figure 4.22, two types of failure criteria for the iber and matrix materials were employed in the inite element DMM for predicting failure in each element of the model: (a) maximum principal stress criterion and (b) von Mises criterion, whereas iber/matrix interfacial failure at the element level was modeled using the maximum tensile interfacial stress and the maximum interfacial shear stress. Failure envelopes were generated using the DMM and compared with the corresponding failure envelopes that were generated using the applied macromechanical stresses in the Tsai–Wu criterion, the maximum stress criterion, the maximum strain criterion, and the combined Tsai–Wu and maximum stress criteria. From all the different cases examined, it was found that the combination of the Tsai–Wu and maximum Principles of Composite Material Mechanics 182 Maximum principal stress criterion and von Mises yield criterion for fiber and matrix failure Finite element model of unit cell Maximum tensile and shear interfacial stress criteria applied for fiber/matrix interfacial failure FIGURE 4.22 Failure criteria employed in the inite element unit cells using the DMM. (Adapted from Zhu, H., Sankar, B. V., and Marrey, R. V. 1998. Journal of Composite Materials, 32(8), 766–782.) stress criteria led to the most conservative failure envelope in the biaxial stress space, and that the failure criteria for the matrix and the iber/matrix interface played dominant roles in the failure criteria for the composite. For off-axis tensile test models, the Tsai–Wu criterion showed the best agreement with the DMM approach for iber orientations in the range 0 < θ < 30°, the maximum stress criterion gave the best agreement in the range 60° < θ < 90°, and the criterion that gave the lowest strength prediction of the two criteria worked best in the range 30° < θ < 60°. In conclusion, only the basics of micromechanical strength prediction have been discussed here. More detailed micromechanics analyses of strength under other types of loading such as interlaminar shear and lexure as well as micromechanical effects of voids and residual stresses on strength have been summarized by Chamis [69]. More recently, a critical review of the state of the art in methodologies for material constitutive modeling and composite failure theories has been published by Oriici et al. [72]. EXAMPLE 4.6 Assume that experimental tensile test data is available for the longitudinal modulus, E1, of a composite and the corresponding tensile failure strain, eL(+ ). Use this information to ind an alternative to Equation 4.22 for predicting the longitudinal tensile strength, sL(+ ), of the composite when the ibers fail irst. How can this alternative expression be used to interpret the composite stress–strain curve in Figure 4.14a? Similarly, ind an alternative to Equation 4.26 for predicting sL(+ ) when the matrix fails irst and explain how it can be used to interpret the composite stress–strain curve in Figure 4.14b. Solution From Equation 4.1, sL( + ) = E1eL( + ), and for the iber failure mode, eL( + ) = ef1( + ). Thus, an alternative to Equation 4.22 is sL( + ) = E1ef( 1+ ) and E1 can be interpreted as the slope of the composite stress–strain curve in Figure 4.14a. Strength of a Continuous Fiber-Reinforced Lamina (+ ) , an alternative to Equation Similarly, for the matrix failure mode, eL( + ) = em1 (+ ) (+ ) 4.26 is sL = E1em1 and E1 can be interpreted as the slope of the composite stress–strain curve in Figure 4.14b. EXAMPLE 4.7 Determine the longitudinal and transverse tensile strengths of the carbon/epoxy material described in Examples 3.2, 3.3, and 3.6 if the tensile strengths of iber and matrix materials are 2413 and 103 MPa, respectively. Solution The iber tensile failure strain is (+ ) = ef1 (+ ) 2.413 sf1 = = 0.011 220 Ef1 The matrix tensile failure strain is (+) = em (+) 0.103 sm = = 0.03 3.45 Em Thus, the material fails as described in Figure 4.14a at a strain level of (+ ) = 0.011. Since υf = 0.506 and υm = 0.482, from Example 3.2, the comef1 posite longitudinal tensile strength is given by Equation 4.22: sL( + ) = sf1( + )υf + smf1υm = sf1( + )υf + Em ef1( + )υm = 2413(0.506) + 3450((0.011)(0.482) = 1239 MPa(180,000 psi) Note that the matrix contribution here is only 18.3 MPa out of 1239 MPa or about 1.5%. The strain concentration factor for the calculation of the transverse tensile strength is given by Equation 4.39: F= 1 1 = = 2.52 (d/s)[(Em /Ef 2 ) − 1] + 1 (0.0127/0.0158)[(3.45/13.79) − 1] + 1 If linear elastic behavior to failure can be assumed, the transverse tensile strength is given by Equation 4.36. sT( + ) = (+ ) 5.65(103) E2Sm = = 66.9 MPa(9703 psi) 3.45(2.52) Em F 183 Principles of Composite Material Mechanics 184 EXAMPLE 4.8 Determine the longitudinal tensile strength of the hybrid carbon/ aramid/epoxy composite described in Problem 3.4 and Figure 3.10 of Chapter 3 if the iber packing array is triangular with the closest possible packing. Solution For the triangular array of ibers of the same diameter with the closest possible packing, the maximum iber volume fraction is given by Equation 3.17: υfmax = π = 0.907 2 3 Therefore, the sum of the iber volume fractions of carbon and aramid ibers must be υc + υa = υfmax = 0.907 Since there are two carbon ibers for each aramid iber υc = 2υa Neglecting voids, the sum of the volume fractions for the carbon, aramid, and epoxy must be υc + υa + υe = 1 Solving the above equations simultaneously, it is found that the volume fractions for the carbon, aramid, and epoxy, respectively, are υc = 0.604, υa = 0.302, υe = 0.094 From Figure 3.10, it is seen that the carbon ibers fail irst at a strain level of 0.0054. At this strain level, the corresponding stresses in the carbon, aramid, and epoxy, respectively, are (+ ) (+ ) sc( +1 ) = 2.1 GPa, sac sec 1 = 0.72 GPa , 1 = 0.0164 GPa Finally, generalizing Equation 4.22 for the case of the hybrid composite with three constituents, we ind that the composite longitudinal tensile strength is (+ ) (+ ) sL( + ) = sc( +1 )υc + sac 1υa + sec 1υe = 2.1(0.604) + 0.72(0.302) + 0.0164(0.094) = 1.487 GPa Strength of a Continuous Fiber-Reinforced Lamina 185 PROBLEM 4.14 Determine the longitudinal tensile strength of the hybrid carbon/aramid/ epoxy composite described in Problem 3.4 and Figure 3.10 of Chapter 3 if the iber packing array is square with the closest possible packing. PROBLEM 4.15 Compare and discuss the estimated longitudinal compressive strengths of Scotchply 1002 E-glass/epoxy based on (a) iber microbuckling and (b) transverse tensile rupture. Assume linear elastic behavior to failure. For the epoxy matrix, assume that the modulus of elasticity is Em = 3.79 GPa, the Poisson’s ratio is νm = 0.35, and the iber volume fraction is υf = 0.45. PROBLEM 4.16 Using the maximum strain criterion and micromechanics, set up the equations for predicting the averaged isotropic strength of a randomly oriented continuous iber composite. Your answer should be expressed in terms of the appropriate iber and matrix properties and volume fractions, the variable iber orientation angle θ, and the appropriate strengths of the corresponding unidirectional lamina that consists of the same iber and matrix materials and volume fractions. In the micromechanics analysis, assume that the matrix failure strain is greater than the iber failure strain (i.e., that the materials behave as shown in Figure 4.14a). Deine all parameters used, but do not try to solve the equation. PROBLEM 4.17 Assuming that the failure mode for longitudinal compression of unidirectional E-glass/epoxy with iber volume fraction υf = 0.6 is a transverse tensile rupture due to Poisson strains, (a) estimate the longitudinal compressive strength of this material and (b) if the volume fraction of the material in part (a) is varied, what effect would this have on the longitudinal compressive strength? PROBLEM 4.18 For the IM-9/8551-7 carbon/epoxy composite rod design of Problem 3.3 in Chapter 3, what would be the increase in the longitudinal tensile strength compared with that of the original 6061-T6 aluminum alloy design? PROBLEM 4.19 How would the answer to Problem 1.6 in Chapter 1 change if the lywheel ring is made of IM-7/8552 carbon/epoxy composite with ibers oriented in the circumferential direction? Assume a iber volume fraction υf = 0.6. 186 Principles of Composite Material Mechanics PROBLEM 4.20 For a unidirectional IM-9/8551-7 carbon/epoxy composite under tensile loading, what is the critical iber volume fraction, υfcrit, when the mode of failure is iber failure as described in Figure 4.14a? How does this value of υfcrit compare with the typical iber volume fraction, υf, for IM-9/8551-7 as described in Table 4.1, and what is the physical meaning of this observation? References 1. Chamis, C. C. 1987. Simpliied composite micromechanics thermal and moisture-related properties. In Weeton, J. W., Peters, D. M., and Thomas, K. L., eds., Engineers’ Guide to Composite Materials, pp. 3-8–3-24. ASM International, Materials Park, OH. 2. Daniel, I. M. and Ishai, O. 1994. Engineering Mechanics of Composite Materials. Oxford University Press, New York, NY. 3. Hashin, Z. 1983. Analysis of composite materials—A survey. Journal of Applied Mechanics, 50, 481–505. 4. Hashin, Z. 1980. Failure criteria for unidirectional iber composites. Journal of Applied Mechanics, 47, 329–334. 5. Wu, E. M. 1974. Phenomenological anisotropic failure criterion. In Sendeckyj, G. P. ed., Composite Materials, Mechanics of Composite Materials, Vol. 2, pp. 353–431. Academic Press, New York, NY. 6. Sendeckyj, G. P. 1972. A brief survey of empirical multiaxial strength criteria for composites. Composite Materials: Testing and Design (Second Conference), ASTM STP 497, pp. 41–51. American Society for Testing and Materials, Philadelphia, PA. 7. Chamis, C. C. 1969. Failure criteria for ilamentary composites. Composite Materials: Testing and Design, ASTM STP 460, pp. 336–351. American Society for Testing and Materials, Philadelphia, PA. 8. Kaminski, B. E. and Lantz, R. B. 1969. Strength theories of failure for anisotropic materials. Composite Materials: Testing and Design, ASTM STP 460, pp. 160–169. American Society for Testing and Materials, Philadelphia, PA. 9. Franklin, H. G. 1968. Classical theories of failure of anisotropic materials. Fiber Science and Technology, 1(2), 137–150. 10. Tsai, S. W. 1984. A survey of macroscopic failure criteria for composite materials. Journal of Reinforced Plastics and Composites, 3, 40–62. 11. Christensen, R. M. 1997. Stress based yield/failure criteria for iber composites. International Journal of Solids and Structures, 34(5), 529–543. 12. Zhu, H., Sankar, B. V., and Marrey, R. V. 1998. Evaluation of failure criteria for iber composites using inite element micromechanics. Journal of Composite Materials, 32(8), 766–782. 13. Soden, P. D., Hinton, M. J., and Kaddour, A. S. 1998. A comparison of the predictive capabilities of current failure theories for composite laminates. Composites Science and Technology, 58(7), 1125–1254. Strength of a Continuous Fiber-Reinforced Lamina 187 14. Soden, P. D., Hinton, M. J., and Kaddour, A. S. 1998. Lamina properties, lay-up conigurations and loading conditions for a range of ibre-reinforced composite laminates. Composites Science and Technology, 58(7), 1011–1022. 15. Hinton, M. J. and Soden, P. D. 1998. Predicting failure in composite laminates: The background to the exercise. Composites Science and Technology, 58(7), 1001–1010. 16. Hinton, M. J., Kaddour, A. S., and Soden, P. D. 2002. A comparison of the predictive capabilities of current failure theories for composite laminates, judged against experimental evidence. Composites Science and Technology, 62(12–13), 1725–1797. 17. Soden, P. D., Hinton, M. J., and Kaddour, A. S. 2002. Biaxial test results for strength and deformation of a range of E-glass and carbon ibre reinforced composite laminates: Failure exercise benchmark data. Composites Science and Technology, 62(12–13), 1489–1514. 18. Hinton, M. J., Kaddour, A. S., and Soden, P. D. 2002. Evaluation of failure prediction in composite laminates: Background to “part B” of the exercise. Composites Science and Technology, 62(12–13), 1481–1488. 19. Soden, P. D., Kaddour, A. S., and Hinton, M. J. 2004. Recommendations for designers and researchers resulting from the world-wide failure exercise. Composites Science and Technology, 64(3–4), 589–604. 20. Hinton, M. J., Kaddour, A. S., and Soden, P. D. 2004. A further assessment of the predictive capabilities of current failure theories for composite laminates: Comparison with experimental evidence. Composites Science and Technology, 64(3–4), 549–588. 21. Kaddour, A. S., Hinton, M. J., and Soden, P. D. 2004. A comparison of the predictive capabilities of current failure theories for composite laminates: Additional contributions. Composites Science and Technology, 64(3–4), 449–476. 22. Hinton, M. J., Kaddour, A. S., and Soden, P. D. 2004. Evaluation of failure prediction in composite laminates: Background to “part C” of the exercise. Composites Science and Technology, 64(3–4), 321–327. 23. Hinton, M. J., Soden, P. D., and Kaddour, A. S. 2004. Failure Criteria in FibreReinforced Polymer Composites. Elsevier, London. 24. Jenkins, C. F. 1920. Report on materials of construction used in aircraft and aircraft engines. Great Britain Aeronautical Research Council, London, UK. 25. Higdon, A., Ohlsen, E. H., Stiles, W. B., Weese, J. A., and Riley, W. F. 1976. Mechanics of Materials, 3rd ed. John Wiley & Sons, New York, NY. 26. Burk, R. C. 1983. Standard failure criteria needed for advanced composites. Astronautics and Aeronautics, 21(6), 58–62. 27. Pipes, R. B. and Cole, B. W. 1973. On the off-axis strength test for anisotropic materials. Journal of Composite Materials, 7, 246–256. 28. Jones, R. M. 1999. Mechanics of Composite Materials, 2nd ed. Taylor & Francis, Philadelphia, PA. 29. Waddoups, M. E. 1967. Advanced composite material mechanics for the design and stress analyst. General Dynamics. Fort Worth Division Report FZM-4763, Fort Worth, TX. 30. Hill, R. 1948. A theory of the yielding and plastic low of anisotropic metals. Proceedings of the Royal Society of London, Series A, 193, 281–297. 31. Azzi, V. D. and Tsai, S. W. 1965. Anisotropic strength of composites. Proceedings of the Society for Experimental Stress Analysis, XXII(2), 283–288. 188 Principles of Composite Material Mechanics 32. Tsai, S. W. 1968. Strength theories of ilamentary structures. In Schwartz, R. T. and Schwartz, H. S., eds., Fundamental Aspects of Fiber Reinforced Plastic Composites, Chapter 1, pp. 3–11. Wiley Interscience, New York, NY. 33. Hoffman, O. 1967. The brittle strength of orthotropic materials. Journal of Composite Materials, 1, 200–206. 34. Tsai, S. W. and Wu, E. M. 1971. A general theory of strength for anisotropic materials. Journal of Composite Materials, 5, 58–80. 35. Goldenblat, I. and Kopnov, V. A. 1965. Strength of glass reinforced plastics in the complex stress state. Mekhanika Polimerov, 1, 70–78 (English translation: Polymer Mechanics, 1, 54–60, 1966). 36. Wu, E. M. 1972. Optimal experimental measurements of anisotropic failure tensors. Journal of Composite Materials, 6, 472–489. 37. Tsai, S. W. and Hahn, H. T. 1980. Introduction to Composite Materials. Technomic Publishing Co., Lancaster, PA. 38. Zinoviev, P., Grigoriev, S. V., Lebedeva, O. V., and Tairova, L. R. 1998. Strength of multilayered composites under plane stress state. Composites Science and Technology, 58(7), 1209–1224. 39. Zinoviev, P. A., Lebedeva, O. V., and Tairova, L. R. 2002. Coupled analysis of experimental and theoretical results of the deformation and failure of laminated composites under a plane state of stress. Composites Science and Technology, 62(12–13), 1711–1723. 40. Bogetti, T. A., Hoppel, C. P. R., Harik, V. M., Newill, J. F., and Burns, B. P. 2004. Predicting the nonlinear response and progressive failure of composite laminates. Composites Science and Technology, 64(3–4), 329–342. 41. Bogetti, T. A., Hoppel, C. P. R., Harik, V. M., Newill, J. F., and Burns, B. P. 2004. Predicting the nonlinear response and progressive failure of composite laminates: Correlation with experimental results. Composites Science and Technology, 64(3–4), 477–485. 42. Liu, K. S. and Tsai, S. W. 1998. A progressive quadratic failure criterion for a laminate. Composites Science and Technology, 58(7), 1023–1032. 43. Kuraishi, A., Tsai, S. W., and Liu, K. S. 2002. A progressive quadratic failure criterion, part B. Composites Science and Technology, 62(12–13), 1683–1695. 44. Puck, A. and Schurmann, H. 1998. Failure analysis of FRP laminates by means of physically based phenomenological models. Composites Science and Technology, 58(7), 1045–1067. 45. Puck, A. and Schurmann, H. 2002. Failure analysis of FRP laminates by means of physically based phenomenological models. Composites Science and Technology, 62(12–13), 1633–1662. 46. Cuntze, R. G. and Freund, A. 2004. The predictive capability of failure mode concept-based strength criteria for multidirectional laminates. Composites Science and Technology, 64(3–4), 343–377. 47. Cuntze, R. G. 2004. The predictive capability of failure mode concept-based strength criteria for multidirectional laminates—Part B. Composites Science and Technology, 64(3–4), 487–516. 48. Tennyson, R. C., MacDonald, D., and Nanyaro, A. P. 1978. Evaluation of the tensor polynomial failure criterion for composite materials. Journal of Composite Materials, 12, 63–75. 49. Weeton, J. W., Peters, D. M., and Thomas, K. L., eds. 1987. Engineers’ Guide to Composite Materials. ASM International, Materials Park, OH. Strength of a Continuous Fiber-Reinforced Lamina 189 50. Kelly, A. and Davies, G. J. 1965. The principles of the ibre reinforcement of metals. Metallurgical Review, 10, 1–77. 51. Hull, D. 1981. An Introduction to Composite Materials. Cambridge University Press, Cambridge, MA. 52. Rosen, B. W. 1964. Tensile failure of ibrous composites. AIAA Journal, 2, 1985–1991. 53. Zweben, C. and Rosen, B. W. 1970. A statistical theory of material strength with applications to composite materials. Journal of Mechanics and Physics of Solids, 18, 180–206. 54. Rosen, B. W. 1987. Composite materials analysis and design. In Reinhart, T. J. ed., Engineered Materials Handbook, Composites, Vol. 1, Section 4, pp. 173–281. ASM International, Materials Park, OH. 55. Holister, G. S. and Thomas, C. 1966. Fibre Reinforced Materials. Elsevier Publishing Co., Ltd., New York, NY. 56. Whitney, J. M. 1991. Failure modes in compression testing of composite materials, How Concept Becomes Reality. Proceedings of 36th International SAMPE Symposium, Vol. 36, pp. 1069–1078. Society for Advancement of Material and Process Engineering, Covina, CA. 57. Hahn, H. T. and Williams, J. G. 1986. Compression failure mechanisms in unidirectional composites. In Whitney, J. M. ed., Composite Materials: Testing and Design (Seventh Conference), ASTM STP 893, pp. 115–139. American Society for Testing and Materials, Philadelphia, PA. 58. Rosen, B. W. 1965. Mechanics of composite strengthening. In Fiber Composite Materials, Chapter 3, pp. 37–75. American Society for Metals, Metals Park, OH. 59. Schuerch, H. 1966. Prediction of compressive strength in uniaxial boron iber metal matrix composites. AIAA Journal, 4, 102–106. 60. Greszczuk, L. B. 1974. Microbuckling of lamina-reinforced composites. In Berg, C. A., McGarry, F. J., and Elliott, S. Y., eds., Composite Materials: Testing and Design (Third Conference), ASTM STP 546, pp. 5–29. American Society for Testing and Materials, Philadelphia, PA. 61. Agarwal, B. D. and Broutman, L. J. 1990. Analysis and Performance of Fiber Composites, 2nd ed. John Wiley & Sons, Inc., New York, NY. 62. Hancox, N. L. 1975. The compression strength of unidirectional carbon ibre reinforced plastics. Journal of Materials Science, 10(2), 234–242. 63. Crasto, A. S. and Kim, R. Y. 1991. Compression strengths of advanced composites from a novel mini-sandwich beam. SAMPE Quarterly, 22(3), 29–39. 64. Madhukar, M. S. and Drzal, L. T. 1990. Effect of iber–matrix adhesion on longitudinal compressive properties of graphite/epoxy composites. Proceedings of the American Society for Composites Fifth Technical Conference, pp. 849–858. Technomic Publishing Co., Lancaster, PA. 65. de Kok, J. M. M. and Peijs, T. 1999. Deformation, yield and fracture of unidirectional composites in transverse loading: 2. Inluence of ibre–matrix adhesion. Composites Part A: Applied Science and Manufacturing, 30(7), 917–932. 66. Kies, J. A. 1962. Maximum strains in the resin of iber glass composites. U.S. Naval Research Laboratory Report No. 5752. 67. Gibson, R. F. 1975. Elastic and dissipative properties of iber reinforced composite materials in lexural vibration. PhD dissertation, University of Minnesota, Minneapolis, MN. 68. Adams, D. F. and Doner, D. R. 1967. Transverse normal loading of a unidirectional composite. Journal of Composite Materials, 1, 152–164. 190 Principles of Composite Material Mechanics 69. Chamis, C. C. 1974. Micromechanics strength theories. In Broutman, L. J. ed., Composite Materials: Fracture and Fatigue, Vol. 5, Chapter 3. Academic Press, New York, NY. 70. Piggott, M. R. 1980. Load Bearing Fibre Composites. Pergamon Press Ltd., Oxford, England. 71. de Kok, J. M. M. and Meijer, H. E. H. 1999. Deformation, yield and fracture of unidirectional composites in transverse loading: 1. Inluence of ibre volume fraction and test temperature. Composites Part A: Applied Science and Manufacturing, 30(7), 905–916. 72. Oriici, A. C., Herszberg, I., and Thomson, R. S. 2008, Review of methodologies for composite material modeling incorporating failure. Composite Structures, 86, 194–210. 5 Analysis of Lamina Hygrothermal Behavior 5.1 Introduction The analytical models for composite mechanical behavior presented up to now have been based on the assumption of constant environmental conditions. Composites are usually subjected to changing environmental conditions during both initial fabrication and inal use, however, and it is important to be able to include the effects of such changes in the analysis. Among the many environmental conditions that may inluence composite mechanical behavior, changes in temperature and moisture content are singled out for discussion here because of the particularly important effects they have on polymer matrix materials and those properties of polymer composites that are matrix dominated. Effects of temperature are usually referred to as “thermal” effects, whereas those of moisture are often referred to as “hygroscopic” effects. The word “hygrothermal” has evolved as a way of describing the combined effects of temperature and moisture. There are two principal effects of changes in the hygrothermal environment on the mechanical behavior of polymer composites: 1. Matrix-dominated properties such as stiffness and strength under transverse, off-axis, or shear loading are altered. Increased temperature causes a gradual softening of the polymer matrix material up to a point. If the temperature is increased beyond the so-called “glass transition” region (indicating a transition from glassy behavior to rubbery behavior), however, the polymer becomes too soft for use as a structural material (Figure 5.1). Plasticization of the polymer by absorbed moisture causes a reduction in the glass transition temperature, Tg, and a corresponding degradation of composite properties. As shown in Figure 5.1, the glass transition temperature of the dry material is characterized by Tgo (i.e., the “dry” Tg), and when the material is fully saturated with moisture content Mm, it is characterized by Tgw (the “wet” Tg). Saturation moisture contents of 3%–4% by weight, and moisture-induced reductions in Tg on the order of 20% are typical for polymer matrix materials, as shown by 191 Principles of Composite Material Mechanics 192 Glassy region Glass transition region Dry Stiffness Wet Increasing moisture content Rubbery region Typical operating temperature below Tg for structural polymers Tgw Tgo Temperature FIGURE 5.1 Variation of stiffness with temperature for a typical polymer showing the glass transition temperature, Tg, and the effect of absorbed moisture on Tg. Note: Tg0 = dry Tg and Tgw = wet Tg. the numerical data in Table 5.1. Figure 5.1 also shows that, at a typical operating temperature below Tg, the stiffness is signiicantly reduced as the material picks up moisture. Table 5.1 shows that the maximum service temperature is typically well below Tg, as properties such as stiffness become undesirably sensitive to temperature if the service temperature gets too close to the glass transition region. 2. Hygrothermal expansions or contractions change the stress and strain distributions in the composite. Increased temperature and/ or moisture content causes swelling of the polymer matrix, whereas reduced temperature and/or moisture content causes contraction. Since the ibers are typically not affected as much by hygrothermal conditions, the swelling or contraction of the matrix is resisted by the ibers and residual stresses develop in the composite. A similar effect at the laminate level is due to differential expansions or contractions of constituent laminae. This chapter is therefore concerned with the analytical modeling of hygrothermal degradation of matrix-dominated properties and modiication of the lamina stress–strain relationships to include hygrothermal effects. Analysis of Lamina Hygrothermal Behavior 193 TABLE 5.1 Hygrothermal Properties for Various Polymer Matrix Materials Tgo (Dry) [°F (°C)] Tgw (Wet) [°F (°C)] Maximum Service Temperature (Dry) [°F (°C)] 400(204) Material Supplier Saturation Moisture Content, M m (wt.%) Hexply® F655 bismaleimide Hexcel 4.1 550(288) 400(204) Hexply® 8551-7 epoxy Hexcel 3.1 315(157) 240(116) 200(93) Hexply® 8552 epoxy Hexcel – 392(200) 309(154) 250(121) Hexply® 954-3A cyanate Hexcel – 400(204) – – CyCom® 2237 polyimide Cytec 4.4 640(338) 509(265) 550(208) CyCom® 934 epoxy Cytec – 381(194) 320(160) 350(177) Avimid® R polyimide Cytec 2.8 581(305) 487(253) 550(288) Derakane® 411-350 vinylester Ashland 1.5 250(120) – 220(105) Ultem® 2300 polyetherimide Sabic 0.9 419(215) – 340(171) Victrex 150G polyetherether-ketone Victrex plc 0.5 289(143) – 356(180) Cetex® polyphenylene sulide Tencate 0.02 194(90) – 212(100) ® Micromechanical prediction of mechanical and thermophysical properties will also be discussed because of its importance in the analytical modeling of both the effects. 5.2 Hygrothermal Degradation of Properties As evidence of hygrothermal degradation of properties, consider the data of Browning et al. [1], who tested graphite/epoxy composites and their epoxy matrix materials under various hygrothermal conditions. Figure 5.2 shows the stress–strain curves for a typical epoxy matrix material under the various combinations of temperature and absorbed moisture. The corresponding stress– strain curves for the graphite/epoxy composite under transverse loading are shown in Figure 5.3. Note that the imposed hygrothermal conditions cause substantial reductions of both strength and stiffness in both cases, with the so-called “hot–wet” conditions (combined high temperature and high moisture content) generating the most severe degradation. Similar degradation was observed in the case of in-plane shear loading of the composite since the behavior is matrix dominated in both the cases. On the other hand, the corresponding stress–strain curves for the composite under longitudinal loading showed little effect because longitudinal strength and stiffness are iber dominated. Principles of Composite Material Mechanics 194 10 250° dry 8 300° dry RT dry Stress (ksi) RT wet 6 3501-5 neat resin 250° dry 200° wet 4 250° wet Wet = 5.6% wt. gain 300° wet 2 = 24% 0 1 2 4 3 Strain (%) 5 6 7 FIGURE 5.2 Stress–strain curves for 3501-5 epoxy resin at different temperatures and moisture contents. (Reprinted from Browning, C. E., Husman, G. E., and Whitney, J. M. 1977. Composite Materials: Testing and Design: Fourth Conference, ASTM STP 617, pp. 481–496. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. With permission.) Another example of the hygrothermal sensitivity of matrix-dominated composite properties are the data of Gibson et al. [2], who used a vibrating beam method to measure the lexural moduli of several E-glass/polyester sheet-molding compounds after soaking for various times in a water bath. Table 5.2 gives a description of the materials, Figure 5.4 shows the percent weight gain due to moisture pickup, and Figure 5.5 shows the variation in modulus with soaking time. Composites having some continuous ibers and high iber content absorbed little moisture and showed negligible change in modulus with soaking time. On the other hand, composites having matrixdominated behavior (those with chopped ibers only and low iber content) exhibited the most moisture pickup and the greatest reduction in modulus. Considerable insight into the physics of temperature and moisture distribution in a material is gained from the analysis of Shen and Springer [3], who considered the one-dimensional (1D) distributions of temperature, T, and moisture concentration, c, in a plate of thickness, h, which is suddenly exposed on both sides to an environment of temperature, Ta, and moisture concentration, ca (Figure 5.6). The temperature and moisture concentration are assumed to vary only through the thickness along the z-direction and the initial temperature, Ti, and initial moisture concentration, ci, are assumed to be uniform. The temperature distribution is governed by the Fourier heat conduction equation: ρC ∂T ∂ ∂T = Kz ∂t ∂z ∂z (5.1) Analysis of Lamina Hygrothermal Behavior 195 Wet 75% R.H. = 1.05% wt. gain Wet 95% R.H. = 1.60% wt. gain R.T. dry 9 8 AS/3501-5 (90)S υf = 63% 7 Stress (ksi) 6 250° dry 300° dry R.T. 75 5 4 250° 75% 3 R.T. 95% 2 250° 95% 300° 75% 1 300° 95% 0 0 0.2 0.4 0.6 Strain (%) 0.8 1.0 FIGURE 5.3 Stress–strain curves for AS/3501-5 graphite/epoxy composite under transverse loading at different temperatures and moisture contents. (Reprinted from Browning, C. E., Husman, G. E., and Whitney, J. M. 1977. Composite Materials: Testing and Design: Fourth Conference, ASTM STP 617, pp. 481–496. American Society for Testing and Materials, Philadelphia, PA. Copyright, ASTM. With permission.) TABLE 5.2 Description of Composite Materials for Figures 5.4 and 5.5 Weight Percentages of Constituents Material Chopped E-Glass Fibers PPG SMC-R25a PPG SMC-R65 PPG XMC-3 25 65 25 OCF SMC-R25b OCF C20/R30 25 30 Continuous E-Glass Fibers 0 0 50 (±7.5°, X-pattern) 0 20 (aligned) Polyester Resin, Fillers, etc. 75 35 25 75 50 Source: From Gibson, R. F. et al. 1982. Journal of Reinforced Plastics and Composites, 1(3), 225–241. With permission. a Manufactured by PPG Industries, Fiber Glass Division, Pittsburgh, PA. b Manufactured by Owens-Corning Fiberglas Corporation, Toledo, OH. Principles of Composite Material Mechanics 196 PPG SMC-R25 PPG SMC-R65 PPG XMC-3 (L) OCF SMC-R25 OCF C20/R30 (L) Percent weight gain 3 2 1 100 200 300 400 500 600 Time (h) 700 800 900 1000 FIGURE 5.4 Percent weight gain due to moisture pickup versus soaking time for several E-glass/polyester sheet-molding compounds. Materials described in Table 5.2. (From Gibson, R. F. et al. 1982. Journal of Reinforced Plastics and Composites, 1(3), 225–241. Reprinted by permission of Technomic Publishing Co.) 50 7 40 5 30 4 GPa Modulus (106 psi) 6 3 20 2 10 1 0 100 200 300 400 500 600 Time (h) 700 800 900 1000 FIGURE 5.5 Variation of lexural modulus of several E-glass/polyester sheet-molding compounds with soaking time in distilled water at 21–24°C. Materials described in Table 5.2 and in Figure 5.4. (From Gibson, R. F. et al. 1982. Journal of Reinforced Plastics and Composites, 1(3), 225–241. Reprinted by permission of Technomic Publishing Co.) Analysis of Lamina Hygrothermal Behavior Ta 197 Ambient temperature, Ta, and ambient moisture concentration, ca Plate ca z Thickness h T c z FIGURE 5.6 Schematic representation of temperature and moisture distributions through the thickness of a plate that is exposed to an environment of temperature, Ta, and moisture concentration, ca, on both sides. whereas the moisture distribution is governed by Fick’s second law, ∂c ∂ ∂c = Dz ∂t ∂z ∂z (5.2) where ρ = density of the material C = speciic heat of the material Kz = thermal conductivity of the material along the z-direction Dz = mass diffusivity along the z-direction t = time These equations are solved subject to the initial and boundary conditions, T = Ti 0 < z < h, t ≤ 0 c = ci T = Ta z = 0; z = h; t > 0 c = ca Shen and Springer [3] point out that, due to the numerical values of the thermophysical properties C, K z, Dz, and ρ for typical polymer composites, Principles of Composite Material Mechanics 198 the temperature approaches equilibrium about 1 million times faster than the moisture concentration. Thus, the material temperature can usually be assumed to be the same as the ambient temperature, but the moisture distribution requires further analysis. If the diffusivity is assumed to be constant, Fick’s second law becomes ∂c ∂ 2c = Dz 2 ∂t ∂z (5.3) The solution to this equation subject to the previously stated initial and boundary conditions is [3,4] c − ci 4 = 1− cm − ci π ∞ ∑ j=0 (2 j + 1)2 π 2Dzt (2 j + 1)πz 1 × exp − sin h (2 j + 1) h2 (5.4) where the moisture concentration at the surface of the material, cm, is related to the moisture content of the environment, ca. Browning et al. [1] used Equation 5.4 to predict moisture proiles for a graphite/epoxy plate after drying out for various periods of time, as shown in Figure 5.7. While Equation 5.4 gives the local moisture concentration, c(z,t), we normally measure the AS/3501-5 1.0 0.8 T = 300°F Dz = 2.476 × 10–4 in. 2/h 6 min 12 min 18 min Mi = 1.05% h = 0.044 in 0.6 z h M = 0.782% M = 0.671% 0.4 M = 0.586% 0.2 0 0.2 0.4 0.6 0.8 Moisture content (wt.%) 1.0 1.2 FIGURE 5.7 Predicted moisture proiles through the thickness of a graphite/epoxy plate after drying out for various periods of time. (From Browning, C. E., Husman, G. E., and Whitney, J. M. 1977. Composite Materials: Testing and Design: Fourth Conference, ASTM STP 617, pp. 481–496. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. Reprinted with permission.) Analysis of Lamina Hygrothermal Behavior 199 total amount of moisture averaged over the sample. The average concentration is given by [4] c= h 1 8 c( z , t) dz = (cm − ci ) × 1 − 2 h π 0 ∫ ∞ ∑ j=0 exp[−(2 j + 1)2 π 2 (Dzt/h 2 )] + ci (2 j + 1)2 (5.5) The weight percent moisture, M, is the quantity that is normally measured, and since c is linearly related to M, we can write [3] G= M − Mi 8 = 1− 2 Mm − Mi π ∞ ∑ j=0 exp[−(2 j + 1)2 π 2 (Dzt/h 2 )] (2 j + 1)2 (5.6) where Mi is the initial weight percent of moisture in the material and Mm is the weight percent of moisture in the material when the material reaches fully saturated equilibrium with the ambient conditions. Thus, the parameter G describes the moisture weight gain as a function of time. Such data can be obtained experimentally by weighing the specimen at various times during exposure to a moist environment. Figure 5.8 from Reference 3 shows a comparison of measured and predicted values of G as a function of the 1.0 M – Mi Mm – M i 0.6 G= 0.8 0.4 Graphite T-300 Fiberite 1034 (υf = 0.65–0.68) Analytical absorption and desorption 0.2 0.0 0.001 0.01 0.1 1.0 t ∗ = Dt/h2 FIGURE 5.8 Comparison of predicted (Equation 5.6) and measured moisture absorption and desorption of T300/1034 graphite/epoxy composites. Open symbols represent measured absorption and dark symbols represent measured desorption. (From Shen, C. H. and Springer, G. S. 1976. Journal of Composite Materials, 10, 2–20. Reprinted by permission of Technomic Publishing Co.) 200 Principles of Composite Material Mechanics dimensionless ratio Dzt/h2 for graphite/epoxy. The agreement is seen to be excellent. Thus, the moisture diffusion process in these composites seems to follow Fick’s law. In fact, the diffusivity is often determined indirectly by itting the Fick’s law prediction to such experimental moisture pickup data, using the diffusivity as a curve-itting parameter. Non-Fickian diffusion has also been observed in some cases where microcracking developes as a result of the hygrothermal degradation [5]. The time-dependent viscoelastic response of polymers has also been found to lead to non-Fickian moisture diffusion in polymer composites [6]. For more information on these and various other moisture effects in polymer composites, the reader is referred to several review articles by Weitsman [7] and Weitsman and Elahi [8]. The hygrothermal degradation of composite strength and/or stiffness can be estimated by using an empirical equation to degrade the corresponding matrix property, then by using the degraded matrix property in the appropriate micromechanics equation. Chamis and Sinclair [9] and Chamis [10] have demonstrated such a procedure based on the equation P Tgw − T Fm = = Po Tgo − To 1/2 (5.7) where Fm = matrix mechanical property retention ratio P = matrix strength or stiffness after hygrothermal degradation Po = reference matrix strength or stiffness before degradation T = temperature at which P is to be predicted (°F) Tgo = glass transition temperature for reference dry condition (°F) Tgw = glass transition temperature for wet matrix material at moisture content corresponding to property P (°F) (Figure 5.1) To = test temperature at which Po was measured (°F) (All temperatures are in °F.) The form of Equation 5.7 is based on the experimental observation that degradation is gradual until the temperature T approaches Tgw, whereupon the degradation accelerates. The value of Tgw can be obtained from experimental data on the glass transition temperature of the matrix resin as a function of absorbed moisture. For example, the data of DeIasi and Whiteside [11] show the reduction in Tgw with increasing moisture content for six epoxy resins (Figure 5.9). Chamis [10] suggests that Tgw can be estimated by using the following empirical equation: Tgw = (0.005 Mr2 − 0.10 Mr + 1.0)Tgo (5.8) where Mr is the weight percent of moisture in the matrix resin and values of Tgo for several matrix materials are found in Tables 3.2 and 5.1. DeIasi and Analysis of Lamina Hygrothermal Behavior 201 240 3501-5 5208 NMD2373 3502 3501-6 934 Glass transition temperature (°C) 220 200 180 160 140 120 100 80 60 0 2 4 6 Moisture content (wt.%) 8 10 FIGURE 5.9 Variation of glass transition temperature with equilibrium moisture content for several epoxy resins. (Reprinted from DeIasi, R. and Whiteside, J. B. 1987. In Vinson, J. R. ed., Advanced Composite Materials—Environmental Effects, ASTM STP 658, pp. 2–20. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. With permission.) Whiteside [11] and Browning et al. [1] also found that data such as that in Figure 5.9 are in good agreement with predictions from the theory of polymer plasticization by diluents. Once the mechanical property retention ratio is found from Equation 5.7, it is used to degrade the matrix property in the appropriate micromechanics equation. For example, the rule of mixtures for the longitudinal modulus (Equation 3.27) now becomes E1 = Ef1υf + FmEmo υm (5.9) where Emo is the reference value of the matrix modulus in the dry condition. It is assumed that Poisson’s ratio is not hygrothermally degraded [10]. Reasonably accurate predictions are also obtained when Equation 5.7 is applied directly to matrix-dominated composite properties (i.e., P and Po are taken to be matrix-dominated composite properties instead of matrix properties). For example, Chamis and Sinclair [9] found good agreement between the predictions of Equation 5.7 and experimental data on hygrothermal degradation of transverse compression, transverse tension, and intralaminar shear strengths of boron/epoxy and graphite/epoxy composites (Figure 5.10). Thus, the hygrothermally degraded composite property may be estimated Principles of Composite Material Mechanics 202 Measured strength (ksi) 40 30 20 B/E 90° T&C, IS; 70, 250, 350°F (dry) MOD-II/E 90° T&C, IS; 70, 250, 350°F (dry) HMS/E 90° T&C, IS; 70, 250, 350°F (dry) AS/E 90°, ± 45°; 73, 218°F, dry and 1.1% moisture Filled symbols denote reference strength. 10 0 30 10 20 Predicted strength (ksi) 40 FIGURE 5.10 Comparison of predicted (Equation 5.7) and measured strengths of several hygrothermally degraded composites. (Reprinted from Chamis, C. C. and Sinclair, J. H. 1982. In Daniel, I. M. ed., Composite Materials: Testing and Design (Sixth Conference), ASTM STP 787, pp. 498–512. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. With permission.) by applying Equation 5.7 directly to the matrix-dominated composite property measured under reference conditions, or by applying Equation 5.7 to matrix data measured under reference conditions, then substituting the result into the appropriate micromechanics equation. Empirical equations such as Equations 5.7 and 5.8 should always be used with caution. Curve-itting parameters such as the exponent of 1/2 in Equation 5.7 and the coeficients of Mr in Equation 5.8 are based on experimental data for epoxy matrix materials. While the equations may be suitable for other composites as well, the user should check predictions against available experimental data where possible. The procedure just outlined is based on the combined effects of temperature and moisture, and the two effects were seen to be coupled by the lowering of the glass transition temperature due to absorbed moisture. There is another important connection between the two effects. Moisture absorption occurs by diffusion, which is known to be a thermally activated process. The diffusivity D that appears in Fick’s law is related to temperature by the Arrhenius relationship: −E D = Doexp a RT (5.10) Analysis of Lamina Hygrothermal Behavior 203 where Do = material constant Ea = activation energy for diffusion R = universal gas constant T = absolute temperature Proof that this relationship holds for composites is given by the fact that plots of experimentally determined values of log D versus 1/T fall on a straight line, as shown in Figure 5.11 from Loos and Springer [12]. The result of this relationship is that increased temperature causes an increase in the rate of moisture absorption, as shown in Figure 5.12. The applied stress also has an effect on moisture absorption in polymers and polymer composites [13–15]. For example, Fahmy and Hurt [13] have shown that the diffusivity of a polymer is increased under tensile stress and decreased under compressive stress. Thus, in a composite, the residual stresses due to differential thermal expansion of iber and matrix materials may cause increased moisture absorption along a path running through a tensile stress ield. Starting from the basic principles of continuum mechanics and irreversible thermodynamics, Weitsman [15] showed that, for both elastic and viscoelastic materials, both the diffusion process and the saturation moisture levels are stress dependent, and that the diffusion process is nonlinear with respect to stress. Temperature, T (K) 350 300 400 Diﬀusivity, D (mm2/s) 5722 Dave = 6.51 exp – T 10–6 10–7 Present data DeIasi and Whiteside (1978) Whitney and Browning (1978) 10–8 2.4 2.6 2.8 3.0 3.2 l/T × 103 (1/K) 3.4 3.6 FIGURE 5.11 Variation of transverse diffusivity with temperature for AS/3501-5 graphite/epoxy composite. (From Loos, A. C. and Springer, G. S. 1981. In Springer, G. S. ed., Environmental Effects on Composite Materials, pp. 34–50. Technomic Publishing Co., Lancaster, PA. Reprinted by permission of Technomic Publishing Co.) Principles of Composite Material Mechanics 204 2.0 77°C 1.8 Moisture content (wt.%) 1.6 49°C 1.4 1.2 23°C 1.0 0.8 0.6 0.4 0.2 2 4 6 8 10 12 Time1/2 (days)1/2 14 16 FIGURE 5.12 Effect of temperature on rate of moisture absorption in AS/3501-5 graphite/epoxy composite. (Reprinted from DeIasi, R. and Whiteside, J. B. 1987. In Vinson, J. R. ed., Advanced Composite Materials—Environmental Effects, ASTM STP 658, pp. 2–20. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. With permission.) EXAMPLE 5.1 Based on the stress–strain data for a 3501-5 epoxy matrix material in Figure 5.2, determine the reduction in the Young’s modulus, Em, as the hygrothermal conditions change from room temperature (RT) dry to 300°F wet. Similarly, based on the stress–strain data for transverse loading of the corresponding AS/3501-5 graphite/epoxy composite in Figure 5.3, determine the reduction in the transverse Young’s modulus, E2, for the same change in the hygrothermal conditions, then compare and comment on the reductions in the modulus values for the epoxy matrix and the transverse composite. Solution The modulus values are estimated from the slopes of the linear portions of the stress–strain curves for the two hygrothermal conditions in Figures 5.2 and 5.3. For Figure 5.2 at an arbitrary strain level of 1%, the approximate stress level for the RT dry condition is 5.2 ksi and the modulus, Em = 5.2/0.01 = 520 ksi. The corresponding stress level for the 300°F wet condition at a strain level of 1% is approximately 0.8 ksi and the modulus, Em = 0.8/0.01 = 80 ksi. For Figure 5.3 at an arbitrary strain level of 0.4%, the approximate stress level for the RT dry condition is 5.5 ksi and the transverse modulus, E2 = 5.5/0.004 = 1375 ksi. The corresponding stress level for the 300oF wet condition is approximately 0.8 ksi Analysis of Lamina Hygrothermal Behavior 205 and the transverse modulus, E2 = 0.8/0.004 = 200 ksi. The percent reduction in the modulus values of both the epoxy matrix and the corresponding transverse composite as the hygrothermal conditions change from RT dry to 300°F is around 80%. Thus, the combination of elevated temperature and moisture signiicantly degrades the stiffnesses of both the epoxy matrix and the transverse composite, and the effects of hygrothermal conditions on the transverse properties of the composite are matrix dominated. EXAMPLE 5.2 An epoxy resin sample has a thickness h = 5 mm and a diffusivity D = 3 × 10−8 mm2/s. Determine the moisture absorption of an initially dry sample after a time t = 100 days. Solution The moisture absorption is predicted by Equation 5.6, which involves an ininite series. In order to examine the convergence characteristics of the series, we will look at the irst four terms. Each term in the series contains the dimensionless ratio π2Dt/h2, which has the numerical value π 2Dt π 2 (3 × 10 −8 )(100)(60)(60)(24) = = 0.102 (5)2 h2 Since the sample was initially dry, the initial weight of moisture in the material is Mt = 0. Thus, Equation 5.6 reduces to the ratio M/Mm, which is the ratio of the weight percent of moisture at time t to the weight percent of moisture in the fully saturated equilibrium condition. The irst four terms are exp(−9(0.102)) M 8 = 1 − 2 exp(−0.102) + Mm π 9 + exp(−25(0.102)) exp(−49(0.102)) + ⋯ + 49 25 The values of M/Mm corresponding to the different number of terms are: 0.267 (one term), 0.230 (two terms), 0.228 (three terms), and 0.228 (four terms). Thus, the series has converged after three terms. Rapid convergence is a characteristic of this solution, and in many cases, only one term is suficient [4]. EXAMPLE 5.3 The composite described in Examples 3.2, 3.3, and 3.6 is to be used in a “hot–wet” environment with temperature T = 200°F (93°C) and resin moisture content M r = 3%. If the glass transition temperature of the dry matrix resin is 350°F (177°C) and if the properties given in Examples 3.2, 3.3, and 3.6 are for a temperature of 70°F (21°C), determine the Principles of Composite Material Mechanics 206 hygrothermally degraded values of the longitudinal and transverse moduli. Solution From Equation 5.8, the glass transition temperature in the wet condition is Tgw = [0.005(3)2 − 0.1(3) + 1.0]350 = 261°F (127°C) From Equation 5.7, the hygrothermally degraded Young’s modulus of the epoxy resin is Em = [(261 − 200)/(350 − 7 0)]1/2 (0.5)(10 6 ) = 0.233(10 6 ) psi (1.61GPa) From Equation 5.9, the hygrothermally degraded longitudinal modulus is E1 = 32(10 6 )(0.506) + 0.233(10 6 )(0.482) = 16.3(10 6 ) psi (112 GPa) Thus, the hygrothermally degraded value of E1 is 99.2% of the reference value calculated in Example 3.6. As stated earlier, the iber-dominated properties are not affected much by temperature and moisture. Similarly, using the degraded value of Em in Equation 3.40, we ind that the hygrothermally degraded transverse modulus is estimated to be E2 = 0.434(106) psi (3.0 GPa), which is only 53% of the reference value calculated in Example 3.6. Thus, the matrix-dominated properties such as the transverse modulus are strongly affected by hygrothermal conditions. PROBLEM 5.1 Repeat Example 5.1 for the cases where the hygrothermal conditions change from (a) RT dry to 300°F dry, and (b) from RT dry to RT wet, then compare with the results from Example 5.1. That is, compare the effect of combined elevated temperature and moisture (Example 5.1) on the moduli of the epoxy matrix and the transverse composite with the separate effects of elevated temperature (Problem 5.1(a)) and elevated moisture (Problem 5.1(b)) on these moduli. PROBLEM 5.2 Using Equation 5.6 for moisture diffusion, derive an equation for the time required for an initially dry material to reach 99.9% of its fully saturated equilibrium moisture content. The series in Equation 5.6 converges rapidly, so for the purposes of this problem, it is necessary only to consider the irst term. The answer should be expressed in terms of the thickness, h, and the diffusivity, Dz. Analysis of Lamina Hygrothermal Behavior 207 PROBLEM 5.3 The dependence of the transverse (through-the-thickness) diffusivity of unidirectional AS/3501-5 graphite/epoxy composite on temperature is given in Figure 5.11. For a temperature of 77°C and a thickness of 2.54 mm, use the results from Figure 5.11 and Problem 5.2 to estimate the time required for this material to reach 99.9% of its fully saturated equilibrium moisture content from an initially dry condition. Compare your estimate with the experimental data in Figure 5.12. Does the estimate seem to be reasonable? PROBLEM 5.4 For the material described in Problems 5.2 and 5.3 above at a temperature of 77°C, determine the time required for drying the material from 99.9% to 50% of its fully saturated equilibrium moisture content. PROBLEM 5.5 Using only the linear part of the moisture absorption curve for a temperature of 77°C in Figure 5.12, and assuming a thickness of 2.54 mm, estimate the diffusivity Dz. Compare this value with the estimate from Figure 5.11. PROBLEM 5.6 For the composite properties and environmental conditions described in Examples 3.6, 4.7, and 5.3, determine the hygrothermally degraded values of the longitudinal and transverse tensile strengths. Compare with the reference values of these strengths from Example 4.7. PROBLEM 5.7 For the composite properties and environmental conditions described in Examples 3.6, 4.7, and 5.3, compare the reference and hygrothermally degraded values of the longitudinal compressive strength. Assume ν12 = 0.3. Compare and discuss the different effects that hygrothermal conditions have on longitudinal tensile and compressive strengths. PROBLEM 5.8 The ilament-wound E-glass/epoxy pressure vessel described in Example 4.4 is to be used in a hot–wet environment with temperature T = 100°F (38°C) and moisture content Mr = 4%. The glass transition temperature of the dry epoxy resin is 250°F (121°C), and the lamina strengths listed in Table 4.1 are for a temperature of 70°F (21°C) and a moisture content of zero. Determine the internal pressure p that would cause failure of the vessel according to the maximum stress criterion. Compare with the result from Example 4.4. 208 Principles of Composite Material Mechanics 5.3 Lamina Stress–Strain Relationships including Hygrothermal Effects In Chapter 2, the lamina stress–strain relationships were developed for linear elastic behavior and constant environmental conditions. The thermal expansion or contraction of structural materials due to temperature change is a well-known phenomenon, however, and the thermal strains for an isotropic material are usually described by an equation of the form α∆T if i = 1, 2, 3 ε iT = 0 if i = 4, 5, 6 (5.11) where i = 1, 2, …, 6 (recall contracted notation) ΔT = temperature change (T − To) T = inal temperature To = initial temperature, where ε Ti = 0 for all i α = coeficient of thermal expansion (CTE) This relationship is based on the experimental observation that a temperature change in an unrestrained isotropic material induces an equal expansion or contraction in all directions, with no distortion due to shear deformation. In this case α > 0, because an increase in temperature causes an increase in thermal strain. As we will see later, however, some anisotropic iber materials have negative CTEs along the iber axis and positive CTEs along the transverse direction. In general, the strain–temperature relationship is nonlinear, but the assumption of linearity is valid over a suficiently narrow temperature range. Typical thermal expansion data for an epoxy resin are shown in Figure 5.13. If operation over a wide temperature range is expected, the reader is referred to data such as that of Cairns and Adams [16], who have developed cubic polynomial expressions to it experimental thermal expansion data for epoxy, glass/epoxy, and graphite/epoxy from −73°C to 175°C. A procedure for estimating the hygrothermal degradation of matrix-dominated thermal properties will be discussed in Section 5.4. In polymeric materials, moisture has been shown to cause hygroscopic expansions or contractions analogous to thermal strains. For example, the experimentally determined moisture-induced swelling of several epoxy resins is shown in Figure 5.14. The experimental observation is that the moisture-induced strains in isotropic materials can be expressed as βc if i = 1, 2, 3 ε iM = 0 if i = 4, 5, 6 (5.12) Analysis of Lamina Hygrothermal Behavior 209 10 8 Strain (10–3) 6 4 2 0 –2 –4 –100 0 100 Temperature (°C) 200 FIGURE 5.13 Thermal expansion versus temperature for 3501-6 epoxy resin. (From Cairns, D. S. and Adams, D. F. 1984. In Springer, G. S. ed., Environmental Effects on Composite Materials, Vol. 2, pp. 300–316. Technomic Publishing Co., Lancaster, PA. Reprinted by permission of Technomic Publishing Co.) 8 Volumetric change (%) 7 6 5 4 3 2 3501-5 NMD2373 1 0 2 4 6 Moisture content (wt.%) 8 10 FIGURE 5.14 Hygroscopic expansion versus moisture content for two epoxy resins. (Reprinted from DeIasi, R. and Whiteside, J. B. 1987. In Vinson, J. R. ed., Advanced Composite Materials—Environmental Effects, ASTM STP 658, pp. 2–20. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. With permission.) Principles of Composite Material Mechanics 210 where c = moisture concentration = (mass of moisture in unit volume/mass of dry material in unit volume) β = coeficient of hygroscopic expansion (CHE) The reference condition is assumed to be the moisture-free state c = 0, where ε iM = 0. Hygroscopic strains are generally nonlinear functions of moisture content [16], but the linear relationship in Equation 5.12 is valid if the range of moisture contents is not too wide. Thus, in an isotropic material, the total hygrothermal strain can be written as T M εH i = εi + εi (5.13) Because ibers usually have CTEs and CHEs that are quite different from those of matrix materials, the hygrothermal strains in a composite lamina are different in the longitudinal and transverse directions. For example, the experimental thermal strain versus temperature data in Figure 5.15 (from Reference 17) shows the large differences between longitudinal (ε1) and transverse (ε2) thermal strains for unidirectional Kevlar 49/epoxy and S-glass/epoxy composites. Notice that the longitudinal thermal strains ε1 for Kevlar 49/epoxy are negative, whereas the corresponding transverse thermal strains ε2 are positive, which implies that the longitudinal CTE, α1, is negative and the transverse CTE, α2, is positive for this material. Carbon iber-reinforced composites often have similar characteristics. Notice 1.2 Induced strain (%) 1.0 0.8 , , O = Kevlar 49/epoxy = S-Glass/e poxy 2 1 8 0.6 2 0.4 2 0.2 1 0 –0.2 20 1 60 100 140 Temperature (°C) 180 220 FIGURE 5.15 Variation of measured longitudinal and transverse thermal strains for unidirectional Kevlar 49/epoxy and S-glass/epoxy with temperature. (From Adams, D. F., Carlsson, L. A., and Pipes, R. B., 2003. Experimental Characterization of Advanced Composite Materials. CRC Press, Boca Raton, FL. With permission.) Analysis of Lamina Hygrothermal Behavior 211 also in Table 3.1 that the longitudinal CTEs of some other ibers are negative, whereas the transverse CTEs are positive. As shown later, this leads to the interesting possibility of designing a composite with a CTE of near zero. Thus, subscripts are needed for α and β, and the hygrothermal strains associated with the 1,2 principal material axes in the specially orthotropic lamina should be expressed as α i ∆T + βic if i = 1, 2, 3 εH i = 0 if i = 4, 5, 6 (5.14) If the material is transversely isotropic, α2 = α3 and β2 = β3. Typical values of αi and βi for several composites are given in Table 5.3 from Reference 18. Representative CTEs for iber and matrix materials and CHEs for polymer matrix materials are given in Tables 3.1 and 3.2. Notice that the negative longitudinal CTE of carbon ibers leads to a very small longitudinal CTE for the carbon/epoxy lamina. Notice also the large differences between the longitudinal and transverse hygrothermal coeficients. The total strains along the principal material axes in the specially orthotropic lamina are found by summing the mechanical strains due to applied stresses (Equation 2.24) and the hygrothermal strains (Equation 5.14): ε1 S11 ε 2 = S21 γ 0 12 S12 S22 0 β1 σ1 α 1 σ 2 + α 2 ∆T + β 2 c 0 S66 τ12 0 0 0 (5.15) or, in more concise matrix notation, {ε} = [S]{σ} + {α}∆T + {β}c (5.16) TABLE 5.3 Typical Thermal and Hygroscopic Expansion Properties Thermal Expansion Coeficients ([10 −6 m/m]/°C) Material AS carbon/epoxy E-glass/epoxy AF-126-2 adhesive 1020 steel α1 0.88 6.3 29.0 12.0 Hygroscopic Expansion Coeficients (m/m) α2 β1 β2 31.0 20.0 29.0 12.0 0.09 0.014 0.20 – 0.30 0.29 0.20 – Source: From Graves, S. R. and Adams, D. F. 1981. Journal of Composite Materials, 15, 211–224. With permission. Principles of Composite Material Mechanics 212 whereupon the stresses are given by {σ} = [S]−1({ε} − {α}∆T − {β}c) (5.17) Note that if the material is unrestrained during the hygrothermal exposure, there are no stresses generated and the strains are given by {ε} = {α}∆T + {β}c (5.18) If the material is completely restrained during hygrothermal exposure, however, the total strain must be zero. Thus, {ε} = 0 = [S]{σ} + {α}∆T + {β}c (5.19) and the resulting hygrothermal stresses are given by {σ} = [S]−1(−{α}∆T − {β}c) (5.20) Note that there are no hygrothermal shear strains or shear stresses along the principal material axes. This is not true for the generally orthotropic (offaxis) case, however. For an arbitrary set of axes xy oriented at an angle θ to the 1,2 axes, the stress–strain relationships can be transformed as in Chapter 2. The complete stress–strain relations for the generally orthotropic lamina are ε x S11 ε y = S12 γ S xy 16 S12 S22 S26 βx S16 σ x α x S26 σ y + α y ∆T + β y c β S66 τ xy α xy xy (5.21) In the transformations, it must be remembered that the CTEs and the CHEs transform like tensor strains (recall Equation 2.33), so that αx α 1 −1 α y = [T ] α 2 α 0 xy/2 (5.22) and a similar equation is used for the CHEs. Notice that the hygrothermal effects do induce shear strains in the off-axis case due to αxy and βxy, the shear coeficients of thermal and hygroscopic expansion, respectively. This is quite different from the case of isotropic materials, where hygrothermal effects do not cause shear strains along any axes. The variations of αx, αy, and αxy with lamina orientation according to Equation 5.22 are shown in Figure 5.16. Analysis of Lamina Hygrothermal Behavior αy α2 αx αxy α1 0° 45° Lamina orientation (θ) 213 α2 α1 90° FIGURE 5.16 Variation of lamina thermal expansion coeficients with lamina orientation for a lamina having α2 > α1 > 0. Similar curves could also be used for βx, βy, and βxy. The hygrothermal shear coeficients αxy and βxy have their maximum values at θ = 45° and are proportional to the differences (α1 − α2) and (β1 − β2), respectively. Thus, the greater the degree of anisotropy (i.e., the larger the ratio α1/α2 or β1/β2), the greater the hygrothermally induced shear strains. It is important to note that if α1 < 0 and α2 > 0, it is possible to ind an angle θ, where αx = 0. Thus, we can design a laminate consisting of plies of such a material, so that the CTE along a particular direction is zero. EXAMPLE 5.4 An orthotropic lamina forms one layer of a laminate which is initially at temperature To. Assuming that the lamina is initially stress free, that adjacent lamina are rigid, that the properties do not change as a result of the temperature change, and that the lamina picks up no moisture, determine the maximum temperature that the lamina can withstand according to the maximum stress criterion. Solution Owing to the assumption that adjacent laminae are rigid, deformation is prevented and the total strains must all be zero. The resulting hygrothermal stresses are therefore given by Equation 5.20 with c = 0, {σ} = −[S]−1 {α}(T − To ) = −[Q]{α}(T − To ) Thus, for the maximum stress criterion, it is necessary to check each of the following conditions: For tensile stresses −(Q11α 1 + Q12α 2 )(T − To ) = sL( + ) −(Q12α 1 + Q22α 2 )(T − To ) = sT( + ) Principles of Composite Material Mechanics 214 For compressive stresses −(Q11α 1 + Q12α 2 )(T − To ) = sL( − ) −(Q12α 1 + Q22α 2 )(T − To ) = sT( − ) (Note: There are no hygrothermal shear stresses along the 1,2 axes.) After substituting numerical values for the initial temperature, To, the lamina stiffness, Qtj, the coeficients of thermal expansion, αi, the strengths sL(+ ) , and so on, in the above equations, the equation that yields the lowest temperature T would be the condition governing failure. It is worthwhile to note that adjacent laminae are not really rigid, but we will need to use laminate theory later to consider deformations of adjacent laminae. It is also worthwhile to note that if hygrothermal degradation of properties is to be taken into account, Equation 5.7 could be used to express the hygrothermally degraded lamina strengths and stiffnesses in terms of the temperature T. In this case, T would appear on both sides of the above equations and the problem would be more dificult to solve. EXAMPLE 5.5 A sample of a unidirectional E-glass/epoxy lamina is completely unrestrained as it is heated from 20°C to 70°C. Determine all components of stress and strain associated with the 1,2 axes and the x,y axes, if the x,y axes are oriented at θ = 45°. See Table 5.3 for the required properties of E-glass/epoxy. Solution Since the lamina is unrestrained during heating, there are no stresses along either the 1,2 or the x,y axes, but the thermal strains are found as follows. From Equation 5.15 with no stresses or hygroscopic strains, the thermal strains along the 1,2 axes for ΔT = 50°C are 6.3(10 −6 ) 0.000315 ε1 α 1 −6 ε 2 = α 2 ∆T = 20.0(10 ) (50) = 0.001 γ 0 0 0 12 From the inverted form of Equation 2.33, with θ = 45°, the thermal strains along the x,y axes can be found directly as ε 0.5 εx 1 −1 ε y = [T ] ε 2 = 0.5 γ γ 0.5 xy/2 12/2 0.55 0.5 −0.5 −1.0 0.000315 0.00066 1.0 0.001 = 0.00066 0 0 −0.00034 Alternatively, the same result for the thermal strains along the x,y axes can be obtained by irst transforming the CTE values from the 1,2 axes to Analysis of Lamina Hygrothermal Behavior 215 the x,y axes using Equation 5.22, then substituting the transformed CTEs in Equation 5.21 to calculate the thermal strains along the x,y axes. Note that, although there was no thermal shear strain along the 1,2 axes, there is an off-axis thermal shear strain along the x,y axes. Thus, there will be thermal distortion associated with the off-axis directions, and this is another example of the shear coupling phenomenon. PROBLEM 5.9 An orthotropic lamina forms one layer of a laminate which is initially at temperature T0. Assuming that the lamina is initially stress free, that the adjacent laminae are rigid, that the properties do not change as a result of the temperature change, and that the lamina picks up no moisture, determine the maximum temperature that the lamina can withstand according to the Tsai–Hill failure criterion. PROBLEM 5.10 A carbon/epoxy lamina is clamped between rigid plates in a mold (Figure 5.17), while curing at a temperature of 125°C. After curing, the lamina/mold assembly (still clamped together) is cooled from 125°C to 25°C. The cooling process occurs in moist air and the lamina absorbs 0.5% of its weight in moisture. The lamina has the following properties: E1 = 140 GPa E2 = 10 GPa ν12 = 0.3 G12 = 7 GPa α 1 = −0.3 × 10 −6 /K α 2 = 28 × 10 −6 /K β1 = 0 β 2 = 0.44 Assuming that the lamina properties do not change over this temperature range and that the lamina is initially dry and stress free, determine the residual hygrothermal stresses in the lamina at 25°C for angles θ = 0° and 45°. PROBLEM 5.11 Samples of unidirectional Kevlar 49/epoxy and S-glass/epoxy composites are subjected to elevated temperatures in an oven and the resulting thermal strains are measured by using strain gages oriented along the 1 and 2 Rigid plate Lamina Rigid plate FIGURE 5.17 Lamina clamped between rigid plates in a mold. Principles of Composite Material Mechanics 216 directions, as shown in Figure 5.15. From the data in Figure 5.15, estimate the longitudinal thermal expansion coeficient α1 and the transverse thermal expansion coeficient α2 for both materials. PROBLEM 5.12 A unidirectional 45° off-axis E-glass/epoxy composite lamina is supported on frictionless rollers between rigid walls as shown in Figure 5.18. The lamina is ixed against displacements in the y-direction, but is free to move in the x-direction. Determine all of the lamina strains associated with the x,y axes if the lamina is heated from 20°C to 120°C. The required properties for E-glass/epoxy are given in Tables 2.2 and 5.3. PROBLEM 5.13 An orthotropic lamina has thermal expansion coeficients α1 = −4.0 (10−6) m/m/K and α2 = 79(10−6) m/m/K. Determine (a) the angle θ for which the thermal expansion coeficient αy = 0, and (b) the angle θ for which the thermal expansion coeficient αxy has its maximum value. PROBLEM 5.14 A carbon/epoxy lamina having the properties listed in Problem 5.10 is clamped between two rigid plates as shown in Figure 5.17. If the lamina is heated from 20°C to 120°C, determine the thermal stresses associated with the principal material axes of the lamina. PROBLEM 5.15 A unidirectional E-glass/epoxy lamina is securely attached to rigid supports on both ends in two different ways as shown in Figure 5.19. In Figure 5.19a, the iber direction is perpendicular to the rigid supports, and in Figure 5.19b, the ibers are oriented parallel to the rigid supports. The lamina is to be heated by the amount ΔT in both cases. Using the properties in Tables 2.2, 2 y 1 45° Rigid walls FIGURE 5.18 Off-axis composite lamina ixed between rigid walls for Problem 5.12. x Analysis of Lamina Hygrothermal Behavior (a) 217 2 1 Rigid support Rigid support (b) 1 2 Rigid support Rigid support FIGURE 5.19 Rigidly supported E-glass epoxy lamina in two different orientations for Problem 5.15. 4.1, and 5.3, determine the maximum temperature increase ΔT that the composites can withstand in both Figure 5.19a and b, according to the maximum stress criterion. Based on the maximum service temperatures for typical epoxies in Table 5.1, what can you say about the practical limits on ΔT in these cases? 5.4 Micromechanics Models for Hygrothermal Properties We have seen in Chapters 3 and 4 that the mechanical properties of a composite lamina can be estimated from the corresponding properties of the constituent materials using micromechanics models. Similarly, micromechanics equations for the thermophysical properties that appear in hygrothermal analysis can be developed. Various theoretical approaches ranging from elementary mechanics of materials to energy methods and inite element analysis (FEA) have been used. An equation for the longitudinal CTE, α1, can be developed using the elementary mechanics of materials approach from Chapter 3. Recall that in the derivation of the rule of mixtures for the longitudinal modulus (Equation 3.27), the 1D forms of the stress–strain relationships along the 1 direction for the lamina, iber, and matrix materials (Equation 3.24) were substituted in the rule of mixtures for longitudinal stress, Equation 3.23. The Principles of Composite Material Mechanics 218 corresponding 1D form of the lamina stress–strain relationship including the thermal effect is εc1 = σ c1 + α 1∆T E1 (5.23) or σ c1 = E1( εc1 − α 1∆T ) (5.24) If we now substitute equations similar to Equation 5.24 for composite, iber, and matrix, respectively, into Equation 3.23, the result is E1( εc1 − α 1∆T ) = Ef 1( εf 1 − α f 1∆T )υf + Em1( εm1 − α m1∆T )υm (5.25) where αf1 and αm1 are the longitudinal CTEs of iber and matrix materials, respectively (see Tables 3.1 and 3.2), and the remaining terms are deined in Chapter 3. By combining Equations 5.25, 3.26, and 3.27, we get a modiied rule of mixtures for the longitudinal CTE: α1 = Ef 1α f 1υf + Em1α m1υm Ef 1α f 1υf + Em1α m1υm = E1 Ef 1υf + Em1υm (5.26) For the case of isotropic constituents, the above equation becomes α1 = Ef α f υf + Emα m υm Ef υf + Em υm (5.27) This equation, derived by a mechanics of materials approach, turns out to be the same as the result obtained by Schapery [19], who used a more rigorous energy method. This should not be surprising, given the proven validity of the assumptions that were used in the derivation of the rule of mixtures for E1 and the accuracy of Equation 3.27. Hashin [20] derived a more complicated expression for the case of orthotropic constituents. Similarly, an elementary mechanics of materials approach can be used to ind a micromechanics equation for α2, the transverse CTE of the lamina. In this case, the appropriate 1D form of the lamina stress–strain relationship including the thermal effect is εc2 = σ c2 + α 2∆T E2 (5.28) Analysis of Lamina Hygrothermal Behavior 219 Substituting equations similar to Equation 5.28 for composite, iber, and matrix, respectively, in the transverse geometric compatibility condition given by Equation 3.37, the result is σ c2 σ σ + α 2∆T = f 2 + α f 2∆T υf + m 2 + α m 2∆T υm E2 Ef 2 Em2 (5.29) where αf2 and αm2 are the transverse CTEs of iber and matrix materials, respectively (see Tables 3.1 and 3.2) and the remaining terms are deined in Chapter 3. By combining Equation 5.29 with Equation 3.39 and assuming that the stresses in the composite, iber, and matrix are all equal (as in the development of Equation 3.40), we get another rule of mixtures type equation α 2 = α f2υf + α m2υm (5.30) In many cases, the matrix is isotropic, so Em1 = Em2 = Em and αm1 = αm2 = αm. If both iber and matrix materials are isotropic, Equation 5.30 becomes α 2 = α f υf + α m υm (5.31) However, as indicated earlier, the assumption of equal stresses in composite, iber, and matrix leading to the inverse rule of mixtures for E2 in Equation 3.40 is not very accurate, so Equations 5.30 and 5.31 should only be considered as rough estimates for α2. Schapery [19] used a more rigorous energy method to derive the following expression for the transverse CTE of a composite with isotropic constituents: α 2 = (1 + νm )α m υm + (1 + νf )α f υf − α 1 ν12 (5.32) where α1 is the longitudinal CTE given by Equation 5.27 and ν12 is the major Poisson’s ratio of the lamina given by Equation 3.45. The variations of α1 and α2 with iber-volume fraction for a typical graphite/epoxy composite are shown in Figure 5.20. Rosen [21] has observed that for such composites having high iber-volume fractions, the predicted α1 is practically zero. Measurements of the CTEs for such materials by Ishikawa et al. [22] have conirmed that α1 is so small as to luctuate between positive and negative values due to small changes in temperature or iber-volume fraction. Over the range of practical iber-volume fractions, α2 is much greater than α1. It is also interesting to note that at low iber-volume fractions, α2 can be greater than αm. FEA of unit cells is a versatile numerical approach to micromechanical modeling of composite CTEs. FEA unit cells similar to those described in Section 3.4.2 are subjected to a temperature change, ΔT, and then the resulting Transverse expansion coeﬃcient, α2 (10–6/K) 60 Ef 1 = 340 GPa 50 Matrix αm 40 30 α2 20 10 Transverse ﬁber αf 2 6 4 0 α1 2 0 0 0.20 0.40 0.60 0.80 Fiber volume fraction (υf) 1.00 Longitudinal expansion coeﬃcient, α1 (10–6/K) Principles of Composite Material Mechanics 220 FIGURE 5.20 Variation of predicted longitudinal and transverse coeficients of thermal expansion with iber-volume fraction for typical unidirectional graphite/epoxy composite. (From Rosen, B. W. 1987. In Reinhart, T. J. ed., Engineered Materials Handbook, Composites, Vol. 1, Section 4. ASM International, Materials Park, OH. Reprinted by permission of ASM International.) FEA-calculated thermally induced displacements are used to determine the CTEs. Required input properties are the elastic constants and the CTEs of each inite element in the iber and matrix materials, and either orthotropic or isotropic constituents are easily accommodated. Dimensions of the unit cell are selected so as to simulate the appropriate iber-volume fraction. In fact, the FEA approach is just a numerical simulation of the experiment that is done to measure the CTE, as discussed later in Chapter 10. For example, Karadeniz and Kumlutas [23] developed three-dimensional FEA unit cell models such as the one shown in Figure 5.21 to predict α1 and α2 for several types of composites. In the model shown in Figure 5.21, the iber lies along the X-axis, whereas Y and Z are the transverse directions. Displacements of the model along the ixed reference planes X = 0, Y = 0, and Z = 0 in Figure 5.21 were restricted to be perpendicular to those planes. The free boundary planes X = l0, Y = l0, and Z = l0 were restricted to move parallel to their original positions after the change in temperature ΔT in order to maintain geometric compatibility with neighboring unit cells (see Figure 3.25 and corresponding discussion of geometric compatibility and multipoint constraint in Section 3.4.2). The longitudinal CTE, α1 (same as αX in Figure 5.21), was then calculated from α1 = α X = ∆lX 1 l0 ∆T (5.33) Analysis of Lamina Hygrothermal Behavior l0 221 l0 X Z FIGURE 5.21 Typical FEA unit cell for prediction of composite longitudinal and transverse CTEs. (Reprinted from Composite Structures, 78, Karadeniz, Z. and Kumlutas, D., A numerical study on the coeficients of thermal expansion of iber-reinforced composite materials, 1–10. Copyright 2007, with permission from Elsevier.) where ΔlX is the FEA-calculated thermal displacement of the plane X = l0 along the X-direction. Similarly, the transverse CTE, α2 (same as αZ or αY in Figure 5.21, assuming transverse isotropy), was calculated from α2 = αZ = ∆l 1 ∆lZ 1 = αY = Y l0 ∆T l0 ∆T (5.34) where ΔlZ and ΔlY are the FEA-calculated thermal displacements of the planes Z = l0 and Y = l0, along the Z- and Y-directions, respectively. In Reference 23, predictions from these FEA models were compared with experimental data for several composites from Sideris [24] and with results from other micromechanics models such as the rule of mixtures equations, the Schapery equations [19], and the Rosen–Hashin equations [25]. It was concluded that all of the models, including the FEA models, were in good agreement with experiments for the longitudinal CTE, but that the FEA models and the Rosen– Hashin models agreed most closely with experiments for the transverse CTE. While the Rosen–Hashin models were found to be quite accurate, they are dificult to use, and are beyond the scope of this text. The accuracy of the FEA approach has been demonstrated for the transverse CTE calculation by Dong [26]. In Figure 5.22, Gibson and Muller [27] compared analytical solutions from Equation 5.27 (longitudinal CTE) and Equation 5.32 (transverse CTE) with FEA numerical predictions from Equations 5.33 and 5.34, respectively, for a SiO2/epoxy composite. The FEA micromechanics model was Principles of Composite Material Mechanics 222 7.00 × 10–05 6.00 × 10–05 CTE (°C) 5.00 × 10–05 4.00 × 10–05 CTE (transverse) numerical CTE (transverse) analytical 3.00 × 10–05 CTE (long itudinal) numerical 2.00 × 10–05 CTE (long itudinal) analytical 1.00 × 10–05 0.00 × 10+05 0 20 40 60 80 100 Volume percentage of SiO2 FIGURE 5.22 Comparison of analytical and FEA numerical predictions of longitudinal and transverse CTEs for SiO2/epoxy composites of various SiO2 volume fractions. (Adapted from Gibson, R. F. and Muller, A. 2010. Unpublished Research, University of Nevada, Reno, NV.) based on the simple block model shown in Figure 3.5a, and the agreement is seen to be excellent. Both materials were assumed to be isotropic with the following properties: For the SiO2 ibers; Ef = 70 GPa, νf = 0.17, αf = 5 × 10−6/°C For the epoxy matrix; Em = 2.83 GPa, νm = 0.3, αm = 57.85 × 10−6/°C In summary, FEA has proven to be a very useful and accurate method for the micromechanical prediction of composite CTEs. By substituting the 1D forms of the stress–strain relationships with hygroscopic effects into Equation 3.23 and following the procedure outlined in the derivation of Equation 5.26, a similar relationship is found for the longitudinal CHE: β1 = Ef1βf1υf + Em1βm1υm Ef1υf + Em1υm (5.35) Similarly, the hygroscopic counterpart of Equation 5.30 is found to be β 2 = βf2υf + βm2υm (5.36) In polymer matrix composites, the amount of moisture absorbed by the ibers is usually negligible in comparison with the moisture absorbed by the matrix, so that the terms involving βf1 and βf2 can often be ignored. Analysis of Lamina Hygrothermal Behavior 223 For isotropic constituents, the equation for β1 would be analogous to Equation 5.31. According to Ashton et al. [28], the equations derived by Schapery (i.e., Equations 5.27 and 5.32) can be used for any expansional coeficients such as the CTE or the CHE. Thus, the transverse CHE for isotropic constituents would be given by β 2 = (1 + νm )βm υm + (1 + νf )βf υf − β1 ν12 (5.37) where β1 is given by the isotropic form of Equation 5.35. FEA micromechanics models for composite CHEs may be developed using a procedure similar to that previously outlined for composite CTEs, assuming that the FEA code being used has the capability of calculating hygroscopic strains. Recall that in the equations governing the temperature and moisture distributions (Equations 5.1 and 5.2), thermophysical properties such as speciic heat, thermal conductivity, and diffusivity appeared. According to Chamis [10], the composite speciic heat is given by Cc = 1 (ρf Cf υf + ρmCm υm ) ρc (5.38) where Cf and Cm are the speciic heat of iber and matrix, respectively; the composite density, ρc, is given by Equation 3.6, and the remaining terms are deined in Chapter 3. Ashton et al. [28] and Shen and Springer [3] have observed that the rule of mixtures formulations, K1 = K f υf + K m υm (5.39) D1 = Df υf + Dm υm (5.40) and can be used to ind the longitudinal thermal conductivity and mass diffusivity, respectively, as well as other transport properties. Equations for the transverse thermal conductivity and diffusivity based on the method of subregions (see Section 3.3) have been presented by Hopkins and Chamis [29] and Chamis [10]. These equations can be formed by substituting the appropriate properties (thermal conductivities or diffusivities instead of transverse moduli) in an equation of the form shown in Equation 3.54. Ashton et al. [27] have suggested that the Halpin–Tsai equations (see Section 3.5) can also be used for transverse transport properties such as thermal conductivity and mass diffusivity. Off-axis properties can be found by recognizing that thermal conductivity and diffusivity are both second-order tensor quantities that transform according to the form shown in Equation 2.30. Principles of Composite Material Mechanics 224 Finally, a procedure for estimating hygrothermal degradation of matrix properties such as α, β, K, and C has been proposed by Chamis [10]. Based on the observation that the effect of increased temperature on these properties is opposite to the corresponding effect on strength and stiffness, Chamis suggests that the matrix hygrothermal property retention ratio can be approximated by R Tgo − To Fh = = Ro Tgw − T 1/2 (5.41) where R = matrix hygrothermal property after hygrothermal degradation Ro = reference matrix hygrothermal property before degradation Following a procedure similar to that outlined in Section 5.2, the matrix hygrothermal property is degraded according to Equation 5.34. Then, the degraded matrix property is used in a micromechanics equation such as Equations 5.26 through 5.40 to estimate the hygrothermally degraded composite property. EXAMPLE 5.6 A composite lamina is to be designed to have a speciied CTE along a given direction. Outline a procedure to be used in the design. Solution First, it is necessary to use micromechanics equations such as Equations 5.26 and 5.30 to ind a combination of iber and matrix materials having constituent CTEs and moduli and volume fractions, so that the speciied CTE lies between the values of α1 and α2. As shown by Equation 5.22 and Figure 5.16, the value of the speciied αx along the direction deined by the angle must lie between the values of α1 and α2. The required angle θ is then found by setting αx equal to the speciied value and solving the irst of Equation 5.22. In a practical design problem, other requirements such as strength and stiffness may have to be considered as well. EXAMPLE 5.7 Develop an analytical model for determination of the CHE, β, for a randomly oriented continuous iber composite in terms of iber and matrix properties and volume fractions. Assume that the composite is planar isotropic, and ind the β for in-plane hygroscopic expansion. Solution For the planar isotropic case, β is independent of orientation in the plane, and it is appropriate to use an averaging approach similar to that used in Example 2.7. Thus, the isotropic β is found by irst using a transformation Analysis of Lamina Hygrothermal Behavior 225 equation similar to Equation 5.22 to ind the βx for the orthotropic lamina of the same material along the x-direction as β x = β1 cos 2 θ + β 2 sin 2 θ This value is now averaged over all possible angles between θ = 0 and θ = π to get the isotropic property as π β= ∫ β dθ ∫ dθ x 0 π 0 π ∫ (β = 1 cos 2 θ + β 2 sin 2 θ)dθ 0 π π β2 sin 2θ θ 4 + 2 + π 0 = β1 π = β1 + β 2 2 π −sin 2θ θ + 4 2 0 where the orthotropic properties β1 and β2 may be estimated from iber and matrix properties and volume fractions by using micromechanics equations such as Equations 5.35 and 5.36. EXAMPLE 5.8 A hybrid unidirectional S-glass/Kevlar/high-modulus (HM) epoxy composite lamina has twice as many S-glass ibers as Kevlar ibers and the total iber-volume fraction is 0.6. Determine the longitudinal and transverse CTEs for the composite. Solution From Table 3.1, the properties for the S-glass ibers are ES1 = 12.4 × 106 psi αS1 = 2.8 × 10−6 in./in./°F αS2 = 2.8 × 10−6 in./in./°F The properties for the Kevlar ibers are EK1 = 22 × 106 psi αK1 = −2.2 × 10−6 in./in./°F αK2 = 30 × 10−6 in./in./°F Principles of Composite Material Mechanics 226 From Table 3.2, the properties of the HM epoxy matrix are Em = 0.75 × 106 psi αm1 = αm2 = αm = 40 × 10−6 in./in./°F The iber-volume fractions for S-glass and Kevlar are related by υS = 2υK and υS + υK = 0.6 and all of the constituent volume fractions are related by υS + υK + υm = 1.0 so υS = 0.4, υK = 0.2, υm = 0.4. Generalizing Equation 5.26 for the hybrid composite with three constituents, the longitudinal CTE is α1 = ES1α S1υS + EK1α K1υK + Emα m υm = 1.68 × 10 −6 /in./in./°F ES1υS + EK1υK + Em υm Similarly, generalizing Equation 5.30 for the hybrid composite, the transverse CTE is estimated to be α 2 = α S 2 υS + α K 2 υK + α m υm = 23 × 10 −6 /in./in./°F Note that α2 ≫ α1. This is due to the negative longitudinal CTE of the Kevlar ibers, the large positive transverse CTE of the Kevlar ibers and the strong inluence of the matrix CTE on α2. PROBLEM 5.16 Derive Equation 5.35. PROBLEM 5.17 Develop an analytical model for determination of the CTE, α, for a randomly oriented continuous iber composite in terms of iber and matrix properties and volume fractions. Assume that the composite is planar isotropic and ind the α for in-plane thermal expansion. PROBLEM 5.18 A unidirectional continuous iber composite is to be made from T300 graphite ibers in a HM epoxy matrix, and the composite is to have a longitudinal CTE of zero. Using the iber and matrix properties in Tables 3.1 and 3.2, Analysis of Lamina Hygrothermal Behavior 227 determine the required iber-volume fraction. Is this a practical composite? Sketch a graph showing the longitudinal CTE of the composite versus the iber-volume fraction, and show the range of iber-volume fractions over which the longitudinal CTE would be negative. PROBLEM 5.19 A unidirectional graphite/epoxy lamina having the properties described in Problem 5.10 is to be designed to have a CTE of zero along a particular axis. Determine the required lamina orientation for such a design. PROBLEM 5.20 A representative volume element (RVE) consisting of a cylindrical isotropic iber embedded and perfectly bonded in a cylinder of isotropic matrix material is shown in Figure 5.23. If the ends of the RVE at x = 0 and x = L and the outer surface of the RVE are stress free and the RVE is subjected to a uniform temperature change ΔT, determine the iber stress, σf, and the matrix stress, σm, along the iber direction at the midpoint of the RVE (at x = L/2). Use a mechanics of materials approach and express answers in terms of the coeficients of thermal expansion αf and αm, the cross-sectional areas Af and Am, the Young’s moduli Ef and Em, and the temperature change, ΔT, where the subscripts f and m refer to iber and matrix, respectively. PROBLEM 5.21 A hybrid unidirectional E-glass/T-300 carbon/intermediate-modulus high-strength epoxy composite is to be designed to have an overall longitudinal thermal expansion coeficient of zero in order to ensure the best possible thermal stability under varying service temperatures. It is also required that in order to ensure that the material will be suficiently stiff, the volume fraction of T-300 carbon ibers is to be twice the volume fraction of the E-glass ibers. (a) Using the properties in Tables 3.1 and 3.2 and neglecting voids in the material, determine the required volume fractions of T-300 carbon ibers and E-glass ibers. (b) Assuming that the T-300 carbon ibers and E-glass ibers have approximately the same diameters, and Fiber: Af , Ef , αf , and σf Matrix: Am, Em, αm, and σm x FIGURE 5.23 RVE for Problem 5.20. L 228 Principles of Composite Material Mechanics that the ibers are packed in a triangular array, is the composite design of part (a) feasible? PROBLEM 5.22 Derive Equations 5.26 and 5.30. References 1. Browning, C. E., Husman, G. E., and Whitney, J. M. 1977. Moisture effects in epoxy matrix composites. Composite Materials: Testing and Design: Fourth Conference, ASTM STP 617, pp. 481–496. American Society for Testing and Materials, Philadelphia, PA. 2. Gibson, R. F., Yau, A., Mende, E. W., and Osborn, W. E. 1982. The inluence of environmental conditions on the vibration characteristics of chopped iber reinforced composite materials. Journal of Reinforced Plastics and Composites, 1(3), 225–241. 3. Shen, C. H. and Springer, G. S. 1976. Moisture absorption and desorption of composite materials. Journal of Composite Materials, 10, 2–20. 4. Jost, W. 1952. Diffusion in Solids, Liquids, Gases. Academic Press, Inc., New York, NY. 5. Loos, A. C., Springer, G. S., Sanders, B. A., and Tung, R. W. 1981. Moisture absorption of polyester-E glass composites. In Springer, G. S. ed., Environmental Effects on Composite Materials, pp. 51–62. Technomic Publishing Co., Lancaster, PA. 6. Cai, L. W. and Weitsman, Y. 1994. Non-Fickian moisture diffusion in polymeric composites. Journal of Composite Materials, 28(2), 130–154. 7. Weitsman, Y. 2000. Effects of luids on polymeric composites—A review. In Kelly, A. and Zweben, C., editors-in-chief, Comprehensive Composite Materials, Talreja, R. and Manson, J.-A. E., eds., Polymeric Matrix Composites, Vol. 2, pp. 369–401. Elsevier Science Publishers, Amsterdam. 8. Weitsman, Y. and Elahi, M. 2000. Effects of luids on the deformation, strength and durability of polymeric composites—An overview. Mechanics of TimeDependent Materials, 4, 107–126. 9. Chamis, C. C. and Sinclair, J. H. 1982. Durability/life of iber composites in hygrothermomechanical environments. In Daniel, I. M. ed., Composite Materials: Testing and Design (Sixth Conference), ASTM STP 787, pp. 498–512. American Society for Testing and Materials, Philadelphia, PA. 10. Chamis, C. C. 1987. Simpliied composite micromechanics equations for mechanical, thermal, and moisture-related properties. In Weeton, J. W. et al., eds., Engineers’ Guide to Composite Materials, pp. 3-8–3-24. ASM International, Materials Park, OH. 11. DeIasi, R. and Whiteside, J. B. 1987. Effect of moisture on epoxy resins and composites. In Vinson, J. R. ed., Advanced Composite Materials—Environmental Effects, ASTM STP 658, pp. 2–20. American Society for Testing and Materials, Philadelphia, PA. Analysis of Lamina Hygrothermal Behavior 229 12. Loos, A. C. and Springer, G. S. 1981. Moisture absorption of graphite/epoxy composites immersed in liquids and in humid air. In Springer, G. S. ed., Environmental Effects on Composite Materials, pp. 34–50. Technomic Publishing Co., Lancaster, PA. 13. Fahmy, A. A. and Hurt, J. C. 1980. Stress dependence of water diffusion in epoxy resins. Polymer Composites, 1(2), 77–80. 14. Marom, G. and Broutman, L. J. 1981. Moisture penetration into composites under external stress. Polymer Composites, 2(3), 132–136. 15. Weitsman, Y. 1987. Stress assisted diffusion in elastic and viscoelastic materials. Journal of the Mechanics and Physics of Solids, 35(1), 73–94. 16. Cairns, D. S. and Adams, D. F. 1984. Moisture and thermal expansion properties of unidirectional composite materials and the epoxy matrix. In Springer, G. S. ed., Environmental Effects on Composite Materials, Vol. 2, pp. 300–316. Technomic Publishing Co., Lancaster, PA. 17. Adams, D. F., Carlsson, L. A., and Pipes, R. B., 2003. Experimental Characterization of Advanced Composite Materials. CRC Press, Boca Raton, FL. 18. Graves, S. R. and Adams, D. F. 1981. Analysis of a bonded joint in a composite tube subjected to torsion. Journal of Composite Materials, 15, 211–224. 19. Schapery, R. A. 1968. Thermal expansion coeficients of composite materials based on energy principles. Journal of Composite Materials, 2(3), 380–404. 20. Hashin, Z. 1979. Analysis of properties of iber composites with anisotropic constituents. Journal of Applied Mechanics, 46, 543–550. 21. Rosen, B. W. 1987. Composite materials analysis and design. In Reinhart, T. J. ed., Engineered Materials Handbook, Vol. 1, Composites, Section 4, pp. 173–281. ASM International, Materials Park, OH. 22. Ishikawa, T., Koyama, K., and Kobayashi, S. 1978. Thermal expansion coeficients of unidirectional composites. Journal of Composite Materials, 12, 153–168. 23. Karadeniz, Z. and Kumlutas, D. 2007. A numerical study on the coeficients of thermal expansion of iber reinforced composite materials. Composite Structures, 78, 1–10. 24. Sideridis, E. 1994. Thermal expansion coeficient of iber composites deined by the concept of an interphase. Composites Science and Technology, 51, 301–317. 25. Rosen, B. W. and Hashin, Z. 1970. Effective thermal expansion coeficients and speciic heats of composite materials. International Journal of Engineering Science, 8, 157–173. 26. Dong, C. 2008. Development of a model for predicting the transverse coeficients of thermal expansion of unidirectional carbon ibre reinforced composite materials. Applied Composite Materials, 15, 171–182. 27. Gibson, R. F. and Muller, A. 2010. Unpublished research, University of Nevada, Reno, NV. 28. Ashton, J. E., Halpin, J. C., and Petit, P. H. 1969. Primer on Composite Materials: Analysis. Technomic Publishing Co., Lancaster, PA. 29. Hopkins, D. A. and Chamis, C. C. 1988. A unique set of micromechanics equations for high temperature metal matrix composites. In DiGiovanni, P. R. and Adsit, N. R., eds., Testing Technology of Metal Matrix Composites, ASTM STP 964, pp. 159–176. American Society for Testing and Materials, Philadelphia, PA. 6 Analysis of a Discontinuously Reinforced Lamina 6.1 Introduction In Chapters 2 through 5, we discussed the analysis of continuous iberreinforced composites. The effects of iber discontinuity or iber length on composite mechanical behavior were not taken into account in these analyses since it was assumed that the ibers extended from one end of the lamina to the other. This chapter is concerned with the mechanical behavior of laminae featured by discontinuous iber or particulate reinforcement. Short-iber-reinforced or particulate-reinforced composites are typically not as strong or as stiff as continuous iber-reinforced composites and are not likely to be used in critical structural applications such as aircraft primary structures (but this may change as the full potential of new discontinuous reinforcements such as carbon nanotubes [CNTs] or nanoparticles is realized). On the other hand, discontinuously reinforced composites do have several attractive characteristics that make them worthy of consideration for other applications. For example, in components characterized by complex geometrical contours, continuous ibers may not be practical because they may not conform to the desired shape without being damaged or distorted from the desired pattern. However, short ibers or particles can be easily mixed with the liquid matrix resin, and the resin/iber or resin/particle mixture can be injection or compression molded to produce parts with complex shapes. Such processing methods are also fast and inexpensive, which makes them very attractive for high-volume applications. Composites having randomly oriented, short-iber reinforcements or particulate reinforcements are nearly isotropic, whereas unidirectional continuous iber composites are highly anisotropic. In many applications, the advantages of low cost, ease of fabricating complex parts, and isotropic behavior are enough to make short-iber or particulate composites the material of choice. This has been especially true since the 1991 discovery of CNTs (the “ultimate short ibers,” which are currently believed to be the strongest materials that mankind is 231 Principles of Composite Material Mechanics 232 (a) (b) (d) (c) (e) FIGURE 6.1 Types of discontinuous reinforcement. (a) Aligned discontinuous ibers, (b) off-axis-aligned discontinuous ibers, (c) randomly oriented discontinuous ibers, (d) particulate reinforcement, and (e) hybrid multiscale reinforcement. capable of producing), and much attention has been directed toward their use as reinforcement in composites. Short-iber composites with three types of iber reinforcement will be considered here: aligned discontinuous ibers (Figure 6.1a), off-axis-aligned discontinuous ibers (Figure 6.1b), and randomly oriented discontinuous ibers (Figure 6.1c). Particulate-reinforced composites (Figure 6.1d) and hybrid multiscale composites having both iber and particulate reinforcements of different size scales (Figure 6.1e) are also considered. Nanoibers, nanoparticles, or nanotubes can be used in any of these arrangements, but because of their extremely tiny dimensions, they are most often randomly oriented in all three dimensions. As indicated earlier in Section 1.4, nanoenhancement of the matrix materials (i.e., replacing the polymer matrix material with a nanocomposite) in conventional iber-reinforced composites has made possible the development of a variety of new multifunctional composites. Although the randomly oriented, short-iber composites (Figure 6.1c) are currently the most widely used, the development of the analytical models logically begins with the simplest case, that of aligned short ibers in Figure 6.1a. 6.2 Aligned Discontinuous Fibers The analysis of the specially orthotropic aligned discontinuous iber composite in Figure 6.1a begins with the selection of an representative volume element (RVE) consisting of a short iber embedded in a cylinder of matrix material, as shown in Figure 6.2. Several models are based on the simpliied RVE in Figure 6.2b, which does not include matrix material at the ends of Analysis of a Discontinuously Reinforced Lamina (a) 233 Matrix Fiber L (b) Matrix Fiber d D FIGURE 6.2 RVEs for aligned discontinuous iber composite. (a) Matrix material included at ends of iber and (b) matrix material not included at ends of iber. the iber as the model in Figure 6.2a does. Before beginning the analysis, however, it is instructive to consider the geometry of deformation in the RVE of Figure 6.2a. As shown by the grid lines before and after deformation in Figure 6.3, the stiffness mismatch between iber and matrix (Ef ≫ Em) leads to large shear deformations near the iber ends but no shear deformation at the middle of the iber. That is, if Ef = Em, there is no mismatch in stiffness between iber and matrix, and no iber–matrix interfacial shear takes place. But as Ef increases relative to Em, the interfacial shear stress and distortion increases. As we will see later, the stress transfer between matrix and iber occurs primarily through interfacial shear, which is the greatest near the iber ends. On the other hand, the normal stress in the iber builds from a minimum at the iber ends to a maximum in the middle of the iber. 6.2.1 Stress and Strength Analysis The above observations based on the geometry of deformation will now be conirmed by considering the free-body diagram of a differential element of Before deformation Fiber After deformation Fiber FIGURE 6.3 Schematic representation of matrix shear deformation in a short-iber composite. Principles of Composite Material Mechanics 234 L d D dx x σf σf + dσf τ FIGURE 6.4 Stresses acting on a differential element of iber. the iber from the RVE, as shown in Figure 6.4. For static equilibrium of the forces along the x-direction, ∑ Fx = (σ f + dσ f ) πd 2 πd 2 − σf − τ(πd) dx = 0 4 4 (6.1) where σf = iber normal stress along the x-direction at a distance x from the end of the iber Fx = force along the x-direction τ = interfacial shear stress at a distance x from the end of the iber d = iber diameter, a constant dx = length of the differential element dσf = differential change in stress σf Simplifying and rearranging the above equation, we obtain the differential equation relating the rate of change of the iber normal stress along the x-direction to the interfacial shear stress: dσ f 4τ = dx d (6.2) Separating variables and integrating, we ind that σf ∫ σ0 x dσ f = 4 τ dx d ∫ 0 (6.3) Analysis of a Discontinuously Reinforced Lamina 235 It is commonly assumed that essentially all of the stress transfer from matrix to iber occurs by interfacial shear around the periphery of the iber, and that the iber normal stress, σ0, which is transferred across the ends of the iber, is negligible. With this assumption, Equation 6.3 becomes x 4 σf = τ dx d ∫ (6.4) 0 Thus, if we want to determine the iber stress, σf, we must know the interfacial shear stress, τ, as a function of the distance x. Two basic approaches have been proposed, both of which are based on assumptions regarding the behavior of the matrix material. Kelly and Tyson [1] assumed that the matrix is rigid plastic, as shown in the stress–strain curve in Figure 6.5a. Cox [2] assumed that the matrix is linear elastic, as shown in Figure 6.5b. Both models are based on the assumption of linear elastic ibers. We will consider both models, but it is convenient to use the Kelly–Tyson model for illustrative purposes at this point. The Kelly–Tyson model is much simpler than the Cox model because the interfacial shear stress, τ, is everywhere equal to the matrix yield stress in shear, τy. Thus, for the Kelly–Tyson model, the resulting iber stress from Equation 6.4 is now σf = 4 τyx d (6.5) This equation tells us that the iber stress varies linearly with the distance from the iber end, but we also know that the iber stress distribution must be symmetric about x = L/2. Since it has been assumed that σf = σ0 = 0 at x = 0 and, by symmetry, at x = L, the iber stress distribution and the corresponding shear stress distribution must be as shown in Figure 6.6. The stress distributions in Figure 6.6 are actually valid only for ibers having lengths less (b) τy Shear strain (γ ) Shear stress (τ) Shear stress (τ) (a) Gm Shear strain (γ ) FIGURE 6.5 Assumed stress–strain curves for matrix material in the (a) Kelly–Tyson and (b) Cox models. Principles of Composite Material Mechanics 236 τ τy τy x L L 2 σf σfmax x FIGURE 6.6 Variation of interfacial shear stress, τ, and iber normal stress, σf, with distance along the iber according to the Kelly–Tyson model. than a certain value, as we will see later. The maximum iber stress for such a iber occurs at x = L/2 and is given by σ f max = 4 L 2τ y L τy = d 2 d (6.6) The maximum iber stress cannot keep increasing indeinitely as the iber length L is increased, however. If the iber is assumed to be elastic, σfmax cannot exceed the value Ef1 σc1/E1, which is the iber stress in a continuous iber composite under longitudinal composite stress, σc1 (recall Section 3.2.1). Thus, as σfmax approaches the limiting value Ef1 σc1/E1, the iber length, L, approaches a value Li, which has been referred to as the “ineffective length” [3] or the “load transfer length” [4]. The equation for Li is therefore Li = dEf1σ c1 2τ y E1 (6.7) The effect of increasing iber length on the iber stress and shear stress distributions is shown graphically in Figure 6.7. Note that no matter how long the iber is, the load transfer between iber and matrix (by virtue of the interfacial shear stress, τ) only occurs over the length, Li. The length Li has been referred to as the “ineffective length” because the iber stress is less than its maximum value for this portion of the iber. The term “load transfer length” comes from the fact that the load transfer between iber and matrix only occurs over this portion of the iber. Although these results are for the Kelly–Tyson model, similar results are obtained from the Cox model. The stress distributions along the iber in Figure 6.7 are based on the Kelly–Tyson assumption that the interfacial shear stress is constant. For comparison, Analysis of a Discontinuously Reinforced Lamina L < Li Li 2 τ τy L = Li Li 2 237 L > Li Li 2 Li 2 x σf Ef1 σc1/E1 x FIGURE 6.7 Effect of iber length on stress distributions along the iber according to the Kelly–Tyson model. Figure 6.8 shows the corresponding stress distributions when the interfacial shear stress is assumed to vary linearly along the iber. Another limiting value of the iber stress occurs when σfmax is equal to the iber tensile strength, sf1(+ ) . In this case, the applied composite stress is such that Ef1σ c1 = σ f max = sf1( + ) E1 (a) (6.8) τ = τmax 1 – τmax 2 x L τ x L 2 L (b) σf = σf 4τmax d x– x2 L FIGURE 6.8 (a) Linear interfacial shear stress distribution along a short-iber and (b) corresponding iber tensile normal stress distribution. Principles of Composite Material Mechanics 238 The corresponding iber length now becomes L = Lc, where L c is referred to as the “critical length.” For this condition, substitution of Equation 6.8 into Equation 6.6 yields the equation for the critical length as dsf1( + ) 2τ y Lc = (6.9) The critical length has important implications for the calculation of longitudinal composite strength. Recall from Equation 3.23 that the average longitudinal composite stress for loading along the iber direction is given by σ c1 = σ f 1υf + σ m1υm (3.23) Then Equation 4.22 for longitudinal composite strength of a continuous iber-reinforced lamina was developed from Equation 3.23 by assuming that the continuous ibers were uniformly stressed along their entire lengths, and that the ibers failed before the matrix when the average iber stress σ f1 reached the iber tensile strength sf1(+ ) . However, in the case of discontinuous ibers, it should be clear from the previous developments in this section that the ibers are not uniformly stressed along their entire lengths, and that the iber length must be taken into account. For the discontinuous ibers, the average longitudinal iber stress in Equation 3.23 may be found from σ f1 = ∫ L/ 2 σ f1 dx (6.10) 0 L/2 Evaluation of this integral depends on the iber length. From Figure 6.7, it can be seen that for L ≤ Li, the iber stress varies linearly with x as σ f1 = σ f max x Li /2 (6.11) and Equation 6.10 becomes σ f1 = ∫ L/ 2 [σ f max x/(Li /2)] dx 0 L/2 = σ f max L 2Li (6.12) whereas for the case L ≥ Li, the corresponding average stress is σ f1 ∫ = Li /2 [σ f max x/(Li /2)] dx + 0 L/2 ∫ L/ 2 σ f max dx Li/2 L = 1 − i σ f max 2L (6.13) Analysis of a Discontinuously Reinforced Lamina 239 It should be kept in mind here that L is the variable iber length and Li is the speciic value of iber length over which load transfer takes place. Therefore, for the speciic case of iber failure and corresponding composite failure, substitution of the conditions σ f max = s(f +1 ) , σ c1 = sL( + ) , σ m = s(mf+ )1 , and Li = Lc along with Equation 6.12 into Equation 3.23 gives the longitudinal composite strength as sL( + ) = sf1( + )L (+ ) (1 − υf ) for L ≤ Lc υf + smf1 2Lc (6.14) while similar substitution of the conditions σ f max = sf1( + ) , σ c1 = sL( + ) , σ m = s(mf+ )1 , and Li = Lc along with Equation 6.13 into Equation 3.23 gives the longitudinal composite strength as L (+ ) sL( + ) = 1 − c sf1( + )υf + smf1 (1 − υf ) for L ≥ Lc 2L (6.15) It has been assumed in Equations 6.14 and 6.15 that the average stress in the matrix at iber failure is σ m = s(mf+ )1 in accordance with Figure 4.12a and Equation 4.22. Note that, when L ≫ Lc, Equation 6.15 approaches Equation 4.22 for continuous ibers. Alternatively, Equation 6.9 can be rearranged to give the interfacial shear strength, τy, corresponding to the critical length τy = dsf1( + ) 2Lc (6.16) This equation has been used by Drzal et al. [5,6] and others to determine the interfacial shear strength from measurements of critical length. In such an experiment, a specimen consisting of a single iber embedded in a strip of translucent matrix material is mounted under a microscope and then subjected to an increasing tensile load. Once the iber stress reaches sf1(+ ) , the iber breaks up into segments having a statistical distribution about the critical length, L c, and the corresponding statistical parameters describing the interfacial shear strength are calculated using Equation 6.9. 6.2.2 Modulus Analysis Expressions for the longitudinal modulus of the aligned discontinuous iber composite can be found using either the Kelly–Tyson model or the Cox model, but only the derivation of the Cox model, extended further by Kelly [7], will be discussed here. A similar model, which is often referred to as a “shear-lag” model, was developed by Rosen [8]. For the RVE of Figure 6.2b, Principles of Composite Material Mechanics 240 recall from Equation 6.2 that the rate of change of the axial load in the iber with respect to distance along the iber is a linear function of the interfacial shear stress. Cox further assumed that the interfacial shear stress is proportional to the difference between u and v, where u is the axial displacement at a point in the iber, and v is the axial displacement that the matrix would have at the same point in the RVE with no iber present. Thus, the rate of change of the iber axial load P is given by dP = H (u − v ) dx (6.17) where H is a proportionality constant to be determined from geometrical and material property data. Differentiating Equation 6.17 once with respect to x, we ind that d2P p du dv = H − = H −e 2 dx dx Af Ef 1 dx (6.18) where the expression du P = dx Af Ef1 is taken from the elementary mechanics of materials and dv =e dx is the matrix strain with no iber present. Equation 6.18 can be rearranged in the standard form of a second-order differential equation with constant coeficients as d2P − β 2P = − He dx 2 (6.19) where β2 = H Af Ef1 The solution to Equation 6.19 is of the form P = Pp + Ph (6.20) Analysis of a Discontinuously Reinforced Lamina 241 where Pp = particular solution = AfEf1e Ph = homogeneous solution = R sinh βx + S cosh βx The coeficients R and S must be determined from the boundary conditions P = 0 at x = 0 and x = L. After using trigonometric identities and further manipulation, the resulting iber stress is σ f1 = coshβ (0.5L − x) P = Ef1e Af cosh (0.5βL) (6.21) The average iber stress is then σ f1 = ∫ L/ 2 σ f1 dx 0 L/2 tanh (βL/2) = Ef1e 1 − βL/2 (6.22) From the equilibrium of the composite for longitudinal loading, recall the rule of mixtures for stress (Equation 3.22), which is also valid for the RVE of Figure 6.2b: σ c1 = σ f 1υf + σ m1υm (6.23) Substituting Equation 6.22 into Equation 6.23, dividing Equation 6.23 by e, assuming that the applied composite stress produces a strain, e, in composite, iber, and matrix, and using Hooke’s law for composite and matrix, we ind the equation for the longitudinal modulus of the Cox model: tanh (βL/2) Ec1 = Ef 1 1 − υf + Em υm βL/2 (6.24) Note that the assumption of equal strains in iber and matrix here does not violate the original assumptions about the displacements u and v being different, because v is the displacement in a piece of unreinforced matrix material. The term inside the brackets represents the effect of iber length on the composite modulus. The parameter β in the above equations and the interfacial shear stress, τ, can be determined by considering the shear strain in the matrix, as shown by Kelly [7]. The results are β2 = 2πGm Af Ef1ln (D/d) (6.25) Principles of Composite Material Mechanics 242 and τ= dEf1eβ sinh β (0.5L − x) 4 cosh (0.5βL) (6.26) where Gm is the matrix shear modulus and D is the outside diameter of the RVE, as shown in Figure 6.2. The predicted variations of the iber stress and the interfacial shear stress from the Cox model when the iber length L < Li are shown schematically in Figure 6.9. Notice the difference between these stress distributions and the ones from the Kelly–Tyson model in Figure 6.6. For the Cox stresses evaluated at the midpoint of the iber (x = L/2), as L → Li, the term in brackets in Equation 6.21 approaches the value 1.0, whereas the term in brackets in Equation 6.26 approaches zero. Figure 6.10 graphically shows how the longitudinal modulus Ec1 in Equation 6.24 varies with iber length L. As we might expect, Ec1 increases with increasing iber length. Note that as the iber length L → ∞, Ec1 → Ef1υf + Emυm, the rule of mixtures value for a continuous iber composite, and that as L → 0, Ec1 → Emυm, which represents the matrix contribution only. Another variation on the Cox model was developed by Gibson et al. [9], who used the Cox stresses, σf and τ, in a strain energy method similar to that outlined in Equations 3.28 and 3.29. The longitudinal modulus calculated by the energy method was found to agree closely with Equation 6.24, and the predicted variation of Ec1 with iber aspect ratio, L/d, is shown for several composites in Figure 6.11. It is also interesting to see that the iber length does not have to be very large relative to the iber diameter to bring the modulus Ec1 very close to the limiting value for a continuous iber composite, as given by the rule of mixtures. For all practical purposes, Equation 6.24 predicts that the aligned discontinuous iber composites of the types shown in Figure 6.11 have the longitudinal modulus of a continuous iber composite if the iber aspect ratio L/d > 100. τ x L σf x FIGURE 6.9 Variation of interfacial shear stress, τ, and iber normal stress, σf, with distance along the iber according to the Cox model. Analysis of a Discontinuously Reinforced Lamina 243 Ef1υf + Emυm (3.27) Ec1 Ec1 = Ef1 1– E mυm tanh(βL/2) υf + Emυm βL/2 (6.24) as L → ∞, Ec1 → Ef1υf + Emυm L as L → 0, Ec1 → Emυ m FIGURE 6.10 Variation of longitudinal modulus Ec1 with iber length L according to Equation 6.24. Although the Kelly–Tyson model and the Cox model both provide valuable insight into the concepts of load transfer, iber length effects, and strength and modulus analysis, neither model accurately predicts the stress distributions. For example, more recent results from inite element analyses [10,11] and experimental photoelasticity [7,12,13] indicate that both the magnitude and the rate of change of the interfacial shear stresses near the end of the iber are much higher than those predicted by the Kelly–Tyson or Cox models. A typical comparison of predicted shear stress distributions along the iber from inite element analysis (FEA) and from the Cox model is shown in Figure 6.12. The inite element predictions of Sun and Wu [11] also showed good agreement with experimental photoelasticity results. FEAs have also been used to study the effects of different iber end shapes on the stress distributions [10,11]. 100 3 2 10 Ecl/Em 1 Energy model, υf = 0.5 1. Glass–epoxy. Ef/Em = 19 2. Graphite–epoxy. Ef/Em = 104 2. Whisker–epoxy. Ef/Em = 182 1 0.1 10 102 103 Fiber aspect ratio (L/d ) 104 105 FIGURE 6.11 Variation of modulus ratio, Ec1/Em, with iber aspect ratio, L/d, for several composites. (From Gibson, R. F., Chaturvedi, S. K., and Sun, C. T. 1982. Journal of Materials Science, 17, 3499–3509. Reprinted with permission from Chapman & Hall.) Principles of Composite Material Mechanics 244 6 Boron/epoxy model Fiber volume fraction 0.56 Fiber aspect ratio 15.625 Shear stress (102 psi) 5 4 Legend Analytical data from ﬁnite element method Theoretical curve from Cox’s model 3 2 1 0 0 0.1 0.2 0.3 0.4 Dimensionless distance from ﬁber end (x/L) 0.5 FIGURE 6.12 Predicted shear stress distributions along the iber from FEA and the Cox model. (From Hwang, S. J. 1985. Finite element modeling of damping in discontinuous iber composites. MS thesis, University of Idaho, Moscow, ID. With permission.) It is important to remember that both the Kelly–Tyson and the Cox models were derived for the RVE in Figure 6.2b, which does not include matrix material at the ends of the iber. One result is that the actual modulus values are lower than predicted by Equation 6.24. For example, the experimental results of Suarez et al. [14] on aligned discontinuous graphite/epoxy composites having various iber aspect ratios, L/d, are shown in Figure 6.13. The experimental modulus data at different iber aspect ratios in Figure 6.13 were obtained from the test specimens shown schematically in Figure 6.14, which were manufactured using a conventional unidirectional prepreg tape that had been cut at intervals of length L before being processed with a standard autoclave-style cure cycle. The measured moduli are seen to be well below the predicted curve from the Cox model. In order to shift the predicted curve to match the experimental results better, Suarez et al. introduced the concept of an “effective iber aspect ratio,” (L/d)eff, which would account for the fact that the reinforcement was not a single iber but, rather, a bundle of ibers having an aspect ratio lower than that of a single iber. The effective iber aspect ratio is deined as L L = Z d eff d (6.27) where Z is a curve-itting parameter that accomplishes a horizontal shift of the curve of Ec1 versus L/d. Before the horizontal shift, the predicted curve was shifted vertically by using a reduced iber modulus to account for Analysis of a Discontinuously Reinforced Lamina 245 40 Graphite epoxy specimens Fiber volume fraction 0.654 Ecl/Em 30 20 Legend Force-balance approach Mean experimental values (0.632 < υf < 0.666) Experimental scatter 10 0 1E+001 1E+002 1E+003 1E+004 Fiber aspect ratio (L/d ) 1E+005 FIGURE 6.13 Comparison of measured and predicted (Cox model) longitudinal moduli of aligned discontinuous iber graphite/epoxy for various iber aspect ratios. (L/d)eff = L/d. (From Suarez, S. A. et al. 1986. Experimental Mechanics, 26(2), 175–184. With permission.) possible degradation of iber properties or iber misalignment during fabrication. The results of vertical and horizontal shifting of the graphite/epoxy curve of Figure 6.13 are shown in Figure 6.15, and the agreement is very good. Similar results were reported for aramid/epoxy and boron/epoxy. This approach did not take into account the matrix material between the iber ends, however. Hwang and Gibson [15] studied the effect of the iber end gap on the composite modulus by using both FEA and a modiied Cox model. The modiied L L L L L Unidirectional laminate made from prepreg tape cut with a knife at intervals of length L FIGURE 6.14 Aligned discontinuous iber composite test specimen fabricated from a unidirectional prepreg tape cut at intervals of length L before curing. Principles of Composite Material Mechanics 246 40 Graphite epoxy specimens Fiber volume fraction 0.654 Ecl/Em 30 20 Legend Corrected force-balance approach (parameter for L/d = 0.03) Mean experimental values Experimental scatter 10 0 1E+001 1E+002 1E+003 1E+004 Fiber aspect ratio (L/d ) 1E+005 FIGURE 6.15 Comparison of measured and predicted (Cox model corrected for iber aspect ratio) longitudinal moduli of aligned discontinuous iber graphite/epoxy for various iber aspect ratios. (L/d)eff = 0.03 L/d. (From Suarez, S. A. et al. 1986. Experimental Mechanics, 26(2), 175–184. With permission.) Cox model consists of the Cox model (Figure 6.2b) with one piece of matrix material attached on each end, as shown schematically in Figure 6.16. Following the development of Equation 3.36 for the series arrangement of elements under longitudinal stress, with the assumption of equal stresses in each element, the modiied Cox modulus is 1 υ υ L/(L + e) e/(L + e ) = c1 + m = + EMc1 Ec1 Em Ec1 Em (6.28) where EMc1 = longitudinal modulus of the modiied Cox model υc1 = volume fraction of the Cox model in the modiied Cox model L = length of the Cox model e = distance between iber ends in the modiied Cox model L + e = length of the modiied Cox model Figure 6.17 shows a comparison of predictions from a inite element model and the modiied Cox model, with experimental data for boron/epoxy. Micromechanical predictions using the inite element method in Figure 6.17 were obtained using quarter domain models from RVEs of discontinuous aligned composites, as shown schematically in Figure 6.18. The moduli of the inite element models having different iber aspect ratios, L/d, and abutting iber end separations, e, were calculated using an equation similar to Analysis of a Discontinuously Reinforced Lamina e L 247 e Fiber Fiber Fiber Matrix Matrix Matrix d Modified Cox model e 2 L e 2 Matrix Composite Matrix Cox model FIGURE 6.16 Modiied Cox model including matrix material at ends of iber. (From Hwang, S. J. and Gibson, R. F. 1987. Journal of Engineering Materials and Technology, 109, 47–52. Reprinted with permission from ASME.) 50 Modified Cox model e for = 0.125 d 2 e for = 0.250 d 2 for e = 0.375 d 2 Modulus ratio (El/Em) 40 30 Experimental data 20 FEM data for e = 0.125 d 2 FEM data for e = 0.250 d 2 FEM data for e = 0.375 d 2 10 0 0 10 20 30 40 50 Fiber aspect ratio (L/d ) 60 70 80 FIGURE 6.17 Comparison of predictions from the modiied Cox model and FEA with experimental data for boron/epoxy-aligned discontinuous iber composite at different iber aspect ratios. (From Hwang, S. J. and Gibson, R. F. 1987. Journal of Engineering Materials and Technology, 109, 47–52. Reprinted with permission from ASME.) Principles of Composite Material Mechanics 248 Representative volume element Matrix Fiber d L e 2 Quarter domain finite element mesh σc FIGURE 6.18 Quarter domain inite element model from RVE of discontinuous aligned iber. Equation 3.62 and a procedure similar to that described in the discussion of Equation 3.62. The modiied Cox model shows good agreement with both the FEA and experimental data. Halpin [16] has proposed a modiication of the Halpin–Tsai equations (recall Section 3.5) as another approach to estimate the longitudinal modulus of the aligned discontinuous iber composite. The proposed equations are E1 1 + ξηυf = Em 1 − ηυf (6.29) where η= (Ef1/Em ) − 1 (Ef1/Em ) + ξ (6.30) and the suggested value of the curve-itting parameter is ξ = 2L/d. Figure 6.19 shows that the predictions from these equations give good agreement with experimental data. Halpin also concluded that E2, G12, and ν12 are not signiicantly affected by the iber length [16]. Thus, Equations 3.63 and 3.64 for E2 in the continuous iber case can also be used for the discontinuous iber case. Similar equations can be used for Gl2, as described in Section 3.5, and Equation 3.45 can be used for ν12. Other micromechanics equations for predicting stiffness of unidirectional short-iber composites are summarized in the review article by Tucker and Liang [17]. Analysis of a Discontinuously Reinforced Lamina 249 105 El (psi) Halpin–Tsai equation 104 υf = 0.35 Ef = 97.3 Em Nylon/rubber 103 0 102 10 103 L/d FIGURE 6.19 Dependence of longitudinal modulus on iber aspect ratio for aligned discontinuous iber nylon/rubber composite. Predictions from the Halpin–Tsai equations are compared with experimental results. (From Halpin, J. C. 1969. Journal of Composite Materials, 3, 732–734. Reprinted with permission from Technomic Publishing Co.) 6.3 Off-Axis-Aligned Discontinuous Fibers 6.3.1 Stress and Strength Analysis The generally orthotropic aligned discontinuous iber composite can be conveniently analyzed by using the RVE shown in Figure 6.20, where the short iber is oriented at an angle with the loading axis. Chon and Sun [18] used this RVE to develop a generalized shear-lag analysis of the off-axis short-iber composite. Only the key results will be summarized here as the equations are quite lengthy. The predicted variations of the interfacial shear stress and the iber stress with the distance along the iber for various angles are shown in Figure 6.21. Note that the results from the Cox model (recall Figure 6.9) are recovered for the case of iber orientation α = 0°, and that the stress distribution curves are just shifted up or down as the angle α changes. Maximum values of shear stresses and iber stresses normalized to the applied composite stress are shown for various angles α in Figure 6.22. It is seen that the maximum interfacial shear stress, τmax, occurs at some off-axis angle, that τmax decreases with increasing Ef/Gm, and that the angle corresponding to τmax increases with increasing Ef/Gm. Thus, the maximum interfacial shear stresses according to the Kelly–Tyson and Cox models are only maximum values in the case of α = 0. On the basis of these results, Chon and Sun suggest that if iber failure is the composite failure mode, the matrix should be modiied to reduce the ratio of Ef/Gm, but if failure is due to interfacial shear, Principles of Composite Material Mechanics 250 z σ ra z α z, z σf + dσf y l y lf y y x, x rm rf 0 x dz τ(0, z) x σf σ FIGURE 6.20 RVE for an off-axis short-iber composite. (From Chon, C. T. and Sun, C. T. 1980. Journal of Materials Science, 15, 931–938. Reprinted with permission from Chapman & Hall.) Ef/Gm should be increased. In more recent work, FEAs of off-axis short-iber composites, including the effects of iber angle and iber end geometry, were conducted by Sun and Wu [11]. Calculation of the off-axis strength of an aligned discontinuous iber composite can be accomplished by considering the off-axis uniaxial loading situation in Figure 4.5, where the ibers are discontinuous. For example, if the corresponding off-axis stress state described in Equation 4.3 is substituted in the Tsai–Hill criterion (Equation 4.14), the result for the off-axis strength is cos 4 θ 1 1 sin 4 θ σ x = 2 + 2 − 2 sin 2 θ cos 2 θ + 2 sLT sL sT sL −1/2 (6.31) In the evaluation of such equations for discontinuous iber composites, it is often assumed that only the longitudinal strength, sL, depends on iber length, and that the other strengths are essentially independent of iber length. In this case, depending on whether the iber length is less than or greater than the critical length, either Equation 6.14 or 6.15 can be used to estimate sL(+ ) , while the other strengths can be estimated using the micromechanical models for continuous iber composites described in Section 4.3. Analysis of a Discontinuously Reinforced Lamina 251 0.5 τ σ 0 0.2 0.4 0.6 0.8 1.0 Z = z/lf –0.5 α = 45°, θ = –90° α = 45°, θ = 0° α = 0°, 0° ≤ θ ≤ 90° α = 45°, θ = 90° α = 90°, 0° ≤ θ ≤ 90° 10 5 σf σ 0 0.2 0.4 0.6 0.8 1.0 Z = z/lf α = 90° α = 45° α = 0° FIGURE 6.21 Variation of interfacial shear stress and iber normal stress along the iber for the Chon–Sun model at various off-axis angles. (From Chon, C. T. and Sun, C. T. 1980. Journal of Materials Science, 15, 931–938. Reprinted with permission from Chapman & Hall.) 6.3.2 Modulus Analysis Elastic constants for the off-axis-aligned discontinuous iber composite may be estimated by using equations developed earlier in this chapter and in Chapters 2 and 3. Following the procedure outlined by Sun et al. [19] and Suarez et al. [14], the Cox model (Equation 6.24) is used to ind the longitudinal modulus along the 1 direction. The transverse modulus, E2, the in-plane shear modulus, G12, and the major Poisson’s ratio, ν12, are assumed to be independent of iber length [16,17] and are calculated using the micromechanics equations developed in Chapter 3. The off-axis modulus of elasticity, Ex, is then found by substituting the Cox modulus, Ec1, for E1 in the transformation equation (the irst of Equation 2.40), along with the calculated values of E2, E12, ν12, and θ. The other off-axis properties Ey, Gxy, and νxy are found by using a similar approach. The resulting set of equations is of the form Principles of Composite Material Mechanics 252 Ex = f1(Ec1 , E2 , G12 , ν12 , θ) Ey = f 2 (Ec1 , E2 , G12 , ν12 , θ) Gxy = f 3 (Ec1 , E2 , G12 , ν12 , θ) (6.32) νxy = f 4 (Ec1 , E2 , G12 , ν12 , θ) τ (Z = 1, θ = 90°) σ max A comparison of the predicted off-axis modulus, Ex, for graphite/epoxy with experimental values for various angles, θ, is shown in Figure 6.23. It should be mentioned that the good agreement between theory and experiment seen in Figure 6.23 was not possible as long as the ibers were assumed to be isotropic. Once the orthotropic nature of the graphite ibers was taken into account (i.e., Ef1 ≫ Ef2), the agreement between theory and experiment improved signiicantly. The same analysis was used to generate a tridimensional plot of the off-axis modulus, Ex, versus the iber aspect ratio and the iber orientation, as shown in Figure 6.24. Due to the assumption that E2, G12, Ef/Gm = 12.0 (boron/aluminum) 1.0 Ef/Gm = 57.3 (SMC) Ef/Gm = 216.2 (graphite/epoxy) Ef/Gm = 324.3 (boron/epoxy) 0.5 ∗Max. 0 30° 60° τ point changes with Ef/Gm 90° α 50 Ef/Gm = 324.3 (boron/epoxy) 40 σf σ Ef/Gm = 216.2 (graphite/epoxy) max 30 Ef/Gm = 57.3 (SMC) 20 νf = 0.24 R = 0.05 rf = 0.01. l f = 1.04 l – lf Note: R = lf as shown in Figure 6.18 Ef/Gm = 12.0 (boron/aluminum) 10 0 30° 60° 90° α FIGURE 6.22 Variation of maximum interfacial shear stress and maximum iber stress with off-axis angle from the Chon–Sun model. (From Chon, C. T. and Sun, C. T. 1980. Journal of Materials Science, 15, 931–938. Reprinted with permission from Chapman & Hall.) Analysis of a Discontinuously Reinforced Lamina 253 40 Graphite epoxy specimens Continuous fiber Fiber volume fraction 0.675 Ex/Em 30 Legend Force-balance approach Mean experimental values Experimental scatter 20 10 0 0 15 30 45 60 Fiber direction (θ degrees) 75 90 FIGURE 6.23 Comparison of predicted and measured off-axis modulus ratio, Ex/Em, for graphite/epoxy. (From Suarez, S. A. et al. 1986. Experimental Mechanics, 26(2), 175–184. With permission.) and ν12 are independent of the iber aspect ratio, L/d has little effect on the calculated Ex for iber orientations other than those near θ = 0°. As shown in the previous section, the iber length required to attain the maximum composite stiffness at θ = 0° is quite small. Thus, the relatively low stiffness of practical short-iber composites is more likely to be caused by the off-axis orientation of the ibers than by the short length of the ibers. Another important factor eg (d r be Fi 40 e) re 90 n io ct e ir 45 d Ex/Em 30 20 10 0 1E+001 1E+002 1E+003 1E+004 Fiber aspect ratio (L/d ) 1E+005 FIGURE 6.24 Tridimensional plot of Ex/Em as a function of iber aspect ratio and iber orientation for graphite/ epoxy. (From Suarez, S. A. et al. 1986. Experimental Mechanics, 26(2), 175–184. With permission.) Principles of Composite Material Mechanics 254 that should not be overlooked is the iber volume fraction. In most short-iber composites, the maximum iber volume fraction is quite low due to processing limitations. That is, the viscosity of the iber/resin mixture must be kept below a certain limit for proper low during the molding process. All these conclusions have important implications for the behavior of randomly oriented short-iber composites, which are discussed in Section 6.4. EXAMPLE 6.1 The interfacial shear stresses, τ, and the iber normal stresses, σf, acting on a differential element at a distance x from the end of the iber are shown in Figure 6.4, where the iber is assumed to be round having a circular cross section of diameter d. For a iber that has a rectangular cross section of width, a, and depth, b, ind the differential equation governing the variation of the stresses τ and σf along the length of the iber. Solution For static equilibrium of forces along the rectangular iber in the x-direction, ∑ F = (σ + dσ )ab − σ ab − τ [2(a + b)] dx = 0. f x f f Rearranging and simplifying, the differential equation governing the variation of stresses τ and σf along the length of the iber is dσf/ dx = 2τ(a + b)/ab. EXAMPLE 6.2 Equation 6.5 gives the variation of the iber normal stress, σf, with the distance along the iber, x, for the Kelly–Tyson model whose matrix shear stress–shear strain diagram is illustrated in Figure 6.5a. Find the corresponding equation for variation of the iber normal stress, σf, for the Cox model whose matrix shear stress–shear strain diagram is illustrated in Figure 6.5b, and for which the shear strain varies linearly with the distance x. Solution For the Cox model whose matrix shear stress–shear strain diagram is illustrated in Figure 6.5b, the matrix shear stress–shear strain relationship is given by τ = Gm γ , where Gm is the matrix shear modulus. In addition, the matrix shear strain varies linearly with x, so γ = kx, where k is a constant. Equation 6.4 now becomes x σf = x 4 4 4G Gm γdx = m τdx = d d d ∫ 0 ∫ 0 x ∫ 0 kxdx = 2Gm kx 2 d Analysis of a Discontinuously Reinforced Lamina 255 EXAMPLE 6.3 If the distribution of the interfacial shear stress, τ, along the discontinuous iber in Figure 6.4 is described by the linear function shown in Figure 6.8a, ind the corresponding expression for the iber tensile normal stress, σf, and sketch its distribution. Solution The equation for the linear variation of the interfacial shear stress in Figure 6.8a is 2 τ = τ max 1 − x L Substituting this equation into Equation 6.4, the iber tensile normal stress distribution is found to be x σf = x 4 4 2 4τ τ dx = τ max 1 − x dx = max d d L d ∫ ∫ 0 0 x2 x − L This distribution is shown graphically in Figure 6.8b. The maximum value of this stress occurs at x = L/2. EXAMPLE 6.4 An aligned short-iber carbon–epoxy composite is to be fabricated so that it behaves as a continuous iber composite with a composite modulus of E1 = 80 GPa. The 0.01-mm-diameter ibers have a modulus of elasticity (+ ) = 2.5 GPa. The epoxy matrix can Ef1 = 240 GPa and a tensile strength sf1 be assumed to be a rigid plastic material with a yield strength of 20 MPa in shear. Determine (a) the iber length necessary to just reach the “continuous iber stress” at the midpoint for a composite stress of 50 MPa and (b) the iber length and the composite stress necessary to develop the ultimate tensile strength in the iber. Solution a. The “continuous iber stress” is σ f max = Ef 1σ c1 240(50) = = 150 MPa 80 E1 and the corresponding iber length from Equation 6.6 is L= dσ f max 0.01(150) = = 0.0375 mm 2τ y 2(20) Principles of Composite Material Mechanics 256 (+ ) is found b. The iber length corresponding to a iber stress sf1 from Equation 6.9: Lc = ds(f1+ ) 0.01(2500) = = 0.625 mm 2(20) 2τ y and the corresponding composite stress is σ c1 = E1s(f1+ ) 80(2.5) = = 0.833 GPa = 833 MPa 240 Ef 1 EXAMPLE 6.5 For the differential element in Figure 6.4 and the stress distributions given in Example 6.3, ind the corresponding equation for the longitudinal composite modulus Ec1. Assume that the iber and matrix materials are linear elastic and that the iber length L is less than the ineffective length Li. Solution This derivation follows that of Equation 6.24, with different stress distributions along the iber. In this case, the average iber stress is given by σ f1 = ∫ L/ 2 σ f 1 dx 0 L/2 = ∫ L/ 2 0 4τ max x2 x − dx L d 2τ L = max 3d L/2 The rule of mixtures for longitudinal composite stress is σ c 1 = σ f 1υ f + σ m υ m = 2τ max L υf + σ m υm 3d Assuming that the applied composite stress produces equal strains, e, in the composite, iber and matrix, dividing both sides of the above equation by e, and applying Hooke’s law for composite and matrix materials, we get Ec1 = 2τ max L υf + Em υm 3de So for this model, the longitudinal composite modulus Ec1 increases linearly with increasing iber length L, starting at Em vm when L = 0. EXAMPLE 6.6 The RVE for an aligned discontinuous iber composite is shown in Figure 6.16. Assume that the composite part of the RVE has length L and longitudinal coeficient of thermal expansion (CTE) αc, whereas the matrix Analysis of a Discontinuously Reinforced Lamina material has total length e and longitudinal CTE αm. Develop a micromechanical equation for predicting the effective longitudinal thermal expansion coeficient, αeff, for the RVE, which has a total length L + e. Solution The overall thermal deformation of the RVE along the iber direction due to a temperature change ΔT is given by δ total = α eff (L + e)∆T But for the series arrangement of the composite and matrix, geometric compatibility requires the total thermal expansion to be δ total = δ c + δ m = α c L∆T + α m e∆T where δc = thermal deformation of the composite part δm = thermal deformation of the matrix part Equating the above two expressions for the total thermal deformation and solving for αeff, it is seen that the effective thermal expansion coeficient for the RVE is α eff = αcL + αme L+e EXAMPLE 6.7 Set up the equations for predicting the off-axis tensile strength of an aligned discontinuous iber composite based on the maximum strain criterion. Solution Refer to the solution for Example 4.4, which is for an off-axis continuous iber composite. Based on the maximum strain criterion, the off-axis tensile strength is given by σx = SL(+)/(cos2 θ − ν12 sin2 θ) for longitudinal tensile failure when 0 ≤ θ ≤ θ1 σx = SLT/(sin θ cos θ) for in-plane shear failure when θ1 ≤ θ ≤ θ2 σx = ST(+)/(sin2 θ − ν21 cos2 θ) for transverse tensile failure when θ2 ≤ θ ≤ π/2 where θ1 is the solution of SL( + ) SLT = cos θ1 − ν12sin 2 θ1 sin θ1cos θ1 2 257 Principles of Composite Material Mechanics 258 and θ2 is the solution of SLT ST( ) = sin θ 2cos θ 2 sin 2 θ 2 − ν21cos 2 θ 2 + For the discontinuous aligned iber composite, sL(+ ) is found by using either Equation 6.14 or 6.15, depending on whether the iber length is less than or greater than the critical length. The other strengths SLT and sT(+ ) are assumed to be independent of iber length, and are calculated from the corresponding micromechanics equations for strengths of continuous iber composites in Section 4.3. PROBLEM 6.1 The interfacial shear stresses, τ, and the iber normal stresses, σf, acting on a differential element at a distance x from the end of the iber are shown in Figure 6.4, where the iber is assumed to have a circular cross section of diameter d. In some cases, ibers may have cross sections that are more elliptical than circular (see Figure 3.2). For a iber that has an elliptical cross section of major diameter, a, and minor diameter, b, ind the differential equation governing the variation of the stresses τ and σf along the length of the iber. PROBLEM 6.2 A short-iber composite is to be modeled using the RVE in Figure 6.2b. Assuming that the matrix is rigid plastic in shear but that both the iber and matrix are elastic in extension, develop an equation for the longitudinal modulus of the RVE. What values of the longitudinal modulus does the model give as the iber length becomes—very large or very small? PROBLEM 6.3 Using the result from Problem 6.2, develop an expression for the longitudinal modulus of the RVE shown in Figure 6.2a that includes the effect of the matrix material at the iber ends. PROBLEM 6.4 A carbon/epoxy single iber test specimen is subjected to a uniaxial tensile stress that is increased until the iber breaks up into pieces having a length of 0.625 mm. If the iber has a diameter of 0.01 mm, a longitudinal modulus of 240 GPa, and an ultimate tensile strength of 2.5 GPa, what is the interfacial shear strength of the specimen? If the composite longitudinal modulus is 80 GPa, what applied composite stress is required to produce the condition above? Analysis of a Discontinuously Reinforced Lamina 259 PROBLEM 6.5 A linear elastic iber of rectangular cross section is embedded in a linear elastic matrix material, and the composite is subjected to a uniaxial stress as shown in Figure 6.25a. The interfacial shear stress distribution along the iber is to be approximated by a linear function, as shown in Figure 6.25b. Determine the iber length, L, that is required to develop the ultimate tensile stress, s(f1+ ) , at the midpoint of the iber. Neglect the stress transmitted across the ends of the iber. PROBLEM 6.6 The RVE for an aligned discontinuous iber composite without matrix material at its ends is shown in Figure 6.4. Assume that when the RVE is loaded along the iber direction, the interfacial shear stress distribution is given by τ= 2τ max L − x L 2 and the iber tensile stress is given by σf = 4σ fmax x(L − x) L2 where L = iber length, x = distance from the left end of RVE, τmax = maximum interfacial shear stress, and σfmax = maximum iber tensile normal stress. (a) Matrix b Fiber a L (b) τmax τ x L 2 L FIGURE 6.25 (a) Fiber with rectangular cross section embedded in matrix. (b) Interfacial shear stress distribution along the iber shown in (a). Principles of Composite Material Mechanics 260 a. Sketch the distributions of τ and σf along the length of the iber. b. Neglecting the stress transmitted across the ends of the iber, derive the relationship between τmax and σfmax. c. If the interfacial shear strength is about the same as the iber tensile strength, and the iber aspect ratio L/d is very large (say L/d > 1000), will the most likely mode of failure be interfacial shear failure or iber tensile failure? PROBLEM 6.7 For the RVE in Figure 6.4, assume that the iber length is greater than the ineffective length, and that the distribution of the iber tensile normal stress is given by σf = 4σ fmax x(Li − x) L2i σ f = σ fmax for for 0 ≤ x ≤ Li 2 Li L ≤x≤ 2 2 a. Determine the expression for the iber/matrix interfacial stress, τ, and plot its distribution along the iber length. b. Determine the magnitude and location of the maximum interfacial shear stress, τmax, and show it on the shear stress distribution from part (a). 6.4 Randomly Oriented Discontinuous Fibers If the iber orientation in a composite is truly random in a three-dimensional (3D) sense, the composite exhibits 3D isotropy. Such a situation is likely to exist when the iber length, L, is much less than the thickness of the part, t, as shown in Figure 6.26a. Composites with low aspect ratio reinforcement such as whiskers, microibers, and nanotubes generally fall into this category. However, in many short-iber composite parts (e.g., panels made from sheetmolding compounds or resin transfer moldings), the iber length is much greater than the thickness of the part, as shown in Figure 6.26b. In this case, iber orientation in the thickness direction is not possible, and the material exhibits two-dimensional (2D) isotropy or planar isotropy. The analysis of both types of materials will be discussed here, but the emphasis will be on the 2D case. Analysis of a Discontinuously Reinforced Lamina (a) 261 (b) L <t L >t t t FIGURE 6.26 3D and 2D random orientations of ibers. (a) Fiber length is less than thickness of part, so ibers are randomly oriented in three dimensions. (b) Fiber length is greater than thickness of part, so ibers are randomly oriented in only two dimensions. 6.4.1 Stress and Strength Analysis The use of geometric averaging techniques for analyzing randomly oriented iber composites has been introduced in Example 2.7, and models for predicting strength and modulus of such composites are typically based on averaging. For example, Baxter [20] developed a model for predicting the strength of randomly oriented iber-reinforced metal matrix composites by averaging the Tsai–Hill equation for off-axis strength (Equation 6.31) as σɶ x = ∫ π σ xdθ 0 π = ∫ π /2 σ xdθ 0 (6.33) π/2 Numerical integration was employed, since the integral could not be evaluated in closed form. The model was used to establish upper and lower limits of composite strength. The composite longitudinal strength was estimated from Equation 6.14 or 6.15, and the other strengths in Equation 6.31 were estimated according to the most likely failure modes. Lees [21] assumed that the angular dependence of the failure stress, σx, for such a material under uniaxial off-axis loading could be described by using the maximum stress criterion. Lees also assumed that there are three failure mechanisms according to the maximum stress criterion, each operating over a range of angles as follows (recall Equation 4.3 for uniaxial off-axis loading): for 0 ≤ θ ≤ θ1 , σ x = sL( + ) cos 2 θ for θ1 ≤ θ ≤ θ 2 , σ x = for θ 2 ≤ θ ≤ (longitudinal tensile failure) sLT sin θ cos θ s( + ) π , σx = T2 2 sin θ (interfacial shear failure) (transverse tensile failure) Principles of Composite Material Mechanics 262 where cot θ1 = sL( + ) sLT and tan θ 2 = sT( + ) sLT With regard to the randomly oriented iber composite, Lees assumed that the average strength over all angles is given by θ2 π /2 θ1 sLT sT( + ) 2 sL( + ) + + d d d θ σɶ x = θ θ 2 2 sin θ sin θ cos θ π cos θ 0 θ θ 1 2 ∫ ∫ ∫ (6.34) After integrating and using Equation 4.24 for sL(+ ) for continuous ibers, and then making some simplifying approximations, Lees found that σɶ x ≃ 2sLT π sT( + ) sT( + )smf1 1 + + ln s 2 sLT mf1 (6.35) where smf1 is the matrix stress corresponding to the iber failure strain. The same approach was later taken by Chen [22], who included a strength eficiency factor, ψ, to account for discontinuous ibers and obtained the equation σɶ x = 2sLT π ψsL( + )sT( + ) 2 + ln 2 sLT (6.36) Lees and Chen both reported reasonable agreement of their predictions with experimental data. Although Lees [21] and Chen [22] did not propose the use of equations like Equations 6.14 and 6.15 to estimate the effects of iber length on sL(+ ) in the above equations, it seems consistent with the approach of Baxter [20] and others. Another approach suggested by Halpin and Kardos [23] is based on the assumption that the strength of a randomly oriented iber composite is the same as the strength of a quasi-isotropic laminate of the same material. Quasi-isotropic laminates, which are laminates of certain stacking sequences that behave in a planar isotropic manner, will be discussed in Chapter 7 on laminates. Halpin and Kardos [23] reported that the quasi-isotropic laminate model with the maximum strain criterion for lamina failure gave good agreement with experimental data for a glass–epoxy composite. 6.4.2 Modulus Analysis One major conclusion from Section 6.3.2 was that iber orientation is more important than iber length in the determination of off-axis elastic constants Analysis of a Discontinuously Reinforced Lamina 263 of unidirectional composites. Further support for this conclusion is provided by the observation that continuous iber models give reasonably accurate predictions of elastic properties of randomly oriented iber-reinforced composites. The concept of averaging the elastic constants over all possible orientations by integration was apparently introduced by Cox [2], who modeled paper as a planar mat of continuous ibers without matrix material. The Cox formulas for the averaged isotropic elastic constants of random arrays of ibers are given here for later reference, but they are not considered to be accurate enough for design use. For the 2D case, Eυ Eυ 1 Eɶ = f f , Gɶ = f f , νɶ = 3 8 3 (6.37) Eυ Eυ 1 Eɶ = f f , Gɶ = f f , νɶ = 6 15 4 (6.38) and for the 3D case, where Eɶ = averaged Young’s modulus for the randomly oriented iber composite Gɶ = averaged shear modulus for the randomly oriented iber composite νɶ = averaged Poisson’s ratio for the randomly oriented iber composite Nielsen and Chen [24] used the averaging concept, along with micromechanics equations and transformation equations for a unidirectional continuous iber-reinforced lamina, to analyze a planar isotropic composite. The geometrically averaged Young’s modulus, which is assumed to be the same as the in-plane Young’s modulus of the isotropic composite, is given by π Eɶ = ∫ E dθ ∫ dθ x 0 π (6.39) 0 where the off-axis Young’s modulus, Ex, is deined by the irst of Equation 2.40, and the angle θ is deined in Figure 2.12. Nielsen and Chen used a set of micromechanics equations for a unidirectional continuous iber composite to calculate E1, E2, G12, and ν12. Figure 6.27 shows that the averaged modulus for the randomly oriented iber composite is much lower than the corresponding longitudinal modulus, E1, for most practical composites. Since the analysis is based on a continuous iber model, the predicted reduction in modulus is due to iber orientation, and not to iber length. The equation Principles of Composite Material Mechanics 264 Ef/Em = 1 ~ Modulus ratio (E/El) 1.0 Ef/Em = 5 0.8 Ef/Em = 10 0.6 Ef/Em = 20 0.4 Ef/Em = 50 0.2 Ef/Em = 100 0 0 0.2 0.3 0.4 0.5 0.6 0.7 Volume fraction of fibers (υf ) 0.1 0.8 0.9 FIGURE 6.27 Dependence of modulus ratio, Eɶ/E1, on iber volume fraction for several values of Ef/Em from Nielsen–Chen model. (From Nielsen, L. E. and Chen, P. E. 1968. Journal of Materials, 3(2), 352– 358. Copyright ASTM. Reprinted with permission.) that Nielsen and Chen used for E2 was known to give values lower than measured values, and so the predictions of Equation 6.39 were also lower than the corresponding experimental values. The evaluation of Equation 6.39 requires the integration of the expression for Ex given by Equation 2.40, which is quite cumbersome. The integration is much simpler if the invariant forms of the transformed lamina stiffnesses are used. For example, the averaged value of the transformed lamina stiffness Q11 is given by Qɶ 11 = ∫ π Q11 dθ 0 ∫ π π = ∫ [U + U cos θ + U cos 4θ] dθ = U 1 2 3 0 π dθ 1 (6.40) 0 Similarly, (U − U 4 ) , Qɶ 16 = Qɶ 26 = 0 Qɶ 22 = U1 , Qɶ 12 = Qɶ 21 = U 4 , Qɶ 66 = 1 2 and the stress–strain relations for any set of axes x,y in the plane are σ x U1 σ y = U 4 τ 0 xy U4 U1 0 εx 0 0 εy (U1 − U 4 )/2 γ xy (6.41) Analysis of a Discontinuously Reinforced Lamina 265 Since this is an isotropic material, we can write Qɶ 11 = U1 = Eɶ = Qɶ 22 1 − νɶ 2 νɶ Eɶ Qɶ 12 = U 4 = 1 − νɶ 2 Qɶ 66 = Gɶ = (6.42) Eɶ U − U4 = 1 2 2(1 + νɶ ) Tsai and Pagano [25] and Halpin and Pagano [26] have obtained the same results by using invariant concepts along with quasi-isotropic laminate theory, which will be discussed in Chapter 7. Solving these equations for the isotropic engineering constants, we get (U − U 4 )(U1 + U 4 ) Eɶ = 1 U1 U − U4 Gɶ = 1 2 νɶ = (6.43) U4 U1 Using the equations relating the invariants in Equation 6.43 to the engineering constants E1, E2, G12, and ν12 for the orthotropic lamina (recall Equations 2.45 and 2.27), Tsai and Pagano [25] also developed the following approximate expressions: 3 5 1 1 Eɶ = E1 + E2 , Gɶ = E1 + E2 8 8 8 4 (6.44) These equations, along with the Halpin–Tsai equations for E1 and E2, were used to estimate the elastic moduli of randomly oriented boron iberreinforced epoxy, and the results compare favorably with experimental results (Figure 6.28). Manera [27] also got good agreement with experimental results by using Equation 6.43 with a different set of micromechanics equations for E1, E2, G12, and ν12. Christensen and Waals [28] also used the averaging approach to ind the isotropic elastic constants for continuous iber composites with 2D and 3D random iber orientation. This appears to be the irst published report of the analysis of a composite with 3D oriented ibers, although Cox [2] derived Equation 6.38 with regard to the case of ibers without matrix material. Only the 3D analysis of Christensen and Waals is summarized here, since the 2D analysis is quite similar to those that have already been discussed. Principles of Composite Material Mechanics 266 10.0 ~ E (106 psi) 8.0 υ f = 0.40 6.0 4.0 Random short-length boron filament reinforcement 2.0 D = 0.004 in. 0 0 0.25 (32) 0.75 0.50 1.0 (125) (250) Length, in. (Aspect ratio, L/d) FIGURE 6.28 Dependence of Young’s modulus of randomly oriented short-iber boron/epoxy composite on iber aspect ratio. Comparison of predictions from Halpin–Tsai equations and invariant expressions with experimental data. (Reprinted from Halpin, J. C. and Pagano, N. J. 1969. Journal of Composite Materials, 3, 720–724. With permission from Technomic Publishing Co.) For the 3D Christensen–Waals analysis, the spherical coordinate system shown in Figure 6.29 is used. An orthotropic, transversely isotropic composite with ibers oriented along the 1 direction is subjected to an arbitrary normal strain such as ε′33 along the 3′ direction. For the purpose of the analysis, the 3 axis is taken to be in the 1′2′ plane. The basic premise of the solution is that the resulting ratio of stress to strain σ ′ij /ε′33 (i, j = 1, 2, 3) for a random orientation of ibers can be found by calculating the average value of σ ′ij /ε′33 over all possible orientations of the iber direction (1 axis) relative to the ixed xi′ axes. Using the 3D stress–strain relationships for a generally orthotropic, transversely isotropic material (i.e., the stiffness matrix of Equation 2.17 transformed to an arbitrary 1′2′3′ off-axis coordinate system), it can be shown that σ ′33 4 4 = C11λ 31 + (2C12 + 4C66 )λ 231λ 232 + C22λ 32 ε′33 (6.45) and that σ ′22 2 2 2 = C11λ 31 λ 21 + C12 (λ 32 λ 221 + λ 231λ 222 + λ 231λ 223 ) ε′33 + C22λ 232λ 222 + 4C66λ 31λ 32λ 21λ 22 + C23λ 232λ 223 (6.46) Analysis of a Discontinuously Reinforced Lamina 267 3′ 1 2 θ 2′ ϕ 1′ 2′ 3′ fixed coordinate system 1 2 3 rotated coordinate system Axis 1 fiber direction Axis 3 lines in the 1′ 2′ plane 3 1′ FIGURE 6.29 Spherical coordinates for 3D Christensen–Waals analysis. (Reprinted from Christensen, R. M. and Waals, F. M. 1972. Journal of Composite Materials, 6, 518–532. With permission from Technomic Publishing Co.) where the direction cosines λij are given by sin θ cos φ λ ij = sin θ sin φ cos θ − cos θ cos φ − cos θ sin φ sin θ sin φ − cos φ 0 (6.47) Averaging over all possible orientations of the iber direction, we have σ ′ij |Random = ε′33 π π 0 0 ∫ ∫ (σ′ /ε′ )sin θdθ dφ ∫ ∫ sin θdθ dφ 33 ij π π 0 0 (6.48) After substituting Equation 6.45 into Equation 6.48, we get σ ′33 1 |Random = (3C11 + 4C12 + 8C22 + 8C23 ) ε′33 15 (6.49) For an equivalent homogeneous isotropic material, the corresponding ratio of stress to strain is ɶ 1 − νɶ ) σ ′33 E( = ε′33 (1 + νɶ )(1 − 2 νɶ ) (6.50) Principles of Composite Material Mechanics 268 Similarly, after substituting Equation 6.46 into Equation 6.48, we get σ ′22 1 |Random = (C11 + 8C12 + C22 − 4C66 + 5C23 ) ε′33 15 (6.51) and the corresponding ratio of stress to strain for an equivalent homogeneous isotropic material is σ ′22 νɶ Eɶ = ε′33 (1 + νɶ )(1 − 2 νɶ ) (6.52) Equating the ratio in Equation 6.49 to that in Equation 6.50, then equating the ratio in Equation 6.51 to that in Equation 6.52, and solving the two resulting equations simultaneously for the effective isotropic engineering constants, Christensen and Waals found that ( ) ( ) 2 2 E1 + 4 ν12 − 4 ν12 + 1 K 23 + 6(G12 + G23 ) + 8 ν12 + 4 K 23 E1 + 4 ν12 ɶ E= 2 3 2E1 + 8 ν12 + 12 ν12 + 7 K 23 + 2(G12 + G23 ) ( ) (6.53) and υɶ = 2 E1 + ( 4 ν12 + 16 ν12 + 6)K 23 − 4(G12 + G23 ) 2 4E1 + (16 ν12 + 24 ν12 + 14)K 23 + 4(G12 + G23 ) (6.54) where K 23 is the plane strain bulk modulus for dilatation in the 2–3 plane with ε11 = 0, and the other properties are deined in Chapter 2. Christensen and Waals used the previously developed micromechanics equations by Hashin [29,30] and Hill [31] to calculate the ive independent engineering constants E1, ν12, G12, G23, and K 23, which appear in Equations 6.53 and 6.54. Predictions from Equation 6.53 for a glass–epoxy composite are shown in Figure 6.30, along with the rule of mixtures prediction from Equation 3.23 and the Cox prediction from Equation 6.38. The prediction from the Cox model is well below that of the Christensen–Waals model, and the rule of mixtures prediction is much too high. Using the same averaging technique, Christensen and Waals also developed a set of equations analogous to Equations 6.53 and 6.54 for the 2D case. The results are [23] ( 1 2 Eɶ = u1 − u22 u1 ) (6.55) and νɶ = u2 u1 (6.56) Analysis of a Discontinuously Reinforced Lamina Ef = 26.25 Em 25 υf = 0.20 υm = 0.35 20 ~ Modulus ratio (E /Em) 269 15 Rule of mixtures Equation 3.27 10 Equation 6.53 5 Cox approximation Equation 6.38 0 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0 Fiber volume fraction (υf) FIGURE 6.30 Comparison of Christensen–Waals 3D analysis for Young’s modulus of randomly oriented iber composite with rule of mixtures and Cox approximation for a glass/epoxy composite. (From Christensen, R. M. and Waals, F. M. 1972. Journal of Composite Materials, 6, 518–532. Reprinted with permission from Technomic Publishing Co.) where u1 = 2 3 G (3 + 2 ν12 + 3 ν12 )G23 K 23 E1 + 12 + 8 2 2(G23 + K 23 ) 2 (1 + 6 ν12 + ν12 )G23 K 23 1 G u2 = E1 − 12 + 2(G23 + K 23 ) 8 2 (6.57) The results from Equations 6.55 through 6.57 for a glass–polystyrene composite are shown in Figure 6.31. The Christensen–Waals model is seen to give much better agreement with the measurements than either the Cox model or the rule of mixtures, although none of the models takes into account the iber length. Chang and Weng [32] also obtained good agreement with experimental results for glass/polyester sheet-molding compounds by using Equations 6.55 through 6.57. Christensen later presented simpliied versions of these equations based on an asymptotic expansion [33,34]. Weng and Sun [35] used the Christensen–Waals equations along with micromechanics equations, which were modiied to account for the effect of iber length. The effect of iber length was modeled by using a so-called “ictitious iber,” which included the effect of matrix material at the ends of Principles of Composite Material Mechanics 270 = Experimental data Glass fibers in polystyrene Ef = 10.5 × 106 psi υf = 0.20 Em = 10.47 × 106 psi υm = 0.32 1.5 Rule of mixtures Equation 6.55 ~ E (106 psi) Equation 3.27 1.0 0.5 Cox approximation Equation 6.37 0 0 0.2 0.1 Fiber volume fraction (υf) FIGURE 6.31 Comparison of Christensen–Waals 2D analysis for Young′s modulus of randomly oriented iber composite with rule of mixtures and Cox approximation for a glass/polystyrene composite. (Adapted from Christensen, R. M. and Waals, F. M. 1972. Journal of Composite Materials, 6, 518–532.) the iber in the RVE shown in Figure 6.2a. The effects of varying stresses along the iber were not accounted for; however, as it was assumed that the stresses were equal in the iber and matrix portions of the ictitious iber. The equation for the effective modulus of the ictitious iber is analogous to Equation 6.28 for the modiied Cox model, except that the stress distribution along the iber is assumed to be uniform. Figure 6.32 shows a comparison of the predictions of the modiied Christensen–Waals theory with the original Christensen–Waals theory, the rule of mixtures, the Halpin–Tsai equations, and experimental data. For the glass/polyester sheet-molding compound material used, the effect of iber length is apparently not very great, as the predictions of modiied and original Christensen–Waals theories are almost the same. Both theories give predictions that are in good agreement with the experimental data. The effects of iber length and nonuniform stress distribution along the discontinuous iber were accounted for by Sun et al. [36], who developed equations for the elastic moduli of 2D randomly oriented, short-iber composites as part of a study of vibration damping properties. A modiied Cox model was used to determine E1, while the other lamina properties were assumed to be independent of iber length. The modiied Cox model in this case is of the form 1 − tanh (βL/2) EMC1 = Ef1 υf α + Em υm γ βL/2 (6.58) Analysis of a Discontinuously Reinforced Lamina Ru H le o a fm Ch lpin ixtu ris –T he res t en sa or se i a y nd n an an d d Ch Ch W ris ris aa te te ls’ ns ns th en en eo an an ry d d W W aa aa ls ls SMC system 25 (3.63) 20 (2.90) es 10 (1.45) nd r bou lowe ’s l u Pa 5 (0.73) 0 en tt O rig in al 15 (2.18) Pr ~ E,GPa (Msi) 271 Owens/Corning test data 0 0.1 0.2 0.3 0.4 0.5 υf FIGURE 6.32 Comparison of various theories for prediction of Young’s modulus of randomly oriented chopped glass/polyester sheet molding compound. (Reprinted from Weng, G. J. and Sun, C. T. 1979. In Tsai, S. W., ed., Composite Materials: Testing and Design (Fifth Conference), ASTM STP 674. American Society for Testing and Materials, Philadelphia, PA, pp. 149–162. Copyright ASTM. With permission.) where α and γ are strain magniication factors, which are determined from an FEA. The modiied Cox model for E1, along with the rule of mixtures (Equation 3.45) for ν12 and the Halpin–Tsai equations (Equations 3.63 and 3.64) for E2 and G12, are used in transformation equations of the form described in Equation 6.32, which are then used in Equation 6.43 to determine the averaged isotropic engineering constants for the randomly oriented iber composite. A tridimensional plot of the Young’s modulus versus the iber aspect ratio, L/d, and the ratio Ef/Em is shown in Figure 6.33. It is seen that high Ef/ Em and high L/d are required in order to have a high composite modulus. As with the aligned discontinuous case, the iber aspect ratio required to attain maximum stiffness for given iber and matrix materials is quite low. 6.5 Nanofibers and Nanotubes The development of nanoibers and nanotubes has played a major role in the recent nanotechnology revolution, and the use of these materials as reinforcements in composites has received particular attention. With Principles of Composite Material Mechanics 272 12.56 ~ E/Em 9.05 5.55 109.0 79.2 2.04 1.00 49.1 167.3 L/d 333.7 Ef/Em 19.1 500.0 FIGURE 6.33 Tridimensional plot of as a function of L/d and Ef/Em for a randomly oriented short-iber composite. (Reprinted from Sun, C. T., Wu, J. K., and Gibson, R. F. 1985. Journal of Reinforced Plastics and Composites, 4, 262–272. With permission from Technomic Publishing Co.) dimensions in the nanometer range, nanoibers have solid cylindrical shapes and nanotubes have hollow tubular geometries. Although aspect ratios L/d may range up into thousands, they are both generally considered to be discontinuous in nature, and so it is particularly appropriate to discuss them in this chapter. There has been intense interest in CNTs since they were discovered in 1991 by Iijima [37], and the number of publications on CNTs and CNT-reinforced composite materials has grown very quickly since that time. Several review articles on the mechanical behavior of CNTs have appeared [38,39], and a special issue of a leading composites journal was dedicated to the modeling and characterization of nanostructured materials [40]. CNTs are available in single-wall (SWNT) or multiwalled (MWNT) conigurations, and the geometrical arrangement of carbon atoms in the nanotubes can be described as being either zigzag or armchair [38,39]. Microscopic images of carbon nanoibers (CNFs) and CNTs in various polymer matrices are shown in Figure 6.34 from Reference 41 and Figure 6.35 from Reference 42, respectively, whereas the typical geometrical and mechanical properties of nanoibers and nanotubes are listed in Table 6.1, which is partially taken from Reference 43. From Figures 6.34 and 6.35 and Table 6.1, it is clear that two key geometrical features must be accounted for in the development of micromechanical models for nanocomposites reinforced with nanoibers and/ or nanotubes. Due to their microscopic dimensions by comparison with Analysis of a Discontinuously Reinforced Lamina 273 10 μm Nanotube wt.% FIGURE 6.34 Scanning electron microscope (SEM) image of vapor-grown CNFs in a polypropylene matrix. (From Tibbetts, G. G. and McHugh, J. J. 1999. Journal of Materials Research, 14(7), 2871–2880. With permission.) 1.4 1.2 1 0.8 0.6 0 0.2 0.4 0.6 0.8 1 1.2 1.4 Length scale (μm) 300 nm 300 nm FIGURE 6.35 Transmission electron microscope image of MWNTs in a polystyrene matrix. (Reprinted with permission from Qian, D. et al. Load transfer and deformation mechanisms in carbon nanotube–polystyrene composites. Applied Physics Letters, 76(20), 2868–2870. Copyright 2000, American Institute of Physics.) Principles of Composite Material Mechanics 274 TABLE 6.1 Geometrical and Mechanical Properties of Typical CNFs and Nanotubes Material Vapor-grown CNFs SWNT a b c Diameter (nm) Length (nm) Young’s Modulus (GPa) Tensile Strength (GPa) 100–200a ~1.3b 30,000–100,000a 500–40,000b 400–600a 320–1470c 2.7–7.0a 13–52c Nanoiber geometrical and mechanical properties from Applied Sciences, Inc., Cedarville, Ohio. Nanotube geometrical properties from Helix Material Solutions, Inc., Richardson, Texas. Nanotube mechanical properties from Yu, M.-F., Files, B., Arepalli, S., and Ruoff, R. S. 2000. Physical Review Letters, 84(24), 5552–5555. With permission. typical thicknesses of composite structures, nanoibers or nanotubes will almost certainly have random orientations in all three dimensions within the composite as in Figure 6.26a, and so the resulting nanocomposite will be macroscopically isotropic. Nanoibers and nanotubes exhibit signiicant waviness, but all the previously discussed micromechanics models as in Figures 6.2, 6.16, and 6.18 have been based on the assumption of straight iber reinforcement. 6.5.1 Stress and Strength Analysis Models for predicting the strength of nanocomposites with randomly oriented nanoibers or nanotubes are not as well developed as those for predicting elastic modulus. Tibbetts and McHugh [41] presented experimental and analytical results for randomly oriented CNF-reinforced polypropylene and nylon composites. Strength predictions were based on the averaging method of Baxter [20], which was described in Section 6.4.1. Nanoibers were assumed to have lengths less than the critical length, so Equation 6.14 was used to estimate the longitudinal composite strength as input to the Tsai–Hill equation (Equation 6.31) before performing the averaging in Equation 6.33, but the effect of nanoiber waviness was not considered. The authors concluded that the experimental results for asgrown nanoibers were generally disappointing due to inadequate iniltration of the iber clumps by the matrix resin during the injection molding of the specimens, but ball milling of the nanoibers reduced the size of the clumps, resulting in signiicant improvement in the properties, as did etching of the surfaces of the nanoibers. Experimental strength data generally fell between the predictions of one-dimensional and 3D models based on Baxter’s approach, but since nanoiber waviness was not included in the models, it is dificult to draw conclusions from comparisons of predictions with measurements. Analysis of a Discontinuously Reinforced Lamina 275 6.5.2 Modulus Analysis Micromechanics models for the elastic moduli of nanocomposites, which include the effects of both 3D random orientation and waviness of the reinforcement, have been developed by Fisher et al. [44–46] and by Anumandla and Gibson [47,48]. The approach of Fisher et al. [44–46] is based on 3D inite element models, whereas the model of Anumandla and Gibson [47,48] is an approximate closed-form solution. Only the latter approach is summarized in the following. The Anumandla–Gibson approach [47,48] consists of a combination of the waviness models of Chan and Wang [49] and Hsiao and Daniel [50] for locally orthotropic materials, the Chamis micromechanics equations ([14] of Chapter 3) for predicting the elastic constants of the locally orthotropic material, and the Christensen–Waals model [28], which accounts for the 3D random orientation of the ibers (or in this case, nanotubes). The wavy iberreinforced composite is divided into segments along its length, each of which is locally orthotropic but with off-axis orientation. The strains are averaged over one wavelength along the loading direction for uniaxial loading, and the effective Young’s modulus is determined from the ratio of applied stress to resulting average strains. The RVEs are shown in Figure 6.36, where the waviness and orientation of the nanotube are accounted for in RVE1, and the overall length of RVE2 includes the matrix material between ibers. The nanotube waviness is characterized by the waviness factor w= z (6.59) 1 z 2 A LNT θ x RVE1 y, 3 Nanotube (wavy) Matrix A Matrix x Matrix LNT RVE1 Lm/2 LNT Lm/2 RVE2 FIGURE 6.36 RVEs for Anumandla–Gibson model. (From Anumandla, V. and Gibson, R. F. 2006. Composites Part A: Applied Science and Manufacturing 37(12), 2178–2185. With permission.) Principles of Composite Material Mechanics 276 where A is the amplitude of the waviness, LNT is the nanotube length, and coordinates x and z, describing the waviness, are deined in Figure 6.36 and Equation 6.60: 2πx z = Asin LNT (6.60) The effective Young’s modulus, Ex, of RVE1, with uniform waviness of the embedded nanotube, is assumed to be the same as that of an element in a locally orthotropic lamina containing wavy ibers as described by Hsiao and Daniel [50]. Following this approach, the transformed compliances of an offaxis orthotropic lamina are averaged over one wavelength of iber waviness, and the deinition of an effective Young’s modulus is used to ind [50] Ex = σx 1 = = ERVE1 εx S11I1 + (2S12 + S66 )I 3 + S22I 5 (6.61) where σx is the applied uniaxial stress, εx is the resulting average strain, S11, S12, S22, and S66 are the locally orthotropic compliances referred to the principal material coordinates, and I1, I3, and I5 are functions that depend only on the waviness factor. The locally orthotropic compliances are estimated from micromechanics using the Chamis equations ([14] of Chapter 3). The effective elastic modulus Eɶ (= E3D − RVE1 ) for the 3D random orientation of the nanotubes is assumed to be the same as the modulus for a iber-reinforced composite containing ibers that are randomly oriented in all three dimensions as given by Christensen and Waals [28]. For the purpose of the present discussion, the Christensen–Waals analysis described in Section 6.4 is modiied by replacing the (1,2,3), and (1′,2′,3′) coordinate systems in Figure 6.29 by the (x, y, z) and (x′, y′, z′) coordinate systems, respectively. Then, according to the modiied Christensen–Waals analysis, an orthotropic, transversely isotropic composite with nanotube waviness along the x-direction is subjected to an arbitrary normal strain such as ε′zz along the z′-direction (the z-axis is taken to be in the x′y′-plane for the purpose of the analysis). The resulting ratio of stress to strain, σ ′ij /ε′zz (i, j = x, y, z), for random orientation of ibers is found by calculating the average value of σ ′ij /ε′zz over all possible orientations of the nanotube waviness direction (x-axis) relative to the ixed xi′ -axis. Equation 6.62 indicates the averaging over all possible orientations of the wavy nanotube σ ′ij |Random = ε′zz π π σ ′ij 0 0 zz ∫ ∫ ε′ sin θdθ dφ = 1 σ′ sin θdθ dφ 2π ∫ ∫ ε ′ ∫ ∫ sin θ dθ dφ π π π π ij 0 0 0 0 zz (6.62) Analysis of a Discontinuously Reinforced Lamina 277 where the angles θ and a are deined in Figure 6.29. The equations resulting from Equation 6.62 on substituting the 3D stress–strain relationships for a generally orthotropic transversely isotropic material and solving simultaneously with the stress–strain relations for an equivalent homogeneous isotropic material yield the effective composite elastic modulus Eɶ (= E3D-RVE1 ) for the 3D random orientation of the nanotube as Ex + (4 ν2xz + 8 νxz + 4) K zy Ex + (4 ν2xz − 4 νxz + 1) K zy + 6(Gxz + Gzy ) Eɶ = 3 2Ex + (8 ν2xz +12 νxz + 7 ) K zy + 2(Gxz + Gzy ) = E3D-RVE1 (6.63) where Ex(=ERVE1) is the effective elastic modulus of RVE1 according to Equation 6.61, K zy is the plane bulk modulus for dilatation in the y–z-plane with εxx = 0, and all other properties in Equation 6.63 are for RVE1 in accordance with those deined in Reference 50. Note that Equation 6.63 is the same as Equation 6.53, except for the substitution of coordinates described above. An expression for the effective elastic modulus of RVE2 with 3D random orientation of nanotubes, E3D-RVE2, is approximated by means of another inverse rule of mixtures for the series arrangement in RVE2 (Figure 6.36) as 1 1 LNT 1 Lm + = E3D-RVE2 E3D-RVE1 Lm + LNT Em Lm + LNT (6.64) where E3D-RVE1 is the effective elastic modulus of RVE1 for 3D random orientation of the nanotubes according to Equation 6.63. Figure 6.37 shows a comparison of the predictions of E3D-RVE2 from Equation 6.64 with experimental results on MWNT/polystyrene composites published by Andrews et al. [51]. In the predictions, the modulus of the polystyrene matrix was assumed to be 1.9 GPa, the local modulus of the nanotube was assumed to be 1 TPa, and the nanotube volume fraction in RVE2 was varied by assuming LNT/Lm ratios of 0, 1, 2, 3, 4, and 5. It is seen that if waviness is neglected (i.e., w = 0), Equation 6.64 signiicantly overpredicts the experimental data, but as waviness increases, the predicted modulus is reduced accordingly. For waviness factors lying within the range of 0.075–0.25, the predictions are in best agreement with the published experimental results. These values of waviness seem quite reasonable in view of microscopic images such as the one in Figure 6.34. Nanoibers and nanotubes can be used not only as the principal reinforcement in composites, but also as a third phase in composites consisting of conventional iber reinforcement. Such a nanocomposite matrix material can improve the matrix-dominated properties of a conventional continuous iber composite such as compressive strength. A nanocomposite matrix material typically has a higher modulus than the plain polymer matrix, Principles of Composite Material Mechanics 278 12 E3D-RVE2 (in GPa) 10 w=0 8 w = 0.05 w = 0.1 6 w = 0.25 w = 0.5 4 Exp 2 0 0 0.05 0.1 0.15 0.2 0.25 True volume fraction of nanotube in RVE2 FIGURE 6.37 Comparison of experimental modulus data for MWNT/polystyrene composite. (Reprinted from Micromolecular Materials Engineering, 287(6), Andrews, R. et al., Fabrication of carbon multiwall nanotube/polymer composites by shear mixing, 395–403, Copyright 2006. With micromechanics predictions from Equation 6.64; Reprinted from Composites Part A: Applied Science and Manufacturing, 37(12), Anumandla, V. and Gibson, R. F., A comprehensive closed form micromechanics model for estimating the elastic modulus of nanotube-reinforced composites, 2178–2185, Copyright 2006, with permission from Elsevier.) thus increasing the lateral support for the continuous ibers, increasing the buckling load, and improving the compressive strength of the conventional composite. For example, Vlasveld et al. [52] developed hybrid composites consisting of conventional glass or carbon ibers (CFs) in a nanocomposite matrix (Figure 6.38), where the nanocomposite matrix was made of polyamide 6 polymer reinforced with synthetic mica-layered silica nanoparticles. FIGURE 6.38 Nanoparticle reinforcement of the matrix in a conventional continuous iber composite. (Reprinted from Polymer, 46, Vlasveld, D. P. N., Bersee, H. E. N., and Picken, S. J., Nanocomposite matrix for increased ibre composite strength, 10269–10278, Copyright 2005, with permission from Elsevier.) Analysis of a Discontinuously Reinforced Lamina (a) 279 (b) 1 μm 1 μm FIGURE 6.39 SEM micrographs of CFs (a) before and (b) after CNT growth on the iber surface. (Reprinted with permission from Thostenson, E. T. et al. Carbon nanotube/carbon iber hybrid multiscale composite. Journal of Applied Physics, 91(9), 6034–6037. Copyright 2002, American Institute of Physics.) The nanocomposite matrix led to signiicant increases in lexural strength, which was dominated by iber microbuckling on the compression side of the specimens. The effect was particularly signiicant at elevated temperatures. Thostenson et al. [53] developed a hybrid multiscale composite by growing CNTs directly on the surfaces of conventional CFs, which were then combined with a conventional epoxy matrix. Figure 6.39 shows micrographs of the CF before and after nanotube growth. 6.6 Particulates Particulate-reinforced composites (Figure 6.1d) are typically less expensive and more quickly processed than iber-reinforced composites, but due to their relatively low mechanical properties, they are used mainly in nonstructural applications. In fact, particles are often used as nonstructural illers rather than as reinforcements. However, as shown later in Section 6.7, nanometer (nm)-scale particles, or nanoparticles, are increasingly used to enhance the properties of conventional iber-reinforced composites in a new class of composites known as hybrid multiscale composites. This section mainly deals with conventional micron (µm)-scale particulate reinforcements in polymer matrix materials. Typically, as shown in Figure 6.40, when the volume fraction of conventional micron-scale particles is increased, the composite modulus increases, but both the corresponding elongation and strength of the composite decrease. In Figure 6.40, Sahu and Broutman [54] show experimental stress–strain curves from lexural tests of 30-µm-diameter spherical glass bead-reinforced epoxy composites of various bead volume fractions, where the glass beads have been treated with a coupling agent to promote interfacial adhesion. In the same paper, it was shown Principles of Composite Material Mechanics 280 20 50 Flexural stress (KSI) 16 40 30 20 10 0 12 8 4 0 0 1 2 3 4 Flexural strain (%) 5 6 FIGURE 6.40 Flexural stress–strain curves for glass bead-reinforced epoxy composites of various bead volume fractions. (Sahu, S. and Broutman, L. J., Mechanical properties of particulate composites. Polymer Engineering and Science, 1972, 12(2), 91–100. Copyright Wiley-VCH Verlag GmbH & Co. KGaA. Reproduced with permission.) that when the glass beads were treated with a commercial mold release to prevent interfacial adhesion, the composite modulus did not change much with increasing bead volume fraction, but the elongation and strength both decreased signiicantly. This section briely summarizes several analytical approaches to predicting the strength and modulus of conventional particle-reinforced composites as functions of the particle volume fraction. Particle-reinforced composites are assumed to be isotropic. Accordingly, each composite is assumed to have a single composite strength and a single composite Young’s modulus. 6.6.1 Stress and Strength Analysis As seen in Figure 6.40, the presence of particles in a polymer matrix material typically reduces the elongation and strength of the matrix material. An important contributing factor to this phenomenon is the stress and strain concentration in the matrix around the particles. So one approximate analytical approach is analogous to the model for the transverse strength of a iber-reinforced composite, as discussed in Section 4.3.2 (see Figure 4.18 and Equations 4.35 through 4.39). There are two problems with this approach, however. One problem is that the analysis in Section 4.3.2 is a 2D analysis, whereas the particulate composite contains 3D particles such as spheres. The second problem is that Equations 4.35 through 4.39 are based on linear Analysis of a Discontinuously Reinforced Lamina 281 elastic behavior, but as shown in Figure 6.40, the stress–strain behavior of particulate composites is typically nonlinear. In order to avoid these problems, several publications have presented semiempirical equations for estimating the strength of particulate composites. For example, Nicolais and Narkis [55] suggested that the yield strength of a spherical particle-reinforced composite with no adhesion between particles and matrix can be adequately predicted by Syc = Sym (1 − 1.21υp2/3 ) (6.65) where Sym is the yield strength of the matrix material and υp is the volume fraction of particles. The coeficient 1.21 and the exponent 2/3 for υp were selected so as to insure that Syc decreases with increasing υp, that Syc = Sym when υp = 0, and that Syc = 0 when υp = 0.74. The particle volume fraction υp = 0.74 corresponds to the maximum packing fraction for spherical particles of the same size in a hexagonal close-packed arrangement, in which case the particles are all in direct contact with each other [56]. Subsequently, Liang and Li [57] and Liang [58] have suggested that Equation 6.65 can be modiied to include particle/matrix interfacial adhesion by adding a term to account for the interfacial bonding angle, θ, which characterizes interfacial adhesion as in Syc = Sym (1 − 1.21 sin 2 θυ2p/3 ) (6.66) where θ = 0° corresponds to good adhesion and θ = 90° corresponds to poor bonding. The best its to experimental data for different composites were found to be θ = 70° for solid spherical glass beads in polypropylene [57] and θ = 40° for hollow glass beads in polypropylene [58]. The glass beads were surface treated with a silane coupling agent in both cases to promote adhesion. Finite element micromechanics models have been employed to predict the strength of particle-reinforced composites. For example, Sahu and Broutman [54] used a quarter domain model with an embedded spherical particle based on axisymmetric ring elements in combination with the von Mises failure criterion (recall Equation 4.40) to predict failure of the matrix. Due to stress concentration around the particle, the predicted failure occurred at the particle/matrix interface, but a detailed study of the effects of interface bonding on the composite strength was not conducted. More recently, Cho et al. [59] used axisymmetric inite element models (Figure 6.41) of spherical particlereinforced composites and fracture mechanics to study the effects of the interface debonding angle and particle size on composite fracture behavior. Related work has been done on the effects of particle shape [60], particle size [59,61], and particle agglomeration [61]. As previously shown in Figure 1.3, the surface area-to-volume ratio is greatest when the particle aspect ratio Principles of Composite Material Mechanics 282 (a) − σ − σ − σ Ro − σ − σ − σ (b) 2Ro − σ − σ y x FIGURE 6.41 Finite element models for spherical particle-reinforced composite. (a) Development of axisymmetric RVE and (b) inite element models of RVE with half and full axisymmetric planes. (Reprinted from Composites Science and Technology, 66, Cho, J., Joshi, M. S., and Sun, C. T., Effect of inclusion size on mechanical properties of polymeric composites with micro and nano particles, 1941–1952. Copyright 2006, with permission from Elsevier.) is either large (iber) or small (platelet), so a spherical particle is at a comparative disadvantage with regard to the interfacial area available for stress transfer per unit volume. Tensile strength improves as the particle size is reduced, and this has motivated recent studies of the strength of nanocomposites [59]. However, an important limitation on the use of nanoparticles for strengthening composites is that particle agglomeration during processing becomes more of a problem as the particle volume fraction is increased, and agglomeration tends to reduce the composite strength [61]. 6.6.2 Modulus Analysis As shown in Figure 6.40, the Young’s modulus of a particle-reinforced composite increases with increasing particle volume fraction, assuming that the particle modulus is greater than the matrix modulus. There are obvious Analysis of a Discontinuously Reinforced Lamina 283 geometric similarities between a plane passing through a particle-reinforced composite (Figure 6.1d) and a plane passing through the transverse direction in a unidirectional iber-reinforced composite (Figure 4.18a), so it is not surprising that analytical models for the Young’s modulus of a particle composite, Ec, are often similar to models for the transverse Young’s modulus of a unidirectional iber composite, E2. Recall from Section 3.2.2 that the most widely used semiempirical model for E2 is based on the Halpin–Tsai equations (Equations 3.63 and 3.64). Katz and Milewski [56] and Nielsen and Landel [61] suggested the following generalizations of the Halpin–Tsai equations for the Young’s modulus of a particulate composite: Ec 1 + ABυp = Em 1 − Bψυp (6.67) where A = kE − 1 B = (Ep /Em ) − 1 (Ep /Em ) + A 1 − υpmax ψ = 1+ 2 υp υpmax Ec is the Young’s modulus of the composite Ep is the Young’s modulus of the particle Em is the Young’s modulus of the matrix kE is the Einstein coeficient υp is the particle volume fraction υpmax is the maximum particle packing fraction It was also suggested that, with the appropriate substitutions of input properties, equations of the same form can be used to estimate the shear modulus or the bulk modulus. Recall from Chapter 3 that Paul ([29] in Chapter 3) used variational methods to derive the upper and lower bounds on the moduli of a particle composite or the transverse moduli of a iber composite. The upper bound turned out to be the rule of mixtures (Equation 3.27) and the lower bound turned out to be the inverse rule of mixtures (Equation 3.40). Richard [62] measured the Young’s moduli of glass microsphere-reinforced polyester composites having various particle volume fractions, and the results are compared here with analytical predictions from Equations 3.27, 3.40, and 6.67 in Figure 6.42. The predicted values in all three equations were based on input moduli Ep = 10.2 × 106 psi, Em = 0.25 × 106 psi [62], Einstein coeficient kE = 2.5, and maximum particle packing fraction υpmax = 0.6 for randomly loose packed spheres [56]. It is seen in Figure 6.42 that the experimental values agree closely with the predicted values from the Halpin–Tsai equations, but are well below the predicted upper bound and slightly above the predicted lower bound. The Halpin–Tsai prediction is fairly sensitive to the Principles of Composite Material Mechanics 284 Young's modulus (106 psi) 6 5 4 Experimental (62) 3 Equation 3.27 2 Equation 3.40 Equation 6.67 1 0 0 0.1 0.2 0.3 0.4 Particle volume fraction 0.5 FIGURE 6.42 Comparison of predicted and measured values of Young’s modulus for glass microspherereinforced polyester composites of various particle volume fractions. assumed value of υpmax, which in turn depends on the particle shape and packing arrangement [56,61]. It is important to note that little improvement is seen in the composite modulus for υp less than about 0.2. Recent research has shown that as the particle size is reduced to the nanometer range, unexpected improvements in the composite modulus may occur. For example, Cho et al. [59] have shown experimentally that the Young’s modulus of a particulate composite is essentially independent of particle size if the particle is of micron or larger size, but if the particle size is reduced to the nanometer range, the Young’s modulus increases with decreasing particle size. Later, Cho and Sun [63] employed molecular dynamics simulations to show that this phenomenon could be explained by the creation of a layer of dense polymer matrix material around the nanoparticle if the strength of the polymer–nanoparticle interaction is greater than or equal to that of the polymer–polymer interaction. Finite element micromechanics models such as the ones illustrated in Figure 6.41 have also been used to study the dependence of the Young’s modulus on the particle size. For example, Boutaleb et al. [64] used inite element models to show that the development of a particle/matrix interphase region around the nanoparticle may be responsible for the improved modulus of the nanocomposite. Further research on this important phenomenon is warranted. 6.7 Hybrid Multiscale Reinforcements Recent research has shown that signiicant improvements of multiple properties in conventional composites can be achieved by using new hybrid multiscale reinforcements which incorporate nanoscale reinforcements as well (a) Oﬀ-axis compressive strength (MPa) Analysis of a Discontinuously Reinforced Lamina 400 350 300 +41% Neat Nano +33% +21% 250 +35% +20% 200 +12% 150 100 50 0 5 deg 10 deg 15 deg 5 deg +32% 25 20 15 10 5 0 Neat 10 deg 15 deg Cf = 50% Transverse modulus (GPa) Transverse tensile strength (MPa) Cf = 42% (b) 285 Nano 8 7 6 5 4 3 2 1 0 41% Neat Nano FIGURE 6.43 Improvement of mechanical properties of conventional unidirectional E-glass/epoxy composites by using silica nanoparticle-enhanced epoxy matrix. (a) Off-axis compressive strength and (b) transverse tensile strength and transverse modulus. (Reprinted from Composites Science and Technology, 68(7–8), Uddin, M. F. and Sun, C. T., Improved dispersion and mechanical properties of hybrid nanocomposites, 1637–1643. Copyright 2008, with permission from Elsevier.) as conventional micron-scale iber or particle reinforcements (Figure 6.1e). For example, while iber-dominated properties (i.e., longitudinal tensile strength and elastic modulus) of conventional unidirectional polymer composites with micron size iber reinforcements are excellent, the corresponding matrix-dominated transverse tensile strength, transverse modulus, and longitudinal compressive strength properties are often poor. However, these traditionally poor properties can be signiicantly improved by (a) replacing the neat resin polymer matrix with a nanocomposite matrix (see Figure 6.38) and/or (b) growing nanoreinforcements like CNTs on the surface of the ibers (see Figure 6.39). In one example of approach (a), Uddin and Sun [65] reported that when a silica nanoparticle-enhanced epoxy was used as the matrix material in a unidirectional E-glass/epoxy composite, the off-axis compressive strength (Figure 6.43a) and the transverse tensile strength and transverse modulus (Figure 6.43b) were all simultaneously and signiicantly improved in comparison with the composites having a neat epoxy matrix. Minimization of particle agglomeration and resulting improved dispersion of silica nanoparticles in the epoxy matrix due to the use of a sol–gel 286 Principles of Composite Material Mechanics process based on the use of organosilicasol (colloidal silica in organic solvent) is believed to be the primary reason for these improvements. More recent research by the same authors extended the approach to hybrid multiscale composites containing not only the silica nanoparticles from the sol– gel process but also alumina nanoparticles and CNFs in an epoxy matrix [66]. It was shown that simultaneous improvements of at least 30% in modulus, strength, and strain at break are possible with several types of these hybrid nanocomposites. Similarly, Liu et al. [67] and Zhang et al. [68] found that the Young′s modulus, tensile strength, and fracture toughness of epoxy all simultaneously improved with the addition of sol–gel-formed nanosilica particles, and that the dispersion of the particles was excellent. Manjunatha et al. [69] observed that the addition of 10 wt.% sol–gel-formed nanosilica to the epoxy matrix resulted in simultaneous improvements of 4.4% in tensile strength, 7.4% in tensile modulus, and a factor of 2–3 in tensile fatigue life of a glass fabric-reinforced epoxy composite. The presence of the nanoparticles was believed to suppress matrix cracking and reduce delamination growth rate, thus improving the fatigue life. Since hybrid multiscale composites typically have reinforcement sizes ranging from the micron scale to the nanoscale, it is essential to understand the effects of particle size on the resulting composite properties. As previously mentioned, important observations regarding such effects were reported by Cho et al. [59], who measured modulus and strength of vinyl ester polymer matrix composites containing spherical alumina particles or glass beads, with particle sizes ranging from 0.5 mm down to 15 nm. It was found that the Young’s modulus was not affected by varying particle sizes in the micron range, but as the particle size was reduced in the nanorange, the Young’s modulus increased with decreasing particle size. The tensile strength increased with decreasing particle sizes in both micron and nanoranges as long as particle agglomeration was avoided. Cho and Sun [63] later used molecular dynamics simulation to show that if the polymer–nanoparticle interaction strength is greater than the polymer–polymer interaction strength, the polymer density near the polymer–nanoparticle interface and the Young’s modulus of the nanocomposite both increase signiicantly with reduced particle size. More research is needed about particle size effects on both structural and nonstructural properties of nanocomposites and hybrid multiscale composites. This is particularly true for analytical modeling, since most of the publications to date involve experimental work. Approach (b) which involves the growth of nanotubes on the surfaces of micron-sized ibers has also been the subject of numerous investigations. Thostenson et al. [53] grew CNTs on the surface of CFs using chemical vapor deposition (CVD), and then conducted single iber fragmentation tests of the modiied CFs in an epoxy matrix to determine the iber/matrix interfacial shear strength. It was found that the interfacial shear strength of the modiied CFs was 15% greater than that of the baseline CFs. Veedu et al. [70] also used CVD to grow aligned CNT forests perpendicular to the surface of 2D woven Analysis of a Discontinuously Reinforced Lamina 287 SiC fabric cloth consisting of micron-sized SiC ibers. The fabrics were then iniltrated with epoxy resin and stacked to form a 3D composite. Compared with the baseline composite, the 3D composite was found to exhibit simultaneous and signiicant improvements in the lexural modulus, the lexural strength, the lexural toughness, the CTE, the thermal conductivity, and the electrical conductivity. This is a true multifunctional composite combining structural and nonstructural functions. Further studies and applications of aligned CNT forests to conventional iber composites have been reported by Wardle et al. [71–75], who focused on the use of the aligned CNT forests to improve interlaminar strength and toughness. These are major concerns about conventional composite laminates because of the weak matrix resinrich regions that exist between the composite laminae. As shown in Figure 6.44, vertically aligned CNT forests can bridge and strengthen this interlaminar region [72]. The so-called “fuzzy iber” (CNTs grown on CFs) concept applied to composite laminates can provide both interlaminar and intralaminar reinforcement. As indicated earlier in Section 1.4, hybrid multiscale reinforcements have not only resulted in signiicant and simultaneous improvements in many structural properties, but also they have opened up many new possibilities for the development of multifunctional composites. Among the most important nonstructural functions made possible by hybrid multiscale reinforcements are electrical and thermal conductivity, sensing and actuation, energy harvesting/storage, self-healing capability, electromagnetic interference shielding, recyclability, and biodegradability. Recent publications related to (a) CNTs bridging the crack (b) Advanced fibers Matrix Composite plies CNTs bridging the crack FIGURE 6.44 Use of aligned CNT forests to strengthen intelaminar region in conventional iber-reinforced composite laminates. (a) Vertically aligned CNTs placed between two plies of a laminated composite and (b) close-up of the crack, showing vertically aligned CNTs bridging the crack between the two plies. (Reprinted from Composites Part A: Applied Science and Manufacturing, 39, Garcia, E. J., Wardle, B. L., and Hart, A. J., Joining prepreg composite interfaces with aligned carbon nanotubes, 1065–1070. Copyright 2008, with permission from Elsevier.) Principles of Composite Material Mechanics 288 the mechanics of multifunctional composite materials and structures have been reviewed by Gibson [76]. Finally, since nanoparticles or other nanoreinforcements play such an important role in hybrid multiscale composites, it is appropriate to mention an experimental observation that has important implications for analytical modeling of the behavior of these materials. In some cases, a so-called “interphase” region develops at the reinforcement/matrix interface (see Figure 3.27) due to either a chemical reaction between the materials or partial immobilization of the polymer matrix due to mechanical interactions with the reinforcements at the interface. The presence of this interphase region essentially enlarges the region of inluence of the reinforcement, leading to an “effective volume fraction” of reinforcement that is larger than the actual volume fraction of reinforcement. There is experimental evidence that this effect is greater for nanoreinforcements than for microreinforcements. For example, for a spherical particle and its interphase having the dimensions shown in Figure 3.27, it can be shown that the ratio of the effective particle volume fraction to the actual particle volume fraction is given by ∆R υeff = 1+ R υact 3 (6.68) where R = df/2 is the particle radius and ΔR = (di − df)/2 is the interphase thickness. Experimental evidence suggests that, as the particle radius R is reduced, the ratio ΔR/R increases, causing a corresponding increase in the ratio υeff/υact. For example, Zhang et al. [77] have reported that for nano silica/epoxy, ΔR/R was in the range 0.22–0.84, which is much larger than the corresponding range of 0.02–0.07 for similar microparticle-illed composites. This obviously has important implications for accurate prediction of nano composite properties, and the reader is encouraged to consult current journal publications for further developments. EXAMPLE 6.8 A carbon–epoxy composite with randomly oriented short ibers is made of the same constituent materials with the same iber volume fraction as the material described in Examples 3.2, 3.6, and 4.7. Assuming that the in-plane shear strength sLT = 60 MPa, and that the iber length is much greater than the thickness of the material, estimate the Young’s modulus, shear modulus, Poisson’s ratio, and tensile strength of this composite. Solution From Equation 6.44, the Young’s modulus is approximately 5 3 5 3 Eɶ = E1 + E2 = (113) + (5.65) = 45.9 GPa 8 8 8 8 Analysis of a Discontinuously Reinforced Lamina 289 and the shear modulus is approximately 1 1 1 1 Gɶ = E1 + E2 = (113) + (5.65) = 15.54 GPa 8 4 8 4 which means that Poisson’s ratio is Eɶ 45.9 νɶ = ɶ − 1 = − 1 = 0.47 2(15.54) 2G From Equation 6.35, the tensile strength is approximately 2s σɶ x = LT π 66.9 sT( + ) s( + )s 2(60) 66.9(37.95) + ln T 2 mf1 = 1 + 1 + 37.995 + ln (60)2 s s π mf1 LT = 92.2 MPa Note that the isotropic Young’s modulus for the randomly oriented composite is much greater than the transverse modulus but less than half the longitudinal modulus of the corresponding orthotropic lamina. Likewise, the isotropic strength is greater than the orthotropic transverse strength but well below the orthotropic longitudinal strength. It is also important to remember that these predictions are based on randomly oriented continuous ibers, so that the differences between the isotropic properties and the orthotropic properties are due to iber orientation, and not to iber length. EXAMPLE 6.9 Determine the Young’s modulus of a randomly oriented iber composite if the unidirectional form of the composite has an off-axis Young’s modulus that can be described by an equation of the form 2θ 1/3 Ex (θ) = E2 + (E1 − E2 ) 1 − π where θ is the iber angle in radians and E1 and E2 are the longitudinal and transverse Young’s moduli, respectively, of the unidirectional composite. Solution The Young’s modulus of the randomly oriented iber composite, averaged over all angles, is 2 Eɶ = π π /2 ∫ 0 Ex (θ) dθ = 2 π π /2 2θ ∫ E + (E − E ) 1 − π 0 2 1 2 1/3 dθ = 0.25E1 + 0.75E2 Principles of Composite Material Mechanics 290 If, say, E2 = 0.1E1 for carbon/epoxy composite, then Eɶ = 0.25E1 + 0.75(0.1E1 ) = 0.325E1 or 3.25E2 These results again relect the magnitude of the reduction in stiffness that can be expected because of iber orientation effects alone, since the iber length has not been considered in this analysis. EXAMPLE 6.10 A particle-reinforced composite has its reinforcement in a simple cubic array of spherical particles as shown in Figure 6.45. Determine (a) the relationship between the particle center-to-center spacing, s, the particle diameter, d, and the particle volume fraction, υp, (b) the maximum particle packing fraction, υpmax, and (c) the yield strength and the Young’s modulus for a composite having the maximum particle volume fraction υp = υpmax and constituent material properties Ep = 10.2 × 106 psi, Em = 0.25 × 106 psi, Sym = 5 × 103 psi, and bonding angle θ = 45°. Solution a. Following the analogous derivation for the square packing array of ibers in Section 3.1, the volume of a spherical particle is Vp = (π/6)d3. The volume of the eight corners of the spherical particles that are enclosed in the cube having sides of equal length s is then Vp = (Vp/8)8 = Vp and the particle volume fraction in the cube is υp = Vp/s3 = (π/6)(d/s)3. b. The maximum particle packing fraction is equal to υp when s = d or υpmax = π/6 = 0.5236. d s s s FIGURE 6.45 Simple cubic array of spherical particles. Analysis of a Discontinuously Reinforced Lamina 291 c. When the particle volume fraction υp = 0.5236, the yield strength is Syc = Sym(1 − 1.21 sin 2 θ υp2/3) = 5000(1 − 1.21(sin 2 45°)0.52362/3) = 3034 psi and the Young’s modulus is found from A = kE − 1 = 2.5 − 1 = 1.5, B = = ( E /E ) − 1 ( E /E ) + A p m p m (10.2/0.25) − 1 = 0.9409 (10.2/0.225) + 1.5 1 − υpmax 1 − 0.5236 ψ = 1+ υ p = 1 + 0.5236 2 0.5236 = 1.9098 2 υ pmax Ec 1 + ABυp 1 + 1.5(0.9409)(0.5236) = 29.4 = = Em 1 − Bψυp 1 − 0.9409(1.9098)(0.55236) Ec = 29.4Em = 29.4(0.25 × 10 6 ) = 7.35 × 10 6 psi PROBLEM 6.8 A short-iber composite is made from boron ibers of length 0.125 in. (3.175 mm) and diameter 0.0056 in. (0.142 mm) randomly oriented in a highmodulus epoxy matrix with a iber volume fraction of 0.4. Using the iber and matrix properties in Tables 3.1 and 3.2, respectively, estimate the modulus of elasticity for the composite. Compare the modulus for the randomly oriented short-iber composite with the longitudinal and transverse moduli of an orthotropically aligned discontinuous iber lamina of the same material. PROBLEM 6.9 Express the isotropic moduli Eɶ and Gɶ of a randomly oriented iber composite in Equation 6.43 in terms of the orthotropic lamina stiffnesses Qij. PROBLEM 6.10 Determine the isotropic moduli Eɶ and Gɶ for a composite consisting of randomly oriented T300 CFs in a 934 epoxy matrix if the ibers are long enough to be considered continuous. Use the properties in Table 2.2. Compare the values of Eɶ and Gɶ calculated from the invariant expressions (Equation 6.43) with those calculated from the approximate expressions in Equation 6.44. PROBLEM 6.11 In order to reduce material costs, a composite panel is to be made by placing ibers in the matrix material in an X-pattern of ±α as shown in Figure 6.46, instead of randomly distributing the ibers over all angles. The X-pattern composite is to be designed so that it has at least 90% of the stiffness of the randomly oriented iber composite along the longitudinal (L) axis. Principles of Composite Material Mechanics 292 Fiber and matrix T Matrix θ α L α Matrix FIGURE 6.46 Composite panel with ibers arranged in X-pattern. From tensile tests of a unidirectional composite consisting of the same iber and matrix materials and the same iber volume fraction, it is found that the off-axis Young’s modulus of the composite can be described by the equation π Ex (θ) = 100 − 90 sin θ (GPa) 0 ≤ θ ≤ 2 whereas the Young’s modulus of the matrix material is Em = 3.5 GPa. Determine the angle α in Figure 6.46 such that the longitudinal Young’s modulus of the X-pattern composite is equal to 90% of the Young’s modulus of the randomly oriented iber composite. PROBLEM 6.12 Determine the CTE for a randomly oriented iber composite in terms of the longitudinal and transverse CTEs α1 and α2 of the corresponding unidirectional composite lamina. PROBLEM 6.13 Using micromechanics and the Tsai–Hill criterion, set up the equation for the averaged isotropic tensile strength for a randomly oriented short-iber composite. The equation should be in terms of iber and matrix properties and volume fractions and the angle θ. PROBLEM 6.14 Using the maximum strain criterion and the appropriate micromechanics equations, set up the equation for predicting the averaged isotropic strength of a randomly oriented short-iber-reinforced composite. You may assume that the matrix failure strain is greater than the iber failure strain. Your answer should be given in terms of the appropriate iber and matrix properties and volume fractions and trigonometric functions of the iber orientation angle θ. It is not necessary to solve the equation. Analysis of a Discontinuously Reinforced Lamina 293 PROBLEM 6.15 The off-axis Young’s modulus for a particular unidirectional iber-reinforced orthotropic composite lamina is given by Ex = E1 − (E1 − E2 ) sin θ where θ is the lamina orientation in radians, E1 is the longitudinal Young’s modulus of the lamina, and E2 is the transverse Young’s modulus of the lamina. (a) For the material described above, ind the equation for the Young’s modulus of the composite if the ibers are randomly oriented with respect to θ. Express your answer in terms of E1 and E2. Derive your own equation and do not use the Tsai–Pagano equation (Equation 6.44). (b) For the equation derived in part (a), what would be the appropriate micromechanics equations to use in the derived equation if the ibers are continuous? (c) For the equation derived in part (a), what would be the appropriate micromechanics equations to use in the derived equation if the ibers are discontinuous? PROBLEM 6.16 Set up the equations for predicting the averaged isotropic shear modulus of a randomly oriented short-iber composite. Your answer should be in terms of the iber and matrix properties and volume fractions and trigonometric functions of the iber orientation angle, θ. It is not necessary to solve the equation. PROBLEM 6.17 Using the Tsai–Hill criterion and the appropriate micromechanics equations, set up the equation for predicting the averaged isotropic shear strength for a randomly oriented short-iber composite. Your answer should be in terms of the iber and matrix properties and volume fractions and trigonometric functions of the iber orientation angle, θ. It is not necessary to solve the equation. PROBLEM 6.18 Verify the three predictions (i.e., Equations 3.27, 3.40, and 6.67) for the Young’s modulus of the glass microsphere-reinforced polyester composite in Figure 6.42 for the speciic case of a particle volume fraction of 0.464. The required input data are given in the text accompanying the discussion of Figure 6.42. Compare these results with the corresponding experimental value of the Young’s modulus of 1.01 × 106 psi and discuss. PROBLEM 6.19 Derive Equation 6.68. 294 Principles of Composite Material Mechanics References 1. Kelly, A. and Tyson, W. R. 1965. Tensile properties of ibre reinforced metals: Copper/tungsten and copper/molybdenum. Journal of the Mechanics and Physics of Solids, 13, 329–350. 2. Cox, H. L. 1952. The elasticity and strength of paper and other ibrous materials. British Journal of Applied Physics, 3, 72–79. 3. Rosen, B. W. 1987. Composite materials analysis and design. In Reinhart, T. J. ed., Engineered Materials Handbook, Composites, Vol. 1, Section 4, pp. 173–281. ASM International, Materials Park, OH. 4. Agarwal, B. D. and Broutman, L. J. 1990. Analysis and Performance of Fiber Composites, 2nd edn. John Wiley & Sons Inc., New York, NY. 5. Drzal, L. T., Rich, M. J., and Lloyd, P. F. 1982. Adhesion of graphite ibers to epoxy matrices: I. The role of iber surface treatment. Journal of Adhesion, 16, 1–30. 6. Drzal, L. T., Rich, M. J., Koenig, M. F., and Lloyd, P. F. 1983. Adhesion of graphite ibers to epoxy matrices: II. The effect of iber inish. Journal of Adhesion, 16, 133–152. 7. Kelly, A. 1973. Strong Solids, 2nd edn. Clarendon Press, Oxford. 8. Rosen, B. W. 1965. Mechanics of composite strengthening. In Bush, S. H. ed., Fiber Composite Materials, Chapter 3, pp. 37–75. American Society for Metals, Metals Park, OH. 9. Gibson, R. F., Chaturvedi, S. K., and Sun, C. T. 1982. Complex moduli of aligned discontinuous ibre reinforced polymer composites. Journal of Materials Science, 17, 3499–3509. 10. Hwang, S. J. 1985. Finite element modeling of damping in discontinuous iber composites. MS Thesis, University of Idaho, Moscow, ID. 11. Sun, C. T. and Wu, J. K. 1984. Stress distribution of aligned short iber composites under axial load. Journal of Reinforced Plastics and Composites, 3, 130–144. 12. Tyson, W. R. and Davies, G. J. 1965. A photoelastic study of the shear stress associated with the transfer of stress during iber reinforcement. British Journal of Applied Physics, 16, 199–205. 13. MacLaughlin, T. F. 1968. A photoelastic analysis of iber discontinuities in composite materials. Journal of Composite Materials, 2(1), 44–45. 14. Suarez, S. A., Gibson, R. F., Sun, C. T., and Chaturvedi, S. K. 1986. The inluence of iber length and iber orientation on damping and stiffness of polymer composite materials. Experimental Mechanics, 26(2), 175–184. 15. Hwang, S. J. and Gibson, R. F. 1987. Micromechanical modeling of damping in discontinuous iber composites using a strain energy/inite element approach. Journal of Engineering Materials and Technology, 109, 47–52. 16. Halpin, J. C. 1969. Stiffness and expansion estimates for oriented short iber composites. Journal of Composite Materials, 3, 732–734. 17. Tucker, C. L. and Liang, E. 1999. Stiffness predictions for unidirectional short iber composites: Review and evaluation. Composites Science and Technology, 59(5), 655–671. 18. Chon, C. T. and Sun, C. T. 1980. Stress distribution along a short iber in iber reinforced plastics. Journal of Materials Science, 15, 931–938. Analysis of a Discontinuously Reinforced Lamina 295 19. Sun, C. T., Gibson, R. F., and Chaturvedi, S. K. 1985. Internal damping of polymer matrix composites under off-axis loading. Journal of Materials Science, 20, 2575–2585. 20. Baxter, W. J. 1992. The strength of metal matrix composites reinforced with randomly oriented discontinuous ibers. Metallurgical Transactions A, 23A, 3045–3053. 21. Lees, J. K. 1968. A study of the tensile strength of short iber reinforced plastics. Polymer Engineering and Science, 8(3), 195–201. 22. Chen, P. E. 1971. Strength properties of discontinuous iber composites. Polymer Engineering and Science, 11(1), 51–55. 23. Halpin, J. C. and Kardos, J. L. 1978. Strength of discontinuous reinforced composites: I. Fiber reinforced composites. Polymer Engineering and Science, 18(6), 496–504. 24. Nielsen, L. E. and Chen, P. E. 1968. Young’s modulus of composites illed with randomly oriented ibers. Journal of Materials, 3(2), 352–358. 25. Tsai, S. W. and Pagano, N. J. 1968. Invariant properties of composite materials. In Tsai, S. W., Halpin, J. C., and Pagano, N. J., eds., Composite Materials Workshop, pp. 233–252. Technomic Publishing Co., Lancaster, PA. 26. Halpin, J. C. and Pagano, N. J. 1969. The laminate approximation for randomly oriented ibrous composites. Journal of Composite Materials, 3, 720–724. 27. Manera, M. 1977. Elastic properties of randomly oriented short iber-glass composites. Journal of Composite Materials, 11, 235–247. 28. Christensen, R. M. and Waals, F. M. 1972. Effective stiffness of randomly oriented ibre composites. Journal of Composite Materials, 6, 518–532. 29. Hashin, Z. 1965. On elastic behavior of ibre reinforced materials of arbitrary transverse phase geometry. Journal of the Mechanics and Physics of Solids, 13, 119–134. 30. Hashin, Z. 1966. Viscoelastic iber reinforced materials. AIAA Journal, 4, 1411–1417. 31. Hill, R. 1964. Theory of mechanical properties of iber-strengthened materials: I. Elastic behavior. Journal of the Mechanics and Physics of Solids, 12, 199–212. 32. Chang, D. C. and Weng, G. J. 1979. Elastic moduli of randomly oriented chopped ibre composites with illed resin. Journal of Materials Science, 14, 2183–2190. 33. Christensen, R. M. 1976. Asymptotic modulus results for composites containing randomly oriented ibers. International Journal of Solids and Structures, 12, 537–544. 34. Christensen, R. M. 1979. Mechanics of Composite Materials. John Wiley & Sons, New York, NY. 35. Weng, G. J. and Sun, C. T. 1979. Effects of iber length on elastic moduli of randomly oriented chopped iber composites. In Tsai, S. W. ed., Composite Materials: Testing and Design (Fifth Conference), ASTM STP 674, pp. 149–162. American Society for Testing and Materials, Philadelphia, PA. 36. Sun, C. T., Wu, J. K., and Gibson, R. F. 1985. Prediction of material damping in randomly oriented short iber polymer matrix composites. Journal of Reinforced Plastics and Composites, 4, 262–272. 37. Iijima, S. 1991. Helical microtubules of graphitic carbon. Nature, 354, 56–58. 38. Qian, D., Wagner, J. G., Liu, W. K., Yu, M. F., and Ruoff, R. S. 2002. Mechanics of carbon nanotubes. Applied Mechanics Reviews, 55(6), 495–533. 296 Principles of Composite Material Mechanics 39. Thostenson, E. T., Ren, Z., and Chou, T. W. 2001. Advances in the science and technology of carbon nanotubes and their composites: A review. Composites Science and Technology, 61(13), 1899–1912. 40. Gates, T. S. ed. 2003. Modeling and characterization of nanostructured materials. Composites Science and Technology (Special Issue), 63(11), 1497–1724. 41. Tibbetts, G. G. and McHugh, J. J. 1999. Mechanical properties of vapor-grown carbon iber composites with thermoplastic matrices. Journal of Materials Research, 14(7), 2871–2880. 42. Qian, D., Dickey, E. C., Andrews, R., and Rantell, T. 2000. Load transfer and deformation mechanisms in carbon nanotube–polystyrene composites. Applied Physics Letters, 76(20), 2868–2870. 43. Yu, M.-F., Files, B., Arepalli, S., and Ruoff, R. S. 2000. Tensile loading of ropes of single wall carbon nanotubes and their mechanical properties. Physical Review Letters, 84(24), 5552–5555. 44. Fisher, F. T. 2002. Nanomechanics of carbon nanotube-reinforced polymers. PhD thesis, Department of Mechanical Engineering, Northwestern University, Evanston, IL. 45. Fisher, F. T., Bradshaw, R. D., and Brinson, L. C. 2003. Fiber waviness in nanotubereinforced polymer composites—I: Modulus predictions using effective nanotube properties. Composites Science and Technology, 63(11), 1689–1703. 46. Bradshaw, R. D., Fisher, F. T., and Brinson, L. C. 2003. Fiber waviness in nanotube-reinforced polymer composites—II: Modeling via numerical approximation of the dilute strain concentration tensor. Composites Science and Technology, 63(11), 1705–1722. 47. Anumandla, V. 2004. A comprehensive closed form micromechanics model for estimating the elastic modulus of nanotube-reinforced composites. MS thesis, Department of Mechanical Engineering, Wayne State University, Detroit, MI. 48. Anumandla, V. and Gibson, R. F. 2006. A comprehensive closed form micromechanics model for estimating the elastic modulus of nanotube-reinforced composites. Composites Part A: Applied Science and Manufacturing, 37(12), 2178–2185. 49. Chan, W. S. and Wang, J. S. 1994. Inluence of iber waviness on the structural response of composite laminates. Journal of Thermoplastic Composite Materials, 7(3), 243–260. 50. Hsiao, H. M. and Daniel, I. M. 1996. Elastic properties of composites with iber waviness. Composites Part A: Applied Science and Manufacturing, 27(10), 931–941. 51. Andrews, R., Jacques, D., Minot, M., and Ratnell, T. 2002. Fabrication of carbon multiwall nanotube/polymer composites by shear mixing. Micromolecular Materials Engineering, 287(6), 395–403. 52. Vlasveld, D. P. N., Bersee, H. E. N., and Picken, S. J. 2005. Nanocomposite matrix for increased ibre composite strength. Polymer, 46, 10269–10278. 53. Thostenson, E. T., Li, W. Z., Wang, D. Z., Ren, Z. F., and Chou, T. W. 2002. Carbon nanotube/carbon iber hybrid multiscale composite. Journal of Applied Physics, 91(9), 6034–6037. 54. Sahu, S. and Broutman, L. J. 1972. Mechanical properties of particulate composites. Polymer Engineering and Science, 12(2), 91–100. 55. Nicolais, L. and Narkis, M. 1971. Stress–strain behavior of styrene-acrylonitrile/ glass bead composites in the glassy region. Polymer Engineering and Science, 11(3), 194–199. Analysis of a Discontinuously Reinforced Lamina 297 56. Katz, H. S. and Milewski, J. V., eds. 1978. Handbook of Fillers and Reinforcements for Plastics. Van Nostrand Reinhold Co., New York, NY. 57. Liang, J. Z. and Li, R. K. Y. 1998. Mechanical properties and morphology of glass bead-illed polypropylene composites. Polymer Composites, 19(6), 698–703. 58. Liang, J. Z. 2007. Tensile properties of hollow glass bead-illed polypropylene composites. Journal of Applied Polymer Science, 104, 1697–1701. 59. Cho, J., Joshi, M. S., and Sun, C. T. 2006. Effect of inclusion size on mechanical properties of polymeric composites with micro and nano particles. Composites Science and Technology, 66, 1941–1952. 60. Nicolais, L. and Nicodemo, L. 1974. The effect of particle shape on tensile properties of glassy thermoplastic composites. International Journal of Polymeric Materials, 3(3), 229–243. 61. Nielsen, L. E. and Landel, R. F. 1994. Mechanical Properties of Polymers and Polymer Composites, 2nd edn. Marcel Dekker Inc., New York, NY. 62. Richard, T. G. 1975. The mechanical behavior of a solid microsphere illed composite. Journal of Composite Materials, 9, 108–113. 63. Cho, J. and Sun, C. T. 2007. A molecular dynamics simulation study of inclusion size effect on polymeric composites. Computational Materials Science, 41, 54–62. 64. Boutaleb, S., Zairi, F., Mesbah, A., Nait-Abdelaziz, M., Gloaguen, J. M., Boukharouba, T., and Lefebre, J. M. 2009. Micromechanics-based modeling of stiffness and yield stress for silica/polymer nanocomposites. International Journal of Solids and Structures, 46, 1716–1726. 65. Uddin, M. F. and Sun, C. T. 2008. Strength of unidirectional glass/epoxy composite with silica nanoparticle-enhanced matrix. Composites Science and Technology, 68, 1637–1643. 66. Uddin, M. F. and Sun, C. T. 2010. Improved dispersion and mechanical properties of hybrid nanocomposites. Composites Science and Technology, 70, 223–230. 67. Liu, S., Zhang, H., Zhang, Z., Zhang, T., and Sprenger, S. 2008. Tailoring the mechanical properties of epoxy resin by various nanoparticles. Polymers and Polymer Composites, 16(8), 471–477. 68. Zhang, H., Tang, L.-C., Zhang Z., Friedrich, K., and Sprenger, S. 2008. Fracture behavior of in situ nanoparticle-illed epoxy at different temperatures. Polymer, 49, 3816–3825. 69. Manjunatha, C. M., Taylor, A. C., and Kinloch, A. J. 2009. The effect of rubber micro-particles and silica nano-particles on the tensile fatigue behavior of a glass ibre epoxy composite. Journal of Materials Science, 44, 342–345. 70. Veedu, V. P., Cao, A., Li, X., Ma, K., Soldano, C., Kar, S., Ajayan, P. M., and Ghasemi-Nejhad, M. N. 2006. Multifunctional composites using reinforced laminae with carbon nanotube forests. Nature Materials, 5, 457–462. 71. Garcia, E. J., Hart, A. J., and Wardle, B. L. 2008. Long carbon nanotubes grown on the surface of ibers for hybrid composites. AIAA Journal, 46(6), 1405–1412. 72. Garcia, E. J., Wardle, B. L., and Hart, A. J. 2008. Joining prepreg composite interfaces with aligned carbon nanotubes. Composites Part A: Applied Science and Manufacturing, 39, 1065–1070. 73. Garcia, E. J., Wardle, B. L., Hart, A. J., and Yamamoto, N. 2008. Fabrication and multifunctional properties of a hybrid laminate with aligned carbon nanotubes grown in situ. Composites Science and Technology, 68, 2034–2041. 298 Principles of Composite Material Mechanics 74. Blanco, J., Garcia, E. J., Guzman de Viloria, R., and Wardle, B. L., 2009. Limitations of mode I interlaminar toughening of composites reinforced with aligned carbon nanotubes. Journal of Composite Materials, 43, 825–841. 75. Wick, S., Guzman de Viloria, R., and Wardle, B. L. 2010. Interlaminar and intralaminar reinforcement of composite laminates with aligned carbon nanotubes. Composites Science and Technology, 70, 20–28. 76. Gibson, R. F. 2010. A review of recent research on mechanics of multifunctional composite materials and structures. Composite Structures, 92, 2793–2810. 77. Zhang, H., Zhang, Z., Friedrich, K., and Eger, C. 2006. Property improvements of in situ epoxy nanocomposites with reduced interparticle distance at high nanosilica content. Acta Materialia, 54, 1833–1842. 7 Analysis of Laminates 7.1 Introduction While an understanding of lamina mechanical behavior is essential to the development of theories for the analysis of composite structures, the unidirectional lamina alone is generally not very useful as a structural element because of its poor transverse properties. Composite structures are more likely to be in the form of laminates consisting of multiple laminae or plies oriented in the desired directions and bonded together in a structural unit. The virtually limitless combinations of ply materials, ply orientations, and ply-stacking sequences offered by laminated construction considerably enhance the design lexibility inherent in composite structures. In this chapter, the analysis of laminates will be introduced by considering a simpliied theory of laminated beams in pure lexure, and then the effects of the transverse shear force will be treated separately. This will be followed by a discussion of the more general classical lamination theory (CLT), which makes it possible to analyze the complex coupling effects that may occur in laminates. Other aspects of laminate analysis such as prediction of thermal and residual stresses, interlaminar stresses, and laminate strength are also discussed. Owing to the need for adequate description of many possible combinations of ply orientations and stacking sequences in laminates, a laminate orientation code has evolved in the composites literature. The basis of the code is that ply angles, separated by slashes, are listed in order from the top surface to the bottom surface and enclosed in square brackets, as shown by the examples in Figure 7.1. Note that symmetric laminates can be described by listing only the ply angles for the top half of the laminate and by using the subscript “s” outside the brackets, and that adjacent plies having the same orientations can be described by using a numerical subscript on the appropriate ply angle. In the case of symmetric laminates having an odd number of plies, the center ply angle is denoted by an overbar. Sets of ply angles that are repeated in the laminate are identiied by enclosing the set of angles in parentheses. The examples shown in Figure 7.1 are for laminates consisting of plies of the same material. For hybrid laminates having plies of different 299 Principles of Composite Material Mechanics 300 [0/90/45]s 0° 90° 45° 45° 90° 0° [(0/ – + 30)2] 0° –30° +30° 0° –30° +30° [±45/02/90]s [(0/90)2/45]s 0° 90° 0° 90° 45° 90° 0° 90° 0° +45° –45° 0° 0° 90° 90° 0° 0° –45° +45° [0/ – + 45/0/90]s 0° –45° +45° 0° 90° 0° +45° –45° 0° [90/45/30/0/90/45] 90° 45° 30° 0° 90° 45° FIGURE 7.1 Examples of laminate stacking sequences and the corresponding laminate orientation codes. materials, additional subscripts on the ply angles may be used to identify the ply material. 7.2 Theory of Laminated Beams 7.2.1 Flexural Stresses and Deflections For the purpose of analysis, the simplest laminated structure is a laminated beam that is subjected to pure bending. A theory of laminated beams in pure lexure can be developed from the Bernoulli–Euler theory of the elementary mechanics of materials. Although the application of this theory is quite restricted, it yields considerable insight into the analysis of laminated structures and provides a natural introduction to the more general CLT, which Analysis of Laminates 301 is described in the next section. The theory described here is based on the analysis of Pagano [1]. A section of a rectangular laminated beam of depth h and width b is shown in Figure 7.2 before and after the application of a bending moment M. The assumptions used in developing the analysis are as follows: 1. Plane sections that are initially normal to the longitudinal axis of the beam remain plane and normal during lexure. 2. The beam has both geometric and material property symmetry about the neutral surface (i.e., the plies are symmetrically arranged about the xy-plane). 3. Each ply is linearly elastic with no shear coupling (i.e., ply orientations are either 0° or 90°). 4. The plies are perfectly bonded together, so that no slip occurs at ply interfaces. 5. The only stress components present are σx and τxz. As a result of Assumption 1, the longitudinal normal strain at a distance z from the neutral surface is given by the familiar equation εx = (ρ + z)φ − ρφ z = ρφ ρ (7.1) where ρ is the radius of curvature of the neutral surface during lexure, ϕ is the angle deined in Figure 7.2, and z is the distance from neutral surface deined by the xy-plane. ρϕ ρ ϕ M z0 = 0 zj zj–1 1 M x h x j N/2 b y z Before deformation y z After flexural deformation FIGURE 7.2 Element of a laminated beam before and after the application of a bending moment. Principles of Composite Material Mechanics 302 From Assumption 3, the longitudinal stress in the jth ply is given by (σ x ) j = (Ex ) j (ε x ) (7.2) where (Ex)j is the Young’s modulus of jth ply along the x-direction and (εx)j is the longitudinal strain in the jth ply along the x-direction. From Equations 7.1 and 7.2, the longitudinal stress is seen to be (σ x ) j = (Ex ) j z ρ (7.3) Static equilibrium requires that the applied bending moment M must be related to the longitudinal stresses by h/ 2 M=2 ∫ σ zb dz x (7.4) 0 where the symmetry Assumption 2 has been used. Substitution of Equation 7.3 into Equation 7.4 gives 2b M= 3ρ N /2 ∑(E ) (z x j 3 j − z 3j −1 ) (7.5) j =1 where N is the total number of plies and zj is the distance from the neutral surface to the outside of the jth ply. For an even number of plies of uniform thickness zj = jh/N and Equation 7.5 becomes 2bh 3 M= 3ρN 3 N /2 ∑(E ) (3 j x j 2 − 3 j + 1) (7.6) j =1 Equation 7.6 can also be used for an odd number of plies if we simply divide each ply into two identical plies having half the thickness of the original ply, so that the total number of plies is now even. Recall from the mechanics of materials that for a homogeneous, isotropic beam, the moment–curvature relation is given by M= Ef I yy Ef bh 3 = ρ 12ρ (7.7) where Iyy = ∫z2 dA = bh3/12 is the moment of inertia of the cross section about the neutral axis (y-axis), A is the cross-sectional area, and Ef is the effective Analysis of Laminates 303 lexural modulus of the beam (which is same as the Young’s modulus of the beam material for a homogeneous, isotropic beam). Note that the subscript “f” here denotes “lexural” and not “iber.” Combining Equations 7.5 and 7.7, we ind that the effective lexural modulus of the laminated beam can be expressed as N /2 ∑(E ) (z 8 Ef = 3 h x j 3 j − z 3j −1 ) (7.8) j =1 or for an even number of uniform thickness plies, we can combine Equations 7.6 and 7.7 to get 8 Ef = 3 N N /2 ∑(E ) (3 j x j 2 − 3 j + 1) (7.9) j =1 Thus, the lexural modulus of the laminated beam, unlike the Young’s modulus of the homogeneous isotropic beam, depends on the ply-stacking sequence and the ply moduli. That is, if the properties do not change through the thickness of a beam, the lexural modulus is the same as the Young’s modulus. The lexural delections of laminated beams can now be calculated by using the lexural modulus in place of the Young’s modulus in the beam delection equations from the elementary mechanics of materials [2]. For example, the differential equation for the transverse lexural delection, wf, of a laminated beam would be of the form Ef I yy d 2 wf =M dx 2 (7.10) and the maximum lexural delection, wfmax, at the tip of the laminated cantilever beam in Figure 7.3 would be given by the familiar equation wfmax = PL3 3Ef I yy at x = L (7.11) P Ef Iyy x L z FIGURE 7.3 Cantilevered laminated beam under a concentrated tip load. Principles of Composite Material Mechanics 304 where P is the applied tip load and L is the beam length. If the beam is loaded as a column in axial compression, the Euler buckling load, Pcr, for a laminated beam can be estimated by the formula Pcr = π 2Ef I yy L2e (7.12) where L e is the effective length that includes the effect of end conditions. Similarly, other beam equations involving the Young’s modulus can now be modiied for use with laminated beams. An alternative expression for the stress in the jth ply can be obtained by combining Equations 7.3 and 7.7 and by eliminating the radius of curvature: (σ x ) j = M Mz (Ex ) j (Ex ) j z = Ef I yy I yy Ef (7.13) Thus, the term in square brackets can be thought of as a correction term, which when multiplied by the familiar homogeneous isotropic beam stress, Mz/Iyy gives the stress in the jth ply of the laminated beam. Another important observation is that the maximum stress in the laminated beam does not always occur on the outer surface as it does in the homogeneous, isotropic beam. At each section in a laminated beam, the ratio M/EfIyy is constant, and the remaining term (Ex)jz determines the maximum stress. The maximum stress in the laminated beam therefore occurs in the ply having the greatest product of modulus (Ex)j and distance from the neutral axis, z. For the homogeneous isotropic beam, the stress at a given point in the cross section depends only on the distance z, and the maximum stress occurs at the outer surface, where z is the greatest. The stress distributions in homogeneous isotropic beams and laminated beams are compared schematically in Figure 7.4. Failure of laminated beams can be estimated by using the stress from Equation 7.13 in one of the failure criteria that was discussed in Chapter 4. For example, if the jth ply is a longitudinal (0°) ply in compression, failure in this ply according to the maximum stress criterion will occur when (σ xmax ) j = sL( − ) , where (σxmax)j is the maximum stress in the jth ply at z = zj. From Equation 7.13, the applied bending moment that would cause this condition is Mmax = Ef I yy sL( − ) (E1 ) j z j (7.14) where (E1)j is the longitudinal modulus of the jth ply. Similarly, for a transverse (90°) ply in tension, the maximum bending moment is Analysis of Laminates 305 Homogenous, isotropic σx Laminated σx σx 3 2 2 1 x 3 (Ex)3 > (Ex)2 > (Ex)1 x 1 x (Ex)1 = (Ex)3 < (Ex)2 FIGURE 7.4 Stress distributions in homogeneous, isotropic beams, and in laminated beams. Mmax = Ef I yy sT( + ) (E2 ) j z j (7.15) Laminate failure would therefore occur when the bending moment reaches the value that would cause irst ply failure. This value can be determined by applying the failure criterion to each ply until the lowest Mmax is found. The internal bending moment can be related to the external applied loads by the equations of static equilibrium, so that the applied loads corresponding to irst ply failure can also be determined. Since the maximum stress does not necessarily occur on the outer surface, irst ply failure may occur in an interior ply. One of the dificulties encountered in inspection for ply failure in laminates is that only failures on the outer surfaces can be observed with the naked eye. Interior ply failures can only be detected by methods such as ultrasonic or X-ray inspection. 7.2.2 Shear Stresses and Deflections In most practical cases, the applied loads on a beam would be such that not only bending moments, but also transverse shear forces would be developed. These transverse shear forces cause corresponding transverse shear stresses and delections. In laminated beams, the transverse shear stresses are often referred to as interlaminar shear stresses. Pagano [1] has also developed a mechanics of materials approach for estimating interlaminar shear stresses, as summarized here. Recall from the mechanics of materials [2] that the bending moment, M, is related to the transverse shear force, V, by the equation dM =V dx (7.16) Principles of Composite Material Mechanics 306 Thus, the presence of the shear force implies that the bending moment must change along the length of the beam (the x-direction). From Equation 7.13, we see that if the bending moment changes with respect to x, so, too, must the normal stresses, σx. This means that the normal stresses acting on the two faces of the jth ply in a differential element must be different, as shown in Figure 7.5. Since the element cannot be in static equilibrium under these normal stresses alone, the interlaminar shear stress, (τxz)k, must act at the inner edge of the kth ply, as shown in Figure 7.5. From static equilibrium of the element with respect to the forces along the x-direction, N /2 z j (τ xz )k dx + N /2 z j ∑ ∫ (σ ) dz − ∑ ∫ (σ ) + x j x j j = k z j−1 j = k z j−1 d(σ x ) j dx dz = 0 dx (7.17) or N /2 z j (τ xz )k = ∑∫ j = k z j−1 d(σ x ) j dz dx (7.18) Substituting Equations 7.13 and 7.16 into Equation 7.18 and integrating, we ind that the interlaminar stress at the inner edge of the kth ply is x dx (τxz)k (σx)k zj zj–1 (σx)j (σx)k + d (σx)k dx dx k j (σx)j + d (σx)j dx dx z (σx)N/2 N/2 (σx)N/2 + d (σx)N/2 dx dx FIGURE 7.5 Differential element of a laminated beam showing interlaminar shear stress that is necessary for static equilibrium when the bending moment varies along the length. Analysis of Laminates 307 V (τ xz )k = Ef I yy N /2 z j ∑ ∫ (E ) z dz x j (7.19) j = k z j−1 For a rectangular beam having an even number of plies of uniform thickness, zj = jh/N, and Equation 7.19 reduces to 3V S 2bh Ef (7.20) ∑(E ) (2 j − 1) (7.21) (τ xz )k = where S= 4 N2 N /2 x j j=k Equation 7.20 is seen to be similar to the “mechanics of materials” equation for transverse shear stress in a homogeneous isotropic beam, which is τ xz = 2 3V z − 1 4 h 2bh (7.22) Thus, the transverse shear stress is given by τ xz = 3V β 2bh (7.23) where 2 z 1 − 4 for a homogeneous isotropic beam h β= S E for a laminated beam f The shear stress distribution, as governed by the variation of the factor β, is shown for both types of beams in Figure 7.6. As the number of plies increases, the shear stress distribution for the laminated beam can be expected to approach the parabolic distribution described by Equation 7.22. For a small number of plies, however, the laminated beam shear stress distribution departs signiicantly from the parabolic distribution. Principles of Composite Material Mechanics 308 Homogenous isotropic Laminated, large N Homogenous isotropic Laminated, small N 0.5 0.5 z h z h β 1.0 β Many plies 1.0 Few plies FIGURE 7.6 Variation of shear stress, as governed by the factor β, across half the beam thickness for homogeneous, isotropic beams, and for laminated beams. Results are given for laminated beams with a small number of plies and a large number of plies. Interlaminar stresses are responsible for an important failure mode in composites known as delamination. Recall that the failure criteria discussed in Chapter 4 were based only on in-plane stresses in the lamina. Both normal and shear components of the interlaminar stresses in laminated plates along with failure criteria, which include the interlaminar stresses, will be discussed later. Equation 7.10 is the differential equation for the lexural delection, wf, of laminated beams due to the bending moment, M. The corresponding differential equation for the shear delection, ws, of a laminated beam due to the shear force V is approximately dws V = dx AGt (7.24) where A is the cross-sectional area of the beam and Gt is the effective transverse (or through the thickness) shear modulus of the beam. The total delection of the beam is then w = wf + ws (7.25) For the cantilever beam in Figure 7.3, the maximum shear delection, wsmax, at x = L is given by wsmax = PL AGt (7.26) Analysis of Laminates 309 Note that, while wfmax in Equation 7.10 is proportional to L3, wsmax in Equation 7.26 is proportional to L, and so for long beams, the lexural delection is typically much greater than the shear delection. However, due to the relatively low effective shear modulus Gt for some laminates, the shear delection may be signiicant, especially for short beams. As will be shown later in Section 7.11.1, Gt may be particularly low in sandwich beams due to the low shear modulus of the foam or honeycomb core material. EXAMPLE 7.1 Determine the lexural and Young’s moduli of E-glass/epoxy laminated beams having stacking sequences of [0/90/0]s and [90/0/90]s. The ply moduli are E1 = 5 × 106 psi (34.48 GPa) and E2 = 1.5 × 106 psi (10.34 GPa), and the plies all have the same thickness. Solution The total number of plies is N = 6 in each case, and only the stacking sequences are different. Since the ply thicknesses are all the same, we can use Equation 7.9 for the lexural modulus in both cases. For the [0/90/0]s beam, Ef = 8 N3 N /2 ∑(E ) (3 j x j 2 − 3 j + 1) j =1 or Ef = { } 8 5[3(1)2 − 3 + 1] + 1.5[3(2)2 − 3(2) + 1] + 5[3(3)2 − 3(3) + 1] × 10 6 psi (6 )3 = 4.09 × 10 6 psi (28.2 GPa) The Young’s modulus or extensional modulus, can be estimated by using the rule of mixtures Ex = E1υ1 + E2 υ2 where υ1 = volume fraction of longitudinal (0°) plies and υ2 = volume fraction of transverse (90°) plies. Therefore, 4 2 Ex = 5 + 1.5 × 106 psi = 3.83 × 10 6 psi (26.4 GPa) 6 6 For the [90/0/90]s beam, Ef = 8 {1.5(1) + 5(7 ) + 1.5(19)} × 10 6 psi = 2.4 × 10 6 psi (16.55 GPa) (6 )3 Principles of Composite Material Mechanics 310 and 4 2 Ex = 1.5 + 5 × 10 6 psi = 2.66 × 10 6 psi (18.34 GPa) 6 6 Note that the lexural modulus depends on the stacking sequence and is not the same as the Young’s modulus. The Young’s modulus does not depend on the stacking sequence (i.e., the rule of mixtures gives the same result regardless of the ply-stacking sequence, as long as the number of longitudinal and transverse plies remains unchanged). EXAMPLE 7.2 If the two laminated beams described in Example 7.1 are each 0.6 mm thick and 10 mm wide and the ply strengths are SL( + ) = SL( − ) = 700 MPa, ST( + ) = ST( − ) = 7.0 MPa, use the maximum stress criterion to determine the maximum allowable bending moment that each beam can withstand. Compare the maximum allowable bending moments for the two beams. Solution Rearranging Equation 7.13, the bending moment is found to be M = Ef I yy (σ x ) j (Ex ) j z where, for the rectangular cross-section beam, I yy = bh 3 10(0.6)3 = = 0.18 mm 4 12 12 The maximum stress in each ply occurs at the outer edge of the ply, so the maximum allowable bending moment is found by calculating the value of M corresponding to the maximum stress in each ply, then selecting the smallest of these values of M. For the [0/90/0]s beam, from Example 7.1, the lexural modulus is Ef = 28.2 GPa. For the outer 0° ply, (Ex ) j = E1 = 34.48 GPa, (σ x ) j = SL( + ) = SL( − ) = 700 MPa, z = 0.3 mm at the outer edge of the outer 0° ply, therefore M = (28.2 × 10 9 N/m 2 )(0.18 mm 4 ) m 700 × 10 6 N/m 2 (34.48 × 10 9 N/m 2 )(0.3 mm) 10 3 mm = 0.3435 N m Similarly, for the outer edge of the 90° ply, 3 Analysis of Laminates M = (28.2 × 10 9 N/m 2 )(0.18 mm 4 ) 311 m 7 × 10 6 N/m 2 9 2 (10.34 × 10 N/m )(0.2 mm) 10 3 mm 3 = 0.0172 N m And for the outer edge of the inner 0° ply, (Ex ) j = E1 = 34.48 GPa, (σ x ) j = S = SL( − ) = 700 MPa, z = 0.1 mm (+ ) L M = (28.2 × 10 9 N/m 2 )(0.18 mm 4 ) m 700 × 10 6 N/m 2 9 2 (34.48 × 10 N/m )(0.1 mm) 10 3 mm = 1.03 N m So, the 90° ply fails irst and the maximum allowable bending moment is 0.0172 N m. For the [90/0/90]s beam, similar calculations with Ef = 16.55 GPa from Example 7.1 show that the outer 90° ply fails irst and the corresponding maximum allowable bending moment is 0.00672 Nm. Therefore, the maximum allowable bending moment for the [0/90/0]s beam is about 2.5 times greater than that of the [90/0/90]s beam, whereas the lexural modulus of the [0/90/0]s beam is about 1.7 times greater than that of the [90/0/90]s beam. The location of the 0° ply on the outside is the main reason for the superior properties of the [0/90/0]s beam. EXAMPLE 7.3 For the [90/0/90]s E-glass/epoxy beam described in Example 7.1, sketch the distribution of normal and shear stresses through the thickness of the beam. Assume a ply thickness of 0.01 in. (0.254 mm). Solution The normal stress is given by Equation 7.13, but the ratio M/EfIyy is constant for a given cross section, and the stress distribution across the thickness is governed by the product (Ex)jz. Thus, the stress distribution can be determined to within a constant K1 = M/EfIyy by inding the corresponding variation of (Ex)jz. For the outer surface of ply number 3 (the outer transverse ply), the ply modulus is (Ex)3 = E2 = 1.5 × 106 psi, z = 0.03 in. and the stress is σx = K1(1.5 × 106)(0.03) = 4.5 × 104 K1. For the inner surface of ply number 3, z = 0.02 in. and the stress is σx = K1(1.5 × 106)(0.02) = 3.0 × 104 K1. Similarly, for the outer surface of ply number 2, the stress is σx = K1(5 × 106)(0.02) = 10 × 104 K1. 3 Principles of Composite Material Mechanics 312 For the inner surface of ply number 2, σx = K1(5 × 106)(0.01) = 5 × 104 K1. For the outer surface of ply number 1, σx = K1(1.5 × 106)(0.01) = 1.5 × 104 K1. For the inner surface of ply number 1 (on the neutral surface), σx = 0. The predicted distribution of σx across the thickness is plotted in Figure 7.7a. It is seen that the maximum normal stress occurs not on the outer surface as in a homogeneous isotropic beam but, rather, at the outer edge of ply number 2. The interlaminar shear stress at the inner surface of the kth ply for a beam with an even number of uniform thickness plies is given by Equations 7.20 and 7.21. For a given cross section, however, the ratio 3V/2bhEf can be set equal to a constant, K 2, and the shear stress can be written as (τxz)k = K 2S, where S is deined by Equation 7.21. The shear stress distribution can then be determined to within a constant K 2 by inding the variation of S across the thickness. From Equations 7.20 and 7.21, (τ xz )k = 3V S = K 2S 2bh Ef where S= (a) 4 N2 N /2 ∑(E ) (2 j − 1) x j j=k (b) 0.5 0.5 3 3 z h z h 2 1 2 1 σx 10 × 104 K1 τxz 3 × 106 K2 FIGURE 7.7 Stress distributions for the beam described in Example 7.3. (a) Normal stresses and (b) shear stresses. Analysis of Laminates 313 for k = 1, S= 4 {1.5[2(1) − 1] + 5[2(2) − 1] + 1.5[2(3) − 1]} × 106 (6 )2 = 2.66 × 106 psi (18.34 GPa) for k = 2, S= 4 {5[2(2) − 1] + 1.5[2(3) − 1]} × 10 6 (6 )2 = 2.5 × 10 6 psi (17.24 GPa) for k = 3, S= 4 {1.5[2(3) − 1]} × 10 6 (6 )2 = 0.833 × 10 6 psi (5.74 GPa) Finally, for k = 4, Equation 7.20 gives the shear stress at the inner surface of an “imaginary ply” whose inner surface is the same as the outer surface of ply number 3 or the outer surface of the laminate. Since there is no material in this “imaginary ply,” S = 0 and the shear stress must be zero on the outer surface. This also satisies the boundary condition that the outer surface must be stress free. The predicted distribution of τxz across the thickness is plotted in Figure 7.7b. As with the shear stress in a homogeneous isotropic beam, the maximum shear stress occurs on the neutral surface and the shear stress at the outer surface is zero. The deviation from the parabolic distribution is substantial, however, because of the small number of plies. EXAMPLE 7.4 Derive the differential Equation 7.24 for the shear delection of a laminated beam due to the shear force, V, and then apply it to ind Equation 7.26, the maximum shear delection for the cantilever beam in Figure 7.3. Solution A differential element of a deformed beam loaded in transverse shear is shown in Figure 7.8. For small deformations, the average shear strain, γ, is approximated by γ ≃ tan γ = dws /dx = τ/Gt , where τ is the average transverse shear stress, which is approximately equal to V/A, A is the cross-sectional area of the beam, and Gt is the effective transverse shear modulus of the beam. The result is Equation 7.24, dws V = dx AGt Principles of Composite Material Mechanics 314 ws dws γ V V x dx FIGURE 7.8 Differential element of deformed beam loaded in transverse shear. Separating variables and integrating both sides of the equation along the length of the cantilever beam in Figure 7.3, we ind that w smax ∫ L dws = 0 1 V dx AGt ∫ 0 For the cantilever beam with load P at x = L, the shear force is a constant V = P along the entire length of the beam, which leads to Equation 7.26: wsmax = PL AGt PROBLEM 7.1 A laminated [0/90/0/90]s carbon/epoxy beam is 1 mm thick, 20 mm wide, and has 0.125-mm-thick plies. The lamina properties are E1 = 180 GPa sL( + ) = 1700 MPa E2 = 10 GPa sL( − ) = 1400 MPa G12 = 7 GPa sT( + ) = 40 MPa ν12 = 0.28 sT( − ) = 230 MPa a. Determine the lexural modulus for the beam. Analysis of Laminates 315 b. How could the lexural modulus be improved without changing the ply materials, the number of plies, or the ply orientations? c. Using the maximum stress criterion for each ply, determine the magnitude of the maximum allowable bending moment that the beam can withstand. Which ply fails irst? d. What type of analysis would be required if the ply orientations are [+45/90/−45/0]s? PROBLEM 7.2 The laminated beam shown in Figure 7.9 is made up of two outer plies of material “A” having Young’s modulus EA, two inner plies of material “B” having Young’s modulus EB, and a honeycomb core of negligible stiffness. Materials A and B are isotropic, but they have different thicknesses. The laminate is symmetric about the middle surface. Find the expression for the lexural modulus in terms of the given properties and the dimensions shown in Figure 7.9. PROBLEM 7.3 A [0/90/0] laminated beam of length L is simply supported at both ends and is loaded by a single concentrated load P at midspan. Find the equation for the maximum lexural delection of the beam at midspan. PROBLEM 7.4 A thin-walled composite tube having an outside diameter of 48 mm is made by securely bonding an aluminum tube inside a steel tube, as shown in Figure 7.10. Determine the maximum allowable bending moment, M, that the Material “A” Material “B” ZA ZB Z C Core Middle surface ZA ZB ZC Material “B” Material “A” FIGURE 7.9 Laminated beam for Problem 7.2. Principles of Composite Material Mechanics 316 Steel M x y M Aluminum 48 mm z FIGURE 7.10 Composite tube for Problem 7.4. composite tube can withstand without exceeding the yield stress of either the steel or the aluminum. The tube properties are Young’s modulus (GPa) Yield stress (MPa) Wall thickness (mm) Steel Aluminum 200 259 3 78 98 6 PROBLEM 7.5 The nonsymmetrically laminated beam shown in Figure 7.11 consists of a substrate material having a Young’s modulus ES and a coating material having a Young’s modulus EC, and both materials are linear elastic, isotropic, and homogeneous. Using a modiied laminated beam theory, derive the equation for the lexural modulus Ef for the beam. Your answer should be in terms of the given parameters. Hint: Assumption #2 for laminated beam theory in Section 7.2 is violated here, so how must the derivation of the lexural modulus in Section 7.2 be modiied? Substrate, ES Coating, EC tc h x a z FIGURE 7.11 Nonsymmesrically laminated beam for Problem 7.5. b Analysis of Laminates 317 7.3 Theory of Laminated Plates with Coupling While the simpliied theory of laminated beams in pure lexure is useful and instructive, it is restricted to symmetric laminates without coupling that are subjected to a single bending moment. In this section, we will discuss the more general CLT, which does not have these restrictions. Using this theory, we can analyze nonsymmetric laminates whose arbitrarily oriented plies may have various coupling effects that may lead to complex combinations of extensional, lexural, and torsional deformations. In addition, in-plane loading due to shear and axial forces and both bending and twisting moments are included. The most important limitation of the CLT is that each ply is assumed to be in a state of plane stress and that interlaminar stresses are neglected. What is now referred to as the CLT has apparently evolved from work in the 1950s and 1960s by investigators such as Smith [3], Pister and Dong [4], Reissner and Stavsky [5], Stavsky [6], Lekhnitskii [7], and Stavsky and Hoff [8]. The major difference between this theory and the classical theory of homogeneous, isotropic plates [9] is in the form of the lamina stress–strain relationships. Other elements of the theory such as the deformation hypothesis, the equilibrium equations (Appendix B), and the strain–displacement relationships (Appendix C) are the same as those used in the classical plate theory [9]. Although the laminate is made up of multiple laminae, it is assumed that the individual laminae are perfectly bonded together so as to behave as a unitary, nonhomogeneous anisotropic plate. Interfacial slip is not allowed, and the interfacial bonds are not allowed to deform in shear, which means that displacements across lamina interfaces are assumed to be continuous. These assumptions mean that the deformation hypothesis from the classical homogeneous plate theory can be used for the laminated plate. The laminate force–deformation equations resulting from this deformation hypothesis are now derived following the procedure outlined by Whitney [10]. Although Whitney has presented a general analysis including the equations of motion, only the static analysis will be considered here. Figure 7.12 deines the coordinate system to be used in developing the laminated plate analysis. The xyz coordinate system is assumed to have its origin on the middle surface of the plate, so that the middle surface lies in the xy-plane. The displacements at a point in the x-, y-, and z-directions are u, v, and w, respectively. The basic assumptions relevant to the present static analysis are [10]: 1. The plate consists of orthotropic laminae bonded together, with the principal material axes of the orthotropic laminae oriented along arbitrary directions with respect to the xy-axes. 2. The thickness of the plate, t, is much smaller than the lengths along the plate edges, a and b. 318 Principles of Composite Material Mechanics FIGURE 7.12 Coordinate system and stress resultants for laminated plate. 3. The displacements u, v, and w are small compared with the plate thickness. 4. The in-plane strains εx, εy, and γxy are small compared with unity. 5. Transverse shear strains γxz and γyz are negligible. 6. Tangential displacements u and v are linear functions of the z coordinate. 7. The transverse normal strain εz is negligible. 8. Each ply obeys Hooke’s law. 9. The plate thickness t is constant. 10. Transverse shear stresses τxz and τyz vanish on the plate surfaces deined by z = ±t/2. Assumption 5 is a result of the assumed state of plane stress in each ply, whereas Assumptions 5 and 6 together deine the Kirchhoff deformation hypothesis that normals to the middle surface remain straight and normal during deformation. According to Assumptions 6 and 7, the displacements can be expressed as u = u0 ( x , y ) + zF1( x , y ) v = v0 ( x , y ) + zF2 ( x , y ) (7.27) w = w 0 ( x , y ) = w( x , y ) where u0 and v0 are the tangential displacements of the middle surface along the x- and y-directions, respectively. Due to Assumption 7, the transverse displacement at the middle surface, w0(x, y), is the same as the transverse Analysis of Laminates 319 displacement of any point having the same x and y coordinates, and so w0(x, y) = w(x, y). At this point, it is appropriate to mention that to account for possible warping of the cross section of the laminate and resulting transverse shear deformations, it is necessary to use a so-called higher-order lamination theory. For example, Christensen [11] describes one such theory, which is based on the assumption that the displacements are nonlinear functions of the z coordinate as follows: u = u0 ( x , y ) + zψ x ( x , y ) + z 2ζ x ( x , y ) + z 3φ x ( x , y ) v = v0 ( x , y ) + zψ y ( x , y ) + z 2ζ y ( x , y ) + z 3φ y ( x , y ) (7.28) w = w 0 ( x , y ) + zψ z ( x , y ) + z 2ζ z ( x , y ) Such a theory is beyond the scope of this book, however, and we will only develop the CLT based on Equation 7.27. Substituting Equation 7.27 in the strain–displacement equations (Appendix C) for the transverse shear strains and using Assumption 5, we ind that γ xz = ∂u ∂w ∂w = F1( x , y ) + + =0 ∂z ∂x ∂x γ yz = ∂w ∂v ∂w =0 = F2 ( x , y ) + + ∂y ∂z ∂y (7.29) and that F1( x , y ) = − ∂w ∂w , F2 ( x , y ) = − ∂x ∂y (7.30) Substituting Equations 7.27 and 7.30 in the strain–displacement relations for the in-plane strains (Appendix C), we ind that εx = ∂u = ε 0x + zκ x ∂x εy = ∂v = ε 0y + zκ y ∂y γ xy = ∂u ∂v + = γ 0xy + zκ xy ∂y ∂x where the strains on the middle surface are (7.31) Principles of Composite Material Mechanics 320 ε 0x = ∂u 0 ∂v 0 ∂u 0 ∂v 0 + , ε 0y = , γ 0xy = ∂y ∂y ∂x ∂x (7.32) and the curvatures of the middle surface are κx = − ∂ 2w ∂ 2w ∂ 2w , κ y = − 2 , κ xy = −2 2 ∂x ∂y ∂x ∂y (7.33) where κx is a bending curvature associated with bending of the middle surface in the xz-plane, κy is a bending curvature associated with bending of the middle surface in the yz-plane, and κxy is a twisting curvature associated with out-of-plane twisting of the middle surface, which lies in the xy-plane before deformation. Since Equation 7.31 gives the strains at any distance z from the middle surface, the stresses along arbitrary xy-axes in the kth lamina of a laminate may be found by substituting Equation 7.31 into the lamina stress–strain relationships from Equation 2.35 as follows: Q11 σx σ y = Q12 τ xy κ Q16 Q12 Q22 Q26 Q16 Q26 Q66 k ε 0x + zκ x 0 ε y + zκ y γ 0 + zκ x xy (7.34) where the subscript k refers to the kth lamina. Comparing the laminated plate stresses in Equation 7.34 with the laminated beam stress given by Equation 7.3, we notice several differences. The laminated beam analysis only gives the uniaxial stress, σx, due to the bending curvature, whereas the laminated plate analysis gives the two-dimensional (2D) lamina stresses σx, σy, and τxy due to bending and twisting curvatures and to the midplane biaxial extension and shear. In addition, the laminated plate analysis includes the stresses due to shear coupling, as discussed in Chapter 2. In the laminated beam analysis, Equation 7.3 for lamina stress is seen to be of limited practical use because the curvature is not generally known and is dificult to measure. Thus, the lamina stress was related to the applied bending moment by using the static equilibrium relationship in Equation 7.4. The result was that a more useful equation for stress, Equation 7.13, was developed. The bending moment can be related to the loads on the structure by additional static equilibrium equations. Similarly, in the laminated plate analysis, the midplane strains and curvatures in Equation 7.34 must be related to applied forces and moments by static equilibrium equations to make these equations more useful. In the laminated plate analysis, however, it is convenient to use forces and moments per unit length rather than forces Analysis of Laminates 321 and moments. The forces and moments per unit length shown in Figure 7.12 are also referred to as stress resultants. For example, the force per unit length, Nx, is given by t /2 Nx = N zk (σ x )k dz zk −1 ∫ σ dz = ∑ ∫ x k =1 − t /2 (7.35) and the moment per unit length, Mx, is given by t /2 Mx = ∫σ N x z dz = ∑ ∫ k =1 − t /2 zk (σ x )k z dz zk −1 (7.36) where t is the laminate thickness, (σx)k is the stress in the kth lamina, zk−1 is the distance from middle surface to inner surface of the kth lamina, and zk is the corresponding distance from middle surface to outer surface of the kth lamina, as shown in Figure 7.13. Substituting the lamina stress–strain relationships from Equation 7.34 into Equations 7.35 and 7.36, respectively, we ind that N Nx = zk ∑ ∫ {(Q } ) (ε 0x + zκ x ) + (Q12 )k (ε 0y + zκ y ) + (Q16 )( γ 0xy + zκ xy ) dz (7.37) 11 k k = 1 zk −1 and zk N Mx = ∑ ∫ {(Q } ) (ε 0x + zκ x ) + (Q12 )k (ε 0y + zκ y ) + (Q16 )k ( γ 0xy + zκ xy ) z dz (7.38) 11 k k = 1 zk −1 1 2 3 z3 Middle surface t t 2 z zk–1 zk z2 z1 zN–1 z0 zN k N FIGURE 7.13 Laminated plate geometry and ply numbering system. Caution: The ply numbering system here is different from that used in Figure 7.2 for the laminated beam analysis. Principles of Composite Material Mechanics 322 Combining terms and rearranging Equations 7.37 and 7.38, we ind that N x = A11ε 0x + A12ε 0y + A16 γ 0xy + B11κ x + B12κ y + B16κ xy (7.39) Mx = B11ε 0x + B12ε 0y + B16 γ 0xy + D11κ x + D12κ y + D16κ xy (7.40) and where the laminate extensional stiffnesses are given by t /2 Aij = ∫ N (Qij )k dz = − t /2 ∑(Q ) (z − z ij k k k −1 ) (7.41) k =1 The laminate-coupling stiffnesses are given by t /2 Bij = ∫ (Qij )k z dz = − t /2 1 2 N ∑(Q ) (z ij k 2 k − zk2−1 ) (7.42) − zk3−1 ) (7.43) k =1 and the laminate-bending stiffnesses are given by t/2 Dij = ∫ (Qij )k z 2 dz = − t/2 1 3 N ∑(Q ) (z ij k 3 k k =1 where the subscripts i, j = 1, 2, or 6. The other stress resultants can be written in similar form, and the complete set of equations can be expressed in matrix form as N x A11 A12 A16 B11 B12 B16 ε 0x N y A12 A22 A26 B12 B22 B26 ε 0y 0 N xy A16 A26 A66 B16 B26 B66 γ xy = Mx B11 B12 B16 D11 D12 D16 κ x M κ y B12 B22 B26 D12 D22 D26 y M B B B D D D κ xy 16 26 66 16 26 66 xy (7.44) or in partitioned form as N A = M B B ε 0 D κ (7.45) Analysis of Laminates Nx = A11εx0 + A12ε0y 323 0 + A16γxy + B11κx + B12κy + B16 κxy Bending along x- and y-directions Stretching of middle surface Shearing of middle surface Twisting of xy-plane Note: If B11 = B12 = B16 = 0, no bending or twisting and if A16 = 0, pure stretching of middle surface FIGURE 7.14 Illustration of decomposition of coupling effects in a general laminate loaded by a single force per unit length Nx. From Equation 7.45, we can see that the extensional stiffness matrix [A] relates the in-plane forces {N} to the midplane strains {ε0} and the bending stiffness matrix [D] relates the moments {M} to the curvatures {κ}. The coupling stiffness matrix [B] couples the in-plane forces {N} with the curvatures {κ} and the moments [M] with the midplane strains {ε0}. A laminate having nonzero Bij will bend or twist under in-plane loads. Such a laminate will also exhibit midplane stretching under bending and twisting moment loading. It can be easily shown that laminate geometric and material property symmetry with respect to the middle surface leads to the condition that all Bij = 0 and that asymmetry about the middle surface leads to nonzero Bij. The decomposition of typical force and moment terms in Equation 7.44 is illustrated in Figures 7.14 and 7.15, respectively. Note in Figure 7.14 that the corresponding force–deformation relationship for a homogeneous isotropic plate would only include the irst two terms and no coupling terms of any kind, whereas in Figure 7.15, the corresponding moment–curvature relationship for a homogeneous isotropic plate would only include the fourth and ifth terms and no coupling terms of any kind. 0 + D κ + D κ + D κxy Mx = B11ε0x + B12ε0y + B16γxy 11 x 12 y 16 Stretching of middle surface Shearing of middle surface Bending along x and y axes Twisting of xy plane Note: If B11 = B12 = B16 = 0, no stretching or shearing and if D16 = 0, pure bending Conclusion: Major simplifications possible if Bij = 0 FIGURE 7.15 Illustration of decomposition of coupling effects in a general laminate loaded by a singlebending moment per unit length Mx. Principles of Composite Material Mechanics 324 Example: Expanding expression for Nx 0 + B κ + B κ + B κx Nx = A11εx0 + A12εy0 + A16γxy 11 x 12 y 16 0 term due to coupling A16γxy at lamina level since N A16 = ∑ (Q16 )k (zk − zk−1) k=1 and Q16 is due to shear coupling in off-axis lamina (Q16 = 0 for 0° or 90° lamina) B11κx + B12κy terms cause coupling at the laminate level even though lamina coupling terms such as Q16 and Q26 may not be present. Bij terms present due to nonsymmetrical arrangement of plies about middle surface. FIGURE 7.16 Illustration of the difference between lamina level coupling and laminate level coupling in a general laminate loaded by a single force per unit length Nx. It is now clear that there may be coupling effects at both the lamina level and the laminate level, but the two types of coupling are not necessarily related. Lamina shear coupling is a result of anisotropic material behavior and the presence of 16 and 26 terms in the lamina stiffness or compliance matrices (recall Section 2.6). This type of coupling at the lamina level also leads to coupling at the laminate level due to terms such as A16, A26, D16, and D26. On the other hand, the Bij-type coupling at the laminate level is due to geometric and/or material property asymmetry with respect to the middle surface and is unrelated to material anisotropy. For example, it is possible for a laminate to have nonzero Bij even with isotropic laminae if they are stacked in nonsymmetrical fashion, but the isotropic lamina properties lead to the condition A16 = A26 = D16 = D26 = 0. Figure 7.16 illustrates the two different types of coupling that appear in one speciic laminate force–deformation equation. In the next section, the nature of the stiffness matrices for several special types of laminates will be summarized. 7.4 Stiffness Characteristics of Selected Laminate Configurations As shown in the previous section, the number of nonzero terms in the laminate stiffness matrices is reduced for certain laminate conigurations. Symmetry or antisymmetry of geometric and material properties about the middle surface, ply orientations, and ply-stacking sequences are all factors that govern the form of the laminate stiffness matrices. It is particularly important to be able to understand the effects of these factors on the Analysis of Laminates 325 type of coupling that may exist in the stiffness matrices of commonly used laminates. Before beginning the discussion of special laminate conigurations, it is useful to deine several terms that are associated with special ply orientations. Although these ply orientations, by themselves, do not necessarily produce simpliications in the stiffness matrices, they are often used in combination with other terms to describe special laminates that do have simpliied stiffness matrices. “Angle-ply” laminates have lamina orientations of either +θ or −θ, where 0° ≤ θ ≤ 90°. Depending on ply-stacking sequences, angle-ply laminates may be symmetric, antisymmetric, or asymmetric with respect to the middle surface. “Cross-ply” laminates consist of plies oriented at either θ = 0° or θ = 90°. A balanced cross-ply laminate has equal numbers of 0° and 90° plies. Depending on the ply arrangement, cross-ply laminates may be either symmetric or asymmetric with respect to the middle surface, but not antisymmetric. Since all plies in a cross-ply laminate behave as specially orthotropic laminae, such a laminate will always have Al6 = A26 = D16 = D26 = 0. However, since all plies in an angle-ply laminate behave as generally orthotropic laminae, the 16 and 26 terms may not vanish. 7.4.1 Specially Orthotropic Laminates One of the simplest possible laminates is the specially orthotropic laminate, which is nothing more than a specially orthotropic lamina (Figure 2.4, where the laminate is aligned with the principal 1,2,3 axes) of thickness t. The multilayered laminate would typically be thicker than a single lamina. From Equations 7.41 through 7.43, the laminate stiffnesses for this coniguration are A11 = Q11t , A12 = Q12t , A22 = Q22t , A66 = Q66t , A16 = A26 = 0 D11 = Q11t 3 Q t3 Q t3 Q t3 , D12 = 12 , D22 = 22 , D66 = 66 , D16 = D26 = 0 12 12 12 12 all Bij = 0 (7.46) where the lamina stiffnesses, Qij, were deined in Section 2.5. Note that, since there are no off-axis laminae, A16 = A26 = D16 = D26 = 0, and due to symmetry of the laminate about the middle surface, all Bij = 0. 7.4.2 Generally Orthotropic Laminates The generally orthotropic laminate is simply an off-axis version of the specially orthotropic laminate or a generally orthotropic lamina (Figure 2.4, where the laminate is aligned with the nonprincipal x-, y-, and z-axes) of thickness t. From Equations 7.41 through 7.43, the laminate stiffnesses for this coniguration are Principles of Composite Material Mechanics 326 A11 = Q11t , A12 = Q12t , A22 = Q22t , A66 = Q66t , A16 = Q16t , A26 = Q26t D11 = Q11t 3 Q t3 Q t3 Q t3 Q , D12 = 12 , D22 = 22 , D66 = 66 , D16 = 16 t 3 , 12 12 12 12 12 D26 = Q26 3 t 12 all Bij = 0 (7.47) where the transformed, or off-axis lamina stiffnesses, Qij , were deined in Section 2.6. In this case, due to the off-axis orientation, the 16 and 26 stiffness terms are no longer equal to zero, but since the laminate is symmetric about the middle surface, the coupling stiffnesses Bij = 0 as with the specially orthotropic laminate. 7.4.3 Symmetric Laminates A symmetric laminate has both geometric and material property symmetry about the middle surface. That is, the ply material, ply orientation, and ply thickness at a positive distance z from the middle surface are identical to the corresponding values at an equal negative distance z from the middle surface. Examples of symmetric angle-ply and cross-ply laminates are shown in Figure 7.17a and b, respectively. Such a symmetry condition when substituted in Equation 7.42 leads to the major simpliication that all Bij = 0. This means that bending–stretching coupling will not be present in such laminates. Consequently, in-plane loads will not generate bending and twisting curvatures that cause out-of-plane warping, and bending or twisting moments will not produce an extension of the middle surface. This can be particularly (a) +45° –45° +45° –45° +45° +45° –45° +45° –45° +45° z (b) x 90° 0° 90° 90° 0° 0° 90° 90° 0° 90° x z FIGURE 7.17 Examples of symmetric laminates. Ply orientations and material properties are symmetric about the middle surface. (a) Symmetric angle-ply and (b) symmetric cross-ply. Analysis of Laminates 327 important in structures that are subjected to changes in environmental conditions, where the resulting hygrothermal forces would lead to undesirable warping in nonsymmetric laminates. 7.4.4 Antisymmetric Laminates An antisymmetric laminate has plies of identical material and thickness at equal positive and negative distances from the middle surface, but the ply orientations are antisymmetric with respect to the middle surface. That is, the ply orientation at a positive distance z is +θ, if the ply orientation at an equal negative distance z is −θ. Examples of antisymmetric angle-ply laminates are shown in Figure 7.18. Note that the antisymmetric deinition has no meaning for a cross-ply laminate, which must be either symmetric or nonsymmetric. It can be shown that by substituting the antisymmetric condition into Equations 7.41 and 7.43, the coupling terms A16 = A26 = D16 = D26 = 0. From Equation 7.42, it can also be shown that B11 = B12 = B22 = B66 = 0 for the antisymmetric angle-ply laminate. 7.4.5 Quasi-Isotropic Laminates Although it may seem unlikely, it is possible to use orthotropic laminae to construct a laminate that exhibits some elements of isotropic behavior. For example, if a laminate consists of three or more identical orthotropic laminae (i.e., all have the same material and geometric properties) that are oriented at the same angle relative to adjacent laminae, the extensional stiffness matrix [A] will be isotropic, but the other stiffness matrices [B] and [D] will not necessarily have isotropic form. Such a laminate is called a quasi-isotropic or planar isotropic laminate, and the angle between adjacent laminae must be π /N, where N is the total number of laminae. For example, [60/0/−60] and [90/45/0/−45] laminates are quasi-isotropic. –45° +45° +45° –45° –45° +45° +45° –45° –45° +45° z +30° –30° x +30° x –30° +30° –30° z FIGURE 7.18 Examples of antisymmetric angle-ply laminates. Although ply orientations are antisymmetric about the middle surface, the material distribution is symmetric. Principles of Composite Material Mechanics 328 Recall that in Section 6.4, it was mentioned that randomly oriented iber composites could be modeled as planar isotropic or quasi-isotropic laminates. Now it is clear that although a randomly oriented iber composite must theoretically have an ininite number of iber orientations to be isotropic, the in-plane behavior of such materials can be modeled by using a quasiisotropic laminate having only three laminae, as in the [60/0/−60] laminate. Recall also that the stress–strain relationships for an isotropic lamina are given by Equation 2.26, with the additional requirements that Q11 = Q22, Q66 = (Q11 − Q12)/2, and Ql6 = Q26 = 0. Similarly, the extensional force–deformation relationships for the quasi-isotropic laminate are given by N x A11 N x = A12 N 0 xy A12 A11 0 ε 0x 0 ey ( A11 − A12 )/2 γ 0xy 0 0 (7.48) In general, such simpliications are not possible for the [B] and [D] matrices, as can be shown by calculating the stiffness matrices for quasi-isotropic laminates such as [60/0/−60] or [90/45/0/−45]. In Section 6.4, it was shown that the invariants could be useful in the development of the stress–strain relationships and equations for the engineering constants of a planar isotropic, randomly oriented iber composite. Similarly, the invariants can be used in the study of quasi-isotropic laminates. For example, by substituting the lamina stiffnesses in terms of invariants from Equation 2.44 in Equation 7.41 for the laminate extensional stiffnesses, we ind that A11 = A22 = U1t A12 = U 4t (7.49) (U − U 4 )t A66 = 1 2 Using developments similar to those in Section 6.4, we can show that the effective extensional engineering constants for quasi-isotropic laminates are given by Equation 6.43. EXAMPLE 7.5 Determine the stiffness matrix for a [+45/−45/−45 + 45] symmetric angle-ply laminate consisting of 0.25-mm-thick unidirectional AS/3501 carbon/epoxy laminae. An exploded view of the laminate is shown in Figure 7.19. Analysis of Laminates 329 +45 ° –45 ° y x –45 ° +45 ° z FIGURE 7.19 Exploded view of [+45/−45/−45/+45] symmetric laminate. Solution From Table 2.2, the lamina engineering constants are E1 = 138 GPa E2 = 9 GPa G12 = 6.9 GPa ν12 = 0.3 and ν21 = ν12 E2 9.0 = 0.3 = 0.0196 E1 138.0 Substitution of the above engineering constants in Equation 2.27 yields the components of the lamina stiffness matrix associated with the principal material axes: 138.8 [Q] = 2.72 0 2.72 9.05 0 0 0 GPa 6.9 The transformed lamina stiffness matrices for the +45° and −45° plies are then found by substituting the above stiffnesses in Equation 2.36 or Equations 2.44 and 2.45. For the +45° plies, Q +45° 45.22 = 31.42 32.44 31.42 45.22 32.44 32.44 32.44 GPa 35.6 Principles of Composite Material Mechanics 330 For the −45° plies, [Q]−45° 45.22 = 31.42 −32.44 31.42 45.22 −32.44 −32.44 −32.44 GPa 35.6 Note that the only difference between the stiffness matrices for the plies is that the shear-coupling terms (i.e., the terms with subscripts 16 and 26) for the −45° ply have the opposite sign from the corresponding terms for +45° ply. Before calculating the laminate stiffnesses, we must determine distances from the middle surface on the various ply interfaces, according to Figure 7.13. The distances are z0 = −0.50 mm, z1 = −0.25 mm, z2 = 0, z3 = 0.25 mm, and z4 = 0.5 mm. The laminate extensional stiffnesses are then found by substituting these distances along with the lamina stiffness in Equation 7.41: 45.22 [ A] = 31.42 0 31.42 45.22 0 0 0 GPa mm 35.6 Similarly, the laminate-coupling stiffnesses are found from Equation 7.42: 0 [B] = 0 0 0 0 0 0 0 GPa mm 2 0 and the laminate-bending stiffnesses are found from Equation 7.43: 3.77 [D] = 2.62 2.03 2.62 3.77 2.03 2.03 2.03 GPa mm 3 2.97 EXAMPLE 7.6 Determine the stiffness matrix for a [−45/+45/−45/+45] antisymmetric angle-ply laminate consisting of the same 0.25-mm-thick unidirectional AS/3501 carbon/epoxy laminae that were used in Example 7.5. An exploded view of the laminate is shown in Figure 7.20. Solution Since the lamina orientations are still +45° and −45°, the lamina stiffnesses are the same as those calculated in Example 7.5. The distances zk are also the same as those shown in Example 7.5, since the ply thicknesses and the number of plies are the same. Laminate extensional stiffnesses are then found by substituting these values, along with the antisymmetric stacking sequence, in Equation 7.41: Analysis of Laminates 331 –45 ° +45 ° y x –45 ° +45 ° z FIGURE 7.20 Exploded view of [−45/+45/−45/+45] antisymmetric laminate. 45.22 [ A] = 31.42 0 31.42 45.22 0 0 0 GPa mm 35.6 Note that these results are identical to those in Example 7.5 because we still have two plies at +45° and two plies at −45°. Thus, the stacking sequence has no effect on [A] as long as the number of plies at a given orientation remains the same. The laminate-coupling stiffnesses are found from Equation 7.42: 0 [B] = 0 4.055 0 0 4.055 4.055 4.055 GPa mm 2 0 Note that due to the antisymmetry, B11 = B22 = B12 = B66 = 0, but BI6 and B26 have nonzero values; this is true in general for antisymmetric angleply laminates. Thus, the antisymmetric laminate has extension–twisting and bending–shearing coupling, but the symmetric laminate does not. The laminate-bending stiffnesses are found from Equation 7.43: 3.77 [D] = 2.62 0 2.62 3.77 0 0 0 GPa mm 3 2.97 Principles of Composite Material Mechanics 332 Note that D11, D22, D12, and D66 are the same as the corresponding values in Example 7.5, but we now have D16 = D26 = 0. Thus, bending–twisting coupling is present in symmetric angle-ply laminates, but not in antisymmetric angle-ply laminates. EXAMPLE 7.7 Determine the stiffness matrices and engineering constants for a quasi-isotropic [60/0/−60] laminate consisting of the same laminae that were described in Example 7.5. Figure 7.21 shows an exploded view of the laminate. Solution The required lamina stiffnesses are the Qij in Example 7.5 and the appropriate transformed stiffnesses for 60° and −60° from Equation 2.36 or Equations 2.44 and 2.45. Substituting these stiffnesses in Equation 7.41, we ind that the laminate extensional stiffnesses are 44.68 [ A] = 12.80 0 12.80 44.68 0 0 0 GPa mm 15.94 It is easily shown that this matrix is of the isotropic form shown in Equation 7.48. The laminate-coupling stiffnesses from Equation 7.42 are 0 [B] = 0 −1.96 0 0 −5.06 −1.96 −5.06 GPa mm 2 0 +60 ° x 0° y –60 ° z FIGURE 7.21 Exploded view of [+60/0/−60] quasi-isotropic laminate. Analysis of Laminates 333 and the bending stiffnesses from Equation 7.43 are 0.856 [D] = 0.824 0 0.824 2.88 0 0 0 GPa mm 3 0.972 It is seen that the matrices [B] and [D] do not have the isotropic form of Equation 7.48. It can also be shown that by changing the lamina orientations while maintaining equal angles between adjacent laminae (e.g., [75/15/−45], [30/−30/−90], or [0/−60/−120]), the Aij remain unchanged, but the Bij and Dij do not. Thus, the laminate is isotropic with respect to inplane behavior only. The engineering constants for the laminate may be found by using the invariants. By substituting the Qij from Example 7.5 in Equation 2.45, we ind that U1 = 59.57 GPa and U 4 = 17.07 GPa Substituting these results in Equation 6.43, we ind that the engineering constants are Eɶ = 54.68 GPa, Gɶ = 21.25 GPa, and νɶ = 0.287 Note that the Aij can also be found by using the invariants U1 and U4, along with the laminate thickness, t, in Equation 7.49. EXAMPLE 7.8 A laminate has the stiffnesses shown below. (a) If this laminate is loaded in such a way that the midplane strain ε 0x = 0.001 mm/mm and all other strains and curvatures are equal to zero, determine all of the forces and moments per unit length acting on the laminate and (b) if this laminate is loaded in such a way that the bending curvature κx = 0.01 mm−1 and all other strains and curvatures are equal to zero, determine all of the forces and moments per unit length acting on the laminate. 22.61 [ A] = 15.71 0 0 [B] = 0 −2.027 0.471 [D] = 0.327 0 15.71 22.61 0 0 0 −2.027 0.327 0.471 0 0 0 GPa mm 17.8 −2.027 −2.027 GPa mm 2 0 0 0 GPa mm 3 0.371 Principles of Composite Material Mechanics 334 Solution a. N x = A11ε 0x = (22.61)(0.001) = 0.02261 GPa mm N y = A12 ε 0x = (15.71)(0.001) = 0.01571 GPa mm N xy = A16 ε 0x = 0 Mx = B11ε 0x = 0 M y = B12 ε 0x = 0 Mxy = B16 ε 0x = (−2.027 )(0.001) = −0.002027 GPa mm 2 b. N x = B11κ x = 0 N y = B12κ x = 0 N xy = B16κ x = (−2.027 )(0.01) = −0.02027 GPa mm Mx = D11κ x = (0.471)(0.01) = 0.00471 GPa mm 2 M y = D12κ x = (0.327 )(0.01) = 0.00327 GPa mm 2 Mxy = D16κ x = 0 PROBLEM 7.6 Determine the stiffness matrix for a [+45/−45] antisymmetric laminate consisting of 0.25-mm-thick unidirectional AS/3501 carbon/epoxy plies. PROBLEM 7.7 Show that for symmetric laminates the coupling stiffnesses, Bij, must all be equal to zero. PROBLEM 7.8 By expanding the [A] matrix in terms of ply stiffnesses show that a “balanced” cross-ply laminate having equal numbers of 0° and 90° plies is not necessarily quasi-isotropic. PROBLEM 7.9 A [−60/0/60] laminate and a [0/45/90] laminate both consist of 1.0-mmthick plies having the following properties: E1 = 181 GPa, E2 = 10.3 GPa, G12 = 7.17 GPa, and ν12 = 0.28. Plot the Aij, for both laminates as a function of the orientation to determine which, if any, of the laminates is quasi-isotropic. Analysis of Laminates 335 x′′ d Middle surface x z′′ t Laminate (Aij, Bij, Dij) z FIGURE 7.22 Laminate with parallel axes for Problem 7.10. PROBLEM 7.10 Develop a “parallel axis theorem” for the effective laminate stiffnesses Aij′′ , Bij′′ , and Dij′′ associated with the (x′′, z′′) axes, which are parallel to the original (x, z) axes, as shown in Figure 7.22. Express the new Aij′′ , Bij′′ , and Dij′′ in terms of the original Aij, Bij, and Dij, for the (x, z) axes and the distance d between the parallel axes, where z′′ = z + d. 7.5 Derivation and Use of Laminate Compliances Since the applied loads are generally known rather than the deformations, it is often necessary to use the inverted form of the laminate force–deformation relationships shown in Equations 7.44 and 7.45. The use of the inverted equations means that we must deal with the laminate compliance matrix instead of the laminate stiffness matrix. In this section, the inverted equations are derived and used to calculate the lamina stresses and strains due to known laminate loads. The inverted equations are also used in the derivation of the laminate engineering constants and in the comparison of predicted and measured laminate compliances. 7.5.1 Inversion of Laminate Force–Deformation Equations The general laminate force–deformation equations shown in Equation 7.45 can be expressed as N A = M B 0 B ε 0 ε = [E] D κ κ (7.50) Principles of Composite Material Mechanics 336 where Aij, Bij, and Dij make up the laminate stiffness matrix, [E]. The fully inverted form of this equation can be obtained directly by premultiplying both sides of the equation by the compliance matrix, which is the inverse of the stiffness matrix (see Appendix A) 0 ε A = κ B −1 B N N −1 = [E] D M M (7.51) Alternatively, Equation 7.51 is derived below by the inversion of subdivided smaller matrices, as shown by Halpin [12]. From Equation 7.50, the in-plane forces per unit length are {N } = [ A]{ε 0 } + [B]{κ } (7.52) whereas the moments per unit length are { M} = [B]{ε 0 } + [D]{κ } (7.53) The midplane strains may be obtained from Equation 7.52 as {ε 0 } = [ A]−1 {N } − [ A]−1[B]{κ } (7.54) Substitution of these strains in Equation 7.53 gives { M} = [B][ A]−1 {N } − [B][ A]−1[B]{κ } + [D]{κ } (7.55) Equations 7.54 and 7.55 can be combined to give a partially inverted form of Equation 7.50 as follows: 0 ε A * = M C * B * N D * κ where [ A*] = [ A]−1 [B*] = −[ A]−1[B] [C *] = [B][ A]−1 [D*] = [D] − [B][ A]−1[B] (7.56) Analysis of Laminates 337 Inverting the last set of partitioned Equation 7.56 to solve for the curvatures, we ind that {κ } = [D*]−1 { M} − [D*]−1[C *]{N } (7.57) Now substituting Equation 7.57 into Equation 7.54, we have {ε 0 } = ([ A*] − [B*][D*]−1[C *]){N } + [B*][D*]−1 { M} (7.58) Equations 7.57 and 7.58 can now be combined in partitioned matrix form to give ε 0 A′ = κ C ′ B′ N D′ M (7.59) where [ A′] = [ A*] − [B*][D*]−1[C *] [B′] = [B*][D*]−1 [C ′] = −[D*]−1[C *] = [B ’]T [D′] = [D*]−1 and the compliance matrix is A′ C′ B′ = [E]−1 D′ (7.60) Since the stiffness matrix [E] is symmetric, the compliance matrix must also be symmetric. 7.5.2 Determination of Lamina Stresses and Strains Now that we have the inverted laminate force–deformation relationships in Equation 7.59, the calculation of lamina stresses and strains from known laminate forces and moments is a straightforward procedure. For a laminate at constant temperature and moisture content, the stresses in the kth lamina are given by Equation 7.34, which can be written in abbreviated matrix notation as {σ}k = [Q]k ({ε 0 } + z{κ }) (7.61) Principles of Composite Material Mechanics 338 where the midplane strains {ε0} and curvatures {κ} are given in terms of laminate forces and moments by Equation 7.59. The lamina stresses from Equation 7.61 can then be used in conjunction with a lamina strength criterion to check each lamina against failure. The analysis of hygrothermal stresses will be discussed later in Section 7.6, and laminate strength analysis will be presented in Section 7.8. 7.5.3 Determination of Laminate Engineering Constants It is sometimes more convenient to use effective laminate engineering constants rather than the laminate stiffnesses deined in Equations 7.41 through 7.43. These effective laminate engineering constants may be derived by using laminate compliances. For example, the force–deformation relationships for a symmetric laminate under in-plane loads only are given by N x A11 N y = A12 N A xy 16 A12 A22 A26 A16 ε 0x A26 ε 0y A66 γ 0xy (7.62) and the corresponding inverted force–deformation relationships are ε 0x A11 ′ 0 ′ ε y = A12 γ 0 A′ xy 16 A12 ′ A22 ′ A26 ′ A16 ′ Nx A26 ′ Ny A66 ′ N xy (7.63) If the symmetric laminate has A16 = A26 = 0 as in Example 7.5, the effective longitudinal Young’s modulus of the laminate, Ex, governs the response of the laminate under the single axial load per unit length Nx with Ny = Nxy = 0 (Figure 7.23a) and is deined as Ex = 2 1 ( A11 A22 − A12 ) σx N x /t = = = ε 0x A11 tA22 ′ N x tA11 ′ (a) t (b) Ny (7.64) (c) Nx t t Nxy FIGURE 7.23 In-plane loading of symmetric laminate for deining the in-plane laminate engineering constants. (a) Applied axial load Nx, (b) applied axial load Ny, and (c) applied shear load Nxy. Analysis of Laminates 339 while the effective transverse Young’s modulus of the laminate, Ey, governs the response of the laminate under the single axial load per unit length Ny with Nx = Nxy = 0 (Figure 7.23b) and is deined as Ey = 2 N y /t σy 1 ( A A − A12 ) = = = 11 22 0 N tA tA ε y A22 ′ y ′ 22 11 (7.65) The effective laminate in-plane shear modulus, Gxy, governs the laminate response under the pure shear load per unit length Nxy with Nx = Ny = 0 (Figure 7.23c) and is deined as Gxy = N xy /t τ xy 1 A = = = 66 N tA t γ 0xy A66 ′ xy ′ 66 (7.66) Similarly, the effective laminate longitudinal Poisson’s ratio is νxy = − A12 A ′ = 12 A11 A22 ′ (7.67) and the effective laminate shear-coupling ratios analogous to those given in Equations 2.41 and 2.42 for the orthotropic lamina are ηx , xy = A16 ′ A11 ′ and ηxy , y = A26 ′ A66 ′ (7.68) Using similar derivations, the effective laminate lexural moduli may be expressed in terms of the lexural compliances. For the symmetric laminate subjected to bending only, the laminate moment–curvature relationships are given by Mx D11 M y = D12 M D xy 16 D12 D22 D26 D16 κ x D26 κ y D66 κ xy (7.69) D16 ′ Mx D26 ′ My D66 ′ Mxy (7.70) and the inverted forms are given by κ x D11 ′ ′ κ y = D12 κ D′ xy 16 D12 ′ D22 ′ D26 ′ Principles of Composite Material Mechanics 340 (a) (b) My b b Mx FIGURE 7.24 Bending moment leading of symmetric laminate for deining the laminate lexural moduli. (a) Applied bending moment Mx and (b) applied bending moment My. Thus, when the laminate is subjected to a pure bending moment per unit length Mx with My = Mxy = 0 (Figure 7.24a), the resulting curvature is κ x = D11 ′ Mx = D11 ′ 1 M = ρx b (7.71) where M is the total bending moment, which is Mxb, b is the laminate width, and the radius of curvature ρx = 1/κx. For an equivalent homogeneous beam, the moment–curvature relationship is M 1 = Efx I yy ρx (7.72) where Iyy is the second moment of inertia of the beam about the neutral axis, which is bt3/12, and Efx is the lexural modulus of the beam along the x-direction. Recall that the lexural modulus was also deined by Equations 7.8 and 7.9, according to the laminated beam theory. Combining Equations 7.71 and 7.72, we ind that the lexural modulus is related to the laminate compliance D11 ′ , by the equation Efx = 12 t D11 ′ 3 (7.73) Similarly, the lexural modulus along the y-direction (Figure 7.24b) is found to be Efy = 12 t 3D22 ′ (7.74) Although the laminate stiffnesses Aij, Bij, and Dij are meaningful parameters for all laminate conigurations, the engineering constants may not be. Analysis of Laminates 341 Clearly, the use of effective engineering constants must be restricted to those cases where the deformations are similar to the deformations associated with the engineering constant being used. That is, in the above examples for symmetric laminates, the Bij = 0 and warping under in-plane loads or midplane extension under bending or twisting moments will not occur, so the deformations of the laminate under load would be similar to those for the equivalent homogeneous material. However, the use of engineering constants for the antisymmetric laminate may not be appropriate because of the complex deformations due to coupling effects. 7.5.4 Comparison of Measured and Predicted Compliances Experimental veriication of the laminate theory can be done by applying known loads to a laminate and by measuring resulting deformations and then comparing measured deformations with those predicted from the laminate theory. Alternatively, the compliances that are formed from ratios of strains to loads or ratios of curvature to moments for certain simple loading conditions can be experimentally determined and compared with predicted values. The latter approach has been used by Tsai [13] who reported results for cross-ply and angle-ply glass/epoxy laminates. Only the results for the angle-ply laminates will be discussed here. In order to determine the compliances of the laminates under various loads, electrical resistance strain gage rosettes with gages oriented at 0° (x-direction), 45°, and 90° (y-direction) were attached on both sides of the test specimens (Figure 7.25). From Equation 7.31, the measured normal strains on the upper surface (where z = −t/2) are related to the corresponding midplane strains and curvatures by t ε Ux = ε 0x − κ x 2 (7.75) Strain gages bonded to laminate 45° y FIGURE 7.25 Strain gage rosette bonded to upper surface of laminate. x 342 Principles of Composite Material Mechanics ε Uy = ε 0y − t ky 2 (7.76) where ε Ux is the measured normal strain along the x-direction on the upper surface and ε Uy is the measured normal strain along y-direction on the upper surface. Similarly, the normal strains on the lower surface (where z = t/2) are given by ε Lx = ε 0x + t κx 2 (7.77) ε Ly = ε 0y + t κy 2 (7.78) where ε Lx is the measured normal strain along the x-direction on the lower surface and ε Ly is the measured normal strain along the y-direction on the lower surface. Equations 7.75 and 7.77 can be solved simultaneously for the midplane strain, ε 0x and curvature, κx, whereas ε 0y and κy can be determined from Equations 7.76 and 7.78. Although the surface shear strains γ Uxy and γ Lxy are not measured directly like the normal strains, they can be determined from the measured strains along 0°, 45°, and 90° and the strain transformation relationships similar to Equation 2.33. For example, from Equation 2.33, the measured normal strain along the 45° direction on the upper surface, ε U45 , is related to the corresponding strains along the x- and y-axes by ε U45 = ε Ux cos 2 θ + ε Uy sin 2 θ + γ Uxy sin θ cos θ (7.79) and substituting θ = 45° and solving for γ Uxy , we ind that γ Uxy = 2ε U45 − (ε Ux + ε Uy ) (7.80) Thus, the shear strain is related to the measured strains on the right-hand side of Equation 7.80. Similarly, for the lower surface, γ Lxy = 2ε L45 − (ε Lx + ε Ly ) (7.81) Now the last part of Equation 7.31 is used to relate the surface shear strains to the midplane shear strains and twisting curvatures: t γ Uxy = γ 0xy − κ xy 2 (7.82) Analysis of Laminates 343 γ Lxy = γ 0xy + t κ xy 2 (7.83) These equations can be solved simultaneously for γ 0xy and κxy, so that all midplane strains and curvatures can be determined from the six measured surface strains. For known loading conditions, the compliances can then be found. For a uniaxial loading-test of such a strain-gaged specimen with Nx ≠ 0 and Ny = Nxy = Mx = My = Mxy = 0 (Figure 7.23a), Equation 7.59 can be used to determine six compliances from known loads, midplane strains, and curvatures as follows: A11 ′ = ε 0x κx , B11 ′ = Nx Nx A12 ′ = ε 0y κy , B12 ′ = Nx Nx A16 ′ = γ 0xy κ xy , B16 ′ = Nx Nx (7.84) Similar data from a pure lexure test, with Mx ≠ 0 and Nx = Ny = Nxy = My = Mxy = 0 (Figure 7.24a) can be used to ind the six compliances: B11 ′ = ε 0x κx , D11 ′ = Mx Mx B12 ′ = ε 0y κy , D12 ′ = Mx Mx B16 ′ = γ 0xy κ xy , D16 ′ = Mx Mx (7.85) All compliances can be determined from such tests. In addition, some compliances can be determined from more than one test (e.g., the Bij in the above tests). A comparison of measured and predicted compliances of angle-ply glass/epoxy laminates having either two or three plies of various lamination angles is shown in Figure 7.26 from Tsai [13]. Predicted compliances were determined by using measured lamina properties as follows [13]: E1 = 7.8 × 106 psi (53.8 MPa) E2 = 2.6 × 106 psi (17.9 MPa) G12 = 1.25 × 106 psii (8.6 MPa) ν12 = 0.25 Principles of Composite Material Mechanics 344 3 –B′16 0.2 –D′12 –A′12 0.1 0 15 30 45 60 75 90 0 15 30 45 60 75 90 0 15 30 45 60 75 90 Lamination angle 0.5 2 1 0 5 0.4 n=3 A′11 0.3 4 D′11 3 B′ij = 0 0.2 –A′12 0.1 0 4 D′16 A′16 2 –D′12 0 15 30 45 60 75 90 0 15 30 45 60 75 90 1 D′ij, (106 lb/in.)–1 B′ij, (106 lb)–1 D′11 A′11 0.3 0 A′ij, (106 lb/in.)–1 5 0.4 D′ij, (106 lb/in.)–1 n=2 0.5 0 Lamination angle FIGURE 7.26 Measured and predicted compliances for glass/epoxy angle-ply laminates for various lamination angles. (Adapted from Tsai, S. W. 1964. Structural behavior of composite materials. NASA CR-71.) The agreement between measured and predicted values in Figure 7.26 is quite favorable, which means that the laminate theory must be reasonably accurate. It is interesting to note that the predicted Bij-type coupling occurs for the two-ply antisymmetric laminate, but not for the three-ply symmetric laminate. Note also that the predicted A16, A26, D16, and D26-type coupling occurs for the three-ply laminate, but not for the two-ply laminate. EXAMPLE 7.9 The symmetric angle-ply laminate described in Example 7.5 is subjected to a single uniaxial force per unit length Nx = 50 MPa mm. Determine the resulting stresses associated with the x- and y-axes in each lamina. Solution Owing to symmetry, [B] = 0 and [A′] = [A*] = [A]−1. Since {M} = 0 here, {ε 0 } = [ A′]{N } = [ A]−1 {N } Using the inverse of the [A] matrix from Example 7.5, we ind that ε 0x 0.04276 0 ε y = −0.0297 γ 0 0 xy −0.0297 0.04276 0 0.002138 0 50 0 0 × (10 −3 ) = −0.001485 0.02809 0 0 Analysis of Laminates 345 where (GPa mm)−1 = 10−3 (MPa mm)−1. Substituting the above strains and the lamina stiffnesses from Example 7.5 in Equation 7.61, we ind that the stresses in the +45° plies are σ x 45.22 σ y = 31.42 τ 32.44 xy 31.42 45.22 32.44 32.44 0.002138 50 3 32.44 −0.001485 × 10 = 0 MPa 21.2 35.6 0 where 103 MPa = GPa. Similarly, the stresses in the −45° plies are σ x 45.22 σ y = 31.42 τ −32.44 xy 31.42 45.22 −32.44 −32.44 0.002138 50 3 −32.44 −0.001485 × 10 = 0 MPa −21.2 35.6 0 Note that since the curvatures vanish for this problem, the stresses do not depend on the distance z. EXAMPLE 7.10 The antisymmetric angle-ply laminate described in Example 7.6 is subjected to a single uniaxial force per unit length Nx = 50 MPa mm. Determine the resulting stresses associated with the x- and y-axes in each lamina. Solution Since this laminate is not symmetric, we must invert the full stiffness matrix as in Equation 7.51 or 7.59. Forming the full stiffness matrix from the [A], [B], and [D] matrices in Example 7.6 and inverting, we ind the resulting midplane strains and curvatures to be ε 0x ε 0y 0.04386 −0.02861 0 0 γ xy = 0 κ x 0 κ y 0 02083 − . κ xy −0.02861 0.04386 0 0 0 0.03284 0 0 −0.02083 −0.02083 −0.02083 0 0.002193 mm/mm 50 −0.001430 mm/mm 0 0 mm/m 0 mm −3 × × 10 = −1 0 mm 0 − 1 0 mm 0 −1 −0.001042 mm 0 0 0 −0.02083 0.52625 −0.34331 0 0 0 −0.02083 0.34331 0.52625 0 −0.02083 −0.02083 0 0 0 0.39356 Principles of Composite Material Mechanics 346 where again the factor of 10−3 has been introduced for dimensional consistency. Due to the curvatures, the total strains and stresses now depend on the distance z (unlike Example 7.9). For example, at the top surface of the #1 ply (−45°), z = −0.5 mm and the resulting total strains are ε x = ε 0 + zκ x = 0.002193 + (−0.5)(0) = 0.002193 mm/mm ε y = ε 0y + zκ y = −0.00143 + (−0.5)(0) = −0.00143 mm/mm γ xy = γ 0 + zκ xy = 0 + (−0.5)(−0.001042) = 0.000521 mm/mm Similarly, at the bottom surface of the #1 ply (−45°) or at the top surface of the #2 ply (+45°), z = −0.25 mm and the strains are ε x = 0.002193 + (−0.25)(0) = 0.002193 mm/mm ε y = −0.00143 + (−0.25)(0) = −0.00143 mm/mm γ xy = 0 + (−0.25)(−0.001042) = 0.000261 mm/mm At the top surface of the #3 ply (−45°) or at the bottom surface of the #2 ply, z = 0 and the strains are ε x = 0.002193 mm/mm ε y = −0.00143 mm/mm γ xy = 0 At the top surface of the #4 ply (+45°) or at the bottom surface of the #3 ply (−45°), z = 0.25 mm and ε x = 0.002193 mm/mm ε y = −0.00143 mm/mm γ xy = −0.000261 mm/mm Finally, at the bottom of the #4 ply (+45°), z = +0.5 mm and ε x = 0.002193 mm/mm ε y = −0.00143 mm/mm γ xy = −0.000521 mm/mm The stresses at the top surface of the #1 ply (−45°) are then Analysis of Laminates 347 σ x 45.22 σ x = 31.42 τ −32.44 xy 31.42 45.22 −32.44 −32.44 0.002193 −32.44 −0.001430 × 10 3 35.6 0.000521 37.3 = −12.7 MPa −6.2 where again 103 MPa = GPa. Similar calculations for the other plies yield the values shown in the following table: Location σx(MPa) #1 Top #1 Bottom #2 Top #2 Bottom #3 Top #3 Bottom #4 Top #4 Bottom 37.3 45.8 62.7 54.2 54.2 62.7 45.8 37.3 σy(MPa) τxy(MPa) −12.7 −4.2 12.7 4.2 4.2 12.7 −6.2 −15.5 34.0 24.7 −24.7 −34.0 15.5 6.2 −4.2 −12.7 Thus, the stress distribution across the thickness of the antisymmetric laminate is quite complex, even for simple uniaxial loading. This is typical for laminates that exhibit coupling. EXAMPLE 7.11 For the symmetric laminate described in Examples 7.5 and 7.9, determine the effective Young’s moduli, in-plane shear modulus, longitudinal Poisson’s ratio, and shear-coupling ratios associated with the x- and y-axes. Solution The effective longitudinal Young’s modulus is given by Equation 7.64 Ex = 1 1 = = 23.4 GPa (1)(0.04276) tA11 ′ Note that due to the ±45° ply orientations for this laminate, Ex = Ey. The effective in-plane shear modulus is given by Equation 7.66: Gxy = 1 1 = = 35.6 GPa (1)(0.02809) tA66 ′ Principles of Composite Material Mechanics 348 The effective longitudinal Poisson’s ratio is given by Equation 7.67: νxy = − A12 −0.0297 ′ =− = 0.694 0.04276 A11 ′ Since A16 = A26 = 0 for this laminate, it is seen from Equation 7.68 that the effective shear-coupling ratios ηx,xy = ηxy,y = 0. Due to the complex coupling effects acting in the antisymmetric laminate of Examples 7.6 and 7.10, the use of engineering constants for such a laminate would be questionable. PROBLEM 7.11 The [+45/−45] laminate described in Problem 7.6 is subjected to a uniaxial force per unit length Nx = 30 MPa mm. Find the resulting stresses and strains in each ply along the x- and y-directions. PROBLEM 7.12 A [0/90]s laminate is subjected to a single bending moment per unit length, Mx. If the laminate is unconstrained, so that bending along both the x- and the y-directions occurs freely, determine the ply stresses, (σx)k, in terms of the moment, Mx, the bending stiffnesses, Dij, the ply stiffnesses, Qij, and the distance from the middle surface, z. Determine the ply stresses (σx)k in terms of Mx, z, and a numerical coeficient if the properties are E1 = 129 GPa, E2 = 12.8 GPa, G12 = 4.6 GPa, ν12 = 0.313, and t = 1 mm. PROBLEM 7.13 The laminate described in Problem 7.12 is subjected to a single bending moment per unit length, Mx, and the two edges on which Mx acts are ixed so that bending along the x-direction occurs freely, but bending along the y-direction is prevented. That is, the longitudinal curvature is unconstrained (i.e., κx ≠ 0), but the transverse curvature is constrained (i.e., κy = 0). Determine the ply stresses (σx)k as in Problem 7.12 (give equations and numerical results) and compare with the results of Problem 7.12. PROBLEM 7.14 A [90/0/90]s laminate is fabricated from laminae consisting of isotropic ibers (Ef = 220 GPa, νf = 0.25) embedded in an isotropic matrix (Em = 3.6 GPa, νm = 0.4). Each lamina is 0.25 mm thick, and the 0.01-mm-diameter ibers have been precoated with a 0.00125-mm-thick sizing, which is the same as the matrix material. The precoated ibers are arranged in the closest possible packing array in the matrix. Using both micromechanics and laminate analysis, ind the laminate engineering constants Ex, Ey, Gxy, and νxy. The laminate x-axis is parallel to the 0° lamina orientation. Analysis of Laminates 349 PROBLEM 7.15 A symmetric [0/90/0] laminate is 0.75 mm thick and its full compliance matrix is given below: A B −1 B A′ = D B′ B′ D′ 0.014 −4 −7.235 × 10 0 = 0 0 0 −7.235 × 10 −4 0.026 0 0 0 0 0 0 0.188 0 0 0 0 0 0 0.213 −0.042 0 0 0 0 −0.042 2.066 0 0 0 0 0 0 4.016 where the units of the matrix are A′ B′ B′ [GPa mm]−1 = D′ [GPa mm 2 ]−1 [GPa mm 2 ]−1 [GPa mm 3 ]−1 Determine the following effective engineering constants for the laminate, giving both magnitude and units; (a) the effective longitudinal Young’s modulus, Ex, (b) the effective transverse Young’s modulus, Ey, (c) the effective in-plane shear modulus, Gxy, (d) the effective longitudinal Poisson’s ratio, νxy, and (e) the effective lexural modulus, Efx. PROBLEM 7.16 The laminate described in Problem 7.15 has laminae that are 0.25 mm thick and the stiffness matrix associated with the 0° lamina is given by 138.8 Q = [ ] 2.7 0 2.7 8.965 0 0 0 GPa 7.1 If a single bending moment per unit length Mx = 0.1 GPa mm2 is applied to the laminate, (a) determine the stresses associated with the x- and y-axes on the top surface of the laminate and (b) determine the stresses associated with the x- and y-axes on the middle surface of the laminate. PROBLEM 7.17 A four ply symmetric [0/90]s laminate has the following ply properties; ply thickness = 0.25 mm; 350 Principles of Composite Material Mechanics E1 = 129 GPa, E2 = 12.8 GPa, G12 = 4.6 GPa, ν12 = 0.313 Determine (a) the lexural modulus of the laminate, Ef, using laminated beam theory and (b) the lexural modulus of the laminate, Efx, using CLT. 7.6 Hygrothermal Effects in Laminates The analysis of hygrothermal behavior of the lamina in Chapter 5 can now be extended to laminates. If we again restrict the discussion to polymer matrix composites, the two main effects of changes in the hygrothermal environment on laminate behavior are degradation of properties and changes in the stress and strain distributions. In this section, the analysis of both these effects along with the prediction of laminate hygrothermal expansion coeficients will be discussed. The basic assumption in all these discussions is that of linearity. That is, we assume that mechanical and hygrothermal effects can be treated separately and then combined using superposition. Coupling between the effects is ignored, as this would lead to nonlinear equations. Another key assumption used here is that temperature and moisture distributions in the laminate are uniform. That is, the temperature and moisture concentration are assumed to be the same for each ply in the laminate. 7.6.1 Hygrothermal Degradation of Laminates The analysis of hygrothermal degradation in laminates involves the combination of the lamina degradation analysis in Section 5.2, with the laminate analysis described earlier in this chapter. For example, given a combination of temperature and moisture, Equation 5.7 can be used to estimate the degraded matrix property, which is then substituted in the appropriate micromechanics equations to estimate the degraded lamina properties such as E1, E2, G12, and ν12. The degraded lamina properties are then used in Equations 7.41 through 7.43 to ind the corresponding degraded laminate stiffnesses. Hygrothermal properties such as the coeficients of thermal expansion and hygroscopic expansion can also be degraded using empirical equations such as Equation 5.41. These properties would then be used to estimate hygrothermal stresses, as shown in the next section. 7.6.2 Hygrothermal Stresses in Laminates In Section 5.3, the analysis of hygrothermal stresses in an isolated lamina due to temperature and moisture was developed. We now consider the corresponding lamina stresses due to interaction with other laminae in the laminate. Hygrothermal stresses are not only generated during the use of composite materials in various environmental conditions, but are also Analysis of Laminates 351 generated during fabrication. The hygrothermal stresses induced by fabrication are usually referred to as residual stresses. Composites are processed or cured at elevated temperatures and then cooled to room temperature. Due to differences between iber and matrix coeficient of thermal expansions (CTEs) in the lamina and differences between lamina CTEs in the laminate, residual stresses of fabrication may occur at both the micromechanical and the macromechanical levels. One particularly important result of residual stresses is that in nonsymmetric laminates the Bij-type coupling can cause residual warping of the cured laminate. In Section 7.5.2, the lamina stresses without hygrothermal effects were found by using Equation 7.61. As shown in Section 5.3, however, when changes in temperature and moisture concentration occur, the total strains in the kth lamina are given by {ε}k = [S ]k {σ}k + {α}k ∆T + {β}k c (7.86) and the resulting stresses are given by {σ}k = [Q]k ({ε}k − {α}k ∆T − {β}k c) (7.87) where the subscript k refers to the kth lamina. As shown in Section 5.3, if the lamina is completely restrained by adjacent laminae, the total strains {ε}k = 0 and the resulting hygrothermal stresses are given by {σ}k = [Q]k (−{a}k ∆T − {β}k c) (7.88) In a laminate, however, the total lamina strains generally do not vanish, but are instead given by {ε}k = {ε 0 } + z{κ } (7.89) and the resulting stresses, including hygrothermal effects, are given by {σ}k = [Q]k ({ε 0 } + z{κ } − {α}k ∆T − {β}k c) (7.90) Following the procedure outlined in Equations 7.35 through 7.45, the resultant laminate forces per unit length are found by integrating Equation 7.90 through the thickness of the laminate: ∫ {N } = {σ}k dz = { } ∫ Q ({ε } + z {κ} − {α} ∆T − {β} c) dz 0 k k { } { } = [ A ] ε 0 + [ B] {κ } − N T − N M k (7.91) Principles of Composite Material Mechanics 352 where the thermal forces due to temperature change are given by N ∑[Q] {α} (z − z ∫ {N } = [Q]k {α}k ∆T dz = (∆T ) T k k k k −1 ) (7.92) k =1 and the hygroscopic forces due to moisture are given by N ∑[Q] {β} (z − z ∫ {N M } = [Q]k {β}k c dz = (c) k k k k −1 ) (7.93) k =1 Similarly, the resultant moments per unit length are ∫ ∫ { M} = {σ}k z dz = [Q]k ({ε 0 } + z{κ } − {α}k ∆T − {β}k c)z dz (7.94) = [B]{ε 0 } + [D][κ ] − { M T } − { M M } where the thermal moments due to temperature changes are ∫ { M T } = [Q]k {α}k ∆Tz dz = ∆T 2 N ∑[Q] {α} (z k k 2 k − zk2−1 ) (7.95) k =1 and the hygroscopic moments due to moisture are given by c { M } = [Q]k {β}k cz dz = 2 M ∫ N ∑[Q] {β} (z k k 2 k − zk2−1 ) (7.96) k =1 Rearranging Equations 7.91 and 7.94, we ind that {N } + {N T } + {N M } = [ A]{ε 0 } + [B]{κ } (7.97) { M} + { M T } + { M M } = [B]{ε 0 } + [D]{κ } (7.98) and or N E A E = M B B ε 0 D κ (7.99) Analysis of Laminates 353 where the total effective forces (mechanical plus hygrothermal) are {N E } = {N } + {N T } + {N M } (7.100) and the total effective moments (mechanical plus hygrothermal) are { M E } = { M} + { M T } + { M M } (7.101) Alternatively, the inverted forms of Equation 7.99 are given by ε 0 A′ = κ C ′ B′ N E D′ M E (7.102) Thus, the lamina stresses for combined mechanical and hygrothermal loading are determined by using a procedure similar to that outlined in Section 7.5.2. That is, the midplane strains and curvatures are determined from the total effective forces and moments, according to Equation 7.102; then the lamina stresses are determined from Equation 7.90. 7.6.3 Laminate Hygrothermal Expansion Coefficients The effective hygrothermal expansion coeficients for the laminate can be calculated directly by combining the deinitions of the coeficients with the appropriate laminate equations. For example, the effective CTE of a laminate along the x-direction is αx = ε 0x ∆T (7.103) For a symmetric laminate with Bij = 0, the midplane strain along the x-direction due to a temperature change ΔT only is given by the irst of Equation 7.102: T ε 0x = A11 ′ N xT + A12 ′ N yT + A16 ′ N xy (7.104) The desired thermal expansion coeficient, αx, is then found by substituting the thermal forces from Equation 7.92 in 7.104 and then by substituting the result in Equation 7.103. It is important to note that this procedure effectively relates the laminate CTE to lamina CTEs, lamina stiffnesses, laminate compliances, and laminate geometry. The temperature change, ΔT, will cancel out since it appears in both the numerator and the denominator. Similar results can be obtained for other thermal and hygroscopic Principles of Composite Material Mechanics 354 expansion coeficients. As with the effective laminate engineering constants, it is appropriate to restrict the use of the effective hygrothermal expansion coeficients to those cases where the deformations are similar to the deformations associated with the particular coeficient being used. For example, it is probably not a good practice to use such coeficients to describe the hygrothermal behavior of a laminate that exhibits signiicant warping due to coupling effects. 7.7 Interlaminar Stresses One of the key limitations of the CLT is that each ply is assumed to be in plane stress in the xy-plane (Figure 7.12), and that interlaminar stresses associated with the z-axis are neglected. Such interlaminar stresses can cause delamination or separation of the laminae, which is a failure mode that we have not previously considered. In this section, three-dimensional (3D) stress analyses that yield the interlaminar stresses will be discussed, and the resulting interlaminar stresses will be used later in a laminate strength analysis. A state of plane stress actually does exist in the laminae of a laminate in regions suficiently far away from geometric discontinuities such as free edges. A 3D elasticity solution by Pipes and Pagano [14] has shown, however, that even in a laminate under simple uniaxial loading (Figure 7.27), there is a “boundary layer” region along the free edges where a 3D state of stress exists, and that the boundary layer thickness is roughly equal to the laminate thickness. The behavior of interlaminar stresses near a free edge in a laminate will be demonstrated here by using the three stress equilibrium equations from the theory of elasticity (Appendix B): ∂σ x ∂τ xy ∂τ xz + + =0 ∂x ∂y ∂z (7.105) ∂τ yx ∂σ y ∂τ yz + + =0 ∂x ∂y ∂z (7.106) ∂τ zx ∂τ zy ∂σ z + + =0 ∂x ∂y ∂z (7.107) For the uniaxially loaded laminate in Figure 7.27, we now consider a region near the free edges, where y = ±b, and assume that the stresses do not vary Analysis of Laminates Free edge 355 z Interface +θ –θ –θ +θ σx y 2b Fiber orientation Free edge 4h0 z θ y σz x τyz τxz σx σy σx τxy FIGURE 7.27 Pipes and Pagano model for analysis of interlaminar stresses in a laminate under uniaxial extension. (From Pipes, R. B. and Pagano, N. J. 1970. Journal of Composite Materials, 4, 538–548. With permission.) along the loading direction (the x-axis). It follows that ∂σx/∂x = 0 and from Equation 7.105, the interlaminar shear stress, τxz(z), is given by z τ xz ( z) = − ∫ − t /2 ∂τ xy dz ∂y (7.108) We now assume that the in-plane shear stress, τxy, has a constant value given by the CLT in the interior regions of the laminae. As we move along the y-direction toward a free edge, however, τxy must decrease to zero at the stress-free surfaces, where y = ±b. Thus, as y → ±b, |∂τxy/∂y| must increase. It follows from Equation 7.108 that τxz must increase from zero in the interior region to a very large value as y → ±b, as shown in Figure 7.28. The region where these rapid changes take place is referred to as the interlaminar stress boundary layer region, as shown in Figure 7.28. From Equations 7.106 and 7.107, respectively, the other interlaminar stresses as z τ yz ( z) = − ∫ − t /2 ∂σ y dz ∂y (7.109) Principles of Composite Material Mechanics 356 Interlaminar stress “boundary layer” Plane stress ∂τxy ∂y = 0 ∂τxy ∂y ÷ 0 ∴τxz = 0 Center of laminate ∴τxz ÷ 0 Free edge τxy τxz y b FIGURE 7.28 Schematic representation of in-plane shear stress and interlaminar shear stress distributions at ply interface. z σ z ( z) = − ∫ − t /2 ∂τ yz dz ∂y (7.110) Pipes and Pagano [14] used a inite difference numerical scheme to solve the three governing ield equations that are generated by combining the full 3D stress equilibrium equations (Appendix B and Equations 7.105 through 7.107), the full 3D off-axis lamina stress–strain relationships (Equation 7.111), σ x C11 σ C y 12 σ z C13 = τ yz 0 τ xz 0 τ xy C16 C12 C22 C23 0 0 C26 C13 C23 C33 0 0 C36 0 0 0 0 0 0 C44 C45 0 C45 C55 0 C16 ε x C26 ε y C36 ε z 0 γ yz 0 γ xz C66 γ xy (7.111) And the full 3D strain–displacement relations (Appendix C and Equation 7.112). εx = γ yz ∂u ∂v ∂w , εy = , εz = ∂x ∂y ∂z ∂v ∂w ∂u ∂w ∂u ∂v = + + , γ xz = , γ xy = + ∂z ∂y ∂z ∂x ∂ y ∂x (7.112) Analysis of Laminates 357 5.00 z 4.50 2h0 4.00 b x 3.50 y h0 b Laminate centerline 2.96 2.50 –6 τ/εx × 10 σ/ε x × 10–6 2.00 1.50 Laminate free edge σx 3.00 b=8h θ = +45° τxy 1.15 1.00 Laminate theory σx/ε x = 2.96 τxy/ εx = 1.15 0.50 τxz σy 0 0 0.25 0.50 y/b 0.75 τyz σz 1.00 FIGURE 7.29 Distribution of all stresses from Pipes and Pagano analysis. (From Pipes, R. B. and Pagano, N. J. 1970. Journal of Composite Materials, 4, 538–548. With permission.) The equations were solved subject to stress-free boundary conditions along the free edges of a four-layer ±45° graphite/epoxy laminate under uniform axial strain, εx. Figure 7.29 shows the complete stress results obtained by Pipes and Pagano [14]. It is important to note that the in-plane stresses σx and τxy from the 3D analysis agree with those predicted by the CLT in the central portion of the laminate, but both stresses drop in the boundary layer region near the free edge. On the other hand, the interlaminar stresses σz, τxz, and τyz are all equal to zero in the central portion of the laminate, but change rapidly near the free edge. The shear stress τxz is the largest of the interlaminar stresses, as it appeared to grow without bound at y/b = 1.0. Pipes and Pagano suspected that a singularity for this stress component exists at the free edge, but it was not possible to prove the existence of such a singularity with the approximate inite difference solution. Analytical proof of the existence of these singularities was published later by Wang and Choi [15,16]. Principles of Composite Material Mechanics 358 The numerical results of Pipes and Pagano [14] for a variety of laminate cross-sectional aspect ratios led to the conclusion that the boundary layer region of 3D stresses extends inward approximately one laminate thickness from the free edge. This conclusion was later veriied experimentally by Pipes and Daniel [17] who used a Moiré technique to measure displacements along the x-direction on the surface of the laminate. The measured surface displacement proiles, which also clearly indicated the presence of the boundary layer, agreed closely with those predicted by the Pipes and Pagano analysis. It has been shown both analytically and experimentally that the lamina-stacking sequence inluences interlaminar stresses and, consequently, delamination in laminates. Pipes and Pagano [18] used an approximate elasticity solution to study the effect of the stacking sequence on the interlaminar shear stress in ±45° laminates, as shown in Figure 7.30. It is clear from Figure 7.30 that when layers having the same orientation are stacked together (which increases the apparent layer thickness), the interlaminar shear stress, τxz is higher than for the case where layers of opposite orientation are stacked together. In a separate paper, Pagano and Pipes [19] showed that a change in the stacking sequence can actually cause the interlaminar normal stress, σz, to change from tensile to compressive. Since tensile interlaminar normal stresses would tend to cause separation of the plies, whereas compressive interlaminar normal stresses would tend to keep the plies together, stacking sequences that produce the former stress state should have lower strengths 2.50 (17.24) z 1.50 (10.34) z/h0 = 2.0 B [45/–45/45/–45]s z/h0 = 3.0 ∋ 1.00 (6.89) τxz,/ A [45/45/–45/–45]s x y b × 10–6 psi (GPa) 2.00 (13.79) h b x b/h0 = 16 0.50 (3.45) A B 0 0.25 0.50 0.75 0 1.00 y/b FIGURE 7.30 Effect of stacking sequence on interlaminar shear stress. (From Pipes, R. B. and Pagano, N. J. 1974. Journal of Applied Mechanics, 41, Series E (3), 668–672. Reprinted by permission of The American Society of Mechanical Engineers.) Analysis of Laminates 359 than those producing the latter stress state. Experimental results such as those by Whitney and Browning [20] and Whitney and Kim [21] seem to support this conclusion. Ply orientation also has a strong effect on interlaminar stresses, as shown by Pipes and Pagano [14]. Since the publication of the Pipes and Pagano solution, a number of investigators have used other methods to study the “free-edge” interlaminar stress phenomenon. Rybicki [22], Wang and Crossman [23], Herakovich [24], and Hwang and Gibson [25] all used 3D inite element analyses to investigate interlaminar stresses. The quarter-domain inite element model used by Hwang and Gibson [25] for the analysis of the original Pipes and Pagano [14] laminate is shown in Figure 7.31. Finite element stress distributions near the free edge from Wang and Crossman [23] and Hwang and Gibson [25] are compared with those from an empirical solution derived from the theory of elasticity by Hwang [26] in Figure 7.32. The empirical elasticity solution by Hwang [26] is based on a similar solution by Whitney [27], which, in turn, is an attempt to it the inite difference results of Pipes and Pagano [14] with relatively simple empirical equations that satisfy the stress equilibrium equations (Equations 7.105 through 7.107) and the freeedge boundary conditions. Thus, the empirical results shown by the solid curve in Figure 7.32 should be very close to the original Pipes and Pagano results. Although the stress distributions from the two inite element models show good agreement with each other, both sets of stresses are seen to be greater than those from the empirical solution near the free edge. Improved approximate polynomial solutions have been proposed by Conti and De Paulis [28]. Note: w/t = 4 l/t = 4 l/2 +θ Ply interface −θ w σx t/2 y z Laminate middle surface x FIGURE 7.31 Quarter-domain inite element model of laminate used by Hwang and Gibson to analyze the Pipes–Pagano problem. (Reprinted from Composite Structures, 20, Hwang, S. J. and Gibson, R. F., Contribution of interlaminar stresses to damping in thick composites under uniaxial extension, 29–35, Copyright (1992), with permission from Elsevier.) Principles of Composite Material Mechanics 360 4 30 22.5 3 2 τxy Ref. (7.25) Ref. (7.23) Ref. (7.26) 15 1 1.5 Stress amplitude (Gpa) Stress amplitude (Msi) σx τxz 0 0 0.5 2 2.5 3 3.5 1 1.5 Normalized y coordinate (y/h) 4 FIGURE 7.32 Comparison of stress distributions near the free edge. (Reprinted from Composite Structures, 20, Hwang, S. J. and Gibson, R. F., Contribution of interlaminar stresses to damping in thick composites under uniaxial extension, 29–35, Copyright (1992), with permission from Elsevier.) 7.8 Laminate Strength Analysis Recall that in Section 4.2, we discussed several multiaxial strength criteria for estimating the strength of individual laminae under in-plane stresses. Such strength criteria can also be used on a ply-by-ply basis for a laminate to determine which ply fails irst under in-plane loads. In Section 7.7, however, we have seen that interlaminar stresses in laminates also have to be taken into account because they may lead to a different mode of failure known as delamination. This section deals with the analysis of both irst ply failure due to in-plane stresses and delamination due to interlaminar stresses. The mechanical behavior of the laminate after irst ply failure and subsequent ply failures is also discussed. 7.8.1 First Ply Failure and Subsequent Ply Failures Due to In-Plane Stresses The prediction of irst ply failure due to in-plane stresses is a straightforward application of the appropriate multiaxial lamina strength criterion in combination with the lamina stress analysis from the CLT. The loads corresponding to irst ply failure are not necessarily the laminate failure loads, however, since a laminate generally has plies at several orientations. That is, there will usually be a sequence of ply failures at different loads culminating Analysis of Laminates Load 361 Nx(3) Third ply failure, k = 3 Second ply failure, k = 2 Nx(2) Ultimate laminate failure Nx Total First ply failure, k = 1 Nx(1) n=1 n=2 n=3 εx(1) εx(2) εx(3) εxTotal FIGURE 7.33 Idealized load–strain curve for uniaxially loaded laminate showing multiple sequential ply failures leading up to ultimate laminate failure. in ultimate laminate failure when all plies have failed. Thus, the ultimate load-carrying capacity of the laminate may be signiicantly higher than the irst ply failure load, and prediction of laminate failure based on irst ply failure may be too conservative. In the analysis of irst ply failure and subsequent ply failures, the stiffness matrices for the failed plies and the corresponding laminate stiffness matrix must be modiied after each ply failure to relect the effects of those failures. Figure 7.33 shows an idealized piecewise linear laminate load– deformation curve with several “knees” due to ply failures. The total forces and moments at the kth knee in the curve are related to the corresponding forces and moments for the nth section of such a curve (where n ≤ k) by the summation N = M Total k ∑ n =1 N ( n ) ( n) M (7.113) where the superscript (n) on a parameter denotes the particular value of that parameter associated with the nth section. The corresponding midplane strains and curvatures are given by ε 0 = κ Total k ∑ n =1 ε 0( n ) ( n) κ (7.114) Principles of Composite Material Mechanics 362 Using the piecewise linear assumption, the load–deformation relationship for the nth section can be approximated by modifying Equation 7.45 as (n) (n) N A (n) = (n) M B B( n ) ε 0( n ) D( n ) κ ( n ) (7.115) where the [A(n)], [B(n)], and [D(n)] are the modiied stiffness matrices after the (n − 1)th ply failure. But the calculation of these modiied laminate stiffnesses requires that we know the modiied ply stiffnesses, [Q (n)], and before we can modify the ply stiffness matrices, we must know the type of failure. That is, if the ply failure is caused by the in-plane shear stress exceeding the shear strength, the shear modulus and the transverse modulus of that ply may be severely degraded by longitudinal cracks, but the longitudinal modulus may not be affected signiicantly by these cracks. Alternatively, all the ply stiffnesses for the failed ply could be equated to zero or some very small number in the calculation of the degraded laminate stiffnesses. Halpin [12] has used a procedure similar to the one outlined above to analyze the uniaxial stress–strain response of a [0/±45/90]s glass/epoxy laminate. The maximum strain criterion was used to predict ply failure, and the ply stiffnesses of the failed plies were set equal to zero. The predicted stress– strain curve shows good agreement with the corresponding experimental data, as shown in Figure 7.34. Notice that the curve has two “knees”—the irst one at the strain corresponding to failure of the 90° plies and the second one at the strain corresponding to failure of the ±45° plies. The knee for the ±45° ply failure is more distinct than the one for the 90° ply failure, because σ (ksi) 50 40 Quasi-isotropic glass-epoxy ±45° 30 20 90° 10 0 0 0.01 0.02 ε (in/in.) 0.03 FIGURE 7.34 Comparison of predicted and measured stress–strain response of [0/±45/90]s glass/epoxy laminate. (From Halpin, J. C. 1984. Primer on Composite Materials: Analysis. Technomic Publishing Co., Lancaster, PA. With permission.) Analysis of Laminates 363 the laminate has twice as many ±45° plies as it does 90° plies. Ultimate laminate failure occurs at the longitudinal failure strain for the 0° plies. It is also interesting to note that the experimental data do not show as much of a change in slope at the knees as the theoretical curve does. This may be due to the fact that actual ply failure occurs gradually over a inite strain range, whereas instantaneous ply failure at a single strain level is assumed in the analysis. The same reasoning may explain the absence of jumps in the stress–strain curve after ply failure [29]. A horizontal jump would be predicted if the test data were taken under load-control, whereas a vertical jump would be predicted for a displacement-control test. Hahn and Tsai [29] have observed that the knee in the stress–strain curve for cross-ply laminates is quite obvious if the 90° plies are all stacked adjacent to each other, but the knee is not so obvious if the 0° and 90° plies are arranged in an alternating 0°/90° sequence. Restraint of the failed 90° plies by the remaining 0° plies was thought to be more effective in the alternating 0°/90° sequence, making the failure of the 90° plies more gradual. The in-plane strength of ±θ angle-ply laminates may also be analyzed using a multiaxial lamina strength criterion and the CLT, but the piecewise linear approximation of the stress–strain curve may not be needed. This is because if the lamina tensile and compressive strengths are equal, all plies fail simultaneously in the angle-ply laminate, and the stress–strain curve does not have the characteristic knees shown in Figures 7.33 and 7.34. Tsai [30] has used the Tsai–Hill criterion to predict the strength of glass–epoxy angle-ply laminates as a function of the lamination angle θ, and the predictions are seen to agree well with experimental data in Figure 7.35. The predicted laminate stiffness A11 also shows good agreement with the prediction from the CLT in Figure 7.35. 7.8.2 Delamination Due to Interlaminar Stresses Delamination due to interlaminar stresses can reduce the failure stress of the laminate below that was predicted by the in-plane failure criteria discussed in the previous section. Failure by delamination is not necessarily the same as the initiation of delamination, however. The initiation of delamination is generally followed by stable delamination growth, which eventually leads to unstable growth and ultimate failure. The onset of delamination can be predicted by using either mechanics of materials approaches or fracture mechanics approaches. Fracture mechanics is also the preferred analytical treatment for delamination growth and failure. In this section, we will discuss mechanics of materials approaches to the prediction of delamination initiation, and fracture mechanics will be covered in Chapter 9. The average stress criterion of Kim and Soni [31] was one of the irst mechanics of materials approaches to the prediction of the onset of delamination. This criterion is based on the premise that delamination will begin Principles of Composite Material Mechanics Uniaxal strength Nx/h (ksi) Uniaxal stiﬀness (106 psi) 364 10 7 4 2 Nx/h +θ −θ 100 70 Angle-ply 40 Nx/h 20 10 7 4 2 1 0 15 30 45 60 75 90 Lamination angle θ (degrees) FIGURE 7.35 Comparison of predicted and measured uniaxial strength and stiffness of glass/epoxy angleply laminates. (From Tsai, S. W. 1965. Strength characteristics of composite materials. NASA CR-224.) once the average value of the interlaminar tensile normal stress, σ z , near the free edge reaches the interlaminar tensile strength, sZ( + ) . A similar criterion for failure of notched laminates had been proposed previously by Whitney and Nuismer [32]. In the Kim–Soni criterion, the averaging is done over a critical length, b0, as shown in Equation 7.116 and Figure 7.36: Interlaminar normal stress (σz) Laminate centerline σ− z Free edge b0 y b FIGURE 7.36 Graphical interpretation of average interlaminar normal stress near free edge, according to the Kim–Soni criterion. Analysis of Laminates 365 1 σz = b0 b ∫ σ (y, 0) dy = s (+ ) Z z (7.116) b − b0 The distance b was the half-width of the laminate, as shown in Figure 7.27, and the critical length b0 is assumed to be equal to one ply thickness. Due to the dificulty of measuring sZ( + ) , Kim and Soni assumed that sZ( + ) = sT( + ) . Although this criterion provided reasonably accurate predictions of the onset of delamination in composites, where the tensile normal stress, σz, was the dominant interlaminar stress, a more general criterion was needed for cases, where delamination may be affected by interlaminar shear stresses as well. The need for a more general criterion for predicting the onset of delamination was recognized by Brewer and Lagace [33], who proposed the quadratic delamination criterion: 2 2 2 2 σ xz σ yz σ tz σ cz s + s + s + s = 1 Z Z XZ YZ (7.117) where σ xz and σ yz are the average interlaminar shear stresses, σ tz and σ cz are the average interlaminar tensile and compressive normal stresses, respectively, SXZ and SYZ are the interlaminar shear strengths, and sZ( + ) and sZ( − ) are the interlaminar tensile and compressive strengths, respectively. Each of the average stress components in this case is deined as σ ij = 1 λ avg λ avg ∫ σ dλ ij (7.118) 0 where λ is the distance from some reference point (in this case the free edge), λavg is the averaging dimension, σij is the stress component σxz, σyz, σ tz , or σ cz , and the overbar denotes its average value. Brewer and Lagace found that for the [±15n]s, [±15n/0n]s, and [0n/±15n]s, AS1/3501-6 carbon/epoxy laminates tested the second and fourth terms in Equation 7.117 were negligible, so that the quadratic delamination criterion took on the simpliied form 2 2 σ xz σ tz s + s( + ) = 1 z XZ (7.119) Transverse isotropy was assumed, so that sZ( + ) = sT( + ) = 53.9 MPa. The parameters λavg and sXZ were used as curve-itting parameters to obtain the best Principles of Composite Material Mechanics 366 agreement with experimental data. In the corresponding experiments, laminate specimens were tested under displacement control, and an instantaneous drop in the tensile load at delamination onset was observed. The “best-it” parameters for all laminate conigurations tested were λavg = 0.178 mm and sXZ = 105 MPa. Further support for the validity of the quadratic delamination criterion and the assumption of transverse isotropy was discovered with the observation that the best-it value of sXZ was the same as sLT, the in-plane shear strength of this material. Although the value of λavg was not assumed to be equal to the ply thickness as in the Kim–Soni analysis, the best-it value of 0.178 mm was of the same order as the ply thickness. A comparison of the measured and predicted delamination onset stresses for various normalized ply thicknesses, n, are shown for the [±15n]s laminate in Figure 7.37. Specimens were made by stacking single plies of the same orientation together to form a ply with greater effective thickness, and the value of n is this effective ply thickness divided by the single ply thickness. Also shown in Figure 7.37 are the predictions from a fracture mechanics approach, which will be discussed later. Catastrophic failure of laminated structures is not the only undesirable result of delamination. The reduction in stiffness of a laminate during delamination growth may make the structure unsafe even if fracture does not occur. Conversely, stiffness loss can be used to characterize the growth of delamination. Thus, analytical models are needed for estimating this stiffness loss during delamination. Delamination initiation stress (MPa) 1000 [±15n]s Data QDC 800 Gc approach 600 400 200 1 2 3 4 5 6 Normalized eﬀective ply thickness (n) FIGURE 7.37 Predicted and measured delamination initiation stresses for [+15n]s laminates. (From Brewer, J. C. and Lagace, P. A. 1988. Journal of Composite Materials, 22, 1141–1155. With permission.) Analysis of Laminates 367 O’Brien [34] has developed an analysis of stiffness reduction in symmetric laminates during delamination based on a simple “rule of mixtures” and the CLT. Recall from Equation 7.64 that the effective longitudinal Young’s modulus of a symmetric laminate is given by Ex = 1 tA11 ′ (7.120) This equation was used by O’Brien to model the stiffness of the laminate without delaminations, as shown in Figure 7.38a. The corresponding stiffness of a laminate, which has been totally delaminated along one or more interfaces (Figure 7.38b), but whose sublaminates must still have the same longitudinal strain, is given by the rule of mixtures formula Etd = ∑ im=1 Exiti t (7.121) where Etd is the longitudinal Young’s modulus of a laminate totally delaminated along one or more interfaces, Exi is the longitudinal Young’s modulus of ith sublaminate formed by the delamination, ti is the thickness of the ith sublaminate, and m is the number of sublaminates formed by the delamination. The longitudinal Young’s modulus of a laminate that has been partially delaminated along the same interfaces (Figure 7.38c) is given by the rule of mixtures formula (b) (a) (c) t ti a b FIGURE 7.38 Rule of mixtures analysis of stiffness loss due to delamination. (a) Laminated, (b) totally delaminated, and (c) partially delaminated. (From O’Brien, T. K. 1982. In Reifsnider, K. L. ed., Damage in Composite Materials, ASTM STP 775, pp. 140–167. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. With permission.) Principles of Composite Material Mechanics 368 a E = (Etd − Ex ) + Ex b (7.122) where E is the longitudinal Young’s modulus of a laminate partially delaminated along one or more interfaces, a is the distance that delamination extends in from the free edge and b is the half-width of the laminate. A more general form of Equation 7.122 is given by Equation 7.123: E = (Etd − Ex ) Ad + Ex At (7.123) where Ad is the delaminated area and At the total interfacial area. The predicted values of E normalized to the initial modulus, E0, are compared with measured values of E/E0 for various delamination sizes in [±30/±30/90/90]s graphite/epoxy laminates in Figure 7.39, and the agreement is seen to be excellent. As shown in Figure 7.39, complete delamination of this laminate would result in a 25.8% reduction in the laminate stiffness. Such a loss of stiffness would lead to an undesirable increase in the delection of the structure under load. In this section, we have only been concerned with delamination near free edges in laminates, but interlaminar stresses and delamination may occur at other discontinuities such as holes, ply drops, and joints (see Figure 7.40 from Reference 35). Low-velocity impact (e.g., dropping a wrench) on a composite structure may cause internal delaminations that may reduce the in-plane compressive strength (Figure 7.41). The so-called “compression after impact” 1.0 0.8 ROM analysis E 0.6 E0 0.4 Data from four specimens 0.2 0 0.2 0.4 0.6 0.8 1.0 a b FIGURE 7.39 Predicted and measured laminate stiffness as a function of delamination size. (From O’Brien, T. K. 1982. In Reifsnider, K.L. ed., Damage in Composite Materials, ASTM STP 775, pp. 140–167. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. Reprinted with permission.) Analysis of Laminates Free edge 369 Notch (hole) Ply drop Bond joint Bolted joint FIGURE 7.40 Interlaminar stresses occur at a variety of discontinuities in composite structures. (From Newaz, G. M. ed. 1991. Delamination in Advanced Composites. Technomic Publishing, Co., Lancaster, PA. With permission.) Impact force Internal delamination caused by impact In-plane compressive loading after impact causes local buckling and reduction of compressive strength FIGURE 7.41 Reduction of in-plane compressive strength of laminate after transverse impact. (CAI) problem is of considerable interest, and CAI testing will be discussed later in Chapter 10. The analysis of delamination under such complex states of stress generally requires the use of fracture mechanics and inite element numerical approaches, some of which are discussed in Chapter 9. The reader is also encouraged to refer to numerous analytical and experimental studies in several recent books [35–37]. There is obviously a lot of interest in the improvement of delamination resistance in laminates, and a number of such approaches will be discussed later in Chapter 9. EXAMPLE 7.12 The antisymmetric angle-ply laminate described in Example 7.6 is heated from 20°C (68°F) to 100°C (212°F). Assuming that the lamina properties do not change over this temperature range, determine the hygrothermal stresses. Principles of Composite Material Mechanics 370 Solution From Table 5.3, the lamina CTEs associated with the principal material axes are α 1 = 0.88 × 10 −6 /°C, α 2 = 31.0 × 10 −6 /°C The CTEs associated with the +45° and −45° lamina orientations are found by using the transformations in Equation 5.22: αx 0.5 = 0.5 αy α /2 xy +45° 0.5 0.5 0.5 −0.5 −1.0 0.88 15.94 1.0 31.0 × 10 −6 = 15.94 × 10 −6 /°C 0 0 −15.06 αx 0.5 = 0.5 αy α /2 xy −45° −0.5 0.5 0.5 0.5 1.0 0.88 15.94 −1.0 31.0 × 10 −6 = 15.94 × 10 −6 /°C 15.06 0 0 Next, the thermal forces due to temperature change are found by substituting the above values and the lamina stiffnesses from Example 7.5 into Equation 7.92. Note also that the third element in column vector {α}k in Equation 7.92 is αxy, not αxy/2 as in the above transformations. Since zk − zk−1 = t/4 for all laminae, t {N T } = ([Q]+45° {α}+45° + [Q]−45° {α}−45° )2(∆T ) 4 or N xT 45.22 T N y = 31.42 N T 32.44 xy 45.22 + 31.42 −32.44 31.42 45.22 32.44 32.44 15.94 32.44 15.94 (10 −6 )(2)(80)(0.25) 35.6 −30.12 31.42 45.22 −32.44 −32.44 15.94 −32.44 15.94 (10 −6 )(2)(80)(0.25) 35.6 30.12 1.956 = 1.956 × 10 −2 GPa mm 0 Similarly, the thermal moments are found from Equation 7.95 as { M T } = ([Q]−45° {α}−45° ( z12 − z02 ) + [Q]+45° {α}+45° ( z22 − z12 ) + [Q]−45° {α}−45° ( z32 − z22 ) + [Q]+45° {α}+45° ( z42 − z32 )) ∆T 2 Analysis of Laminates 371 or MxT 0 T 2 −4 M y = 0 × 10 GPa mm M T −3.81 xy From Equations 7.100 and 7.101, we have {NE} = {NT} and {ME} = {MT}. Using these results along with the compliances from Example 7.10 in Equation 7.102, we ind that the midplane strains and curvatures are ε 0x 3.06 mm/mm 0 ε y 3.06 mm/mm γ 0xy 0 mm/mm −4 × 10 = −1 0 mm κ x κ y 0 mm −1 −1 κ xy −9.65 mm T Note that the thermal twisting moment, Mxy , causes a corresponding twisting curvature, κxy, which means that the laminate will warp under the temperature change. Stresses along the x- and y-axes are now found by substituting the above midplane strains and curvatures, along with the lamina stiffnesses from Example 7.5, in Equation 7.90. Stresses at the top and bottom of each ply are given in the following table: Location #l Top #1 Bottom #2 Top #2 Bottom #3 Top #3 Bottom #4 Top #4 Bottom σx (MPa) σy (MPa) −11.8 −3.9 11.8 3.9 3.9 11.8 −11.8 −3.9 11.8 3.9 3.9 11.8 −3.9 −11.8 −3.9 −11.8 τxy (MPa) −5.7 −14.3 31.6 23.0 −23.0 −31.6 14.3 5.7 As with Example 7.10, the stress distribution is quite complex because of the coupling effect. EXAMPLE 7.13 A [90/0/90]s laminate consisting of the AS/3501 laminae described in Example 7.5 is subjected to tensile uniaxial loading along the x-direction. Using the maximum strain criterion, ind the loads corresponding to irst ply failure and subsequent ply failures; then plot the load–strain curve up to failure. Principles of Composite Material Mechanics 372 Solution The failure strains are found by substituting the data from Tables 2.2 and 4.1 in Equation 4.1: eL( + ) = 1448 sL( + ) = = 0.0105 E1 138 × 10 3 eT( + ) = 48.3 sT( + ) = 0.0054 = 9 × 10 3 E2 Using these results in the maximum strain criterion, we see that irst ply failure occurs at a strain ε x = eT(+ ) = 0.0054. In order to ind the corresponding load Nx at irst ply failure, it is necessary to ind the initial laminate stiffness matrix [A(1)]. From Example 7.5, the lamina stiffness matrix for the 0° plies is given by 138.8 [Q]0° = [Q] = 2.72 0 2.72 9.05 0 0 0 GPa 6.9 The stiffness matrix for the 90° plies is formed by simply interchanging the 11 and 22 terms in the stiffness matrix for the 0° plies: [Q]90° 9.05 = 2.72 0 2.72 138.8 0 0 0 GPa 6.9 For the irst section of the load–strain curve, the laminate stiffness matrix is therefore [ A(1) ] = [Q]0° (2)(0.25) + [Q]90° ( 4)(0.25) = 0.5[Q]0° + [Q]90° or 78.45 [ A ] = 4.08 0 (1) 4.08 143.3 0 0 0 GPa mm 10.35 At irst ply failure, the laminate load–deformation equations can be written as N x 78.45 0 = 4.08 0 0 4.08 143.3 0 0 0.0054 0 εy 10.35 γ xy Analysis of Laminates 373 These equations can be solved simultaneously to get the following values of loads and strains at irst ply failure: N x(1) = 0.423 GPa mm ; ε(y1) = −0.000154; γ (xy1) = 0 We will now demonstrate two different approaches for modifying the laminate stiffness matrix after irst ply failure. a. In the irst approach, we simply set all ply stiffnesses equal to zero for the failed 90° plies. The adjusted laminate stiffness matrix is then 69.4 [ A( 2) ] = 0.5[Q]0° = 1.36 0 1.36 4.52 0 0 0 GPa mm 3.45 Now the 0° ply failure and the ultimate laminate failure occurs at a strain level ε x = eL(+ ) = 0.0105, which means that the strain increment for the second section of the load–strain curve is ε(x2) = eL( + ) − ε(x1) = 0.0105 − 0.0054 = 0.0051 The load–deformation equations describing the second section of the load–strain curve are N x( 2) 69.4 0 = 1.36 0 0 1.36 4.52 0 0 0.0051 0 ε(y2) 3.45 γ (xy2) and the simultaneous solution of these equations yields the results N x( 2) = 0.352 GPa mm ; ε(y2) = −0.00153; γ (xy2) = 0 The total laminate failure load is then N xTotal = N (1) + N ( 2) = 0.423 + 0.352 = 0.775 GPa mm and the load–strain curve is shown as curve (a) in Figure 7.42. b. In the second approach, we set only E2 = G12 = ν21 = 0 for the failed 90° plies, but we assume that E1, for the 90° plies is not affected by the transverse failure. According to these assumptions, [Q22 ]90° = E1 = 138 GPa; [Q11 ]90° = [Q12 ]90° = [Q66 ]90° = 0 Principles of Composite Material Mechanics Nx (GPa-mm) 374 Not to scale 0.777 0.775 (b) (a) 0.423 0.0054 0.0105 εx FIGURE 7.42 Predicted load-strain curves for Example 7.13. (a) All ply stiffnesses equal to zero for failed 90° plies, and (b) E2 = G12 = ν21 = 0, E1 ≠ 0 for failed 90° plies. and the adjusted laminate stiffness matrix is 69.4 [ A( 2) ] = 1.36 0 1.36 142.52 0 0 0 GPa mm 3.45 The laminate load–deformation equations for the second section are N x( 2) 69.4 0 = 1.36 0 0 1.36 142.52 0 0 0.0051 0 ε(y2) ( ) 2 3.45 γ xy and the resulting loads and strains for the second section are N x( 2) = 0.354 GPa mm ; ε(y2) = −0.0000487 ; γ (xy2) = 0 The total load at laminate failure is N xTotal = 0.423 + 0.354 = 0.777 GPa mm and the load–strain curve is shown as curve (b) in Figure 7.42. It is interesting to note that although the assumptions regarding degradation of the failed plies are quite different for curves (a) and (b), the predicted load–strain curves for the two approaches are virtually the same. In general, differences in predictions from the two approaches would depend on ply properties and stacking sequences. It is also interesting to note Analysis of Laminates 375 that we might intuitively expect approach (a) to be more conservative than approach (b) and this turns out to be the case. EXAMPLE 7.14 Repeat Example 7.13 using the maximum stress criterion. Solution From Example 7.13, the load–strain relationship for the irst increment is ε(x1) 78.45 N x(1) (1) (1) 0 = A ε y = 4.08 0 γ (1) 0 xy 0 ε(x1) 0 ε(y1) GPa mm 10.35 γ (xy1) 4.08 143.3 0 Note that, unlike Example 7.13 where, according to the maximum strain criterion, the irst ply failure strain along the x-direction was known to be the transverse tensile failure strain in the 90° plies, we do not know the corresponding strains here, and we must ind them using the maximum stress criterion. Expanding the above equation, N x(1) = 78.45ε(x1) + 4.08ε(y1) 0 = 4.08ε(x1) + 143.3ε(y1) 0 = 10.35γ (xy1) Solving these equations simultaneously, ε(y1) = −0.0285ε(x1) γ (xy1) = 0 N x(1) = 78.33ε(x1) So for the irst ply failure of the 90° plies, the stresses along the x- and y-axes are σ (x1) (1) σ y τ(1) xy 90° 9.05 ε(x1) (1) = [Q]90o −0.0285ε x = 2.72 0 0 8.972ε(x1) = −1.2358ε(x1) GPa 0 2.72 138.8 0 0 ε(x1) (1) 0 −0.0285ε x 6.9 0 Principles of Composite Material Mechanics 376 The corresponding stresses in the 90° plies along the principal material axes are σ (11) (1) σ 2 τ(1) 12 90° 8.972ε(x1) 0 = [T ]90° −1.2358ε(x1) = 1 0 0 1 0 0 0 8.972ε(x1) 0 −1.2358ε(x1) −1 0 −1.2358ε(x1) = 8.972ε(x1) GPa 0 Applying the maximum stress criterion for the 90° plies, we ind that σ 1(1) = −1.2358ε(x1) = −SL( − ) = −1172 MPa = −1.172 GPa or σ (21) = 8.972ε(x1) = ST( + ) = 48.3 MPa = 0.0483 GPa ε(x1) = 0.00538 or ε(x1) = 0.94837 Choosing the smallest of these failure strains, we ind that for irst ply failure, we have ε (x1) = 0.00538 ε (y1) = −0.0285ε (x1) = −0.0285 (0.00538 ) = −0.000153 N x(1) = 78.33ε (x1) = 78.33 (0.00538 ) = 0.4216 GPa mm The corresponding stresses in the 0° plies at irst ply failure are ε(x1) 138.8 σ (x1) (1) (1) σ y = [Q]0° ε y = 2.72 γ (1) 0 τ(1) xy xy 0° σ 1(1) = σ (21) τ(1) 12 2.72 9.05 0 0 0.00538 0.746 0 −0.0001533 = 0.0132 GPa 0 6.9 0 0° For the second increment after irst ply failure, setting all the ply stiffnesses equal to zero for the failed 90° plies and using the corresponding degraded laminate stiffness matrix from Example 7.11, we ind that Analysis of Laminates 377 ε(x2) 69.4 N x( 2) ( 2) ( 2) 0 = [ A ] ε y = 1.36 0 γ ( 2) 0 xy 1.36 4.52 0 0 ε(x2) m 0 ε(y2) GPa mm ( ) 2 3.45 γ xy Solving these equations simultaneously, ε(y2) = −0.3ε(x2) N x( 2) = 68.992ε(x2) γ (xy2) = 0 The incremental stresses for the 0° plies are then ε(x2) 138.8 σ (x2) ( 2) ( 2) σ y = [Q]0° ε y = 2.72 γ ( 2) 0 τ( 2) xy xy 0° σ (12) = σ (22) τ( 2) 12 2.72 9.05 0 0 ε(x2) 137.98ε(x2) 0 −0.3ε(x2) = 0.005ε(x2) GPa 6.9 0 0 0° Substituting the total stresses in the 0° plies at the end of the second increment in the maximum stress criterion, (σ1 )total = σ(11) + σ(12) = 0.746 + 137.98ε(x2) = SL( + ) = 1.448 GPa or ε(x2) = 0.00508 (σ 2 )total = σ(21) + σ(22) = 0.0132 + 0.005ε(x2) = ST( + ) = 0.0483 GPa or ε(x2) = 7.02 Choosing the smallest of the incremental strains to cause failure of the 0° plies, ε(x2) = 0.00508 N x( 2) = 68.992(0.00508) = 0.3505 GPa mm The total loads and strains at inal failure are then ( N x )total = N x(1) + N x( 2) = 0.4216 + 0.3505 = 0.7721 GPa mm (ε x )total = ε(x1) + ε(x2) = 0.00538 + 0.00508 = 0.01046 Principles of Composite Material Mechanics 378 Nx (GPa mm) 0.7721 0.4216 0.00538 0.01046 εx FIGURE 7.43 Predicted load–strain curve for Example 7.14. The resulting load strain plot in Figure 7.43 is seen to be quite similar to the corresponding plots for the maximum strain criterion in Figure 7.42, but this is not necessarily the case in general. EXAMPLE 7.15 The composite power transmission shaft shown in Figure 7.44 has mean radius R = 50 mm and wall thickness t = 1 mm. The material is ilamentwound AS/3501 carbon/epoxy, and the wall of the shaft has a symmetric angle-ply [+45/−45/−45/+45] lay-up sequence (same as the material in Example 7.5) for maximum torsional stiffness. Determine the largest torque T that can be transmitted by the shaft without failure, according to the maximum stress criterion. Solution From the mechanics of materials, the torsional shear stress in a thinwalled tube is approximately τ xy = T 2πR 2t +θ –θ FIGURE 7.44 Composite shaft for Example 7.15. T Analysis of Laminates 379 where T = torque in N m, R = mean wall radius in m, and t = wall thickness in m. For the laminate analysis, the loads per unit length acting on an element of the tube wall are therefore N xy = τ xy t = N T T = = 63.66T = 63.66(10 −6 )T GPa mm m 2πR 2 2π(0.05)2 N x = N y = Mx = M y = Mxy = 0 As in Example 7.9, we can take advantage of the symmetry of the laminate and invert the [A] matrix to solve for the strains in terms of the loads as ε 0x 0 0.04276 0 ε y = [ A′ ] 0 = −0.0297 N 0 γ 0 xy xy −0.0297 0.04276 0 0 0 0 0 6 − 0.02809 63.66(10 )T 0 = 0 − 6 1.788(10 )T Using the lamina stiffness matrices from Example 7.5, the corresponding stresses in the +45° plies along the x- and y-axes are ε ox 45.22 σx = [Q]+45° ε oy = 31.42 σy γ o 32.44 τ xy +45° xy 31.442 45.22 32.44 32.44 0 32.44 0 35.6 1.788(10 −66 )T 0.058T 58.0T −6 = 58.0T (10 ) GPa = 0.058T MPa 63.65T 0.06365T Similarly, for the −45° plies, ε ox 45.22 σx = [Q]−45° ε oy = 31.42 σy γ o −32.44 τ xy −45° xy 31.42 45.22 −32.44 0 −32.44 0 −32.44 − 6 35.6 1.788(10 )T −58.0T −0.058T = −58.0T (10 −6 ) GPa = −0.058T MPa 63.65T 0.06365T Principles of Composite Material Mechanics 380 In order to use the maximum stress criterion, the stresses must be transformed to the principal material axes. Accordingly, for the +45° plies, σ x 0.5 σ1 = [ T ] σ +45° σ y = 0.5 2 τ −0.5 τ 12 +45° xy 0.5 0.5 0.5 1.0 0.058T 0.12165T −1.0 0.058T = −0.00565T MPa 0 0.06365T (0 ) T Note that it is important to distinguish here between the stress transformation matrix, [T] and the applied torque, T. Similarly, for the −45° plies, σ x 0.5 σ1 = [ T ] σ −45° σ y = 0.5 2 τ 0.5 τ 12 −45° xy 0.5 0.5 −0.5 −1.0 −0.058T −0.12165T 1.0 −0.058T = 0.00565T MPa 0 0.06365T (0)T Applying the maximum stress criterion for the +45° plies and using the strength data for AS/3501 from Table 4.1, σ 1 = 0.12165T = SL( + ) = 1448 MPa and T = 11, 903 N m σ 2 = −0.00565T = −ST( − ) = −248 MPa and T = 43, 894 N m τ12 = 0(T ) = SLT = 62.1 MPa and T = ∞ Similarly, for the −45° plies, σ 1 = −0.12165T = −SL( − ) − 1172 MPa and T = 9634 N m σ 2 = 0.00565T = ST( + ) = 48.3 MPa and T = 8549 N m τ12 = 0(T ) = SLT = 62.1 MPa and T = ∞ Note that, since the shear stress is zero along the 1,2 axes and the resulting torque needed to cause shear failure is ininite, failure due to shear is not possible. Of the remaining values, it is seen that the value of T = 8549 N m for transverse tensile failure in the −45° plies is the smallest, and so this would be the largest torque that could be transmitted without failure. It is also important to note that, if the strengths were the same in tension and compression, all plies would fail simultaneously, but as the strengths are different in tension and compression, this is not the case here. PROBLEM 7.18 An antisymmetric angle-ply [+θ/−θ] laminate is to be made of carbon/ epoxy and designed to have a laminate CTE, αx, as close to zero as possible. Determine the ply orientation θ needed to meet this requirement. The lamina properties are as follows: Analysis of Laminates 381 E1 = 138 GPa, laminate thickness = 0.125 mm E2 = 8.96 GPa α1 = −0.3 × 10−6 m/m/K G12 = 7.1 GPa α2 = 28.1 × 10−6 m/m/K ν12 = 0.3 This Problem requires extensive calculations, and the use of a computer is recommended. PROBLEM 7.19 Repeat Problem 7.18 for a Kevlar®/epoxy composite having lamina properties as follows: E1 = 76 GPa, lamina thickness = 0.125 mm E2 = 5.5 GPa α1 = −4.0 × 10−6 m/m/K G12 = 2.3 GPa α2 = 79.0 × 10−6 m/m/K ν12 = 0.34 PROBLEM 7.20 The sensing element in many thermostats is a bimetallic strip (Figure 7.45), which is a nonsymmetric laminate consisting of two plies made from different metals. If the strip is subjected to a temperature change ΔT, the differential thermal expansion of the two plies causes a corresponding change in the radius of curvature of the strip, ρx, and this motion activates the temperature control system. In the strip shown in Figure 7.45, ply #1 is aluminum, ply #2 is steel, both plies are isotropic, and each ply is 0.005 in. thick. It has been determined that the effects of Bij-type coupling on the thermal response of the strip can be neglected. Find the relationship between the temperature change ΔT and the radius of curvature, ρx. Recall that the curvature κx = 1/ρx. The required properties are given below. Ply thermal expansion coeficients: Aluminum: αAl = 12.5 × 10−6/°F Steel: αSt = 6.6 × 10−6/°F x Ply #1, aluminum, t = 0.005 in. y z ρx FIGURE 7.45 Bimetallic strip for Problem 7.20. Ply #2, steel, t = 0.005 in. Principles of Composite Material Mechanics 382 Laminate-bending compliances: −0.227 0.739 0 0.739 [D′] = −0.227 0 0 0 (psi in.3 )−1 1.928 Ply stiffness matrices: 32.817 [Q]St = 9.615 0 11.11 [Q]Al = 3.51 0 0 0 106 psi 11.6 9.615 32.817 0 3.51 11.11 0 0 0 106 psi 3.8 PROBLEM 7.21 The distribution of the in-plane shear stress, τxy, along the y direction at a particular distance z from the middle surface of a uniaxially loaded laminate is idealized, as shown in Figure 7.46. The interlaminar stress boundary layer region is assumed to extend inward from the free edge at y = b by a distance “a,” the in-plane shear stress τxy = τc in the region 0 ≤ y ≤ (b – a) is assumed to be the shear stress from the CLT, and the in-plane shear stress in the boundary layer region (b – a) ≤ y ≤ b is assumed to be of the form τ xy = τc ( y − b)(b − 2a − y ) a2 τxy a τc y b FIGURE 7.46 In-plane shear stress distribution for Problem 7.21. Analysis of Laminates 383 For the same location, determine the distribution of the interlaminar shear stress, τxz along the y-direction. PROBLEM 7.22 A [0/90/0]s laminate consisting of AS/3501 carbon/epoxy laminae is subjected to uniaxial loading along the x-direction. Use the maximum strain criterion to ind the loads corresponding to irst ply failure and ultimate laminate failure; then plot the load–strain curve up to failure. Compare these results with those of Example 7.13 and discuss any differences. PROBLEM 7.23 Solve Example 7.15 using the Tsai–Hill criterion instead of the maximum stress criterion. That is, determine the largest torque T that can be transmitted by the shaft without failure, according to the Tsai–Hill criterion. Also indicate which plies fail irst (i.e., the +45° or the −45° plies), according to the Tsai–Hill criterion. You may use any relevant results from Examples 7.15 and 7.5 without repeating their derivations, but you must clearly explain your analysis procedure. PROBLEM 7.24 Solve Example 7.15 using the maximum strain criterion instead of the maximum stress criterion. See Problem 7.23, for additional information. PROBLEM 7.25 Repeat Problem 7.23 for a 0° unidirectional AS/3501 carbon/epoxy composite shaft which has the same total wall thickness t = 1 mm and mean radius R = 50 mm. That is, ind the largest torque T that can be transmitted by the shaft, according to the Tsai–Hill criterion. You may use any relevant results from Examples 7.15 and 7.5 without repeating their derivations, but you must clearly explain your analysis procedure. Compare and discuss the results of this problem with those of Problem 7.23. 7.9 Deflection and Buckling of Laminates This section is concerned with the analysis of transverse delections of laminates under transverse loading and the prediction of laminate buckling forces. Transverse delections of laminates due to bending are generally much larger than in-plane delections, because lexural stiffnesses are lower than extensional stiffnesses. Thus, transverse delections are an important design consideration, and developments of analytical models for predicting Principles of Composite Material Mechanics 384 such delections are of interest. Buckling of laminates is an instability that is characterized by excessive transverse delections under in-plane compressive or shear forces. The general equilibrium equations governing transverse delections involve both in-plane and out-of-plane forces, but the coupling between in-plane forces and transverse delections is usually taken into account only for buckling or large delection analysis. In the analysis of small transverse delections alone, the out-of-plane forces are the most important because the laminate is normally designed in such a way that the in-plane forces are less than the corresponding buckling loads. Only a brief introduction to delection and buckling is given here. For more detailed coverage of these subjects, the reader is referred to the works of Whitney [10], Lekhnitskii [7], Vinson and Sierakowski [38], and Liessa [39]. 7.9.1 Analysis of Small Transverse Deflections The analysis of transverse delections of laminated plates has its basis in the CLT, which was outlined in Section 7.3 and in the differential equations of equilibrium. In order to develop the differential equations governing plate delections, it is convenient to use an ininitesimal element, as shown in Figure 7.47a–c from Halpin [12]. The in-plane stress resultants and moment resultants are shown in Figure 7.47a, the moment resultants are shown in dx Nxy (a) Ny x Nxy Nx z dy Nxy + y Ny + ∂Ny ∂y Nxy + dy ∂Nxy dy ∂y ∂Nxy ∂x Nx + dx ∂Nx ∂x dx Mxy My Mxy Mx Mxy + + My + (b) ∂My ∂y Mx + dy Mxy + ∂Mxy ∂y dy + ∂Mxy ∂x dx ∂Mx dx ∂x Qx Qy (c) q(x,y) Qy + ∂ Qy ∂y Qx + ∂ Qx dx ∂x dy FIGURE 7.47 Stress resultants and external loads acting on laminate. (a) In-plane stress resultants, (b) moment resultants, and (c) transverse loads and shear stress resultants. (From Halpin, J. C. 1984. Primer on Composite Materials: Analysis. Technomic Publishing Co., Lancaster, PA. With permission.) Analysis of Laminates 385 Figure 7.47b, and the transverse shear stress resultants are shown in Figure 7.47c. Transverse shear stress resultants were not considered in Section 7.3, but they must be considered here in the transverse delection analysis. In these diagrams, it is assumed that the transverse delections are small, so that the out-of-plane components of the in-plane resultants Nx, Ny, and Nxy are negligible. However, these out-of-plane components will be considered in the next section on buckling analysis because of the large transverse delections associated with buckling. Along with the stress and moment resultants such as those deined previously in Figure 7.10 and in Equations 7.35 and 7.36, the transverse shear stress resultants Qx and Qy are similarly deined as t /2 Qx = ∫τ xz dz (7.124) yz dz (7.125) − t /2 and t /2 Qy = ∫τ − t /2 Also included in Figure 7.47 is a distributed transverse load q(x, y). Following the derivation by Halpin [12] for static equilibrium according to Newton’s second law, the summation of forces along the x-direction must be N x dy + ∂N xy ∂N x dx dy + N xy dx + dx dy − N x dy − N xy dx = 0 ∂x ∂y (7.126) Equation 7.126 may be simpliied as ∂N x ∂N xy + =0 ∂x ∂y (7.127) The summation of forces along the y-direction yields N y dx + ∂N y ∂N xy dx dy + N xy dy + dx dy − N y dx − N xy dy = 0 ∂y ∂x (7.128) ∂N y ∂N xy + =0 ∂y ∂x (7.129) or Principles of Composite Material Mechanics 386 The summation of forces along the z-direction gives Qx dy + ∂Q y ∂ Qx dx dy + Qy dx + dy dx − Qx dy − Qy dx ∂x ∂y + q( x , y) dx dy = 0 (7.130) or ∂ Qx ∂ Q y + q( x , y ) = 0 + ∂x ∂y (7.131) The summation of moments about the x-axis yields − M y dx − ∂M y ∂Mxy dy dx − Mxy dy − dx dy + Qy dx dy ∂y ∂x + ∂Q y dy dx dy + q( x , y )d dx dy dy/2 + Qx dy dy/2 ∂y + ∂ Qx dx dy dy/2 + M y dx + Mxy dy − Qxdy dy/2 = 0 ∂x (7.132) Simplifying and neglecting products of differentials, we get ∂M y ∂Mxy +− = Qy ∂y ∂x (7.133) A similar summation of moments about the y-axis gives ∂Mx ∂Mxy + = Qx ∂x ∂y (7.134) Substitution of Equations 7.133 and 7.134 into Equation 7.131 yields ∂ 2 Mxy ∂ 2 M y ∂ 2 Mx + + 2 + q( x , y ) = 0 ∂y 2 ∂x ∂y ∂x 2 (7.135) Equations 7.127, 7.129, and 7.135 are the differential equations of equilibrium of the plate in terms of stress and moment resultants. The corresponding equilibrium equations in terms of displacements can be derived by substituting the laminate force–deformation Equation 7.44, the strain–displacement Analysis of Laminates 387 relations (7.32), and the curvature–displacement Equation 7.33 in Equations 7.127, 7.129, and 7.135. The resulting set of coupled partial differential equations in the displacements u0, v0, and w are A11 ∂ 2 υ0 ∂ 2 υ0 ∂ 2u 0 ∂ 2u 0 ∂ 2u 0 + A66 + A16 + ( A12 + A66 ) + 2 A16 2 2 2 ∂x ∂x ∂y ∂y ∂x ∂x ∂y + A26 A16 ∂3w ∂ 2 υ0 ∂3w ∂3w ∂ 3w − = 0 (7.136) 3 2 − − − + B B B B ( ) B 12 66 16 11 26 ∂y 3 ∂y 2 ∂x 3 ∂x 2 ∂y ∂x ∂y 2 ∂ 2u 0 ∂ 2u 0 ∂ 2u 0 ∂ 2 υ0 ∂ 2 υ0 + ( A12 + A66 ) + A26 + A66 + 2 A26 2 2 2 ∂x ∂x ∂y ∂y ∂x ∂x ∂y + A22 ∂3w ∂ 2 υ0 ∂3w ∂3w ∂3w − B22 3 = 0 (7.137) − B16 3 − (B12 + 2B66 ) 2 − 3B26 2 2 ∂y ∂y ∂x ∂x ∂y ∂x ∂y D11 ∂ 4w ∂ 4w ∂ 4w ∂ 4w + 4D16 3 + 2(D12 + 2D66 ) 2 2 + 4D26 4 ∂x ∂x ∂y ∂x ∂y ∂x ∂y 3 + D22 ∂ 4w ∂ 3 u0 ∂ 3 u0 ∂ 3 u0 − B11 − 3B16 2 − (B12 + 2B66 ) 3 4 ∂y ∂x ∂x ∂y ∂x ∂y 2 − B26 ∂ 3u0 ∂ 3 υ0 ∂ 3 υ0 ∂ 3 υ0 − − + − 2 3 B B B B ( ) 26 12 66 16 ∂y 3 ∂x 3 ∂x 2 ∂y ∂x ∂y 2 − B22 ∂ 3 υ0 = q( x , y ) ∂y 3 (7.138) Note that the in-plane displacements u0 and v0 are coupled with the transverse displacements, w, when the coupling stiffnesses, Bij, are present. For symmetric laminates with Bij = 0, Equation 7.138 alone becomes the governing equation for transverse displacements. These governing partial differential equations must be solved subject to the appropriate boundary conditions. In the general case, when the in-plane displacements are coupled with the transverse displacements, the boundary conditions must be a combination of boundary conditions for a planar theory of elasticity problem and boundary conditions for a plate-bending problem [10]. In this section, however, we will restrict the discussion to the bending of symmetric laminated plates. That is, we will only consider transverse displacements, according to Equation 7.138 with all Bij = 0. Let us now consider the case of transverse delection of the rectangular, specially orthotropic plate, which is simply supported on all edges and Principles of Composite Material Mechanics 388 a b x q(x, y) y Simple supports on all edges FIGURE 7.48 Simply supported, specially orthotropic plate with distributed loading. loaded with a distributed load, q(x, y), as shown in Figure 7.48. For a specially orthotropic plate, all Bij = 0, A16 = A26 = D16 = D26 = 0 and Equation 7.138 becomes D11 ∂ 4w ∂ 4w ∂ 4w 2 2 + + + D D ( ) = q( x , y ) D 22 12 66 ∂x 4 ∂x 2 ∂y 2 ∂y 4 (7.139) For the simply supported boundary condition, the transverse displacements and bending moments must vanish at the edges. In order to use the bending moment boundary conditions to solve the differential equation for displacements, however, the bending moments must be expressed in terms of displacements. Such expressions can be obtained from Equations 7.33 and 7.44 for the specially orthotropic plate as follows: Mx = D11κ x + D12κ y = −D11 ∂ 2w ∂ 2w − D12 2 2 ∂x ∂y (7.140) M y = D12κ x + D22κ y = −D12 ∂ 2w ∂ 2w − D22 2 2 ∂x ∂y (7.141) and Thus, along x = 0 and x = a, w=0 Analysis of Laminates 389 and Mx = −D11 ∂ 2w ∂ 2w D − =0 12 ∂x 2 ∂y 2 (7.142) and along y = 0 and y = b, w=0 and M y = −D12 ∂ 2w ∂ 2w − D22 2 = 0 2 ∂x ∂y (7.143) Several approaches to the solution of such problems have been proposed [10,38]. The simplest method involves the use of double Fourier sine series to represent both the load q(x, y) and the displacements w(x, y). If the load can be represented as ∞ q( x , y ) = ∞ ∑∑q mn sin m =1 n =1 nπy mπx sin a b (7.144) then it can be shown that the differential equation and the boundary conditions are satisied by solutions of the form ∞ w( x , y ) = ∞ ∑∑w m =1 n =1 mn sin nπy mπx sin a b (7.145) Substitution of Equations 7.145 and 7.144 into Equation 7.139 yields the displacement coeficients wmn = a 4 qmn π D11m + 2(D12 + 2D66 )(mnR)2 + D22 (nR)4 4 4 (7.146) where the plate aspect ratio R = a/b [10]. The Fourier coeficients qmn can be found for the particular assumed load distribution [9,10]. For the uniform load q(x, y) = q 0, a constant, it can be shown that the Fourier coeficients are Principles of Composite Material Mechanics 390 qmn = 16q0 π 2mn for m, n = 1, 3, 5,… and (7.147) qmn = 0 for m, n = 2, 4, 6,… Displacements w(x, y) for the uniformly loaded, simply supported plate may now be found by substituting Equations 7.146 and 7.147 into Equation 7.145. Moment resultants may be found by substituting these equations into Equation 7.33 and then substituting the result into Equation 7.44. Finally, lamina stresses may be found by combining Equations 7.33, 7.34, 7.145, 7.146, and 7.147. For boundary conditions such as clamped edges or free edges, exact series solutions similar to Equation 7.145 are generally not possible. For such cases, approximate solutions must be derived using approaches such as the Rayleigh–Ritz method or the Galerkin method. For a detailed discussion of these methods and other boundary conditions, the reader is referred to the book by Whitney [10]. 7.9.2 Buckling Analysis In the derivations of Equations 7.127, 7.129, and 7.131, the coupling between the in-plane forces Nx, Ny, and Nxy and the out-of-plane delections, w, was ignored because of the assumption of small displacements. In order to develop the equations to predict buckling under in-plane loads, however, this coupling must be considered due to the large delections associated with buckling. Such equations can be derived by assuming the differential element of Figure 7.47a to be oriented in a general out-of-plane position, as shown in Figure 7.49. Using Figure 7.49, and taking into account the vertical components of the in-plane forces, the summation of forces in the z-direction now becomes ∂ 2w ∂ Qx ∂ Q y ∂ 2w ∂ 2w + q( x , y ) + N x 2 + 2N xy + + Ny 2 = 0 ∂y ∂x ∂x ∂x ∂y ∂y (7.148) Note that Equation 7.148 consists of the terms from Equation 7.131 plus the terms involving the in-plane forces. Combining Equations 7.148, 7.133, and 7.134, we ind that ∂ 2 Mxy ∂ 2 M y ∂ 2w ∂ 2w ∂ 2w ∂ 2 Mx + N x 2 + 2N xy + + N y 2 + q( x , y ) = 0 +2 2 2 ∂y ∂x ∂x ∂y ∂x ∂y ∂y ∂x (7.149) Analysis of Laminates 391 Ny ∂w ∂y ∂w ∂x x Nxy ∂Nx dx ∂x ∂w ∂ ∂w + dx ∂x ∂x ∂x Nx + Nxy ∂w ∂x z Nxy + ∂w ∂ ∂w + dy ∂x ∂y ∂x Nx Nxy + y ∂Nxy ∂y ∂Nxy ∂x dx dy ∂w ∂w dy + ∂y ∂y Ny + ∂Ny ∂y dy FIGURE 7.49 Differential element of laminate in out-of-plane position for buckling analysis. Equation 7.149 consists of all the terms in Equation 7.135 plus the terms involving the in-plane forces. Substitution of Equations 7.148, 7.32, and 7.33 into Equation 7.149 yields the equation D11 ∂ 4w ∂ 4w ∂ 4w ∂ 4w + + + + ( ) 4 2 2 4 D D D D 26 12 66 16 ∂x 4 ∂x 3 ∂y ∂x 2 ∂y 2 ∂x ∂y 3 + D22 ∂ 4w ∂ 3 u0 ∂ 3 u0 ∂ 3 u0 − − − + B B B B ( ) 3 2 12 66 16 11 ∂y 4 ∂x 3 ∂x 2 ∂y ∂x ∂y 2 − B26 ∂ 3u0 ∂ 3 υ0 ∂ 3 υ0 ∂ 3 υ0 − B16 − (B12 + 2B66 ) 2 − 3B26 3 3 ∂y ∂x ∂x ∂y ∂x ∂y 2 − B22 ∂ 3 υ0 ∂ 2w ∂ 2w ∂ 2w = q( x , y ) + N x 2 + 2N xy + Ny 2 3 ∂y ∂x ∂x ∂y ∂y (7.150) Note that Equation 7.150 consists of the terms in Equation 7.138 and the additional terms due to the in-plane forces. We now consider the case of buckling of a rectangular, simply supported, specially orthotropic plate under a single compressive axial load, Nx = –N, as Principles of Composite Material Mechanics 392 a x b N y FIGURE 7.50 Simply supported, specially orthotropic plate under compressive uniaxial in-plane loading. shown in Figure 7.50. In this case, the loads Ny = Nxy = q(x, y) = 0, all Bij = 0, the stiffnesses A16 = A26 = D16 = D26 = 0 and Equation 7.150 becomes D11 ∂ 4w ∂ 4w ∂ 4w ∂ 2w + 2(D12 + 2D66 ) 2 2 + D22 4 = − N 2 4 ∂x ∂x ∂y ∂y ∂x (7.151) For the simply supported boundary condition described previously by Equations 7.142 and 7.143, we may assume a solution of the form ∞ w( x , y ) = ∞ ∑∑w m =1 n =1 mn sin nπy mπx sin a b (7.152) The mode shape for a particular buckling mode is described by the subscripts m and n, since m is the number of half-sine waves along the x-direction and n is the number of half-sine waves along the y-direction. Substitution of this solution in the governing differential Equation 7.151 leads to the equation wmn π 2 [(D11m 4 + 2(D12 + 2D66 )(mnR)2 + D22 (nR)4 )] = wmn Na 2m2 (7.153) where again R = a/b. This equation has the trivial solution wmn = 0, which is of no interest. For nontrivial solutions, the critical buckling load must be N cr = ( ) π2 2 4 D11m 4 + 2 (D12 + 2D66 )( mnR) + D22 ( nR) a m2 2 (7.154) where the smallest buckling load occurs for n = 1, and the lowest value of the load corresponding to a particular value of m can only be determined if the Dij and the plate dimensions a and b are known. As shown in Analysis of Laminates 393 Nxb2 (N ⋅ m) 2000 m=1 m=2 Data 1000 m=1 0 1 3 2 4 a/b FIGURE 7.51 Comparison of predicted and measured normalized buckling load, Nxb2, versus plate aspect ratio, a/b, for [012] graphite/epoxy laminates. (From Hatcher, D. and Tuttle, M. 1991. In Chung, H. H. and Kwon, Y. W. eds., Recent Advances in Structural Mechanics, PVP-Vol. 225/NE-Vol. 7, pp. 21–26. American Society of Mechanical Engineers, New York, NY. Reprinted by permission of The American Society of Mechanical Engineers.) Figure 7.51, Hatcher and Tuttle [40] have compared experimentally determined buckling loads for simply supported, specially orthotropic graphite/ epoxy panels with predicted buckling loads from Equation 7.154. The value n = 1 is used for all predicted curves, and the curves for m = 1 and m = 2 are shown. Measurement of critical buckling loads is shown schematically in Figures 7.52 and 7.53, where the compressive axial load on the laminate is N N δ FIGURE 7.52 Measurement of critical axial buckling load for laminate. δ Onset of buckling at critical load Ncr N FIGURE 7.53 Variation of lateral delection with in-plane axial load during buckling test. Principles of Composite Material Mechanics 394 Nxy Nxy FIGURE 7.54 Buckling due to in-plane shear loads. increased until the lateral delection starts to increase dramatically and the instability known as buckling soon follows. Although the predictions are reasonably accurate for this case, it was found that the agreement for some other laminate conigurations was not quite as good. Dificulties in simulating the simply supported boundary conditions and in measuring the critical buckling loads, along with other problems such as the existence of imperfections in the test panels, were cited as possible reasons for the disagreement. Other types of buckling can occur in laminates in addition to buckling under in-plane axial loads. For example, if the critical in-plane shear load is exceeded, shear buckling can occur as shown in Figure 7.54. For laminates other than specially orthotropic and boundary conditions other than simply supported, closed-form solutions similar to Equation 7.154 are generally not possible, and approximate methods such as Rayleigh–Ritz or Galerkin must be used. Exceptions include the antisymmetric cross-ply and antisymmetric angle-ply laminates, which do admit closed-form solutions [41]. 7.10 Selection of Laminate Designs When designing with conventional isotropic materials, the problem of material selection is usually solved by simply looking up the appropriate properties of candidate materials in a handbook. The selection of a composite laminate design can be a formidable task, however, due to the large number of available iber and matrix materials and the endless variety of laminate conigurations. The major differences between the analysis of laminates and the design of laminates are best explained by giving examples. A typical analysis problem would be given a composite laminate and allowable Analysis of Laminates 395 Micromechanics Lamina properties Ply orientations and stacking sequence Laminate properties Design FIGURE 7.55 Flow chart for laminate analysis. ply stresses, determine the loads that it will support, or given the laminate, loads, and properties, determine the resulting stresses and strains. Either way, the analysis problem has a unique solution. A typical design problem would be, given a set of loads and other design constraints, select the materials and laminate coniguration to withstand the loads. As opposed to the analysis problem, the design problem may have an ininite number of solutions. Depending on the number of constraints, it may be possible to reduce the number of feasible designs or to even optimize the design. A general low chart showing the laminate design sequence is shown in Figure 7.55. Depending on the degree of design lexibility desired and the availability of measured lamina level properties, the laminate design may begin either with micromechanics modeling at the iber/matrix level or directly from measured lamina properties. Obviously, the nature of the applied loads must be known in order to start the design process. Uniaxial loading on a unidirectional laminate is clearly the simplest case to deal with, but, unfortunately, most practical loading situations are multiaxial, and this requires the design of a multidirectional laminate. For example, if the loading is biaxial as shown in Figure 7.56a, only a (a) (b) FIGURE 7.56 Lamina orientations to resist different loading conditions. (a) Cross plies required to resist biaxial different loading conditions and (b) angle plies required to resist shear loads. Principles of Composite Material Mechanics 396 Unidirectional Quasi-isotropic A11 0° φ 90° FIGURE 7.57 Variation of laminate extensional stiffness with laminate orientation for unidirectional and quasi-isotropic laminates. cross-ply [0/90] laminate may be needed. However, if shear loads are present as in Figure 7.56b, some angle plies will be required as well. In the beginning stages of a design, it may be helpful to establish some practical bounds on the laminate properties based on knowledge of the mechanical behavior of certain special types of laminates. For example, Figure 7.57 shows the variation of the in-plane laminate stiffness, A11, with ϕ, the orientation of the laminate with respect to the loading direction, for both unidirectional and quasi-isotropic laminates. The unidirectional laminate stiffness for ϕ = 0 may be considered to represent the practical upper bound on laminate stiffness, and the quasi-isotropic laminate may be considered to represent the practical lower bound on laminate extensional stiffness. An essential component of any design problem is the identiication of all the possible failure modes. Whether intentional or not, if a particular failure mode is overlooked in the design process, that failure mode is the one that will most likely come back to haunt the designer. A list of the major design criteria for composite laminates and the associated failure modes are provided in Table 7.1. It is beyond the scope of this book to cover the analytical tools needed for all these design criteria, and the focus here is on strength, stiffness, stability, hygrothermal effects, and creep. In order to use the laminate analysis equations that were derived and discussed earlier in this chapter, extensive matrix algebra is obviously required. In addition, the proper evaluation of laminate designs requires numerous repetitive calculations resulting from changes in loading conditions, material properties, and laminate geometry. These computational requirements are ideally suited for solutions by digital computers, and a variety of software packages for laminate analysis now exist. A list of some of the available software packages is given in Table 7.2. Most of these programs have been developed for use on microcomputers, and many of them will do both micromechanical analysis of laminae and laminate analysis, according to the Analysis of Laminates 397 TABLE 7.1 Design Criteria for Composite Laminates and the Associated Failure Modes Design Criteria Strength Stiffness Stability Hygrothermal effects Life or durability Weight Cost Manufacturability Associated Failure Modes Fracture (either partial or complete) Excessive deformation Buckling Property degradation, expansion and contraction, residual stresses Fatigue, creep Heavier than conventional design Not affordable Impractical to build, warping due to residual stresses CLT. The two basic approaches used in many of these programs are (1) stress and strain analysis for prescribed loads and (2) irst ply failure analysis and ultimate laminate failure analysis according to one of the multiaxial lamina strength criteria that were discussed in Chapter 4. In addition, some of the programs will do specialized tasks such as delection and buckling analyses, interlaminar stress calculations, effective property calculations, and hygrothermal and transport property calculations. Such programs are indispensable in design and analysis because hand calculations are not only too time consuming, but also the possibilities for errors in such hand calculations are endless. TABLE 7.2 Composite Analysis Software Software Helius: CompositePro Company MicMac, Super MicMac MicMac/FEA FiberSim Firehole Technologies Think Composites Vistagy, Inc. HyperSizer Collier Research Lamona AdTech Systems Research, Inc. LAP Anaglyph Ltd. The Laminator RegSoft.com Address 210 South 3rd St., Suite 202, Laramie, WY 82070; web address: http://www.ireholetech.com 101 Alma Street, #703, Palo Alto, CA 94301, web address: http://www.thinkcomposites.com/ 200 Fifth Avenue, 5th Floor, Waltham, MA 02451, web address: http://www.vistagy.com 45 Diamond Hill Road, Hampton, VA 23666, web address: http://www.hypersizer.com 1342 N. Fairield Road, Beavercreek, OH 45432-2698, web address: http://www. adtech25.com/ Suite 33, 10 Barley Mow Passage, London W4 4PH, United Kingdom, web address: http:// www.anaglyph.co.uk/ http://www.thelaminator.net/ 398 Principles of Composite Material Mechanics For composite structures having complex geometries, the preferred analytical tool is the inite element method. The use of the inite element method in micromechanical analysis has already been discussed in Chapter 3. Macromechanical inite element analysis of laminated structures is also widely used, and most of the popular inite element codes have special elements such as orthotropic 3D solid elements, orthotropic 2D and 3D shell elements, and orthotropic axisymmetric solid elements [42]. Although computer software gives the designer great lexibility in the selection of materials and laminate geometries, graphical representations that show the range of properties that can be attained with different laminate conigurations are also helpful. One type of graphical representation, known as a carpet plot, is particularly useful. For example, if the ply orientations in a laminate are restricted to certain angles such as 0°, ±45°, and 90°, then a carpet plot can be generated, which shows how a given laminate property depends on the percentages of the plies at the various orientations. The carpet plots in Figure 7.58 from Reference 43 show how Ex, Gxy, νxy, and αx for [0i/±45j/90k] Kevlar/epoxy laminates vary with the percentages of the plies at the three angles. In this case, i is the number of 0° plies, j is the number of ±45° plies, and k is the number of 90° plies. Therefore, the percentage of 0° plies is i/(i + j + k), the percentage of ±45° plies is j/(i + j + k), and the percentage of 90° plies is k/(i + j + k). For example, the various ply combinations that will give a certain value of longitudinal modulus, Ex, can be determined by drawing a horizontal line in Figure 7.58a at the value of Ex and then reading off the percentage of the plies at the three angles corresponding to a particular point on the line. Obviously, there are many possible combinations that will give the same value of Ex, and the design lexibility inherent in composite construction is again demonstrated. Carpet plots for laminate strength are also widely used. Since there would normally be more than one design constraint, an iterative approach involving the repeated use of carpet plots for several different properties may be needed for the selection of the required ply combinations. Carpet plots can be quickly generated using the output of laminate analysis software. While composite analysis software packages and carpet plots are very convenient and eficient design tools for dealing with micromechanics analysis and laminate analysis using CLT, they generally do not include consideration of interlaminar stresses or other “secondary stresses.” Indeed, the secondary stresses are often neglected in the design process, which tends to focus on the “primary” in-plane stresses that are directly associated with the loading. As seen in Section 7.7, the interlaminar stresses often develop near free edges such as bolt holes or other discontinuities. An example of this is shown in Figure 7.59, where the transverse interlaminar stresses around the bolt holes in the composite link may lead to failure before the primary axial stresses do. Thus, the maximum applied axial load on the link may be limited by the secondary stresses more than by the primary axial stresses. There are other secondary stresses besides Analysis of Laminates 399 60 7 % @ 0° 50 2.0 50 6 40 40 5 30 4 30 20 3 10 2 1 0 2.5 50 40 30 20 10 70 60 % @ 90° 90 80 0 20 40 60 15.0 12.5 1.5 10.0 7.5 1.0 20 5.0 0.5 10 0 100 80 17.5 0 2.5 0 20 40 (c) 1.0 (d) 70 10 30 20 10 90 0.5 20 0.4 30 0.3 40 50 0.2 60 70 0.1 0.0 90 0 40 2.8 5.0 90 2.0 1.6 70 60 1.2 % @ 45° 80 3.0 % @ 90° 2.0 50 40 0.8 30 20 0.4 10 100 –0.8 1.0 0.0 90 80 70 60 50 40 30 20 % @ 0° –0.4 60 4.0 80 0.0 % @ 90° 80 20 6.0 2.4 80 0.6 νxy 60 40 αx (10–5 in./in.°F) 0.7 50 0 100 3.2 % @ 0° 0.8 80 % @ 45° % @ 45° 0.9 60 αx (10–5 m/m°C) Ex (106 psi) 8 60 20.0 Gxy (GPa) 70 Ex (GPa) 80 9 (b) 3.0 70 90 10 Gxy (106 psi) (a) 11 0 20 40 60 80 10 –1.0 100 % @ 45° FIGURE 7.58 Carpet plots for [0i/±45j/90k] Kevlar®/epoxy laminates. (a) Axial modulus of elasticity, Ex, (b) shear modulus, Gxy, (c) Poisson’s ratio, νxy, and (d) linear coeficient of thermal expansion, αx. (From Peters, S. T., Humphrey, W. D., and Foral, R. F. 1991. Filament Winding Composite Structure Fabrication, pp. 5–45. Society for Advancement of Materials and Process Engineering, Covina, CA. Reprinted by permission of The Society for the Advancement of Material and Process Engineering.) interlaminar stresses that may limit the applied loading on the composite more than the primary stresses do. For example, in the ilament-wound, composite cylindrical pressure vessel shown in Figure 7.60, axial bending stresses in the composite cylinder may be generated due to rotational deformation of the lip of the metal end cap as the cylinder is internally pressurized. Since the ibers in such a ilament-wound vessel are oriented primarily in the circumferential or “hoop” direction, the axial direction in the cylinder corresponds to the transverse direction in the composite. As shown in Chapter 4, the transverse tensile strength is generally the lowest Principles of Composite Material Mechanics 400 Load Interlaminar stresses around edges of holes FIGURE 7.59 Interlaminar stresses in axially loaded composite link. of all the composite strengths, so the secondary bending stresses rather than the hoop stresses may limit the internal pressure that the cylinder can withstand. A number of available handbooks and design guides are useful in the design of composite laminates and structures. These books contain not only the necessary analytical tools, but also the material property data that is required for the use of the tools. Among the recent composites handbooks are those edited by Kelly and Zweben [44], Mallick [45], Harper [46], and Donaldson and Miracle [47]. Of particular note is the ive volume series Composite Materials Handbook, MIL-HDBK-17 [48], which is sponsored by the U.S. Department of Defense, and is available online. Transverse cracking of filament wound pressure vessel at the edge of metal end cap Metal end cap Deformed shape Internal pressure Transverse cracks in the wall of vessel due to bending Filament wound cylindrical pressure vessel FIGURE 7.60 Axial bending stresses in ilament-wound composite cylinder caused by metal end cap. Analysis of Laminates 401 7.11 Application of Laminate Analysis to Composite Structures Composite structures often consist of components in the form of beams, plates, shells, sandwich panels, and grids, and for detailed coverage of the mechanics of composite structures, the reader is referred to books by Vinson and Sierakowski [49], Kollar and Springer [50], and Sun [51]. The purpose of this section is to show how the previously described CLT can be applied to composite structures that are not usually thought of as being laminates. More speciically, the application of CLT to composite sandwich structures and composite grid structures will be discussed briely. Applications of laminated beam theory to the analysis of sandwich beams will also be given. Detailed discussion of these structures is beyond the scope of this book, as both types of structures have been the subject of numerous books and journal articles, some of which are referred to here. 7.11.1 Composite Sandwich Structures Composite sandwich structures such as the one shown in Figure 1.5 are widely used in aerospace and marine applications due to the extremely high lexural stiffness-to-weight ratios and lexural strength-to-weight ratios that can be achieved with such structures. The mechanical behavior of composite sandwich structures has been described in detail by Vinson [52]. As shown in Figure 1.5, composite sandwich structures consist of two composite face sheets adhesively bonded on both sides of a lightweight foam or honeycomb core. The equivalent laminate stiffnesses of composite sandwich panels can be found directly from CLT. As shown in Figures 1.5 and 7.61, such structures are typically symmetric with respect to the middle surface, and so the corresponding coupling stiffnesses Bij = 0. The equivalent laminate extensional stiffnesses for the symmetric sandwich structure geometry in Figure 7.61 are given by substitution in Equation 7.41, as shown by Vinson [52]: 3 Aij = ∑ [Q ] (z − z ij k k k −1 ) k =1 h h h h h h = [Qij ]f − c − c − tf + [Qij ]c c − − c + [Qij ]f c + tf − c 2 2 2 2 2 2 = [Qij ]f (2tf ) + [Qij ]c hc (7.155) where facing properties are denoted by the subscript f and core properties are denoted by the subscript c. Similarly, Equation 7.42 leads to Bij = 0, and Principles of Composite Material Mechanics 402 tf Face sheets Middle surface hc Core tf z FIGURE 7.61 Geometry of composite sandwich structure for laminate analysis. Equation 7.43 gives the following equivalent laminate lexural stiffnesses, as shown by Vinson [52]: Dij = = 1 3 3 ∑ [Q ] (z ij k 3 k − zk3−1 ) k =1 3 h 3 h h 3 h 3 1 1 [Qij ]f − c − − c − tf + [Qij ]c c − − c 3 3 2 2 2 2 3 3 h 1 h + [Qij ]f c + tf − c 2 3 2 (7.156) Once the equivalent laminate stiffnesses are known, the stresses and deformations can be predicted using the approaches outlined earlier in this chapter. However, there are some corrections to laminate analysis that may be required for use on sandwich structures. For example, one of the assumptions of CLT was that the transverse shear strains γxz and γyz are negligible. This may not be the case in sandwich structures, because the core is often made of foam or honeycomb material that has a low shear modulus. If the transverse shear strains are to be considered, the transverse shear stress resultants Qx and Qy in Figure 7.47 would be related to the transverse shear strains γxz and γyz by a transverse shear stiffness matrix, there will be additional strain–displacement equations to supplement Equation 7.32, and the governing partial differential equations (Equations 7.136 through 7.138) will include additional transverse shear terms [50,52]. The importance of shear delections in sandwich structures can be demonstrated by using the laminated beam theory from Section 7.2, along with the mechanics of materials beam theory [53] to compare lexural delections and shear delections of sandwich beams, as shown later in Example 7.19. The application of laminate analysis in the prediction of strength in composite sandwich structures is signiicantly limited by the existence of Analysis of Laminates 403 P P Core shear Micro buckling P/2 P/2 P/2 P P/2 P Indentation P/2 Face wrinkling P/2 P/2 P/2 FIGURE 7.62 Failure modes of a sandwich beam in three-point bending. (Reprinted from International Journal of Mechanical Sciences, 46, Steeves, C. A. and Fleck, N. A., Collapse mechanisms of sandwich beams with composite faces and a foam core, loaded in three-point bending. Part II: Experimental investigation and numerical modeling, 585–608, Copyright (2004), with permission from Elsevier.) important failure modes in sandwich structures that are not present in composite laminates. Laminate failure modes would only be relevant for the face sheets in the sandwich, but other possible failure modes are due to the core or core/face sheet interactions. For example, Steeves and Fleck [54] have investigated the failure modes in foam-cored composite sandwich beams under three-point lexure, and the observed failure modes are summarized in Figure 7.62. The failure load, P, can be estimated from the simple mechanics of materials formulas for each of the failure modes once the beam parameters and dimensions are known. The lowest of the predicted failure loads would govern the design of the sandwich structure. In Figure 7.63, the midpoint of the beam delects by a transverse displacement u due to the applied load P of the mid-roller. L is the beam length between the supports, H is the overhang at each end, b is the width of the beam, c is the core thickness, and tf is the face sheet thickness. The relevant mechanical properties of the isotropic core are the Young’s modulus Ec, shear modulus G c, compressive strength σc, and shear strength τc. For the face sheets, the relevant properties are the axial compressive strength, σf, the Young’s modulus, Ef, and the distance between the centroids of the face sheets, d = c + tf. According to Zenkert [55], the predicted collapse load for face yielding or microbuckling is given as P= 4σ f btf d L (7.157) Principles of Composite Material Mechanics 404 P, u Ef , σ f tf Gc, Ec, σc, Tc c P/2 P/2 L H H FIGURE 7.63 Geometry of a sandwich beam in three-point bending. (Reprinted from International Journal of Mechanical Sciences, 46, Steeves, C. A. and Fleck, N. A., Collapse mechanisms of sandwich beams with composite faces and a foam core, loaded in three-point bending. Part II: Experimental investigation and numerical modeling, 585–608, Copyright (2004), with permission from Elsevier.) whereas the corresponding critical load for core shear failure can be estimated as P = 2τ cbd (7.158) and the load required to produce face sheet wrinkling is P= 2btf d 3 Ef EcGc L (7.159) Steeves and Fleck [56] have suggested that the load required for indentation failure is π 2σ c2Ef d P = btf 3L 1/3 (7.160) 7.11.2 Composite Grid Structures Grid-stiffened geodesic structural conigurations date back to the 1920s [57] when they were irst used in aircraft construction with a metal grid and fabric skin. The structures of these aircraft were known for their excellent tolerance to battle damage. Along with the maturation of composite technology, there has been increasing interest in composite grid structures for the last several decades. The most common grid structures are the orthogrid, with the ribs oriented at 0° or 90° (Figure 7.64) and the isogrid, with the ribs Analysis of Laminates 405 e d FIGURE 7.64 Orthogrid structure. oriented at 0° and ±60° (Figure 7.65). Composite grid structures are a promising concept for applications in plate or shell-like components of systems such as spacecraft, aircraft, automobiles, containers, bridges, ships, and propellers. These structures have several advantages over traditional construction methods that use panels, sandwich cores, or expensive framework. As the ribs of the grids are made of unidirectional continuous iber-reinforced composites, they are strong, tough, damage tolerant, and do not delaminate. As grids are open structures, they are easy to inspect and repair. With such processes as automated iber placement and pultrusion, the potential also exists for completely automating the grid fabrication process and reducing the processing cost. θ = 60 FIGURE 7.65 Isogrid structure. Principles of Composite Material Mechanics 406 The use of laminate analysis in modeling the mechanical behavior of grid structures is based on the concept of replacing the grid with a laminated plate having equivalent stiffnesses, as described by Chen and Tsai [58] and Huybrechts and Tsai [59]. The grid structure can be considered as a combination of sets of parallel ribs. The equivalent axial, lexural, and torsional stiffnesses of each family of parallel ribs can be calculated separately, and then the overall stiffnesses of the grid structure are obtained by the principle of superposition. Following the analysis by Chen and Tsai [58], consider the family of N parallel ribs in Figure 7.66, each of which has center-to-center spacing d (Figure 7.64), cross-sectional area A, and longitudinal modulus Ex. The direction of the local (x, y, z) coordinate axes are along and perpendicular to the ribs. Let θ be the angle between the local and global axes (1, 2, 3). It should be noted that the normal strain along the y-direction, εy, the shear strains γxy and γyz, and the curvature κy in the ribs were not considered. If all N ribs are identical, static equilibrium and geometric compatibility requirements lead to the following equation relating the force per unit length along the x-direction to the corresponding strain εx [58]: Nx = AEx ε x d (7.161) In this case, the force per unit length is based on the effective width (N − 1)d + 2e for the parallel family of ribs, where the distance e in Figure 7.64 approaches d/2. Thus, the corresponding effective width becomes approximately Nd. Transforming both the force per unit length and the strain to the Mxy Nx Mx Mx y 2 Nx Mxy FIGURE 7.66 Family of parallel ribs for modeling of grid structure. x θ 1 Analysis of Laminates 407 global coordinates and factoring out the resulting extensional stiffnesses Aij for an equivalent lat laminated plate, m4 Ex A 2 2 mn [ A] = d 3 m n m2n2 n4 mn3 m3 n A11 mn3 = A211 m2n2 A16 A12 A22 A26 A16 A26 A66 (7.162) where m = cos θ and n = sin θ. Applying a similar approach for bending of the parallel family of ribs, the lexural stiffness matrix for an equivalent lat laminated plate is found to be 4 2 2 Ex Im + GJm n E Im2 n2 − GJm2n2 1 x [D] = d 3 3 Ex Im n − GJm n E Im3 n + GJmn3 x D11 = D21 D16 D12 D22 D26 Ex Im2n2 + GJm2n2 Ex In 4 + GJm2n2 Ex Im3 n + GJm3 n Ex Im3 n − GJmn3 GJmn(m2 − n2 ) 2 2 2 GJmn(m − n ) 3 Ex Im n + 2 2 2 2 GJm (m − n ) 2 2 Ex Im n + 2 2 2 2 GJn (m − n ) Ex Im2n2 − 2 Ex Im3 n − D16 D26 D66 (7.163) where J= hw 3 16 w w4 − 3.36 1 − h 16 3 12h 4 (7.164) and Ex and G are longitudinal and shear modulus of the rib, respectively, h is rib height, and I and J are the moment of inertia with respect to the midplane and the torsional constant of the rib cross section, respectively. For the orthogrid case, the [D] matrix becomes a 3 × 3 symmetric matrix with D16, and D26 equal to zero. The A66 term for the orthogrid must be taken into account because the bending and shear effects of ribs tangential to the midplane cannot be neglected and it becomes as [58] A66 = 1 a66 (7.165) Principles of Composite Material Mechanics 408 where a66 = 2 1 d90 d0 1 d90 d02 d0 d90 + + + t t 12 Ex I 0 12 Ex I 90 κGA0 κGA90 (7.166) G is the shear modulus of the ribs, d0 and d90 are horizontal and vertical spacing of ribs, and κ is the shear correction factor, which is taken as 5/6. The total stiffnesses for the grid can be obtained from superposition by summing up the stiffnesses of each parallel family of ribs taking into account the orientation of each family of ribs. For example, the [A] and [D] matrices for the orthogrid with two families of identical ribs at θ = 0° and 90° are [ A]orthogrid Ex A d = 0 0 [D]orthogrid Ex I 1 = 0 d 0 0 Ex A d 0 0 Ex I 0 0 0 A66 (7.167) 0 0 GJ 2 (7.168) Similarly, for the isogrid with three parallel families of identical ribs at θ = 0°, 60°, and −60°, [ A]isogrid = [D]isogrid = 3 3 Ex A 1 4d 0 3 + τ 3 Ex I 1+ τ 4d 0 where τ= GJ Ex I 1 3 0 1+ τ 3+τ 0 0 0 1 0 0 1 + τ (7.169) (7.170) Analysis of Laminates 409 I= 1 wh 3 12 and J= hw 3 16 w w4 − 3.36 1 − h 16 3 12h 4 (7.171) and h is the rib height, d is the length of each side of the equilateral triangles in the isogrid, and I and J are the moment of inertia with respect to the midplane and torsional constant of the rib cross section, respectively. All the above equations apply to the case of the grid alone, but the method can also be applied to the case where the ribs are attached to a composite laminate skin on one or both sides [58]. EXAMPLE 7.16 Derive the differential equation and the boundary conditions governing the small transverse delections of a simply supported, rectangular, symmetric cross-ply laminate that is subjected to distributed loading. If the loading is described by Equation 7.144, does a solution of the form given in Equation 7.145 satisfy the differential equation and the boundary conditions? Why? Solution For a symmetric cross-ply laminate, A16 = A26 = D16 = D26 = 0 and all Bij = 0, so the differential equation (Equation 7.138) reduces to Equation 7.139. Thus, the differential equation and the boundary conditions are the same as those found for the specially orthotropic laminate in Equations 7.139 through 7.143. Likewise, the equations describing the loading and the delection are the same as those found for the specially orthotropic laminate in Equations 7.144 and 7.145, respectively. EXAMPLE 7.17 Using the carpet plots for Kevlar/epoxy laminates in Figure 7.58a, specify the required percentages of plies at 0°, 45°, and 90° if the longitudinal modulus of the laminate is to be Ex = 30 GPa. Solution The reader should be able to use Figure 7.58a to verify that a Kevlar/epoxy laminate with a longitudinal modulus of Ex = 30 GPa can be obtained with the following ply combinations: (1) 35% at 0°, 0% at 45°, and 65% at 90°; (2) 30% at 0°, 30% at 45°, and 40% at 90°; and (3) 30% at 0°, 60% at 45°, and 10% at 90°. These are only three of many possible combinations that will give the same result. Additional design constraints may also be taken into account with other carpet plots. For example, if a shear modulus, Gxy, of Principles of Composite Material Mechanics 410 at least 5.0 GPa is needed, Figure 7.58b indicates that the laminate should have at least 20% of its plies at 45°. Thus, laminates (2) and (3) above both satisfy the constraints on Ex and Gxy, but laminate (1) does not. EXAMPLE 7.18 An existing power transmission shaft consists of a hollow composite tube as shown in Figure 7.44, and the tube wall is a ilament-wound quasi-isotropic [60/0/−60]s laminate of thickness t. A new shaft of the same wall thickness t is to be designed from the same lamina material, but the new laminate is to have a shear stiffness greater than that of the existing shaft. Over what range of angles θ will a [+θ/−θ/−θ]s angle-ply laminate achieve this design objective? Solution The shear stiffness of the new angle-ply laminate is t /2 ( A66 )ap = ∫Q 66 dz = (Q66 )+ θ − t /2 2t t + (Q66 )− θ 3 3 Recalling that the lamina stiffnesses can be expressed in terms of invariants as Q66 = U1 − U 4 − U 3 cos 4θ 2 and that cos 4θ = cos(−4θ), the new laminate stiffness can be written as U1 − U 4 t − U 3 cos 4θ 2 3 ( A66 ) = = 2t U − U4 + 1 − U 3 cos(−4θ) 2 3 U1 − U 4 t − U 3t cos 4θ 2 The shear stiffness of a quasi-isotropic laminate is ( A66 )QI = U1 − U 4 t 2 Therefore, the shear stiffness of the new laminate can be expressed as ( A66 )ap = ( A66 )QI − U 3t cos 4θ The variations of (A66)ap and (A66)QI with θ are shown in Figure 7.67, where it can be seen that ( A66 )ap > ( A66 )QI for angles θ in the range 22.5° ≤ θ ≤ 67.5°. Analysis of Laminates 411 (A66)ap A66 (A66)QI 0° 22.5° 45° θ 67.5° 90° FIGURE 7.67 Variation of laminate shear stiffness with ply orientation for angle-ply and quasi-isotropic laminates. EXAMPLE 7.19 A sandwich beam is loaded in 4-point lexure, as shown in Figure 7.68, along with the shear force and bending moment diagrams. The overall dimensions of the beam are s = 120 mm, d = 41.6 mm, hc = 12.7 mm, tf = 0.711 mm, and b = 25.4 mm. The ibers in the unidirectional carbon/epoxy face sheets are aligned with the beam axis, the longitudinal Young’s modulus of the face sheets is Efs = 139.4 Pa and the shear modulus is Gfs = 3.36 GPa. The isotropic foam core material has a Young’s modulus Ec = 0.092 GPa and a shear modulus Gc = 0.035 GPa. Compare the b P/2 d P/2 s tf d hc P/2 P/2 Vmax = P/2 tf Loading points V x Mmax = Pd/2 M x FIGURE 7.68 Sandwich beam in 4-point lexural loading, along with corresponding shear force and bending moment diagrams. Principles of Composite Material Mechanics 412 beam delections (displacements) due to lexure and shear at the loading points (i.e., at x = d). Solution Since the sandwich beam to be analyzed here is symmetric about its middle surface and there are no coupling effects, a simple laminated beam analysis can be used. It can be shown using mechanics of materials beam theory (e.g., Popov [53]) that the solution to Equation 7.10 for the loading point lexural delection at x = d is wf = (Pd 2 /12Ef I yy )(3L − 4d), where the Young’s modulus from beam theory has been replaced with the lexural modulus, Ef, for a laminated beam, Iyy is the moment of inertia of the cross section, and the support span L = s + 2d. The lexural modulus from Equation 7.8 and Figure 7.2 is Ef = = 8 h3 N /2 ∑(E ) (z x j 3 j − z 3j − 1 ) j =1 8 [0.092(6.353 − 0) + 139.4(7.0613 − 6.353 )] = 38.08 GPa (14.122)3 Therefore, the lexural delection at the loading point is wf = P( 41.6)2 (3(203.2) − 4( 41.6))(10 6 ) 12(38.08 × 10 9 )(25.4)(14.122)3 /12 = 2.82 × 10 −4 P where P is in N and wf is in mm The shear delection at x = d is found by separating variables and integrating Equation 7.24 as ws ∫ 0 d dws = 1 V dx AGt ∫ 0 As shown in Figure 7.68, the shear force V = P/2, a constant, in 0 ≤ x ≤ d, so that the shear delection at x = d is ws = Pd 2 AGt where the effective transverse shear modulus for the sandwich can be approximated by Equation 3.47 as 1 u u = fs + c Gt Gfs Gc Analysis of Laminates 413 The volume fraction of face sheets is ufs = 2tf /( hc + 2tf ) = 2(0.711)/14.122 = 0.1 and the volume fraction of core material is uc = hc /( hc + 2tf ) = 12.7/14.122 = 0.9 Assuming that the face sheets are specially orthotropic and transversely isotropic, Gt = 1 = 0.0388 GPa (0.1/3.36) + (0.9/0.035) and the loading point shear delection is ws = P( 41.6)(10 6 ) = 1.495 × 10 −3 P 2(14.122)(25.4)(0.0388 × 10 9 ) where P is in N and ws is in mm. The total loading point delection is then w = wf + ws = 2.82 × 10 −4 P + 1.495 × 10 −3 P = 0.001777 P The fraction of the total delection due to lexure is wf 0.000282P = = 0.1587 w 0.001777 P whereas the fraction of the total delection due to shear is ws 0.001495 P = = 0.8446 w 0.001777 P The fraction of total delection due to shear is so large because the ratio ws/wf is proportional to Ef /Gt, which can be very large for such beams. In this case, the effective transverse shear modulus, Gt, is typically dominated by the low shear modulus of the core, Gc, and the high volume fraction of the core, uc. That is, uc/Gc ≫ ufs/Gfs in the above equation for Gt. It is clear that predicted delections that do not include the shear component would be signiicantly in error. While shear delection is typically important for sandwich structures, it is less likely to be important for conventional composite laminates, where the composite laminae would typically have much higher transverse shear moduli and much lower core volume fractions than would a foam core sandwich beam. Principles of Composite Material Mechanics 414 EXAMPLE 7.20 For the sandwich beam in 4-point lexure described in Example 7.19, use the maximum stress criterion and laminated beam theory to determine the applied load P that would cause core shear failure if the core shear strength is τc = 1.3 MPa. Solution Since Equation 7.158 only applies to 3-point lexure of a sandwich beam, a new equation must be developed here. As shown in Figure 7.6, the maximum transverse shear stress occurs at the middle surface, where z = 0. From Equation 7.19, the shear stress is V (τ xz )k = Ef I yy N /2 z j ∑∫ j = k z j −1 (Ex ) j z dz = V 2Ef I yy N /2 ∑(E ) (z x j 2 j − z 2j − 1 ) j=k Failure would occur when this shear stress is equal to the shear strength at the middle surface z = 0 in the region 0 ≤ x ≤ d, where the maximum shear force Vmax = P/2. Substituting these conditions in the above equation, along with the value of Ef from Example 7.19, 1.3 = 3P[0.092(6.352 − 0) + 139.4(7.0612 − 6.352 )] 38.08(25.4)(14.122)3 and solving for the failure load, we ind that P = 885.6 N. Note that this problem only involves core shear failure, and that a complete failure analysis would include investigation of other possible failure modes such as those described in Figure 7.62. There are many other aspects of composite sandwich structures that are not necessarily relevant to laminate analysis. For more detailed studies on composite sandwich structures, the reader is encouraged to explore the publications referred to earlier in this section. PROBLEM 7.26 Prove that for the specially orthotropic plate shown in Figure 7.48 under the loading described by Equation 7.144, the solution given by Equation 7.146 satisies the differential Equation 7.139 and the boundary conditions in Equations 7.142 and 7.143. PROBLEM 7.27 Find expressions for the moments Mx, My, and Mxy and the stresses (σx)k, (σy)k, and (τxy)k in the kth ply of the uniformly loaded, specially orthotropic laminate with simply supported edges shown in Figure 7.48. Analysis of Laminates 415 PROBLEM 7.28 Derive the differential equation and the boundary conditions governing the small transverse delections of a simply supported, rectangular, symmetric angle-ply laminate that is subjected to distributed loading. If the loading is described by Equation 7.144, does a solution of the form given in Equation 7.145 satisfy this differential equation and boundary conditions? Why? PROBLEM 7.29 Derive the coupled differential equations and the boundary conditions governing the small transverse delections of a simply supported, rectangular, antisymmetric angle-ply laminate that is subjected to distributed loading. Propose solutions for the displacements u, v, and w that satisfy the differential equations and boundary conditions. PROBLEM 7.30 A simply supported, specially orthotropic plate is subjected to an in-plane compressive load per unit length Nx and an in-plane tensile load per unit length Ny = −0.5 Nx, as shown in Figure 7.69. Derive the expression for the critical buckling load. PROBLEM 7.31 Derive the differential equation and the boundary conditions governing the buckling of a simply supported, rectangular, symmetric angle-ply laminate that is subjected to a uniaxial in-plane load, Nx. Does a solution of the form given in Equation 7.152 satisfy this differential equation and boundary conditions? Why? a 0.5 N x b y Nx Nx y 0.5 N x FIGURE 7.69 Simply supported, specially orthotropic plate under in-plane loads for Problem 7.30. Principles of Composite Material Mechanics 416 a b x Nxy Nxy y FIGURE 7.70 Simply supported laminated plate under in-plane shear loads for Problem 7.32. PROBLEM 7.32 The plate in Figure 7.70 has edge dimensions a and b and is made from a [90/0/90]s symmetric cross-ply laminate. The plate is simply supported on all edges and is subjected to a single in-plane shear load Nxy along its edges as shown. Answer the following questions below in terms of variables, not numerical values. Do not try to solve the equations, just set them up: (a) write the differential equation governing the buckling behavior of the plate, (b) write the boundary conditions for the plate, and (c) is a solution of the form shown in Equation 7.152 in the textbook possible for this problem? If so, why? If not, why not? PROBLEM 7.33 A ilament-wound composite drive shaft for a helicopter transmits a torque T that generates shear loading of the shaft material, as shown in Figure 7.71. The shaft is to be designed as a hollow tube with a two-ply [+θ/−θ] laminated wall. If the outside diameter, the length, and the material density are ixed, use invariants to determine the angle θ, which should be used to maximize the shear stiffness-to-weight ratio, A66/W, where A66 is the laminate shear D T t Nxy T θ –θ Nxy FIGURE 7.71 Filament-wound shaft for Problem 7.33. x Analysis of Laminates 417 stiffness and W is the shaft weight. It may be assumed that the shaft diameter, D, is much greater than the wall thickness, t. PROBLEM 7.34 Using the carpet plots of Figure 7.58, select the percentages of 0°, ±45°, and 90° plies that are needed in a [0i/±45j/90k] laminate if the longitudinal modulus, Ex, is to be at least 20 GPa, the in-plane shear modulus, Gxy, is to be at least 10 GPa, and the longitudinal CTE, αx, is equal to zero. References 1. Pagano, N. J. 1967. Analysis of the lexure test of bidirectional composites. Journal of Composite Materials, 1, 336–342. 2. Higdon, A., Ohlsen, E. H., Stiles, W. B., Weese, J. A., and Riley, W. F. 1976. Mechanics of Materials, 3rd ed. John Wiley & Sons, New York, NY. 3. Smith, C. B. 1953. Some new types of orthotropic plates laminated of orthotropic material. Journal of Applied Mechanics, 20, 286–288. 4. Pister, K. S. and Dong, S. B. 1959. Elastic bending of layered plates. Proceedings of the American Society of Civil Engineers (Journal of Engineering Mechanics Division), 85, EM4, 1–10. 5. Reissner, E. and Stavsky, Y. 1961. Bending and stretching of certain types of heterogeneous aeolotropic elastic plates. Journal of Applied Mechanics, 28, 402–408. 6. Stavsky, Y. 1964. On the general theory of heterogeneous aeolotropic plates. Aeronautical Quarterly, 15, 29–38. 7. Lekhnitskii, S. G. 1968. Anisotropic Plates (translation from Russian by S. W. Tsai and T. Cheron). Gordon and Breach Science Publishers, New York 8. Stavsky, Y. and Hoff, N. J. 1969. Mechanics of composite structures. In Dietz, A. G. H. ed., Composite Engineering Laminates. MIT Press, Cambridge, MA. 9. Timoshenko, S. A. and Woinowsky-Krieger, S. 1959. Theory of Plates and Shells, 2nd ed. McGraw-Hill, Inc., New York, NY. 10. Whitney, J. M. 1987. Structural Analysis of Laminated Plates. Technomic Publishing Co. Inc., Lancaster, PA. 11. Christensen, R. M. 1979. Mechanics of Composite Materials. John Wiley & Sons, Inc., New York, NY. 12. Halpin, J. C. 1984. Primer on Composite Materials: Analysis. Technomic Publishing Co., Lancaster, PA. 13. Tsai, S. W. 1964. Structural behavior of composite materials. NASA CR-71. 14. Pipes, R. B. and Pagano, N. J. 1970. Interlaminar stresses in composite laminates under uniform axial extension. Journal of Composite Materials, 4, 538–548. 15. Wang, S. S. and Choi, I. 1982. Boundary layer effects in composite laminates. Part 1: Free edge singularities. Journal of Applied Mechanics, 49, 541–548. 16. Wang, S. S. and Choi, I. 1982. Boundary layer effects in composite laminates. Part 2: Free edge solutions and basic characteristics. Journal of Applied Mechanics, 49, 549–560. 418 Principles of Composite Material Mechanics 17. Pipes, R. B. and Daniel, I. M. 1971. Moiré analysis of the interlaminar shear edge effect in laminated composites. Journal of Composite Materials, 5, 255–259. 18. Pipes, R. B. and Pagano, N. J. 1974. Interlaminar stresses in composite laminates—An approximate elasticity solution. Journal of Applied Mechanics, 41, Series E (3), 668–672. 19. Pagano, N. J. and Pipes, R. B. 1971. The inluence of stacking sequence on laminate strength. Journal of Composite Materials, 5(1), 50–57. 20. Whitney, J. M. and Browning, C. E. 1972. Free-edge delamination of tensile coupons. Journal of Composite Materials, 6(2), 300–303. 21. Whitney, J. M. and Kim, R. Y. 1977. Effect of stacking sequence on the notched strength of laminated composites. Composite Materials: Testing and Design (Fourth Conference), ASTM STP 617, pp. 229–242. American Society for Testing and Materials, Philadelphia, PA. 22. Rybicki, E. F. 1971. Approximate three-dimensional solutions for symmetric laminates under in-plane loading. Journal of Composite Materials, 5(3), 354–360. 23. Wang, A. S. D. and Crossman, F. W. 1977. Some new results on edge effect in symmetric composite laminates. Journal of Composite Materials, 11, 92–106. 24. Herakovich, C. T. 1981. On the relationship between engineering properties and delamination of composite materials. Journal of Composite Materials, 15, 336–348. 25. Hwang, S. J. and Gibson, R. F. 1992. Contribution of interlaminar stresses to damping in thick composites under uniaxial extension. Composite Structures, 20, 29–35. 26. Hwang, S. J. 1988. Characterization of the effects of three-dimensional states of stress on damping of laminated composites. PhD dissertation, Mechanical Engineering Department, University of Idaho, Moscow, ID. 27. Whitney, J. M. 1973. Free edge effects in the characterization of composite materials. Analysis of the Test Methods for High Modulus Fibers and Composites, ASTM STP 521, pp. 167–180. American Society for Testing and Materials, Philadelphia, PA. 28. Conti, P. and De Paulis, A. 1985. A simple model to simulate the interlaminar stresses generated near the free edge of a composite laminate. In Johnson, W.S. ed., Delamination and Debonding of Materials, ASTM STP 876, pp. 35–51. American Society for Testing and Materials, Philadelphia, PA. 29. Hahn, H. T. and Tsai, S. W. 1974. On the behavior of composite laminates after initial failures. Journal of Composite Materials, 8(3), 288–305. 30. Tsai, S. W. 1965. Strength characteristics of composite materials. NASA CR-224. 31. Kim, R. Y. and Soni, S. R. 1984. Experimental and analytical studies on the onset of delamination in laminated composites. Journal of Composite Materials, 18, 70–80. 32. Whitney, J. M. and Nuismer, R. J. 1974. Stress fracture criteria for laminated composites containing stress concentrations. Journal of Composite Materials, 8, 253–265. 33. Brewer, J. C. and Lagace, P. A. 1988. Quadratic stress criterion for initiation of delamination. Journal of Composite Materials, 22, 1141–1155. 34. O’Brien, T. K. 1982. Characterization of delamination onset and growth in a composite laminate. In Reifsnider, K. L. ed., Damage in Composite Materials, ASTM STP 775, pp. 140–167. American Society for Testing and Materials, Philadelphia, PA. 35. Newaz, G. M. ed. 1991. Delamination in Advanced Composites. Technomic Publishing Co., Lancaster, PA. Analysis of Laminates 419 36. Johnson, W. S. ed. 1985. Delamination and Debonding of Materials. ASTM STP 876, American Society for Testing and Materials, Philadelphia, PA. 37. Pagano, N. J. ed. 1989. In Pipes, R. B. Series ed., Interlaminar Response of Composite Laminates, Composite Laminates Series, Vol. 5, pp. 1–66. Elsevier Science Publishers, Amsterdam. 38. Vinson, J. R. and Sierakowski, R. L. 1986. The Behavior of Structures Composed of Composite Materials. Martinus Mijhoff Publishers, Dordrecht, The Netherlands. 39. Leissa, A. W. 1985. Buckling of laminated composite plates and shell panels. AFWAL-TR-85-3069, Air Force Wright Aeronautical Laboratories, WrightPatterson Air Force Base, Fairborn, OH. 40. Hatcher, D. and Tuttle, M. 1991. Measurement of critical buckling loads and mode shapes of composite panels. In Chung, H. H. and Kwon, Y. W. eds., Recent Advances in Structural Mechanics, PVP-Vol. 225/NE-Vol. 7, pp. 21–26. American Society of Mechanical Engineers, New York, NY. 41. Jones, R. M. 1975. Mechanics of Composite Materials, pp. 264–270. Hemisphere Publishing Co., New York, NY. 42. Dropek, R. K. 1987. Numerical design and analysis of structures. In Reinhart, T. J. ed., Engineered Materials Handbook, Composites, Vol. 1, pp. 463–478. ASM International, Materials Park, OH. 43. Peters, S. T., Humphrey, W. D., and Foral, R. F. 1991. Filament Winding Composite Structure Fabrication, pp. 5–45. Society for Advancement of Materials and Process Engineering, Covina, CA. 44. Kelly, A. and Zweben, C. eds. 2000. Comprehensive Composite Materials, Vols. 1–6. Elsevier, Amsterdam. 45. Mallick, P. K. ed. 1997. Composites Engineering Handbook. Marcel Dekker, Inc., New York, NY. 46. Harper, C. A. ed. 2002. Handbook of Plastics, Elastomers and Composites. McGrawHill Co., New York, NY. 47. Donaldson, S. L. and Miracle, D. B. eds. 2001. ASM Handbook, Composites, Vol. 21. ASM International, Materials Park, OH. 48. U.S. Department of Defense. 2002. MIL-HDBK-17, Composite Materials Handbook, Vols. 1–5. Available online at http://www.everyspec.com/MIL-HDBK/ MIL-HDBK+(0001+-+0099)/. 49. Vinson, J. R. and Sierakowski, R. L. 2002. The Behavior of Structures Composed of Composite Materials, 2nd ed. Kluwer Academic Publishers, Dordrecht, The Netherlands. 50. Kollar, L. P. and Springer, G. S. 2003. Mechanics of Composite Structures. Cambridge University Press, Cambridge. 51. Sun, C. T. 1998. Mechanics of Aircraft Structures. John Wiley & Sons, Inc., New York, NY. 52. Vinson, J. R. 1999. The Behavior of Sandwich Structures of Isotropic and Composite Materials. CRC Press, Boca Raton, FL. 53. Popov, E. P. 1999. Engineering Mechanics of Solids. Prentice-Hall, Upper Saddle River, NJ. 54. Steeves, C. A. and Fleck, N. A. 2004. Collapse mechanisms of sandwich beams with composite faces and a foam core, loaded in three-point bending. Part II: Experimental investigation and numerical modeling. International Journal of Mechanical Sciences, 46, 585–608. 55. Zenkert, D. 1995. An Introduction to Sandwich Construction. Chameleon, London. 420 Principles of Composite Material Mechanics 56. Steeves, C. A. and Fleck, N. A. 2004. Collapse mechanisms of sandwich beams with composite faces and a foam core, loaded in three-point bending. Part I: Analytical models and minimum weight design. International Journal of Mechanical Sciences, 46, 561–583. 57. Rehield, L. W. 1999. A brief history of analysis methodology for grid-stiffened geodesic composite structures. Proceedings of the 44th International SAMPE Symposium, CD-ROM. Society for Advancement of Material and Process Engineering, Covina, CA. 58. Chen, H. J. and Tsai, S. W. 1996. Analysis and optimum design of composite grid structures. Journal of Composite Materials, 30(4), 503–534. 59. Huybrechts, S. and Tsai, S. W. 1996. Analysis and behavior of grid structures. Composites Science and Technology, 56(9), 1001–1015. 8 Analysis of Viscoelastic and Dynamic Behavior 8.1 Introduction In the analyses of Chapters 1 through 7, it has been assumed that the applied loads are static in nature and that the composite and its constituents exhibit time-independent linear elastic behavior. However, composite structures are often subjected to dynamic loading caused by vibration or wave propagation. In addition, many composites exhibit time-dependent viscoelastic behavior under load; this is particularly true for composites having polymeric constituents. This chapter contains the basic information needed for the analysis of both viscoelastic and dynamic behavior of composites and their constituents. The word “viscoelastic” has evolved as a way of describing materials that exhibit characteristics of both viscous luids and elastic solids. Polymeric materials, which are known to be viscoelastic, may behave like luids or solids, depending on the timescale and/or the temperature. For example, polycarbonate, a thermoplastic polymer, is a liquid during molding at processing temperatures, but is a glassy solid at service (ambient) temperatures. It will deform like a rubber at temperatures just above the glass transition temperature, Tg. At temperatures below Tg, however, it will deform just as much, and in the same way if the test time is long enough. We know that ideal Hookean elastic solids are capable of energy storage under load, but not energy dissipation, whereas ideal Newtonian luids under nonhydrostatic stresses are capable of energy dissipation, but not energy storage. Viscoelastic materials, however, are capable of both storage and dissipation of energy under load. Another characteristic of viscoelastic materials is memory. Perfectly elastic solids are said to have only “simple memory” because they remember only the unstrained state and the current strains depend only on the current stresses. Viscoelastic materials have what is often referred to as “fading memory” because they remember the past in such a way that the current strains depend more strongly on the recent stress–time history than on the more distant stress–time history. 421 Principles of Composite Material Mechanics 422 There are four important physical manifestations of viscoelastic behavior in structural materials, as illustrated by the various conditions of the uniaxially loaded viscoelastic rod in Figure 8.1. First, if the rod is subjected to a constant stress, the resulting strain will exhibit time-dependent “creep,” as shown in Figure 8.1a. The time-dependent creep strains are superimposed on the initial elastic strains. Second, if the rod is subjected to a constant strain or displacement, the resulting stress will exhibit time-dependent “relaxation,” as shown in Figure 8.1b. That is, the stress relaxes from the initial elastic stress. Third, if the bar is subjected to oscillatory loading, the resulting stress–strain curve will describe a “hysteresis loop,” as shown in Figure 8.1c. The area enclosed by the hysteresis loop is a measure of the damping, or dissipation, of energy in the material. Fourth, if the bar is loaded at various strain rates, the stress–strain curves will exhibit strain–rate dependence, as shown in Figure 8.1d. That is, the stress corresponding to a given strain depends on the rate of straining. An ideal elastic material exhibits none of the above characteristics. All structural materials exhibit some degree of viscoelasticity, and the extent of such behavior often depends on environmental conditions such (b) Strain (ε) Stress (σ) (a) Time (t) Time (t) L Stress (σ = constant) (c) L–Δ Strain (ε = constant) Stress (σ) Stress (σ) (d) Strain (ε) Increasing strain rate Strain (ε) FIGURE 8.1 Physical manifestations of viscoelastic behavior in structural materials, as demonstrated by various types of loading applied to a viscoelastic rod. (a) Creep under constant stress, (b) relaxation under constant strain, (c) hysteresis loop due to cyclic stress, and (d) strain rate dependence of stress–strain curve. Analysis of Viscoelastic and Dynamic Behavior 423 as temperature. For example, while a structural steel or aluminum material may be essentially elastic at room temperature, viscoelastic effects become apparent at elevated temperatures approaching half the melting temperature. Polymeric materials are viscoelastic at room temperature, and the viscoelastic effects become stronger as the temperature approaches the glass transition temperature. Recall from Chapter 5 that the glass transition region (Figure 5.1) is a region of transition between glassy behavior and rubbery behavior and a region characterized by the onset of pronounced viscoelastic behavior. Polymers with amorphous microstructures tend to be more viscoelastic than those with crystalline microstructures. As shown in Figure 8.2, amorphous microstructures consist of three-dimensional (3D) arrangements of randomly entangled long-chain polymer molecules that are often characterized by analogy to a “bowl of spaghetti.” On the other hand, crystalline microstructures consist of regular, ordered crystalline arrays of atoms (Figure 8.2). Some polymers have both amorphous and crystalline components in their microstructures, and some polymers are purely amorphous. For example, a semicrystalline polymer may consist of crystalline “islands” in an amorphous “sea,” and the degree of crystallinity typically depends on the rates of heating and cooling during processing. On the basis of the previous discussion, we conclude that viscoelastic behavior of composite materials is typically more signiicant for composites having one or more polymeric constituents. Viscoelastic effects in polymer matrix composites are most pronounced in matrix-dominated response to off-axis or shear loading. Viscoelastic deformations and plastic deformations are similar in that both are driven by shear stresses. Indeed, elements of the theory of plasticity are often borrowed for use in the theory of viscoelasticity. For example, it is sometimes assumed in viscoelasticity analysis that Amorphous FIGURE 8.2 Amorphous and crystalline microstructures in polymers. Crystalline 424 Principles of Composite Material Mechanics the dilatational response to hydrostatic stresses is elastic, but that the distortional response to shear stresses is viscoelastic. This chapter concerns the development of stress–strain relationships for linear viscoelastic materials and their composites. These stress–strain relationships take on special forms for creep, relaxation, and sinusoidal oscillation. Following the use of certain integral transforms, the viscoelastic stress–strain relationships turn out to be analogous to Hookean elastic stress–strain relationships, leading to the so-called Elastic–Viscoelastic Correspondence Principle. Dynamic loading is usually categorized as being either impulsive or oscillatory. Dynamic response consists of either a propagating wave or a vibration, depending on the elapsed time and the relative magnitudes of the wavelength of the response and the characteristic structural dimension. Both types of excitation usually cause wave propagation initially. Wave propagation will continue if the response wavelength is much shorter than the characteristic structural dimension, otherwise standing waves (i.e., vibrations) will be set up as the waves begin to relect back from the boundaries. Wave propagation in composites may involve complex relection and/or refraction effects at iber–matrix interfaces or ply interfaces, complicating matters further. The dynamic response of composites may also be complicated by their anisotropic behavior. For example, the speed of a propagating wave in an isotropic material is independent of orientation, whereas the wave speed in an anisotropic composite depends on the direction of propagation. Anisotropic coupling effects often lead to complex waves or modes of vibration. For example, an isotropic beam subjected to an oscillatory bending moment will respond in pure lexural modes of vibration, but a nonsymmetric laminate may respond in a coupled bending–twisting mode or some other complex mode. In this chapter, however, the focus is on the analyses for vibrations and wave propagation in specially orthotropic composites or laminates without coupling. Damping, which is one of the manifestations of viscoelastic behavior, is obviously important for noise and vibration control. Composites generally have better damping than conventional metallic structural materials, especially if the composite has one or more polymeric constituents. It will be shown that the complex modulus notation and the Elastic–Viscoelastic Correspondence Principle from viscoelasticity theory are particularly useful in the development of analytical models for predicting the damping behavior of composites. Finally, it will be shown that the effective modulus theory, which was introduced in Chapters 2 and 3, is indispensable in both viscoelastic and dynamic analyses of composites. Under certain restrictions, the concept of an effective modulus or effective compliance will be used to extend various viscoelastic analyses and dynamic analyses of homogeneous materials to the corresponding analyses of heterogeneous composites. Analysis of Viscoelastic and Dynamic Behavior 425 8.2 Linear Viscoelastic Behavior of Composites A linear elastic solid exhibits linearity between stress and strain, and this linear relationship is independent of time. A linear viscoelastic solid also exhibits a linearity between stress and strain, but the linear relationship depends on the time history of the input. The mathematical criteria for linear viscoelastic behavior are similar to those for the linear behavior of any system. Following the notation of Schapery [1], the criteria can be stated as follows. Let the response R to an input I be written as R = R{I}, where R{I} denotes that the current value of R is a function of the time history of the input I. For linear viscoelastic behavior, the response R{I} must satisfy both the following conditions: 1. Proportionality: that is, R{cI} = cR{I}, where c is a constant. 2. Superposition: that is, R{Ia + Ib} = R{Ia} + R{Ib}, where Ia and Ib may be the same or different time histories. Any response not satisfying these criteria would be a nonlinear response. These criteria form the basis of the stress–strain relationship known as the Boltzmann superposition integral, which is developed in Section 8.2.1. Before getting into the analytical modeling of linear viscoelastic behavior, however, it is instructive to briely discuss a phenomenological approach to veriication of linear viscoelastic behavior. Probably, the most widely used method of characterizing viscoelastic behavior is the tensile creep test described in Figures 8.1a and 8.3, which involves the application of a constant tensile stress to a specimen and measurement of the resulting time-dependent strain. The strain versus time curves are known as creep curves, and, as shown in Figure 8.3, the total strain at any time is the sum of the initial elastic strain, ε0, and the time-dependent creep strain, ε(t). At this point, we focus on isotropic viscoelastic materials, and more details on creep tests of anisotropic composites will be presented in Chapter 10. If a number of creep curves are generated at different stress levels as shown schematically in Figure 8.4a, these creep curves can be used to plot stress–strain curves at different times. For example, by taking the ratio of stress to strain at each stress level corresponding to time t1 in Figure 8.4a, we can plot the so-called isochronous stress–strain curve at time t = t1, as shown in Figure 8.4b. The slope of the isochronous stress–strain curve is E(t), the time-dependent Young’s modulus at time t. When t = 0, the value of E(t) corresponds to the elastic Young’s modulus, and E(t) typically decreases from this value as time increases. Thus, from a set of creep curves at different stress levels as in Figure 8.4a, a family of isochronous stress–strain curves at Principles of Composite Material Mechanics 426 Constant applied stress (σ0) Strain gage Strain (ε) Total strain = ε0 + ε(t) Creep strain (ε(t)) Initial elastic strain (ε0) Test specimen Time (t) FIGURE 8.3 Tensile creep test of a viscoelastic specimen under constant stress. different times can be developed for design use. The creep compliance for a constant stress σ is S(t) = ε(t) 1 ≅ σ E(t) (8.1) And obviously S(t) increases with time. Phenomenologically speaking, a material is linear viscoelastic within the range of stresses and times for which (a) (b) Strain (ε(t)) σ4 Stress σ4 σ3 ε(t1)4 σ2 ε(t1)3 σ1 ε(t1)2 σ3 σ2 σ1 ε(t1)1 t1 Time (t) ε(t1)1 ε(t1)2 ε(t1)3 ε(t1)4 Strain at time t1 FIGURE 8.4 Illustration of creep curves at constant stress and corresponding isochronous stress–strain curves. (a) Creep curves at constant stress, where σ4 > σ3 > σ2 > σ1 and (b) isochronous stress– strain curve at time t = t1. Analysis of Viscoelastic and Dynamic Behavior 427 its isochronous stress–strain curves are linear. There are always limits on the ranges of stress and time within which a material will continue to behave in a linear viscoelastic manner. For example, if the stress level becomes high enough, the isochronous stress–strain curve will become nonlinear, and this means that the material becomes nonlinear viscoelastic. In this book, it is always assumed that the viscoelastic materials being discussed are linear viscoelastic. Typically, the creep compliance for linear viscoelastic creep curves such as those shown in Figure 8.4a can be described empirically using a power-law expression of the form S(t) = S0 + S1t n (8.2) where S 0 is the initial elastic compliance and S1 and n are empirically determined parameters. It has been shown experimentally by Beckwith [2] that for linear viscoelastic polymer matrix composites, the creep exponent n depends only on the polymer matrix, and indeed that n is the same for the composite and the polymer matrix material. Since creep experiments are generally conducted over several decades, it is often convenient to use log– log scales to plot creep compliance data. A power law plotted on a log–log scale becomes a straight line, and this provides another way to check for linear viscoelastic behavior. For example, moving S0 to the left-hand side of Equation 8.2 and taking the log of both sides of the resulting equation yields log[S(t) − S0 ] = log S1 + n log t (8.3) which is the equation for a straight line on a log–log plot of log[S(t) − S 0] versus log t with slope n and vertical axis intercept log S1, as shown in Figure 8.5. log[S(t) − S0] Slope = n log S1 log[S(t) − S0] = log S1 + n log t log t FIGURE 8.5 Illustration of log creep compliance versus log time plot. Principles of Composite Material Mechanics 428 8.2.1 Boltzmann Superposition Integrals for Creep and Relaxation The stress–strain relationships for a linear viscoelastic material can be developed by using the Boltzmann Superposition Principle [3]. If the material is at a constant temperature and is “nonaging,” then the response at any time t due to an input at time t = τ is a function of the input and the elapsed time (t – τ) only. Aging is a time-dependent change in the material, which is different from viscoelastic creep or relaxation. Both temperature and aging effects are considered in Section 8.2.6. Consider the one-dimensional (1D) isothermal loading of a nonaging, isotropic, homogeneous linear viscoelastic material by the stresses Δσ1, Δσ2, and Δσ3 at times τ1, τ2, and τ3, respectively, as shown in Figure 8.6. According to the Boltzmann Superposition Principle, the strain response is linearly proportional to the input stress, but the proportionality factor is a function of the elapsed time since the application of the input stress. Thus, for the stress–time history in Figure 8.6, the total strain response at any time t > τ3 is given by ε(t) = ∆σ 1S(t − τ1 ) + ∆σ 2S(t − τ 2 ) + ∆σ 3S(t − τ 3 ) (8.4) Δσ3 Δσ2 Δσ1 τ1 τ2 τ3 Time (t) τ1 τ2 τ3 Time (t) Strain response (ε(t)) Input stress (σ(t)) where S(t) is the creep compliance, which is zero for t < 0. For input stresses having arbitrary time histories, Equation 8.4 can be generalized as the Boltzmann superposition integral or hereditary law: FIGURE 8.6 Input stress and strain response in 1D loading of a linear viscoelastic material for illustration of the Boltzmann Superposition Principle. Analysis of Viscoelastic and Dynamic Behavior t ∫ ε(t) = S(t − τ) −∞ 429 dσ(τ) dτ dτ (8.5) Alternatively, the stress resulting from arbitrary strain inputs may be given by t dε(τ) dτ dτ ∫ σ(t) = C(t − τ) −∞ (8.6) where C(t) is the relaxation modulus, which is zero for t < 0. Equation 8.5 can be extended to the more general case of a homogeneous, anisotropic, linear viscoelastic material with multiaxial inputs and responses by using the contracted notation and writing t ∫ ε i (t) = Sij (t − τ) −∞ dσ j (τ) dτ dτ (8.7) where i, j = 1, 2, …, 6 Sij(t) = creep compliances For the speciic case of the homogeneous, linear viscoelastic, specially orthotropic lamina in plane stress, Equation 8.7 becomes t ε1(t) = ∫ S11(t − τ) −∞ t ε 2 (t) = ∫ −∞ dσ (τ) S12 (t − τ) 1 dτ + dτ t γ 12 (t) = ∫S 66 −∞ dσ 1(τ) dτ + dτ (t − τ) t ∫S 12 (t − τ) dσ 2 (τ) dτ dτ (t − τ) dσ 2 (τ) dτ dτ −∞ t ∫S 22 −∞ (8.8) dτ12 (τ) dτ dτ Similarly, Equation 8.6 can be generalized to the form t ∫ σ i (t) = Cij (t − τ) −∞ dε j (τ) dτ dτ (8.9) where Cij(t) are the relaxation moduli. Note that Equations 8.7 and 8.9 are analogous to the generalized Hooke’s law for linear elastic materials given Principles of Composite Material Mechanics 430 by Equations 2.5 and 2.3, respectively, and that Equation 8.8 are analogous to the Hooke’s law for the specially orthotropic lamina given by Equation 2.24. Thus, the creep compliances, Sij(t), for the viscoelastic material are analogous to the elastic compliances, Sij, and the viscoelastic relaxation moduli, Cij(t), are analogous to the elastic stiffnesses, Cij. In order to apply the stress–strain relationships in Equations 8.7 through 8.9 to heterogeneous, anisotropic, linear viscoelastic composites, we again make use of the “effective modulus theory” that was introduced in Chapters 2 and 3. Recall that in order to apply the stress–strain relationships at a point in a homogeneous material (i.e., Equations 2.3 and 2.5) to the case of a heterogeneous composite, we replaced the stresses and strains at a point with the volume-averaged stresses and strains (Equations 2.7 and 2.8) and also replaced the elastic moduli of the heterogeneous composite by effective moduli of an equivalent homogeneous material (Equations 2.9 and 2.10). Recall also that the criterion for the use of the effective modulus theory was that the scale of the inhomogeneity, d, had to be much smaller than the characteristic structural dimension, L, over which the averaging is done (Figure 8.7). However, since this chapter also deals with dynamic behavior, it is appropriate to add another criterion related to dynamic effects. That is, the scale of the inhomogeneity, d, must also be much smaller than the characteristic wavelength, λ, of the dynamic stress distribution (Figure 8.7). Thus, the criteria for the use of the effective modulus theory in dynamic loading of viscoelastic composites are d ≪ L and d ≪ λ. σ σ L d x Stress (σ) λ Distance (x) FIGURE 8.7 Critical dimensions that are used in the criteria for the application of the effective modulus theory. Analysis of Viscoelastic and Dynamic Behavior 431 Practically speaking, the second criterion becomes important only when dealing with the propagation of high-frequency waves having very short wavelengths. On the other hand, the wavelengths associated with typical mechanical vibrations will almost always be suficiently large so as to satisfy d ≪ λ. The book by Christensen [4] provides a more detailed discussion on the effective modulus theory. Thus, Equations 8.7 through 8.9 are valid for heterogeneous, anisotropic, linear viscoelastic composites if at an arbitrary time, t, we simply replace the stresses and strains at a point with the volume-averaged stresses and strains, replace the creep compliances with the effective creep compliances, and replace the relaxation moduli with the effective relaxation moduli. Thus, the effective creep compliance matrix for the specially orthotropic lamina in plane stress is given by S11(t) Sij (t) = S21(t) 0 S12 (t) S22 (t) 0 0 0 S66 (t) (8.10) Note the close resemblance of this creep compliance matrix to the corresponding elastic compliance matrix in Equation 2.24. For the generally orthotropic lamina, we have S11(t) Sij (t) = S21(t) S16 (t) S12 (t) S22 (t) S26 (t) S16 (t) S26 (t) S66 (t) (8.11) where Sij (t) are the transformed effective creep compliances. Note the close resemblance of this matrix to the corresponding transformed elastic compliance matrix in Equation 2.37. Halpin and Pagano [5] have shown that Sij (t) are related to Sij(t) by the transformations S11(t) = S11(t)c 4 + [2S12 (t) + S66 (t)]c 2s2 + S22 (t)s 4 S12 (t) = S12 (t)(s 4 + c 4 ) + [S11(t) − S22 (t) − S66 (t)]s2c 2 S22 (t) = S11(t)s 4 + [2S12 (t) + S66 (t)]s2c 2 + S22 (t)c 4 S66 (t) = 2[2S11(t) + 2S22 (t) − 4S12 (t) − S66 (t)]c 2s2 + S66 (t)(s 4 + c 4 ) S16 (t) = [2S11(t) − 2S12 (t) − S66 (t)]sc 3 − [2S22 (t) − 2S12 (t) − S66 (t)]s3c S26 (t) = [2S11(t) − 2S12 (t) − S66 (t))]s3c − [2S22 (t) − 2S12 (t) − S66 (t)]sc 3 (8.12) 432 Principles of Composite Material Mechanics where s = sin θ, c = cos θ, and the angle θ has been deined in Figure 2.12. Note that these equations are entirely analogous to the corresponding elastic compliance transformations in Equation 2.38. Further justiication for such direct correspondence between elastic and viscoelastic equations is provided by the Elastic–Viscoelastic Correspondence Principle, which is discussed later in Section 8.2.5. Recall that for the elastic case, strain energy considerations led to the symmetry conditions Sij = Sji and Cij = Cji. For the viscoelastic case, Schapery [1] has used thermodynamic arguments to show that if Sij(t) = Sji(t) for the constituent materials, then the same is true for the composite. Halpin and Pagano [5] and others have presented experimental evidence to show that for transversely isotropic composites under plane stress, S12(t) = S21(t). In both elastic and viscoelastic cases, further reductions in the number of independent moduli or compliances depend on material property symmetry and the coordinate system used. 8.2.2 Differential Equations and Spring–Dashpot Models Although the Boltzmann superposition integral is a valid mathematical expression of the stress–strain relationship for a linear viscoelastic material, it does not lend itself easily to the use of physical models that help us to understand viscoelastic behavior better. In this section, Laplace transforms will be used to convert the Boltzmann superposition integral to an ordinary differential equation involving time derivatives of stress and strain. Physical models for viscoelastic behavior can be easily interpreted by using differential equations. The Laplace transform, L[f(t)] or f (s), of a function f(t) is deined by ∞ ∫ L[ f (t)] = f (s) = f (t)e− stdt (8.13) 0 where s is the Laplace parameter. For purposes of illustration, we now take the Laplace transform of the 1D Boltzmann superposition integral given by Equation 8.6. The Laplace transform of both sides of the equation is given by t dε(τ) dt L[σ(t)] = σ(s) = L C(t − τ) dt −∞ ∫ (8.14) Noting that the right-hand side of Equation 8.14 is in the form of a convolution integral [6], we can also write t d ε (s) dε(τ) C(s) dτ = L C(t − τ) dτ dτ −∞ ∫ (8.15) Analysis of Viscoelastic and Dynamic Behavior 433 Taking the inverse Laplace transform of Equation 8.15, we ind that t d ε (s) dε(τ) dτ L C(s) = C(t − τ) dτ dτ −∞ ∫ −1 (8.16) Thus, Equation 8.14 can be written as d ε (s) d ε (s) σ(s) = L L−1 C(s) = C(s) dτ dτ (8.17) But from the properties of Laplace transforms of derivatives [6], dε(τ) d ε (s) L = = s ε (s) − ε(0) dτ dτ (8.18) where ε(0) is the initial strain. If we neglect the initial conditions, Equation 8.17 becomes σ(s) = sC(s) ε (s) (8.19) If we perform similar operations on Equation 8.5, we ind that ε (s) = sS (s)σ(s) (8.20) Note that Equations 8.19 and 8.20 are now of the same form as Hooke’s law for linear elastic materials, except that the Laplace transforms of the stresses and strains are linearly related, and the proportionality constants are the Laplace transform of the creep compliance and the Laplace transform of the relaxation modulus. This is another example of the correspondence between the equations for elastic and viscoelastic materials and is another building block in the Elastic–Viscoelastic Correspondence Principle, which will be discussed in Section 8.2.5. Note also that according to Equations 8.19 and 8.20, the Laplace transform of the creep compliance and the Laplace transform of the relaxation modulus must be related by S (s) = 1 s C(s) 2 (8.21) Principles of Composite Material Mechanics 434 However, the corresponding time-domain properties are not mathematically related by a simple inverse relationship. That is, in general, S(t) ≠ 1 C(t) (8.22) However, a usually good approximation is S(t) ≈ 1 C(t) (8.23) and it can be shown by using the initial value theorem and the inal value theorem of Laplace transforms that for short times or for long times, the mathematically exact relationship is S(t) = 1 , when t → 0 or when t → ∞ C(t) (8.24) The coeficient term in Equation 8.20 can also be written as a ratio of two polynomials in the Laplace parameter s as follows: ε (s) = sS (s)σ(s) = Q(s) σ(s) P(s) (8.25) where P(s) = a0 + a1s + a2s2 + ⋯ + an sn Q(s) = b0 + b1s + b2s2 + ⋯ + bn sn Thus, we can write P(s) ε (s) = Q(s)σ(s) (8.26) But if we neglect the initial conditions, the Laplace transform of the nth derivative of a function f(t) is d n f (t) n L = s f (s) n dt (8.27) Analysis of Viscoelastic and Dynamic Behavior (a) (b) 435 (c) S(t) k 1 C(t) μ 2 k 1 k t t FIGURE 8.8 Maxwell model, with corresponding creep and relaxation curves. (a) Spring–dashpot arrangement, (b) creep compliance versus time, and (c) relaxation modulus versus time. Making use of Equation 8.27 and taking the inverse Laplace transform of Equation 8.26, we ind that an d2ε dε dσ d 2σ d nσ dnε + + + + ε = σ + + + + ⋯ a a a b b b ⋯ b 1 0 0 1 2 n 2 dt n dt 2 dt dt dt 2 dt n (8.28) Thus, linear viscoelastic behavior may also be described by an ordinary differential equation as well as by the Boltzmann superposition integral. Note that the linear elastic material described by Hooke’s law is a special case of Equation 8.28 when all time derivatives of stress and strain vanish (i.e., a0ε = b0σ). Recall that one of the physical manifestations of viscoelastic behavior is the dependence of stress on strain rate; such strain rate effects can be modeled with Equation 8.28. We now consider several simple physical models of linear viscoelastic behavior that include various time derivatives of stress and strain. As shown in Figures 8.8 through 8.10, useful physical models can be constructed from simple elements such as the elastic spring and the viscous (a) (b) (c) S(t) C(t) k k μ t t FIGURE 8.9 Kelvin–Voigt model, with corresponding creep and relaxation curves. (a) Spring–dashpot arrangement, (b) creep compliance versus time, and (c) relaxation modulus versus time. Principles of Composite Material Mechanics 436 (a) (b) (c) C(t) S(t) k0 k1 μ1 1 at t = ∞ k0 1 k0 + k1 t k0 + k1 t k0 at t=∞ FIGURE 8.10 Standard linear solid or Zener model, with corresponding creep and relaxation curves. (a) Spring–dashpot arrangement, (b) creep compliance versus time, and (c) relaxation modulus versus time. dashpot, where the spring of modulus k is assumed to follow Hooke’s law and the dashpot is assumed to be illed with a Newtonian luid of viscosity µ. Thus, the stress–strain relationship for the elastic spring element is of the form ε = σ/k, whereas the corresponding equation for the viscous dashpot is dε/dt = σ/µ. The Maxwell model consists of a spring and a dashpot in series, as shown in Figure 8.8a. The total strain across a model of unit length must equal the sum of the strains in the spring and the dashpot, so that ε = ε1 + ε 2 (8.29) and the strain rate across the model is then dε dε1 dε 2 1 dσ σ = + = + dt dt dt k dt µ (8.30) Note that Equation 8.30 is just a special case of Equation 8.28, with only irst derivatives of stress and strain. For creep at constant stress σ = σ0, Equation 8.30 reduces to dε σ 0 = dt µ (8.31) Integrating Equation 8.31 once, we ind that ε(t) = σ0 t + C1 µ (8.32) where the constant of integration, C1, is found from the initial condition ε(0) = C1 = σ0/k. Thus, the creep strain for the Maxwell model is given by Analysis of Viscoelastic and Dynamic Behavior 437 σ0 σ t+ 0 µ k (8.33) ε(t) = and the corresponding creep compliance is given by S(t) = ε(t) t 1 = + σ0 µ k (8.34) A plot of the creep compliance versus time according to Equation 8.34 is shown in Figure 8.8b. The type of creep behavior that is actually observed in experiments is more like that shown in Figure 8.6, however. Thus, the Maxwell model does not adequately describe creep. For relaxation at constant strain ε = ε0, the Maxwell model stress–strain relationship in Equation 8.30 becomes 0= 1 dσ σ + k dt µ (8.35) Integrating Equation 8.35 once, we ind ln σ = − k t + C2 µ (8.36) where the constant of integration, C2, is found from the initial condition σ(0) = σ0. The resulting stress relaxation function is σ(t) = σ 0 e − kt/µ = σ 0 e − t/λ (8.37) where λ = µ/k is the relaxation time, or the time required for the stress to relax to 1/e, or 37% of its initial value. The relaxation time is therefore a measure of the internal timescale of the material. The corresponding relaxation modulus is C(t) = σ(t) σ 0 − t/λ = e = ke− t/λ ε0 ε0 (8.38) Figure 8.8c shows the relaxation modulus versus time from Equation 8.38, which is in general agreement with the type of relaxation observed experimentally. Thus, the Maxwell model appears to describe adequately the relaxation phenomenon, but not the creep response. Figure 8.9a shows the Kelvin–Voigt model, which consists of a spring and a dashpot in parallel. Using the appropriate equations for a parallel Principles of Composite Material Mechanics 438 arrangement and following a procedure similar to the one just outlined, it can be shown that the differential equation describing the behavior of the Kelvin–Voigt model is given by σ = kε + µ dε dt (8.39) Equation 8.39 is seen to be another special case of Equation 8.28, with only irst derivatives of strain. It can also be shown that the creep compliance for the Kelvin–Voigt model is given by S(t) = 1 [1 − e− t/ρ ] k (8.40) where ρ = µ/k is now referred to as the retardation time. Similarly, the relaxation modulus is given by C(t) = k (8.41) Equations 8.40 and 8.41 are plotted in Figure 8.9b and c, respectively. The creep compliance curve agrees with experimental observation, except that the initial elastic response is missing. On the other hand, the relaxation modulus has not been observed to be constant, as shown in Figure 8.9c. Thus, like the Maxwell model, the Kelvin–Voigt model does not adequately describe all features of experimentally observed creep and relaxation. One obvious way to improve the spring–dashpot model is to add more elements. One such improved model, shown in Figure 8.10a, is referred to as the standard linear solid or Zener model. It can be shown that the differential equation for the Zener model is given by σ+ µ1 dσ µ dε = k 0 ε + 1 ( k 0 + k1 ) dt k1 dt k1 (8.42) where parameters k0, k1, and µ1 are deined in Figure 8.10a. Equation 8.42 is obviously another special case of the general differential Equation 8.28. It is also interesting to note that the Zener model shown in Figure 8.10a is just a Maxwell model in parallel with a spring. The creep compliance for the Zener model is given by S(t) = 1 k0 k1 − t/ρ1 1 − k + k e 0 1 where ρ1 = (µ1/k0 k1)(k0 + k1) is the retardation time. (8.43) Analysis of Viscoelastic and Dynamic Behavior 439 As shown in Figure 8.10b, the shape of the creep compliance curve from Equation 8.43 matches the expected shape based on experimental observations. The relaxation modulus for the Zener model is given by C(t) = k0 + k1 e− t/λ1 (8.44) where λ1 = µ1/k1 is the relaxation time. Note that λ1 is just the relaxation time for the Maxwell model consisting of µ1 and k1. Figure 8.10c shows the predicted relaxation modulus curve from Equation 8.44, and, again, the general shape of the curve appears to be similar to what is experimentally observed. Although the Zener model is the simplest spring–dashpot model that correctly describes all expected features of experimentally observed creep and relaxation behavior in linear viscoelastic materials, it still is not completely adequate. This remaining inadequacy is best described by plotting the relaxation modulus versus the logarithm of time, as shown in Figure 8.11. Practically speaking, complete relaxation for the Zener model occurs in less than a decade in time, but relaxation for real polymers happens over a much longer timescale. For example, the glass-to-rubber transition, which is only one of several regions of polymer viscoelastic behavior, takes about six to eight decades in time to complete [7]. This extended relaxation period for polymers is due to the existence of a distribution of relaxation times. By using an improved Zener model, such as the parallel arrangement shown in Figure 8.12, we can introduce such a distribution of relaxation times, λi, that makes it possible to extend the range of relaxation to more realistic values. This form of the improved Zener model consists of n Maxwell elements in parallel with the elastic spring, k 0. It Increasing number of relaxation times (n) Improved Zener model Zener model 1 2 3 4 5 6 7 8 log t FIGURE 8.11 Effect of increasing number of relaxation times on relaxation curve of the Zener model. Principles of Composite Material Mechanics 440 k1 k2 k3 kn k0 μ2 μ1 μn μ3 FIGURE 8.12 Improved Zener model, parallel arrangement. can be easily shown that the relaxation modulus for this improved Zener model is given by n C(t) = k0 + ∑k e i − t /λ i (8.45) i =1 where λi = µi/ki is the relaxation time for the ith Maxwell element. As shown in Figure 8.11, the effect of increasing n and the corresponding number of relaxation times is to broaden the range of relaxation. The number of relaxation times needed to describe adequately the viscoelastic behavior of a particular material must be determined experimentally. For an ininite number of elements in the improved Zener model of Figure 8.12 and a continuous distribution of relaxation times, the relaxation modulus can be expressed as [8] ∞ ∫ C(t) = k0 + k(λ )e− t/λ dλ (8.46) 0 where k(λ) is the distribution of relaxation times or the relaxation spectrum, which is shown schematically in Figure 8.13. By considering an alternative form of an improved Zener model consisting of a spring in series with n Kelvin–Voigt elements, as shown in Figure 8.14, it can be shown that the corresponding creep compliance expression is S(t) = 1 + k0 n ∑ k [1 − e i =1 1 − t/ρi ] (8.47) i where ρi = µi/ki is the retardation time for the ith Kelvin–Voigt element. Analysis of Viscoelastic and Dynamic Behavior k(λ) 441 λ FIGURE 8.13 Continuous distribution of relaxation times or relaxation spectrum k(λ), for improved Zener model of Figure 8.13, with an ininite number of elements. Although the above equations have been derived on the basis of simple spring–dashpot models, the generalized relaxation modulus and creep compliance expressions for anisotropic linear viscoelastic composites have the same forms as Equations 8.45 and 8.47, respectively. According to Schapery [1], if the elastic moduli are positive deinite (i.e., always either positive or equal to zero), it can be shown using thermodynamic theory that the generalized expressions corresponding to Equations 8.45 and 8.47 are, respectively, n Cij (t) = ∑C ij ( m ) − t /λ m e + Cij (8.48) m =1 and n Sij (t) = ∑S ij ( m) [1 − e− t/ρm ] + Sij (8.49) m =1 k0 μ1 μ2 μ3 μn k1 k2 k3 kn FIGURE 8.14 Improved Zener model, series arrangement. 442 Principles of Composite Material Mechanics where i, j = 1, 2, …, 6 Cij, Sij = elastic moduli and compliances, respectively λm, ρm = relaxation times and retardation times, respectively LCij(m), Sij(m) = coeficients corresponding to λm and ρm, respectively As with the simple spring–dashpot models, the numerical values of the parameters on the right-hand side of Equations 8.48 and 8.49 must be determined experimentally. The relaxation times and retardation times are strongly dependent on temperature, and such temperature dependence is the basis of the time–temperature superposition (TTS) method, which will be discussed later. It is assumed here that the materials are “thermorheologically simple.” That is, all the relaxation times, λi, and the retardation times, ρi, are assumed to have the same temperature dependence. A similar argument holds for the effect of aging, which will also be discussed later. 8.2.3 Quasielastic Analysis From the previous section, it should be clear that the generalized Boltzmann superposition integrals in Equations 8.7 and 8.9 can be Laplace transformed to yield equations of the form εi (s) = sSij (s)σ j (s) (8.50) σ i (s) = sCij (s) ε j (s) (8.51) and These equations are of the same form as the corresponding elastic stress– strain relationships and are presumably easier to work with than the integral equations. In a practical analysis or design problem involving the use of these equations, however, the problem solution in the Laplace domain would then have to be inverse transformed to get the desired time-domain result, and this can present dificulties. Schapery [1] has presented several approximate methods for performing such inversions. If the input stresses or strains are constant, however, there is no need for inverse transforms and the timedomain equations turn out to be very simple. Schapery refers to this as a “quasielastic analysis,” and the equations used in such an analysis will be developed in the remainder of this section. Consider a generalized creep problem with time-varying stresses σj(t) given by σ j (t) = σ ′j H (t) (8.52) Analysis of Viscoelastic and Dynamic Behavior δ(t) (b) H(t) (a) 443 Note: ε 0 1 ε t 1 ε ε t FIGURE 8.15 Unit step function and Dirac delta function. (a) Unit step function and (b) Dirac delta function. where j = 1, 2, … , 6, σ ′j are constant stresses and H(t) is the unit step function, or Heaviside function, shown in Figure 8.15a and deined as follows [3]: for t ≤ 0 0 lim H (t) = t/ε for 0 ≤ t ≤ ε ε→0 1 for t ≥ ε (8.53) The unit step function can be easily shifted along the time axis by an amount ξ by writing the function as H(t − ξ). Substituting the stresses from Equation 8.52 into the Boltzmann superposition integral, Equation 8.7, we ind that the resulting strains are given by t ∫ ε i (t) = Sij (t − τ) σ ′j −∞ dH (τ) dτ dτ (8.54) but according to Equation 8.53, the derivative of the step function must be for t ≤ 0 0 dH (t) = δ(t) = 1/ε for 0 ≤ t ≤ ε dt 0 for t ≥ 0 (8.55) where the parameter ε can be made arbitrarily small, the derivative in Equation 8.55 is taken before ε → 0, and Δ(t) is the Dirac delta function shown in Figure 8.15b. Thus, the integral in Equation 8.54 can be written as t ε i (t) = Sij (t − τ)δ(τ) dτ σ ′j −∞ ∫ (8.56) Principles of Composite Material Mechanics 444 where the constants σ′j have been moved outside the integral. According to the properties of convolution integrals [6], we can also write t ε i (t) = Sij (τ)δ(t − τ) dτ σ ′j −∞ ∫ (8.57) This integral can be broken down and rewritten as follows: t t − ε ε i (t) = (0) dτ + Sij (t)δ(t − τ) dτ σ ′j t−ε −∞ ∫ ∫ (8.58) where Sij(τ) evaluated over the interval t − ε ≤ τ ≤ t can be approximated as Sij(t) since ε is very small. Sij(t) can now be moved outside the integral, leaving the integral of the Dirac delta function, which is deined as [6] t ∫ δ(t − τ)dτ = 1 (8.59) ε i (t) = Sij (t)σ ′j (8.60) t−ε Thus, the inal result is The form of this equation suggests that we can solve for creep strains under constant stresses, σ ′j , by simply replacing the elastic compliances, Sij, in Hooke’s law (Equation 2.5) with the corresponding viscoelastic creep compliances, Sij(t). Similarly, it can be shown that if the constant strain inputs ε j (t) = ε′j H (t) (8.61) are substituted into Equation 8.9, the resulting stresses must be σ i (t) = Cij (t)ε′j (8.62) Thus, the stress relaxation under constant strains can be found by replacing the elastic moduli, Cij, in Hooke’s law (Equation 2.3) with the corresponding viscoelastic relaxation moduli, Cij(t). Equations 8.60 and 8.62 form the basis of the so-called “quasielastic analysis” and obviously eliminate the need for Laplace transform analysis in the stress–strain relationships. It should be Analysis of Viscoelastic and Dynamic Behavior 445 emphasized again, however, that Equations 8.60 and 8.62 are only valid for constant or near-constant inputs. Such equations give additional hints of a direct correspondence between the equations for linear elastic systems and those for linear viscoelastic systems, and this correspondence will be discussed in more detail later. The quasielastic approach has been successfully used in a number of practical applications such as micromechanical modeling of creep in polymer composites [9], prediction of creep in rotating viscoelastic disks [10], analysis of creep in prestressed composite connectors [11], and modeling of creep in prestressed polymer composite lubricators [12]. Many of these applications involve inite element implementations of the quasielastic approach, where inite element models are employed to solve a series of elastic problems, and the time dependence is accounted for by using different elastic moduli at each time step. 8.2.4 Sinusoidal Oscillations and Complex Modulus Notation In the previous section, it was shown that when the inputs are constant, the Boltzmann superposition integrals are reduced to simple algebraic equations that resemble the linear elastic Hooke’s law. In this section, an analogous simpliication will be demonstrated for the case of stresses or strains that vary sinusoidally with time. The results will make it much easier to analyze sinusoidal vibrations of viscoelastic composites. The general procedure here follows was presented by Fung [3]. Consider the case where the stresses vary sinusoidally with frequency ω. Using the contracted notation and complex exponentials, such stresses can be written as σɶ n (t) = Aneiωt (8.63) where n = 1, 2, …, 6 i = imaginary operator, is −1 An = complex stress amplitudes ~ = superscript denoting a sinusoidally varying quantity Substituting Equation 8.63 into Equation 8.7, we ind that the resulting sinusoidally varying strains are given by t ∫ εɶ m (t) = Smn (t − τ)iωAneiωτ dτ −∞ where m, n = 1, 2, …, 6. (8.64) Principles of Composite Material Mechanics 446 It is now convenient to deine a new variable ξ = t − τ, so that ∞ ∫ εɶ m (t) = Smn (ξ)e− iωξiωAneiωt dξ (8.65) 0 The terms not involving functions of ξ may be moved outside the integral, and since Smn(t) = 0 for t < 0, the lower limit on the integral can be changed to –∞, so that ∞ εɶ m (t) = iωAne i ωt ∫S mn (ξ)e− iωξ dξ (8.66) −∞ The integral in Equation 8.66 is just the Fourier transform of the creep compliances, F[Smn(ξ)], or Smn(ω), which is written as ∞ ∫ F[Smn (ξ)] = Smn (ω) = Smn (ξ)e− iωξ dξ (8.67) −∞ Thus, the stress–strain relationship reduces to εɶ m (t) = iωSmn (ω)Aneiωt = iωSmn (ω)σɶ n (t) (8.68) In order to obtain this equation to resemble Hooke’s law more closely, we simply deine the frequency-domain complex compliances as follows: * Smn (ω ) = iωSmn (ω ) (8.69) so that Equation 8.68 becomes * (ω)σɶ n (t) εɶ m (t) = Smn (8.70) Thus, in linear viscoelastic materials, the sinusoidally varying stresses are related to the sinusoidally varying strains by complex compliances in the same way that static stresses and strains are related by elastic compliances in the linear elastic material. In addition, the time-domain creep compliances are related to frequency-domain complex compliances by Fourier transforms. It is important to note, however, that the complex compliance is not simply equal to the Fourier transform of the corresponding creep com* pliance. According to Equation 8.69, the complex compliance, Smn (ω ), is equal Analysis of Viscoelastic and Dynamic Behavior 447 to a factor of iω times Smn(ω), and Smn(ω) is the Fourier transform of the creep compliance Smn(t). Alternatively, if we substitute sinusoidally varying strains into Equation 8.9, we ind that the sinusoidally varying stresses are * (ω )εɶ n (t) σɶ m (t) = Cmn (8.71) where the complex moduli are deined by * Cmn (ω ) = iωCmn (ω) (8.72) and the Cmn(ω) are the Fourier transforms of the corresponding relaxation moduli, Cmn(t). Alternatively, Equations 8.70 and 8.71 may be written in matrix form as {εɶ (t)} = [S* (ω)]{σɶ (t)} (8.73) {σɶ (t)} = [C * (ω)]{εɶ (t)} (8.74) and respectively, where the complex compliance matrix and the complex modulus matrix must be related by [S*(ω)] = [C*(ω)]−1. The complex modulus notation not only has a mathematical basis in viscoelasticity theory, but it also has a straightforward physical interpretation. Since the complex modulus is a complex variable, we can write it in terms of its real and imaginary parts as follows: * * Cmn (ω) = Cmn (ω )|e− iδ mn (ω) ′ (ω) + iCmn ′′ (ω) = Cmn ′ (ω)[1 + iηmn (ω)] =|Cmn (8.75) (no summation on m and n in Equation 8.75), where Cmn ′ (ω) = storage modulus C ″ mn (ω) = loss modulus ηmn(ω) = loss factor = tan[δ mn (ω)] = (Cmn ′′ (ω)/Cmn ′ (ω)) ɶ ɶ δmn(ω) = phase lag between σ m (t) and ε n (t) Thus, the real part of the complex modulus is associated with elastic energy storage, whereas the imaginary part is associated with energy dissipation, or damping. A physical interpretation of the 1D forms of these equations may be given with the aid of the rotating vector diagram in Figure 8.16. The stress Principles of Composite Material Mechanics 448 ~ σ(t) ~ ε(t) σ″ δ(ω) ωt δ σ′ FIGURE 8.16 Rotating vector diagram for physical interpretation of the complex modulus. and strain vectors are both assumed to be rotating with angular velocity ω, and the physical oscillation is generated by either the horizontal or the vertical projection of the vectors. The complex exponential representations of the rotating stress and strain vectors in the diagram are σɶ (t) = σei(ωt + δ ) and εɶ (t) = εeiωt (8.76) so that the 1D complex modulus is deined as C * (ω) = σɶ (t) σeiδ σ σ′ σ ′′ = = (cos δ + isin δ ) = +i εɶ (t) ε ε ε ε = C ′(ω ) + iC ′′(ω) = C ′(ω)[1 + iη(ω)] (8.77) It is seen that the strain lags the stress by the phase angle δ; the storage modulus, C′(ω) is the in-phase component of the stress, σ′, divided by the strain, ε; the loss modulus, C′(ω) is the out-of-phase component of stress, σ′, divided by the strain, ε; and the loss factor, η(ω) is the tangent of the phase angle δ. Experimental determination of the complex modulus involves the measurement of the storage modulus, C′(ω), and the loss factor, η(ω), as a function of frequency, ω; several techniques for doing this will be described in Chapter 10. The inverse Fourier transform of the parameter Smn(ω) is the creep compliance Smn(t), as given by F −1[Smn (ω)] = Smn (t) = 1 2π ∞ ∫S mn −∞ (ω )e iωt dω (8.78) Analysis of Viscoelastic and Dynamic Behavior 449 where F−1 is the inverse Fourier transform operator. Equations 8.67 and 8.78 form the so-called Fourier transform pair, which makes it possible to transform back and forth between the time domain and the frequency domain [13]. Since experimental frequency data are usually expressed in units of cycles per second, or Hertz, it is convenient to deine the frequency as f = ω/2π (Hz), so that the Fourier transform pair now becomes symmetric in form: ∞ ∫ F[Smn (t)] = Smn ( f ) = Smn (t)e− i2πft dt (8.79) −∞ and ∞ ∫ F [Smn ( f )] = Smn (t) = Smn ( f )ei 2 πft df −1 (8.80) −∞ It can be shown that the time-domain relaxation modulus and the corresponding frequency-domain complex modulus are related by a similar Fourier transform pair. As a further indication of the usefulness of such equations, inverse Fourier transforms have been used to estimate time-domain creep behavior of composites from frequency-domain complex modulus data obtained from vibration tests of the same materials [14]. 8.2.5 Elastic–Viscoelastic Correspondence Principle In the previous sections, we have seen a number of examples where the form of the stress–strain relationships for linear viscoelastic materials is the same as that for linear elastic materials. Such analogies between the equations for elastic and viscoelastic analysis have led to the formal recognition of an “Elastic–Viscoelastic Correspondence Principle.” The correspondence principle for isotropic materials was apparently introduced by Lee [15], whereas the application to anisotropic materials was proposed by Biot [16]. The speciic application of the correspondence principle to the viscoelastic analysis of anisotropic composites has been discussed in detail by Schapery [1,17] and Christensen [6]. A summary of the correspondences between elastic and viscoelastic stress–strain relationships is given in Table 8.1. The implication of this table is that if we have the necessary equations for a linear elastic solution to a problem, we simply make the corresponding substitutions in the equations to get the corresponding linear viscoelastic solution. Although Table 8.1 is only concerned with the correspondences in the stress–strain relationships, there are obviously other equations involved in a complete Principles of Composite Material Mechanics 450 TABLE 8.1 Elastic–Viscoelastic Correspondence in Stress–Strain Relationships Material and Input Stresses Strains Linear elastic Input stresses Input strains σj σi εi εj Sij Cij (2.5) (2.3) Linear viscoelastic Generalized creep Constant stress creep σ j (s) σ ′j εi (s) εi(t) sSij (s) Sij(t) (8.50) (8.60) σ i (s) σi(t) σɶ j (t) σɶ i (t) ε j (s) ε′j εɶ i (t) εɶ j (t) sCij (s) Cij(t) (8.51) (8.62) (8.70) Generalized relaxation Constant strain relaxation Sinusoidal stress input Sinusoidal strain input Properties Sij* (ω) Cij* (ω) Equation (8.71) Note: i, j = 1, 2, …, 6. solution to an elasticity problem. The correspondences in the equilibrium equations, the strain–displacement relations, the boundary conditions, and the variational methods of elastic analysis are beyond the scope of this book, but detailed discussions of these are given by Schapery [1,17] and Christensen [4,6]. One of the most important implications of the correspondence principle is that analytical models for predicting elastic properties of composites at both the micromechanical and the macromechanical levels can be easily converted for prediction of the corresponding viscoelastic properties. For example, the rule of mixtures for predicting the longitudinal modulus of a unidirectional composite can now be converted for viscoelastic relaxation problems by rewriting Equation 3.27 as E1(t) = Ef1(t)υf + Em (t)υm (8.81) where E1(t) = longitudinal relaxation modulus of composite Ef1(t) = longitudinal relaxation modulus of iber Em(t) = relaxation modulus of isotropic matrix υf = iber volume fraction υm = matrix volume fraction The relative viscoelasticity of iber and matrix materials may make further simpliication possible. In most polymer matrix composites, the time dependency of the matrix material would be much more signiicant than Analysis of Viscoelastic and Dynamic Behavior 451 Principal compliances (Sij × 10–6 psi–1) 1.6 Temperature 75°F ° 1.2 Experimental Halpin–Tsai (ξE = 2.0, ξG = 1.0) compliance S66 0.8 0.4 S22 0 –4 –2 0 Log time (min) 2 4 FIGURE 8.17 Measured and predicted creep compliances for glass–epoxy composite. (From Beckwith, S. W. 1974. Viscoelastic characterization of a nonlinear glass–epoxy composite including the effects of damage. PhD dissertation, Texas A&M University, College Station, TX. With permission.) that of the iber, so the iber modulus could be assumed to be elastic, and the time dependency of E1(t) would be governed by Em(t) alone. The results of a similar analysis of the creep compliances S22(t) and S66(t) for a glass–epoxy composite are shown in Figure 8.17 from Reference 18. From these results, it appears that the compliances can be accurately predicted by using the viscoelastic properties of the epoxy matrix in the corresponding viscoelastic forms of the Halpin–Tsai Equations 3.63 and 3.64. As mentioned earlier, Beckwith [2] showed experimentally that the creep exponent n, which governs the time dependency in the power-law expression (Equation 8.2), depends only on the polymer matrix. Similarly, Wen et al. [9] modeled transverse creep compliances of thermoplastic polymer matrix composites by applying the correspondence principle to both the Tsai–Hahn Equation 3.66 and inite element micromechanical models, and agreement with experimental results was shown to be excellent. Gibson et al. [11,12] applied the correspondence principle and inite element models to predict creep in prestressed viscoelastic composite connectors [11], and prestressed viscoelastic composite timing devices for extended interval lubricators [12]. At the macromechanical level, equations such as laminate force– deformation relationships can be converted to viscoelastic form using the correspondence principle. For example, the creep strains in a symmetric laminate under constant in-plane loading can be analyzed by 452 Principles of Composite Material Mechanics employing the correspondence principle and a quasielastic analysis to rewrite Equation 7.63 as ε 0x (t) A11 ′ (t) A12 ′ (t) A16 ′ (t) N x 0 ′ (t) A26 ′ (t) N y ε y (t) = A1′2 (t) A22 ′ (t) A26 ′ (t) A66 ′ (t) N xy γ 0xy (t) A16 (8.82) where A′ij(t) = laminate creep compliances Nx, Ny, Nxy = constant loads Sims and Halpin [19] have used these equations, along with uniaxial creep tests, to determine the creep compliances of glass/epoxy laminates for comparison with predictions. For example, the compliance A′11(t) was determined by applying a constant load Nx and by measuring the creep strain, ε 0x (t), and then using the equation A11 ′ (t) = ε 0x (t) Nx (8.83) These measured values were compared with predicted values from a combined micromechanics–macromechanics analysis that was based on the use of the correspondence principle, the Halpin–Tsai equations, and Classical Lamination Theory (CLT). The agreement between measurements and predictions was excellent, as shown in Figure 8.18. When the correspondence principle is used for problems involving sinusoidally varying stresses and strains in viscoelastic composites, we must be particularly careful to make sure that the criteria for using the effective modulus theory are met. These restrictions are discussed in more detail, and applications of the correspondence principle to the prediction of complex moduli of particle and iber composites are given in papers by Hashin [20,21]. For example, assuming that these criteria have been met, micromechanics equations such as Equation 3.27 can be modiied for the case of sinusoidal oscillations as E1* (ω) = Ef1* (ω)υf + Em* (ω )υm where E1* (ω) = longitudinal complex modulus of composite Ef1*(ω) = longitudinal complex modulus of iber Em* (ω) = complex modulus of isotropic matrix (8.84) Analysis of Viscoelastic and Dynamic Behavior 453 Log creep compliance (in.2 Ib–1) Quasi-isotropic glass–epoxy –6.370 82°F 117°F 153°F 176°F From laminated plate analysis –6.390 –6.410 –6.430 –6.450 Tr = 82°F –6.470 –6.490 –6.510 –6.530 5.0 0.0 10.0 14.0 Log t/aT (s) FIGURE 8.18 Predicted and measured creep compliance for a quasi-isotropic glass/epoxy laminate. (Reprinted from Sims, D. F. and Halpin, J. C. 1974. Composite Materials: Testing and Design (Third Conference), ASTM 546. American Society for Testing and Materials, Philadelphia, PA. Copyright ASTM. With permission.) By setting the real parts of both sides of Equation 8.84 equal, we ind the composite longitudinal storage modulus to be E1′(ω ) = Ef1′ (ω)υf + Em ′ (ω )υm (8.85) where E1′ (ω) = longitudinal storage modulus of composite Ef1′ (ω) = longitudinal storage modulus of iber E′(ω) = storage modulus of isotropic matrix Similarly, by setting the imaginary parts of both sides of Equation 8.84 equal, we ind that the composite longitudinal loss modulus is E1′′(ω ) = Ef1′′ (ω)υf + Em ′′ (ω )υm (8.86) where E1′′ (ω) = longitudinal loss modulus of composite Ef1′′ (ω) = longitudinal loss modulus of iber Em ′′ (ω) = loss modulus of isotropic matrix The composite longitudinal loss factor is found by dividing Equation 8.86 by Equation 8.85: η1(ω) = E1′′(ω) Ef1′′ (ω)υf + Em ′′ (ω )υm = E1′ (ω) Ef1′ (ω)υf + Em ′ (ω )υm (8.87) Principles of Composite Material Mechanics 454 The complex forms of the other lamina properties can be determined in a similar fashion. In studies of the complex moduli of aligned discontinuous iber composites, Suarez et al. [22] used the complex forms of * * Equations 6.24, 3.45, and 3.63 to determine E1* (ω ) , ν12 (ω ), E2* (ω) , and G12 (ω ). These properties were then substituted into the complex form of Equation 2.40 to obtain the off-axis complex modulus, Ex* (ω ) . The predicted off-axis storage moduli and loss factors for various iber orientations are compared with experimental data for a continuous iber graphite–epoxy composite in Figure 8.19, and the agreement is seen to be quite reasonable. Similar results were obtained for discontinuous iber composites, but the iber length effect is dominated by the iber orientation effect, except for iber 40 Graphite–epoxy specimens Continuous fiber Fiber volume fraction 0.675 Fiber loss factor 0.0015 30 E′x/E′m Legend 20 Corrected force-balance approach Mean experimental value Experimental scatter 10 0 0 15 30 45 60 75 90 Fiber direction (degrees) 0.06 Loss factor (η) 0.05 Graphite–epoxy specimens Continuous fiber Fiber volume fraction 0.675 Fiber loss factor 0.0015 0.04 Legend Corrected force-balance approach Mean experimental value Experimental scatter 0.03 0.02 0.01 0 0 15 30 45 60 75 90 Fiber direction (degrees) FIGURE 8.19 Predicted and measured off-axis storage modulus ratio, Ex′ /Em′ and loss factor, η, of graphite/ epoxy for various iber orientations. (From Suarez, S. A. et al. 1986. Experimental Mechanics, 26(2), 175–184. With permission.) Analysis of Viscoelastic and Dynamic Behavior 455 orientations of θ ≃ 0°. It is also interesting to note that there is an optimum iber orientation for maximizing the loss factor. Thus, damping is another design variable in composite structures. For oscillatory loading of symmetric viscoelastic laminates, Equation 7.63 can be rewritten, so that the sinusoidally varying strains are related to the sinusoidally varying loads by εɶ 0x (t) A11 ′ * (ω ) A12 ′ * (ω ) A16 ′ * (ω ) Nɶ x (t) * ɶ0 ɶ * * = ( ) ( ) ( ) ω ω ω t ( ) ( ) ε A A A N t ′ ′ ′ 22 26 y 12 y γɶ 0xy (t) A16 ′ * (ω ) A26 ′ * (ω ) A66 ′ * (ω ) Nɶ xy (t) (8.88) where A′ * (ω ) are the laminate complex extensional compliances. The laminate stiffnesses can also be written in complex form (i.e., the Aij* (ω) , Bij* (ω ), and Dij* (ω) ), and the resulting equations have been used by Sun et al. [23] and others in the studies of damping in laminates. Damping in composites will be discussed in more detail later in this chapter. 8.2.6 Temperature and Aging Effects In the previous sections of this chapter, the effects of temperature and aging on viscoelastic behavior have not been taken into account. We now consider these effects, as well as the corresponding methods of analysis. It is convenient to discuss irst the effects of temperature. In Section 8.2.2, a thermorheologically simple material was deined as having relaxation times, λi, and retardation times, ρi, which all have the same temperature dependence. Considering only the temperature dependence, the relaxation times at different temperatures can then be related by the equation λ i (T ) = aTλ i (Tr ) (8.89) where λi(T) = ith relaxation time at temperature T λi(Tr) = ith relaxation time at reference temperature, Tr aT = temperature-dependent shift factor A similar equation can be used to express the temperature dependence of the retardation times. The effect of increasing temperature is to reduce the relaxation and retardation times and to speed up the relaxation and creep processes. This “speeding up” of the viscoelastic response can also be thought of as a process operating in “reduced time” [24]. For the purpose of illustration, we now consider the effect of the temperature-dependent Principles of Composite Material Mechanics 456 relaxation times on the relaxation modulus by using the Zener single-relaxation model in Figure 8.11. The relaxation modulus at time t and temperature T is determined by modifying Equation 8.44 as C(t , T ) = k0 + k1e− t/λ1 (T ) (8.90) whereas the relaxation modulus at time t and reference temperature Tr is C(t , Tr ) = k0 + k1e− t/λ1 (Tr ) (8.91) If we let the time at the reference temperature Tr be the “reduced time,” ξ= t aT (8.92) then Equation 8.91 becomes C(ξ , Tr ) = k0 + k1e− t/aT λ1 (Tr ) = k0 + k1e− t/λ1 (T ) = C(t , T ) (8.93) Thus, the effect of changing temperature on the relaxation modulus is the same as the effect of a corresponding change in the timescale, and this is the basis of the well-known TTS Principle, or the method of reduced variables [25]. One of the most useful applications of TTS is to extend the time range of short-term creep or relaxation test data by taking such data at various temperatures and then shifting the data along the time axis to form a “master curve” at a reference temperature, as shown in Figure 8.20. However, the usefulness of the method depends on the ability to determine the shift factor, aT. When the temperature, T, is greater than the glass transition temperature, T6 > T5 > T4 > T3 > T2 > T1 > Tr T5 T4 T3 T2 T1 Tr 1 2 3 log t 4 Master curve at T = Tr log S(t) log S(t) T6 5 1 2 3 4 5 6 7 log t FIGURE 8.20 Shifting of creep data at various temperatures to generate a master curve at a reference temperature. Analysis of Viscoelastic and Dynamic Behavior 457 Tg, the shift factor can be determined empirically with the well-known Williams–Landel–Ferry (WLF) equation [25]: log aT = −c1(T − Tr ) c2 + (T − Tr ) (8.94) where c1 and c2 are material constants that must be determined from the experimental data. It has been found that when Tr is approximately 50°C above Tg, the values c1 = 8.86 and c2 = 101.6 K are valid for a variety of polymers. TTS has been successfully applied to many polymers at temperatures above Tg, but it is a different matter below the glass transition. Although TTS has been shown to be suitable for short-term creep or relaxation data at those temperatures, it does not produce valid results when applied to long-term test data. The reason is that a process called “physical aging” occurs in a polymer below Tg, and this aging process changes the viscoelastic response of the material during a long-term creep test. In a short-term test, because the test duration is much lesser than the aging time, no signiicant aging occurs during the test. Physical aging in polymers is associated with a slow loss of free volume that has been trapped in the polymer microstructure after quenching below Tg [26]. As shown in Figure 8.21, as the temperature of a polymer increases, its total volume consists of V0, the volume occupied by the polymer molecules, and VF, the so-called free volume between the molecules. Volume Total volume V = V0 + VF VF = Free volume V0 = Volume occupied by molecules Temperature Tg FIGURE 8.21 Polymer volume expansion with increasing temperature, showing how free volume increases sharply above the glass transition temperature. 458 Principles of Composite Material Mechanics Below the glass transition temperature Tg, most of the total volume is occupied by the molecules, but as the temperature increases above Tg, VF increases much faster than V0. The polymer is usually processed in its molten form at temperatures above Tg; then, when it is cooled or quenched to room temperature after molding, a signiicant amount of free volume is “locked in.” This is a thermodynamically unstable condition, and as a result, the polymer will slowly give up free volume with time, to approach a more stable thermodynamic condition. As the polymer gives up free volume, the polymer chain mobility decreases and the relaxation times increase, thus reducing the speed of the relaxation or creep [7]. Pioneering work on aging of polymers has been done by Struik [26,27], and more recent work has been reported by Janas and McCullough [28] and Ogale and McCullough [29]. Still more recently, Sullivan [30] has shown that physical aging signiicantly affects the creep behavior of polymer matrix composites. Since aging time, ta, and temperature, T, both affect the relaxation times, Sullivan [30] has suggested that a new shift factor, a(T, ta), be deined by modifying Equation 8.89 as a = a(T , ta ) = λ i (T , ta ) λ i (Tr , tar ) (8.95) where λi(T, ta) = ith relaxation time at temperature T and aging time ta λi(Tr, tar) = ith relaxation time at reference temperature Tr and reference aging time tar Struik [26] proposes that the TTS relationship for creep compliance be modiied to include aging time effects by writing S(t , T , ta ) = B(T )S( at , Tr , tar ) (8.96) where B(t) = temperature-dependent vertical shift factor S(t, T, ta) = creep compliance at time t, temperature T, and aging time ta S(at, Tr, tar) = creep compliance at shifted time at, reference temperature Tr, and reference aging time tar Note that Equation 8.96 is analogous to the TTS relationship for relaxation in Equation 8.93, and a modiied equation similar to Equation 8.96 can be written for relaxation. This new shift factor may be related to aT , the temperature shift factor below Tg, and ata, the shift factor for aging time, by the equation [30] loga = logar + logata (8.97) Analysis of Viscoelastic and Dynamic Behavior 459 log S66(t), (GPa)–1 T = 115°C θ = 45° –0.10 ta(h) 2 8 –0.20 32 160 879 –0.30 0 1.00 2.00 3.00 log t (s) 4.00 5.00 FIGURE 8.22 Effect of aging time, ta, on shear creep compliance of 45° off-axis glass–vinyl ester composite at a test temperature of 115°C. (Reprinted from Composites Science and Technology, 39, Sullivan, J. L., Creep and physical aging of composites, 207–232, Copyright 1990, with permission from Elsevier.) Figure 8.22 shows Sullivan’s data on the effect of aging time on the shear creep compliance S66(t) of a glass–vinyl ester composite [30]. Clearly, the creep rate decreases with increased aging time, indicating an increase in the relaxation times and a slowing of the creep process. Support for the conclusion that TTS works well for short-term creep at constant age is provided by additional data from Sullivan [30] in Figures 8.23 and 8.24. Figure 8.23 shows log S66(t), (GPa)–1 0 –0.10 –0.20 40°C 60°C 80°C 90°C 115°C 120°C –0.30 –0.40 –0.50 0 1.0 2.0 3.0 log t (s) 4.0 5.0 FIGURE 8.23 Momentary shear creep compliance data for glass–vinyl ester composite at various temperatures and constant aging time, ta = 166 h. (Reprinted from Composites Science and Technology, 39, Sullivan, J. L., Creep and physical aging of composites, 207–232, Copyright 1990, with permission from Elsevier.) Principles of Composite Material Mechanics log S66(t), (GPa)–1 460 –0.20 120°C 115°C 90°C 80°C 60°C 40°C –0.30 –0.40 1.0 2.0 3.0 4.0 log t (s) 5.0 6.0 FIGURE 8.24 Momentary master curve for glass–vinyl ester composite at ta = 166 h, Tr = 60°C, based on the test data from Figure 8.23. (Reprinted from Composites Science and Technology, 39, Sullivan, J. L., Creep and physical aging of composites, 207–232, Copyright 1990, with permission from Elsevier.) the short-term (or momentary) creep at various temperatures and “constant age,” where the creep testing time is limited to no more than 10% of the aging time used in preconditioning the specimens. Figure 8.24 shows the corresponding momentary master curve at a reference temperature of 60°C. Both horizontal and vertical shifting of the momentary creep data were necessary to obtain the master curve [30]. The difference between long-term creep curves and the master curve from momentary creep data is shown in Figure 8.25. Again, the conclusion is that aging slows down the creep process and that TTS does not work for long-term creep. Also shown in Figure 8.25 are predicted long-term creep curves based on effective time theory [30], which is not discussed here. In conclusion, the reader is encouraged to refer to journal review articles for more information on various aspects of viscoelastic behavior of composites. For example, Schapery [1] has summarized the theoretical approaches to modeling of viscoelastic behavior of composites, and Scott et al. [31] have published a useful review of the technical literature on creep of iberreinforced composites. EXAMPLE 8.1 Assume that the tensile isochronous stress–strain curve in Figure 8.4 is for a linear viscoelastic material at time t = t1 = 1 h, and that for a stress level σ1 = 10 MPa at t1 = 1 h, the corresponding strain ε(t1)1 = 0.004. What are the time-dependent Young’s modulus E(t1) and the time-dependent creep compliance S(t1) of the material at t1 = 1 h? log S66(t), (GPa)–1 Analysis of Viscoelastic and Dynamic Behavior 461 –0.10 MMC –0.20 –0.30 –0.40 5% 90°C 60°C 40°C 0 1.00 2.00 3.00 4.00 5.00 6.00 log t (s) FIGURE 8.25 Long-term shear creep compliance and a momentary master curve for glass–vinyl ester composite, ta = 1 h. Also shown are predicted curves from the effective time theory, which is not discussed here. (Reprinted from Composites Science and Technology, 39, Sullivan, J. L., Creep and physical aging of composites, 207–232, Copyright 1990, with permission from Elsevier.) Solution The time-dependent Young’s modulus is E(t1 ) = 10 MPa σ1 = = 2500 MPa 0.004 ε(t1 )1 and the time-dependent creep compliance is S(t1 ) = 1 1 = = 0.0004 (MPa)−1 E(t1 ) 2500 MPa EXAMPLE 8.2 A specially orthotropic, linear viscoelastic composite lamina is subjected to the shear stress–time history shown in Figure 8.26. If the effective shear creep compliance is given by S66 (t) = A + Bt , t ≥ 0; S66 (t) = 0, t < 0 where A and B are material constants and t is time, ind the expressions for the creep strain at t < T0 and t > T0. Solution The creep strain is given by Equation 8.7: t ∫ ε i (t) = Sij (t − τ) −∞ dσ j (τ) dτ dτ Principles of Composite Material Mechanics Shear stress (τ12 (t)) 462 to ∞ τmax Time (t) T0 FIGURE 8.26 Shear stress time history for Example 8.2. which, for the case of t < T0, reduces to t ∫ ε 6 (t) = γ 12 (t) = [ A + B(t − τ)] 0 Bτ Aτ max τ max t + max t 2 dτ = T0 T0 2T0 For t > T0, we have T0 t ∫ ε 6 (t) = γ 12 (t) = [ A + B(t − τ)] 0 τ max dτ + (0) dτ T0 ∫ T0 = Aτ max + Bτ maxt − Bτ maxT0 2 EXAMPLE 8.3 For the problem in Example 8.2, the effective shear compliance is to be approximated by a Kelvin–Voigt model of the form 1 (1 − e − t/λ ), when t ≥ 0 k when t < 0 S66 (t) = 0, S66 (t) = Determine the creep strain at t < T0 and t > T0. Solution For the case of t < T0, Equation 8.7 reduces to t γ 12 (t) = 1 ∫ k [1 − e 0 and for t > T0, we have − ( t − τ )/λ ] τ max τ dτ = max [t − λ(1 − e − t/λ )] T0 kT0 Analysis of Viscoelastic and Dynamic Behavior T0 γ 12 (t) = 1 ∫ k [1 − e 0 − ( t − τ )/λ ] 463 τ max τ dτ + (0) = max [T0 − λe − t/λ (eT0 /λ − 1)] T0 kT0 EXAMPLE 8.4 The ilament-wound pressure vessel described in Example 2.5 is constructed of a viscoelastic composite having creep compliances that can be modeled by using one-term series representations of the form shown in Equation 8.49. Assuming that the internal pressure, p, is constant, determine the creep strains along the principal material directions in the wall of the vessel. Solution Since the internal pressure, p, is constant, the stresses in the wall of the vessel are all constants, and we can use a quasielastic analysis to predict the creep strains. From Equation 8.60, we ind that the creep strains along the principal material directions are given by ε1 (t) = S11 (t)σ 1 + S12 (t)σ 2 ε 2 (t) = S12 (t)σ 1 + S22 (t)σ 2 and ε 6 (t) = γ 12 (t) = S66 (t)τ12 From Example 2.5, stresses along the principal material directions were found to be σ 1 = 20.5 p MPa σ 1 = 17.0 p MPa σ 6 = σ 12 = τ12 = 6.0 p MPa Substituting these stresses and the creep compliances from Equation 8.49 into the above expressions for the strains, we ind that ( ) ( ) ( ) ( ) ( ) (1) (1) ε1 (t) = S11 [1 − e − t/ρ1 ] + S11 (20.5 p) + S12 [1 − e − t/ρ1 ] + S12 (17.0p) (1) (1) ε 2 (t) = S12 [1 − e − t/ρ1 ] + S12 (20.5p) + S22 [1 − e − t/ρ1 ] + S22 (17.0p) (1) γ 12 (t) = S66 [1 − e − t/ρ1 ] + S66 (6.0 p) Principles of Composite Material Mechanics 464 EXAMPLE 8.5 The composite pressure vessel described in Examples 2.5 and 8.4 has an internal pressure p that varies sinusoidally with time, as shown in Figure 8.27. If the complex compliances of the composite material are given by * Smn (ω) = Smn ′ (ω) + iSmn ′′ (ω) determine all the time-dependent strains associated with the principal material axes. Solution From Example 2.5 and Figure 8.27, the stresses along the 12 directions are σɶ 1 (t) = 20.5 p = 20.5P sin ωt (MPa) σɶ 2 (t) = 17.0 p = 17.0P sin ωt (MPa) σɶ 6 (t) = τɶ 12 (t) = 6.0 p = 6.0P sin ωt (MPa) The corresponding strains from Equation 8.70 are * * εɶ 1 (t) = S11 (ω)σɶ 1 (t) + S12 (ω)σɶ 2 (t) + (0)σɶ 6 (t) = [S11 ′ (ω) + iS1′′1 (ω)]20.5P sin ωt + [S12 ′ (ω) + iS12 ′′ (ω)]17.0P sin ωt * * εɶ 2 (t) = S12 (ω)σɶ 1 (t) + S22 (ω)σɶ 2 (t) + (0)σɶ 6 (t) = [S12 ′ (ω) + iS12 ′′ (ω)]20.5P sin ωt + [S22 ′ (ω) + iS22 ′′ (ω)]17.0P sin ωt * * * (ω)τɶ 12 (t) εɶ 6 (t) = γɶ 12 (t) = S66 (ω)σɶ 6 (t) = S66 = [S66 ′ (ω) + iS66 ′′ (ω)]6.0P sin ωt EXAMPLE 8.6 Derive the equation for the complex modulus of the Kelvin–Voigt spring– dashpot model described in Figure 8.9. P(t) p(t) = P sin ωt P t P FIGURE 8.27 Sinusoidally varying pressure for Example 8.5. Analysis of Viscoelastic and Dynamic Behavior Solution The differential equation for the Kelvin–Voigt model is given by Equation 8.39 as σ = kε + µ dε dt For sinusoidally varying stress and strain, the stress–strain relationship can be expressed as σeiωt σɶ (t) = σeiωt = [E* (ω)]εɶ (t) or εɶ (t) = * E (ω) where E*(ω) is the complex modulus and ω is the frequency. Substituting this stress–strain relationship into the differential equation for the Kelvin–Voigt model, we ind that σeiωt = k iωσeiωt σeiωt +µ * * E (ω) E (ω) Solving for the complex modulus, we obtain E* (ω) = k + iωµ Note that the creep compliance, the relaxation modulus, and the complex modulus are all expressed in terms of the Kelvin–Voigt model parameters k and µ. Similar relationships can be derived for the other spring–dashpot models. EXAMPLE 8.7 Using the Elastic–Viscoelastic Correspondence Principle, set up a micromechanics model for predicting the transverse creep compliance, S22(t), of a unidirectional composite, which consists of linear elastic isotropic ibers in a linear viscoelastic isotropic polymer matrix. Solution One approach is to start with a micromechanics equation for the transverse elastic modulus such as the semiempirical Tsai–Hahn Equation 3.66 1 1 υ f η2 υ m = + E2 υf + η2 υm Ef Em 465 Principles of Composite Material Mechanics 466 Converting this equation to compliances, S22 = 1 [Sf υf + η2υmSm ] υ f + η2 υ m where Sf = 1/Ef, Sm = 1/Em, and S22 = 1/E2 are the elastic compliances of iber, matrix, and transverse composite materials, respectively. Now using the correspondence principle and the assumption that the ibers are elastic, whereas the matrix is viscoelastic, the equation for the transverse creep compliance of the composite is S22 (t) = 1 [Sf υf + η2 υmSm (t)] υ f + η2 υ m where Sm(t) is the creep compliance of the viscoelastic matrix material, which would need to be measured in a creep test of the pure matrix material. Creep testing will be discussed in more detail in Chapter 10. EXAMPLE 8.8 The momentary master curve for the shear creep compliance, S66(t), of a unidirectional glass–vinyl ester composite at a reference temperature of 60°C and a reference aging time of 166 h is shown on a log–log scale in Figure 8.24. (a) Neglecting aging effects, determine the time required to reach compliance of 0.63 GPa−1 at a temperature of 60°C and (b) neglecting vertical shifting, estimate the time required to reach the same compliance of 0.63 GPa−1 at a temperature of 100°C. From experimental data, it is known that for this material, the WLF parameters are c1 = −1.01 and c2 = −89.2. Solution a. From Figure 8.24, at a value of log S66(t) = log(0.63) = 0.2, the corresponding value from the curve is log t = 6, and so t = 106 s at T = 60°C b. From Equation 8.96, we have S66 (t , T , ta ) = B(T )S66 ( at , Tr , tar ) Since we neglect vertical shifting, B(t) = 1. Since the data are for a constant aging time, we have a = aT and Equation 8.96 becomes S66 (t , T ) = S66 ( at , Tr ) = S66 ( aTt , Tr ) where the shift factor, aT is found from the WLF equation log aT = −c1 (T − Tr ) −(−1.01)(100 − 60) = = −0.8211 c2 + (T − Tr ) −89.2 + (100 − 60) Analysis of Viscoelastic and Dynamic Behavior 467 or aT = 0.151, which means that aTt = 0.151(106) = 1.51 × 105 s. Thus, the creep compliance curve at 100°C is shifted to the left of the curve at the reference temperature of 60°C, and it takes only 15% as much time to reach the compliance of 0.63 GPa−1 at 100°C as it does at 60°C. EXAMPLE 8.9 The transverse relaxation modulus of an orthotropic lamina is deined as E2(t) = Ae−t over the time interval 0 ≤ t ≤ ∞ and E2(t) = 0 for all other times t, where A is a constant. Find the corresponding equation for the complex transverse modulus,E2* (ω) = E2′ (ω) + iE2′′(ω) , where E′2 (ω) is the transverse storage modulus, E2" (ω) is the transverse loss modulus, and ω is the frequency in radians per second. Solution The Fourier transform of the time-varying function f(t) is given by F(ω) = ∫ ∞−∞ f (t)e − iωtdt . It is important to note that such an integral exists only when f(t) is deined and bounded over the region −∞ ≤ t ≤ ∞, and when the integral ∫ ∞−∞|f (t)|dt is convergent. These conditions are satisied by the given function E2(t), so the Fourier transform of E2(t) is given by E2 (ω) = = ∫ ∞ −∞ E2 (t)e − iωtdt = ∫ ∞ Ae − t e − iωtdt = A 0 ∫ ∞ e −(1+ iω )tdt 0 A − A(e −(1+ iω )( ∞ ) − e −(1+ iω )( 0 ) ) = 1 + iω 1 + iω Using Equation 8.72 and multiplying both numerator and denominator by the complex conjugate of (1 + iω), the complex transverse modulus is E2* (ω) = iωE2 (ω) = Aω 2 + iAω iAω iAω(1 − iω) = = 1 + iω (1 − iω)(1 + iω) 1 + ω2 Therefore, the transverse storage and loss moduli are, respectively, E2′ (ω) = Aω 2 1 + ω2 and E2′′(ω) = Aω 1 + ω2 PROBLEM 8.1 The isochronous stress–strain curves for an epoxy material at different times are shown in Figure 8.28. This material is used as the matrix in a unidirectional E-glass–epoxy composite having a iber volume fraction of 0.6. Using micromechanics and the Elastic–Viscoelastic Correspondence Principle, determine the longitudinal relaxation modulus E1(t) for the composite at t = 1 h and t = 10,000 h. Note that the strain in Figure 8.28 is given in percent Principles of Composite Material Mechanics 468 3.0 ct ed oj e pr h 0 00 10 15 2.5 0, 100 0 500 h 0h 10,0 00 h 1h 10 h 100 h 20 1.5 10 Stress level (103 psi) Stress level (MPa) 2.0 1.0 5 0.5 0 0 0.5 1.0 1.5 2.0 2.5 Total strain, % at indicated stress and time mm/mm or in./in. × 100 FIGURE 8.28 Isochronous stress–strain curves for epoxy matrix material in Problem 8.1. strain (e.g., a percent strain value of 1.5 corresponds to a strain of 0.015). Elastic properties of ibers are given in Table 1.1. PROBLEM 8.2 A thin-walled cylindrical pressure vessel has mean diameter d = 18 in. and wall thickness h = 0.25 in. The vessel is made of ilament-wound unidirectional composite material with all ibers oriented in the circumferential, or hoop, direction. The internal pressure in the vessel can be assumed to be constant. From creep tests of specimens of the unidirectional composite material, it is found that the principal creep compliances can be described by the following power-law expressions: S11(t) = 0.121 + 0.0003t 0.19 S12 (t) = −0.0315 + 0.004t 0.19 S22 (t) = 0.3115 + 0.0025t 0.19 S66 (t) = 0.839 + 0.003t 0.19 Analysis of Viscoelastic and Dynamic Behavior 469 where t is the time in minutes and all compliances are given in units of (×10−6 psi−1). The ultimate failure strains for the material are found to be as follows: e(+) e(+) eLT = 0.010 L = 0.0194, T = 0.00125, a. According to the maximum strain criterion, what is the allowable internal pressure in the vessel, if it is to be designed to last for at least 20 years under constant pressure? b. How would you change the design of the vessel so as to increase the allowable internal pressure, while maintaining the 20-year design life? PROBLEM 8.3 For a linear viscoelastic material, the creep response under a constant stress is followed by a “recovery response” after the stress is removed at some time, t0. Using the Boltzmann Superposition Principle, ind an expression for the uniaxial recovery compliance, R(t) for times t > t0 in terms of the creep compliance, S(t), the time of stress removal, t0, and the time, t. PROBLEM 8.4 In general, the creep compliances, Sij(t) and the relaxation moduli, Cij(t) are not related by a simple inverse relationship. Show that only when t → 0 and when t → ∞, can we say that [Cij (t)] = [Sij (t)]−1 PROBLEM 8.5 The shear creep compliance, S66(t) for a unidirectional viscoelastic composite is given by S66(t) = γ12(t)/τ12, where γ12(t) is the time-dependent shear creep strain and τ12 is the constant shear stress. If S66(t) can be approximated by a power law as S66(t) = atb, where a and b are material constants and t is time, determine the “constant loading rate compliance” U66(t) = γ12(t)/τ12(t), where the shear stress is due to a constant loading rate, so that τ12(t) = Kt, where K is a constant. PROBLEM 8.6 The time-dependent axial stress, σx(t) and the time-dependent circumferential stress, σy(t) in the wall of the ilament-wound, thin-walled composite pressure vessel shown in Figure 8.29 are caused by the internal pressure p(t), where t is time. The required dimensions of the vessel are the wall thickness h and the mean radius r. Note that x and y are not the principal material axes, but, rather, are the longitudinal and transverse axes for the vessel. The Principles of Composite Material Mechanics 470 σy(t) y y 2r x x σx(t) h Pressure p(t) Pressure vessel p0 2T0 T0 Time (t) FIGURE 8.29 State of stress in composite pressure vessel and variation of internal pressure with time for Problem 8.6. variation of p(t) with time is also shown in Figure 8.29. If the creep compliances associated with the x and y axes are given in contracted notation by Sij (t) = Eij + Fijt , i , j = 1, 2, … , 6 where Eij and Fij are material constants, determine all the time-dependent strains along the x and y axes for t > 2T0. Answers should be given in terms of p0, r, h, T0, t, and the individual Eij and Fij . PROBLEM 8.7 A linear viscoelastic, orthotropic lamina has principal creep compliances given in contracted notation by Sij (t) = Eij = Fijt , i , j = 1, 2,. . ., 6 where Eij and Fij are material constants and t is time. The lamina is subjected to plane stress with constant stresses σ i (t) = σ ′ i H (t), i , j = 1, 2,. . ., 6 where σ′i are constants and H(t) is the unit step function. If the failure strains for pure longitudinal, transverse, and shear loading of the lamina are eL, eT, and eLT, respectively, ind the expressions for the time to failure for each of the three strains. Analysis of Viscoelastic and Dynamic Behavior 471 PROBLEM 8.8 Derive the equations for the stress–strain relationship, the creep compliance, and the relaxation modulus for the Kelvin–Voigt model. PROBLEM 8.9 Derive the equations for the stress–strain relationship, the creep compliance, and the relaxation modulus for the Zener model. PROBLEM 8.10 Derive Equation 8.45. PROBLEM 8.11 Derive Equation 8.47. PROBLEM 8.12 The shear relaxation modulus, G12(t), for an orthotropic lamina is idealized, as shown in Figure 8.30. Find the corresponding equations for the shear storage modulus, G12 ′ (ω) and the shear loss modulus, G12 ′′ (ω ), and draw sketches of both parts of the complex modulus in the frequency domain. PROBLEM 8.13 For the Maxwell model in Figure 8.8, express the storage modulus, E′(ω), the loss modulus, E″(ω), and the loss factor, η(ω), in terms of the parameters µ and k and the frequency ω. Sketch the variation of E′(ω), E″(ω), and η(ω) in the frequency domain. It is not necessary to use Fourier transforms here. G12(t) PROBLEM 8.14 The composite pressure vessel in Problem 8.6 is subjected to an internal pressure that varies sinusoidally with time according to the relationship p(t) = P0 sin t, and the principal complex compliances are given by A T Time (t) FIGURE 8.30 Variation of shear relaxation modulus, G12(t) with time for Problem 8.12. Principles of Composite Material Mechanics 472 * Smn (ω ) = Smn ′ (ω ) + iSmn ′′ (ω ), m, n = 1, 2, … , 6 where ω is the frequency. Determine all the time-dependent strains associated with the x and y axes in terms of P0, r, h, ω, and the individual Smn ′ (ω ) and Smn ′′ (ω). PROBLEM 8.15 The polymer matrix material in a linear viscoelastic, unidirectional composite material has a relaxation modulus that can be characterized by the Maxwell model in Figure 8.8. The ibers are assumed to be linear elastic. If the composite longitudinal strain–time history is as shown in Figure 8.31, express the composite longitudinal stress as a function of time. PROBLEM 8.16 The matrix material in a linear viscoelastic, unidirectional composite material is to be modeled by using a Maxwell model having parameters km and µm, whereas the iber is to be modeled by using a Kelvin–Voigt model having parameters kf and µf. a. Determine the complex extensional moduli of iber and matrix materials in terms of the Maxwell and Kelvin–Voigt parameters and the frequency, ω. b. Determine the complex longitudinal modulus of the unidirectional composite. Assume that iber and matrix materials are isotropic. It is not necessary to use the Fourier transforms. PROBLEM 8.17 The dynamic mechanical behavior of an isotropic polymer matrix material may be characterized by two independent complex moduli such as the complex extensional modulus, E*(ω) and the complex shear modulus, G*(ω). Based on experimental evidence, however, the imaginary parts of E*(ω) and G*(ω) Strain ε1(t) to ∞ 3ε0 ε0 t0 Time (t) FIGURE 8.31 Composite longitudinal strain–time history for Problem 8.15. Analysis of Viscoelastic and Dynamic Behavior 473 are not independent, because the material can be assumed to be viscoelastic in shear but elastic in dilatation (i.e., the shear modulus, G*(ω) is complex and frequency dependent, but the bulk modulus, k is real and frequency independent). Use this simplifying assumption to develop an expression for the shear loss factor, ηG(ω) in terms of the extensional loss factor, ηE(ω), the extensional storage modulus, E′(ω), and the bulk modulus, k. Assume all loss factors ≪ 1. PROBLEM 8.18 A drive shaft in the shape of a hollow tube and made of a linear viscoelastic angle-ply laminate is subjected to a torque, T, as shown in Figure 8.32. Develop an analytical model for predicting the vibratory shear deformation in the shaft from the vibratory shear force, N xy (t), when the torque T varies sinusoidally with time. The input to the model should include the properties and volume fractions of iber and matrix materials, lamina orientations, and lamina-stacking sequences. That is, the model should include both micromechanical and macromechanical components. No calculations are necessary, but the key equations should be described, all parameters should be deined, and key assumptions should be delineated. PROBLEM 8.19 Part of the required input to the viscoelastic option in some inite element codes is a table showing the time-dependent, isotropic shear modulus G(t) at different times t. Explain how you would generate such a table from tensile isochronous stress–strain curves such as the ones in Figure 8.28. Include the key equations and a list of assumptions in your explanation. PROBLEM 8.20 For the Maxwell model shown in Figure 8.8, it can be shown that the complex modulus is given by E *(ω) = E′(ω)[1 + iη(ω)] T y t x θ T θ D Nxy FIGURE 8.32 Composite drive under applied torque for Problem 8.18. 474 Principles of Composite Material Mechanics where the frequency-dependent storage modulus is given by E′(ω) = k ω 2λ 2 1 + ω 2λ 2 and the frequency-dependent loss factor is given by η(ω) = 1 ωλ where ω is the frequency and λ = µ/k is the relaxation time. Let us assume that the Maxwell model adequately describes the viscoelastic behavior of a particular material. Explain how you would use the Maxwell model and frequency-domain vibration test data to indirectly determine the numerical value of the relaxation modulus C(t) for this material. 8.3 Dynamic Behavior of Composites In this section, the basic concepts of dynamic behavior of composites will be introduced by discussing wave propagation, vibration, and damping of specially orthotropic composites without coupling. Only 1D wave propagation without dispersion, relection, or refraction will be considered, as 3D wave propagation, wave dispersion, and relection/refraction effects are beyond the scope of this book. For detailed discussions on these topics, the reader is referred to publications by Christensen [4], Hearmon [32], Achenbach [33], Ross and Sierakowski [34], and Moon [35]. Longitudinal vibrations of composite bars and lexural vibrations of composite beams and plates without coupling will also be considered. Vibrations of laminates with coupling and laminated plate boundary conditions other than the simply supported ones will not be emphasized. These topics are discussed in detail in books by Whitney [36], Vinson and Sierakowski [37], and Sierakowski and Chaturvedi [38]. The use of the Elastic–Viscoelastic Correspondence Principle and a strain energy method to analyze damping in composites will also be discussed. The basic premise of all analyses presented in this section is that the criteria for valid use of the effective modulus theory have been met. That is, the scale of the inhomogeneity, d, is assumed to be much smaller than the characteristic structural dimension, L, and the characteristic wavelength of the dynamic stress distribution, λ (d ≪ L and d ≪ λ in Figure 8.7). Thus, all heterogeneous composite material properties are assumed to be effective properties of equivalent homogeneous materials. If the wavelength is not long in comparison with the scale of the inhomogeneity in the material, the Analysis of Viscoelastic and Dynamic Behavior 475 wave shape is distorted as it travels through the material, and this is referred to as dispersion. Dispersion in composites has been discussed in several previous publications [4,33,35,38]. 8.3.1 Longitudinal Wave Propagation and Vibrations in Specially Orthotropic Composite Bars As will be shown in any book on vibrations [39], longitudinal wave propagation and vibration in a homogeneous, isotropic, linear elastic bar (Figure 8.33) are governed by the 1D wave equation ∂ ∂u ∂ 2u AE = ρA 2 ∂x ∂x ∂t (8.98) where x = distance from the end of the bar t = time u = u(x,t) is the longitudinal displacement of a cross section in the bar at a distance x and time t A = A(x) is the cross-sectional area of the bar ρ = mass density of the bar E = E(x) is the modulus of elasticity of the bar It is assumed that the displacement u(x, t) is uniform across a given cross section. Using effective modulus theory for a heterogeneous, specially orthotropic, linear elastic composite bar, we simply replace the properties ρ and E with the corresponding effective properties of an equivalent homogeneous material. The effective modulus E then depends on the orientation of ibers relative to the axis of the bar. For ibers oriented along the x-direction, E = E1; for ibers oriented along the transverse direction, E = E2; and for a specially orthotropic laminate, we use the effective laminate engineering constant E = Ex. For laminates with coupling, the analysis is much more dificult, as shown in Section 8.3.3. If the area and the modulus are not functions of position, x, Equation 8.98 reduces to c2 ∂ 2u ∂ 2u = ∂x 2 ∂t 2 ρ, A, E x L FIGURE 8.33 Bar of density ρ, cross-sectional area A, modulus E, and length L, ixed on both ends. (8.99) Principles of Composite Material Mechanics 476 where c = E/ρ is the wave speed. The most common solutions to the 1D wave equation are of the d’Alembert type or the separation of variables type. The d’Alembert solution is of the form u( x , t) = p( x + ct) + q( x − ct) (8.100) The function p(x + ct) represents a wave traveling to the left with velocity c. That is, a point located at ξ = x + ct moves to the left with velocity c if ξ is a constant, since x = ξ − ct. Similarly, q(x − ct) represents a wave traveling to the right with velocity c. For a sine wave, we have u( x , t) = A sin 2π 2π ( x + ct) + A sin ( x − ct) λ λ (8.101) where λ is the wavelength. Note that this is the wavelength that must be greater than the scale of the inhomogeneity, d, in order for the effective modulus theory to be valid. Alternatively, we can write Equation 8.101 as u( x , t) = A sin(2πkx + ωt) + A sin( 2πkx − ωt) (8.102) where k = 1/λ = wave number = the number of wavelengths per unit distance ω = 2πc/λ = frequency of the wave Using trigonometric identities, we ind that u( x , t) = 2 A sin 2πkx cos ωt (8.103) which represents a standing wave of proile 2A sin2πkx, which oscillates with frequency ω. Generally, the combined wave motion in opposite directions is caused by relections from the boundaries. Thus, wave propagation without relection will not lead to a standing wave (or vibration). A separation of variables solution is found by letting u( x , t) = U ( x)F(t) (8.104) where U(x) is a function of x alone and F(t) is a function of t alone. Substituting this solution into Equation 8.99 and separating variables, we obtain c2 1 d 2U 1 d 2 F = U dx 2 F dt 2 (8.105) Analysis of Viscoelastic and Dynamic Behavior 477 The left-hand side of Equation 8.105 is a function of x alone and the righthand side is a function of t alone; therefore, each side must be equal to a constant. If we let this constant be, say, −ω2, then Equation 8.105 gives the two ordinary differential equations, d2F + ω2F = 0 dt 2 (8.106a) 2 d 2U ω + U = 0 dx 2 c (8.106b) and the solutions to these equations are of the form F(t) = A1 sin ωt + B1 cos ωt (8.107) ω ω U ( x) = A2sin x + B2cos x c c (8.108) where A1 and B1 depend on the initial conditions and A2 and B2 depend on the boundary conditions. For a bar that is ixed at both ends (Figure 8.33), the substitution of the boundary conditions u(0, t) = u(L, t) = 0 leads to the conclusion that B2 = 0 and ω sin L = 0 c (8.109) Equation 8.109 is the eigenvalue equation, which has an ininite number of solutions, ωn, such that ω nL = nπ c (8.110) where n = mode number = 1,2,3, …, ∞ ωn = eigenvalues, or natural frequencies (rad/s) = 2πfn fn = natural frequencies (Hz) Thus, fn = nc n E = 2L 2L ρ 1/2 (8.111) Principles of Composite Material Mechanics 478 For the nth mode of vibration, the displacements are then nπx un ( x , t) = ( A′ sin ω nt + B′ cos ω nt) sin L (8.112) where A′ = A1 A2 and B′ = B1 A2. The mode shape for the nth mode is given by the eigenfunction nπx U n ( x) = sin L (8.113) and the general solution is the superposition of all modal responses ∞ u( x , t) = ∑(A′sinω t + B′cosω t)sin n n n =1 nπx L (8.114) Mode shapes, natural frequencies, and wavelengths for the irst three modes of the ixed–ixed bar are shown in Figure 8.34. An important point U1(x) n=1 x L U2(x) f1 = 1 2L E ρ ; λ1 = 2L n=2 x f2 = 1 L L 2 E ; ρ λ2 = L L U3(x) n=3 L 3 x f3 = 3 2L 2L E ρ ; λ3 = 3 2L 3 L FIGURE 8.34 Mode shapes, natural frequencies, and wavelengths for the irst three modes of longitudinal vibration of a bar with both ends ixed (Figure 8.33). Analysis of Viscoelastic and Dynamic Behavior 479 is that as the mode number increases, the wavelength decreases and the use of effective modulus theory becomes more questionable. In general, the wavelengths associated with typical mechanical vibration frequencies of structures in the audio frequency range will satisfy the effective modulus criterion d ≪ λ. However, the wavelengths associated with ultrasonic wave propagation may be short enough to cause concern about the use of effective modulus theory. Validation of the application of effective modulus theory to the 1D wave equation has been demonstrated. For example, a comparison of measured and predicted wave speeds in unidirectional stainless-steel ilamentreinforced epoxy rods was reported by Ross and Sierakowski [34] and Sierakowski and Chaturvedi [38]. Figure 8.35 shows drawings of the (a) longitudinal and (b) transverse composite rod specimens. Stress waves in the specimens were induced by using a gas gun to propel short epoxy striker rods against one end of the specimens, and strain gages separated by known distances were used to measure the wave speeds. Stress wavelengths were much greater than the diameters of the ilaments, so the use of effective modulus theory was valid. The predicted longitudinal wave speeds, c1, were calculated from the 1D wave speed equation, the rule of (a) (b) FIGURE 8.35 Unidirectional composite rods with longitudinal (a) and transverse (b) ilaments. (Sierakowski, R. L. and Chaturvedi, S. K. Dynamic Loading and Characterization of Fiber-Reinforced Composites. 1997. Copyright Wiley-VCH Verlag GmbH & Co. KGaA. New York, NY. Reproduced with permission.) Principles of Composite Material Mechanics 480 mixtures for the longitudinal modulus, and the corresponding rule of mixtures for composite density as c1 = E1 = ρc Ef υf + Em υm ρf υf + ρm υm (8.115) while the transverse wave speeds, c2, were calculated from the 1D wave speed equation, the semiempirical Halpin–Tsai equations for transverse modulus and the rule of mixtures for composite density as c2 = E2 Em (1 + ξηυf ) = ρc (1 − ηυf )(ρf υf + ρm υm ) (8.116) where η= (Ef /Em ) − 1 (Ef /Em ) + ξ (8.117) and the Halpin–Tsai parameter was assumed to be ξ = 2 as mentioned in Section 3.5. Measured and predicted wave speeds for composites having several iber volume fractions and iber diameters show good agreement, as shown in Figure 8.36. The equations developed in this section are instructive not only from the point of view of the limitations of effective modulus theory, but also for material characterization as well. The two basic approaches to measurement of dynamic mechanical properties of materials involve the use of either wave propagation experiments or vibration experiments. Assuming that the criteria for the use of effective modulus theory have been met, the effective modulus of a specially orthotropic composite can be determined by measuring the longitudinal wave speed, c, in a specimen of density, ρ, and then solving for E = c2ρ. Alternatively, the nth mode natural frequency, fn, can be measured in a vibration experiment, and the effective modulus can be found from an equation such as Equation 8.111. Dynamic mechanical testing of composites will be discussed in more detail in Chapter 10. Finally, the equations presented here can be modiied for linear viscoelastic composites in sinusoidal vibration by using the Elastic–Viscoelastic Correspondence Principle. This means that the effective modulus E will be replaced by the complex modulus E*(ω). Alternatively, the stress–strain relationship used in deriving the equation of motion could be an equation of the form shown in Equation 8.28 or a special case of that equation. Analysis of Viscoelastic and Dynamic Behavior 481 5 Longitudinal Wave speed (km/s) 4 3 2 Transverse 1 0.406 mm dia. fiber 0.203 mm dia. fiber 0 0 20 60 40 80 100 Volume percent of fiber FIGURE 8.36 Comparison of predicted and measured longitudinal and transverse wave speeds for stainless-steel ilament-reinforced epoxy rods. (Sierakowski, R. L. and Chaturvedi, S. K. Dynamic Loading and Characterization of Fiber-Reinforced Composites. 1997. Copyright Wiley-VCH Verlag GmbH & Co. KGaA. New York, NY. Reproduced with permission.) 8.3.2 Flexural Vibration of Composite Beams Transverse or lexural motion of a homogeneous, isotropic, linear elastic beam (Figure 8.37) without shear or rotary inertia effects is described by the well-known Bernoulli–Euler equation − ∂ 2 ∂ 2w ∂ 2w EI 2 = ρA 2 2 ∂x ∂x ∂t ρ, A, EI x L FIGURE 8.37 Cantilever beam for the Bernoulli–Euler beam theory. (8.118) 482 Principles of Composite Material Mechanics where I = area moment of inertia of the cross section about the centroidal axis of the beam w = w(x, t) is the transverse displacement of the centroidal axis of the beam x, t, ρ, A, and E are as deined in Equation 8.98 If the beam is such that EI is constant along the length, Equation 8.118 reduces to ∂ 4w ∂ 2w EI 4 + ρA 2 = 0 ∂t ∂x (8.119) Assuming that the criteria for the use of effective modulus theory have been met, these equations can be used for specially orthotropic composites or laminates without coupling if the modulus E is replaced by the effective lexural modulus Ef. Recall that, depending on the laminate coniguration, Ef may be found from equations such as Equation 7.8, 7.9, 7.73, or 7.74. For laminates with coupling, the equations of motion based on the CLT will be developed in the next section. As an example of a solution of the Bernoulli–Euler equation, consider a separation of variables solution for harmonic free vibration: w( x , t) = W ( x)eiωt (8.120) where ω is the frequency and W(x) is the mode shape function. Substituting this solution into Equation 8.119 yields d 4W ( x) − k 4W ( x) = 0 dx 4 (8.121) where k = (ω2 ρA/EI)1/4. The solution for Equation 8.121 is of the form W ( x) = C1 sin kx + C2 cos kx + C3 sinh kx + C4 cosh kx (8.122) where the constants C1, C2, C3, and C4 depend on the boundary conditions. For example, for a cantilever beam (Figure 8.37), the four boundary conditions yield the following relationships: W ( x) = 0 when x = 0; therefore, C2 = −C4 dW ( x) = 0 when w = 0; therefore, C1 = −C3 dx d 2W ( x) = 0 when x = L dx 2 Analysis of Viscoelastic and Dynamic Behavior 483 Therefore, C1(sin kL + sinh kL) + C2(cos kL + cosh kL) = 0. d 3W ( x) = 0 when x = L dx 3 Therefore, C1(cos kL + cosh kL) + C2(sin kL − sinh kL) = 0. For nontrivial solutions C1 and C2 in the last two equations, the determinant of the coeficients must be equal to zero and cos kL cosh kL + 1 = 0 (8.123) This is the eigenvalue equation for the cantilever beam, which has an ininite number of solutions, knL. The subscript n refers to the mode number. The eigenvalues for the irst three modes are k1L = 1.875, k 2L = 4.694, k 3 L = 7.855 (8.124) Substituting the eigenvalues in the deinition of k (see Equation 8.121 and rearranging), then using the relationship ω = 2πf, we have the frequency equation fn = (k n L)2 EI 2πL2 ρA 1/2 (8.125) The mode shape function for the nth mode is then Wn ( x) = C2 [cos k n x − cosh k n x + σ n (sin k n x − sinh k n x)] (8.126) where σn = sink n L − sinhk n L cosk n L + coshk n L The mode shapes and frequencies for the irst three modes of the cantilever beam are shown in Figure 8.38. The effect of increasing the mode number and the corresponding reduction in wavelength is again apparent. If transverse shear and rotary inertia effects are included in the derivation of the equation of motion for transverse vibration of a beam, the result is the well-known Timoshenko beam equation [40]: ∂ 4w EIρ ∂ 4 w ∂ 2 w Jρ ∂ 4 w EI 4 + ρA 2 + J − + =0 FG ∂t 4 FG ∂x 2∂t 2 ∂t ∂x (8.127) Principles of Composite Material Mechanics 484 n=1 f1 = (1.875)2 2πL2 EI ρA f2 = (4.694)2 2πL2 EI ρA f3 = (7.855)2 2πL2 EI ρA L n=2 0.783L L n=3 0.5L 0.868L L FIGURE 8.38 Mode shapes and natural frequencies for the irst three modes of lexural vibration of the cantilever beam in Figure 8.37. where J = rotary inertia per unit length F = shape factor for the cross section G = shear modulus This equation can also be used for specially orthotropic composites and laminates without coupling by replacing E and G with the effective lexural modulus, Ef, and the effective through-the-thickness shear modulus, respectively, for the composite. For example, for a unidirectional, transversely isotropic composite with the ibers along the beam axis, the appropriate shear modulus to use is G = G13 = G12. If the ibers are oriented in the transverse direction, G = G23. Both shear and rotary inertia effects become more important as the mode number increases, and both effects reduce the natural frequencies below the Bernoulli–Euler values. The beam length-to-thickness ratio, L/h, is an important factor in the determination of the shear effect, with decreasing L/h generating increased shear effects. It appears that for highly anisotropic composite beams, shear effects may be signiicant unless L/h is greater than about 100 [41]. The transverse shear effect is also strongly Analysis of Viscoelastic and Dynamic Behavior 485 dependent on the ratio E/G, which is much greater for composite beams than for isotropic beams. For a typical isotropic metal E/G ≃ 2.6, but for composites such as unidirectional carbon/epoxy, E1/G12 ≃ 20 or higher. Sandwich beams with foam or honeycomb cores have even higher E/G ratios due to the low shear stiffness and high volume fraction of the core and are very susceptible to transverse shear effects. As in the previous section, the equations developed here can be used in dynamic mechanical testing to determine the effective moduli of a composite specimen. The equations can also be converted to linear viscoelastic form by replacing the elastic moduli with the corresponding complex moduli, or by deriving the equation of motion from a viscoelastic stress–strain relationship. More sophisticated analytical models for vibrating composite beams, including various effects such as viscoelastic behavior, transverse shear, and bending–twisting coupling, have been developed [36,37,38,42–44], but these are beyond the scope of this book. 8.3.3 Transverse Vibration of Laminated Plates Although the equations for vibration of composite beams in the previous section are useful, they are limited to laminates without coupling. The more general equations of motion for transverse vibration of a laminated plate can be derived by modifying the static equilibrium equations that were developed for the analysis of static delections of laminated plates in Section 7.9. For example, according to Newton’s second law, Equation 7.126 must now be modiied, so that the summation of forces along the x-direction in Figure 7.47 is given by N x dy + ∂N xy ∂N x dx dy + N xy dx + dx dy ∂x ∂y − N x dy − N xy dx = ρ0 dx dy ∂ 2u 0 ∂t 2 (8.128) where ρ0 = mass per unit area of laminate (equal to ρh) ρ = mass density of laminate is the mass per unit volume h = thickness of laminate (since t is used for time here) u0 = u0(x, y, t) is the middle surface displacement in the x-direction Equation 8.128 may be simpliied as ∂ 2u 0 ∂N x ∂N xy = ρ0 2 + ∂y ∂t ∂x (8.129) Principles of Composite Material Mechanics 486 Similarly, the summation of forces along the y-direction yields N x dx + ∂N xy ∂N x dx dy + N xy dy + dx dy ∂y ∂x − N y dx − N xy dy = ρ0 dx dy ∂ 2v 0 ∂t 2 (8.130) or ∂N y ∂N xy ∂ 2v 0 = ρ0 2 + ∂x ∂t ∂y (8.131) where v0 = v0(x, y, t) is the middle surface displacement in the y-direction. The summation of forces along the z-direction gives Qx dy + ∂Q y ∂ Qx dx dy + Qy dx + dx dy − Qx dy ∂x ∂y − Qydx + q( x , y ) = ρ0 ∂ 2w ∂t 2 (8.132) or ∂ 2w ∂ Qx ∂ Q y + q( x , y ) = ρ0 2 + ∂y ∂t ∂x (8.133) where w = w(x, y, t) is the displacement in the z-direction. For moment equilibrium, we consider the moments about the x-and the y-axis, while neglecting rotary inertia. Thus, the summation of moments about the x-axis gives − M ydx − ∂M y ∂Mxy dy dx − Mxydy − dx dy + Qydx dy ∂y ∂x + ∂Q y dy dx dy + q( x , y )d dx dy dy/2 + Qx dy dy/2 ∂y + ∂ Qx dx dy dy/2 + M ydx + Mxydy − Qxdy dy/2 = 0 ∂x Simplifying and neglecting products of differentials, we obtain (8.134) Analysis of Viscoelastic and Dynamic Behavior ∂M y ∂Mxy = Qy + ∂x ∂y 487 (8.135) A similar summation of moments about the y-axis gives ∂Mx ∂Mxy + = Qx ∂x ∂y (8.136) Substitution of Equations 8.135 and 8.136 into Equation 8.133 yields ∂ 2 Mxy ∂ 2 M y ∂ 2w ∂ 2 Mx + = + + 2 q x y ( , ) ρ 0 ∂y 2 ∂t 2 ∂x ∂y ∂x 2 (8.137) Equations 8.129, 8.131, and 8.137 are differential equations of motion of the plate in terms of stress and moment resultants. The corresponding equations of motion in terms of displacements can be derived by substituting the laminate force–deformation Equation 7.44, the strain–displacement relations (7.32), and the curvature–displacement Equation 7.33 into Equations 8.129, 8.133, and 8.137. The resulting equations are A11 ∂ 2u 0 ∂ 2u 0 ∂ 2u 0 ∂ 2v 0 ∂ 2v 0 ∂ 2v 0 2 + A + A + A + ( + ) A A + A 12 66 16 16 66 26 ∂x 2 ∂x ∂y ∂y 2 ∂x 2 ∂x ∂y ∂y 2 − B11 A16 (8.138) ∂ 2u 0 ∂ 2u 0 ∂ 2u 0 ∂ 2v 0 ∂ 2v 0 ∂ 2v 0 A A 2 A + + A + A + ( ) + + A 26 66 12 66 26 22 ∂x 2 ∂x ∂y ∂y 2 ∂x 2 ∂x ∂y ∂y 2 − B16 D11 ∂3w ∂3w ∂3w ∂3w ∂ 2u 0 − 3B16 2 − (B12 + 2B66 ) − B26 3 = ρ0 2 3 2 ∂x ∂x ∂y ∂x ∂y ∂y ∂t ∂3w ∂3w ∂3w ∂3w ∂ 3v 0 − (B12 + 2B66 ) 2 − 3B26 − B22 3 = ρ0 2 3 2 ∂x ∂x ∂y ∂x ∂y ∂y ∂t (8.139) ∂ 4w ∂ 4w ∂ 4w ∂ 4w ∂ 4w + 4D16 3 + 2(D12 + 2D66 ) 2 2 + 4D26 + D22 4 3 4 ∂x ∂x ∂y ∂x ∂y ∂x ∂y ∂y − B11 ∂ 3u0 ∂ 3v 0 ∂ 3 u0 ∂ 3 u0 ∂ 3 u0 − 3 2 − − + − B B B ( ) B B 26 12 66 16 16 ∂y 3 ∂x 3 ∂x 3 ∂x 2 ∂y ∂x ∂y 2 + (B12 + 2B66 ) ∂ 3v 0 ∂ 3v 0 ∂ 3v0 ∂ 2w − − + ρ = q( x , y ) 3 B B 22 26 0 ∂x 2 ∂y ∂x ∂y 2 ∂y 3 ∂t 2 (8.140) Principles of Composite Material Mechanics 488 As with the static case in Section 7.9, the in-plane displacements u0 and v are coupled with the transverse displacements w when the Bij are present. For symmetric laminates with Bij = 0, Equation 8.140 alone becomes the governing equation for transverse displacements. These governing partial differential equations must be solved subject to the appropriate boundary conditions. As in the static case, when the in-plane displacements are coupled with the transverse displacements, the boundary conditions must be a combination of boundary conditions for a planar theory of elasticity problem and boundary conditions for a plate-bending problem. In this section, we focus on transverse vibrations according to Equation 8.140 with all Bij = 0 and the transverse distributed load q(x, y) = 0. An example of coupling effects will be given in Example 8.13. Let us now consider the case of free transverse vibration of the rectangular, specially orthotropic plate that is simply supported on all edges, as shown in Figure 8.39. The discussion here follows the analysis of Whitney [36]. For a specially orthotropic plate, all Bij = 0, A16 = A26 = D16 = D26 = 0 and Equation 8.140 becomes 0 D11 ∂ 4w ∂ 4w ∂ 4w ∂ 2w + 2(D12 + 2D66 ) 2 2 + D22 4 + ρ0 2 = 0 4 ∂x ∂x ∂y ∂y ∂t (8.141) For free harmonic vibration at frequency ω, we can assume that w( x , y , t) = W ( x , y )eiωt (8.142) where W(x, y) is a mode shape function. Substituting Equation 8.142 into 8.141, we have D11 ∂ 4W ∂ 4W ∂ 4W + 2(D12 + 2D66 ) 2 2 + D22 − ρ0ω 2W = 0 4 ∂x ∂x ∂y ∂y 4 a x b y FIGURE 8.39 Simply supported, specially orthotropic plate for free transverse vibration analysis. (8.143) Analysis of Viscoelastic and Dynamic Behavior 489 For the simply supported boundary condition, the transverse displacements and bending moments must vanish at the edges as in the static case. Thus, from Equations 7.142 and 7.143, we have, again, along x = 0 and x = a, W (x, y) = 0 and Mx = −D11 ∂ 2W ∂ 2W D − =0 12 ∂x 2 ∂y 2 (8.144) and along y = 0 and y = b, W (x, y) = 0 and M y = −D12 ∂ 2W ∂ 2W D − =0 22 ∂x 2 ∂y 2 (8.145) It can be shown that the equation of motion and the boundary conditions are satisied by solutions of the form nπy mπx W ( x , y ) = Amnsin sin a b (8.146) where m and n are mode indices that refer to the number of half wavelengths along the x- and y-directions, respectively, for mode mn, and a and b are the plate dimensions along the x-and y-directions, respectively. Substitution of Equation 8.146 into Equation 8.143 yields the frequency equation ω 2mn = π4 [D11m 4 + 2(D12 + 2D66 )(mnR)2 + D22 (nR)4 ] ρ0 a 4 (8.147) where the plate aspect ratio R = a/b, and ωmn is the natural frequency for mode mn [36]. For the fundamental mode, where m = n = 1, the natural frequency is given by 2 = ω11 π 4 D11 (2D12 + 2D66 ) D22 + + 4 a 2b 2 b ρ0 a 4 (8.148) Principles of Composite Material Mechanics 490 and the mode shape function is given by πy πx W ( x , y ) = sin sin a b (8.149) We now consider numerical results given by Whitney [36] for frequencies and mode shapes of two square plates. One plate is orthotropic with D11/D22 = 10 and (D12 + 2D66)/D22 = 1; the other is isotropic with D11/D22 = 1 and (D12 + 2D66)/D22 = 1. The four lowest natural frequencies for the two plates are compared in Table 8.2 and the corresponding mode shapes are compared in Figure 8.40. The dotted lines in Figure 8.40 denote the nodal lines of zero displacement for a particular mode. It is interesting to note that, in order of increasing frequency, the sequence of mode numbers is different for the isotropic and orthotropic plates. Owing to the high stiffness of the orthotropic plate along the x-direction, its frequencies are higher than the corresponding isotropic plate frequencies. It is also interesting to note that for the isotropic plate ω12 = ω21, but for the orthotropic plate ω21 > ω12. As with the static case, it is generally not possible to ind exact mode shape functions similar to those given by Equation 8.146 for boundary conditions such as clamped edges or free edges. For such cases, approximate solutions must be derived using approaches such as the Rayleigh–Ritz method or the Galerkin method. For more detailed discussions of these methods, the reader is referred to books by Whitney [36] and Vinson and Sierakowski [37]. The equation of motion for a specially orthotropic, laminated beam is found by reducing Equation 8.141 to the 1D form TABLE 8.2 Predicted Natural Frequencies for the First Four Modes of Simply Supported Plates Made of Specially Orthotropic and Isotropic Materials Orthotropic Isotropic ω = kπ 2 /b2 D22 /ρ0 ω = kπ 2 /b2 D/ρ0 Mode m n m n k 1st 2nd 3rd 4th 1 1 1 2 1 2 3 1 1 1 2 2 1 2 1 2 2.0 5.0 5.0 8.0 k 3.62 5.68 10.45 13.0 Source: From Whitney, J. M. 1987. Structural Analysis of Laminated Anisotropic Plates. Technomic Publishing Co., Lancaster, PA. With permission. Analysis of Viscoelastic and Dynamic Behavior Orthotropic 491 Isotropic 1st mode 2nd mode 3rd mode 4th mode FIGURE 8.40 Mode shapes for the irst four modes of simply supported plates mode of specially orthotropic and isotropic materials. (From Whitney, J. M. 1987. Structural Analysis of Laminated Anisotropic Plates. Technomic Publishing Co., Lancaster, PA. With permission.) D11 ∂ 4w ∂ 2w + ρ =0 ∂x 4 ∂t 2 (8.150) If we substitute ρ0 = ρh, and if we multiply Equation 8.150 by the beam width, b, we have bD11 ∂ 4w ∂ 2w + ρ bh =0 ∂x 4 ∂t 2 (8.151) For the 1D case, D11 = 1/D′11 and since bh = A, we have b ∂ 4w ∂ 2w + ρA 2 = 0 4 D11 ∂t ′ ∂x (8.152) which is the same as the equation that is derived from the beam theory in Example 8.11. 492 Principles of Composite Material Mechanics 8.3.4 Analysis of Damping in Composites Damping is simply the dissipation of energy during dynamic deformation. As structures and machines are pushed to higher and higher levels of precision and performance, and as the control of noise and vibration becomes more of a societal concern, it becomes essential to take damping into account in the design process. In conventional metallic structures, it is commonly accepted that much of the damping comes from friction in structural joints or from add-on surface damping treatments because the damping in the metal itself is typically very low. On the other hand, polymer composites have generated increased interest in the development of highly damped, lightweight, structural composites because of their good damping characteristics and the inherent design lexibility, which allows trade-offs between such properties as damping and stiffness. The purpose of this section is to provide a brief overview of the analysis of linear viscoelastic damping in composites. Dynamic mechanical testing of composites, which includes experimental determination of damping, will be discussed in Chapter 10. More detailed treatments of damping in composites are presented in publications by Gibson [45–47], Bert [48], Adams [49], Chaturvedi [50], Kinra and Wolfenden [51], and Sun and Lu [52]. As described in Section 8.1, damping is one of the important physical manifestations of viscoelastic behavior in dynamically loaded structural materials, and the stress–strain hysteresis loop in Figure 8.1c is typical of damped response under cyclic loading. Viscoelastic behavior of iber and/or matrix materials is not the only mechanism for structural damping in composite materials although it does appear to be the dominant mechanism in undamaged polymer composites vibrating at small amplitudes. Other damping mechanisms include thermoelastic damping due to cyclic heat low, coulomb friction due to slip in unbonded regions of the iber–matrix interface, and energy dissipation at sites of cracks and/or delaminations [45]. Thermoelastic damping is generally more important for metal composites than for polymer composites. Damping due to poor interface bonding, cracks, and/or delaminations cannot be relied upon in the design of structures, but the measurement of such damping may be the basis of a valuable nondestructive evaluation methodology [46]. In order to understand linear viscoelastic damping better, it is important to recognize the relationship between the timescale of the applied deformation and the internal timescale of the material. The timescale for cyclic deformation is determined by the oscillation frequency, ω. Recall that the relaxation times, λi or retardation times, ρi are measures of the internal timescale of the material. We will now use the Zener single-relaxation model to illustrate how damping depends on the relationship between these two timescales. For sinusoidal oscillation of the Zener single-relaxation model (Figure 8.10a), we can write σ = σ 0eiωt = (E′ + iE″ )ε (8.153) Analysis of Viscoelastic and Dynamic Behavior where σ = stress σ0 = stress amplitude ε = strain ω = frequency E′ = storage modulus is E′(ω) E″ = loss modulus is E″(ω) i = imaginary operator, which is 493 −1 Substituting Equation 8.153 into the stress–strain relationship for the Zener model (Equation 8.42) and separating into real and imaginary parts, we ind that E′ = E′(ω ) = k0 + (k0 + k1 )ω 2λ 12 1 + ω 2λ 12 (8.154) ωλ 1k1 1 + ω 2λ 12 (8.155) E′′ = E′′(ω) = and η = η(ω) = ωλ 1k1 E′′(ω) = E′(ω) k0 + (k0 + k1 )ω 2λ 12 (8.156) where λ1 = µ1/k1 is the relaxation time from Equation 8.44 η = η(ω) is the loss factor The variations of E′ and E″ with frequency ω are shown schematically in Figure 8.41. Note that when the frequency is the reciprocal of the relaxation time, ω = 1/λ1, the loss modulus peaks and the storage modulus passes through a transition region. Such damping peaks in the frequency domain are often referred to as “relaxation peaks.” The loss factor has a peak at a different frequency, not shown in Figure 8.41 because the relative position of that peak depends on the numerical values of the parameters. But the important point is that the dissipation of energy, whether characterized by the loss modulus or the loss factor is maximized when the timescale of the deformation is the same as the internal timescale of the material. If the two timescales are substantially different, the energy dissipation is reduced. For example, note in Figure 8.41 that E″ → 0 as ω → 0 and as ω → ∞. This behavior is typical for viscoelastic materials, but, as mentioned earlier, the actual transitions occur over a wider range (in this case a wider frequency range) than the single-relaxation model produces. Thus, as before, an improved Zener model (Figure 8.12 or 8.15) with a distribution of relaxation times Principles of Composite Material Mechanics 494 k0 + k1 k0 + E′(ω) k1 2 k1 2 k0 E″(ω) 1 λ1 Frequency (ω) FIGURE 8.41 Variation of storage modulus, E′(ω) and loss modulus, E″(ω) with frequency for the Zener single-relaxation model. makes it possible to extend the range of the relaxation to approximate the actual behavior better. Analytical models have been developed for predicting damping in composites at both the micromechanical and macromechanical levels. Only in certain special cases, such as thermoelastic damping [53] or dislocation damping [54] in metals, can the damping be predicted from irst principles without knowledge of constituent material damping properties. (These damping mechanisms are not discussed here.) If the damping mechanism is of the linear viscoelastic type, there are two basic approaches to the development of analytical models, both of which are based on the existence of experimental damping data for constituent materials. The two approaches are as follows: 1. The use of the Elastic–Viscoelastic Correspondence Principle in combination with elastic solutions from the mechanics of materials, elasticity theory, or numerical simulations. 2. The use of a strain energy formulation that relates the total damping in the structure to the damping of each element and the fraction of the total strain energy stored in that element. The basis of the irst approach is that linear elastostatic analyses can be converted to vibratory linear viscoelastic analyses by replacing static stresses and strains with the corresponding vibratory stresses and strains, and by replacing the elastic moduli or compliances with the corresponding complex moduli or compliances, respectively. According to this procedure, the elastostatic stress–strain relationships in Equation 2.5 would be converted to the viscoelastic vibratory Equation 8.70, and Equation 2.3 would be converted to Equation 8.71, as described in Section 8.2.5. The use of this approach to derive the micromechanics equation for the longitudinal loss factor of a Analysis of Viscoelastic and Dynamic Behavior 495 unidirectional composite (Equation 8.87) has already been demonstrated. The same approach has been used to derive micromechanics equations for the prediction of damping in aligned discontinuous iber composites having various iber aspect ratios and iber orientations [22,55] in randomly oriented short iber composites [56], in metal matrix and ceramic matrix composites at elevated temperatures [57], in hybrid composites with coated ibers [58], and in woven iber-reinforced composites [59]. The correspondence principle has also been used in combination with the CLT to develop equations for the laminate loss factors [23]. For example, the extensional loss factors for a laminate can be expressed in terms of the real and imaginary parts of the corresponding laminate extensional stiffnesses: η(ijA) = Aij′′ Aij′ (8.157) Similar equations can be used to describe laminate coupling and lexural loss factors [23]. The major limitation of such analyses is that the CLT neglects interlaminar stresses, so that interlaminar damping is not included. As shown later in this section, a more general 3D analysis including interlaminar damping may be developed by using a strain energy method. Although sinusoidally varying stresses and strains were assumed in the development of the complex modulus notation in Section 8.2.4, it has been shown that as long as the stiffness and damping show some frequency dependence, the complex modulus notation is also valid for the more general nonsinusoidal case [60]. Anomalous analytical results such as noncausal response can occur if the components of the complex modulus are independent of frequency. Composite materials (particularly polymer composites) generally have frequency-dependent complex moduli, however. The second approach involves the use of a strain–energy relationship that was irst presented in 1962 by Ungar and Kerwin [61]. Ungar and Kerwin found that for an arbitrary system of linear viscoelastic elements, the system loss factor can be expressed as a summation of the products of the individual element loss factors and the fraction of the total strain energy stored in each element: ∑ ηW η= ∑ W n i =1 n i =1 i i (8.158) i where ηi = loss factor for the ith element in the system Wi = strain energy stored in the ith element at maximum vibratory displacement n = total number of elements in the system Principles of Composite Material Mechanics 496 When applying this equation to composite damping analysis, the composite becomes the “system,” and the nature of the elements depends on whether the analysis is micromechanical or macromechanical. For example, this equation has been used in combination with mechanics of materials solutions for the strain energy of aligned discontinuous iber composites [62]. In this analysis, the damping in the iber was neglected (i.e., the iber loss factor ηf = 0), so that the longitudinal loss factor of the aligned discontinuous iber composite was approximated by the following form of Equation 8.158: η1 = ηmWm Wf + Wm (8.159) where ηm = matrix loss factor Wm = strain energy in the matrix at maximum vibratory displacement Wf = strain energy in the iber at maximum vibratory displacement The strain energy terms Wf and Wm were determined from mechanics of materials by using the stress distributions from the Cox model (Equations 6.21 and 6.26). The longitudinal storage modulus, E1′ , was also determined from the Cox model (Equation 6.24) and the loss modulus was found from ′′ with E1′′ = E1′η1. Figure 8.42 shows the variation of the predicted ratio E1′′/Em iber length-to-diameter ratio, L/d for several iber–matrix combinations [62]. It is seen that each composite has an optimum L/d where the ratio E1′′/Em ′′ is ′′ and the optimum L/d maximized, and that both the peak value of E1′′/Em 100 Energy model, ηf = 0 and υf = 0.5 3 2 E1′′/Em′′ 10 1. Glass–epoxy, Ef/Em = 19 2. Graphite–epoxy, Ef/Em = 104 3. Whisker–epoxy, Ef/Em = 182 1 1 0.1 1 10 103 102 Fiber aspect ratio (L/d ) 104 105 FIGURE 8.42 Variation of loss modulus ratio, E1′′/Em′′ with iber aspect ratio, L/d for several aligned discontinuous iber composite systems. (Reprinted from Gibson, R. F., Chaturvedi, S. K., and Sun, C. T. 1982. Journal of Materials Science, 17, 3499–3509. With permission from Chapman & Hall.) Analysis of Viscoelastic and Dynamic Behavior 497 shift to higher values as the modulus ratio Ef/Em increases. This means that the damping, which is primarily due to interfacial shear deformation, is increased when the mismatch between the iber and the matrix stiffnesses (as determined by Ef/Em) is increased. The Ungar–Kerwin equation is ideally suited for inite element implementation in the analysis of complex structures. In the inite element implementation, the element index “i” in Equation 8.158 refers to the element number, n refers to the total number of inite elements, and the strain energy terms, Wi, are determined from the inite element analysis (FEA). It appears that the equation was irst implemented in the inite element form in the so-called “modal strain energy” approach for the analysis of modal damping in complex structures [63]. The strain energy/inite element approach has also been used in numerous composite analysis applications at both the micromechanical level [58,59,64,65] and the laminate level [66–68]. For example, in studies of the iber–matrix interphase, the inite element models shown in Figure 8.43 were used in conjunction with the equation η= ηfWf + ηmWm + ηiWi Wf + Wm + Wi (8.160) where ηf = iber loss factor ηi = interphase loss factor Wi = strain energy in the interphase region at maximum vibratory displacement z z z σy y Di Df τyz y y Quarter domain RVE y Half domain y y τyz σx x x RVE Quarter domain x Half domain FIGURE 8.43 Models used for strain energy/FEA of effect of interphase on damping or unidirectional graphite/epoxy under different loading conditions. (Reprinted from Gibson, R. F., Hwang, S. J., and Kwak, H. 1991. How Concept Becomes Reality—Proceedings of 36th International SAMPE Symposium, Vol. 1, pp. 592–606. With permission from the Society for the Advancement of Material and Process Engineering, Covina, CA.) Principles of Composite Material Mechanics 498 Typical results for four different loading conditions are shown in Figure 8.44. It appears that the in-plane shear loss factor, ηxy, is the most sensitive of the four loss factors to the size of the interphase region. 3D FEA has been used in conjunction with the Ungar–Kerwin equation to study interlaminar damping and the effects of coupling on damping in laminates [66–68]. In these studies, the laminate loss factor was modeled using the equation N η= ∑ η Wx( k ) + η(yk )Wy( k ) + η(xyk)Wxy( k ) + η(zk )Wz( k ) + η(yzk)Wyz( k ) + η(xzk)Wxz( k ) /Wt (k ) x k =1 (8.161) where k = lamina number N = total number of laminae Wt = total strain energy stored in laminate at maximum vibratory displacement: N Wt = ∑ W (k ) x k =1 + Wy( k ) + Wxy( k ) + Wz( k ) + Wyz( k ) + Wxz( k ) 0.018 Loss factor 0.015 0.012 0.009 0.006 ηy ηyz ηxy ηx 0.003 0.000 1.02 1.03 1.04 1.05 1.06 1.07 1.08 1.09 1.10 Interphase size (Di/Df ) FIGURE 8.44 Predicted effect of interphase size on loss factor for material and loading conditions described in Figure 8.43. (Reprinted from Gibson, R. F., Hwang, S. J., and Kwak, H. 1991. How Concept Becomes Reality—Proceedings of 36th International SAMPE Symposium, Vol. 1, pp. 592–606. With permission from the Society for the Advancement of Material and Process Engineering, Covina, CA.) Analysis of Viscoelastic and Dynamic Behavior 499 x, y, z = global laminate coordinates η(xk ) , η(yk ) , η(xyk) = in-plane loss factors for the kth lamina η(zk ) , η(yzk) , η(xzk) = out-of-plane loss factors for the kth lamina Wx( k ) , Wy( k ) , Wxy( k ) = in-plane strain energy terms for the kth lamina Wz( k ) , Wyz( k ) , Wxz( k ) = out-of-plane strain energy terms for the kth lamina Conribution of interlaminar damping (%) Thus, the decomposition of the total damping into contributions associated with each stress component is a relatively simple task with the strain energy approach. For example, Figure 8.45 shows the contribution of the different components of interlaminar damping as a function of iber orientation for angle-ply graphite laminates under uniaxial extension [66]. The inite element model for this work was shown in Figure 7.31. It is seen that the interlaminar damping is maximized at a particular iber orientation, and that the interlaminar shear stress, τyz, is the most signiicant contributor to interlaminar damping in this case. A similar approach was used to study damping in composite beams with constrained viscoelastic layer damping treatments, and Figure 8.46 shows the effect of constrained viscoelastic layer (damping tape) length on damping for a glass/epoxy beam [69]. In this case, damping is seen to be strongly dependent on the ratio of damping tape length to beam length and the tape end ixity condition. A review of the applications of the strain energy method for studying various aspects of damping in composite materials and structures has been published by Hwang and Gibson [70]. At the structural level, this method has 16 14 Predicted data from FEM Total contribution Contribution due to τyz Contribution due to τxz Contribution due to σz 12 10 8 6 4 2 0 0 10 20 30 40 60 70 50 Fiber orientation (degrees) 80 90 FIGURE 8.45 Contribution of different components of interlaminar damping for various iber orientations for [±θ]s graphite/epoxy laminates (with laminate width/thickness = 4 and length/thickness = 6) under uniaxial loading. (Reprinted from Composites Science and Technology, 41, Hwang, S. J. and Gibson, R. F. The effects of 3D states of stress on damping of laminated composites, 41, 379–393, Copyright 1991, with permission from Elsevier.) Principles of Composite Material Mechanics Loss factor ratio (taped/untaped) 500 30 28 26 24 22 20 18 16 14 12 10 8 6 4 2 0 Base structure: glass–epoxy (15 ply—0°) Damping tape: 3M’s SJ—2052X N T L Mode 1 Tape fixed at root (N/L = 0) Tape free at root (N/L = 0) FEM predictions Experimental scatter 0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1 Tape length/beam length (T/L) FIGURE 8.46 Measured and predicted damping for unidirectional glass/epoxy beam with constrained viscoelastic layer damping tapes of different lengths and tape end ixity conditions. (From Mantena, P. R., Gibson, R. F., and Hwang, S. J. 1991. AIAA Journal, 29(10), 1678–1685. Copyright AIAA, 1990. With permission.) been used to predict damping in composite grid structures [71], curvilinear laminates and composite shell structures [72], and composite sandwich structures [73]. For example, Chen and Gibson [71] used a inite element implementation of the strain energy approach to study integral passive damping in composite isogrid structures. Figure 8.47 shows a typical 3D inite element model for the composite isogrid structure, which has an integral layer of polymeric damping material at the rib–skin interface. Figure 8.48 shows that the predicted and measured damping can be increased signiicantly by using the integral damping layer. Further discussions on the experimental aspects of this work can be found in Chapter 10. Although the loss factor is a convenient measure of damping because of its connection with the complex modulus notation, it is not the only parameter used to describe damping. For materials with small damping (η ≪ 1), other measures of damping that appear in the literature are related to the loss factor as follows [48]: η= ψ ∆ 1 = = 2ζ = 2π π Q where Ψ = speciic damping capacity Δ = logarithmic decrement ζ = damping ratio or damping factor Q = quality factor (8.162) Analysis of Viscoelastic and Dynamic Behavior 501 Integral polymeric damping layers at rib/skin interface, 0.25 mm thick Ribs 6.2 mm × 6.4 mm Skin 1.5 mm thick 304 mm 264 mm FIGURE 8.47 Finite element model for analysis of vibration and damping in composite isogrid structure with integral passive damping. (From Chen, Y. and Gibson, R. F. 2003. Mechanics of Advanced Materials and Structures, 10(2), 127–143. With permission.) 0.25 Loss factor 0.2 0.15 0.1 0.05 0 0 50 100 150 200 Frequency (Hz) 250 300 350 FEA prediction Measured (sample 1, comolding) Measured (sample 2, comolding) Measured (sample 3, secondary bonding) FIGURE 8.48 Comparison of predicted and measured damping loss factors in composite isogrid structures with and without integral passive damping. (From Chen, Y. and Gibson, R. F. 2003. Mechanics of Advanced Materials and Structures, 10(2), 127–143. With permission.) 502 Principles of Composite Material Mechanics Most of these parameters are associated with the damping of a singledegree-of-freedom vibration model and are used to obtain damping from vibration test data. Such tests will be discussed in more detail in Chapter 10. In summary, damping has become an important consideration in the design of dynamically loaded composite materials and structures. As a result, there is increased interest in the prediction of damping in composites. Several analytical methods for making such predictions have been reviewed, and sample results have been presented. Because of the design lexibility that is inherent in composite materials, the potential for improvement and optimization of damping appears to be much greater than that for conventional structural materials. 8.4 Nanoenhancement of Viscoelastic and Dynamic Properties As part of the nanotechnology revolution, the study of vibration and damping in nanocomposites has been the subject of numerous investigations in recent years. A review of the literature on vibrations of carbon nanotubes (CNTs) and their composites has been published by Gibson et al. [74]. Several papers have reported signiicant increases in internal damping of polymer nanocomposites when very small amounts of CNTs are used as reinforcement. For example, as shown in Figure 8.49, increases in the loss modulus of more than 1000% were reported by Koratkar et al. [75] for single wall nanotube (SWNT)–polycarbonate nanocomposites containing up to 2% by weight SWNTs. It was shown that the increase in damping was primarily due to frictional sliding at the nanotube–polymer interfaces as the strain level increases. This points out an advantage of nanoillers in that they present a very large interfacial contact area with the matrix material by comparison with conventional reinforcements. Zhou et al. [76] fabricated and tested SWNT/epoxy beams with varying amounts of SWNT reinforcement and developed a “stick–slip” micromechanical model that captured the observed trends in the damping. The increased damping effect (i.e., more rapid free vibration decay) with increased CNT content is clearly shown in Figure 8.50. Another key conclusion from the analytical model developed here was that the size and speciic surface area of iller materials are extremely important factors that affect damping in composites, and that the very large interfacial contact area of nanotubes is a deinite advantage when it comes to damping. Rajoria and Jalili [77] generated a large amount of experimental data on damping of CNT–epoxy–steel sandwich beams having various weight percentages of CNTs. As shown in Figure 8.51, beams containing multiwall nanotube (MWNT) reinforcement had greater damping than those containing either SWNT reinforcement or conventional carbon iber (CF) Analysis of Viscoelastic and Dynamic Behavior 503 200 Pure polycarbonate As-received SWNT (1.0 wt.%)-PC Oxidized SWNT (1.0 wt.%)-PC Oxidized SWNT (2.0 wt.%)-PC 180 160 Loss modulus (MPa) 140 120 1150% increase 100 80 60 40 20 0 0 0.25 0.5 0.75 Strain (%) 1 1.25 1.5 FIGURE 8.49 Variation of loss modulus with increasing strain for SWNT–polycarbonate nanocomposite. (Reprinted with permission from Koratkar, N. A. et al. 2005. Characterizing energy dissipation in single-walled carbon nanotube polycarbonate composites. Applied Physics Letters, 87, 063102. Copyright 2005, American Institute of Physics.) reinforcement. In addition, the frequency dependence of CNT-reinforced beams was more pronounced than that of the other beams, and it appears that once the weight percentage of either SWNTs or MWNTs reaches 5%, there is no further improvement in damping. Up to 700% improvement in damping for 5% MWNT-reinforced beams was reported. On the other hand, corresponding changes in the storage modulus were found to be much less pronounced. Most of the studies of damping in nanocomposites so far have been of an experimental nature, and there is a need for more analytical work. For example, the analytical predictions of Gibson et al. [62] in Figure 8.42 show that there is an optimum iber aspect ratio for maximizing the loss modulus of a discontinuous-aligned iber composite, and that the optimum loss modulus increases with increasing iber/matrix stiffness mismatch, as quantiied by the ratio Ef/Em. The maximum ratio Ef/Em = 182 shown in Figure 8.42 is for a whisker–epoxy composite, but the corresponding Ef/Em ratio for a CNT nanocomposite should be at least 500 or so, and the optimum loss modulus should be much greater than those shown in Figure 8.42. This model is for a discontinuous-aligned iber composite, however, and such Principles of Composite Material Mechanics 504 0.03 Acceleration (V) 0.02 0.01 0.00 0% CNT –0.01 –0.02 –0.03 0.0 0.5 1.0 Time (s) 1.5 2.0 0.03 Acceleration (V) 0.02 0.01 0.00 0.5% CNT –0.01 –0.02 –0.03 0.0 0.5 1.0 Time (s) 1.5 2.0 0.03 Acceleration (V) 0.02 0.01 0.00 1% CNT –0.01 –0.02 –0.03 0.0 0.5 1.0 Time (s) 1.5 2.0 FIGURE 8.50 Free vibration decay curves for SWNT–epoxy nanocomposite beams having different amounts of SWNT reinforcement. (Reprinted from Composites Science and Technology, 64, Zhou, X. et al. 2004. Interfacial damping characteristics of carbon nanotube composites, 2425–2437, Copyright 2004, with permission from Elsevier.) Analysis of Viscoelastic and Dynamic Behavior 0.035 0.03 Dampimg ratio (ζ) 0.025 505 Plain epoxy beam 2.5% MWNT–epoxy beam 5.0% MWNT–epoxy beam 7.5% MWNT–epoxy beam 2.5% SWNT–epoxy beam 5.0% SWNT–epoxy beam 7.5% SWNT–epoxy beam 5.0% CF–epoxy beam 0.02 0.015 0.01 0.005 0 0 50 100 150 200 250 Frequency ω (Hz) FIGURE 8.51 Measured frequency dependence of damping ratio for various composite beams. (Reprinted from Composites Science and Technology, 65, Rajoria, H. and Jalili, N., Passive vibration damping enhancement using carbon nanotube–epoxy reinforced composites, 2079–2093. Copyright 2005, with permission from Elsevier.) models need to be revised to include the waviness and 3D orientation of nanotubes or nanoibers. Another example of the nanoenhancement of viscoelastic behavior is the use of nanoreinforcements to improve creep resistance in polymers and polymer composites. For example, as shown in Figure 8.52, Zhang et al. [78] demonstrated that the tensile creep strain of epoxy is markedly reduced by adding only 0.1 wt.% of well-dispersed SWNTs. It is believed that the reason for the improved creep performance is that the SWNTs limit the time-dependent, load-induced reorientation of the polymer chains. In this case, the SWNTs were more effective than either MWNTs or C60 fullerene nanoparticles in reducing creep. However, it was found that for SWNT weight fractions greater than about 0.1 wt.%, the creep response deteriorated signiicantly due to poor dispersion of the SWNTs. Numerous other examples of improved creep performance of polymers due to the addition of small amounts of nanoillers have been reported in the literature. For example, Yang et al. [79] studied creep of TiO2 nanoparticle-enhanced polypropylene (PP), Zhou et al. [80] characterized creep of SiO2 nanoparticle-enhanced PP, and Varela-Rizo et al. [81] conducted creep tests of polymethylmethacrylate (PMMA) reinforced with either chopped CFs, MWNTs, or CNFs. As with the dynamic properties of nanocomposites, much of the research on creep of nanocomposites has been experimental, and there is a need for more analytical modeling work. Principles of Composite Material Mechanics 506 (a) Pure epoxy 0.1% MWNT 0.1% C60 0.8 Strain (%) 0.1% SWNT 0.7 0.6 0.5 0.4 (b) 0 2000 4000 6000 Time (s) 8000 10,000 12,000 0.85 0.8 Strain (%) 0.75 0.7 0.65 0.6 0.55 Pure epoxy 0.1% MWNT 0.1% C60 0.1% SWNT FIGURE 8.52 Effect of nanoillers on the creep response of epoxy composites. (a) Creep strain versus time for pure epoxy sample and epoxy nanocomposite samples with 0.1 wt.% of SWNT, MWNT, and C60 additives. Creep tests were performed at room temperature at an applied stress of 10 MPa. (b) Measured creep strain after 3 h of continuous testing for the pure epoxy and nanocomposite samples. (From Zhang, W. et al. 2007. Nanotechnology, 18, 185703. With permission.) EXAMPLE 8.10 Derive Equations 8.154 and 8.155 for the complex modulus of the Zener model. Solution Combining Equation 8.153, which deines the complex modulus, and Equation 8.42, which is the stress–strain relationship for the Zener model, we obtain Analysis of Viscoelastic and Dynamic Behavior σeiωt + 507 iωµ1 (k o + k1 )σeiωt µ1 σeiωt + (iωσeiωt ) = k o k1 E′ + iE′′ k1 (E′ + iE′′) Dividing both sides by σeiωt, using λ1 = µ1/k1, rearranging to obtain E′ + iE″ on the left-hand side, then multiplying both the numerator and the denominator of the right-hand side by 1 − iωλ1, which is the complex conjugate of 1 + iωλ1, we obtain E′ + iE′′ = ωλ 1k1 k o + (k o + k1 )ω 2λ 12 +i 1 + ω 2λ 12 1 + ω 2λ 12 Now setting the real parts of both sides equal and the imaginary parts of both side equal, we obtain E′ = k o + (k o + k1 )ω 2λ 12 1 + ω 2λ 12 and E′′ = ωλ 1k1 1 + ω 2λ 12 EXAMPLE 8.11 For a symmetric laminated beam having a rectangular cross section of width b and thickness h, determine (a) the equation of motion for free vibration and (b) the natural frequencies. Assume that the criteria for use of the effective modulus theory have been met. Solution a. Substituting the lexural modulus, Efx, from Equation 7.73 into the expression for EI, we ind that EI = E fxI = 12 bh 3 b = h D11 ′ 12 D11 ′ 3 (Note that h is used to denote thickness and t is used for time.) Thus, the Bernoulli–Euler beam Equation 8.111 becomes ∂2w b ∂4w + ρA 2 = 0 4 ∂x D11 ′ ∂x b. The natural frequencies are then found from Equation 8.125: fn = (k n L)2 b 2πL2 D11 ′ ρA 1/2 where the eigenvalues, kn, depend on the boundary conditions. Principles of Composite Material Mechanics 508 EXAMPLE 8.12 A unidirectional AS/3501 carbon–epoxy plate is simply supported on all four edges. The plate is 300 mm × 300 mm square, 2 mm thick, and has a mass density of 1.6 mg mm 3. Determine the frequency of the fundamental mode of the plate. Solution Using the lamina stiffnesses, Qij, from Example 7.5 and the thickness of 2 mm in Equation 7.43 for a laminate consisting of a single orthotropic lamina, we ind the laminate bending stiffnesses to be D11 = 92.53 GPa mm 3 , D12 = 1.813 GPa mm 3 D11 = 6.03 GPa mm 3 , D66 = 4.6 GPa mm 3 The mass per unit area is ρ0 = ρh = (1.6 mg/mm 3 )(2 mm) = 3.2 mg/mm 2 = 0.0032 g/mm 2 The fundamental frequency is then found from Equation 8.148 as 2 = ω11 π4 [92.53 + 2(1.813 + 2( 4.6)) + 6.03](10 9 ) (0.0032)(300)4 = 4.53(10 5 ) rad 2/s 2 or ω11 = 673 rad/s (Note: GPa mm3 = 109 g mm2/s2 in the above equation.) EXAMPLE 8.13 Investigate the effects of coupling on the lexural vibration frequencies of a nonsymmetrically laminated [0/90] cross-ply composite beam that is simply supported on each end. The beam has length L and the x-axis is parallel to the longitudinal axis of the beam. Solution Since the plies are all oriented at either 0° or 90°, there is no shear coupling, and A16 = A26 = B16 = B26 = D16 = D26 = 0. In addition, for a 1D beam oriented along the x-direction, all terms in the equations of motion (Equations 8.138 through 8.140) involving v0 and y, and derivatives in y may be neglected. Finally, we neglect the longitudinal inertia term on the right-hand side of Equation 8.138, and the transverse loading term q(x, y) on the right-hand side of Equation 8.140. With these simpliications, Equation 8.139 becomes Analysis of Viscoelastic and Dynamic Behavior identically zero on both sides, whereas Equations 8.138 and 8.140 reduce to the coupled partial differential equations, respectively, A11 ∂3w ∂ 2u0 − B11 3 = 0 2 ∂x ∂x and ∂4w ∂ 3 u0 ∂2w − B11 = −ρ0 2 4 3 ∂x ∂x ∂t D11 For free harmonic vibration at frequency, ω, we can assume separation of variables solutions of the form u 0 ( x , t) = U( x)eiωt and w( x , t) = W ( x)eiωt where U(x), W(x) are mode-shape functions. Substitution of these assumed shape functions into the two equations of motion above yields the ordinary differential equations A11 d 3W d 2U − B11 =0 2 dx dx 3 and D11 d 4W d 3U − B11 = ρ0ω 2W 4 dx dx 3 For the simple supports at x = 0 and x = L, the boundary conditions are given by specifying that the transverse displacement W(x) and the bending moment per unit length Mx(x) must both vanish at x = 0 and x = L. Therefore, W (0 ) = 0 W ( L) = 0 dU d 2W (0) − D11 (0 ) = 0 dx dx 2 dU d 2W (L) = 0 (L) − D11 Mx (L) = B11 dx dx 2 Mx (0) = B11 where the equations for the bending moment per unit length, Mx(x) are found by substituting the simpliications listed above in Equations 7.32 509 Principles of Composite Material Mechanics 510 through 7.44, and evaluating the resulting expressions at x = 0 and x = L. It can be shown by substitution that the boundary conditions are all satisied by mode-shape functions of the form nπx U( x) = U 0 cos L nπx W ( x) = W0 sin L where n = 1, 2, 3, …, is the mode number. It can also be shown that these functions satisfy the in-plane boundary conditions Nx(0) = Nx(L) = Nxy(0) = Nxy(L) = 0. Substitution of these mode-shape functions in the two differential equations yields the algebraic equations, 2 nπ A11 L 3 −B11 nπ L U 0 = 0 4 W0 0 nπ D11 − ρ0ω n L nπ −B11 L 3 where ω = ωn for vibration in mode n. For nontrivial solutions of the displacements, the determinant of the coeficient matrix must be equal to zero, and this yields the frequency equation for mode n: 4 ωn = 1 nπ B112 D11 − A11 ρ0 L It is easily shown from the deinitions of the laminate stiffnesses that for this [0/90] laminate, A11, B112, and D11 are all positive, and that as a result, the bending–extension coupling term B112/A11 causes the frequencies to be reduced below those of a symmetrically laminated beam that has the nth mode frequency, 4 nπ D ω n = 11 L ρ0 Similarly, Jones [82] has shown that, for antisymmetric cross-ply laminated plates of various aspect ratios and various numbers of plies, bending–extension coupling always reduces the frequencies. However, it was found that the frequency reduction is greatest for the case of only two plies (i.e., [0/90]), and that the coupling effect was reduced as the number of plies was increased. Similar results have been found for antisymmetric angle-ply laminates. Analysis of Viscoelastic and Dynamic Behavior EXAMPLE 8.14 The constituent materials in a unidirectional carbon/epoxy material have the following dynamic mechanical properties at a certain frequency: Ef′1 = 220 GPa (32 × 10 6 psi); ηf 1 = 0.002; υf = 0.6 Em ′ = 3.45 GPa (0.5 × 10 6 psi); ηm = 0.02; υm = 0.4 Determine the composite longitudinal loss factor and the percentage of the total longitudinal damping due to each constituent. Solution Substituting the above data into Equation 8.87 from the Elastic–Viscoelastic Correspondence Principle, or using the strain energy approach and Equation 8.158, we ind that the composite longitudinal loss factor is η1 = Ef′′1vf + Em ′′ vm ηf 1Ef′1vf + ηm Em ′ vm 0.002(220)(0.6) + 0.02(3.45)(0.4) = = Ef′1vf + Em Ef′1vf + Em 220(0.6) + 3.45(0.4) ′ vm ′ vm = 0.001979 + 0.000207 = 0.002186 Thus, the iber contributes (0.001979/0.002186) × 100 = 90.5% of the damping and the matrix contributes the remaining 9.5%. Even though the matrix has a greater loss factor than the iber, most of the strain energy is stored in the iber, and this is why the iber contributes more to the total composite damping. This is not true for the off-axis case, however, as the strain energy in the matrix becomes more signiicant. For example, the composite transverse loss factor is dominated by the matrix contribution. EXAMPLE 8.15 A [0/90/0]S symmetric laminated beam consists of six plies of equal thickness and the plies have the following complex Young’s moduli at a certain frequency: For the 0 0 plies, E1* = E1′ + iE1′′ = [(5 × 10 6 ) + i(5 × 10 3 )] psi For the 90° plies, E2* = E2′ + iE2′′ = [(1.5 × 10 6 ) + i(1.5 × 10 4 )] psi Find the lexural loss factor, ηf for the beam, assuming that the complex moduli for the plies and the laminate are all determined at the same frequency. Note that the subscript f here refers to lexural, not iber. 511 Principles of Composite Material Mechanics 512 Solution The equation for the complex lexural modulus of the laminated beam is found by applying the Elastic–Viscoelastic Correspondence Principle to the equation for the elastic lexural modulus. The elastic lexural modulus of a laminated beam having an even number of equal thickness plies is given by Equation 7.9 Ef = 8 N3 N /2 ∑(E ) (3 j x j 2 − 3 j + 1) j =1 The corresponding equation for the complex lexural modulus is Ef* = 8 N3 N /2 ∑(E ) (3 j * x j 2 − 3 j + 1) j =1 Substituting into the complex moduli of the plies, Ex* , and the associated ply numbers, j, we ind that Ef* = 8 [(5 × 106 ) + i(5 × 10 3 )](3(1)2 − 3(1) + 1) ( 6 )3 + 8 (1.5 × 106 ) + i(1.5 × 10 4 ) (3(2)2 − 3(2) + 1) ( 6 )3 + 8 (5 × 10 6 ) + i(5 × 10 3 ) (3(3)2 − 3(3) + 1) (6 )3 or Ef* = Ef′ + iEf′′ = ( 4.088 × 106 ) + i(7.585 × 10 3 ) psi Setting the real parts of both sides of the equation equal, the lexural storage modulus is Ef′ = 4.088 × 10 6 psi . Setting the imaginary parts of both sides of the equation equal, the lexural loss modulus is Ef′′= 7.585 × 10 3 psi. Finally, the lexural loss factor is given by ηf = Ef′′ 7.585 × 10 3 = 0.00185 = Ef′ 4.088 × 10 6 PROBLEM 8.21 Longitudinal vibration of an isotropic, particle-reinforced composite bar may be modeled by using the 1D wave equation (Equation 8.99) if the material is linear elastic. Derive the equation of motion for longitudinal vibration Analysis of Viscoelastic and Dynamic Behavior 513 of the bar if it can be assumed to be a Kelvin–Voigt linear viscoelastic material having the stress–strain relationship given by Equation 8.39. PROBLEM 8.22 Find the separation of variables solution for the longitudinal displacement, u(x, t), of the equation derived in Problem 8.21. Leave the answer in terms of constants, which must be determined from the boundary conditions and the initial conditions. PROBLEM 8.23 Derive the equation of motion for free transverse vibration of a simply supported, specially orthotropic plate that is subjected to in-plane loads per unit length Nx and Ny, as shown in Figure 8.53. PROBLEM 8.24 For the plate described in Problem 8.23, ind the equations for the plate natural frequencies and determine the effects of positive (tensile) and negative (compressive) in-plane loads Nx and Ny on the natural frequencies. PROBLEM 8.25 If the plate described in Problem 8.23 is clamped on all edges, investigate solutions of the form 2πy 2πx W ( x , y ) = Amn 1 − cos 1 − cos a b Does this solution satisfy the boundary conditions? Can it be used to ind the natural frequencies? Explain your answers. Ny a Nx x b Nx y Ny FIGURE 8.53 Simply supported, specially orthotropic plate under in-plane loads for Problem 8.23. 514 Principles of Composite Material Mechanics PROBLEM 8.26 For the nonsymmetrical laminated beam of Problem 7.5, determine the effects of Bij-type coupling on the lexural vibration frequencies. PROBLEM 8.27 If the complex moduli of the 0° and 90° plies in a laminated beam are the same as those described in Example 8.15, but the laminate has a stacking sequence of [90/0/90]S instead of [0/90/0]S, determine the corresponding lexural loss factor. Compare and contrast these results with those of Example 8.15. References 1. Schapery, R. A. 1974. Viscoelastic behavior and analysis of composite materials. In Sendeckyj, G. P. ed., Composite Materials, Mechanics of Composite Materials, Vol. 2, pp. 85–168. Academic Press, New York, NY. 2. Beckwith, S. W. 1984. Viscoelastic creep behavior of ilament-wound case materials. Journal of Spacecraft and Rockets, 21(6), 546–552. 3. Fung, Y. C. 1979. Foundations of Solid Mechanics. Prentice-Hall, Inc., Englewood Cliffs, NJ. 4. Christensen, R. M. 1979. Mechanics of Composite Materials. John Wiley & Sons, New York, NY. 5. Halpin, J. C. and Pagano, N. J. 1968. Observations on linear anisotropic viscoelasticity. Journal of Composite Materials, 2(1), 68–80. 6. Christensen, R. M. 1982. Theory of Viscoelasticity: An Introduction, 2nd ed. Academic Press, New York, NY. 7. Sullivan, J. L. 1992. Polymer viscoelasticity. Unpublished notes, Ford Motor Co., Dearborn, MI. 8. McCrum, N. G., Buckley, C. P., and Bucknall, C. B. 1988. Principles of Polymer Engineering. Oxford University Press, Oxford. 9. Wen, Y. F., Gibson, R. F., and Sullivan, J. L. 1997. Prediction of momentary transverse creep behavior of thermoplastic polymer matrix composites using micromechanical models. Journal of Composite Materials, 31(21), 2124–2145. 10. Gibson, R. F. 1979. Measurement of creep in rotating viscoelastic disks. Experimental Mechanics, 19(10), 378–383. 11. Gibson, R. F., Baxi, J., Bettinger, D., Stoll, F., and Johnson, V. 1999. Simulation of assembly and operation of pre-stressed, heat-shrinkable structural composite connectors. Proceedings of ASME Noise Control and Acoustics Division, NCA Vol. 26, pp. 319–332. American Society of Mechanical Engineers, New York, NY. 12. Gibson, R. F., Younus, M., Kumar, P., Stoll, F., and Bettinger, D. 1998. Viscoelastic behavior of extended interval lubricator cartridges made from nylon and glass/nylon composites. Proceedings of 43rd International SAMPE Symposium & Exhibition, pp. 2144–2157. Society for the Advancement of Material and Process Engineering, Covina, CA. Analysis of Viscoelastic and Dynamic Behavior 515 13. Bracewell, R. N. 1978. The Fourier Transform and Its Application, 2nd ed. McGrawHill, Inc., New York, NY. 14. Gibson, R. F., Hwang, S. J., and Sheppard, C. H. 1990. Characterization of creep in polymer composites by the use of frequency–time transformations. Journal of Composite Materials, 24, 441–453. 15. Lee, E. H. 1955. Stress analysis in viscoelastic bodies. Quarterly of Applied Mathematics, 13, 183–190. 16. Biot, M. A. 1958. Linear thermodynamics and the mechanics of solids. Proceedings of the Third U.S. National Congress of Applied Mechanics, pp. 1–18. The National Academies, Washington, DC. 17. Schapery, R. A. 1967. Stress analysis of viscoelastic composite materials. Journal of Composite Materials, 1, 228–267. 18. Beckwith, S. W. 1974. Viscoelastic characterization of a nonlinear glass/epoxy composite including the effects of damage. PhD dissertation, Texas A&M University, College Station, TX. 19. Sims, D. F. and Halpin, J. C. 1974. Methods for determining the elastic and viscoelastic response of composite materials. Composite Materials: Testing and Design (Third Conference), ASTM STP 546, pp. 46–66. American Society for Testing and Materials, Philadelphia, PA. 20. Hashin, Z. 1970. Complex moduli of viscoelastic composites. I: General theory and application to particulate composites. International Journal of Solids and Structures, 6, 539–552. 21. Hashin, Z. 1970. Complex moduli of viscoelastic composites. II: Fiber reinforced materials. International Journal of Solids and Structures, 6, 797–807. 22. Suarez, S. A., Gibson, R. F., Sun, C. T., and Chaturvedi, S. K. 1986. The inluence of iber length and iber orientation on damping and stiffness of polymer composite materials. Experimental Mechanics, 26(2), 175–184. 23. Sun, C. T., Wu, J. K., and Gibson, R. F. 1987. Prediction of material damping of laminated polymer matrix composites. Journal of Materials Science, 22, 1006–1012. 24. Findley, W. N., Lai, J. S., and Onaran, K. 1976. Creep and Relaxation of Nonlinear Viscoelastic Materials. Dover Publications, New York, NY. 25. Ferry, J. D. 1970. Viscoelastic Properties of Polymers, 2nd ed. John Wiley & Sons, New York, NY. 26. Struik, L. C. E. 1977. Physical aging in plastics and other glassy materials. Polymer Engineering and Science, 17, 165–173. 27. Struik, L. C. E. 1978. Physical Aging in Amorphous Polymers and Other Materials. Elsevier, Amsterdam. 28. Janas, V. F. and McCullough, R. L. 1987. The effects of physical aging on the viscoelastic behavior of a thermoset polyester. Composites Science and Technology, 30, 99–118. 29. Ogale, A. A. and McCullough, R. L. 1987. Physical aging of polyether ether ketone. Composites Science and Technology, 30, 137–148. 30. Sullivan, J. L. 1990. Creep and physical aging of composites. Composites Science and Technology, 39, 207–232. 31. Scott, D. W., Lai, J. S., and Zureick, A. -H. 1995. Creep behavior of iberreinforced polymeric composites: A review of the technical literature. Journal of Reinforced Plastics and Composites, 14, 588–617. 32. Hearmon, R. F. S. 1961. An Introduction to Applied Anisotropic Elasticity. Oxford University Press, Oxford. 516 Principles of Composite Material Mechanics 33. Achenbach, J. D. 1974. Waves and vibrations in directionally reinforced composites. In Sendeckyj, G. P. ed., Composite Materials, Vol. 2, Mechanics of Composite Materials. Academic Press, New York, NY. 34. Ross, C. A. and Sierakowski, R. L. 1975. Elastic waves in iber reinforced materials. The Shock and Vibration Digest, 7(1), 1–12. 35. Moon, F. C. 1974. Wave propagation and impact in composite materials. In Chamis, C. C. ed., Composite Materials, Vol. 7. Academic Press, New York, NY. 36. Whitney, J. M. 1987. Structural Analysis of Laminated Anisotropic Plates. Technomic Publishing Co., Lancaster, PA. 37. Vinson, J. R. and Sierakowski, R. L. 1986. The Behavior of Structures Composed of Composite Materials. Martinus Nijhoff Publishers, Dordrecht, The Netherlands. 38. Sierakowski, R. L. and Chaturvedi, S. K. 1997. Dynamic Loading and Characterization of Fiber-Reinforced Composites. John Wiley & Sons, Inc., New York, NY. 39. Meirovitch, L. 1986. Elements of Vibration Analysis, 2nd ed. McGraw-Hill, Inc., New York, NY. 40. Timoshenko, S. P., Young, D. H., and Weaver, W. Jr. 1974. Vibration Problems in Engineering. John Wiley & Sons, New York, NY. 41. Dudek, T. J. 1970. Young’s and shear moduli of unidirectional composites by a resonant beam method. Journal of Composite Materials, 4, 232–241. 42. Ni, R. G. and Adams, R. D. 1984. The damping and dynamic moduli of symmetric laminated beams—Theoretical and experimental results. Journal of Composite Materials, 18, 104–121. 43. Huang, T. C. and Huang, C. C. 1971. Free vibrations of viscoelastic Timoshenko beam. Journal of Applied Mechanics, 38, Series E(2), 515–521. 44. Nakao, T., Okano, T., and Asano, I. 1985. Theoretical and experimental analysis of lexural vibration of the viscoelastic Timoshenko beam. Journal of Applied Mechanics, 52(3), 728–731. 45. Gibson, R. F. 1992. Damping characteristics of composite materials and structures. Journal of Engineering Materials and Performance, 1(1), 11–20. 46. Gibson, R. F. 1987. Dynamic mechanical properties of advanced composite materials and structures: A review. The Shock and Vibration Digest, 19(7), 13–22. 47. Gibson, R. F. 1990. Dynamic mechanical properties of advanced composite materials and structures: A review of recent research. The Shock and Vibration Digest, 22(8), 3–12. 48. Bert, C. W. 1980. Composite materials: A survey of the damping capacity of iber reinforced composites. In Torvik, P. J. ed., Damping Applications for Vibration Control, AMD Vol. 38, pp. 53–63. American Society of Mechanical Engineers, New York, NY. 49. Adams, R. D. 1987. Damping properties analysis of composites. In Reinhart, T. J. ed., Engineered Materials Handbook, Vol. 1, Composites, pp. 206–217. ASM International, Materials Park, OH. 50. Chaturvedi, S. K. 1989. Damping of polymer matrix composite materials. In Lee, S. ed., Encyclopedia of Composites. VCH Publishing Co., New York, NY. 51. Kinra, V. K. and Wolfenden, A. eds. 1992. M3D: Mechanics and Mechanisms of Material Damping, ASTM STP 1169. American Society for Testing and Materials, Philadelphia, PA. 52. Sun, C. T. and Lu, Y. P. 1995. Vibration Damping of Structural Elements. PrenticeHall, Englewood Cliffs, NJ. Analysis of Viscoelastic and Dynamic Behavior 517 53. Zener, C. 1948. Elasticity and Anelasticity of Metals. The University of Chicago Press, Chicago, IL. 54. Granato, A. V. and Lucke, K. 1956. Application of dislocation theory to internal friction phenomena at high frequencies. Journal of Applied Physics, 27(7), 789–805. 55. Sun, C. T., Chaturvedi, S. K., and Gibson, R. F. 1985. Internal material damping of polymer matrix composites under off-axis loading. Journal of Materials Science, 20, 2575–2585. 56. Sun, C. T., Wu, J. K., and Gibson, R. F. 1985. Prediction of material damping in randomly oriented short iber polymer matrix composites. Journal of Reinforced, Plastics and Composites, 4, 262–272. 57. Pant, R. H. and Gibson, R. F. 1996. Analysis and testing of dynamic micromechanical behavior of composite materials at elevated temperatures. Journal of Engineering Materials and Technology, 118, 554–560. 58. Finegan, I. C. and Gibson, R. F. 2000. Analytical modeling of damping at micromechanical level in polymer composites reinforced with coated ibers. Composites Science and Technology, 60, 1077–1084. 59. Guan, H. and Gibson, R. F. 2001. Micromechanical models for damping in woven fabric-reinforced polymer matrix composites. Journal of Composite Materials, 35(16), 1417–1434. 60. Nashif, A. D., Jones, D. I. G., and Henderson, J. P. 1985. Vibration Damping. John Wiley & Sons, New York, NY. 61. Ungar, E. E. and Kerwin, E. M. Jr. 1962. Loss factors of viscoelastic systems in terms of strain energy. Journal of the Acoustical Society of America, 34(2), 954–958. 62. Gibson, R. F., Chaturvedi, S. K., and Sun, C. T. 1982. Complex moduli of aligned discontinuous iber reinforced polymer composites. Journal of Materials Science, 17, 3499–3509. 63. Johnson, C. D. and Kienholz, D. A. 1982. Finite element prediction of damping in structures with constrained viscoelastic layers. AIAA Journal, 20(9), 1284–1290. 64. Hwang, S. J. and Gibson, R. F. 1987. Micromechanical modeling of damping in discontinuous iber composites using a strain energy/inite element approach. Journal of Engineering Materials and Technology, 109, 47–52. 65. Gibson, R. F., Hwang, S. J., and Kwak, H. 1991. Micromechanical modeling of damping in composites including interphase effects. How Concept Becomes Reality—Proceedings of 36th International SAMPE Symposium, Vol. 1, pp. 592–606. Society for the Advancement of Material and Process Engineering, Covina, CA. 66. Hwang, S. J. and Gibson, R. F. 1991. The effects of 3-D states of stress on damping of laminated composites. Composites Science and Technology, 41, 379–393. 67. Hwang, S. J. and Gibson, R. F. 1992. Contribution of interlaminar stresses to damping in thick laminated composites under uniaxial extension. Composite Structures, 20, 29–35. 68. Hwang, S. J., Gibson, R. F., and Singh, J. 1992. Decomposition of coupling effects on damping of laminated composites under lexural vibration. Composites Science and Technology, 43, 159–169. 69. Mantena, P. R., Gibson, R. F., and Hwang, S. J. 1991. Optimal constrained viscoelastic tape lengths for maximizing damping in laminated composites. AIAA Journal, 29(10), 1678–1685. 518 Principles of Composite Material Mechanics 70. Hwang, S. J. and Gibson, R. F. 1992. The use of strain energy-based inite element techniques in the analysis of various aspects of damping of composite materials and structures. Journal of Composite Materials, 26(17), 2585–2605. 71. Chen, Y. and Gibson, R. F. 2003. Analytical and experimental studies of composite isogrid structures with integral passive damping. Mechanics of Advanced Materials and Structures, 10(2), 127–143. 72. Plagianakos, T. S. and Saravanos, D. S. 2003. Mechanics and inite elements for the damped dynamic characteristics of curvilinear laminates and composite shell structures. Journal of Sound and Vibration, 263(2), 399–414. 73. Li, Z. and Crocker, M. J. 2005. A review on vibration damping in sandwich composite structures. International Journal of Acoustics and Vibration, 10(4), 159–169. 74. Gibson, R. F., Ayorinde, E. O., and Wen, Y. F. 2007. Vibrations of carbon nanotubes and their composites: A review. Composites Science and Technology, 67(1), 1–28. 75. Koratkar, N. A., Suhr, J., Joshi, A., Kane, R. S., Schadler, L. S., Ajayan, P. M., and Bartolucci, S. 2005. Characterizing energy dissipation in single-walled carbon nanotube polycarbonate composites. Applied Physics Letters, 87, 063102. 76. Zhou, X., Shin, E., Wang, K. W., and Bakis, C. E. 2004. Interfacial damping characteristics of carbon nanotube composites. Composites Science and Technology, 64, 2425–2437. 77. Rajoria, H. and Jalili, N. 2005. Passive vibration damping enhancement using carbon nanotube–epoxy reinforced composites. Composites Science and Technology, 65, 2079–2093. 78. Zhang, W., Joshi, A., Wang, Z., Kane, R. S., and Koratkar, N. 2007. Creep mitigation in composites using carbon nanotube additives. Nanotechnology, 18, 185703. 79. Yang, J., Zhang, Z., Friedrich, K., and Schlarb, A. K. 2007. Resistance to timedependent deformation of nanoparticle/polymer composites. Applied Physics Letters, 91, 011901. 80. Zhou, T. H., Ruan, W. H., Yang, J. L., Rong, M. Z., Zhang, M. Q., and Zhang, Z. 2007. A novel route for improving creep resistance of polymers using nanoparticles. Composites Science and Technology, 67, 2297–2302. 81. Varela-Rizo, H., Weisenberger, M., Bortz, D. R., and Martin-Gullon, I. 2010. Fracture toughness and creep performance of PMMA composites containing micro and nanosized carbon ilaments. Composites Science and Technology, 70, 1189–1195. 82. Jones, R. M. 1973. Buckling and vibration of unsymmetrically laminated crossply rectangular plates. AIAA Journal, 11(12), 1626–1632. 9 Analysis of Fracture 9.1 Introduction Except for a brief discussion in Section 7.8.2, the previous chapters of this book have not considered the analysis of the effects of notches, cracks, delaminations, or other discontinuities in composites. For example, the conventional strength analyses outlined in Chapter 4 involved the use of gross “effective lamina strengths” in various semiempirical failure criteria irrespective of speciic micromechanical failure modes that are related to such discontinuities. While such procedures, along with the use of empirical “safety factors,” may produce a satisfactory design for static loading, failures may still occur due to the growth of cracks or delaminations under dynamic loading. The purpose of this chapter is to give an introduction to the analysis of fracture of composites due to cracks, notches, and delaminations. First, the prediction of the strength of composites with through-thickness cracks and notches is considered by using both fracture mechanics and stress fracture approaches. Next, the use of fracture mechanics in the analysis of interlaminar fracture will be discussed. Each of these topics is the subject of many publications. Thus, only brief introductions to the subjects are given here, along with key references where more detailed analyses may be found. Each of these topics is also the subject of considerable current research, and the reader is encouraged to consult technical journals for the results of the most recent research. Composites handbooks provide information on the basics of composite fracture [1]. The Special Technical Publication series by the American Society for Testing and Materials is a good source of recent research indings [2–7]. The application of fracture mechanics to composites is the subject of a book [8], as is delamination in composites [9]. 9.2 Fracture Mechanics Analyses of Through-Thickness Cracks Much of the early work on fracture in composites involved investigations of the applicability of linear elastic fracture mechanics, which had been 519 Principles of Composite Material Mechanics 520 originally developed for the analysis of through-thickness cracks in homogeneous, isotropic metals. The origin of fracture mechanics can be traced back to the seminal work of Grifith [10], who explained the discrepancy between the measured and predicted strength of glass by considering the stability of a small crack. The stability criterion was developed by using an energy balance on the crack. Consider the through-thickness crack in the uniaxially loaded homogeneous, isotropic, and linear elastic plate of ininite width shown in Figure 9.1. Grifith reasoned that the strain energy of the cracked plate would be less than the corresponding strain energy of the uncracked plate, and from a stress analysis, he estimated that the strain energy released by the creation of the crack under plane stress conditions would be Ur = πσ 2 a 2t E (9.1) where Ur = strain energy released σ = applied stress a = half-crack length t = plate thickness E = modulus of elasticity of the plate The corresponding expression in Grifith’s original paper was later found to be in error, and Equation 9.1 is consistent with the corrected expression σ t Crack 4a 2a Elliptical zone assumed to be relaxed due to presence of crack FIGURE 9.1 Grifith crack: a through-thickness crack in a uniaxially stressed plate of ininite width. Analysis of Fracture 521 in more recent publications [11,12]. In addition, Grifith’s energy terms were given on a per unit thickness basis. Equation 9.1 is also consistent with the strain energy released by relaxation of an elliptical zone having major and minor axes of lengths 4a and 2a, respectively, where the minor axis is coincident with the crack and the major axis is perpendicular to the crack. The volume of such an ellipse is V = π(2a)( a)(t) = 2πa 2t (9.2) Since the plate was assumed to be uniformly stressed before the introduction of the crack, the strain energy released due to relaxation of the elliptical volume around the crack is Ur = 1 σ2 πσ 2 a 2t V= E 2 E (9.3) Grifith also assumed that the creation of new crack surfaces required the absorption of an amount of energy given by U s = 4 at γ s (9.4) where Us = energy absorbed by creation of new crack surfaces γs = surface energy per unit area As the crack grows, if the rate at which energy is absorbed by creating new surfaces is greater than the rate at which strain energy is released, then ∂U s ∂U r > ∂a ∂a (9.5) and the crack growth is stable. If the strain energy is released at a greater rate than it can be absorbed, then ∂U r ∂U s > ∂a ∂a (9.6) and the crack growth is unstable. The threshold of stability or the condition of neutral equilibrium, is therefore given by ∂U r ∂U s = ∂a ∂a (9.7) 522 Principles of Composite Material Mechanics or πσ 2 a = 2γ s E (9.8) Thus, the critical stress, σc, for self-sustaining extension of the crack in plane stress is σc = 2Eγ s πa (9.9) Alternatively, the critical law size for plane stress at stress level σ is ac = 2Eγ s πσ 2 (9.10) It is interesting to note that when we rearrange Equation 9.8 as σ πa = 2Eγ s (9.11) the terms on the left-hand side depend only on loading and geometry, whereas the terms on the right-hand side depend only on material properties. Thus, when the stress reaches the critical fracture stress, σc, the lefthand side becomes σ c πa . The term σ c πa is now referred to as the fracture toughness, Kc. This is a very important concept, which we will return to later. The application of the Grifith-type analysis to composites presents some dificulties, but, fortunately, many of these problems have been solved over the years since Grifith’s work. For example, for metals and many polymers, the energy absorbed in crack extension is actually greater than the surface energy. Recognizing this, both Irwin [13] and Orowan [14] modiied the Grifith analysis to include energy absorption due to plastic deformation at the crack tip. In this analysis, the factor 2γs on the right-hand side of Equation 9.8 and in all subsequent equations is replaced by the factor 2(γs + γp), where γp is the energy of plastic deformation. The solutions of several other problems encountered in the development of composite fracture mechanics have been made possible by the use of several different analytical techniques. Two of these techniques, now referred to as the “stress intensity factor” approach and the “strain energy release rate” approach, will be discussed in the following sections. 9.2.1 Stress Intensity Factor Approach The Grifith analysis was originally developed for homogeneous, isotropic materials. Using effective modulus theory, we can replace the heterogeneous, Analysis of Fracture 523 anisotropic composite with an equivalent homogeneous, anisotropic material. It turns out that by considering the stress distribution around the crack tip, we can develop another interpretation of the Grifith analysis which can be applied equally well to homogeneous isotropic or anisotropic materials and to states of stress other than the simple uniaxial stress that Grifith used. Referring to the plane stress condition in the vicinity of the uniaxially loaded crack in Figure 9.2, Westergaard [15] used a complex stress function approach to show that the stresses for the isotropic case at a point P deined by polar coordinates (r, θ) can be expressed as σx = KI f1(θ) 2πr (9.12) σy = KI f 2 (θ) 2πr (9.13) τ xy = KI f 3 (θ) 2πr (9.14) where KI is the stress intensity factor for the crack opening mode, as deined by K I = σ πa (9.15) and the fi(θ) are trigonometric functions of the angle. Irwin [16] recognized that the term σ πa controls the magnitudes of the stresses at a point (r, θ) near the crack tip. Returning to the discussion following Equation 9.11, we see that the critical value of the stress intensity factor, KIc, corresponding to the critical stress, σc, is the fracture toughness. That is, K Ic = σ c πa (9.16) σy y τxy P σx p r θ Crack tip FIGURE 9.2 Stresses at the tip of a crack under plane stress. x Principles of Composite Material Mechanics 524 The fracture toughness, KIc, is a material property that can be determined experimentally, as shown later. Thus, if the fracture toughness of the material is known, the fracture mechanics analysis can be used in two ways, depending on whether the applied stress or the crack size is known. If the applied stress, σ, is known, equations such as Equation 9.15 can be used to ind the critical crack size, ac, which will lead to unstable and catastrophic crack growth. Knowing the critical crack size, we can specify inspection of the component in question to make sure that there are no cracks of that size. On the other hand, if the crack size, a, is known, then equations such as Equation 9.15 can be used to ind the critical stress, σc, which will lead to unstable and catastrophic crack growth. Loading on the component in question would then be speciied so as not to exceed this stress. The reader is cautioned that the stress intensity factor is deined as k1 = σ a in some publications. This deinition corresponds to the cancellation of π in both the numerator and the denominator of Equations 9.12 through 9.14, so that the denominator corresponding to k1 would be 2r instead of 2πr , and thus K I = k1 π. Expressions for stress distributions for other types of loading and crack geometries in isotropic materials lead to expressions that are similar to Equations 9.12 through 9.14, and the corresponding stress intensity factors can be found in the same way [17]. Other important results such as inite width correction factors (recall that the Grifith analysis is for a crack in an ininite width plate) have been tabulated in Reference 17. The three basic modes of crack deformation are shown in Figure 9.3. Thus, for the crack opening mode in the above example (mode I), we have the stress intensity factor K I. For the in-plane shear mode (mode II), we have the stress intensity factor K II, and for the antiplane shear mode (mode III), we have K III. For example, for the cases of pure shear loading in modes II and III, we h